655 7 11MB
English Pages 790 Year 2006
SEMICONDUCTOR MATERIAL AND DEVICE CHARACTERIZATION
SEMICONDUCTOR MATERIAL AND DEVICE CHARACTERIZATION Third Edition
DIETER K. SCHRODER Arizona State University Tempe, AZ
A JOHN WILEY & SONS, INC., PUBLICATION
Copyright 2006 by John Wiley & Sons, Inc. All rights reserved. Published by John Wiley & Sons, Inc., Hoboken, New Jersey. Published simultaneously in Canada. No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning, or otherwise, except as permitted under Section 107 or 108 of the 1976 United States Copyright Act, without either the prior written permission of the Publisher, or authorization through payment of the appropriate percopy fee to the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, (978) 7508400, fax (978) 7504470, or on the web at www.copyright.com. Requests to the Publisher for permission should be addressed to the Permissions Department, John Wiley & Sons, Inc., 111 River Street, Hoboken, NJ 07030, (201) 7486011, fax (201) 7486008, or online at http://www.wiley.com/go/permission. Limit of Liability/Disclaimer of Warranty: While the publisher and author have used their best efforts in preparing this book, they make no representations or warranties with respect to the accuracy or completeness of the contents of this book and specifically disclaim any implied warranties of merchantability or fitness for a particular purpose. No warranty may be created or extended by sales representatives or written sales materials. The advice and strategies contained herein may not be suitable for your situation. You should consult with a professional where appropriate. Neither the publisher nor author shall be liable for any loss of profit or any other commercial damages, including but not limited to special, incidental, consequential, or other damages. For general information on our other products and services or for technical support, please contact our Customer Care Department within the United States at (800) 7622974, outside the United States at (317) 5723993 or fax (317) 5724002. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic formats. For more information about Wiley products, visit our web site at www.wiley.com. Library of Congress CataloginginPublication Data: Schroder, Dieter K. Semiconductor material and device characterization / by Dieter K. Schroder. p. cm. “A WileyInterscience Publication.” Includes bibliographical references and index. ISBN13: 9780471739067 (acidfree paper) ISBN10: 0471739065 (acidfree paper) 1. Semiconductors. 2. Semiconductors–Testing. I. Title. QC611.S335 2005 621.3815′ 2—dc22 2005048514 Printed in the United States of America. 10 9 8 7 6 5 4 3 2 1
CONTENTS
Preface to Third Edition 1 Resistivity 1.1 1.2
1.3
1.4
1.5 1.6 1.7
xiii 1
Introduction, 1 TwoPoint Versus FourPoint Probe, 2 1.2.1 Correction Factors, 8 1.2.2 Resistivity of Arbitrarily Shaped Samples, 14 1.2.3 Measurement Circuits, 18 1.2.4 Measurement Errors and Precautions, 18 Wafer Mapping, 21 1.3.1 Double Implant, 21 1.3.2 Modulated Photoreflectance, 23 1.3.3 Carrier Illumination (CI), 24 1.3.4 Optical Densitometry, 25 Resistivity Profiling, 25 1.4.1 Differential Hall Effect (DHE), 26 1.4.2 Spreading Resistance Profiling (SRP), 29 Contactless Methods, 34 1.5.1 Eddy Current, 34 Conductivity Type, 38 Strengths and Weaknesses, 40 Appendix 1.1 Resistivity as a Function of Doping Density, 41 Appendix 1.2 Intrinsic Carrier Density, 43 References, 44 Problems, 50 Review Questions, 59 v
vi
CONTENTS
2 Carrier and Doping Density
61
2.1 Introduction, 61 2.2 CapacitanceVoltage (CV), 61 2.2.1 Differential Capacitance, 61 2.2.2 Band Offsets, 68 2.2.3 MaximumMinimum MOSC Capacitance, 71 2.2.4 Integral Capacitance, 75 2.2.5 Mercury Probe Contacts, 76 2.2.6 Electrochemical C –V Profiler (ECV), 77 2.3 CurrentVoltage (IV), 79 2.3.1 MOSFET Substrate Voltage—Gate Voltage, 79 2.3.2 MOSFET Threshold Voltage, 81 2.3.3 Spreading Resistance, 82 2.4 Measurement Errors and Precautions, 82 2.4.1 Debye Length and Voltage Breakdown, 82 2.4.2 Series Resistance, 83 2.4.3 Minority Carriers and Interface Traps, 89 2.4.4 Diode Edge and Stray Capacitance, 90 2.4.5 Excess Leakage Current, 91 2.4.6 Deep Level Dopants/Traps, 91 2.4.7 SemiInsulating Substrates, 93 2.4.8 Instrumental Limitations, 94 2.5 Hall Effect, 94 2.6 Optical Techniques, 97 2.6.1 Plasma Resonance, 97 2.6.2 Free Carrier Absorption, 98 2.6.3 Infrared Spectroscopy, 99 2.6.4 Photoluminescence (PL), 101 2.7 Secondary Ion Mass Spectrometry (SIMS), 102 2.8 Rutherford Backscattering (RBS), 103 2.9 Lateral Profiling, 104 2.10 Strengths and Weaknesses, 105 Appendix 2.1 Parallel or Series Connection?, 107 Appendix 2.2 Circuit Conversion, 108 References, 109 Problems, 117 Review Questions, 124 3 Contact Resistance and Schottky Barriers 3.1 3.2 3.3 3.4
Introduction, 127 MetalSemiconductor Contacts, 128 Contact Resistance, 131 Measurement Techniques, 135 3.4.1 TwoContact TwoTerminal Method, 135 3.4.2 MultipleContact TwoTerminal Methods, 138 3.4.3 FourTerminal Contact Resistance Method, 149 3.4.4 SixTerminal Contact Resistance Method, 156
127
CONTENTS
3.5
3.6 3.7
3.4.5 NonPlanar Contacts, 156 Schottky Barrier Height, 157 3.5.1 CurrentVoltage, 158 3.5.2 Current—Temperature, 160 3.5.3 CapacitanceVoltage, 161 3.5.4 Photocurrent, 162 3.5.5 Ballistic Electron Emission Microscopy (BEEM), 163 Comparison of Methods, 163 Strengths and Weaknesses, 164 Appendix 3.1 Effect of Parasitic Resistance, 165 Appendix 3.2 Alloys for Contacts to Semiconductors, 167 References, 168 Problems, 174 Review Questions, 184
4 Series Resistance, Channel Length and Width, and Threshold Voltage 4.1 4.2
4.3 4.4
4.5
4.6
4.7 4.8
4.9 4.10
vii
Introduction, 185 PN Junction Diodes, 185 4.2.1 CurrentVoltage, 185 4.2.2 OpenCircuit Voltage Decay (OCVD), 188 4.2.3 CapacitanceVoltage (C –V ), 190 Schottky Barrier Diodes, 190 4.3.1 Series Resistance, 190 Solar Cells, 192 4.4.1 Series Resistance—Multiple Light Intensities, 195 4.4.2 Series Resistance—Constant Light Intensity, 196 4.4.3 Shunt Resistance, 197 Bipolar Junction Transistors, 198 4.5.1 Emitter Resistance, 200 4.5.2 Collector Resistance, 202 4.5.3 Base Resistance, 202 MOSFETS, 206 4.6.1 Series Resistance and Channel Length–CurrentVoltage, 206 4.6.2 Channel Length—CapacitanceVoltage, 216 4.6.3 Channel Width, 218 MESFETS and MODFETS, 219 Threshold Voltage, 222 4.8.1 Linear Extrapolation, 223 4.8.2 Constant Drain Current, 225 4.8.3 Subthreshold Drain Current, 226 4.8.4 Transconductance, 227 4.8.5 Transconductance Derivative, 228 4.8.6 Drain Current Ratio, 228 Pseudo MOSFET, 230 Strengths and Weaknesses, 231 Appendix 4.1 Schottky Diode CurrentVoltage Equation, 231 References, 232
185
viii
CONTENTS
Problems, 238 Review Questions, 250 5 Defects
251
5.1 Introduction, 251 5.2 GenerationRecombination Statistics, 253 5.2.1 A Pictorial View, 253 5.2.2 A Mathematical Description, 255 5.3 Capacitance Measurements, 258 5.3.1 SteadyState Measurements, 259 5.3.2 Transient Measurements, 259 5.4 Current Measurements, 267 5.5 Charge Measurements, 269 5.6 DeepLevel Transient Spectroscopy (DLTS), 270 5.6.1 Conventional DLTS, 270 5.6.2 Interface Trapped Charge DLTS, 280 5.6.3 Optical and Scanning DLTS, 283 5.6.4 Precautions, 285 5.7 Thermally Stimulated Capacitance and Current, 288 5.8 Positron Annihilation Spectroscopy (PAS), 289 5.9 Strengths and Weaknesses, 292 Appendix 5.1 Activation Energy and Capture CrossSection, 293 Appendix 5.2 Time Constant Extraction, 294 Appendix 5.3 Si and GaAs Data, 296 References, 301 Problems, 308 Review Questions, 316 6 Oxide and Interface Trapped Charges, Oxide Thickness 6.1 Introduction, 319 6.2 Fixed, Oxide Trapped, and Mobile Oxide Charge, 321 6.2.1 CapacitanceVoltage Curves, 321 6.2.2 Flatband Voltage, 327 6.2.3 Capacitance Measurements, 331 6.2.4 Fixed Charge, 334 6.2.5 GateSemiconductor Work Function Difference, 335 6.2.6 Oxide Trapped Charge, 338 6.2.7 Mobile Charge, 338 6.3 Interface Trapped Charge, 342 6.3.1 Low Frequency (Quasistatic) Methods, 342 6.3.2 Conductance, 347 6.3.3 High Frequency Methods, 350 6.3.4 Charge Pumping, 352 6.3.5 MOSFET Subthreshold Current, 359 6.3.6 DCIV, 361 6.3.7 Other Methods, 363
319
CONTENTS
6.4
6.5
Oxide Thickness, 364 6.4.1 CapacitanceVoltage, 364 6.4.2 CurrentVoltage, 369 6.4.3 Other Methods, 369 Strengths and Weaknesses, 369 Appendix 6.1 Capacitance Measurement Techniques, 371 Appendix 6.2 Effect of Chuck Capacitance and Leakage Current, 372 References, 374 Problems, 381 Review Questions, 387
7 Carrier Lifetimes 7.1 7.2 7.3 7.4
7.5
7.6
7.7
389
Introduction, 389 Recombination Lifetime/Surface Recombination Velocity, 390 Generation Lifetime/Surface Generation Velocity, 394 Recombination Lifetime—Optical Measurements, 395 7.4.1 Photoconductance Decay (PCD), 399 7.4.2 QuasiSteadyState Photoconductance (QSSPC), 402 7.4.3 ShortCircuit Current/OpenCircuit Voltage Decay (SCCD/OCVD), 402 7.4.4 Photoluminescence Decay (PLD), 404 7.4.5 Surface Photovoltage (SPV), 404 7.4.6 SteadyState ShortCircuit Current (SSSCC), 411 7.4.7 Free Carrier Absorption, 413 7.4.8 Electron Beam Induced Current (EBIC), 416 Recombination Lifetime—Electrical Measurements, 417 7.5.1 Diode CurrentVoltage, 417 7.5.2 Reverse Recovery (RR), 420 7.5.3 OpenCircuit Voltage Decay (OCVD), 422 7.5.4 Pulsed MOS Capacitor, 424 7.5.5 Other Techniques, 428 Generation Lifetime—Electrical Measurements, 429 7.6.1 GateControlled Diode, 429 7.6.2 Pulsed MOS Capacitor, 432 Strengths and Weaknesses, 440 Appendix 7.1 Optical Excitation, 441 Appendix 7.2 Electrical Excitation, 448 References, 448 Problems, 458 Review Questions, 464
8 Mobility 8.1 8.2 8.3
ix
Introduction, 465 Conductivity Mobility, 465 Hall Effect and Mobility, 466 8.3.1 Basic Equations for Uniform Layers or Wafers, 466 8.3.2 Nonuniform Layers, 471
465
x
CONTENTS
8.4 8.5 8.6
8.7 8.8
8.3.3 Multi Layers, 474 8.3.4 Sample Shapes and Measurement Circuits, 475 Magnetoresistance Mobility, 479 TimeofFlight Drift Mobility, 482 MOSFET Mobility, 489 8.6.1 Effective Mobility, 489 8.6.2 FieldEffect Mobility, 500 8.6.3 Saturation Mobility, 502 Contactless Mobility, 502 Strengths and Weaknesses, 502 Appendix 8.1 Semiconductor Bulk Mobilities, 503 Appendix 8.2 Semiconductor Surface Mobilities, 506 Appendix 8.3 Effect of Channel Frequency Response, 506 Appendix 8.4 Effect of Interface Trapped Charge, 507 References, 508 Problems, 514 Review Questions, 521
9 Chargebased and Probe Characterization
523
9.1 9.2 9.3 9.4 9.5
Introduction, 523 Background, 524 Surface Charging, 525 The Kelvin Probe, 526 Applications, 533 9.5.1 Surface Photovoltage (SPV), 533 9.5.2 Carrier Lifetimes, 534 9.5.3 Surface Modification, 537 9.5.4 NearSurface Doping Density, 538 9.5.5 Oxide Charge, 538 9.5.6 Oxide Thickness and Interface Trap Density, 540 9.5.7 Oxide Leakage Current, 541 9.6 Scanning Probe Microscopy (SPM), 542 9.6.1 Scanning Tunneling Microscopy (STM), 543 9.6.2 Atomic Force Microscopy (AFM), 544 9.6.3 Scanning Capacitance Microscopy (SCM), 547 9.6.4 Scanning Kelvin Probe Microscopy (SKPM), 550 9.6.5 Scanning Spreading Resistance Microscopy (SSRM), 553 9.6.6 Ballistic Electron Emission Microscopy (BEEM), 554 9.7 Strengths and Weaknesses, 556 References, 556 Problems, 560 Review Questions, 561 10 Optical Characterization 10.1 Introduction, 563 10.2 Optical Microscopy, 564 10.2.1 Resolution, Magnification, Contrast, 565
563
xi
CONTENTS
10.2.2 DarkField, Phase, and Interference Contrast Microscopy, 568 10.2.3 Confocal Optical Microscopy, 570 10.2.4 Interferometric Microscopy, 572 10.2.5 Defect Etches, 575 10.2.6 NearField Optical Microscopy (NFOM), 575 10.3 Ellipsometry, 579 10.3.1 Theory, 579 10.3.2 Null Ellipsometry, 581 10.3.3 Rotating Analyzer Ellipsometry, 582 10.3.4 Spectroscopic Ellipsometry (SE), 583 10.3.5 Applications, 584 10.4 Transmission, 585 10.4.1 Theory, 585 10.4.2 Instrumentation, 587 10.4.3 Applications, 590 10.5 Reflection, 592 10.5.1 Theory, 592 10.5.2 Applications, 594 10.5.3 Internal Reflection Infrared Spectroscopy, 598 10.6 Light Scattering, 599 10.7 Modulation Spectroscopy, 600 10.8 Line Width, 601 10.8.1 OpticalPhysical Methods, 601 10.8.2 Electrical Methods, 603 10.9 Photoluminescence (PL), 604 10.10 Raman Spectroscopy, 608 10.11 Strengths and Weaknesses, 610 Appendix 10.1 Transmission Equations, 611 Appendix 10.2 Absorption Coefficients and Refractive Indices for Selected Semiconductors, 613 References, 615 Problems, 621 Review Questions, 626 11 Chemical and Physical Characterization 11.1 11.2
11.3
Introduction, 627 Electron Beam Techniques, 628 11.2.1 Scanning Electron Microscopy (SEM), 629 11.2.2 Auger Electron Spectroscopy (AES), 634 11.2.3 Electron Microprobe (EMP), 639 11.2.4 Transmission Electron Microscopy (TEM), 645 11.2.5 Electron Beam Induced Current (EBIC), 649 11.2.6 Cathodoluminescence (CL), 651 11.2.7 LowEnergy, HighEnergy Electron Diffraction (LEED), 652 Ion Beam Techniques, 653 11.3.1 Secondary Ion Mass Spectrometry (SIMS), 654 11.3.2 Rutherford Backscattering Spectrometry (RBS), 659
627
xii
CONTENTS
11.4 XRay and GammaRay Techniques, 665 11.4.1 XRay Fluorescence (XRF), 666 11.4.2 XRay Photoelectron Spectroscopy (XPS), 668 11.4.3 XRay Topography (XRT), 671 11.4.4 Neutron Activation Analysis (NAA), 674 11.5 Strengths and Weaknesses, 676 Appendix 11.1 Selected Features of Some Analytical Techniques, 678 References, 678 Problems, 686 Review Questions, 687 12 Reliability and Failure Analysis
689
12.1 Introduction, 689 12.2 Failure Times and Acceleration Factors, 690 12.2.1 Failure Times, 690 12.2.2 Acceleration Factors, 690 12.3 Distribution Functions, 692 12.4 Reliability Concerns, 695 12.4.1 Electromigration (EM), 695 12.4.2 Hot Carriers, 701 12.4.3 Gate Oxide Integrity (GOI), 704 12.4.4 Negative Bias Temperature Instability (NBTI), 711 12.4.5 Stress Induced Leakage Current (SILC), 712 12.4.6 Electrostatic Discharge (ESD), 712 12.5 Failure Analysis Characterization Techniques, 713 12.5.1 Quiescent Drain Current (IDDQ ), 713 12.5.2 Mechanical Probes, 715 12.5.3 Emission Microscopy (EMMI), 715 12.5.4 Fluorescent Microthermography (FMT), 718 12.5.5 Infrared Thermography (IRT), 718 12.5.6 Voltage Contrast, 718 12.5.7 Laser Voltage Probe (LVP), 719 12.5.8 Liquid Crystals (LC), 720 12.5.9 Optical Beam Induced Resistance Change (OBIRCH), 721 12.5.10 Focused Ion Beam (FIB), 723 12.5.11 Noise, 723 12.6 Strengths and Weaknesses, 726 Appendix 12.1 Gate Currents, 728 References, 730 Problems, 737 Review Questions, 740 Appendix 1 List of Symbols
741
Appendix 2 Abbreviations and Acronyms
749
Index
755
PREFACE TO THIRD EDITION
Semiconductor characterization has continued its relentless advance since the publication of the second edition. New techniques have been developed, others have been refined. In the second edition preface I mentioned that techniques such as scanning probe, totalreflection Xray fluorescence and contactless lifetime/diffusion length measurements had become routine. In the intervening years, probe techniques have further expanded, chargebased techniques have become routine, as has transmission electron microscopy through the use of focused ion beam sample preparation. Line width measurements have become more difficult since lines have become very narrow and the traditional SEM and electrical measurements have been augmented by optical techniques like scatterometry and spectroscopic ellipsometry. In addition to new measurement techniques, the interpretation of existing techniques has changed. For example, the high leakage currents of thin oxides make it necessary to alter existing techniques/theories for many MOSbased techniques. I have rewritten parts of each chapter and added two new chapters, deleted some outdated material, clarified some obscure/confusing parts that have been pointed out to me. I have redone most of the figures, deleted some outdated ones or replaced them with more recent data. The third edition is further enhanced through additional problems and review questions at the end of each chapter and examples throughout the book, to make it a more attractive textbook. I have added 260 new references to bring the book as uptodate as possible. I have also changed the symbol for sheet resistance from ρs to Rsh , to bring it in line with more accepted use. I list the main additional or expanded material here briefly by chapter. There are many other smaller changes throughout the book.
Chapter 1 New sheet resistance explanation; new 4point probe derivation; use of 4point probe for shallow junctions and high sheet resistance sample; added the Carrier Illumination method. xiii
xiv
PREFACE TO THIRD EDITION
Chapter 2 Contactless C –V added; integral capacitance augmented; series capacitance added/augmented; free carrier absorption augmented; new lateral profiling section; added Appendix 2—equivalent circuit derivations. Chapter 3 Augmented circular contact resistance section; added considerations of parasitic resistance in TLM method; expanded barrier height section by adding BEEM; added Appendix dealing with parasitic resistance effects. Chapter 4 Added section of pseudo MOSFETs for silicononinsulator characterization; added several MOSFET effective channel length measurement methods and deleted some of the older methods. Chapter 5 Added Laplace DLTS; added a section to the time constant extraction portion in Appendix 5.2. Chapter 6 Expanded the section on oxide thickness measurements; added considerations for the effect of leaky gate oxides on conductance and charge pumping; added the DCI V method; expanded the section on gate oxide leakage currents; added Appendix 6.2 considering the effects of wafer chuck parasitic capacitance and leakage current. Chapter 7 Clarified the optical lifetime section; added Quasisteadystate Photoconductance; augmented the free carrier absorption and diode current lifetime method; added leaky oxide current considerations to the pulsed MOS capacitor technique. Chapter 8 Added the effects of gate depletion, channel location, gate current, interface traps, and inversion charge frequency response to the extraction of the effective mobility. I also added a section on contactless mobility measurements. Chapter 9 This chapter is new and introduces chargebased measurement and Kelvin probes. I have also included probebased measurements here and expanded these by including scanning capacitance, scanning Kelvin force, scanning spreading resistance, and ballistic electron emission microscopy. Chapter 10 Expanded confocal optical microscopy, photoluminescence, and line width measurement. Chapter 11 Made some small changes.
PREFACE TO THIRD EDITION
xv
Chapter 12 This is a new chapter, dealing with Failure Analysis and Reliability. I have taken some sections from other chapters in the second edition and expanded them. I introduce failure times and distribution functions here, then discuss electromigration; hot carriers; gate oxide integrity; negative bias temperature instability; stress induced leakage current; electrostatic discharge that are of concern for device reliability. The rest of this chapter deals with the more common failure analysis techniques: quiescent drain current; mechanical probes; emission microscopy; fluorescent microthermography; infrared thermography; voltage contrast; laser voltage probe; liquid crystals; optical beam induced resistance change and noise. Several people have supplied experimental data and several concepts were clarified by discussions with experts in the semiconductor industry. I acknowledge their contributions in the figure captions. Tom Shaffner from the National Institute of Standards and Technology has continued to be an excellent source of knowledge and a good friend and Steve Kilgore from Freescale Semiconductor has helped with electromigration concepts. The recent book Handbook of Silicon Semiconductor Metrology, edited by Alain Diebold, is an excellent companion volume as it gives many of the practical details of semiconductor metrology missing here. I thank executive editor G. Telecki, R. Witmer and M. Yanuzzi from John Wiley & Sons for editorial assistance in bringing this edition to print. DIETER K. SCHRODER Tempe, AZ
1 RESISTIVITY
1.1
INTRODUCTION
The resistivity ρ of a semiconductor is important for starting material as well as for semiconductor devices. Although carefully controlled during crystal growth, it is not truly uniform in the grown ingot due to variability during growth and segregation coefficients less than unity for the common dopant atoms. The resistivity of epitaxially grown layers is generally very uniform. Resistivity is important for devices because it contributes to the device series resistance, capacitance, threshold voltage, hot carrier degradation of MOS devices, latch up of CMOS circuits, and other parameters. The wafers resistivity is usually modified locally during device processing by diffusion and ion implantation, for example. The resistivity depends on the free electron and hole densities n and p, and the electron and hole mobilities µn and µp according to the relationship
ρ=
1 q(nµn + pµp )
(1.1)
ρ can be calculated from the measured carrier densities and mobilities. For extrinsic materials in which the majority carrier density is much higher than the minority carrier density, it is generally sufficient to know the majority carrier density and the majority carrier mobility. The carrier densities and mobilities are generally not known, however. Hence we must look for alternative measurement techniques, ranging from contactless, through temporary contact to permanent contact techniques. Semiconductor Material and Device Characterization, Third Edition, by Dieter K. Schroder Copyright 2006 John Wiley & Sons, Inc.
1
2
RESISTIVITY
1.2
TWOPOINT VERSUS FOURPOINT PROBE
The fourpoint probe is commonly used to measure the semiconductor resistivity. It is an absolute measurement without recourse to calibrated standards and is sometimes used to provide standards for other resistivity measurements. Twopoint probe methods would appear to be easier to implement, because only two probes need to be manipulated. But the interpretation of the measured data is more difficult. Consider the twopoint probe or twocontact arrangement of Fig. 1.1(a). Each contact serves as a current and as a voltage probe. We wish to determine the resistance of the device under test (DUT). The total resistance RT is given by RT = V /I = 2RW + 2RC + RDUT
(1.2)
where RW is the wire or probe resistance, RC the contact resistance, and RDUT the resistance of the device under test. Clearly it is impossible to determine RDUT with this measurement arrangement. The remedy is the fourpoint probe or fourcontact arrangement in Fig. 1.1(b). The current path is identical to that in Fig. 1.1(a). However, the voltage is now measured with two additional contacts. Although the voltage path contains RW and RC as well, the current flowing through the voltage path is very low due to the high input impedance of the voltmeter (around 1012 ohms or higher). Hence, the voltage drops across RW and RC are negligibly small and can be neglected and the measured voltage is essentially the voltage drop across the DUT. By using four rather than two probes, we have eliminated parasitic voltage drops, even though the voltage probes contact the device on the same contact pads as the current probes. Such four contact measurements are frequently referred to as Kelvin measurements, after Lord Kelvin. An example of the effect of two versus four contacts is shown in Fig. 1.2. The drain current–gate voltage characteristics of a metaloxidesemiconductor fieldeffect transistor were measured with one contact on source and drain (no Kelvin), one contact on source and two contacts on drain (KelvinDrain), two contacts on source and one on drain (KelvinSource), and two contacts on source and drain (Full Kelvin). It is quite obvious that eliminating contact and probe resistances in the “Full Kelvin” has a significant effect on the measured current. The probe, contact, and spreading resistances of a twopoint probe arrangement on a semiconductor are illustrated in Fig. 1.3.
RW
RW
RC I
DUT
V RDUT
Fig. 1.1
RC I
DUT
V RDUT
RC
RW
RW
(a)
(b)
RC
Twoterminal and fourterminal resistance measurement arrangements.
TWOPOINT VERSUS FOURPOINT PROBE
3
25 Full Kelvin Drain Current (mA)
20 15
KelvinSource
10
KelvinDrain
5
No Kelvin
0 0
1
2
3
4
5
Gate Voltage (V)
Fig. 1.2 Effect of contact resistance on MOSFET drain current. Data courtesy of J. Wang, Arizona State University.
I
V
I
Rp Rc
Rsp Current Spreading
Fig. 1.3 Twopoint probe arrangement showing the probe resistance Rp , the contact resistance Rc , and the spreading resistance Rsp .
The fourpoint probe was originally proposed by Wenner1 in 1916 to measure the earth’s resistivity. The fourpoint probe measurement technique is referred to in Geophysics as Wenner’s method. Valdes adopted it for semiconductor wafer resistivity measurements in 1954.2 The probes are generally collinear, i.e., arranged inline with equal probe spacing, but other probe configurations are possible.3
Exercise 1.1 Problem: This exercise deals with data presentation. Frequently nonlinear behavior is encountered in presenting data of semiconductor materials or devices, where one parameter may be proportional to another parameter to some power, e.g., y = Kx b , where both the prefactor K and exponent b are constant. One parameter may vary exponentially with another parameter, e.g., I = Io exp(βV ). What is the best way to present the information to be able to extract “b” and “β”?
4
RESISTIVITY
Solution: Consider the relationship y = Kx b = 8x 5 . Plots of y versus x on a linear scale, shown in Fig. E1.1(a) and (b), do not allow “b” do be determined, regardless what scale is used because the curves are nonlinear. However, when the same data are plotted on a loglog plot as in (c), “b” is simply the slope of such a plot. In this case the slope is 5, because log(y) = log(Kx b ) = log(K) + log(x b ) = log(K) + b log(x) and the slope m is m=
d[log(y)] =b=5 d[log(x)]
If the data are plotted as in (d), which is also a loglog plot, the data must first be converted to “log” before the slope is taken. When that is done, the slope is again m = 5. Let us now consider the relationship y = yo exp(βx) = 10−14 exp(40x). Obviously, a linearlinear plot, shown in (e), allows neither yo nor β to be extracted. When, however, the data are plotted on a semilog plot, as in (f), we have ln(y) = ln(yo ) + βx ⇒ log(y) = log(yo ) + βx/ ln(10) 1 × 1016 8 × 1015
y
6 × 1015 4 × 1015 2 × 1015 0
0
200
400
600
800
60
80
1000
x (a)
1 × 1011 8 × 1010
y
6 × 1010 4 × 1010 2 × 1010 0
0
20
40 x (b)
Fig. E1.1
100
TWOPOINT VERSUS FOURPOINT PROBE
1016 1014 1012 1010 y
108 106 104 102 100 10−2 0.1
1
10 x (c)
100
1000
2
3
16 14 12 log( y)
10 8 6 4 2 0 −2 −1
0
1 log(x) (d)
1 0.8
y
0.6 0.4 0.2 0
0
0.2
0.4
0.6 x (e)
Fig. E1.1
(continued)
0.8
1
5
6
RESISTIVITY
100 10−2 10−4 y
10−6 10−8 10−10 10−12 10−14
0
0.2
0.4
0.6
0.8
1
x (f)
(continued)
Fig. E1.1
The slope m is m=
β β 14 d[log(y)] = = = dx ln(10) 2.3036 2.3036 × 0.8
and the intercept at x = 0 is yo = 10−14 . To derive the fourpoint probe resistivity expression, we start with the sample geometry in Fig. 1.4(a). The electric field E is related to the current density J , the resistivity ρ, and the voltage V through the relationship2 E = Jρ = −
I dV ; J = dr 2πr 2
(1.3)
The voltage at point P at a distance r from the probe, is then
V
0
dV = −
I
Iρ 2π
r
0
Iρ dr ⇒V = 2 r 2πr
I
(1.4)
1
I
2
3
4 I
I A = 2pr2 r
∞
∞ P
r1 ∞
s1
r2 ∞
∞
∞
(a)
(b)
s2
∞
s3 ∞
∞ (c)
Fig. 1.4 (a) onepoint probe, (b) twopoint, and (c) collinear fourpoint probe showing current flow and voltage measurement.
TWOPOINT VERSUS FOURPOINT PROBE
7
For the configuration in Fig. 1.4(b), the voltage is V =
Iρ Iρ Iρ − = 2πr1 2πr2 2π
1 1 − r1 r2
(1.5)
where r1 and r2 are the distances from probes 1 and 2, respectively. The minus sign accounts for current leaving through probe 2. For probe spacings s1 , s2 , and s3 , as in Fig. 1.4(c), the voltage at probe 2 is V2 =
Iρ 2π
1 1 − s1 s2 + s3
(1.6)
V3 =
Iρ 2π
1 1 − s1 + s2 s3
(1.7)
and at probe 3 it is
The total measured voltage V = V23 = V2 − V3 becomes Iρ V = 2π
1 1 1 1 − − + s1 s2 + s3 s1 + s2 s3
(1.8)
The resistivity ρ is given by ρ=
2π V (1/s1 − 1/(s1 + s2 ) − 1/(s1 + s2 ) + 1/s3 ) I
(1.9)
usually expressed in units of ohm · cm, with V measured in volts, I in amperes, and s in cm. The current is usually such that the resulting voltage is approximately 10 mV. For most fourpoint probes the probe spacings are equal. With s = s1 = s2 = s3 , Eq. (1.9) reduces to V (1.10) ρ = 2πs I Typical probe radii are 30 to 500 µm and probe spacings range from 0.5 to 1.5 mm. The spacings vary for different sample diameter and thickness.4 For s = 0.1588 cm, 2πs is unity, and ρ becomes simply ρ = V /I . Smaller probe spacings allow measurements closer to wafer edges, an important consideration during wafer mapping. Probes to measure metal films should not be mixed with probes to measure semiconductors. For some applications, e.g. magnetic tunnel junctions, polymer films, and semiconductor defects, microscopic fourpoint probes with probe spacings of 1.5 µm have been used.5 Semiconductor wafers are not semiinfinite in extent in either the lateral or the vertical dimension and Eq. (1.10) must be corrected for finite geometries. For an arbitrarily shaped sample the resistivity is given by
ρ = 2πsF
V I
(1.11)
where F corrects for probe location near sample edges, for sample thickness, sample diameter, probe placement, and sample temperature. It is usually a product of several
8
RESISTIVITY
independent correction factors. For samples thicker than the probe spacing, the simple, independent correction factors contained in F of Eq. (1.11) are no longer adequate due to interactions between thickness and edge effects. Fortunately the samples are generally thinner than the probe spacings, and the correction factors can be independently calculated.
1.2.1
Correction Factors
Fourpoint probe correction factors have been calculated by the method of images,2, 6 complex variable theory,7 the method of Corbino sources,8 Poisson’s equation,9 Green’s functions,10 and conformal mapping.11 – 12 We will give the most appropriate factors here and refer the reader to others where appropriate. The following correction factors are for collinear or inline probes with equal probe spacing, s. We write F as a product of three separate correction factors F = F1 F2 F3
(1.12)
Each of these factors can be further subdivided. F1 corrects for sample thickness, F2 for lateral sample dimensions, and F3 for placement of the probes relative to the sample edges. Other correction factors are discussed later in the chapter. Sample thickness must be corrected for most measurements since semiconductor wafers are not infinitely thick. A detailed derivation of thickness correction factors is given by Weller.13 Sample thicknesses are usually on the order of the probe spacing or less introducing the correction factor14 F11 =
t/s 2 ln{[sinh(t/s)]/[sinh(t/2s)]}
(1.13)
for a nonconducting bottom wafer surface boundary, where t is the wafer or layer thickness. If the sample consists of a semiconducting layer on a semiconductor substrate, it is important that the layer be electrically isolated from the substrate. The simplest way to do this is for the two regions to be of opposite conductivity, i.e., nlayer on a psubstrate or player on an nsubstrate. The spacecharge region is usually sufficiently insulating to confine the current to the layer. For a conducting bottom surface the correction factor becomes F12 =
t/s 2 ln{[cosh(t/s)]/[cosh(t/2s)]}
(1.14)
F11 and F12 are plotted in Fig. 1.5. Conducting bottom boundaries are difficult to achieve. Even a metal deposited on the wafer back surface does not ensure a conducting contact. There is always a contact resistance. Most fourpoint probe measurements are made with insulating bottom boundaries. For thin samples Eq. (1.13) reduces to F11 =
t/s 2 ln(2)
(1.15)
TWOPOINT VERSUS FOURPOINT PROBE
9
103 102 F12
F11, F12
101 100
10−1 F11
10−2 10−3 0.001
0.01
0.1 t/s
1
10
Fig. 1.5 Wafer thickness correction factors versus normalized wafer thickness; t is the wafer thickness, s the probe spacing. The data points are taken from ref. 15.
using the approximation sinh(x) ≈ x for x ≪ 1. Eq. (1.15) is valid for t ≤ s/2. For very thin samples that satisfy the conditions for F2 and F3 to be approximately unity, we find from Eqs. (1.11), (1.12), and (1.15) V π V t = 4.532t ln(2) I I
ρ=
(1.16)
Thin layers are often characterized by their sheet resistance Rsh expressed in units of ohms per square. The sheet resistance of uniformly doped samples is given by
Rsh =
π V V ρ = = 4.532 t ln(2) I I
(1.17)
subject to the constraint t ≤ s/2. The sheet resistance characterizes thin semiconductor sheets or layers, such as diffused or ionimplanted layers, epitaxial films, polycrystalline layers, and metallic conductors. The sheet resistance is a measure of the resistivity averaged over the sample thickness. The sheet resistance is the inverse of the sheet conductance Gsh . For uniformlydoped samples we find 1 1 (1.18) = Rsh = Gsh σt where σ is the conductivity and t the sample thickness. For non uniformlydoped samples Rsh =
0
1 t
[1/ρ(x)] dx
=
0
1 t
σ (x) dx
=
1 q
0
t
[n(x)µn (x) + p(x)µp (x)] dx
(1.19)
10
RESISTIVITY
Exercise 1.2 V+ s1 V−
s2 I
+
s3
s4 I−
Fig. E1.2
Problem: Is there another way to derive the sheet resistance expression? Solution: Consider a sample of thickness t and resistivity ρ. The four probes are arranged as in Fig. E1.2. Current I is injected at probe I + and spreads out cylindrically symmetric. By symmetry and current conservation, the current density at distance r from the probe is I J = 2πrt The electric field is E = Jρ =
Iρ dV =− 2πrt dr
Integrating this expression gives the voltage drop between probes V + and V − , located at distances s1 and s2 from I + as
Vs2
Vs1
Iρ dV = − 2πt
s2
s1
dr Iρ s2 ⇒ Vs1 − Vs2 = V12 = ln r 2πt s1
By the principle of superposition, the voltage drop due to current injected at I − is Iρ s3 ln V34 = − 2πt s4 leading to V = V12 − V34
Iρ s2 s3 ln = 2πt s1 s4
For a collinear arrangement with s1 = s4 = s and s2 = s3 = 2s ρ=
πt V π V ; Rsh = ln(2) I ln(2) I
Exercise 1.3 Problem: What does sheet resistance mean and why does it have such strange units?
TWOPOINT VERSUS FOURPOINT PROBE
11
r t
W
L
Fig. E1.3
Solution: To understand the concept of sheet resistance, consider the sample in Fig. E1.3. The resistance between the two ends is given by R=ρ
L ρ L L =ρ = ohms A Wt t W
Since L/W has no units, ρ/t should have units of ohms. But ρ/t is not the sample resistance. To distinguish between R and ρ/t, the ratio ρ/t is given the units of ohms/square and is named sheet resistance, Rsh . Hence the sample resistance can be written as R = Rsh
L ohms W
The sample is sometimes divided into squares, as in Fig. E1.4. The resistance is then given as R = Rsh (ohms/square) × Number of squares = 5Rsh ohms Looking at it this way, the “square” cancels. The sheet resistance of a semiconductor sample is commonly used to characterize ion implanted and diffused layers, metal films, etc. The depth variation of the dopant atoms need not be known, as is evident from Eq. (1.19). The sheet resistance can be thought of as the depth integral of the dopant atom density in the sample, regardless of its vertical spatial doping density variation. A few sheet resistances are plotted in Fig. E1.5 versus sample thickness as a function of sample resistivity. Also shown are typical values for Al, Cu and heavilydoped Si.
Exercise 1.4 Problem: For the carrier density profiles in Fig. E1.6, do the sheet resistances of the three layers differ?
5 squares
Rsh
Fig. E1.4
12
RESISTIVITY
Sheet Resistance (Ω/square)
102 ρ = 10−3 Ωcm 10
1
Si *
100
10−4 Ωcm
10−1
10−5 Ωcm * Al * Cu
10−2
10−6 Ωcm
10−3 10−5
10−4
10−3
Thickness (cm)
Fig. E1.5
Solution: Eq. (1.19) shows the sheet resistance to be inversely proportional to the conductivitythickness product. For constant mobility, Rsh is inversely proportional to the area under the curves in Fig. E1.6. Since the three areas are equal, this implies that Rsh is the same for all three cases. In other words, it does not matter what the carrier distribution is, only the integrated distribution matters for Rsh .
Fourpoint probe measurements are subject to further sample size correction factors. For circular wafers of diameter D, the correction factor F2 in Eq. (1.12) is given by16 F2 =
ln(2) ln(2) + ln{[(D/s)2 + 3]/[(D/s)2 − 3]}
(1.20)
F2 is plotted in Fig. 1.6 for circular wafers. The sample must have a diameter D ≥ 40 s for F2 to be unity. For a probe spacing of 0.1588 cm, this implies that the wafer must be at least 6.5 cm in diameter. Also shown in Fig. 1.6 is the correction factor for rectangular samples.6 The correction factor 4.532 in Eq. (1.17) is for collinear probes with the current flowing into probe 1, out of probe 4, and with the voltage sensed across probes 2 and 3. For the current applied to and the voltage sensed across other probes, different correction factors obtain.17 For probes perpendicular to and a distance d from a nonconducting boundary, the correction factors, for infinitely thick samples, are shown in Fig. 1.7.2 It is obvious from the figures that as long as the probe distance from the wafer boundary is at least n(x) 0 (c)
n Type xj (a)
p Type x
Fig. E1.6
(b)
TWOPOINT VERSUS FOURPOINT PROBE
13
1 0.8
F2
0.6 Rectangular 0.4 Circular 0.2 0
0
10
20
30
40
D/s Fig. 1.6 Wafer diameter correction factors versus normalized wafer diameter. For circular wafers: D = wafer diameter; for rectangular samples: D = sample width, s = probe spacing.
2
F31, F32, F33, F34
F34
F32,34:
F31,33:
1.5
d
d
F33
1 F32 F31 0.5
0
1
2
3
4
5
d/s
Fig. 1.7 Boundary proximity correction factors versus normalized distance d (s = probe spacing) from the boundary. F31 and F32 are for nonconducting boundaries, F33 and F34 are for conducting boundaries.
three to four probe spacings, the correction factors F31 to F34 reduce to unity. For most fourpoint probe measurements this condition is easily satisfied. Correction factors F31 to F34 only become important for small samples in which the probe is, of necessity, close to the sample boundary. Other corrections must be applied when the probe is not centered even in a wafer of substantial diameter.16 For rectangular samples it has been found that the sensitivity of the geometrical correction factor to positional error is minimized by orienting the probe with its electrodes within about 10% of the center.11 For square arrays the error is minimized by orienting the probe array with its electrodes equidistant from the midpoints of the sides. There is also an angular dependence of the placement of a square array on the rectangular
14
RESISTIVITY
sample.9, 11 We should mention that if the probe spacings are not exactly identical, there is a further small correction.18 The key to high precision fourpoint probe measurements, including reduced geometric effects associated with proximity of the probe to a nonconducting boundary, is the use of two measurement configurations at each probe location.19 – 21 This technique is known as the “dual configuration” or as the “configuration switched” method. The first configuration is usually with current into probe 1 and out of probe 4 and with the voltage sensed across probes 2 and 3. The second measurement is made with current driven through probes 1 and 3 and voltage measured across probes 2 and 4. The advantages are: (i) the probe no longer needs to be in a high symmetry orientation (being perpendicular or parallel to the wafer radius of a circular wafer or to the length or width of a rectangular sample), (ii) the lateral dimensions of the specimen do not have to be known since the geometric correction factor results directly from the two measurements, and (iii) the two measurements selfcorrect for the actual probe spacings. The sheet resistance in the dual configuration is given by21 Rsh = −14.696 + 25.173(Ra /Rb ) − 7.872(Ra /Rb )2 where Ra =
Vf 23 /If 14 + Vr23 /Ir14 Vf 24 /If 13 + Vr24 /Ir13 ; Rb = 2 2
(1.21)
(1.22)
Vf 23 /If 14 is the voltage/current across terminals 2,3 and 1,4 with the current in the forward direction and Vr23 /Ir14 with the current in the reverse direction. The resistivity of semiconductor ingots, measured with the fourpoint probe, is given by ρ = 2πs
V I
(1.23)
only if the ingot diameter D satisfies the relationship D ≥ 10 s.10, 22, 23 1.2.2
Resistivity of Arbitrarily Shaped Samples
The collinear probe configuration is the most common fourpoint probe arrangement. Arrangement of the points in a square has the advantage of occupying a smaller area since the spacing between points is only s or 21/2 s, whereas in a collinear configuration the spacing between the outer two probes is 3s. The square arrangement is more commonly used, not as an array of four mechanical probes, but rather as contacts to square semiconductor samples. The theoretical foundation of measurements on irregularly shaped samples is based on conformal mapping developed by van der Pauw.24, 26 He showed how the specific resistivity of a flat sample of arbitrary shape can be measured without knowing the current pattern, if the following conditions are met: (1) the contacts are at the circumference of the sample, (2) the contacts are sufficiently small, (3) the sample is uniformly thick, and (4) the surface of the sample is singly connected, i.e., the sample does not contain any isolated holes. Consider the flat sample of a conducting material of arbitrary shape, with contacts 1, 2, 3, and 4 along the periphery as shown in Fig. 1.8 to satisfy the conditions above. The resistance R12,34 is defined as V34 R12,34 = (1.24) I12
TWOPOINT VERSUS FOURPOINT PROBE
1
15
4
3 2
Fig. 1.8
Arbitrarily shaped sample with four contacts.
where the current I12 enters the sample through contact 1 and leaves through contact 2 and V34 = V3 − V4 is the voltage difference between the contacts 3 and 4. R23,41 is defined similarly. The resistivity is given by24 ρ=
π (R12,34 + R23,41 ) t F ln(2) 2
(1.25)
where F is a function only of the ratio Rr = R12,34 /R23,41 , satisfying the relation F Rr − 1 exp[ln(2)/F ] = ar cosh Rr + 1 ln(2) 2
(1.26)
The dependence of F on Rr is shown in Fig. 1.9. For a symmetrical sample such as the circle or the square in Fig. 1.10, Rr = 1 and F = 1. This allows Eq. (1.25) to be simplified to ρ=
π tR12,34 = 4.532tR12,34 ln(2)
(1.27)
1
F
0.8
0.6
0.4
0.2
1
10
100
1000
Rr
Fig. 1.9
The van der Pauw correction factor F versus Rr .
16
RESISTIVITY
(a)
Fig. 1.10
(b)
(c)
Typical symmetrical circular and square sample geometries.
The sheet resistance becomes Rsh =
πR12,34 = 4.532R12,34 ln(2)
(1.28)
similar to the fourpoint probe expression in Eq. (1.17). The van der Pauw equations are based on the assumption of negligibly small contacts located on the sample periphery. Real contacts have finite dimensions and may not be exactly on the periphery of the sample. The influence of nonideal peripheral contacts is shown in Fig. 1.11. The correction factor C is plotted as a function of the ratio of contact size to sample side length d/ l. C is defined as ρ = CtR12,34 ; Rsh = CR12,34
(1.29)
Figure 1.11 shows that corner contacts introduce less error than contacts placed in the center of the sample sides. However, if the contact length is less than about 10% of the side length, the correction is negligible for either contact placement. The error introduced by nonideal contacts can be eliminated by the cloverleaf configuration of Fig. 1.10(b). Such configurations make sample preparation more complicated and are undesirable, so square samples are generally used. One of the advantages of the van der Pauw structure is the small sample size compared with the area required for fourpoint probe measurements. For simple processing it is preferable to use the circular or 7 (a) 6
(b)
(a)
C
d l
5
(b)
p/ln2 4
0
0.2
0.4
0.6
0.8
1
d/l
Fig. 1.11 Correction factor C versus d/ l for contacts at the center and at the corners of the square. Data after ref. 25.
17
TWOPOINT VERSUS FOURPOINT PROBE
square sample geometries shown in Fig. 1.10. For such structures it is not always possible to align the contacts exactly. Geometries other than those in Fig. 1.10 are also used. One of these is the Greek cross in Fig. 1.12. Using photolithographic techniques, it is possible to make such structures very small and place many of them on a wafer for uniformity characterization. The sheet resistance of the shaded area is determined in such measurements. For structures with L = W , the contacts should be placed so that d ≤ L/6 from the edge of the cross, where d is the distance of the contact from the edge.27 Surface leakage can introduce errors if L is too large.28 A variety of cross sheet resistor structures have been investigated and their performance compares well with conventional bridgetype structures.29 The measured voltages in cross and van der Pauw structures are lower than those in conventional bridge structures. The cross and the bridge structures are combined in the crossbridge structure in Fig. 1.13, allowing the sheet resistance and the line width to be determined. The sheet resistance, determined in the shaded cross area, is Rsh =
π V34 ln(2) I12
(1.30)
where V34 = V3 − V4 and I12 is the current flowing into contact I1 and out of contact I2 . The left part of Fig. 1.13 is a bridge resistor to determine the line width W . We mention the line width measurement feature only briefly here. Line width measurements are more fully discussed in Chapter 10. The voltage along the bridge resistor is V45 =
Rsh LI26 W
(1.31)
Contact L
L
Diffusion Implant PolySi
W
W d
Fig. 1.12
A Greek cross sheet resistance test structure. d = distance of contact from edge.
1 L 2
6
W Fig. 1.13
5
4
3
A cross bridge sheet resistance and line width test structure.
18
RESISTIVITY
where V45 = V4 − V5 and I26 is the current flowing from contact 2 to contact 6. From Eq. (1.31) the line width is W =
Rsh LI26 V45
(1.32)
with Rsh determined from the cross structure and Eq. (1.30). A key assumption in this measurement is that the sheet resistance be identical for the entire test structure. Since the bridge structure in Fig. 1.13 is suitable for resistance measurements, it can be used to characterize “dishing” during chemicalmechanical polishing of semiconductor wafers, where soft metal lines tend polish thinner in the central portion than at the edges leading to nonuniform thickness. This is particularly important for soft metals such as copper. With the resistance inversely proportional to metal thickness, resistance measurements can be used to determine the amount of dishing.30 1.2.3
Measurement Circuits
Fourpoint probe measurement circuits are given in various ASTM Standards. For example, ASTM F8418 and F7631 give detailed circuit diagrams. Today’s equipment is supplied with computers to provide the current stimulus, measure the voltage and apply appropriate correction factors as well as provide the signals for the probe station stepping for wafer mapping. 1.2.4
Measurement Errors and Precautions
For fourpoint probe measurements to be successful a number of precautions must be taken and appropriate correction factors must be applied to the measured data. Sample Size: As mentioned earlier, a number of corrections must be applied, depending on the location of the probe as well as sample thickness and size. For those cases where the wafer is uniformly doped in the lateral direction and its diameter is appreciably larger than the probe spacing, the wafer thickness is the chief correction. If the wafer or the layer to be measured is appreciably thinner than the probe spacing, the calculated resistivity varies directly with thickness. It is therefore very important to determine the thickness accurately for resistivity determination. For sheet resistance measurements the thickness need not be known. Minority/Majority Carrier Injection: It is often stated that metalsemiconductor contacts do not inject minority carriers. That is not strictly true. Metalsemiconductor contacts do inject minority carriers, but their injection efficiency is low. However, under high current conditions it may not be negligible. Minority carrier injection causes conductivity modulation because increased minority carrier density leads to increased majority carrier density (to maintain charge neutrality) and subsequent enhanced conductivity. To reduce minority carrier injection, the surface should have a high recombination rate for minority carriers. This is best achieved by using lapped surfaces. For a highly polished wafer it may not be possible to achieve the necessary high surface recombination. Injected minority carriers will have decayed by recombination and cause very little error for voltage probes 3–4 minority carrier diffusion lengths from the injecting current probe. However, for high lifetime material the diffusion length may be longer than the probe spacing, and the measured resistivity will be in error. Another possible source of error is the probe pressureinduced band gap narrowing leading to enhanced minority carrier injection.
19
TWOPOINT VERSUS FOURPOINT PROBE
Minority carrier injection may be important for high resistivity materials. For silicon this applies for ρ ≥ 100 ohm · cm. An error of less than 2% is introduced by minority carrier injection if the voltage across the two voltagesensing probes is held to less than 100 mV for 1 mm probe spacings for samples with lapped surfaces. If the current density exceeds the value J = qnv, where n ≈ ND for ntype samples and v is the thermal velocity, excess majority carriers can be injected into the sample, causing the resistivity to change. Majority carrier injection is usually of little concern if the fourpoint probe voltage does not exceed 10 mV. Probe Spacing: A mechanical fourpoint probe exhibits small random probe spacing variations. Such variations give erroneous values of resistivity or sheet resistance, especially when evaluating uniformly doped wafers. In such cases it is very important to know whether any nonuniformities are due to the wafer, due to process variations, or due to measurement errors. An example is the evaluation of ionimplanted layers. It is known that ionimplanted layers can have sheet resistance uniformities better than 1%. For small probe spacing variations the correction factor18 FS ≈ 1 + 1.082(1 − s2 /sm )
(1.33)
must be applied, where s2 is the spacing between the inner two probes and sm is the mean value of the probe spacings. Errors due to probe wander can be reduced by averaging several independent readings. Current: Additional sources of error are the current amplitude and surface leakage current. The current can affect the measured resistivity in two ways: by an apparent resistivity increase produced by wafer heating and by an apparent resistivity decrease due to minority and/or majority carrier injection. The suggested fourpoint probe measurement current for silicon wafers is shown in Fig. 1.14 as a function of resistivity and sheet resistance.18 The data were obtained by measuring the fourpoint probe resistivity as a function of current for a given sample. Such resistivitycurrent curves show typically a flat region bounded by nonlinearities at both low and high currents. The flat region gives the appropriate current. Surface leakage is reduced or eliminated by enclosing the probe in a shielded enclosure held at a potential equal to the inner probe potential.
Resistivity (Ωcm) Sheet Resistance (Ω/square)
104 103
101 r
100 10−1 10−2 10−2
Fig. 1.14
Rsh
102
10−1
100 101 Current (mA)
102
103
Recommended fourpoint probe current versus Si sheet resistance and resistivity.
20
RESISTIVITY
Temperature: It is important that the sample temperature be uniform in order not to introduce thermoelectric voltages. Temperature gradients can be caused by ambient effects but are more likely due to sample heating by the probe current. Current heating is most likely to occur in low resistivity samples where high currents are required to obtain readily measurable voltages. Even if temperature variations are not caused by the measurement apparatus and there are no temperature gradients, there may still be temperature variations due to temperature fluctuations in the measurement room. Since semiconductors have relatively large temperature coefficients of resistivity, errors are easily introduced by failing to compensate for such temperature variations (n and pSi18 and for n and pGe).32 For resistivities of 10 ohm · cm or higher, the Si coefficient is on the order of 1%/◦ C. Temperature corrections are made by using the correction factor18 FT = 1 − CT (T − 23)
(1.34)
where CT is the temperature coefficient of resistivity and T is the temperature in ◦ C. Surface Preparation: Proper surface preparation is important for high sheet resistance Si measurements. For example, positive charge on the surface of a ptype layer on an ntype wafer, leads to a surface chargeinduced spacecharge region leaving only a portion of the layer in its neutral state. This, of course, increases the thicknessdependent sheet resistance. Similarly, a positive surface charge on an ntype implanted layer, leads to surface accumulation and a sheet resistance reduction. An example of this effect is shown in Fig. 1.15. Wafers dipped into boiling water or into H2 SO4 or H2 O2 exhibit stabilized surfaces while those etched in HF exhibit a timedependent sheet resistance.33 High Resistivity, High Sheet Resistance Materials: Materials of very high resistivity are more difficult to measure by fourpoint probe or van der Pauw methods. Moderately doped wafers can become highly resistive at low temperatures and are similarly difficult
B Unpassivated B Passivated As Passivated As Unpassivated
Sheet Resistance (Ω/square)
7 × 104 6 × 104 5 × 104 4 × 104 3 × 104 2 × 104 1 × 104 0 × 100 1 10
102
103
104
Time in Air (min)
Fig. 1.15 Sheet resistance versus time in room temperature air. B implant: 8 × 1011 cm−2 , 70 keV through 59 nm oxide into nSi substrate, annealed 1050◦ C, 15 s; As implant: 8 × 1011 cm−2 into bare pSi substrate, annealed 1000◦ C, 30 min. Both passivated in boiling water for 10 min. After ref. 33.
WAFER MAPPING
21
to measure. Special measurement precautions must be observed. Thin semiconductor films usually have high sheet resistance. These include lightly doped layers, polycrystalline Si films, amorphous Si films, silicononinsulator, etc. It is possible to make fourpoint probe measurements with sheet resistances up to about 1010 –1011 ohms/square, provided one uses a stable low current as low as picoamperes. A further consideration is penetration of the probes through shallow implanted layers. One solution to this problem is to use mercury fourpoint probes instead of metal “needles”. A measurement for highresistivity bulk wafers relies on providing the wafer with a large contact on one side and a small contact on the other side. A current is passed through the contacts and the voltage is measured. This arrangement, by itself, can suffer from surface leakage currents. By surrounding the small contact with a guard ring and holding the guard ring at the same or nearly the same potential as the small contact, surface currents are essentially suppressed.34 It is of course necessary to ensure that the contacts are ohmic or as close to ohmic as possible so that the bulk resistivity and not the contact resistance is measured. Twoterminal measurements are notorious for being complicated by contact effects and the true sample resistivity is not easy to determine as indicated by Eq. (1.2). Conventional van der Pauw measurements suitable for moderate or low resistivity materials are suspect for high resistance samples unless care is taken to eliminate current leakage paths and sample loading by the voltmeter. One approach around this problem is the “guarded” approach using high input impedance, unity gain amplifiers between each probe on the sample, and the external circuitry.35 The unity gain amplifiers drive the shields on the leads between the amplifier and the sample, thereby effectively eliminating the stray capacitance in the leads. This reduces leakage currents and the system time constant. Measurements of resistances up to 1012 ohms have been made with such a system. The “guarded” approach can also be automated.36 1.3
WAFER MAPPING
Wafer mapping, originally developed to characterize ion implantation uniformity, has become a powerful process monitoring tool. Manual wafer mapping originated in the 1970s.37 Today, highly automated systems are used. During wafer mapping the sheet resistance or some other parameter proportional to ion implant dose is measured at many locations across a sample. The data are then converted to twodimensional or threedimensional contour maps. Contour maps are a more powerful display of process uniformity than displaying the same data in tabular form. A welldesigned contour map gives instant information about ion implant uniformity, flow patterns during diffusion, epitaxial reactor nonuniformities, etc. If desired, line scans along one line across the sample can also be displayed to show the uniformity along that line. The most common sheet resistance wafer mapping techniques are: fourpoint probe sheet resistance, modulated photoreflectance, and optical densitometry.38 Of these, the configurationswitched fourpoint probe method is commonly used. It allows for rapid comparison between samples and has been used for ion implantation, diffusion, polySi films, and metal uniformity characterization.39 Example wafer maps are shown in Fig. 1.16. 1.3.1
Double Implant
Precaution needs to be taken to measure the sheet resistance of lowdose, single implanted layers by the fourpoint probe technique, because (1) it is difficult to make good electrical
22
RESISTIVITY
+
+
+
+
+
− − −
+
−
+
−
−
+
−
−
−
−
−
− +
+ +
−
+ +
+
+
+
+ +
−
−
+ −
+
+
+
+
+
+
+ +
+
+
−
+
−
+ +
+
+
+
−
+
+
+
−
−
+
+
−
−
+
+
+
−
−
−
+
+
− −
−
+
− −
+
+
−
−
−
−
+ +
+ +
−
−
+
+
− −
− −
−
Fig. 1.16 Fourpoint probe contour maps; (a) boron, 1015 cm−2 , 40 keV, Rsh (average) = 98.5 ohms/square; (a) arsenic, 1015 cm−2 , 80 keV, Rsh (average) = 98.7 ohms/square; 1% intervals. 200 mm diameter Si wafers. Data courtesy of Marylou Meloni, Varian Ion Implant Systems.
contact from the probe to the semiconductor, (2) low doses give low carrier densities and low conductivity, and (3) the surface leakage current can be comparable to the measurement current. The conventional fourpoint probe method can be used provided the starting wafers are of high resistivity, and they are oxidized before the implant to stabilize the surface resistance and to prevent ion channeling. The wafer is implanted and annealed, the oxide is stripped, and the surface is stabilized in a hot sulfuric acid and hydrogen peroxide solution (piranha etch). A modified fourpoint probe method, the double implant technique, is sometimes used for sheet resistance measurements of such layers.20, 40 It is implemented as follows: A ptype (ntype) impurity is implanted into an ntype (ptype) substrate at a dose 1 and energy E1 . For example, boron is implanted at a dose of 1 = 1014 cm−2 and energy E1 = 120 keV. The wafer is annealed to activate the implanted ions electrically. The sheet resistance Rsh1 is measured and the data are stored. Next the desired lowdose impurity is implanted at dose 2 and energy E2 , with 2 < 1 . E2 should be less than E1 to prevent penetration through the first implant layer. The first implant energy is typically at least 10–20% higher, and the first implant dose is at least two orders of magnitude higher than the second implant. The second implant conditions might be 2 = 1011 cm−2 and E2 = 100 keV. The sheet resistance Rsh2 after the second implant is measured and compared to Rsh1 without annealing the second implant. The second sheet resistance measurement relies on the implant damage of the second implant being proportional to the implant dose. This is true for low implant doses. Implanted, but not activated ions, do not contribute to electrical conduction. Furthermore, due to implant damage, the mobility is reduced making Rsh2 > Rsh1 . The impurity atomic mass of the first implant should be approximately the same mass as the second implant. It has also been found that (111)oriented Si wafers are preferred over (100)oriented wafers to reduce channeling effects. The doubleimplant method allows measurements immediately after the second implant. Implant doses as low as 1010 cm−2 can be measured by this technique. Test wafers can be annealed and reused, provided the anneal temperature is kept sufficiently low to prevent impurity redistribution. The method is also applicable for electrically inactive species, such as oxygen, argon, or nitrogen implants. A more detailed discussion is given in Smith et al.40
WAFER MAPPING
23
The doubleimplant technique suffers from several problems. Any sheet resistance nonuniformities resulting from the first implant and its activation cycle alter the lowdose measurement. Additionally, since this method derives its lowdose sensitivity from ionimplant damage, it is sensitive to postimplant relaxation, where implant damage anneals itself over a period of hours to days following the implant. If the measurement is made immediately after the second implant, damage relaxation has little effect. However, if the measurement is made several hours or days after the implant, damage relaxation can reduce the measured resistance by 10–20% for the types of implant doses and energies typical for lowdose implants. The measurement stability is improved by a 200◦ C, dry N2 anneal for 45 min before making the measurement.40 1.3.2
Modulated Photoreflectance
Modulated photoreflectance is the modulation of the optical reflectance of a sample in response to waves generated when a semiconductor sample is subjected to periodic heat stimuli. In the modulated photoreflectance or thermal wave method an Ar+ ion laser beam, incident on the semiconductor sample, is modulated at a frequency of 0.1 to 10 MHz, creating transient thermal waves near the surface that propagate at different speeds in damaged and crystalline regions. Hence, signals from regions with various damages differ, leading to a measure of crystal damage. The thermal wave diffusion length at a 1 MHz modulation frequency is 2 to 3 µm.41 The small temperature variations cause small volume changes of the wafer near the surface and the surface expands slightly.42 These changes include both thermoelastic and optical effects,43 and they are detected with a second laser—the probe beam—by measuring the reflectivity change. The apparatus is illustrated in Fig. 1.17. Both pump and probe laser beams are focused to approximately 1 µm diameter spots, allowing measurements not only on uniformly implanted wafers but also on patterned wafers. Modulated photoreflectance is commonly used to determine the implant dose of ion implanted wafers. Conversion from thermal wave signal to implant dose requires calibrated standards with known implant doses. The ability to determine ionimplant doses by thermal waves depends on the conversion of the single crystal substrate to a partially Therma Wave Signal
Detector Pump Laser
Probe Laser
Damaged Layer
Fig. 1.17
Sample
Schematic diagram of the modulated photoreflectance apparatus.
24
RESISTIVITY
disordered layer by the implant process. The thermal waveinduced thermoelastic and optical effects are changed in proportion to the number of implanted ions. Modulated photoreflectance implant monitoring is subject to postimplant damage relaxation. However, the laser detection scheme accelerates the damage relaxation process, and the sample stabilizes within a few minutes. The technique is contactless and nondestructive and has been used to measure implant doses from 1011 to 1015 cm−2 .44 Measurements can be made on bare and on oxidized wafers. The ability to characterize oxidized samples has the advantage of allowing measurements of implants through an oxide. The technique can discriminate between implant species since the lattice damage increases with implant atom size and the thermal wave signal depends on the lattice damage. It has been used for ion implantation monitoring, wafer polish damage, and reactive and plasma etch damage studies. Its chief strength lies in the ability to detect lowdose implants contactless and to display the information as contour maps. Example contour maps are shown in Fig. 1.18. 1.3.3
Carrier Illumination (CI)
Somewhat similar to modulated photoreflectance is carrier illumination, to determine junction depth. Optical characterization of activated shallow junctions requires high contrast between the active implant and the underlying layer. The index of refraction of the doped layer is slightly higher than the underlying silicon by virtue of its higher conductivity. However, this is insufficient to enable measurement using conventional methods. In carrier illumination, a focused laser (λ = 830 nm) injects excess carriers into the semiconductor, forming a dc excess carrier distribution and a λ = 980 nm probe beam measures the reflectance.45 The carrier distribution is deduced from the reflected signal. The carrier density in the substrate is flat, and falls rapidly at the junction edge. This creates a steep gradient in the index of refraction at the edge of the doping profile. The index of refraction change n relates to the excess carrier density N as n =
q 2 N 2Ks εo m∗ ω2
(1.35)
Fig. 1.18 Modulated photoreflectance contour maps; (a) boron, 6.5 × 1012 cm−2 , 70 keV, 648 TW units; (a) boron, 5 × 1012 cm−2 , 30 keV, 600 TW units; 0.5% intervals. 200 mm diameter Si wafers. Data courtesy of Marylou Meloni, Varian Ion Implant Systems.
RESISTIVITY PROFILING
25
where ω is the radial frequency of the light. Light is reflected from this distribution and interference with a reference leads to an interference signal correlating directly to the junction depth. By slowly modulating the laser generating the excess carriers, thereby maintaining the static distribution conditions, it is possible to use sensitive phaselocked methods to obtain a reflection signal with several orders of magnitude gain over a dc measurement. The method works best for layers with active doping densities in excess of 1019 cm−3 to avoid highlevel injection conditions in the active implanted region. High depth resolution is achieved because of the high index of refraction of the semiconductor. The measurement wavelength in silicon is about 270 nm, and a full 2π phase shift occurs in 135 nm. With a noiselimited phase resolution better than 0.5◦ , the depth resolution is about 0.2 nm. In addition to junction depth measurements, CI has been shown to be sensitive to the active dopant density and the profile abruptness and can also measure the thickness of the amorphous depth after a preamorphizing implant, making the CI method very sensitive for monitoring asimplanted lowdose ion implants.46 1.3.4
Optical Densitometry
In optical densitometry the doping density is determined by a technique entirely different from any of the methods discussed in this chapter. The method was developed for ion implantation uniformity and dose monitoring and does not use semiconductor wafers. A transparent substrate, typically glass, is coated with a thin film consisting of a polymer carrier and an implant sensitive radiochromic dye. During implant, the dye molecule undergoes heterolytic cleavage, resulting in positive ions with a peak light absorption at a wavelength of 600 nm.47 When this polymercoated glass wafer is ion implanted, the film darkens. The amount of darkening depends on the implant energy, dose, and species. The optical densitometer, using a sensitive microdensitometer, detects the transparency of the entire wafer before and after implant and compares the finaltoinitial difference in optical transparency with internal calibration tables. The optical transparency is measured over the entire implanted wafer and then displayed as a contour map. Calibration curves of optical density as a function of implant dose have been developed for implant doses from 1011 to 1013 cm−2 . The method requires no implantation activation anneal and the results can be displayed within a few minutes of the implantation. The optical density is measured with about 1 mm resolution and lends itself well to ion doses as low 1011 cm−2 . As discussed earlier in this chapter, the doping density of lowdose implants is not easy to measure electrically, and this optical method is a viable alternate technique. It is also very stable. Table 1.1 compares three mapping techniques.38
1.4
RESISTIVITY PROFILING
A fourpoint probe measures the sheet resistance. The resistivity is obtained by multiplying by the sample thickness with the correct resistivity obtained only for uniformlydoped substrates. For nonuniformly doped samples, the sheet resistance measurement averages the resistivity over the sample thickness according to Eq. (1.19). The resistivity profile of a nonuniformly doped layer cannot be determined from a single sheet resistance measurement. Furthermore it is usually the dopant density profile that is desired, not the resistivity profile.
26
RESISTIVITY
TABLE 1.1
Mapping Techniques for Ion Implantation Uniformity Measurements. FourPoint Probe
Double Implant
Spreading Resistance
Modulated Photoreflectance
Optical Densitometry
Resolution (µm) Species
Electrical Sheet Resistance 3000 Active
Electrical Spreading Resistance 5 Active
Optical Crystal Damage 1 Inactive
Optical Polymer Damage 3000 Inactive
Dose Range (cm−2 ) Results Relaxation Requires
1012 −1015 Direct Minor Anneal
Electrical Crystal Damage 3000 Active, Inactive 1011 −1014 Calibration Serious Initial Implant
1011 −1015 Calibration Minor Anneal
1011 −1015 Calibration Serious
1011 −1013 Calibration Serious Measure before and after
Type Measurement
Suitable techniques for determining dopant density profiles include the differential Hall effect, spreading resistance, capacitancevoltage, MOSFET threshold voltage, and secondary ion mass spectrometry. We will discuss the first two methods in this chapter and defer discussion of the others to Chapter 2. 1.4.1
Differential Hall Effect (DHE)
To determine a resistivity or dopant density depth profile, depth information must be provided. It is possible to measure the resistivity profile of a nonuniformly doped sample by measuring the resistivity, removing a thin layer of the sample, measuring the resistivity, removing, measuring, etc. The differential Hall effect is such a measurement procedure. The sheet resistance of a layer of thickness (t − x) is given by Rsh =
1 q
x
t
[n(x)µn (x) + p(x)µp (x)] dx
(1.36)
where x is the coordinate from the surface into the sample as illustrated in Fig. 1.19. If the sample is a thin layer, it must be separated from the substrate by an insulating layer to confine the fourpoint probe current to the layer. For example, an ntype implant into a psubstrate is suitable, with the spacecharge region of the resulting np junction acting as an “insulating” boundary. An ntype implant into an nsubstrate is not suitable as the measuring current is no longer confined to the nlayer. 0 Layer to be measured t x
Fig. 1.19
Insulator or opposite conductivity
Insulating boundary
Sample geometry with measurement proceeding from the surface into the sample.
27
RESISTIVITY PROFILING
The sheet resistance of a uniformly doped layer with constant carrier densities and mobilities is 1 (1.37) Rsh = q(nµn + pµp )t The sheet resistance is a meaningful descriptor not only for uniformly doped layers but also for nonuniformly doped layers, where both carrier densities and mobilities are depth dependent. In Eq. (1.36) Rsh represents an averaged value over the sample thickness (t − x). Obviously, for x = 0, the sheet resistance is given by Eq. (1.19). The sheet resistance is measured by the Hall effect or with a fourpoint probe as a function of depth by incremental layer removal. A plot of 1/Rsh (x) versus x leads to the sample conductivity σ (x) according to the equation48 d[1/Rsh (x)] = −q[n(x)µn (x) + p(x)µp (x)] = −σ (x) dx Equation (1.38) is derived from (1.36) using Leibniz’s theorem b(c) b(c) ∂b ∂a ∂ d f (x, c) dx = [f (x, c)] dx + f (b, c) − f (a, c) dc a(c) ∂c ∂c ∂c a(c)
(1.38)
(1.39)
The resistivity is determined from Eq. (1.38) and from the identity ρ(x) = 1/σ (x) as ρ(x) = −
2 Rsh (x) 1 Rsh (x) = = d[1/Rsh (x)]/dx dRsh (x)/dx d[ln(Rsh (x))]/dx
(1.40)
The dopant density determined by this method is illustrated in Exercise 1.5. Dopant density profiles determined by DHE, spreading resistance profiling, and secondary ion mass spectrometry are shown in Fig. 1.20.
Exercise 1.5 Problem: Given the sheet resistance versus depth plot of an nSi layer on a pSi substrate in Fig. E1.7(a), determine the resistivity and the doping density as a function of depth.
Density (cm−3)
1022 SIMS SRP DHE
1020
1018 xj
1016
1014
0
0.05
0.1
0.15
Depth (µm)
Fig. 1.20 Dopant density profiles determined by DHE, spreading resistance profiling, and secondary ion mass spectrometry. Data after ref. 49. Reprinted from the Jan. 1993 edition of Solid State Technology.
RESISTIVITY
Rsh (Ω/square)
107
106
105
104 0 × 100 2 × 10−5 4 × 10−5 6 × 10−5 8 × 10−5 1 × 10−4 x (cm) (a)
1/Rsh (Ω/square)−1
10−4
10−5
10−6
10−7 0 × 100 2 × 10−5 4 × 10−5 6 × 10−5 8 × 10−5 1 × 10−4
10
1017
1
1016
1015 0.1 −5 0 −5 −5 −5 0 × 10 2 × 10 4 × 10 6 × 10 8 × 10 1 × 10−4 Depth (µm) (c) Fig. E1.7
ND (cm−3)
x (cm) (b)
r (Ωcm)
28
RESISTIVITY PROFILING
29
Solution: Determine the slope of this plot as a function of x. Then determine ρ(x) versus x using Eq. (1.40). Remember, in problems where the data are given in terms of “log” as in the figure above, you need to use the conversion “ln(10) ln(x) = log(x)”. The resistivity and doping density data so derived are shown in Figs. E1.7(b) and (c). Conversion of “ρ to ND ” used a mobility of 800 cm2 /V · s. A word of caution regarding sheet resistance measurements of thin layers is in order here. Surface charges can induce spacecharge regions at the sample surface. If that happens, then the neutral layer that governs the sheet resistance is thinner than the physical layer, introducing an error into the measurement. It is generally not a problem for Si, but can be a problem for GaAs, where surface chargeinduced spacecharge regions are very common. Corrections need to be applied then.50 – 51 Repeated removal of wellcontrolled thin layers from a heavilydoped semiconductor is difficult to do by chemical etching. It can, however, be done with anodic oxidation. During anodic oxidation a semiconductor is immersed in a suitable electrolyte in an anodization cell. A current is passed from an electrode to the semiconductor sample through the electrolyte, causing an oxide to grow at room temperature. The oxide grows by consuming a portion of the semiconductor. By subsequently etching the oxide, that portion of the semiconductor consumed during the oxidation is removed as well. This can be done very reproducibly. Two anodization methods are possible. In the constant voltage method, the anodization current is allowed to fall from an initial to a final predetermined value. In the constant current method, the voltage is allowed to rise until a preset value is attained. The oxide thickness is directly proportional to the net forming voltage in the constant current anodization method, where the net forming voltage is the final cell voltage minus the initial cell voltage. A variety of anodization solutions have been used. The nonaqueous solutions Nmethylacetamide, tetrahydrofurfuryl alcohol and ethylene glycol are suitable for silicon.52 Ethylene glycol containing 0.04N KNO3 and 1–5% water produces uniform, reproducible ˚ of Si oxides at current densities of 2 to 10 mA/cm2 . For the ethylene glycol mixture 2.2 A ˚ of Si. Ge53 , InSb54 , are removed per volt.52 A forming voltage of 100 V removes 220 A and GaAs55 have all been anodically oxidized. The laborious nature of the differential conductivity profiling technique limits its applicability if the entire process is done manually. The measurement time can be substantially reduced by automating the method. Computercontrolled experimental methods have been developed in which the sample is anodized, etched and then the resistivity and the mobility are measured in situ.49, 56 – 57 1.4.2
Spreading Resistance Profiling (SRP)
The spreading resistance probe technique has been in use since the 1960s. Although originally used for lateral resistivity variation determination, it is mainly used today to generate resistivity and dopant density depth profiles. It has very high dynamic range (1012 –1021 cm−3 ) and is capable of profiling very shallow junctions into the nm regime. Substantial progress has been made in data collection and treatment. The latter relates to improved sample preparation and probe conditioning procedures, specialized constrained cubic spline smoothing schemes, universally applicable SchumannGardnerbased correction factors with appropriate radius calibration procedures, and the development of
30
RESISTIVITY
physically based Poisson schemes for the correction of the carrier diffusion (spilling) phenomenon. Reproducibility is sometimes mentioned as an SRP problem. Reproducibility of 10% can be obtained routinely by “qualified” SRP systems, provided qualification procedures are rigorously implemented.58 The spreading resistance concept is illustrated in Fig. 1.21. The instrument consists of two carefully aligned probes that are stepped along the beveled semiconductor surface. The resistance between the probes is given by R = 2Rp + 2Rc + 2Rsp
(1.41)
where Rp is the probe resistance, Rc the contact resistance and Rsp the spreading resistance. The resistance is measured at each location.59 The sample is prepared by mounting it on a bevel block with melted wax. Bevel angles less than 1◦ can be readily prepared. The bevel block is inserted into a wellfitting cylinder, and the sample is lapped using a diamond paste or other polishing compound. Sample preparation is very important for successful SRP measurements.60 – 61 Next the sample is positioned in the measurement apparatus with the bevel edge perpendicular to the probe stepping direction. It is very useful to provide the sample with an insulating (oxide or nitride) coating. The oxide provides a sharp corner at the bevel and also clearly defines the start of the beveled surface because the spreading resistance of the insulator is very high. Spreading resistance measurements should be made in the dark to avoid photoconductance effects and are primarily used for silicon. A good discussion of sample preparation is given by Clarysse et al.58 The bevel angle should be measured with a wellcalibrated profilometer. In the absence of a top oxide, the measurement should be started at least 10–20 points before the bevel edge. The actual starting point can then be determined from a micrograph (dark field illumination, magnification 500×). The error on the starting point should not be larger than a few points (maximum 3). Typically, the raw resistance profile shows a transition at the starting point position. The probe imprints must be visible to be able to count them and to determine the starting point. The bevel edge must be sharp enough to reduce the uncertainty of the starting point as much as possible. Good bevel surfaces require a 0.1 or 0.05 µm, highquality, diamond paste. The rotating glass plate, used for polishing the bevel, should have a peaktopeak roughness of 0.13 µm. The probe separation must be below 30–40 µm. Typically, 100–150 data points are used for sub micrometer implants or epitaxial layers. For sub100 nm structures, one should try to obtain 20–25 data points. To understand spreading resistance, consider a metallic probe contacting a semiconductor surface as in Fig. 1.22. The current I flows from the probe of diameter 2r into a Bevelled surface ∆z
Original surface
Plunger
Metal cylinder
~20 µm ∆x
Slurry
Sample
th
dep ction
Jun
le q
l ang
Beve
Glass plate
ate ubstr
S
Fig. 1.21 Spreading resistance bevel block and the beveled sample with probes and the probe path shown by the dashed line.
RESISTIVITY PROFILING
31
I
2r
r
Fig. 1.22 flow.
A cylindrical contact of diameter 2r to a semiconductor. The arrows represent the current
semiconductor of resistivity ρ. The current is concentrated at the probe tip and spreads out radially from the tip. Hence the name spreading resistance. For a nonindenting, cylindrical contact with a planar, circular interface and a highly conductive probe, the spreading resistance for a semiinfinite sample is62 Rsp =
ρ ohms 4r
(1.42a)
For a hemispherical, indenting probe tip of radius r, the spreading resistance is Rsp =
ρ ohms 2πr
(1.42b)
Equation (1.42a) has been verified by comparing spreading resistance with fourpoint probe measurements. The spreading resistance can be expressed as63 Rmeas = Rcont + Rspread = Rcont +
ρ C 2r
(1.43)
where C is a correction factor that depends on sample resistivity, probe radius, current distribution and probe spacing. It should be noted that the radius r is not necessarily the physical radius. The contact resistance also depends on wafer resistivity and probe pressure and on the surface state density. These surface states dominate the Schottky barrier height of the metal/semiconductor contact. The surface state density and energy distribution are expected to be different for polished and beveled surfaces. High surface state densities induce Fermi level pinning.64 On beveled SRP ptype material the contact is expected to be surrounded by a depleted region while ntype material has an inversion layer near the surface. A weight of approximately 5 g is applied and the probes have to be conditioned to form an area of small microcontacts, believed to be necessary to break through the thin native oxide on the bevel surface. Despite the relatively low weight very high local pressures result. Assuming a 1 µm radius, a straightforward division by the contact area leads to an estimate of the contact pressure of approximately 16 GPa. About 80% of the potential drop due to current spreading occurs within a distance of about five times the contact radius. The probe penetration is about 10 nm for probe loads of 10 to 12 g.65 The relationship between SRP measured resistance and Si resistivity is
32
RESISTIVITY
SRP Resistance (Ω)
108 106 104 102
pSi nSi
1 10−4
10−2
100
102
104
Resistivity (Ωcm) Fig. 1.23
Calibration curves for conventional SRP measurements. After ref. 63.
shown in Fig. 1.23.63 For a contact radius of 1 µm, Eq. (1.42a) predicts Rsp ≈ 2500ρ. The fact that the spreading resistance is about 104 times higher than ρ is the reason that Rsp dominates over Rp and Rc in Eq. (1.41). However, if the metalsemiconductor barrier height is significant, then the measured resistance does include a nonnegligible contact resistance, as in GaAs, for example. The tungstenosmium alloy probes, are mounted in gravityloaded probe arms. The probe tips are shaped so that they can be positioned very close together, often with less than 20 µm spacing. The probe arms are supported by a kinematic bearing system with five contacts giving the arms only one degree of freedom, which is a rotation around the horizontal axis. This virtually eliminates lateral probe motion during contact to the sample minimizing probe wear and damage to the semiconductor. The probes deform only slightly elastically upon contacting the semiconductor, thus making very reproducible contacts. The probes are “conditioned” using the “GoreySchneider technique”63 for the contact area of the probe to consist of a large number of microscopic protrusions to penetrate the thin oxide layer on silicon surfaces. An example SRP plot and the resulting dopant density profile is shown in Fig. 1.24. The conversion of spreading resistance data to a carrier density profile and subsequently to a doping density profile is a complicated task that involves data smoothing to reduce measurement noise, a deconvolution algorithm, and a correct model for the contact.67 An important aspect of SRP is the fact that spreading resistance measures a carrier distribution along a beveled surface. It has often been assumed that this profile is identical to the vertical carrier profile. Furthermore, the vertical carrier profile is often assumed to be identical to the vertical doping profile. This is not true for shallow junctions where the redistribution of mobile carriers, referred to as carrier spilling, distorts the measured SR profiles. For example, electrons from the highly doped n+ layer in an n+ p junction spill into the lowly pdoped substrate. Hence, an SRP plot, that is expected to show a resistance maximum at the metallurgical junction due to the spacecharge region with few carriers, may not show such a maximum at all.67 The actual plot suggests the absence of a junction leading to the conclusion that the junction may be an n+ n junction. Carrier spilling accounts for SRP determined junction depths being usually less than those measured by SIMS.68
RESISTIVITY PROFILING
105
1020 1019
104
1018 1017
103
1016
SRP Resistance (Ω)
Doping Density (cm−3)
1021
33
1015 1014
0
0.025
0.05
0.075
102 0.1
Depth (µm)
Fig. 1.24 Highresolution spreading resistance and dopant density profiles. Data courtesy of S. Weinzierl, Solid State Measurements, Inc.
The voltage between the probes during measurement is kept at around 5 mV to reduce the effect of contact resistance. The probesemiconductor contact is a metalsemiconductor contact with the nonlinear current–voltage characteristic I = I0 (eqV /kT − 1) ≈ I0 qV /kT
(1.44)
for voltages less than kT /q ≈ 25 mV. The spreading resistance profiling technique is a comparative technique. Calibration curves are generated for a particular set of probes at a particular time using samples of known resistivity. Such calibration samples are commercially available for silicon. Comparison of the spreading resistance data to the calibration samples is necessary and sufficient for uniformly doped samples. For samples containing pn or highlow junctions, additional corrections are necessary. These multilayer corrections have evolved over the years where today very sophisticated correction schemes are used.67 – 72 A different approach calculates the spreading resistance profile from an assumed doping profile.73 The calculated profile is then compared to the measured profile and adjusted until they agree. The bevel angle θ is typically 1◦ –5◦ for junction depths of 1–2 µm and θ ≤ 0.5◦ for junction depths less than 0.5 µm. The equivalent depth, z, for each x step along the surface beveled at angle θ , is z = x sin(θ ) (1.45) For a step of 5 µm and an angle of 1◦ , the equivalent step height or measurement resolution is 0.87 nm. A plot of dopant density profiles determined by differential Hall effect, spreading resistance profiling, and secondary ion mass spectrometry (SIMS) is shown in Fig. 1.20. Note the good agreement between DHE and SRP for this sample. SIMS profiling is discussed in Chapter 2. The small SRP angles are determined by measuring a small slit of light that is reflected from the beveled and the unbeveled surfaces so that two images are detected. When the slit is rotated, the two images rotate also, and the rotation angle is measured and related to the bevel angle.74 Surface profilometers can also be used for angle determination.61 Limitations in SRP profiling for very shallow junctions arise due to the large sampling volume induced by the large contact and probe spacing necessitating correction
34
RESISTIVITY
factors which can be as large as 2000. Moreover, additional correction factors have been identified to correct for carrier spilling, surface damage, microcontact distribution, and threedimensional current flow. Unfortunately, all these corrections become increasingly important for very shallow profiles and scale with probe radius and probe separation. Probe penetration and bevel roughness also limit the depth resolution. In order to cope with the limited thickness of the layers, very shallow bevels are required.75 Almost all spreading resistance measurements are made with two probes, but threeprobe arrangements have been used.69 In the threeprobe configuration one probe serves as the common point to both voltage and current circuits and is the only probe contributing to the measured resistance. The threeprobe system is more difficult to keep aligned. Since probe alignment parallel to the bevel intersection with the top surface is crucial for depth profiling, the threepoint spreading resistance probe is rarely used. Micro spreading resistance, known as scanning spreading resistance microscopy is discussed in Chapter 9.
1.5
CONTACTLESS METHODS
Contactless resistivity measurement techniques have become popular in line with the general trend toward other contactless semiconductor measurements. Contactless resistivity measurement methods fall into two broad categories: electrical and nonelectrical measurements. Commercial equipment is available for both. Electrical contactless measurement techniques fall into several categories. (1) the sample is placed into a microwave circuit and perturbs the transmission or reflection characteristics of a waveguide or cavity76 , (2) the sample is capacitively coupled to the measuring apparatus77 , and (3) the sample is inductively coupled to the apparatus.78 – 79 1.5.1
Eddy Current
To be a viable commercial instrument, the apparatus should be simple with no special sample requirements. This rules out special sample configurations to fit microwave cavities, for example, and led to a variation of the inductively coupled approach. The eddy current measurement technique is based on the parallel resonant tank circuit of Fig. 1.25. The quality factor Q of such a circuit is reduced when a conducting material is brought close to the coil due to the power absorbed by the conducting material. An implementation of this concept is shown in Fig. 1.25(a), where the LC circuit is replaced by dual coils on ferrite cores separated to provide a gap for the wafer that is coupled to the circuit via the high permeability ferrite cores. The oscillating magnetic field sets up eddy currents in the semiconductor leading to Joule heating of the material. The absorbed power Pa is80 Pa = K(VT /n)2
t
σ (x) dx
(1.46)
0
where K is a constant involving the coupling parameters of the core, VT the rms primary rf voltage, n the number of primary turns of the coil, σ the semiconductor conductivity, and t the thickness. With power given by Pa = VT IT , where IT is the inphase drive current KV T t KV T 1 IT = (1.47) σ (x) dx = n2 0 n2 Rsh
CONTACTLESS METHODS
35
Sound generator
IT Wafer VT
Sound receiver
Ferrite (a) Drive coil
Wafer
RF coil
. . . . . .
. . . . . .
. . . . . .
. . . . . .
Ferrite core
Sound receiver
Sound generator
Eddy currents (b)
(c)
Fig. 1.25 (a) Schematic eddy current experimental arrangement, (b) practical implementation after Johnson81 , and (c) schematic showing the eddy current coils and the thickness sound generator.
If VT is held constant through a feedback circuit, the current is proportional to the sample conductivitythickness product, or it is inversely proportional to the sample sheet resistance. A more recent implementation is shown in Fig. 1.25(b).81 Eddy current and other contactless techniques are discussed further in Chapter 7 in reference to lifetime measurements. When an alternating current is induced in a conductor, the current is not uniformly distributed, but is displaced toward the surface. For high frequencies most of the current is concentrated in a layer near the surface known as the skin depth. Equation (1.46) is valid provided the sample is thinner than the skin depth δ given by (1.48) δ = ρ/πf µo = 5.03 × 103 ρ/f cm
where ρ is the resistivity ( · cm), f the frequency (Hz), and µo the permeability of free space (4π × 10−9 H/cm). Equation (1.48) is plotted in Fig. 1.26 as a function of frequency. Comparison of fourpoint probe and eddy current wafer maps are shown in Fig. 1.27 for Al and Ti layers. Note the excellent agreement in the contours and the average sheet resistances. To determine the wafer resistivity, its thickness must be known. In contactless measurements provision must be made to measure the wafer thickness without contact. Two methods are used: differential capacitance probe and ultrasound.82 In the ultrasound method sound waves are reflected from the upper and lower wafer surfaces located between the two probes shown in Fig. 1.25(c). The phase shift of the reflected sound caused by the impedance variation of the air gap is detected by the sonic receiver. The phase shift is proportional to the distance from each probe to each surface. With known probe spacing, the wafer thickness can be determined. One system to determine sample thickness by capacitance measurements is illustrated in Fig. 1.28.83 Two capacitive probes of area A are separated by a distance s. The semiconductor wafer is held between the two capacitance probes. Each probe forms one plate of the capacitor, the wafer the other. The capacitance is C1 = εo A/d 1 between the upper
36
RESISTIVITY
f = 105 106 107 108 109 Hz 1010 1011
103 Skin Depth (cm)
102 101 100 10−1 10−2 10−3 10−4 10−3
10−2
10−1
100
101
102
103
Resistivity (ohmcm)
Fig. 1.26
+
+
Skin depth versus resistivity as a function of frequency.
−
− + −
+
+ −
+
−
−
−
+
+
+
− − +
−
−
− −
−
+
+
−
−
−
−
−
− − −
+ + + +
−
+
−
+
+
−
+ +
−
+
+ +
+
−
− +
−
− −
+
(b)
+
− −
−
+ +
−
+ −
+
+
+
+ −
+ +
+ −
+
+
+
+
−
− +
+
+
−
+
−
−
−
+
−
− +
+
−
−
−
−
− −
−
−
−
+
−
−
− −
−
−
+
+
+
−
−−
−
+
−
−
−
−
−
+
+
− −
− −
−
−
+
−
−
+
+
(a)
+
+
+
+
+
− +
−
+
+
+
+
+ +
+
−
−
+
+
+
+
+
+
+
−
− +
+
+
−
−
−
−
+
−
+
−
+
−
−
+
−
−
−
+
−
−
−
+
+
−
−
+ +
−
+
−
− −
+
−
−
−
+
−
−
+ −
−
−
+ +
+
+
−
+
+
+
−
−
+
+
+
−
−
−
−
−
+
+ −
−
+
+
−
−
−
+
+
+
+
Fig. 1.27 (a) Fourpoint probe and (b) eddy current contour maps. Left: 1 µm aluminum layer, Rsh,av (4 pt) = 3.023 × 10−2 ohms/square, Rsh,av (eddy) = 3.023 × 10−2 ohms/square, right: 20 nm titanium layer, Rsh,av (4 pt) = 62.90 ohms/square, Rsh,av (eddy) = 62.56 ohms/square. Data courtesy of W.H. Johnson, KLATencor.
CONTACTLESS METHODS
Probe A
d1
t s
Wafer
Wafer holding fixture
Fig. 1.28
Probe B
37
d2
Capacitive wafer thickness and flatness measurement system.
probe and the wafer and C2 = εo A/d 2 between the lower probe and the wafer. From Fig. 1.28, the thickness t is t = s − (d1 + d2 ) = s − εo A(C1−1 + C2−1 )
(1.49)
To determine t we only need to know the probe separation s and the capacitances C1 and C2 . The wafer thickness measurement is independent of the vertical wafer position in the gap. As the wafer moves in the vertical direction, both d1 and d2 change by equal and opposite amounts leaving the thickness reading unchanged. The median surface is determined by d1 + d2 . By measuring the capacitance at many points on the wafer, the thickness and shape of the entire wafer can be determined. Bow and warpage, due to stress in the wafer, are determined from the median surface reading allowing the stress to be determined.84 The flatness obtained by this capacitive technique is a function of only the wafer, not the mechanical support used in the instrument. Resistivity measurements based on the eddy current technique are useful for uniformlydoped wafers. The technique has also found use for the measurement of highly conductive layers on less conductive substrates. The sheet resistance of the layer should be at least a hundred times lower than the sheet resistance of the substrate to measure the layer and not the substrate. This rules out measurements of diffused or ionimplanted layers on conducting substrates, which generally do not satisfy this rule. For example, sheet resistances of diffused or ionimplanted layers are typically 10 to 100 ohms/square, and the sheet resistance of a 10 ohm · cm, 650 µm thick Si wafer is 154 ohms/square. However, the sheet resistance of implanted or epitaxial layers on semiinsulating substrates (e.g., GaAs) or of metal layers on semiconductor substrates can be measured. The sheet resistance of a ˚ Al layer is typically 0.06 to 0.1 ohms/square, making such layers 2000 times less 5000 A resistive than the Si substrate. The layer thickness is determined from a sheet resistance measurement according to (1.50) t = Rsh /ρ The layer resistivity must be determined from an independent measurement. Contactless resistance measurements are routinely used to determine sheet resistances and thicknesses of conducting layers.
38
RESISTIVITY
Eddy current measurements require calibrated standards. Radial resistivity variations or other ρ nonuniformities under the transducer are averaged and may be different from that of other ρ or Rsh measurement techniques. The measurement frequency should be such that the skin depth is at least five times the sample thickness to be measured.
1.6
CONDUCTIVITY TYPE
The semiconductor conductivity type can be determined by wafer flat location, thermal emf, rectification, optically, and Hall effect. The Hall effect is discussed in Chapter 2. The simplest method utilizes the shape of the wafer flats for those wafers following a standard pattern. Silicon wafers are usually circular. They may have characteristic flats, illustrated in Fig. 1.29, provided for alignment and identification purposes. The primary flat (usually along the 110 direction) and secondary flats identify the conductivity type and orientation. Wafers of diameter ≤150 mm usually have the standard flats of Fig. 1.29. Larger wafers usually do not have flats; instead they are provided with notches that do not provide conductivity type information. In the hot or thermoelectric probe method the conductivity type is determined by the sign of the thermal emf or Seebeck voltage generated by a temperature gradient. Two probes contact the sample surface: one is hot the other is cold as illustrated in Fig. 1.30(a). Thermal gradients generate currents in a semiconductor; the majority carrier currents for n and ptype materials are85 Jn = −qnµn Pn dT /dx; Jp = −qpµp Pp dT /dx
(1.51)
where Pn < 0 and Pp > 0 are the differential thermoelectric power. Consider the experimental arrangement of Fig. 1.30(a). The right probe is hot, the left probe is cold. dT /dx > 0 and the electron current in an ntype sample flows from left to right. The thermoelectric power can be thought of as a current generator. Some of the
45° {111} pType
{111} nType
Secondary Flat
90°
{100} pType
Fig. 1.29
180° Primary Flat {100} nType
Identifying flats on silicon wafers.
CONDUCTIVITY TYPE
39
Vb −V+
V32
Cold
Hot
1
2
3
4
I Electric Field nType
nType
(b)
(a) Vb 2
3
V32 V32 (V)
1
4
nSubstr.
2 0
−4
−2
0
2
4
Vb (V)
−2
I A (c)
−4
pSubstr. (d)
Fig. 1.30 Conductivity type measurements. (a) Hot probe; (b) rectifying probe, (c) equivalent circuit for (b), and (d) experimental data adapted from ref. 88.
current flows through the voltmeter causing the hot probe to develop a positive potential with respect to the cold probe.86 – 87 There is a simple alternative view. Electrons diffuse from the hot to the cold region setting up an electric field that opposes the diffusion. The electric field produces a potential detected by the voltmeter with the hot probe positive with respect to the cold probe. Analogous reasoning leads to the opposite potential for ptype samples. Hot probes are effective over the 10−3 to 103 ohmcm resistivity range. The voltmeter tends to indicate ntype for high resistivity material even if the sample is weakly ptype because the method actually determines the nµn or the pµp product. With µn > µp intrinsic or high resistivity material is measured ntype if n ≈ p. In semiconductors with ni > n or ni > p at room temperature (narrow band gap semiconductors, for example), it may be necessary to cool one of the probes and let the room temperature probe be the “hot” probe. In the rectification method, the sign of the conductivity is determined by the polarity of a rectified ac signal at a point contact to the semiconductor.86 – 87 When two probes are used, one should be rectifying and the other should be ohmic. Current flows through a rectifying contact to ntype material if the metal is positive and for ptype if it is negative. Rectifying and ohmic contacts are difficult to implement with twopoint contacts. Fortunately fourpoint probes can be used with appropriate connections. A dc voltage is applied and current flows between probes 1 and 2, and the resulting potential is measured between probes 3 and 2 in Fig. 1.30(b). For an nsubstrate with positive Vb , the probe 1 metalsemiconductor diode is forward biased and probe 2 diode is reverse biased. Hence the current I is the leakage current of the reversebiased diode and diode 1 in Fig. 1.30(c)
40
RESISTIVITY
has very low forward bias. The voltage at point A is VA = Vb + VD1 ≈ Vb
(1.52)
The voltage is measured with a highinput impedance voltmeter with very low current between points A and 3. Hence, there is negligible voltage drop across diode 3 and V32 ≈ VA . (1.53) V32 ≈ VA ≈ Vb For psubstrates and the same bias arrangement as in Fig. 1.30(c) diode 1 is reverse and diode 2 forward biased. Consequently, V32 ≈ VA ≈ 0
(1.54)
Equations (1.53) and (1.54) show how this probe arrangement can be used for semiconductor type determination. The voltage dependence is shown in Fig. 1.30(d). For thin semiconductor films, e.g., silicononinsulator or polysilicon films, the metallic needle probes have been replaced with mercury probes.88 This method of conductivity type measurement is built into some commercial fourpoint probe instruments. In the optical method, an incident modulated laser beam creates a timevarying surface photovoltage (SPV) in the sample, detected with a nonvibrating, optically transparent Kelvin probe held up to several cm from the sample surface. The principle is the surface photovoltage method discussed in Section 7.4.5. The SPV is negative for ptype and positive for ntype semiconductors.
1.7
STRENGTHS AND WEAKNESSES
FourPoint Probe: The weakness of the fourpoint probe technique is the surface damage it produces and the metal it deposits on the sample. The damage is not very severe but sufficient not to make measurements on wafers to be used for device fabrication. The probe also samples a relatively large volume of the wafer, preventing highresolution measurements. The method’s strength lies in its established use and the fact that it is an absolute measurement without recourse to calibrated standards. It has been used for many years in the semiconductor industry and is well understood. With the advent of wafer mapping, the fourpoint probe has become a very powerful processmonitoring tool. This is where its major strength lies today. Differential Hall Effect: The weakness of this method is its tediousness. The layer removal by anodic oxidation is well controlled, but it is also slow, limiting the method to relatively few data points per profile when done manually. That restriction is lifted when the technique is automated. The sheet resistance can be measured by fourpoint probe or Hall effect. Repeated fourpoint probe measurements on the same area create damage, rendering the measurements questionable. That problem does not exist for Hall samples. The method is destructive. The method’s strength lies in its inexpensive equipment when using “home assembled” equipment. For those dopant profiles that cannot be profiled by capacitancevoltage measurements, only secondary ion mass spectrometry and spreading resistance methods are the alternatives. Equipment for those measurements is significantly more expensive, leaving anodic oxidation/fourpoint probe as a viable, inexpensive alternative.
APPENDIX 1.1
41
Spreading Resistance: The weakness of the spreading resistance profiling technique is the necessity of a skilled operator to obtain reliable profiles. The system must be periodically calibrated against known standards, and the probes must be periodically reconditioned. It does not work well for semiconductors other than Si and Ge. The sample preparation is not trivial, and the measurement is destructive. The conversion of the measured spreading resistance data to doping density profiles depends very much on the algorithm. Several algorithms are in use, and others are being developed. The strengths of SRP lie in the ability to profile practically any combination of layers with very high resolution and no depth limitation and no doping density limitations. Very high resistivity material must be carefully measured and interpreted. The equipment is commercially available and it is used extensively. Hence there is a large background of knowledge related to this method, which has been in use over the past 40 years. Contactless Techniques: The weakness of the eddy current technique is its inability to determine the sheet resistance of thin diffused or ionimplanted layers. In order to detect such sheet resistances, it is necessary for the sheet resistance of the layer to be on the order of a hundred times lower than the sheet resistance of the substrate. This is only attainable when the sheet consists of a metal on a semiconductor or a highly doped layer on an insulating substrate. The eddy current technique is often used to measure the sheet resistance of metal layers on semiconductor substrates to determine their thickness. The strength of the eddy current method lies in its noncontacting nature and the availability of commercial equipment. This is ideal for measuring the resistivity of semiconductor wafers and the layer thickness. Optical Techniques: The weakness of optical techniques is that the measurements are qualitative with quantitative doping measurements requiring calibrated standards. Profiling is generally not possible, and only average values are obtained. The optical densitometry and modulated photoreflectance techniques have become commercially available methods. They are mainly used for wafer mapping of ionimplanted wafers. Their strength lies in their ability to measure the implants nondestructively, with small spot size, and rapidly and in displaying the information in the form of contour plots. The modulated photoreflectance technique is able to measure through an oxide and is routinely used for ion implantation monitoring. Disadvantages are possible laser drift and postimplant damage relaxation. Disadvantages of optical densitometry are the Al backing plate that must be affixed to the wafer rear surface before implantation and removed for optical sensing and the film’s UV sensitivity. Without the backing plate the optical sensors in the ion implanter will register a loading error. APPENDIX 1.1 Resistivity as a Function of Doping Density Figures A1.1(a) and (b) show the resistivity for boron and phosphorusdoped Si. For borondoped Si, the boron density is related to the resistivity by89 NB = ρ=
1.33 × 1016 1.082 × 1017 + [cm−3 ] ρ ρ[1 + (54.56ρ)1.105 ]
1.133 × 1017 1.305 × 1016 [ cm] + NB NB [1 + (2.58 × 10−19 NB )−0.737 ]
(A1.1)
42
RESISTIVITY
Resistivity (ohmcm)
104 Boron
102
100 Phosphorus
10−2
10−4 1012
1014
1016
1018
Dopant Density (a)
(cm−3)
1020
Resistivity (ohmcm)
102
101 Boron 100 Phosphorus
10−1
10−2 1014
1015
1016
1017
1018
1019
Dopant Density (cm−3) (b) 102 nGaP
Resistivity (ohmcm)
101 100 10−1
pGaP pGe
10−2 10
pGaAs nGe
−3
10−4 1014
nGaAs 10
15
10
16
17
10
1018
1019
1020
1021
Dopant Density (cm−3) (c)
Fig. A1.1 (a) and (b) Doping density versus resistivity for ptype (borondoped) and ntype (phosphorusdoped) silicon at 23◦ C. Data from ASTM F723; (c) for Ge, GaAs, and GaP. Data from Ref. 95 and 96.
APPENDIX 1.2
43
For phosphorusdoped Si, the phosphorus density is related to the resistivity by89 NP =
A0 + A1 x + A2 x 2 + A3 x 3 6.242 × 1018 10Z [cm−3 ], where Z = ρ 1 + B1 x + B2 x 2 + B3 x 3
(A1.2a)
where x = log10 (ρ), A0 = −3.1083, A1 = −3.2626, A2 = −1.2196, A3 = −0.13923, B1 = 1.0265, B2 = 0.38755, and B3 = 0.041833. The resistivity is ρ=
C0 + C 1 y + C 2 y 2 + C 3 y 3 6.242 × 1018 10Z [ cm], where Z = NP 1 + D1 y + D2 y 2 + D3 y 3
(A1.2b)
and y = log10 (NP ) − 16, C0 = −3.0769, C1 = 2.2108, C2 = −0.62272, C3 = 0.057501, D1 = −0.68157, D2 = 0.19833, and D3 = −0.018376. Resistivity plots for Ge, GaAs, and GaP are shown in Fig. A1.1(c). APPENDIX 1.2 Intrinsic Carrier Density The intrinsic carrier density ni for Si has been described by a number of equations over the years. The most recent and most accurate expressions are90 – 91 ni = 5.29 × 1019 (T /300)2.54 exp(−6726/T )
(A2.1a)
ni = 2.91 × 10 T
(A2.1b)
15
1.6
exp(−EG (T )/2kT )
where the temperaturedependent band gap is given by92 EG (T ) = 1.17 + 1.059 × 10−5 T − 6.05 × 10−7 T 2
EG (T ) = 1.1785 − 9.025 × 10−5 T − 3.05 × 10−7 T 2
(0 ≤ T ≤ 190 K)
(A2.2a)
(150 ≤ T ≤ 300 K) (A2.2b)
T is in Kelvin. ni and EG are plotted in Figs. A2.1 and A2.2. Eq. (A2.1a) is based on experiments over the 78–340 K temperature range.92 Equation (A2.1a) has been rewritten
Temperature (K)
ni (cm−3)
1015
170
190
210
230
250 108
1014
107
1013
106
1012
105
1011
104
1010
103 102
109 108
ni (cm−3)
150
Si
250
300
350
400
450
10 500
Temperature (K)
Fig. A2.1
Silicon intrinsic carrier density versus temperature.
44
RESISTIVITY
1.17
Band Gap (eV)
1.15 1.13 1.11 1.09 1.07 Si 1.05 150 200
250
300
350
400
450
500
Temperature (K)
Fig. A2.2
Silicon band gap versus temperature.
0.2 pSi nSi
∆EG (eV)
0.15
0.1
0.05
0 1016
1017
1018
1019
1020
1021
−3
Carrier Density (cm )
Fig. A2.3
Silicon band gap narrowing versus carrier density.
as Eq. (A2.1b) by Trupke et al.91 At T = 300 K, ni = 9.7 × 109 cm−3 . This is slightly lower than the earlier value by Sproul and Green93 due to band gap narrowing. Band gap narrowing is expressed by ni,eff = ni exp(EG /kT )
(A2.3)
where the band gap narrowing energy, EG , is shown in Fig. A2.3.94 REFERENCES 1. F. Wenner, “A Method of Measuring Earth Resistivity,” Bulletin of the Bureau of Standards 12, 469–478, 1915. 2. L.B. Valdes, “Resistivity Measurements on Germanium for Transistors,” Proc. IRE 42, 420–427, Feb. 1954. 3. H.H. Wieder, “Four Terminal Nondestructive Electrical and Galvanomagnetic Measurements,” in Nondestructive Evaluation of Semiconductor Materials and Devices (J.N. Zemel, ed.), Plenum Press, New York, 1979, 67–104.
REFERENCES
45
4. R. Hall, “Minimizing Errors of FourPoint Probe Measurements on Circular Wafers,” J. Sci. Instrum. 44, 53–54, Jan. 1967. 5. D.C. Worledge, “Reduction of Positional Errors in a Fourpoint Probe Resistance Measurement,” Appl. Phys. Lett. 84, 1695–1697, March 2004. 6. A. Uhlir, Jr., “The Potentials of Infinite Systems of Sources and Numerical Solutions of Problems in Semiconductor Engineering,” Bell Syst. Tech. J. 34, 105–128, Jan. 1955; F.M. Smits, “Measurement of Sheet Resistivities with the FourPoint Probe,” Bell Syst. Tech. J. 37, 711–718, May 1958. 7. M.G. Buehler, “A Hall FourPoint Probe on Thin Plates,” SolidState Electron. 10, 801–812, Aug. 1967. 8. M.G. Buehler, “Measurement of the Resistivity of a Thin Square Sample with a Square FourProbe Array,” SolidState Electron. 20, 403–406, May 1977. 9. M. Yamashita, “Geometrical Correction Factor for Resistivity of Semiconductors by the Square FourPoint Probe Method,” Japan. J. Appl. Phys. 25, 563–567, April 1986. 10. S. Murashima and F. Ishibashi, “Correction Devisors for the FourPoint Probe Resistivity Measurement on Cylindrical Semiconductors II,” Japan. J. Appl. Phys. 9, 1340–1346, Nov. 1970. 11. D.S. Perloff, “FourPoint Probe Correction Factors for Use in Measuring Large Diameter Doped Semiconductor Wafers,” J. Electrochem. Soc. 123, 1745–1750, Nov. 1976; D.S. Perloff, “FourPoint Probe Sheet Resistance Correction Factors for Thin Rectangular Samples,” SolidState Electron. 20, 681–687, Aug. 1977. 12. M. Yamashita and M. Agu, “Geometrical Correction Factor for Semiconductor Resistivity Measurements by FourPoint Probe Method,” Japan. J. Appl. Phys. 23, 1499–1504, Nov. 1984. 13. R.A. Weller, “An Algorithm for Computing Linear Fourpoint Probe Thickness Correction Factors,” Rev. Sci. Instrument. 72, 3580–3586, Sept. 2001. 14. J. Albers and H.L. Berkowitz, “An Alternative Approach to the Calculation of FourProbe Resistances on Nonuniform Structures,” J. Electrochem. Soc. 132, 2453–2456, Oct. 1985. 15. J.J. Kopanski, J. Albers, G.P. Carver, and J.R. Ehrstein, “Verification of the Relation Between TwoProbe and FourProbe Resistances as Measured on Silicon Wafers,” J. Electrochem. Soc. 137, 3935–3941, Dec. 1990. 16. M.P. Albert and J.F. Combs, “Correction Factors for Radial Resistivity Gradient Evaluation of Semiconductor Slices,” IEEE Trans. Electron Dev. ED11, 148–151, April 1964. 17. R. Rymaszewski, “Relationship Between the Correction Factor of the FourPoint Probe Value and the Selection of Potential and Current Electrodes,” J. Sci. Instrum. 2, 170–174, Feb. 1969. 18. ASTM Standard F8493, “Standard Method for Measuring Resistivity of Silicon Slices With a Collinear FourPoint Probe,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 19. D.S. Perloff, J.N. Gan and F.E. Wahl, “Dose Accuracy and Doping Uniformity of Ion Implantation Equipment,” Solid State Technol. 24, 112–120, Feb. 1981. 20. A.K. Smith, D.S. Perloff, R. Edwards, R. Kleppinger and M.D. Rigik, “The Use of FourPoint Probe Sheet Resistance Measurements for Characterizing Low Dose Ion Implantation,” Nucl. Instrum. and Meth. B6, 382–388, Jan. 1985. 21. ASTM Standard F152994, “Standard Method for Sheet Resistance Uniformity by InLine FourPoint Probe With the DualConfiguration Procedure,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 22. H.H. Gegenwarth, “Correction Factors for the FourPoint Probe Resistivity Measurement on Cylindrical Semiconductors,” SolidState Electron. 11, 787–789, Aug. 1968. 23. S. Murashima, H. Kanamori and F. Ishibashi, “Correction Devisors for the FourPoint Probe Resistivity Measurement on Cylindrical Semiconductors,” Japan. J. Appl. Phys. 9, 58–67, Jan. 1970.
46
RESISTIVITY
24. L.J. van der Pauw, “A Method of Measuring Specific Resistivity and Hall Effect of Discs of Arbitrary Shape,” Phil. Res. Rep. 13, 1–9, Feb. 1958. 25. W. Versnel, “Analysis of Symmetrical van der Pauw Structures With Finite Contacts,” SolidState Electron. 21, 1261–1268, Oct. 1978. 26. L.J. van der Pauw, “A Method of Measuring the Resistivity and Hall Coefficient on Lamellae of Arbitrary Shape,” Phil. Tech. Rev. 20, 220–224, Aug. 1958; R. Chwang, B.J. Smith and C.R. Crowell, “Contact Size Effects on the van der Pauw Method for Resistivity and Hall Coefficient Measurement,” SolidState Electron. 17, 1217–1227, Dec. 1974. 27. Y. Sun, J. Shi, and Q. Meng, “Measurement of Sheet Resistance of Cross Microareas Using a Modified van der Pauw Method,” Semic. Sci. Technol. 11, 805–811, May 1996. 28. M.G. Buehler and W.R. Thurber, “An Experimental Study of Various Cross Sheet Resistor Test Structures,” J. Electrochem. Soc. 125, 645–650, April 1978. 29. M.G. Buehler, S.D. Grant and W.R. Thurber, “Bridge and van der Pauw Sheet Resistors for Characterizing the Line Width of Conducting Layers,” J. Electrochem. Soc. 125, 650–654, April 1978. 30. R. Chang, Y. Cao, and C.J. Spanos, “Modeling the Electrical Effects of Metal Dishing Due to CMP for OnChip Interconnect Optimization,” IEEE Trans. Electron Dev. 51, 1577–1583, Oct. 2004. 31. ASTM Standard F7602, “Standard Test Method for Measuring Resistivity and Hall Coefficient and Determining Hall Mobility in Single Crystal Semiconductors,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 32. DIN Standard 504301980, “Testing of Semiconducting Inorganic Materials: Measurement of the Specific Electrical Resistivity of Si or Ge Single Crystals in Bars Using the TwoProbe DirectCurrent Method,” 1995 Annual Book of ASTM Standards, Am. Soc. Test. Mat., Philadelphia, 1995. 33. J.T.C. Chen, “Monitoring Low Dose Single Implanted Layers With FourPoint Probe Technology,” Nucl. Instrum. and Meth. B21, 526–528, 1987. 34. T. Matsumara, T. Obokata and T. Fukuda, “TwoDimensional Microscopic Uniformity of Resistivity in SemiInsulating GaAs,” J. Appl. Phys. 57, 1182–1185, Feb. 1985. 35. P.M. Hemenger, “Measurement of High Resistivity Semiconductors Using the van der Pauw Method,” Rev. Sci. Instrum. 44, 698–700, June 1973. 36. L. Forbes, J. Tillinghast, B. Hughes and C. Li, “Automated System for the Characterization of High Resistivity Semiconductors by the van der Pauw Method,” Rev. Sci. Instrum. 52, 1047–1050, July 1981. 37. P.A. Crossley and W.E. Ham, “Use of Test Structures and Results of Electrical Test for SiliconOnSapphire Integrated Circuit Processes,” J. Electron. Mat. 2, 465–483, Aug. 1973; D.S. Perloff, F.E. Wahl and J. Conragan, “FourPoint Sheet Resistance Measurements of Semiconductor Doping Uniformity,” J. Electrochem. Soc. 124, 582–590, April 1977. 38. C.B. Yarling, W.H. Johnson, W.A. Keenan, and L.A. Larson, “Uniformity Mapping in Ion Implantation,” Solid State Technol. 34/35, 57–62, Dec. 1991; 29–32, March 1992. 39. J.N. Gan and D.S. Perloff, “PostImplant Methods for Characterizing the Doping Uniformity and Dose Accuracy of Ion Implantation Equipment,” Nucl. Instrum. and Meth. 189, 265–274, Nov. 1981; M.I. Current, N.L. Turner, T.C. Smith and D. Crane, “Planar Channelling Effects in Si (100),” Nucl. Instrum. and Meth. B6, 336–348, Jan. 1985. 40. A.K. Smith, W.H. Johnson, W.A. Keenan, M. Rigik and R. Kleppinger, “Sheet Resistance Monitoring of Low Dose Ion Implants Using the Double Implant Technique,” Nucl. Instrum. and Meth. B21, 529–536, March 1987; S.L. Sundaram and A.C. Carlson, “Double Implant Low Dose Technique in Analog IC Fabrication,” IEEE Trans. Semicond. Manuf. 4, 146–150, Nov. 1989. 41. A. Rosencwaig, “Thermalwave Imaging,” Science 218, 223–228, Oct. 1982.
REFERENCES
47
42. N.M. Amer and M.A. Olmstead, “A Novel Method for the Study of Optical Properties of Surfaces,” Surf. Sci. 132, 68–72, Sept. 1983; N.M. Amer, A. Skumanich, and D. Ripple, “Photothermal Modulation of the Gap Distance in Scanning Tunneling Microscopy,” Appl. Phys. Lett. 49, 137–139, July 1986. 43. A. Rosencwaig, J. Opsal, W.L. Smith and D.L. Willenborg, “Detection of Thermal Waves Through Optical Reflectance,” Appl. Phys. Lett. 46, 1013–1015, June 1985. 44. W.L. Smith, A. Rosencwaig and D.L. Willenborg, “Ion Implant Monitoring with Thermal Wave Technology,” Appl. Phys. Lett. 47, 584–586, Sept. 1985; W.L. Smith, A. Rosencwaig, D.L. Willenborg, J. Opsal and M.W. Taylor, “Ion Implant Monitoring with Thermal Wave Technology,” Solid State Technol. 29, 85–92, Jan. 1986. 45. P. Borden, “Junction Depth Measurement Using Carrier Illumination,” in Characterization and Metrology For ULSI Technology 2000 (D.G. Seiler, A.C. Diebold, T.J. Shaffner, R. McDonald, W.M. Bullis, P.J. Smith, and E.M. Sekula, eds.) Am. Inst. Phys. 550, 175–180, 2001; P. Borden, L. Bechtler, K. Lingel, and R. Nijmeijer, “Carrier Illumination Characterization of UltraShallow Implants,” in Handbook of Silicon Semiconductor Metrology (A.C. Diebold, ed.), Marcel Dekker, New York, 2001, Ch. 5. 46. W. Vandervorst, T. Clarysse, B. Brijs, R. Loo, Y. Peytier, B.J. Pawlak, E. Budiarto, and P. Borden, “Carrier Illumination as a Tool to Probe Implant Dose and Electrical Activation,” in Characterization and Metrology for ULSI Technology 2003 (D.G. Seiler, A.C. Diebold, T.J. Shaffner, R. McDonald, S. Zollner, R.P. Khosla, and E.M. Sekula, eds.) Am. Inst. Phys. 683, 758–763, 2003. 47. J.P. Esteves and M.J. Rendon, “Optical Densitometry Applications for Ion Implantation,” in Characterization and Metrology for ULSI Technology 1998 (D.G. Seiler, A.C. Diebold, W.M. Bullis, T.J. Shaffner, R. McDonald, and E.J. Walters, eds.) Am. Inst. Phys. 449, 369–373, 1998. 48. R.A. Evans and R.P. Donovan, “Alternative Relationship for Converting Incremental Sheet Resistivity Measurements into Profiles of Impurity Concentration,” SolidState Electron. 10, 155–157, Feb. 1967. 49. S.B. Felch, R. Brennan, S.F. Corcoran, and G. Webster, “A Comparison of Three Techniques for Profiling Ultrashallow p+ n Junctions,” Solid State Technol. 36, 45–51, Jan. 1993. 50. R.S. Huang and P.H. Ladbrooke, “The Use of a FourPoint Probe for Profiling SubMicron Layers,” SolidState Electron. 21, 1123–1128, Sept. 1978. 51. D.C. Look, “Hall Effect Depletion Correction in IonImplanted Samples: Si29 in GaAs,” J. Appl. Phys. 66, 2420–2424, Sept. 1989. 52. H.D. Barber, H.B. Lo and J.E. Jones, “Repeated Removal of Thin Layers of Silicon by Anodic Oxidation,” J. Electrochem Soc. 123, 1404–1409, Sept. 1976, and references therein. 53. S. Zwerdling and S. Sheff, “The Growth of Anodic Oxide Films on Germanium,” J. Electrochem Soc. 107, 338–342, April 1960. 54. J.F. Dewald, “The Kinetics and Mechanism of Formation of Anode Films on SingleCrystal InSb,” J. Electrochem Soc. 104, 244–251, April 1957. 55. B. Bayraktaroglu and H.L. Hartnagel, “Anodic Oxides on GaAs: I Anodic Native Oxides on GaAs,” Int. J. Electron. 45, 337–352, Oct. 1978; “II Anodic Al2 O3 and Composite Oxides on GaAs,” Int. J. Electron. 45, 449–463, Nov. 1978; “III Electrical Properties,” Int. J. Electron. 45, 561–571, Dec. 1978; “IV Thin Anodic Oxides on GaAs,” Int. J. Electron. 46, 1–11, Jan. 1979; H. M¨uller, F.H. Eisen and J.W. Mayer, “Anodic Oxidation of GaAs as a Technique to Evaluate Electrical Carrier Concentration Profiles,” J. Electrochem. Soc. 122, 651–655, May 1975. 56. R. Galloni and A. Sardo, “Fully Automatic Apparatus for the Determination of Doping Profiles in Si by Electrical Measurements and Anodic Stripping,” Rev. Sci. Instrum. 54, 369–373, March 1983. 57. L. Bouro and D. Tsoukalas, “Determination of Doping and Mobility Profiles by Automatic Electrical Measurements and Anodic Stripping,” J. Phys. E: Sci. Instrum. 20, 541–544, May 1987.
48
RESISTIVITY
58. T. Clarysse, W. Vandervorst, E.J.H. Collart, and A.J. Murrell, “Electrical Characterization of Ultrashallow Dopant Profiles,” J. Electrochem. Soc. 147, 3569–3574, Sept. 2000. 59. R.G. Mazur and D.H. Dickey, “A Spreading Resistance Technique for Resistivity Measurements in Si,” J. Electrochem Soc. 113, 255–259, March 1966; T. Clarysse, D. Vanhaeren, I. Hoflijk, and W. Vandervorst, “Characterization of Electrically Active Dopant Profiles with the Spreading Resistance Probe,” Mat. Sci. Engineer. R47, 123–206, 2004. 60. M. Pawlik, “Spreading Resistance: A Quantitative Tool for Process Control and Development,” J. Vac. Sci. Technol. B10, 388–396, Jan/Feb. 1992. 61. ASTM Standard F67288, “Standard Method for Measuring Resistivity Profile Perpendicular to the Surface of a Silicon Wafer Using a Spreading Resistance Probe,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 62. R. Holm, Electric Contacts Theory and Application, Springer Verlag, New York, 1967. 63. T. Clarysse, M. Caymax, P. De Wolf, T. Trenkler, W. Vandervorst, J.S. McMurray, J. Kim, and C.C. Williams, J.G. Clark and G. Neubauer, “Epitaxial Staircase Structure for the Calibration of Electrical Characterization Techniques,” J. Vac. Sci. Technol. B16, 394–400, Jan./Feb. 1998. 64. T. Clarysse, P. De Wolf, H. Bender, and W. Vandervorst, “Recent Insights into the Physical Modeling of the Spreading Resistance Point Contact,” J. Vac. Sci. Technol. B14, 358–368, Jan./Feb. 1996. 65. W.B. Vandervorst and H.E. Maes, “Probe Penetration in Spreading Resistance Measurements,” J. Appl. Phys. 56, 1583–1590, Sept. 1984. 66. J.R. Ehrstein, “TwoProbe (Spreading Resistance) Measurements for Evaluation of Semiconductor Materials and Devices,” in Nondestructive Evaluation of Semiconductor Materials and Devices (J.N. Zemel, ed.), Plenum Press, New York, 1979, 1–66. 67. R.G. Mazur and G.A. Gruber, “Dopant Profiling on Thin Layer Silicon Structures with the Spreading Resistance Technique,” Solid State Technol. 24, 64–70, Nov. 1981. 68. W. Vandervorst and T. Clarysse, “Recent Developments in the Interpretation of Spreading Resistance Profiles for VLSITechnology,” J. Electrochem. Soc. 137, 679–683, Feb. 1990; W. Vandervorst and T. Clarysse, “On the Determination of Dopant/Carrier Distributions,” J. Vac. Sci. Technol. B10, 302–315, Jan/Feb. 1992. 69. P.A. Schumann, Jr. and E.E. Gardner, “Application of Multilayer Potential Distribution to Spreading Resistance Correction Factors,” J. Electrochem Soc. 116, 87–91, Jan. 1969. 70. S.C. Choo, M.S. Leong, H.L. Hong, L. Li and L.S. Tan, “Spreading Resistance Calculations by the Use of GaussLaguerre Quadrature,” SolidState Electron. 21, 769–774, May 1978. 71. H.L. Berkowitz and R.A. Lux, “An Efficient Integration Technique for Use in the Multilayer Analysis of Spreading Resistance Profiles,” J. Electrochem Soc. 128, 1137–1141, May 1981. 72. R. Piessens, W.B. Vandervorst and H.E. Maes, “Incorporation of a ResistivityDependent Contact Radius in an Accurate Integration Algorithm for Spreading Resistance Calculations,” J. Electrochem Soc. 130, 468–474, Feb. 1983. 73. R.G. Mazur, “PoissonBased Analysis of Spreading Resistance Profiles,” J. Vac. Sci. Technol. B10, 397–407, Jan/Feb. 1992. 74. A.H. Tong, E.F. Gorey and C.P. Schneider, “Apparatus for the Measurement of Small Angles,” Rev. Sci. Instrum. 43, 320–323, Feb. 1972. 75. W. Vandervorst, T. Clarysse and P. Eyben, “Spreading Resistance Roadmap Towards and Beyond the 70 nm Technology Node,” J. Vac. Sci. Technol. B20, 451–458, Jan./Feb. 2002. 76. J.A. Naber and D.P. Snowden, “Application of Microwave Reflection Technique to the Measurement of Transient and Quiescent Electrical Conductivity of Silicon,” Rev. Sci. Instrum. 40, 1137–1141, Sept. 1969; G.P. Srivastava and A.K. Jain, “Conductivity Measurements of Semiconductors by Microwave Transmission Technique,” Rev. Sci. Instrum. 42, 1793–1796, Dec. 1971.
REFERENCES
49
77. C.A. Bryant and J.B. Gunn, “Noncontact Technique for the Local Measurement of Semiconductor Resistivity,” Rev. Sci. Instrum. 36, 1614–1617, Nov. 1965; N. Miyamoto and J.I. Nishizawa, “Contactless Measurement of Resistivity of Slices of Semiconductor Materials,” Rev. Sci. Instrum. 38, 360–367, March 1967. 78. H.K. Henisch and J. Zucker, “Contactless Method for the Estimation of Resistivity and Lifetime of Semiconductors,” Rev. Sci. Instrum. 27, 409–410, June 1956. 79. J.C. Brice and P. Moore, “Contactless Resistivity Meter for Semiconductors,” J. Sci. Instrum. 38, 307, July 1961. 80. G.L. Miller, D.A.H. Robinson and J.D. Wiley, “Contactless Measurement of Semiconductor Conductivity by Radio FrequencyFree Carrier Power Absorption,” Rev. Sci. Instrum. 47, 799–805, July 1976. 81. W.H. Johnson, “Sheet Resistance Measurements of Interconnect Films,” in Handbook of Silicon Semiconductor Metrology (A.C. Diebold, ed.), Marcel Dekker, New York, 2001, Ch. 11. 82. P.S. Burggraaf, “Resistivity Measurement Systems,” Semicond. Int. 3, 37–44, June 1980. 83. J.L. Kawski and J. Flood, IEEE/SEMI Adv. Man. Conf., 106 (1993); ASTM Standard F153094, “Standard Method for Measuring Flatness, Thickness, and Thickness Variation on Silicon Wafers by Automated Noncontact Scanning,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 84. ADE Flatness Stations Semiconductor Systems Manual. 85. S.M. Sze, Physics of Semiconductor Devices, 2nd ed., Wiley, New York, 1981. 86. W.A. Keenan, C.P. Schneider and C.A. Pillus, “TypeAll System for Determining Semiconductor Conductivity Type,” Solid State Technol. 14, 51–56, March 1971. 87. ASTM Standard F4293, “Standard Test Methods for Conductivity Type of Extrinsic Semiconducting Materials,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 88. S. H´enaux, F. Mondon, F. Gusella, I. Kling, and G. Reimbold, “Doping Measurements in Thin SilicononInsulator Films,” J. Electrochem. Soc. 146, 2737–2743, July 1999. 89. ASTM Standard F72388, “Standard Practice for Conversion Between Resistivity and Dopant Density for BoronDoped and PhosphorusDoped Silicon,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 90. K. Misiakos and D. Tsamakis, “Accurate Measurements of the Silicon Intrinsic Carrier Density from 78 to 340 K,” J. Appl. Phys. 74, 3293–3297, Sept. 1993. 91. T. Trupke, M.A. Green, P. W¨urfel, P.P. Altermatt, A. Wang, J. Zhao, and R. Corkish, “Temperature Dependence of the Radiative Recombination Coefficient of Intrinsic Crystalline Silicon,” J. Appl. Phys. 94, 4930–4937, Oct. 2003. 92. W. Bludau, A. Onton, and W. Heinke, “Temperature Dependence of the Band Gap of Silicon,” J. Appl. Phys. 45, 1846–1848, April 1974. 93. A.B. Sproul and M.A. Green, “Improved Value for the Silicon Intrinsic Carrier Concentration from 275 to 375 K,” J. Appl. Phys. 70, 846–854, July 1991. 94. A. Schenk, “Finitetemperature Full Randomphase Approximation Model of Band Gap Narrowing for Silicon Device Simulation,” J. Appl. Phys. 84, 3684–3695, Oct. 1998; P.P. Altermatt, A. Schenk, F. Geelhaar, and G. Heiser, “Reassessment of the Intrinsic Carrier Density in Crystalline Silicon in View of Bandgap Narrowing,” J. Appl. Phys. 93, 1598–1604, Feb. 2003. 95. D.B. Cuttriss, “Relation Between Surface Concentration and Average Conductivity in Diffused Layers in Germanium,” Bell Syst. Tech. J. 40, 509–521, March 1961. 96. S.M. Sze and J.C. Irvin, “Resistivity, Mobility, and Impurity Levels in GaAs, Ge, and Si at 300 K,” SolidState Electron. 11, 599–602, June 1968.
50
RESISTIVITY
PROBLEMS 1.1
The function y = x n is plotted in Fig. P1.1. Determine n.
y
100
10−1
10−2 101
102
103
104
x
Fig. P1.1
1.2
Determine yo and x1 in the equation y = yo exp((x/x1 ) − 1) plotted in Fig. P1.2. 101 100
y
10−1 10−2 10−3 10−4 10−5
0
0.2
0.4
0.6
0.8
1
x
Fig. P1.2
Plot the log(y) − x data of Fig. P1.3(a) on the x − y figure in Fig. P1.3(b). Write numeric values on the y axis of Fig. P1.3(b). 2 1.5 1
y
log(y)
1.3
0.5 (a) 0
0
0.25
0.5 x
0.75
(b) 1
Fig. P1.3
0
0.25
0.5 x
0.75
1
PROBLEMS
1.4
51
Derive an expression for the resistivity of a semiconductor sample infinite in extent laterally and vertically measured with a square fourpoint probe with the probes spaced a distance s shown in Fig. P1.4. Current I enters probe 1 and leaves probe 4; voltage V is measured between probes 2 and 3. 1
4
2
3
s
Fig. P1.4
1.5
Derive an expression for the resistivity of a semiconductor sample infinite in extent laterally and vertically measured with a fourpoint probe with the probes spaced as shown in Fig. P1.5. Current I enters probe 1 and leaves probe 4; voltage V is measured between probes 2 and 3. 1
2 s
3
4
2s
3s
Fig. P1.5
1.6
Consider an ntype wafer containing small n+ regions. A fourpoint probe is placed on this wafer so that probe 1 of a conventional inline fourpoint probe, is placed on one of those n+ regions. The other three probes are on the nportion of the wafer. In this fourpoint probe, current enters probe 1 and leaves probe 4; the voltage is measured across probes 2 and 3. There are no n+ regions between probes 2 and 4. Is the correct sheet resistance measured in this case?
1.7
The resistance of the semiconductor sample in Fig. P1.7 is measured between the two contacts as a function of wafer thickness t. The results are: t (µm) R ( )
200 318.3
400 623.9
600 929.5
800 1235.1
1000 1540.7
d
ρ
t
Fig. P1.7
Determine the resistivity ρ in · cm and the specific contact resistance ρc in · cm2 for d = 0.01 cm. Assume the current is confined to the area of the contact, shown by the shaded region. The contact is circular with the contact resistance given by Rc = ρc /A, where A is the contact area.
52
1.8
RESISTIVITY
From the I –V curve in Fig. P1.8 determine the conductance g = dI /dV at I = 10−7 A. 10−3 10−4
I (A)
10−5 10−6 10−7 10−8 10−9 10−10 10−11
0
0.1
0.2
0.3
0.4
0.5
V (V)
Fig. P1.8
The resistance R of a semiconductor sample in Fig. P1.9(a) is measured between the two contacts as a function of circular contact of radius r = d/2. R is shown as a function of r and 1/r in P1.9(b) and (c). Derive an expression for the resistance in terms of the resistivity ρ, radius r and thickness t. Neglect contact resistance and assume the current follows the shaded region. Determine the resistivity ρ (in
· cm) for t = 400 µm. d = 2r
ρ
t
(a)
t
104 103 R (Ohms)
1.9
102
(b)
101 100 0.001
0.01
0.1 r (cm)
1
PROBLEMS
53
2400
R (Ohms)
2000 1600 1200
(c)
800 400 0
0
200
400 1/r
Fig. P1.9
600
800
1000
(cm−1) (continued)
1.10 The conducting region in Fig. P1.10 of thickness t = 0.1 µm and resistivity ρ = 0.1 · cm, is deposited on an insulating substrate. L = 1 mm, W = 100 µm. Determine the resistance between contacts A and B.
A
B
W/2
W
L Fig. P1.10
1.11 The semiconductor structure in Fig. P1.11 has thickness t, inside and outside radii r1 and r2 , and resistivity ρ. Determine the resistance R (in ) between the inner ring and the outer ring, i.e., for the doughnutshaped sample, for ρ = 15 · cm, t = 500 µm and r2 /r1 = 100. Current flows radially as indicated by the bold arrows. Hint: R = ρL/A becomes dR = ρdr/A(r).
r1
r2 Fig. P1.11
54
RESISTIVITY
1.12 The sheet resistance is measured in an anodic oxidation experiment. The results are shown in Fig. P1.12. Determine and plot the resistivity, ρ (in · cm), and the carrier density, n (in cm−3 ), versus x for this sample. To determine n(x), use µn = 1180 cm2 /V · s.
Rsh (ohms/square)
107 106 105 104 103 0 × 100
2.5 × 10−5 5 × 10−5 7.5 × 10−5 1 × 10−4 x (cm)
Fig. P1.12
1.13 The semiconductor structure in Fig. P1.13 consists of two films of width W = 20 µm, lengths L1 = 150 µm and L2 = 100 µm, thicknesses t1 = 0.6 µm and t2 = 0.3 µm, and resistivities ρ1 = 10 ohmcm and ρ2 = 1 ohmcm. Determine the sheet resistance of each film (in ohms/square) and the resistance between points A and B (in ohms). The dark regions at points A (not seen) and B are ideal ohmic contacts with zero resistance. The boundary between the two films has zero resistance. L2 W t2
ρ2 B
A
r1 t1
L1
Fig. P1.13
1.14 The resistivity of a semiconductor layer of thickness t varies according to ρ = ρo (1 − kx/t), where k is a constant. L is the sample length, W is the sample width and x is the dimension along the sample thickness. Derive an expression for the sheet resistance of this sample. 1.15 For the ntype layers on a ptype substrate in Fig. P1.15: (a) determine Rsh
PROBLEMS
n
55
p
1016 n (cm−3)
(b)
(a)
(c) 1015 0
10−4
0
x (cm)
Fig. P1.15
(b) calculate and plot: σ versus x (linearlinear plot), ρ versus x (linearlinear plot), Rsh versus x (loglinear plot), and 1/Rsh versus x (loglinear plot) for the three cases. Use µn = 1250 cm2 /V · s. 1.16 An arbitrarily shaped van der Pauw sample of thickness t = 500 µm was measured. The measured resistances were: R12,34 = 74 and R23,41 = 6 . Determine the resistivity and sheet resistance of this sample. 1.17 An arbitrarily shaped van der Pauw sample of thickness t = 350 µm was measured. The measured resistances were: R12,34 = 59 and R23,41 = 11 . Determine the resistivity and sheet resistance of this sample. 1.18 An arbitrarily shaped, uniformly doped van der Pauw sample has a thickness of 500 µm. The measured resistances are R12,34 = 90 and R23,41 = 9 . Determine the resistivity and the sheet resistance of this sample. 1.19 In the cross bridge test structure in Fig. 1.13, consisting of a uniformlydoped layer on an insulating substrate, the following parameters are determined: V34 = 58 mV, I12 = 1 mA, V45 = 1.75 V, I26 = 0.1 mA. An independent measurement has given the resistivity of the film as ρ = 0.0184 · cm and L = 500 µm. Determine the film sheet resistance Rsh (in /square), the film thickness t (in µm), and the line width W (in µm). 1.20 The doping profile ND (x) of an ion implanted layer is given by ND (x) =
φ √
Rp
x − Rp exp −0.5 Rp 2π
2
,
where φ is the implant dose, Rp is the range, and Rp the straggle. Determine the sheet resistance for an arsenic layer implanted (E = 100 keV) into ptype Si ˚ Rp = 204 A, ˚ and doped to NA = 1015 cm−3 . Use φ = 1015 cm−2 , Rp = 577 A, µn = 100 cm2 /V · s. Assume ND (x) = n(x). Hint: First you have to find the junction depth.
56
RESISTIVITY
1.21 The doping profile ND (x) of an ionimplanted layer is given by φ x − Rp 2 , √ exp −0.5 ND (x) = Rp Rp 2π where φ is the implant dose, Rp the range, and Rp the straggle. Determine the sheet resistance for an ntype dopant layer (arsenic) implanted at an energy of 60 keV into ˚ a ptype Si wafer doped to NA = 1016 cm−3 . Use φ = 5 × 1015 cm−2 , Rp = 368 A, ˚ and µn = 50 cm2 /V · s. Assume ND (x) = n(x). Rp = 133 A, Hint: At the junction depth xj : NA = ND . 1.22 (a) In a cross bridge test structure in Fig. 1.13 of a semiconductor layer on an insulating substrate, the following parameters are determined: V34 = 18 mV, I12 = 1 mA, V45 = 1.6 V, I26 = 1 mA. An independent measurement has given the resistivity of the film as ρ = 4 × 10−3 · cm and L = 1 mm. Determine the film sheet resistance Rsh ( /square), the film thickness t (µm), and the line width W (µm). (b) In one particular cross bridge test structure, the leg between contacts V4 and V5 is overetched. For this particular structure V45 = 3.02 V for I26 = 1 mA; it is known that half of the length L has a reduced W , i.e., W ′ , due to a fault during pattern etching. Determine the width W ′ . 1.23 In a cross bridge test structure in Fig. 1.13 consisting of a uniformlydoped layer on an insulating substrate, measurements give: V34 = 58 mV, I12 = 1 mA, V45 = 1.75 V, I26 = 0.1 mA. An independent measurement has given ρ = 1.84 × 10−2 · cm and L = 500 µm. (a) Determine the film sheet resistance Rsh (in /square), the film thickness t (in µm), and the line width W (in µm). It is usually assumed that the sheet resistance Rsh , measured in region A in Fig. P1.23, is the same in the entire structure. Suppose that is not the case. What effect will that have on the line width measurement? (b) Determine the widths W (a) and W (b) in Fig. P1.23 that are calculated if the sheet resistance in the cross hatched region is Rsh1 and in the white region it is Rsh (as determined in (i)), where Rsh = 0.5Rsh1 , but you assumed it was Rsh everywhere. Give your answer as W (a)/W and W (b)/W , where W is the width for uniform sheet resistance.
L
A (a) W/2
L (b) L/2
Fig. P1.23
PROBLEMS
57
1.24 Consider a ptype semiconductor cross bridge test structure on an insulating substrate. The layer, of thickness t, is nonuniformly doped according to NA = 1019 exp(−kx), where k is a constant and x is the dimension along the sample thickness. Determine Rsh , V34 and V45 . Use I12 = I26 = 1 mA, µp = 100 cm2 /V · s, t = 1 µm, k = 105 cm−1 , L = 500 µm, and W = 10 µm. Neglect the electron contribution to the layer resistivity and assume NA = p. 1.25 (a) In the cross bridge test structure in Fig. P1.25, consisting of a uniformly doped layer on an insulating substrate, measurements give: V34 = 11 mV, I12 = 0.5 mA, V45 = 50 mV, I26 = 1 µA. The resistivity of the film is ρ = 5 × 10−3 · cm and L = 100 µm. Determine the film sheet resistance Rsh (in /square), the film thickness t (in µm), and the line width W (in µm). A L 6
1 2
W 5
4
3
Fig. P1.25
(b) It is usually assumed that the resistivity in the “L” region is uniform. Suppose that is not the case. Determine the effective line width Weff if the resistivity in the shaded “L” region varies linearly from 5 × 10−3 · cm at terminal 5 to 10−2 · cm at terminal 4. The resistivity in region “A”, I12 , I26 and the physical width W are the same as in (a). 1.26 A sample with doped regions as shown in Fig. P1.26 is characterized by a spreading resistance probe. The minimum lateral step (along the beveled direction) that the probe can be moved is 2 µm. Determine the maximum bevel angle θ (in degrees) to ensure a minimum of 20 measurement points per doped region?
θ n (0.2 µm) p (0.1 µm) n (0.2 µm)
thick substrate
Fig. P1.26
1.27 Draw the spreading resistance plots, Rsp versus depth, for a p + n and an n+ n junction on the same plot. The nsubstrates are the same and the resistivity of the n+ region is the same that of the p + region. These are qualitative curves, without numerical values.
58
RESISTIVITY
Four Point Probe
0 400 µm x
Fig. P1.28
1.28 Determine the sheet resistance Rsh for a Si wafer of thickness t = 400 µm, shown in Fig. P1.28, for: (a) NA (x) = NA (0) exp(−x/L); ND = 0, i.e., no donors.
(b) NA (x) = NA (0) exp(−x/L); ND = 1016 cm−3 , i.e., uniformly doped with donors. Use p(x) − n(x) − NA (x) + ND (x) = 0, p(x)n(x) = n2i , ni = 1010 cm−3 , NA (0) = 1017 cm−3 , L = 5 µm, µp (x) = 54.3 +
406.9 1+
NA (x) + ND 2.35 × 1017
0.88 ; µn (x) = 92 +
1268 1+
NA (x) + ND 1.3 × 1017
0.91 .
The sheet resistance is measured on the top surface. Assume the pn junction in (b) is an insulating boundary. Neglect the width of the pn junction spacecharge region. Assume that the fourpoint probe spacing s is much larger than the wafer thickness t. 1.29 Consider the sample in Fig. P1.29(a). Give a value for the sheet resistance Rsh . To convert from NA to ρ, use Fig. A1.1. Then positive charge of density 1012 cm−2 is deposited on the upper surface, as in (b), and the charge remains there. This charge sheet does not change the measurement condition, i.e., no surface current flows, but it does change the sample configuration, by causing the player to be partially depleted and this depleted region can be considered an insulating region. Give a value for the new sheet resistance Rsh .
+ + + NA = 1016 cm−3
2 µm
+ + + + + + + NA = 1016 cm−3
Insulator
(a)
(b)
Fig. P1.29
REVIEW QUESTIONS
59
1.30 The hot probe is used to determine the semiconductor type, i.e. ntype or ptype. For the arrangement in Fig. P1.30, determine the conductivity type and draw the band diagram. The sample is uniformly doped and in the dark, i.e., it is not illuminated. +
V
−
Hot
Cold
Fig. P1.30
Hint: The electron current density is Jn = nµn dEF /dx − qnµn Pn dT /dx, where Pn < 0 is the differential thermoelectric power.
REVIEW QUESTIONS • What is the best way to plot power law data?
• What is the best way to plot exponential data?
• Why is a fourpoint probe better than a twopoint probe?
• Why is resistivity inversely proportional to doping density? • What is an important application of wafer mapping?
• What is sheet resistance and why does it have such strange units? • Why is sheet resistance commonly used to describe thin films? • What are van der Pauw measurements?
• What is the main advantage of Eddy current measurements?
• What are advantages and disadvantages of the modulated photoreflectance (therma
wave) technique?
• What is carrier illumination and what material parameters does it provide?
• How is spreading resistance profiling implemented?
• How can conductivity type be determined?
2 CARRIER AND DOPING DENSITY
2.1
INTRODUCTION
The carrier density is related to the resistivity, as shown in Chapter 1. It is, however, usually not derived from resistivity measurements but is measured independently. The carrier density and doping density are frequently assumed to be identical. While that is true for uniformly doped materials, the two may differ substantially for nonuniformly doped materials. We discuss in this chapter methods for determining the carrier and the doping density. Among the electrical methods capacitancevoltage, spreading resistance, and Hall effect techniques are most commonly used. Being currentvoltage or capacitancevoltage techniques, they determine the carrier density. Secondary ion mass spectrometry, an ion beam technique, has also found wide application for measuring the doping density. Optical methods, such as free carrier absorption, infrared spectroscopy, and photoluminescence, are sparingly employed. Infrared spectroscopy and photoluminescence have the advantage of very high sensitivity and the ability to identify the doping impurities.
2.2 2.2.1
CAPACITANCEVOLTAGE (CV) Differential Capacitance
The capacitancevoltage technique relies on the fact that the width of a reversebiased spacecharge region (scr) of a semiconductor junction device depends on the applied voltage. This scr width dependence on voltage lies at the heart of the C –V technique. The C –V profiling method has been used with Schottky barrier diodes using deposited Semiconductor Material and Device Characterization, Third Edition, by Dieter K. Schroder Copyright 2006 John Wiley & Sons, Inc.
61
62
CARRIER AND DOPING DENSITY
NA V v
dW
W ~
(a)
NA, p
p1(x) (V = V) p2(x) (V = V + v) p(x) = 0 0
NA p
dQS W W + dW (b)
x
Fig. 2.1 (a) A reversebiased Schottky diode, and (b) the doping density and majority carrier density profiles in the depletion approximation.
metal, mercury, and liquid electrolyte contacts, pn junctions, MOS capacitors, MOSFETs, and metalairsemiconductor structures. We consider the Schottky barrier diode of Fig. 2.1(a). The semiconductor is ptype with doping density NA . A dc bias V produces a spacecharge region of width W . The differential or small signal capacitance is defined by C=
dQs dQm =− dV dV
(2.1)
where Qm and Qs are the metal and semiconductor charges. The negative sign accounts for negative charge in the semiconductor scr (negatively charged ionized acceptors) for positive voltage on the metal for reverse bias. The capacitance is determined by superimposing a smallamplitude ac voltage v on the dc voltage V . The ac voltage frequency is typically 10 kHz to 1 MHz with 10 to 20 mV amplitude, but other frequencies and other voltages can be used. Let us consider the diode to be biased to dc voltage V plus a sinusoidal ac voltage v. Imagine the ac voltage increasing from zero to a small positive voltage adding a charge increment dQm to the metal contact. The charge increment dQm must be balanced by an equal semiconductor charge increment dQs for overall charge neutrality. The semiconductor charge is given by Qs = qA
0
W
(p − n + ND+ − NA− ) dx ≈ −qA
W
NA dx
(2.2)
0
where the approximation obtains for ND = 0 and p ≈ n ≈ 0 in the depletion approximation. Another assumption is that all acceptors are ionized. For acceptors or donors with energy levels deep within the band gap, the true dopant density profile may not be measured, as discussed further in Section 2.4.6.
CAPACITANCEVOLTAGE (CV)
63
The charge increment dQs in Fig. 2.1(b) comes about through a slight increase in the scr width. From Eqs. (2.1) and (2.2) C=−
d dQs = qA dV dV
0
W
NA dx = qAN A (W )
dW dV
(2.3)
In going from Eq. (2.2) to (2.3), we have neglected the term dNA (W )/dV , assuming NA does not vary over the distance dW , or variations of NA over a distance dW cannot be obtained with the C –V technique. The capacitance in these equations is given in units of F not F/cm2 . The capacitance of a reversebiased junction, when considered as a parallel plate capacitor, is Ks εo A (2.4) C= W Differentiating Eq. (2.4) with respect to voltage and substituting dW/dV into Eq. (2.3) gives 2 C3 NA (W ) = − = (2.5) qKs εo A2 dC/dV qKs εo A2 d(1/C 2 )/dV using the identity d(1/C 2 )/dV = −(2/C 3 ) dC/dV . Note the area dependence in these expressions. Since the area appears as A2 , it is very important that the device area be precisely known for accurate doping profiling. From Eq. (2.4) we find the scr width dependence on capacitance as Ks εo A (2.6) W = C Equations (2.5) and (2.6) are the key equations for doping profiling.1 – 2 The doping density is obtained from the slope dC/dV of a C –V curve or from the slope d(1/C 2 )/dV of a 1/C 2 –V curve. The depth at which the doping density is evaluated is obtained from Eq. (2.6). For a Schottky barrier diode there is no ambiguity in the scr width since it only spreads into the substrate. Spacecharge region spreading into the metal is totally negligible. The doping density profile equations are equally well applicable for asymmetrical pn junctions, i.e., p+ n or n+ p junctions, with one side of the junction more highly doped than the other side. If the doping density of the heavily doped side is 100 or more times higher than that of the lowly doped side, then the scr spreading into the heavily doped region can be neglected, and Eqs. (2.5) and (2.6) hold. If that condition is not met, the equations must be modified or both doping density and depth will be in error.3 The correction, however, is fraught with difficulty. It has been proposed that no unique doping density profile can be derived from C –V measurements under those conditions.4 If the doping density profile of one side of the junction is known, then the profile on the other side can be derived from the measurements.5 Fortunately, most pn junctions for doping density profiling, are of the p + n or n+ p type, and corrections due to doping asymmetries are not necessary. MOS capacitors (MOSC) and MOSFETs can also be used for profiling.6 For an MOSC, the measurement is slightly more complicated because the device must remain in deep depletion during the measurement, ensured with a rapidly varying dc ramp voltage or by using pulsed gate voltages. In the latter case, the gate voltage is pulsed from VG = 0 to VG = VG1 , then from VG = 0 to VG = VG2 , where VG2 > VG1 , etc. The capacitance is measured immediately after the pulse before minority carriers have had time
64
CARRIER AND DOPING DENSITY
to be generated. MOSC doping density profile measurements are influenced by interface traps and minority carrier generation, discussed in more detail in Section 2.4.3. Equation (2.5) applies directly to MOSCs when both interface states and minority carriers can be neglected, but the scr width expression becomes7 – 8 W = Ks εo A
1 1 − C Cox
(2.7)
Equation (2.7) differs from Eq. (2.6) by the oxide capacitance Cox , because part of the gate voltage is dropped across the oxide. The MOSC profiling technique has also been implemented by driving the device into deep depletion and measuring the current instead of the capacitance.9 – 10 The interference of minority carrier generation with differential capacitance profile measurements can be avoided by providing a minority carrier sink, such as a reversebiased pn junction, adjacent to the MOSC. A MOSFET provides such minority carrier collecting junctions. Minority carriers are drained from the channel region of the MOSFET provided the source/drain voltages are equal to or higher than the gate voltage. Since there are no minority carriers in this case, the measurement can be made in steadystate, i.e., no need for pulsed gate voltage. A contactless capacitance and doping profiling version uses a contact held in close proximity to the semiconductor wafer. The sensor electrode, 1 mm diameter and coated with high dielectric strength thin film, is surrounded by an independently biased guard electrode. The sensor electrode is held above the wafer by a porous ceramic air bearing which provides for a very stable distance from the wafer as long as the load on the air bearing does not change, shown in Fig. 2.2. The controlled load is provided by pressurizing a bellows. As air escapes through the porous surface, a cushion of air forms on the wafer that acts like a spring and prevents the porous surface from touching the wafer. The porosity and air pressure are designed such that the disk floats approximately 0.5 µm above the wafer surface. A stainless steel bellows acts to constrain the pressurized air and to raise the porous disk when the air pressure is reduced. If the air pressure fails, the disk moves up, rather than falling down and damaging the wafer.11 To prepare the wafer, it is placed in a lowconcentration ozone environment at a temperature of about 450◦ C, reducing the surface charge on the wafer, especially critical for nSi, makes it more uniform, reduces the surface generation velocity and allows deeper depletion.12 A recent comparison of epitaxial resistivity profiles by the contactless with Hgprobe C –V measurements compared very favorably.13 The capacitance of the air gap is measured by biasing the semiconductor surface in accumulation. Light is used
Pressurized bellows
Porous ceramic
Air Wafer
0.5 µm
Fig. 2.2 Contactless doping profiling arrangement. Pressurized air maintains the electrode at approximately 0.5 µm above the sample surface.
CAPACITANCEVOLTAGE (CV)
65
to collapse any possible spacecharge region due to surface charge while the sensor is lowered and while the air gap modulation due to the electrostatic attraction is determined to eliminate any series spacecharge capacitance. Assuming that the air gap does not vary with changing electrode voltage, the capacitance of the air gap is the measured capacitance at its maximum value. The doping density profile is determined from Eqs. (2.5) and (2.7) with Cox in Eq. (2.7) replaced by Cair . For the derivation of Eq. (2.5) we used the depletion approximation, which neglects minority carriers and assumes total depletion of majority carriers in the spacecharge region to a depth W and perfect charge neutrality beyond W , as illustrated in Fig. 2.1(b). This is a reasonably good approximation when the scr is reverse biased and when the substrate is uniformly doped. Furthermore, we used as the incremental charge variation the acceptor ion density at the edge of the spacecharge region. The ac probe voltage exposes more or less ionized acceptors at the scr edge, as shown in Fig. 2.1. The charges that actually move in response to the ac voltage are the mobile holes, not the acceptor ions. Hence, the differential capacitancevoltage profiling technique determines the carrier density, not the doping density. What is actually measured is an apparent or effective carrier density, which is neither the true carrier density nor the doping density. Fortunately, the apparent density is approximately the majority carrier density and the relevant equations become
p(W ) = −
2 C3 = qKs εo A2 dC/dV qKs εo A2 d(1/C 2 )/dV
W =
W = Ks εo A
Ks εo A C
1 1 − C Cox
(2.8)
(2.9)
(2.10)
The equations for the majority carrier density rather than doping density can be derived from majority carrier currents in diodes14 or from surface potentials in MOS capacitors.15 It is worthwhile to say a few words about the C –V interpretation of Eq. (2.8). Both dC/dV and d(1/C 2 )/dV methods are used, with the d(1/C 2 )/dV the preferred method. We demonstrate this in Fig. 2.3. C –V and 1/C 2 –V curves of a Si pp+ junction are shown in Fig. 2.3(a). It is difficult to tell from the C –V curve whether the doping density of this sample is constant or not. When the C –V curve is converted to a 1/C 2 –V curve, it is immediately obvious that the carrier density is not uniform with a discontinuity at around 3 V. The carrier density profile determined with Eqs. (2.8) and (2.9) is shown in Fig. 2.3(b). The use of the majority carrier density rather than the doping density in the profile equations is an important point and has been the subject of much discussion.16 – 28 We demonstrate the concept for a nonuniform acceptor doping density profile by the heavy curve in Fig. 2.4(a). The majority hole density profile shown by the light line differs from the doping density profile even in thermal equilibrium. Some of the holes diffuse from the highly doped region to the lowly doped region and an equilibrium profile is established as a result of both diffusion and drift. The steeper the doping gradient, the more p and NA
66
CARRIER AND DOPING DENSITY
6 × 1020 1/C2
400
4 × 1020
200
2 × 1020
1/C 2 (F−2)
Capacitance (pF)
600
C 0 −1
1
3
5
7
9
0
Voltage (V) (a)
Carrier Density (cm−3)
1×
1016
8 × 1015 p+
p
6 × 1015 4 × 1015 2 × 1015 0
0
0.5
1 Depth (µm)
1.5
2
(b)
Fig. 2.3
(a) C –V and 1/C 2 –V curves of a Si n+ p diode, (b) p(x)W profile.
NA
NA
p (depl. approx.)
Density
Density
p
p (actual) x (a)
W2 x
W1 (b)
Fig. 2.4 A schematic representation of the doping and majority carrier density profiles of a nonuniformly doped layer. (a) zerobiased junction, (b) reversebiased junction showing the doping density profile, the majority carrier profiles in the depletion approximation and the actual majority carrier profiles for two reversebias voltages.
CAPACITANCEVOLTAGE (CV)
67
differ from one another. The majority carrier density deviation from the doping density is governed by the extrinsic Debye length LD , more generally called the Debye length LD =
kT Ks εo q 2 (p + n)
(2.11)
LD is a measure of the distance over which a charge imbalance is neutralized by majority carriers under steadystate or equilibrium conditions. When a scr forms as a result of a reverse biased Schottky diode, for example, the carrier distribution becomes that in Fig. 2.4(b). We show the majority carrier distribution expected from the depletion approximation for scr widths W1 and W2 , corresponding to two different reversebias voltages. The actual majority carrier distribution is also shown. The two differ appreciably and it is quite obvious from these curves that the doping density profile is not what is measured by differential capacitance profiling. It is also not clear that it is the majority carrier distribution that is measured. It has been shown by detailed computer calculations that what is actually measured is an effective or apparent majority carrier density profile, that is closer to the true majority carrier density profile than to the doping density profile.18 The doping density profile, the majority carrier density profile, and the effective majority carrier density profile are identical for uniformly doped substrates, but not for nonuniformly doped substrates. The Debye length sets a limit to the spatial resolution of the measured profile. This Debye length problem arises because the capacitance is determined by the movement of majority carriers and the majority carrier distribution cannot follow abrupt spatial changes in doping density profiles. Detailed calculations show that if a doping density step occurs within one Debye length, the majority carrier and the apparent densities agree fairly well with one another, but both differ appreciably from the true doping density profile.18 For a more gradual transition, the majority carrier density agrees quite well with the apparent densities with depletion occurring from the lowly doped or from the highly doped side. The agreement with the doping density profile is also quite reasonable. A relationship between the measured majority carrier density and the doping density is16 kT Ks εo d 1 dp(x) (2.12) NA (x) = p(x) − q 2 dx p(x) dx Extensive computer simulations have shown that Eq. (2.12) is too much of a simplification.17 – 18, 26 For lowhigh junctions, e.g., a pp+ junction, the results depend on whether the junction is profiled from the pside or from the p+ side. The simulations show that a step profile cannot be resolved accurately to less than about 2–3LD , with the Debye length determined by the carrier density on the highly doped side of the junction. A doping density ramp profile, for example, cannot be distinguished accurately from a step unless it is appreciably wider than a Debye length. Equations (2.4) to (2.9) are derived in the depletion approximation, which assumes zero mobile carrier density in the spacecharge region. This is a reasonably good approximation for reverse bias. However, for zero or forwardbiased Schottky and pn junctions, the approximation loses its validity, and majority carrier profiling becomes inaccurate. Under forward bias an additional capacitance due to excess minority carrier storage in the quasineutral regions is introduced, rendering the method still less accurate. The concept of a zero or forwardbiased junction does not apply for an MOSC. However, the role of mobile carriers is clearly just as important as it is for junction devices.
68
CARRIER AND DOPING DENSITY
Boron doped 2 × 1016
Density (cm−3)
0 Phosphorus doped 2 × 1016
0 Phosphorus doped 2 × 1016
0 0
0.1
0.2
0.3
W (µ µm)
Fig. 2.5 Doping density profiles for three samples. The solid lines are experimental data. The dashed lines indicate the profiles in the absence of interface states. The dotdash lines show the profiles when the depletion approximation is used. Reprinted with permission after ref. 28.
Neglect of majority carriers has been shown to lead to errors in pulsed MOSC doping density profile determinations for surface potentials below 0.1 V,7, 19, 27 corresponding to a distance of approximately 2–3LD from the SiO2 Si interface. It has been suggested that profiling below this limit is possible by accounting for majority carriers.28 Fairly complex equations are necessary for this correction, but they apply only to uniformly doped substrates. Nevertheless, they are useful, and results of such a modified analysis are shown in Fig. 2.5, where the dashdot lines show the profile under the usual Debye length limitation and the corrected experimental data points show the profile all the way to the surface. Other considerations to be observed during profile measurements are discussed in the ASTM standard F419.29 As with all ASTM methods this is a good source of practical information and precautions to observe during measurement. One more caution: a common technique for the preparation of metalsemiconductor contacts uses chemically etched, hydrogenterminated Si. Hydrogen can diffuse several microns into Si at room temperature and compensate boron acceptors,30 leading to erroneous carrier density profiles. The BH complex dissociates for T ≥ 180◦ C anneals. 2.2.2
Band Offsets
When two semiconductors with different band gaps are joined, the conduction and valence bands cannot both be aligned, as illustrated in Fig. 2.6. Band offsets may exist in the conduction band, Ec , the valence band, Ev , or both. Band offsets can be determined with various techniques. One of the earliest was the infrared absorption method.31 A widely used method is photoemission spectroscopy, where photons incident on a sample eject electrons.32 The electron energy is related to the band gap and band offset and the band offset is measured directly. An electrical technique is based on C –V measurements. It is easiest to determine band offsets on nN or pP isotype heterojunctions. Here the lowercase letters n, p
CAPACITANCEVOLTAGE (CV)
Eg2
Eg1
m2
∆EC
EC EF
Eg1
∆Vpl Cpl
Eg2
∆EV
1/C2
C
V
69
m1 EV
0
xi
−V
x
(b)
(a)
Fig. 2.6 (a) Crosssectional and band diagram of two semiconductors with different band gaps, (b) schematic C –V and 1/C 2 –V plots. Real plots are smeared out and do not exhibit the sharp features shown here.
refer to the narrow band gap, and the upper case letters N, P to the wide band gap semiconductor. Schottky barrier diodes are formed on the structure, as in Fig. 2.6(a). The C –V and 1/C 2 –V curves of such a structure are shown schematically in Fig. 2.6(b). The doping density profiles of the two materials are determined from the slopes m1 and m2 . The plateau capacitance Cpl is related to the thickness of the narrow band semiconductor and the plateau voltage Vpl is related to the band offset. The C –V curve yields an apparent or effective electron density, n∗ , that differs from the true electron density and from the doping density. We follow the theory of Kroemer et al.33 The method was originally shown to be applicable to abrupt junctions, but was later shown to be applicable to graded junctions as well.34 There may be an interfacial charge Qi at the heterointerface, given by ∞ Qi = −q [ND (x) − n∗ (x)] dx (2.13) 0
where ND (x) is the doping density. The conduction band discontinuity is Ec =
q2 Ks εo
0
∞
[ND (x) − n∗ (x)](x − xi ) dx − kT ln
n2 /Nc2 n1 /Nc1
(2.14)
where n1 , n2 are the free electron densities in the layer and the substrate, Nc1 , Nc2 the effective density of states in the conduction band in the layer and the substrate, and xi the location of the heterojunction interface. Knowledge of the position of xi is important. Any error in xi translates into an error in the band offset and it can be determined selfconsistently by comparing the measured apparent carrier density with the calculated carrier density.35 A plot of apparent carrier density of an nGaAs/NAlGaAs heterojunction is shown in Fig. 2.7. The experimental data are shown by the data points. From this plot Qi /q = 2.74 × 1010 cm−2 and Ec = 0.248 eV were extracted. MOS capacitor measurements have also been used to determine band offsets. These measurements rely on a good oxide/semiconductor interface and hence are more applicable to Sibased structures. The technique has been used for determining the band offset of SiGe/Si heterojunctions with the band offset almost entirely in the valence band.36 The
70
CARRIER AND DOPING DENSITY
Doping Density (cm−3)
8 × 1016 6 × 1016 Assumed xi
Assumed ND
4 × 1016 2 × 1016 0
0
0.2
0.4 Depth (µm)
0.6
0.8
Fig. 2.7 Doping density plot of nGaAs/N Al0.3 Ga0.7 As heterojunction; the points are experimental data, the straight line is the assumed donor density. Data adapted from ref. 33.
Accum.
Inv. Ec
1
VT1
10
Ev
VT2
VTS1
VTS2
nSi
110 meV 0.4
80 meV
0.2
VT1
0.6
VTS2
VTS1
8
6
VT2
nSi Si1−yCy C (×10−11 F)
C/Cox
0.8
4 ∆EC = 50 meV
0 −2
−1
0
1
2
2 −3
−2
−1
0
VG (V)
VG (V)
(a)
(b)
1
2
3
Fig. 2.8 (a) Measured (heavy line) and simulated (light lines) Chf –VG curves for Si/Si0.98 C0.013 MOS capacitor (b) Clf –VG characteristics of Si/Si0.7 Ge0.3 MOS capacitor showing threshold voltages and carrier confinement in accumulation and inversion and band diagrams in accumulation and inversion. Data adapted from refs. 37 and 38.
lowfrequency C –V curve exhibits two threshold voltages associated with the SiO2 /Si and the heterojunction interfaces. It also shows a plateau with a width dependent on the band offset. Example MOSC C –VG curves for Si/SiC and Si/SiGe are shown in Fig. 2.8.36 – 37 In both cases, the plateaus due to band offsets are clearly seen. Fig. 2.8(a) shows the highfrequency C –VG offset of the Si/SiC heterojunction.
CAPACITANCEVOLTAGE (CV)
71
The valence band and conduction band alignment of the heterostructure in Fig. 2.8(b) show hole confinement in accumulation and electron confinement in inversion.38 The lowfrequency C –VG characteristic shows the plateaus in accumulation and inversion, due to carrier confinement. The characteristic exhibits two threshold voltages in accumulation VT 1 and VT S1 and two threshold voltages in inversion VT 2 and VT S2 . VT 1 corresponds to hole accumulation at the top strained Si/SiGe heterojunction and VT S1 is related to the Si/SiO2 interface. Similarly, VT 2 and VT S2 correspond to the electron build up in inversion at the SiGe/(buried) strained Si heterojunction and Si/SiO2 interface, respectively. Currentvoltage measurements are generally less reliable for band offset determination. Usually rectification of pn heterojunctions is interpreted for band offset determination. In principle, nN and pP heterojunctions should also show rectification. When they do not, that has been falsely interpreted as no band offset. Deeplevel transient spectroscopy has also been used to determine band offsets.39 Kroemer gives a good discussion and critique of band offset measurements.40 Internal photoemission and corelevel Xray photoemission spectroscopy provide more direct band gap offsets. In internal photoemission (discussed more fully in Section 3.5.4) electrons are excited from the valence and/or conduction band of the narrow band gap semiconductor to the wide band gap semiconductor.41 If the conduction band of the righthand semiconductor is populated by electrons at the interface, then there is a lower photoemission threshold energy which characterizes the conductionband discontinuity Ec . If the narrow band gap semiconductor is ptype, then the valenceband offset Ev is determined. Valence band offsets are most reliably determined from the energy positions of core level lines in Xray photoelectron spectra recorded with bulk samples of the two semiconductors in contact.42 Since the escape depths of the photoelectrons are on the order of 2 nm, one of the two semiconductors must be sufficiently thin. 2.2.3
MaximumMinimum MOSC Capacitance
Equations (2.8) and (2.10) hold for the depletion portion of the equilibrium and the deepdepletion portion of nonequilibrium MOSC C –VG curves but not for strong inversion. The deepdepletion C –VG curve Cdd is shown in Fig. 2.9. A simple method to determine the doping density of an equilibrium MOSC is to measure the maximum highfrequency 200 150 Depletion 100
Chf
C2φF
50
•
Capacitance (pF)
Cox
Cinv Cdd
Deep Depletion 0 −3
−2
−1
0
1
2
3
4
5
Gate Voltage (V) Fig. 2.9 C –VG curve for an SiO2 /Si MOS capacitor. NA = 1017 cm−3 , tox = 10 nm, A = 5 × 10−4 cm2 .
72
CARRIER AND DOPING DENSITY
capacitance of an MOSC in strong accumulation Cox and the minimum highfrequency capacitance in strong inversion Cinv .43 Interface traps play no role in this measurement if the gate voltage is sufficiently high for the device to be in strong inversion. Minority carrier generation does not exist with the device in equilibrium. The maxmin capacitance method yields the average doping density over the scr width with the device in strong inversion. Such a measurement is sufficient for uniformly doped substrates but not accurate for nonuniform doping densities. Information about nonuniformly doped substrates can also be extracted from such equilibrium MOSC C –V curves by linearizing a nonuniformly doped layer on a uniformly doped substrate.44 The measurement requires a knowledge of the substrate doping density and extracts the surface density and layer depth from the measured capacitancevoltage curves by iteration. The maximumminimum capacitance technique relies on the dependence of the scr width of a strongly inverted MOS capacitor on the substrate doping density. The general MOSC capacitance is Cox Cs (2.15) C= Cox + Cs where Cs = Ks εo A/W is the semiconductor capacitance. The capacitance Cinv is the strong inversion or minimum capacitance for which the spacecharge region width is W = Winv =
2Ks εo φs,inv qNA
(2.16a)
where φs,inv is the surface potential in strong inversion. The surface potential φs,inv is frequently approximated by φs,inv ≈ 2φF .45 But φs,inv is actually slightly higher than 2φF , i.e., φs,inv ≈ 2φF + 4kT /q.46 For the approximate case of φs,inv ≈ 2φF = 2(kT /q) ln(NA /ni ) 2Ks εo 2φF W = W2φF = (2.16b) qNA Equations (2.15) and (2.16b) lead to NA =
2 C2φF 4φF 2 qKs εo A (1 − C2φF /Cox )2
(2.17)
where C2φF is indicated on Fig. 2.9. C2φF is, of course, not known for a given C –VG curve. Consequently, Eq. (2.17) is usually given as NA =
2 2 4φF 4φF Cinv R 2 Cox = qKs εo A2 (1 − Cinv /Cox )2 qKs εo A2 (1 − R)2
(2.18)
where R = Cinv /Cox . Cinv and Cox are shown on Fig. 2.9. A small inconsistency in Eq. (2.18) is the use of φs,inv = 2φF in conjunction with Cinv . It should be φs,inv ≈ 2φF + 4kT /q. This is a small error, however. An empirical relationship between Cinv and NA for silicon at room temperature is47 log(NA ) = 30.38759 + 1.68278 log(C1 ) − 0.03177[log(C1 )]2
(2.19)
CAPACITANCEVOLTAGE (CV)
1020
tox = 2 nm
NA, ND (cm−3)
1019
3 nm 5 nm 7.5 nm 10 nm 15 nm 20 nm 30 nm 50 nm 75 nm 100 nm
1018 1017 1016 1015 1014 1013
73
0
0.2
0.4 0.6 Cinv /Cox
0.8
1
1020
NA, ND (cm−3)
1019 1018
125 nm 150 nm 200 nm 300 nm 400 nm 500 nm 700 nm 1000 nm
tox = 100 nm
1017 1016 1015 1014 1013 1012
0
0.2
0.4
0.6
0.8
1
Cinv/Cox Fig. 2.10 Doping density versus Cinv /Cox as a function of oxide thickness for the SiO2 /Si system at T = 300 K.
where “log” is the logarithm to base 10, C1 = RCox /[A(1R)] and the capacitances are in units of F , the area is in units of cm2 , and NA is in units of cm−3 . The equation is identical for ntype substrates with ND substituted for NA . We show in Fig. 2.10 curves calculated from Eq. (2.18), giving the doping density as a function of Cinv /Cox . These curves are useful for a first order estimate of the doping density, but they may hide depthdependent features for spatially varying doping densities. Depthdependent doping density profiles may be measured by gradually immersing the wafer in an etch bath so that the surface becomes a slightly sloped plane along which the impurity gradient is gradually changing. MOS capacitors formed on the etched and oxidized surface can be used to determine the doping density under each MOSC as determined from its Cinv /Cox ratio.48 The doping density of a polySi gate can be determined by the Cinv /Cmax method using the connection of Fig. 2.11(a).49 With source, drain, and substrate connected together and a gate voltage above the threshold voltage, the source/drain/substrate form one continuous nlayer, representing the “gate” of the MOS capacitor. The “substrate” of this capacitor
74
CARRIER AND DOPING DENSITY
VG PolySi Gate
n+
n+
pType
(a) 1
C/Cox
0.9
0.8
0.7 −5
0
5 10 Gate Voltage (V)
15
(b)
Fig. 2.11 (a) MOSFET connection to determine the doping density of the gate, (b) resulting C –V curve calculated, ND = 5 × 1019 cm−3 , tox = 10 nm.
is the polySi gate shown as depleted in Fig. 2.11(a). The resulting C –VG curve has the shape of Fig. 2.11(b). Although Cinv is not much lower than Cox , it is, nevertheless, possible to extract the doping density using Fig. 2.10. However, it takes a significant gate voltage to invert the gate and the gate oxide may break down before inversion is reached. In that case one could match the depletion part of the C –VG curve with theory to extract ND .
Exercise 2.1 Problem: For a ptype Si MOS capacitor, Cinv /Cox = 0.22 and tox = 15 nm. (a) Determine the doping density for this device using Kox = 3.9, Ks = 11.7, ni = 1010 cm−3 , A = 5 × 10−4 cm2 , and T = 27◦ C. (b) Determine Cinv /Cox when NA = 5 × 1015 cm−3 . Use the approach that leads to Eq. (2.18) for this problem. (c) Use Eq. (2.19) to determine NA instead of Eq. (2.18).
CAPACITANCEVOLTAGE (CV)
Solution: NA =
75
2 2 4φF 4φF Cinv R 2 Cox = qKs εo A2 (1 − Cinv /Cox )2 qKs εo A2 (1 − R)2
(a) With R = 0.22, Kox = 3.9 and tox = 15 nm, we find Cox = 1.15 × 10−10 F and Cinv = 2.53 × 10−11 F. Solving the above equation gives: NA = 4 × 1016 cm−3 (b) for NA = 5 × 1015 cm−3 : Cinv /Cox = 0.097 (c) Using Eq. (2.19): NA = 4.48 × 1016 cm−3 Note the 10% difference between NA determined with Eqs. (2.18) and (2.19)
2.2.4
Integral Capacitance
The differential capacitance technique has some limitations when used as a process monitor where accuracy and measurement time are important.50 In particular, the required differentiation often results in noisy profiles. The integral capacitance technique is based on integrating a portion of the pulsed MOSC C –V curve to obtain a partial implant dose P. , with the partial dose proportional to the implanted dose. The chosen dose includes the doping density between x = x1 and x = x2 and contains most of the implanted layer, but does not extend into the region where the doping density equals the uniform background doping density nor into the region within 2 to 3 Debye lengths from the surface. The partial dose is given by50 P =
x2
x1
NA (x) dx =
1 qA
V2
C dV
(2.20)
V1
Note the linear dependence on device area rather than the square dependence of the C –V method. The second parameter that is measured is related to the projected range R or implant depth at the density peak. It is defined by50 x2 Ks εo 1 xNA (x) dx = (V2 − V1 ) + (1 − Ks /Kox )tox (2.21) R = tox + P x 1 qP This expression for R incorporates P with only one integration. The repeatability of this technique for a given device was accurate to 0.1%, and the authors claim that the repeatability in partial dose measurement has been improved by over a factor of ten by going to the integral capacitance technique.50 A different MOS capacitor integral approach gives the implanted dose.51 Example C –VG curves for various implant doses are shown in Fig. 2.12(a). The doping density profiles (symbols) in Fig. 2.12(b) are extracted from measured deep depletion CVcurves using the method of Fig. 2.5. The solid lines represent the simulated implanted doping densities. The deviation of the two profiles illustrates that the simple integration of the C –VG profile does not yield the true doping densities. The proposed technique relies on measuring the deepdepletion MOS capacitor C –VG curve. The depleted majority carrier charge at a certain spacecharge region width is determined from the value of the majority carrier charge in strong accumulation and the corresponding change of majority carrier charge Q when the MOSC is driven into deep depletion. Q is obtained by integrating the deep depletion C –VG curve. A second approach is measuring the depletion C –VG curves of the implanted sample and a reference sample. The implant dose is obtained
76
CARRIER AND DOPING DENSITY
7 × 10−7 1012 cm−2
C (F/cm2)
6 × 10−7 5×
10−7
8 × 1011
4×
10−7
6 × 1011
3 × 10−7
4 × 1011
2 × 10−7
2 × 1011
Bulk
1 × 10−7 0 −2
−1.5 −1 −0.5 Gate Voltage (V)
0
(a)
Doping Density (cm−3)
2.5 × 1017 1012 × cm−2 2 × 1017
8 × 1011
17
1.5 × 10
6 × 1011
17
1 × 10
4 × 1011 2 × 1011
5 × 1016 0 0
20
40
60
80
100
Depth (nm) (b)
Fig. 2.12 (a) Deep depletion C –VG curves as a function of boron ion implant dose at 40 keV into pSi substrates, tox = 4.1 nm, (b) doping profiles determined by conventional C –V profiling (symbols) and simulation (lines). The “bulk” curve in (a) is for the unimplanted substrate. After ref. 51.
from the difference charge Q by integrating the two C –VG curves starting at the same accumulation capacitances to the same deepdepletion capacitance. 2.2.5
Mercury Probe Contacts
Capacitance profiling requires junction devices. At times it is desirable to use a device whose junction can be fabricated without subjecting the material to high temperature treatments. Conventional Schottky barrier device fabrication is done near room temperature, but a metal must be deposited on the wafer. When a temporary contact is needed, as in evaluating epitaxial layers for example, a mercury probe is frequently used, where mercury contacts the sample through a welldefined orifice. Mercury probes can make contact either to the sample bottom or to the top. The contact area is sufficiently well defined to be useful for profile measurements. A mercury probe with a probe diameter as small as 7 µm has been used for C –V measurements, allowing lateral capacitance profiles by continuously dragging the probe across the wafer.52 The mercury contact does not damage the wafer nor leave mercury on the surface.53 The semiconductor surface should be treated before the Hg contacts the surface for reproducible measurements. Current leakage and junction breakdown of the mercury Schottky
CAPACITANCEVOLTAGE (CV)
77
contact, usually at its edge, are the most important limiting factors for accurate doping profiling. To minimize current leakage and maximize junction breakdown voltage, a thin oxide layer is usually grown on nSi surfaces by dipping the wafers in hot nitric acid or hot sulphuric acid. This oxide is about 3 nm thick. Dip pSi wafers in HF for 30 s, rinse in flowing DI water and dry the wafer,53 giving an oxidefree surface which is desirable for most reproducible results. The mercury should be very pure, so periodic mercury changes are recommended. It is also helpful to reduce the junction leakage by applying a wetting agent, e.g., Kodak PhotoFlo, on the wafer surface to reduce moisture accumulation, before making the mercury contact. 2.2.6
Electrochemical C –V Profiler (ECV)
The electrochemical capacitancevoltage profiling technique is based on the measurement of the capacitance of an electrolytesemiconductor Schottky contact at a constant dc bias voltage. Depth profiling is achieved by electrolytically etching the semiconductor between capacitance measurements with no depth limitation. However, the method is destructive because it etches a hole into the sample. Early measurements divided the measurement and etch processes; later they were combined into one operation.54 The present technique uses a combined process in which both etching and measurement are performed with the same apparatus. An excellent review is given by Blood.55 The electrochemical method is schematically shown in Fig. 2.13. The semiconductor wafer is pressed against a sealing ring in the electrochemical cell containing an electrolyte. The ring opening defines the contact area by means of springloaded back contacts pressing the wafer against the sealing ring. The etching and measuring conditions are controlled by the potential across the cell by passing a dc current between the semiconductor and the carbon electrode to maintain the required overpotential measured with respect to the saturated calomel electrode. To reduce series resistance, the ac voltages are measured with a platinum electrode located near the sample. With a small reverse dc bias applied between the electrolyte and the semiconductor, two lowvoltage signals of different frequencies are applied to the electrolyte. The carrier density measurement is based on Eq. (2.8) or on the relationship p(W ) =
2Ks εo V q (W )2
I V ac
Pump
C
(2.22)
Sealing Ring
Pt
Illumination Window
Sample Electrolyte Back Contact
Fig. 2.13 Schematic diagram of the electrochemical cell showing the Pt, saturated calomel and carbon electrodes and the pump to agitate the electrolyte and disperse bubbles on the semiconductor surface. Reprinted with permission after Blood.55
78
CARRIER AND DOPING DENSITY
where V is the modulation component of the applied ac voltage (typically 100–300 mV at 30–40 Hz) and (W )2 is the resulting scr width modulation. W is determined by measuring the imaginary component of the current with a phasesensitive amplifier using typically a 50 mV, 1–5 kHz signal and Eq. (2.9). W and p(W ) are obtained through appropriate electronic circuits.54 The 1–5 kHz frequency is significantly lower than the 0.1–1 MHz frequency typically used for conventional differential capacitance profiling to reduce the rs C time constant, where rs is the series resistance of the electrolyte and C the device capacitance. The resistancecapacitance product must meet certain criteria for the measurements to be valid as discussed in Section 2.4.2 on Series Resistance. ECV profiling is more sensitive to deep traps due to the low frequencies, but for most materials this is rarely a problem. Equations (2.9) and (2.22) provide the density at depth W . Depth profiling is achieved by dissolving the semiconductor electrolytically, which depends on the presence of holes. For ptype semiconductors, holes are plentiful and dissolution is readily achieved by forward biasing the electrolytesemiconductor junction. For ntype material, holes are generated by illuminating and reverse biasing the junction. The depth WR depends on the dissolution current Idis according to the relationship54 t M Idis dt (2.23) WR = zFρA 0 where M is the semiconductor molecular weight, z the dissolution valency (number of charge carriers required to dissolve one semiconductor atom), F the Faraday constant (9.64 × 104 C), ρ the semiconductor density, and A the contact area. WR is determined by integrating the dissolution current electronically. The measurement depth of the carrier density is (2.24) x = W + WR A key advantage of ECV over conventional C –V profiling is the unlimited profile depth, since the semiconductor can be etched to any desirable depth. The electrolyte must be chosen appropriately for each semiconductor and suitable electrolytes are for InP: 0.5 M HCl in H2 O,56 Pear etch (37% HCl:70% HNO3 :methanol (36:24:1000)),57 FAP (48% HF:99% CH3 COOH:30% H2 O2 :H2 O (5:1:0.5:100)), and UNIEL A:B:C (1:4:1) where A:48% HF:99% CH3 COOH:85% oH3 PO4 :H2 O (5:1:2:100), B: 0.1 M Nnbutylpyridinium chloride (C9 H14 ClN), C: 1 M NH3 F2 ; for GaAs Tiron (1,2dihydroxybenzene3.5disulfonic acid disodium salt C6 H2 (OH)2 (SO3 Na)2 · H2 O),58 EDTA (Na2 · EDTA (0.1 M) basified with ethylenediamine to pH of 9.1,55, 59 UNIEL, and ammonium tartrate ((NH4 )2 C4 O6 , FW184.15, basified with NH4 OH to pH of 11.5 or higher); for Si NaF/H2 SO4 and 0.1 M NH4 HF2 .60 – 62 One of the most successful electrolytes for GaAs:AlGaAs and InP based alloys is Na2 EDTA (0.1 M) basified with ethylenediamine to pH 9–10.63 The chemical nature of the electrolyte determines the quality of the etch well and the tendency to avoid film formation, both of which affect the carrier density. The technique is eminently suitable for III–V materials because the dissolution valency, z = 6, is well defined and the electrolyte etches the semiconductor very controllably. The dissolution valency is not well defined for Si where it can vary between 2 and 5, affected by electrolyte concentration, dopant type and density, electrode potential, and illumination intensity. Furthermore hydrogen bubbles generated during the dissolution process hinder the uniformity and degrade the depth resolution. The hydrogen bubble problem is overcome by using a pulsed jet of the electrolyte.61 – 62 Electrochemical profiling of silicon
79
CURRENTVOLTAGE (IV)
1020
1022
Density (cm−3)
Density (cm−3)
1021
SIMS
1019 ECV
1018
1017
1016
1015
SIMS
1020 1019
ECV
1018 1017
0
0.5
1 1.5 Depth (µm)
2
2.5
1016
(a)
0
0.050
1
0.15
Depth (µm) (b)
Fig. 2.14 Profiles obtained with the ECV profiler and with SIMS. (a) p+ (B)/p(B) Si and (b) n+ (As)/p(B) Si. Reprinted after Peiner et al., Ref. 64 by permission of the publisher, the Electrochemical Society, Inc.
has in the past been limited to thin layers. However, 0.1M NH4 HF2 with one drop of Triton X100 added to 100 ml of solution electrolyte, for which z = 3.7 ± 0.1, gives good results for Si. Example density profiles are shown in Fig. 2.14. The etch rate is typically a few microns/hour and depths to 20 µm are readily obtained in III–V materials. The etch rate for Si is on the order of 1 µm/hr. The accuracy and reproducibility of ECS profiling is discussed in detail.65 The cell and sample preparation are the greatest source of error with the most likely causes for variability being the condition of the sealing ring, the difference in the way the sample is mounted and the way trapped air bubbles are cleared from the sample surface. The ring areas should be measured at least three times a week. Ideally, the area of the etch well at the end of each run should be measured and inspected for signs of sealing ring wear or damage and for nonuniform etching, due to bubbles, etc. Sealing rings typically last for 150 measurements, with the wetted area getting progressively larger. Problems may arise due to highly doped surface layers, high contact resistance or poor etching. A highlydoped surface layer, particularly for ntype material, creates difficulties for measuring underlying lowly doped layers, due to seepage at the edge of the ring. Complications arise if the sample exhibits significant parallel conduction, as the device can no longer be modeled by a simple twoelement series or parallel model. The presence of crystalline defects in the sample can also lead to uneven etching. 2.3 2.3.1
CURRENTVOLTAGE (IV) MOSFET Substrate Voltage—Gate Voltage
Differential capacitance profile measurements are typically made at frequencies of 0.1–1 MHz on largediameter devices to reduce stray capacitances and increase the
80
CARRIER AND DOPING DENSITY
signal/noise ratio. These constraints make measurements on smallgeometry MOSFETs difficult because the capacitance is extremely small. To overcome this limitation, several methods have been developed allowing the doping density profile to be extracted from MOSFET currentvoltage measurements. In the MOSFET substrate voltagegate voltage method the MOSFET is biased in its linear region by a low drainsource voltage VDS and an appropriate gatesource voltage VGS . A sourcesubstrate or body potential VSB forces the spacecharge region under the gate to extend into the substrate, allowing the doping density profile to be obtained. The inversion charge density is held constant, approximated by a constant drain current, by adjusting VGS whenever VSB is changed. The relevant equations are66 – 67 p(W ) = W =
Kox εo d 2 VSB 2 dV 2 qKs tox GS
(2.25)
Ks εo dVSB Cox dVGS
(2.26)
A feedback circuit to implement this technique is shown in Fig. 2.15(a). VDS is held constant, VGS is varied, and a constant current I1 is applied between the input terminals of the operational amplifier connected between the source (S) and ground. With the operational amplifier differential input voltage and input current nearly zero, current I1 is forced through the MOSFET and the drain current is ID = I1 . When VGS is changed, the op amp adjusts its output voltage, i.e., the voltage VSB between the source and substrate (B), to maintain ID = I1 .68 A modified version of this technique, where the restriction to slowly varying doping density profiles is overcome by approximating the substrate doping density as a simple analytic function, has been proposed.69 The assumption that constant drain current corresponds to constant inversion charge is only true to a first approximation. It is known that in a MOSFET the effective mobility varies with gate voltage (see Chapter 8), requiring a correction in the analysis.67, 70 However, for the commonly used mobility expression µeff = µo /[1 + θ (VGS − VT )], the mobility dependence on gate voltage does not affect the profile.71 The drainsource voltage should be maintained below about 100 mV to ensure linear MOSFET operation, and the profile is affected by shortchannel effects.67, 72
VDS
VDS ID
ID VSB
B
VGS S
I1
S − +
VBS VT (a)
− +
I1
(b)
Fig. 2.15 Operational amplifier circuit for (a) the MOSFET substrate/gate voltage method, (b) the MOSFET threshold voltage method.
81
CURRENTVOLTAGE (IV)
2.3.2
MOSFET Threshold Voltage
In the MOSFET threshold voltage profiling technique, the threshold voltage is measured as a function of substrate bias.73 – 75 The threshold voltage of a MOSFET is VT = VF B + 2φF +
√
2qKs εo NA (2φF + VSB ) = VF B + 2φF + γ 2φF + VSB (2.27) Cox
where γ = (2qKs εo NA )1/2 /Cox and the substrate bias VSB = VS − VB is positive for nchannel devices. The doping density profile is obtained by measuring VT as a function of VSB , plotting VT against (2φF + VSB )1/2 and measuring the slope γ = dVT /d(2φF + VSB )1/2 of this plot. The doping density is from Eq. (2.27) NA =
2 γ 2 Cox 2qKs εo
(2.28)
assuming we can neglect variations of d(2φF )/d(2φF + VSB )1/2 . The profile depth is W =
2Ks εo (2φF + VSB ) qNA
(2.29)
In Eq. (2.28) φF depends on NA [φF = (kT /q) ln(NA /ni )], but NA is not known a priori. A suitable approach is to plot VT versus (2φF + VSB )1/2 using 2φF = 0.6 V. Then take the slope and find NA . With this value of NA find a new φF , replot VT versus (2φF + VSB )1/2 , repeating the procedure until a profile is obtained. One or two iterations usually suffice. In Fig. 2.16 we show doping density profiles obtained from MOSFET threshold voltage, spreading resistance, and pulsed MOSC C –VG measurements. The pulsed MOSC measurements were made on a test MOSC structure processed identically to the MOSFET. The data are compared to a SUPREM3 calculated profile. The threshold voltage technique can also be used for depletionmode devices.74 – 75 The threshold voltage is measured as a function of substrate bias with the circuit in Fig. 2.15(b). This method is discussed in more detail in Chapter 4 Section 4.8, as the
1 × 1017
Density (cm−3)
8 × 1016 6 × 1016 4 × 1016 2×
SUPREM3 Pulsed MOSC SRP VT
1016 0
0
0.1
0.2 0.3 Depth (µm)
0.4
0.5
Fig. 2.16 Dopant density profiles determined by MOSFET threshold voltage, SRP, pulsed C –V , and SUPREM3. Reprinted after ref. 73 by permission of IEEE ( 1991, IEEE).
82
CARRIER AND DOPING DENSITY
constant drain current method. The current I1 is chosen as typically I1 ≈ 1 µA. The output of the op amp gives the threshold voltage directly. 2.3.3
Spreading Resistance
Spreading resistance profiling is commonly used for Si. The sample is beveled, and two spreading resistance probes are stepped along the beveled surface. The spreading resistance is measured as a function of sample depth, and the doping density profile is calculated from the measured resistance profile. This technique is discussed in Section 1.4.2. Very high resolution profiles can be generated by using shallow bevel angles. An application of SRP to very thin MBE Si layers is given by Jorke and Herzog, who also discuss carrier spilling and lowhigh and highlow transitions.76 2.4
MEASUREMENT ERRORS AND PRECAUTIONS
Many C –V measurements are made with no corrections of any kind because such corrections often only produce small changes in the measured doping density profile. Sometimes corrections are not made because the experimenter is unaware of possible corrections or they are too difficult to make. Nevertheless, one should be aware of possible measurement errors and means of correcting them. 2.4.1
Debye Length and Voltage Breakdown
The Debye length limitation is discussed in Section 2.2.1 and in numerous papers.14 – 28, 77 To summarize briefly, mobile majority carriers do not follow the profile of the dopant atoms if the dopant density profile varies spatially over distances less than the Debye length. The majority carriers are more smeared out than the dopant atoms and a measured profile of steep dopant gradients (abrupt highlow junctions and steepgradient ion implanted samples) will result in neither the doping nor the majority carrier density profile. Instead an effective or apparent carrier density profile is obtained, which is closer to the majority carrier density profile than to the doping density profile. It is possible to correct the measured profile by iterative calculations,23 but due to the mathematical complexity this is rarely done. Another consequence of the Debye length limitation is the inability to profile closer than about 3LD from the surface using MOS devices. Although corrections are possible to calculate the profile to the surface, this is not routinely done. Even considering the Debye length limitation, it is possible to profile closer to the surface with MOSCs and MOSFETs than it is with Schottky barrier diodes or pn junctions. For MOS devices the limit is approximately 3LD , for Schottky diodes it is approximately the zerobias scr width W0V , and for pn junctions it is the junction depth plus the zerobias scr width. The 3LD limit is shown as the lower profile depth limit in Fig. 2.17. For degenerately doped semiconductors the resolution is limited by the ThomasFermi screening length LTF rather than the Debye length.78 LTF is given by 1/6 π πKs εo h ¯2 LTF = (2.30) 2 ∗ 3(p + n) q m where h ¯ is Planck’s constant and m∗ is the effective mass. For semiconductors with quantum confinement, i.e., δdoped semiconductors as well as compositional quantum
MEASUREMENT ERRORS AND PRECAUTIONS
83
103
Distance (µm)
102 101
WBD W0V
100 10−1
3LD
10−2 10−3 1013 1014
1015 1016 1017 1018 1019 1020 NA, ND (cm−3)
Fig. 2.17 Spatial profiling limits. The “3 LD ” line is the lower limit for conventional MOSC profiling, the zero bias “W0V ” line is the lower limit for pn and Schottky diode profiling, and the “WBD ” line is the upper profile limit governed by bulk breakdown.
wells, the resolution is limited by the spatial extent of the ground state wave function given by78 1/3 7 4Ks εo h ¯2 (2.31) Lδ = 2 5 9q 2 N 2D m∗ where N 2D is the twodimensional doping density in units of cm−2 , for example. This equation shows the resolution of high effective mass materials to be better than for low m∗ materials. For example, the resolution for pGaAs is better than that for nGaAs. When the profile is generated by sweeping a reversebias voltage, the upper profile depth limit is determined by semiconductor breakdown. The spacecharge region obviously no longer increases beyond breakdown. The breakdown limit is also shown on Fig. 2.17 as WBD . Breakdown considerations do not apply to the electrochemical profiler. A theoretical study incorporating Debye length and breakdown limitation as well as majority carrier diffusion in steepgradient profiles gives the dose and energy limits of Si and GaAs ionimplanted layers that can be profiled by the differential capacitance technique.26 2.4.2
Series Resistance
A pn or Schottky diode consists of a junction capacitance C, a junction conductance G, and a series resistance rs , as shown in Fig. 2.18(a). The conductance governs the junction leakage current and depends on processing conditions. The series resistance depends on the bulk wafer resistivity and on the contact resistances. Capacitance meters assume the device to be represented by either the parallel equivalent circuit in Fig. 2.18(b) or the series equivalent circuit in Fig. 2.18(c). Comparing the two circuits to the original Fig. 2.18(a) circuit, allows CP , GP , CS , and RS to be written as (see Appendix 2.2)79 C G(1 + rs G) + rs (ωC)2 ; G = P (1 + rs G)2 + (ωrs C)2 (1 + rs G)2 + (ωrs C)2 1 CS = C[1 + (G/ωC)2 ]; RS = rs + G[1 + (ωC/G)2 ]
CP =
(2.32) (2.33)
84
CARRIER AND DOPING DENSITY
G
GP
C
CP
CS
RS rs
(a)
(c)
(b)
Fig. 2.18 (a) Actual circuit, (b) parallel equivalent circuit, and (c) series equivalent circuit for a pn or Schottky diode.
200
Capacitance (pF)
CS rs = 100−2000 Ω
150
100
50
100 Ω 500 Ω 1000 Ω
CP
rs = 2000 Ω 0 10−7
Fig. 2.19
10−6
10−5 10−4 Conductance (S)
10−3
10−2
CS and CP versus G as a function of rs . C = 100 pF, f = 1 MHz.
where ω = 2πf . To determine C from series connected measurements at two different frequencies, CS in Eq. (2.33) can be written as C=
ω22 CS2 − ω12 CS1 ω22 − ω12
(2.34)
where CS1 and CS2 are the measured capacitances at frequencies ω1 and ω2 , respectively. The capacitances CP and CS are plotted in Fig. 2.19. CS is independent of the series resistance rs , whereas CP depends strongly on rs . Both capacitances deviate from C at high G. With the quality factor Q for a parallel circuit defined by Q = ωC/G, we find the true capacitance to be measured for Q ≥ 5. Figure 2.19 clearly shows that for junction devices with Q ≥ 5, the series equivalent circuit is the one to use for capacitance measurements if series resistance is suspected. A real device may have series resistance and capacitance as parasitic elements, shown in Fig. 2.20. This is the case if the back contact is an evaporated metal contact without ohmic contact formation. For example, if a metal is deposited on the wafer front to form a Schottky diode for C –V measurements, the same metal deposited on the wafer back also
MEASUREMENT ERRORS AND PRECAUTIONS
+V
+V
+V
Insulator
pType
pType
85
pType
n+
Insulator
n+ Insulator
pType
pType
Cox
G
C
rs
G
C
Ideal device
C
rs
rs
Cb
Cb (a)
G
(b)
Cb (c)
Fig. 2.20 Equivalent circuits with series resistance and capacitance for (a) front and rear Schottky contacts, (b) front Schottky and rear oxide contact, and (c) front and rear oxide contacts. The elements within the rectangles represent the intrinsic device.
forms a Schottky diode, as in Fig. 2.20(a). Fortunately, the back contact usually has much higher capacitance because it has larger area than the front contact and the back Schottky diode is forward biased when the front Schottky diode is reverse biased. Having two backtoback Schottky diodes allows the necessary current to flow to bias the front diode. If the back contact consists of an insulator, as in 2.20(b), the front Schottky or pn diode is always zero biased, since there is no dc current flow. Hence this configuration does not work for dc doping profiling. On the other hand, the arrangement in 2.20(c), consisting of MOS contacts on the front and the back will work, since MOS C –V measurements do not require dc current to flow. One of the problems with the configuration in 2.20(a) is the voltage distribution between front and back contacts. Although most of the applied voltage drops across the front reversebiased junction, a portion drops across the back forwardbiased rear junction. The measured voltage is, of course, the total voltage. The effect of this is illustrated in Fig. 2.21,80 showing 1/C 2 –V plots of an nSi wafer with front and back Schottky and with front Schottky and back ohmic contacts. An interesting feature is the negative voltage intercept, attributed to the distribution of the applied bias voltage between the front and the back contact diodes for small voltages. Since 1/C 2 –V curves are also used to determine the junction builtin potential Vbi , this curve will obviously yield an incorrect Vbi . To determine the correct builtin potential the curve must be shifted to the right. The 1/C 2 –V curve becomes “normal” when the back Schottky contact is a sintered Au/Sb ohmic contact.
86
CARRIER AND DOPING DENSITY
5 × 1020
1/C 2 (F−2)
4 × 1020
Ohmic back contact
3 × 1020 2 × 1020 Schottky back contact
1 × 1020 0 −20
−16
−12
−8 Voltage (V)
−4
0
Fig. 2.21 1/C 2 versus voltage curves for nSi wafers with A = 3.14 × 10−2 cm2 , t = 640 µm, ND ∼ 5 × 1014 cm−3 . Curve (a): front and back Al Schottky contacts, (b): front Au/Pd Schottky and back Au/Sb ohmic contacts. After Mallik et al., ref. 80.
Care must be exercised when preparing samples for capacitance measurements, especially if the device is at the wafer stage and measurements are made on a probe station. If the wafer is provided with a metallic back contact, there is usually no problem, provided the wafer resistivity itself does not contribute significant series resistance. However, wafers placed on a probe station without any back metallization can have appreciable contact resistance. This can be checked by reducing the measurement frequency. If CP increases it is likely a series resistance problem. Measurement of CS does not have this problem. It is important that a vacuum be pulled for all probe capacitive measurements to reduce the resistance between the wafer and the probe chuck. If an MOS device, e.g., MOS capacitor or MOSFET is measured, and if the back contact resistance is a problem, it may be advantageous to leave the oxide on the back surface and place the wafer on the probe station making a largearea capacitive back contact (Fig. 2.20(c)). The contact capacitance Cb , much larger than the device capacitance because its area is usually the area of the entire sample, approximates a short circuit. Series resistance also interferes with dopant profile measurements. For a wafer with negligible series resistance, there is zero phase shift between the rf voltage applied to the device and the rf current flowing through it when the conductance is measured. For the capacitance measurement there is a 90◦ phase shift, which is the basis of phasesensitive capacitance measurements. When series resistance is not negligible, an additional phase shift φ is introduced into the measurement. This must be taken into account or the measured dopant profile determined from Eqs. (2.5) and (2.6) will be in error.81 An approximate way to consider series resistance is from Eqs. (2.5a), (2.6) and (2.32) with rs G ≪ 1. It can be shown that the measured density, NA,meas (W ), and depth, Wmeas , are related to NA and W by the relationships NA,meas =
NA 1 − (ωrs C)4
Wmeas = W [1 + (ωrs C)2 ] Clearly, both density and depth increase with series resistance.
(2.35) (2.36)
MEASUREMENT ERRORS AND PRECAUTIONS
87
Exercise 2.2 Problem: The parallel circuit (Fig. 2.18(b)) CP –V curve of an n+ p junction, measured at a frequency of 1 MHz, is shown in Fig. E2.1. It is suspected that series resistance is significant in this device. An additional measurement at f = 10 kHz and lower frequencies confirmed this because C(10 kHz) = 200 pF at zero volts. The effect of series resistance is negligible at 10 kHz. A = 4.25 × 10−3 cm2 . Determine the series resistance rs and the carrier density profile. The conductance G of this device is negligibly small. Solution: Solving Eq. (2.32) for rs , neglecting the rs G term, gives rs = (1/ωC) √ C/CP − 1. With CP = 94 pF and C = 200 pF, we find rs= 845 . 1 − 1 − 4(ωrs CP )2 Now solving Eq. (2.32) for C gives C = 2CP (ωrs )2 Substituting rs = 845 and the CP from Fig. E2.1, gives the plot in Fig. E2.2(a). Replotting as 1/C 2 is also shown as is the slope d(1/C 2 )/dV in Fig. E2.2(b). From 100
CP (pF)
90 80 70 60 f = 1 MHz 50
0
5
10
15
10
15
Voltage (V)
Fig. E2.1
CP, C (pF)
150
C
100 CP
f = 1 MHz 50
0
5 Voltage (V) (a)
Fig. E2.2
88
CARRIER AND DOPING DENSITY
3 × 1020 1/C 2
2 × 1020
1 × 1020 d(1/C 2)/dV 0
0
5
10
15
Voltage (V) (b)
Density (cm−3)
1 × 1017 8 × 1016 6 × 1016 4 × 1016 2 × 1016 0 0.2
0.4
0.6
0.8
Depth (µm) (c)
Fig. E2.2
(continued)
Eq. (2.5(b)) we find NA = 6.7 × 1037 /[d(1/C 2 )/dV ]. Using the slope d(1/C 2 )/dV and Eq. (2.6) gives the carrier density profile in Fig. E2.2(c). Another approach is to write CP in Eq. (2.32) as 1 + (2πf rs C)2 (1 + rs G)2 + (2πf rs C)2 1 ≈ = CP C C Then plot 1/CP versus f 2 . The slope is (2πrs )2 C and the intercept is 1/C, allowing both rs and C to be determined.
The effect of series resistance on a dopant profile of an epitaxial GaAs layer grown on a semiinsulating substrate is illustrated in Fig. 2.22. The correct profile is the one labeled rs = 0. To obtain the other curves, external resistors were placed in series with the device to demonstrate the effect. Semiconducting layers on insulating or semiinsulating substrates are particularly prone to series resistance effects since both contacts are made on the top surface and lateral series resistance can be substantial.82 For more details of capacitance measurements for devices with leaky junctions, wafer chuck parasitic capacitance and other considerations see Appendix A6.2.
89
MEASUREMENT ERRORS AND PRECAUTIONS
1018
Density (cm−3)
3.9 kΩ
8.2 kΩ
10 kΩ
2.2 kΩ
1017
rs = 0 1016
1015
0
0.5
1
1.5
Depth (µm)
Fig. 2.22 Measured dopant profiles for a GaAs epitaxial layer on a semiinsulating substrate. The series resistance was obtained by placing resistors in series with the device. Reprinted after ref. 81 by permission of IEEE ( 1975, IEEE).
2.4.3
Minority Carriers and Interface Traps
In a reversebiased Schottky barrier or pn junction diode, the scr width remains constant as a function of time because thermally generated electronhole pairs are swept out of the scr and leave through the ohmic contacts of the device. Thermally generated minority carriers in a deepdepleted MOS capacitor (MOSC), on the other hand, drift to the SiO2 Si interface to form an inversion layer and the device is unable to remain in deep depletion, leading to errors in doping density profile measurements. For a more complete discussion of the behavior of MOS capacitors in their nonequilibrium or deepdepletion state see Section 7.6.2. Minority carriers can be neglected when the MOSC is driven rapidly into deep depletion by applying a high ramp rate gate voltage. Alternately, a pulse train of successively higher gate voltage pulses can be applied with the device being cycled between accumulation and deep depletion. The effect of minority carriers is shown on Fig. 2.23. When the MOSC is driven into deep depletion by a rapidly varying ramp voltage, curve (i) in Fig. 2.23(a) results.
8 × 1014 (ii) Density (cm−3)
Capacitance (pF)
20 15 (iii) 10 5
(ii)
4 8 Gate Voltage (V) (a)
4 × 1014 2×
maxmin
(i)
1014
(iii)
(i) 0
6 × 1014
12
0
0
2 4 Depth (µm)
6
(b)
Fig. 2.23 (a) Equilibrium C –VG curve of an MOSC, (b) deepdepletion curves for (i) 5 V/s and (ii), (iii) 0.1 V/s sweep rates, (c) the carrier density profiles determined from (b). Cox = 98 pF, tox = 120 nm. Courtesy of J.S. Kang, Arizona State University.
90
CARRIER AND DOPING DENSITY
For negligible minority carrier generation the curve is identical for the gate voltage being swept from left to right or from right to left as indicated by the arrows. The doping density profile obtained from this curve is shown in Fig. 2.23(b) by (i). If the curve is swept very slowly, then the equilibrium highfrequency curve is obtained. For an intermediate sweep rate curve (ii) results. This curve lies above curve (i) and the extracted doping density profile, shown in Fig. 2.23(b) by (ii), is in error because dC/dV for (ii) is lower than dC/dV for (i). If curve (ii) is swept from right to left, resulting in curve (iii), its doping density profile is lower for similar reasons, as shown in Fig. 2.23(b) by curve (iii). It is possible to correct for these effects but corrections are not necessary for high sweep rates.83 Using the maxmin MOSC capacitance method to determine NA , we find for equilibrium Cmin /Cox = 0.19, coupled with tox = 120 nm NA ≈ 3.5 × 1014 cm−3 . This value is very close to curve (i) in Fig. 2.23(b). Of course, the Cmin /Cox approach does not give a doping density profile, but considering its simplicity, it yields a density that compares favorably with the differential capacitance derived value. The effects of minority carrier generation are a problem for high carrier generation rates in devices with low generation lifetimes. It is more difficult to drive the MOSC into deep depletion under those conditions. Cooling to liquid nitrogen temperatures for high generation rates works well to reduce the effects of minority carrier generation.84 Providing a collecting junction is another way to reduce the effect of minority carriers. As soon as minority carriers are generated, they are collected by the reversebiased junction as in MOSFETs with source and drain reverse biased and in gatecontrolled diodes. A further complication is introduced by interface traps invariably present in all MOS capacitors. The interface trap density is usually negligibly low for properly annealed, high quality SiO2 Si interfaces. When interface states do play a role, they cause the C –V curves to be stretched out. Their effect on doping profiling can be corrected by measuring the highfrequency capacitance Chf and the lowfrequency capacitance Clf according to85 NA,corr =
1 − Clf /Cox NA,uncorr 1 − Chf /Cox
(2.37)
The effects of interface traps are considerably reduced in the pulsed MOSC doping density profile technique when the modulation frequency is increased. Modulation frequencies of 30 MHz have been suggested,19 but most measurements are made at 1 MHz or lower. Interface trap effects are also reduced when the device is cooled. Interface traps or interfacial layers can also give errors in Schottky barrier capacitance profiling. It has been found that if the diode ideality factor n is larger than 1.1, erroneous profiles are obtained.86 Ideality factors n ≤ 1.1 are satisfactory for profiling. 2.4.4
Diode Edge and Stray Capacitance
C –V profiling relies on an accurate knowledge of the capacitance and of the device area. While the capacitance can be accurately measured, the area cannot always be accurately determined. Furthermore the capacitance may contain stray capacitance components. The device contact area can be measured but the effective area differs from the contact area due to lateral spacecharge region spreading. The effective capacitance is87 Ceff = C(1 + bW/r)
(2.38)
MEASUREMENT ERRORS AND PRECAUTIONS
91
where C = Ks εo A/W , A = πr 2 , r is the contact radius, b ≈ 1.5 for Si and GaAs, and b ≈ 1.46 for Ge. Eq. (2.38) assumes the lateral extent of the spacecharge region to be identical to the vertical extent. The lateral scr effect diminishes as the contact radius increases and r ≥ 100 bW ensures for the second term in the bracket to contribute no more than 1% to the effective capacitance. For W = 1 µm, r ≥ 150 µm whereas for W = 10 µm, r ≥ 1500 µm. This is not a particularly severe limitation. It should be considered, however, because the effective doping density is related to the actual doping density by (2.39) NA,eff = (1 + bW/r)3 NA Equation (2.38) shows the edge capacitance to be a constant, and it can be nulled prior to differential profile measurements by using a dummy capacitor of an appropriate value. For mercuryprobe profiling it has been proposed to make the contact sufficiently large that the edge capacitance effects can be neglected. The minimum recommended contact radius depends on the substrate doping density and should be53 rmin = 0.037(N/1016 )−0.35 cm
(2.40)
where N is the doping density. Equation (2.40) is valid for the doping range of 1013 to 1016 cm−3 . The minimum radius is about 8.3 × 10−2 cm for N = 1015 cm−3 . A diode junction capacitance consists of the true capacitance, C, the perimeter capacitance, Cper and the corner capacitance Ccor . The effective capacitance can be approximated by88 Ceff = AC + P Cper + NCcor (2.41) where A is the area, P the perimeter, and N the number of corners. By using diodes with various areas and perimeters, it is possible to separate the various components and extract the true diode capacitance.88 Stray capacitance is more difficult to determine. It includes cable and probe capacitances, bonding pads, and gate protection diodes in MOSFETs. Cable and probe capacitances can be eliminated by nulling the capacitance meter without contact to the diode. Bonding pad capacitance can usually be calculated. Since the diode, MOSC, or MOSFET can be made much smaller than the bonding pad, it becomes important to know the bonding pad capacitance contribution accurately. 2.4.5
Excess Leakage Current
Junction devices occasionally show excessively high reversebiased leakage currents leading to erroneous doping density profiles, especially for Schottky barrier devices. The assumption in the conventional profile equations is that the voltage is measured across the reversebiased spacecharge region only. For most devices that is a good assumption since the resistance of the reversebiased scr is much higher than the semiconductor quasineutral region resistance. For excessive leakage currents, however, an appreciable voltage can be developed across the quasineutral regions. This voltage is automatically included in the recorded voltage introducing errors in the measured profiles.89 2.4.6
Deep Level Dopants/Traps
Capacitance measurements, being a measure of charge responding to an applied timevarying voltage, will detect any charge that responds to the applied voltage. We have
92
CARRIER AND DOPING DENSITY
already considered the contribution of interface traps to the capacitance. Deep level impurities or traps in the semiconductor bulk can also produce errors in capacitance profiles.90 – 92 The contribution of traps is a complicated function of the density and energy level of the traps as well as the sample temperature and the frequency of the ac voltage. The ac voltage frequency is often assumed to be sufficiently high for the traps to be unable to follow it. Even if that is true, there is still cause for concern because the reverse bias dc voltage usually changes sufficiently slowly for the traps to be able to respond. This can give rise to profile errors that are both time and depth dependent. Fortunately, for trap densities much less than the doping density, say 1% or less, the contribution of traps is usually negligible. Capacitance measurements of traps are discussed in Chapter 5. A potential problem arises for deeplying dopant atoms not fully ionized at the measurement temperature. For the common dopants, e.g., P , As, and B in Si and Si in GaAs, this is of no concern. However, for SiC, for example, some dopant energy levels can lie deep in the band gap. Consider the reversebiased Schottky contact on a ptype substrate illustrated in Fig. 2.24. The dopant impurity has an energy level EA = Ev + E. In the quasineutral region (qnr) the impurities are only partially ionized. The unionized, neutral atoms are indicated by NAo . Obviously p = NA in the qnr and the resistivity ρ is not uniquely related to NA since ρ ∼ 1/p. The degree of ionization depends on E, NA , and the temperature. However, in the spacecharge region (scr) the situation is different. Let us assume the reverse bias V1 has been applied for a sufficiently long time that all
V
pType (qnr)
(scr) W
∆W
N oA 
EC
NA−




p

EA EV ∆E
(a)




(b)
Fig. 2.24 Band diagram of a reversebiased Schottky diode showing complete ionization in the spacecharge region (scr) but only partial ionization in the quasineutral region (qnr). (a) V = V1 , (b) V = V1 + V .
MEASUREMENT ERRORS AND PRECAUTIONS
93
holes have been emitted from neutral acceptors. The emission time constant, discussed in Chapter 5, is exp(E/kT ) (2.42) τe = σp vth Nv where σp is the capture cross section, vth the thermal velocity, and Nv the effective density of states in the valence band. Now consider an ac voltage superimposed on the dc voltage with the ac voltage swinging positively causing the scr width to increase from W to W + W . Some of the neutral acceptors originally in the qnr now find themselves in the scr. If τe < 1/ω, where ω = 2πf , then those holes trapped on acceptors will be emitted during the ac half cycle and the device behaves as a normal, shallowlevel acceptor device. However, for τe > 1/ω there is insufficient time for hole emission and the device will behave abnormally. The premise that it is p or NA that is measured in a uniformly doped sample is no longer true. What is measured is an effective carrier density related to the doping density in an unknown way. During the negative ac voltage swing, the scr narrows and holes are captured rather than emitted. Capture is usually very fast and does not constitute a limit. It is emission that is the limit since τe depends exponentially on E. Whether the true carrier or dopant density profile can be determined depends on the energy level of the dopant, the temperature, and the measurement frequency. The case of In in Si, whose energy level is at EV + 0.16 eV, has been discussed by Schroder et al.90 A more general treatment directed at traps in a semiconductor containing shallow level dopants is given by Kimerling.91 2.4.7
SemiInsulating Substrates
Epitaxial or implanted layers on semiinsulating or insulating substrates present unique profiling problems. Examples include silicononinsulator and GaAs implanted layers on semiinsulating substrates. Due to the high resistance of the substrate, both contacts must be made to the top surface, introducing series resistance, especially when the reversebiased scr extends close to the substrate as illustrated in Fig. 2.25. The remaining neutral region of the layer, indicated by the thickness t, becomes very thin and appreciable series resistance rs results. Similar problems occur when an ntype (ptype) layer is formed on a ptype (ntype) substrate. The measured density profiles sometimes exhibit minima
1
2
Conducting Layer rs t Insulating Substrate
Fig. 2.25 Conducting layer on an insulating substrate showing the increasing series resistance with increasing back bias on contact 1.
94
CARRIER AND DOPING DENSITY
near the interface between the two. Such minima are usually not real, but are artificially introduced by the sample geometry.93 An additional word of caution. Contact 1 in Fig. 2.25 should be rectifying and contact 2 should be ohmic. That is usually not possible when the conducting layer is lightly doped. In that case one should make contact 2, which is forward biased when contact 1 is reverse biased, much larger than contact 1. This ensures the C2 to be much higher than C1 because A2 ≫ A1 and contact 2 is forward biased. As a first approximation, C2 can be treated as a short circuit and C1 is measured. 2.4.8
Instrumental Limitations
Capacitance meters determine the accuracy with which p(x) and W are measured. The depth resolution should be limited by the Debye length rather than by the instrument. The overriding influence on the accuracy of p(x) is the precision with which C is measured.94 There is a temptation to make C large, but this introduces errors in the determination of the local value of C/V because C –V curves are not linear. It also degrades the depth resolution by increasing the modulation of W . It is common practice in analog profilers to keep V constant by using a modulation voltage of constant amplitude. According to Eqs. (2.9) and (2.19) V =
C W qWp(W )W =− and Ks εo W C
so that C = −
Ks εo CV qW 2 p(W )
(2.43)
(2.44)
For constant p(W ) and constant V , C decreases as the sample is profiled because w increases and C decreases. Consequently profiles become noisier as the profile is measured deeper into the sample. Constant electric field increment feedback profilers alleviate this problem somewhat. An excellent discussion of instrumental limitations is given by Blood.55
2.5
HALL EFFECT
Those aspects of the Hall effect pertaining to carrier density measurements are discussed here. A more complete treatment of the Hall effect, including a derivation of the appropriate equations, is given in Chapter 8. The key feature of Hall measurements is the ability to determine the carrier density, the carrier type, and the mobility. Hall theory predicts the Hall coefficient RH as95
RH =
r(p − b2 n) q(p + bn)2
(2.45)
where b = µn /µp and r is the scattering factor whose value lies between 1 and 2, depending on the scattering mechanism in the semiconductor.95 The scattering factor is also a function of magnetic field and temperature. In the high magnetic field limit r → 1. The scattering factor can be determined by measuring RH in the high magnetic field limit, i.e.,
HALL EFFECT
95
r = RH (B)/RH (B = ∞) where B is the magnetic field. The scattering factor in ntype GaAs was found to vary from 1.17 at B = 0.1 kG to 1.006 at B = 83 kG.96 The high fields necessary for r to approach unity are not achievable in most laboratories. Typical magnetic fields are 0.5 to 10 kG, making r > 1 for typical Hall measurements. Since r is usually not known, it is frequently assumed to be unity. The Hall coefficient is determined experimentally as RH =
tVH BI
(2.46)
where t is the sample thickness, VH the Hall voltage, B the magnetic field, and I the current. The thickness is well defined for uniformly doped wafers. However, the active layer thickness is not necessarily the total layer thickness for thin epitaxial or implanted layers on substrates of opposite conductivity type or on semiinsulating substrates. If depletion effects caused by Fermi level pinned band bending at the surface and by band bending at the layersubstrate interface are not considered, the Hall coefficient will be in error as will those semiconductor parameters derived from it.97 Even the temperature dependence of the surface and interface spacecharge regions should be considered for unambiguous measurements.98 For extrinsic ptype material with p ≫ n, Eq. (2.45) reduces to RH =
r qp
(2.47)
and for extrinsic ntype it becomes RH = −
r qn
(2.48)
A knowledge of the Hall coefficient leads to a determination of the carrier type as well as the carrier density, according to Eq. (2.47) and (2.48). Usually r is assumed to be unity—an assumption generally introducing an error of less than 30%.99 The Hall effect is used to measure the carrier density, resistivity and mobility at a given temperature, and the carrier density as a function of temperature to extract additional information. For a ptype semiconductor of doping density NA compensated with donors of density ND , the hole density is determined from the equation100 p(p + ND ) − n2i Nv = exp(−EA /kT ) 2 g NA − ND − p + ni /p
(2.49)
where Nv is the effective density of states in the valence band, g the degeneracy factor for acceptors (usually taken as 4), and EA the energy level of the acceptors above the valence band with the top of the valence band as the reference energy. Equation (2.49) can be simplified for certain conditions. 1. At low temperatures where p ≪ ND , p ≪ (NA − ND ), and ni 2 /p ≈ 0 p≈
(NA − ND )Nv exp(−EA /kT ) gND
(2.50)
96
CARRIER AND DOPING DENSITY
2. When ND is negligibly small, p≈
(NA − ND )Nv exp(−EA /2kT ) g
(2.51)
3. At higher temperatures where p ≫ ni , p ≈ NA − ND
(2.52)
4. At still higher temperatures, where ni ≫ p p ≈ ni
(2.53)
According to Eqs. (2.50) and (2.51), the slope of a log(p) versus 1/T plot gives an activation energy of either EA or EA /2, depending on whether there is a compensating donor density in the material or not. At higher temperatures, typically room temperature, the net majority carrier density is obtained with zero activation energy. At still higher temperatures the activation energy is that of ni . The experimental log(p) versus 1/T data can be fitted with an appropriate model, and a wealth of information can be extracted. Figure 2.26 shows the Hall carrier density data for an indiumdoped silicon sample.101 In addition to In, the sample contains Al, B, and P . For the acceptors (B, Al, and In) both the densities and the energy levels were extracted from the data. This figure demonstrates the powerful nature of Hall measurements. Hall measurements are generally made on samples from which an average carrier density is derived. For uniformly doped samples the true density is obtained, but for nonuniformly doped samples an average value is determined. Occasionally one wants to measure spatially varying carrier density profiles. The Hall technique is suitable through differential Hall effect (DHE) measurements. Layers can be stripped reliably by anodic oxidation and subsequent oxide etch. Anodic oxidation consumes a certain fraction of the
1016 EIn/2
p (cm−3)
1015 1014 1013
EB
1012 1011 1010
0
10
20
30
1000/T (K−1)
Fig. 2.26 Carrier density vs. reciprocal temperature for Si:In with Al and B contamination. NI n = 4.5 × 1016 cm−3 , EI n = 0.164 eV, NAl = 6.4 × 1013 cm−3 , EAl = 0.07 eV, NB = 1.6 × 1013 cm−3 , ND = 2 × 1013 cm−3 . Reprinted after ref. 101 by permission of IEEE ( 1980, IEEE).
OPTICAL TECHNIQUES
97
semiconductor that is removed during the oxide etch. Layers can be removed in increments as small as 2.5 nm.102 For a further discussion of DHE, see Section 1.4.1. The interpretation of the differential Hall data becomes more complex when successive measurements are made. In order to generate a carrier density profile, the sheet Hall coefficient RHsh , given by RHsh = VH /BI , and the sheet conductance GHsh must be measured repeatedly. The carrier density profile is obtained from Hall coefficient versus depth and from sheet conductance versus depth curves according to the relationship103 p(x) =
r(dGHsh /dx)2 qd(RHsh G2Hsh )/dx
(2.54)
where GHsh = 1/RHsh . Occasionally the Hall sample consists of an n or pfilm on a p or nsubstrate. For film and substrate of opposite conductivity, the pn junction between them is usually assumed to be an insulating boundary. If that is not true, then the Hall data must be corrected.104 This correction must also be made if the sample consist of a layer on an oppositely doped substrate and the junction separating the two is a good insulator, but the ohmic contact to the Hall sample is alloyed through the top layer, shorting it to the substrate. This can happen if the upper layer is an unintentional type conversion as has been observed in HgCdTe.105 For a simple twolayer structure with an upper layer of thickness t1 and conductivity σ1 and a substrate of thickness t2 and conductivity σ2 the Hall constant is105 – 106 RH = RH 1
t1 σ1 2 t2 σ2 2 + RH 2 t σ t σ
(2.55)
where RH 1 is the layer 1 Hall constant, RH 2 is the substrate 2 Hall constant, t = t1 + t2 , and σ is t2 σ2 t1 σ1 + (2.56) σ = t t For t1 = 0 we have t = t2 , σ = σ2 , and RH = RH 2 , with the substrate being characterized. If the upper layer is more heavily doped than the substrate or if it is formed by inversion through surface charges, for example, and σ2 ≪ σ1 , then σ ≈
tRH 1 t1 σ1 ; RH ≈ t t1
(2.57)
and the Hall measurement characterizes the surface layer. This can be especially serious if the existence of the upper layer is not suspected.105
2.6 2.6.1
OPTICAL TECHNIQUES Plasma Resonance
The optical reflection coefficient of a semiconductor is given by R=
(n − 1)2 + k 2 (n + 1)2 + k 2
(2.58)
98
CARRIER AND DOPING DENSITY
where n is the refractive index and k = αλ/4π is the extinction coefficient, with α the absorption coefficient and λ the photon wavelength. The reflection coefficient of semiconductors is high at short wavelengths, tends to a constant, and then shows an anomaly at higher wavelengths. First, it decreases toward a minimum and then rises rapidly toward unity. R approaches unity when the photon frequency ν, related to the wavelength through the relation ν = c/λ, approaches the plasma resonance frequency νp . The plasma resonance wavelength λp is given by107 2πc λp = q
Ks εo m∗ p
(2.59)
where p is the free carrier density in the semiconductor and m∗ the effective mass. It is, in principle, possible to determine p from λp . The plasma resonance wavelength is difficult to determine because it is not well defined. It is for this reason that the carrier density is determined not from the plasma resonance wavelength but from the wavelength λmin at the reflectivity minimum, where λmin < λp . The minimum wavelength is related to the carrier density through the empirical relationship (2.60) p = (Aλmin + C)B where the constants A, B, and C are tabulated in ref. 108. The technique is useful only for carrier densities higher than 1018 to 1019 cm−3 . The carrier densities determined with this technique are for uniformly doped substrates or for uniformly doped layers with layer thicknesses at least equal to 1/α. For diffused or implanted layers with varying carrier density profiles, a determination of the surface density is only possible if the shape of the profile and the junction depth are known.109 A further complication for thin epitaxial layers is introduced by the phase shift at the epitaxial layer–substrate interface, adding an oscillatory component to the Rλ curve, making it more difficult to extract λmin .110 2.6.2
Free Carrier Absorption
Photons of energy hν > EG , absorbed in a semiconductor, generate electronhole pairs. Photons of energy hν < EG can excite trapped electrons from the ground state of shallowlevel impurities onto excited states as discussed in Section 2.6.3. It is also possible that photons of energy hν < EG excite free electrons (holes) in the conduction (valence) band to higher energy states in the band, i.e., photons are absorbed by free carriers. This is the basis of free carrier absorption. The free carrier absorption coefficient for holes is given by95 αf c =
q 3 λ2 p 4π 2 εo c3 nm∗2 µp
= 5.27 × 10−17
λ2 p n(m∗ /m)2 µp
(2.61)
where λ is the wavelength, c the velocity of light, n the refractive index, m∗ the effective mass, and µp the hole mobility. However, care should be taken during the measurement not to use wavelengths that coincide with impurity or lattice absorption lines. For example, there is an absorption line in silicon due to interstitial oxygen at λ = 9.05 µm and substitutional carbon at λ = 16.47 µm. Lattice absorption lines are found near λ = 16 µm.
OPTICAL TECHNIQUES
99
By fitting curves to experimental Si data good agreement is observed for111 αf c,n ≈ 10−18 λ2 n; αf c,p ≈ 2.7 × 10−18 λ2 p
(2.62)
where n and p are the free carrier densities in cm−3 for nSi and pSi, respectively, and the wavelength is given in units of µm. Carrier densities of 1017 cm−3 or higher can be measured by this technique. The measurement becomes difficult for lower densities because the absorption coefficient is too low to be reliably determined. A modified expression has recently been published providing better agreement between sheet resistance and free carrier absorption measurements.112 An expression for nGaAs is113 αf c (λ = 1.5 µm) = 0.81 + 4 × 10−18 n; αf c (λ = 0.9 µm) = 61 − 6.5 × 10−18 n (2.63) Free carrier absorption also lends itself to sheet resistance measurements. Good agreement with experiment has been found in transmission using the expression111 T ≈ (1 − R)2 exp(−kλ2 /Rsh )
(2.64)
with k = 0.15 for ntype Si and k = 0.3375 for ptype Si layers, where T is the transmittance. λ is in µm and Rsh in ohms/square. Free carrier density maps have been generated by scanning the infrared light beam. Carrier densities as low as 1016 cm−3 have been determined with a 1 mm resolution using λ = 10.6 µm.114 2.6.3
Infrared Spectroscopy
Infrared spectroscopy relies on optical excitation of electrons (holes) from their respective donors (acceptors) into excited states. Consider the ntype semiconductor, shown in Fig. 2.27(a). At low temperatures most of the electrons are “frozen” onto the donors, and the free carrier density in the conduction band is very low. The electrons are mainly located on the lowest energy level or donor ground state in Fig. 2.27(b). With photons of energy hν ≤ (EC − ED ) incident on the sample, two optical absorption processes can occur: electrons can be excited from the ground state to the conduction band giving a broad absorption continuum, and electrons can be excited from the ground state to one
Ec 3 2 1ED (b)
hν< Eg
Ec ED hν> Eg EA EV (a)
(c)
Fig. 2.27 (a) Energy band diagram for a semiconductor containing donors at low temperature, (b) energy band diagram showing the donor energy levels, (c) band diagram when both donors and acceptors are present. The “aboveband gap” light fills donors and acceptors.
100
CARRIER AND DOPING DENSITY
Relative Transmittance
100 80 60
Phosphorus 9.7 × 1012 cm−3
Arsenic 1.1 × 1013 cm−3
40 20 0 300
350
400
450
500
−1
Wavenumber (cm ) (a)
Relative Transmittance
100 80
Arsenic 2.1 × 1013 cm−3
60
Boron 1.6 × 1013 cm−3
40 20 0 300
Aluminum 1.4 × 1013 cm−3
Phosphorus 350
400
450
500
Wavenumber (cm−1) (b) Fig. 2.28 (a) Donor impurity spectrum for 265 cm nSi at T ≈ 12 K, (b) spectrum for the sample in (a) with “aboveband gap” illumination. Reprinted with permission after ref. 117.
of several excited states producing sharp absorption lines in the transmission spectrum, characteristic of the shallowlevel impurities.115 – 116 Such a transmittance curve is shown in Fig. 2.28(a) for phosphorus and arseniccontaining silicon.117 Additional information can be obtained by splitting the energy levels with a magnetic field.118 Through the use of Fourier transform techniques (Fourier transform infrared spectroscopy is discussed in Chapter 10), high sensitivity is obtained, and the detection limits are extremely low. Doping densities as low 5 × 1011 cm−3 have been measured in Si.117 Such low densities can also be determined by Hall measurements, but contactless optical techniques are simpler, but require low temperatures. Most electrical carrier density measurement methods determine the net carrier density n = ND − NA in an ntype sample. The infrared spectroscopy technique as discussed so far also measures ND − NA , because there are only n = ND − NA electrons frozen onto the donors at the low temperatures. Compensating acceptors are empty of holes because the holes are compensated by electrons. To measure ND and NA , the sample is illuminated with background light of energy hν > EG .117, 119 – 120 Some of the excess electronhole pairs generated by the background light are captured by the ionized donors and acceptors. Virtually all donors and acceptors are neutralized, as shown in Fig. 2.27(c).
OPTICAL TECHNIQUES
101
The long wavelength infrared radiation now can excite electrons into excited donor states and holes into excited acceptor states. A spectrum for a Si sample without and with background light is shown in Fig. 2.28. The upper curve is without and the lower with background light. Two features distinguish Fig. 2.28(a) from 2.28(b): the P and As signals are increased, and the compensating B and Al impurities appear in the spectrum. It is possible to determine the density of all impurities and to identify them because each impurity has unique absorption peaks. The strongest absorption lines for Si are given by Baber.117 The infrared spectroscopy technique is very quantitative in identifying the impurity type but is qualitative in determining the impurity density. In order to determine the relationship between the absorption peak height and the impurity density, calibration data must be established using samples with known doping density. For uncompensated material this is fairly unambiguous. For compensated samples the procedure is more complex.117 The optical transmittance through a semiconductor wafer of thickness t is approximately (2.65) T ≈ (1 − R)2 exp(−αt) For reasonable measurement sensitivity, αt should be on the order of unity or t ≈ 1/α. For α ≈ 1 to 10 cm−1 , applicable for shallow impurity absorption at low densities, the sample must be 1 to 10 mm thick. Samples of this thickness are convenient for bulk wafers but not for epitaxial layers, making IR spectroscopy of thin layers impractical. A variation of this technique is photothermal ionization spectroscopy (PTIS) or photoelectric spectroscopy. Bound donor electrons are optically excited from the ground state to one of the excited states. At T ≈ 5 to 10 K the sample phonon population is sufficiently high for carriers in the excited state to be transferred into the conduction band thermally leading to a change in sample conductivity. It is this photoconductivity change that is detected as a function of wavelength.121 – 123 Doping densities as low as 109 cm−3 boron and gallium acceptors in Ge have been measured by the technique.124 A disadvantage of PTIS is the need for ohmic contacts, but the advantage is its sensitivity for thin films. PTIS has been combined with magnetic fields for easier identification of impurities in GaAs and InP.121 2.6.4
Photoluminescence (PL)
Photoluminescence is a technique to detect and identify impurities in semiconductor materials, described in Chapter 10. PL relies on the creation of electronhole pairs by incident radiation and subsequent radiative recombination photon emission. The radiative emission intensity is proportional to the impurity density. We discuss here briefly the application of PL to the measurement of doping densities in semiconductors. Impurity identification by PL is very precise because the energy resolution is very high. It is the density measurement that is more difficult because it is not easy to draw a correlation between the intensity of a given impurity spectral line and the density of that impurity, due to nonradiative recombination through deeplevel bulk or surface recombination centers.125 Since the density of recombination centers can vary from sample to sample, even for constant shallow level densities, the photoluminescence signal can vary greatly. This problem has been overcome by measuring both the intrinsic and the extrinsic PL peaks and using their ratio. It has been determined that the ratio XTO (BE)/ITO (FE) is proportional to the doping density.126 XTO (BE) is the transverse optical phonon PL intensity
102
CARRIER AND DOPING DENSITY
PL Intensity Ratio
102 101 B 100 P 10−1 10−2 10−3 1011
1012
1013
1014
1015
Doping Density (cm−3)
Fig. 2.29 PL intensity ratio versus doping density for B and P in Si. Reprinted with permission after ref. 128.
peak of bound excitons for element X = B or P , and ITO (FE) is the transverse optical phonon intrinsic PL intensity peak of free excitons. Good agreement is found between the resistivity measured electrically and the resistivity determined from photoluminescence for Si with the PL intensity ratio shown in Fig. 2.29 as a function of doping density. In InP the donor density as well as the compensation ratio was determined.127
2.7
SECONDARY ION MASS SPECTROMETRY (SIMS)
Secondary ion mass spectrometry is a very powerful technique for the analysis of impurities in solids. The details of SIMS are discussed in Chapter 11. In this section we briefly discuss the application of SIMS to semiconductor dopant profiling. The technique relies on removal of material from a solid by sputtering and on analysis of the sputtered ionized species. Most of the sputtered material consists of neutral atoms and cannot be analyzed. Only the ionized atoms can be analyzed by passing them through an energy filter and a mass spectrometer. It can detect all elements. SIMS has good detection sensitivity for many elements, but its sensitivity is not as high as electrical or optical methods. Among the beam techniques it has the highest sensitivity and can detect dopant densities as low as 1014 cm−3 . It allows simultaneous detection of different elements, has a depth resolution of 1 to 5 nm, and can give lateral surface characterization on a scale of several microns. It is a destructive method since the very act of removing material by sputtering leaves a crater in the sample. A SIMS doping density plot is produced by sputtering the sample and monitoring the secondary ion signal of a given element as a function of time. Such an “ion signal versus time” plot contains the necessary information for a dopant density profile. The time axis is converted to a depth axis by measuring the depth of the crater at the end of the measurement assuming a constant sputtering rate. This should be done for each sample, since the sputter rate varies with spot focus and ion current.129 The secondary ion signal is converted to impurity density through standards of known dopant profile. The proportionality between ion signal and density is strictly true only if the matrix which contains the impurity is uniform. The ion yield of a given element is highly dependent on the matrix. For example, boron is implanted into Si at a given energy and dose to create
RUTHERFORD BACKSCATTERING (RBS)
103
Electrical Activation (%)
100 80
0.1 keV 0.5 keV 2.5 keV
60 40 20 0 700
800
900 1000 Temperature (°C)
1100
1200
Fig. 2.30 Electrical activation of a 5 × 1014 cm−2 boron implantation for energies ranging from 100 eV to 5 keV after a 10 s RTA for different temperatures. Adapted from ref. 132.
a standard. The secondary ion signal is calibrated by assuming the total amount of boron in the sample to be equal to the implanted boron. The unknown sample of B implanted into Si is then compared to the standard. SIMS determines the total, not the electrically active impurity density. For example, implanted, nonannealed samples give SIMS profiles very close to the predicted Gaussian distribution. Electrical measurements give very different results, with the ions not yet electrically activated. SIMS and electrical measurement agree quite well for activated samples as shown in Figs. 1.22 and 2.14. Comparisons of SIMS dopant profiles with profiles measured by spreading resistance sometimes show a discrepancy in the lowly doped portions of the profile giving deeper junctions than those obtained by other methods (see Fig. 1.22).130 – 131 The SIMS tail is likely caused by cascade mixing and knockon of dopant atoms by the sputtering beam contributing to slightly deeper junctions or by the limited dynamic range of the SIMS instrument. When sputtering from a highly doped region near the surface to a lowly doped region deeper within the sample, the crater walls contain the entire doping density profile. Any stray signal from the crater walls adds to the signal from the lowly doped region in the central sputtered area giving the appearance of a higher dopant density and hence a deeper profile. Electronic or optical gating can suppress this signal. However, the ultimate limitation is material from the crater edges deposited on the crater floor adding to the crater floor signal. Another reason for the discrepancy is the nature of the species measured. Current is measured in SRP and the density of the electrons/holes depends on the activation of the implanted ions. SIMS, on the other hand, measures the total dopant density, regardless of activation. Figure 2.30 illustrates this point by showing the dependence of electrical activation of boron implanted into silicon on implant dose and activation anneal temperature.132
2.8
RUTHERFORD BACKSCATTERING (RBS)
Rutherford backscattering, discussed in Chapter 11, is a nondestructive, quantitative technique requiring no standards. It is based on backscattering of light ions from a sample. Usually monoenergetic He ions of 1–3 MeV energy are incident on and scattered
104
CARRIER AND DOPING DENSITY
from a sample and detected with a surface barrier detector. RBS is most useful for heavy elements in a light matrix. For example, As in Si or Te in GaAs are suitable, whereas B in Si and Si in GaAs are difficult to quantify, because in the interaction of a light ion (e.g., He) with a heavy ion (e.g., As), He loses less energy than if it interacted with a light ion (e.g., B). No backscattering occurs from ions lighter than the probe ions. The sensitivity of RBS is low compared to SRP and SIMS. The lowest detection limit is on the order of 1014 cm−2 atoms. For a layer 10−5 cm thick this corresponds to 1014 /10−5 = 1019 cm−3 . The sensitivity can be improved by using ions heavier than He, such as carbon. But heavy ions impair the depth resolution. Depth resolution can be improved by target tilting. Resolutions as low as 2–5 nm have been achieved.133 RBS has an additional advantage and that is the ability to determine doping activation of implanted samples through ion channeling where the incoming ions are aligned with a crystal direction. Ions are channeled down the open channels and few ions are backscattered. Implanted, but nonactivated atoms, typically occupy interstitial sites in the lattice causing increased backscattering. Analysis of the backscattered data allows a determination of the degree of electrical activation. None of the previous techniques give this type of information. RBS has also been used in the development of silicides and the effect of silicide formation on dopant distributions of impurities in semiconductors. This is an ideal application where no other technique is suitable. As a silicide forms, its formation is followed by RBS and by measuring the As distribution in the Si below the silicide, one can follow the As “snowplowing” ahead of the silicide front.134
2.9
LATERAL PROFILING
As semiconductor device dimensions shrink it becomes important to know the vertical as well the horizontal or lateral dopant profiles. The lateral profile is required as an input to computer aided design models. However, as device dimensions shrink so does the junction depth. Consequently, the lateral extent of a junction, which is typically assumed to be 0.6–0.7 of the vertical dimension, is very small. It has been proposed that a 10% doping density sensitivity down to 2 × 1017 cm−3 with sub 10 nm resolution is required for measured profiles to be useful for prediction of device characteristics.135 What techniques are suitable for profile measurements at this scale? It is important to distinguish between atomic and electrically active dopant profiles. Many techniques have been attempted but few have given quantitative results. We give a brief summary here of these techniques. More detailed discussions can be found in refs. 136–137. In scanning tunneling microscopy (STM) (discussed in Chapter 9) the probe is moved along the lateral portion of the junction. The tunneling current depends on doping density due to tip induced band bending at the semiconductor surface. A modification of STM is the measurement of the tunneling barrier height. The barrier height is obtained by measuring the tunneling current as a function of probesample distance. Changes of barrier height correspond to changes of dopant density. STM tips are very sharp and the technique has claimed a 1 to 5 nm spatial resolution. However, surface preparation is a significant issue. Scanning or atomic force microscopy (AFM) has been combined with etching.138 A crosssection of the device is first prepared by careful polishing. The sample is then etched in a suitable etch and the resulting topographical feature is determined with a technique
STRENGTHS AND WEAKNESSES
105
capable of highresolution imaging, e.g., AFM, scanning electron microscopy or transmission electron microscopy. The technique relies on a dopant density dependent etch rate. Heavily doped regions etch faster than lightly doped regions. After etching, the surface is profiled and the physical profile is correlated with the dopant profile. Reference samples of known dopant density are required to calibrate the etch rate. Suitable etch solutions are for pSi: HF:HNO3 :CH3 COOH (1:3:8) for a few seconds under strong illumination and for nSi: HF:HNO3 :H2 O (1:100:25).139 A limitation of this technique is the limited sensitivity of ∼ 5 × 1017 cm−3 for pSi and nSi. The two main techniques that have emerged for lateral doping density profiling are scanning capacitance microscopy (SCM)140 and scanning spreading resistance microscopy (SSRM).141 In SCM a smallarea capacitive probe measures the capacitance of a metal/semiconductor or an MOS contact, similar to techniques described earlier in this chapter.142 If the capacitance measurement circuit is sufficiently sensitive, it is possible to measure the small capacitances of these probes. A problem is the nonplanar nature of the contact. SCM is discussed in Chapter 9. SSRM, based on the atomic force microscope (discussed in Chapter 9), measures the local spreading resistance between a sharp conductive tip and a large back surface contact. A precisely controlled force is used while the tip is stepped across the sample. SSRM sensitivity and dynamic range are similar to conventional spreading resistance (SRP discussed in Chapter 1). The small contact size and small stepping distance allows measurements on the device cross section with no probe conditioning. The high spatial resolution allows direct twodimensional nanoSRP measurements, without the need for special test structures.
2.10 STRENGTHS AND WEAKNESSES Differential Capacitance: The major weakness of the differential capacitance profiling method is its limited profile depth, limited at the surface by the zerobias spacecharge region width and in depth by voltage breakdown. The latter limitation is particularly serious for heavily doped regions. Further limitations are due to the Debye limit, which applies to all carrier profiling techniques. A minor weakness is the data differentiation introducing noise into the profile data. The method’s strength lies in its ability to give the carrier density profile with little data processing. A simple differentiation of the C –V data suffices. It is an ideal method for moderately doped materials and is nondestructive when a mercury probe is used. It is well established with available commercial equipment. Its depth profiling capability is extended significantly for the electrochemical profiling method. MaxMin MOSC Capacitance: The weakness of this technique lies in its inability to provide a density profile. It determines only an average doping density in the spacecharge region width of an MOSC in equilibrium. Its strength lies in its simplicity. It merely requires a highfrequency C –V measurement. Integral Capacitance: The integral capacitance technique also does not provide a profile, which limits its usefulness. It does, however, provide, a value for an implant dose and depth, and its major strength lies in its accuracy. This is very important when monitoring ion implants with uniformities of 1%.
106
CARRIER AND DOPING DENSITY
MOSFET CurrentVoltage: The substrate/gate voltage technique requires two differentiations and has not found wide application. The threshold voltage method needs a proper definition of threshold voltage in its interpretation. The advantage of both methods is the fact that a MOSFET is measured directly. No special, largearea test structures are required. This is especially important when such test structures are not available. It is, however, subject to short and narrowchannel effects. Spreading Resistance: The weakness of SRP is the complexity of sample preparation as well as the interpretation of the measured spreading resistance profile. The measured data must be deconvolved, and either the mobility must be known or well calibrated standards must be used to extract the dopant profile. Its strength lies in being a wellknown method that is routinely used by the semiconductor industry for Si profiling. It has no depth limit and can profile through an arbitrary number of pn junctions; it spans a very large doping density range from about 1013 cm−3 to 1021 cm−3 . Hall Effect: The Hall effect is limited in its profiling ability through the inconvenience of providing repeated layer removal. This has been simplified with commercial equipment. Although it is utilized for profiling, it is not a routine method for generating profiles. Its advantage lies in providing average values of carrier density and mobility. For that it is used a great deal, as discussed in Chapter 8. Optical Techniques: Optical techniques require specialized equipment with quantitative doping measurements requiring known standards. Profiling is generally not possible, and only average values are obtained. The major advantage of optical methods is their unprecedented sensitivity and accuracy in impurity identification. Furthermore, optical methods are, as a rule, contactless—a major advantage. Secondary Ion Mass Spectrometry: The weakness of SIMS lies in the complexity of the equipment. It does not have the sensitivity of electrical and optical techniques. It is most sensitive for B in Si, for all other impurities it has reduced sensitivity. It is useless for semiconductors with stoichiometric dopant species. Reference standards must be used for quantitative interpretation of the raw SIMS data, and matrix effects can render measurement interpretation difficult. The strength of SIMS lies in its accepted use for dopant density profiling. It is the most commonly used method. It measures the dopant density profile not the carrier density profile and can be used for implanted samples before any activation anneals. That is not possible with electrical methods. It has high spatial resolution and can be used for any semiconductor. Rutherford Backscattering: The weakness of RBS is its low sensitivity and the requirement of specialized equipment not readily available in most semiconductor laboratories. It is difficult to measure light elements. Its strength lies in its nondestructive and quantitative nature without recourse to standards. It is also capable of detecting activation effectiveness of implanted ions through ion channeling. Lateral Profiling: Lateral profiling, although potentially very important, has not been developed to the point where it is a routine, accurate method. Many techniques are being evaluated, but none stands out as the most dominant method at this time, but capacitance and spreading resistance profiling look promising.
APPENDIX 2.1
107
APPENDIX 2.1 Parallel or Series Connection? Some capacitance meters have provision for parallel or series connection measurements, i.e., the meter assumes the device under test to consist of either a parallel connection as shown in Fig. A2.1(a) or a series connection as in Fig. A2.1(b). The admittance YP of the parallel circuit and the impedance ZS of the series circuit are YP = GP + j ωCP ; ZS = RS + 1/j ωCS
(A2.1)
where ω = 2πf . Equating these two expressions as YP = 1/ZS gives CP =
DS2 1 1 C ; GP = 2 S 1 + DS 1 + DS2 RS
(A2.2)
with the dissipation factor DS : DS = ωCS RS
(A2.3)
Similarly, we can write CS = (1 + DP2 )CP ; RS = with the dissipation factor DP DP =
DP2 1 1 + DP2 GP
(A2.4)
GP ωCP
(A2.5)
The dissipation factor is sometimes expressed in terms of the quality factor Q. For the series and the parallel circuits, Q is given by QS =
1 1 1 ωCP = ; QP = = DS ωCS RS DP GP
GP
CP
(A2.6)
CS
RS
(a)
(b)
Fig. A2.1 (a) Parallel and (b) series connection of a capacitance having parallel conductance or series resistance.
108
CARRIER AND DOPING DENSITY
For an ideal capacitor, GP = 0 and RS = 0, leading to CS = CP . Usually, however, GP = 0 and RS = 0. Unfortunately there is no unique criterion to select the appropriate measurement circuit. Series measurement circuit for lowimpedance and parallel circuit for highimpedance samples are often used. The approximate instrumentation error for high dissipation values is given by % error = 0.1 1 + D 2
(A2.7)
Occasionally these concepts are expressed in terms of the loss tangent, tan(δ), defined as 1 σ = (A2.8) tan(δ) = Ks εo ω Ks εo ωρ APPENDIX 2.2 Circuit Conversion Let us consider the circuits in Figs. A2.2(a) and (b). The easiest way to convert from (a) to (b) is to consider the admittances of both circuits and to equate them. The admittance Y for (a) is Y (a) = =
1 G + j ωC 1 = = Z(a) rs + 1/(G + j ωC) 1 + rs (G + j ωC) (G + j ωC)(1 + rs G − j ωC) (1 + rs G + j ωrs C)(1 + rs G − j ωrs C)
(A2.9)
where Z is the impedance. Y (a) can be written as Y (a) =
G + rs G2 + rs (ωC)2 j ωC + (1 + rs G)2 + (ωrs C)2 (1 + rs G)2 + (ωrs C)2
(A2.10)
The admittance for (b) is simply Y (b) = GP + j ωCP .
G
C
GP
(A2.11)
CP
CS
RS rs
(a) Fig. A2.2
(b)
(c)
(a) actual circuit, (b) parallel equivalent circuit, (c) series equivalent circuit.
109
REFERENCES
Equating the real and imaginary parts of Eqs. (A2.10) and (A2.11) gives
CP =
(1 + rs
G(1 + rs G) + rs (ωC)2 C ; GP = 2 + (ωrs C) (1 + rs G)2 + (ωrs C)2
G)2
(A2.12)
For the circuits in Figs. A2.2(a) and (c), it is best to consider the impedances of both circuits and to equate them. The impedance of (a) is Z(a) = rs + =
1 (rs (G + j ωC) + 1)(G − j ωC) = G + j ωC (G + j ωC)(G − j ωC)
j ωrC rs (G2 + (ωC)2 ) + G − 2 2 2 G + (ωC) G + (ωC)2
(A2.13)
and for (c) it is Z(c) = RS +
j ωCS 1 = RS − j ωCS (ωCS )2
(A2.14)
Equating real and imaginary parts of Eqs. (A2.13) and (A2.14) gives
CS = C(1 + (G/ωC)2 ); RS =
rs (G2 + (ωC)2 ) + G 1 = rs + G2 + (ωC)2 G(1 + (ωC/G)2 (A2.15)
REFERENCES 1. W. Schottky, “Simplified and Expanded Theory of Boundary Layer Rectifiers (in German),” Z. Phys. 118, 539–592, Feb. 1942. 2. J. Hilibrand and R.D. Gold, “Determination of the Impurity Distribution in Junction Diodes from CapacitanceVoltage Measurements,” RCA Rev. 21, 245–252, June 1960. 3. R. Decker, “Measurement of Epitaxial Doping Density vs. Depth,” J. Electrochem. Soc. 115, 1085–1089, Oct. 1968. 4. L.E. Coerver, “Note on the Interpretation of C –V Data in Semiconductor Junctions,” IEEE Trans. Electron Dev. ED17, 436, May 1970. 5. H.J.J. DeMan, “On the Calculation of Doping Profiles from C(V) Measurements on TwoSided Junctions,” IEEE Trans. Electron Dev. ED17, 1087–1088, Dec. 1970. 6. W. van Gelder and E.H. Nicollian, “Silicon Impurity Distribution as Revealed by Pulsed MOS C –V Measurements,” J. Electrochem. Soc. 118, 138–141, Jan. 1971. 7. Y. Zohta, “Rapid Determination of Semiconductor Doping Profiles in MOS Structures,” SolidState Electron. 16, 124–126, Jan. 1973. 8. D.K. Schroder, Advanced MOS Devices, AddisonWesley, Reading, MA, 1987, 64–71. 9. C.D. Bulucea, “Investigation of DeepDepletion Regime of MOS Structures Using RampResponse Method” Electron. Lett. 6, 479–481, July 1970. 10. G. Baccarani, S. Solmi and G. Soncini, “The Silicon Impurity Profile as Revealed by HighFrequency NonEquilibrium MOS C –V Characteristics,” Alta Frequ. 16, 113–115, Feb. 1972. 11. G.G. Barna, B. Van Eck, and J.W. Hosch, “In situ Metrology,” in Handbook of Silicon Semiconductor Technology (A.C. Diebold, ed.), Dekker, New York, 2001.
110
CARRIER AND DOPING DENSITY
12. M. Rommel, Semitest Inc., private correspondence. 13. K. Woolford, L. Newfield, and C. Panczyk, “Monitoring Epitaxial Resistivity Profiles Without Wafer Damage,” Micro, July/Aug. 2002 (www.micromagazine.com). 14. D.P. Kennedy, P.C. Murley and W. Kleinfelder, “On the Measurement of Impurity Atom Distributions in Silicon by the Differential Capacitance Technique,” IBM J. Res. Develop. 12, 399–409, Sept. 1968. 15. J.R. Brews, “Threshold Shifts Due to Nonuniform Doping Profiles in Surface Channel MOSFET’s,” IEEE Trans. Electron Dev. ED26, 1696–1710, Nov. 1979. 16. D.P. Kennedy and R.R. O’Brien, “On the Measurement of Impurity Atom Distributions by the Differential Capacitance Technique,” IBM J. Res. Develop. 13, 212–214, March 1969. 17. W.E Carter, H.K. Gummel and B.R. Chawla, “Interpretation of Capacitance vs. Voltage Measurements of PN Junctions,” SolidState Electron. 15, 195–201, Feb. 1972. 18. W.C. Johnson and P.T. Panousis, “The Influence of Debye Length on the C –V Measurement of Doping Profiles,” IEEE Trans. Electron Dev. ED18, 965–973, Oct. 1971. 19. E.H. Nicollian, M.H. Hanes and J.R. Brews, “Using the MIS Capacitor for Doping Profile Measurements with Minimal Interface State Error,” IEEE Trans. Electron Dev. ED20, 380–389, April 1973. 20. C.P. Wu, E.C. Douglas and C.W. Mueller, “Limitations of the CV Technique for IonImplanted Profiles,” IEEE Trans. Electron Dev. ED22, 319–329, June 1975. 21. M. Nishida, “Depletion Approximation Analysis of the Differential CapacitanceVoltage Characteristics of an MOS Structure with Nonuniformly Doped Semiconductors,” IEEE Trans. Electron Dev. ED26, 1081–1085, July 1979. 22. G. Baccarani, M. Rudan, G. Spadini, H. Maes, W. Vandervorst and R. Van Overstraeten, “Interpretation of C –V Measurements for Determining the Doping Profile in Semiconductors,” SolidState Electron. 23, 65–71, Jan. 1980. 23. C.L. Wilson, “Correction of Differential Capacitance Profiles for DebyeLength Effects,” IEEE Trans. Electron Dev. ED27, 2262–2267, Dec. 1980. 24. D.J. Bartelink, “Limits of Applicability of the Depletion Approximation and Its Recent Augmentation,” Appl. Phys. Lett. 38, 461–463, March 1981. 25. H. Kroemer and W.Y. Chien, “On the Theory of Debye Averaging in the C –V Profiling of Semiconductors,” SolidState Electron. 24, 655–660, July 1981. 26. J. Voves, V. Rybka and V. Trestikova, “C –V Technique on Schottky Contacts—Limitation of Implanted Profiles,” Appl. Phys. A37, 225–229, Aug. 1985. 27. A.R. LeBlanc, D.D. Kleppinger and J.P. Walsh, “A Limitation of the Pulsed Capacitance Technique of Measuring Impurity Profiles,” J. Electrochem. Soc. 119, 1068–1071, Aug. 1972. 28. K. Ziegler, E. Klausmann and S. Kar, “Determination of the Semiconductor Doping Profile Right Up to Its Surface Using the MIS Capacitor,” SolidState Electron. 18, 189–198, Feb. 1975. 29. ASTM Standard F41994, “Standard Test Method for Net Carrier Density in Silicon Epitaxial Layers by VoltageCapacitance of Gated and Ungated Diodes,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 30. J.P. Sullivan, W.R. Graham, R.T. Tung, and F. Schrey, “Pitfalls in the Measurement of Metal/ pSi Contacts: The Effect of Hydrogen Passivation,” Appl. Phys. Lett. 62, 2804–2806, May 1993; A.S. Vercaemst, R.L. Van Meirhaeghe, W.H. Laflere, and F. Cardon, “Hydrogen Passivation Caused by “Soft” Sputter Etch Cleaning of Si,” SolidState Electron. 38, 983–987, May 1995. 31. R. Dingle, “Confined Carrier Quantum States in Ultrathin Semiconductor Heterostructures,” in Festk¨orperprobleme/Advances in Solid State Physics (H.J. Queisser, ed.), Vieweg, Braunschweig Germany, 15, 1975, 21–48.
REFERENCES
111
32. E.A. Kraut, R.W. Grant, J.R. Waldrop, and S.P. Kowalczyk, “Precise Determination of the ValenceBand Edge in XRay Photoemission Spectra: Application to Measurement of Semiconductor Interface Potentials,” Phys. Rev. Lett. 44, 1620–1623, June 1980. 33. H. Kroemer, W.Y. Chien, J.S. Harris, Jr., and D.D. Edwall, “Measurement of Isotype Heterojunction Barriers by C –V Profiling,” Appl. Phys. Lett. 36, 295–297, Feb. 1980; M.A. Rao, E.J. Caine, H. Kroemer, S.I. Long, and D.I. Babic, “Determination of Valence and Conduction Band Discontinuities at the (Ga,In)P/GaAs Heterojunction by C –V Profiling,” J. Appl. Phys. 61, 643–649, Jan. 1987; D.N. Bychkovskii, O.V. Konstantinov, and M.M. Panakhov, “Method for Determination of the Band Offset at a Heterojunction from CapacitanceVoltage Characteristics of an MS Heterostructure,” Sov. Phys. Semicond. 26, 368–376, April 1992. 34. H. Kroemer, “Determination of Heterojunction Band Offsets by CapacitanceVoltage Profiling Through Nonabrupt Isotype Heterojunctions”, Appl. Phys. Lett. 46, 504–505, March 1985. 35. A. Morii, H. Okagawa, K. Hara, J. Yoshino, and H. Kukimoto, “Band Discontinuity at Alx Ga1−x P/GaP Heterointerfaces Studied by CapacitanceVoltage Measurements,” Japan. J. Appl. Phys. 31, L1161–L1163, Aug. 1992. 36. S.P. Voinigescu, K. Iniewski, R. Lisak, C.A.T. Salama, J.P. Noel, and D.C. Houghton, “New Technique for the Characterization of Si/SiGe Layers Using Heterostructure MOS Capacitors,” SolidState Electron. 37, 1491–1501, Aug. 1994. 37. D.V. Singh, K. Rim, T.O. Mitchell, J.L. Hoyt, and J.F. Gibbons, “Measurement of the Conduction Band Offsets in Si/Si1−x−y Gex Cy and Si/Si1−y Cy Heterostructures Using MetalOxideSemiconductor Capacitors,” J. Appl. Phys. 85, 985–993, Jan. 1999. 38. S. Chattopadhyay, K.S.K. Kwa, S.H. Olsen, L.S. Driscoll and A.G. O’Neill, “C –V Characterization of Strained Si/SiGe Multiple Heterojunction Capacitors as a Tool for Heterojunction MOSFET Channel Design,” Semicond. Sci. Technol. 18, 738–744, Aug. 2003. 39. D.V. Lang, “Measurement of Band Offsets by Space Charge Spectroscopy,” in Heterojunctions and Band Discontinuities (F. Capasso and G. Margaritondo, eds.), North Holland, Amsterdam, 1987, Ch. 9. 40. H. Kroemer, “Heterostructure Devices: A Device Physicist Looks at Interfaces,” Surf. Sci. 132, 543–576, Sept. 1983. 41. W. M¨onch, Electronic Properties of Semiconductor Interfaces, Springer, Berlin 2004, 79–82. 42. E.A. Kraut, R.W. Grant, J.R. Waldrop, and S.P. Kowalczyk, “Precise Determination of the ValenceBand Edge in XRay Photoemission Spectra: Application to Measurement of Semiconductor Interface Potentials,” Phys. Rev. Lett. 44, 1620–1623, June 1980. 43. B.E. Deal, A.S. Grove, E.H. Snow and C.T. Sah, “Observation of Impurity Redistribution During Thermal Oxidation of Silicon Using the MOS Structure,” J. Electrochem. Soc. 112, 308–314, March 1965. 44. K. Iniewski and A. Jakubowski, “Procedure for Determination of a Linear Approximation Doping Profile in a MOS Structure,” SolidState Electron. 30, 295–298, March 1987. 45. A.S. Grove, Physics and Technology of Semiconductor Devices, Wiley, New York, 1967. 46. E.H. Nicollian and J.R. Brews, MOS Physics and Technology, Wiley, New York, 1982. 47. W.E. Beadle, J.C.C. Tsai and R.D. Plummer, Quick Reference Manual for Silicon Integrated Circuit Technology, WileyInterscience, New York, 1985, Ch. 14. 48. J. Shappir, A. Kolodny and Y. ShachamDiamand, “Diffusion Profiling Using the Graded C(V) Method,” IEEE Trans. Electron Dev. ED27, 993–995, May 1980. 49. W.W. Lin, “A Simple Method for Extracting Average Doping Concentration in the Polysilicon and Silicon Surface Layer Near the Oxide in Polysilicon Gate MOS Structures,” IEEE Electron Dev. Lett. 15, 51–53, Feb. 1994.
112
CARRIER AND DOPING DENSITY
50. R.O. Deming and W.A. Keenan, “C –V Uniformity Measurements,” Nucl. Instrum. and Meth. B6, 349–356, Jan. 1985; “Low Dose Ion Implant Monitoring,” Solid State Technol. 28, 163–167, Sept. 1985. 51. R. Sorge, “Implant Dose Monitoring by MOS C –V Measurement,” Microelectron. Rel. 43, 167–171, Jan. 2003. 52. R.S. Nakhmanson and S.B. Sevastianov, “Investigations of MetalInsulatorSemiconductor Structure Inhomogeneities Using a SmallSize Mercury Probe,” SolidState Electron. 27, 881–891, Oct. 1984. 53. J.T.C. Chen, Four Dimensions, private communication; P.S. Schaffer and T.R. Lally, “Silicon Epitaxial Wafer Profiling Using the MercurySilicon Schottky Diode Differential Capacitance Method,” Solid State Technol. 26, 229–233, April 1983. 54. T. Ambridge and M.M. Faktor, “An Automatic Carrier Concentration Profile Plotter Using an Electrochemical Technique,” J. Appl. Electrochem. 5, 319–328, Nov. 1975. 55. P. Blood, “CapacitanceVoltage Profiling and the Characterisation of III–V Semiconductors Using Electrolyte Barriers,” Semicond. Sci. Technol. 1, 7–27, 1986. 56. T. Ambridge and D.J. Ashen, “Automatic Electrochemical Profiling of Carrier Concentration in Indium Phosphide,” Electron. Lett. 15, 647–648, Sept. 1979. 57. R.T. Green, D.K. Walker, and C.M. Wolfe, “An Improved Method for the Electrochemical C –V Profiling of InP,” J. Electrochem. Soc. 133, 2278–2283, Nov. 1986. 58. M.M. Faktor and J.L. Stevenson, “The Detection of Structural Defects in GaAs by Electrochemical Etching,” J. Electrochem. Soc. 125, 621–629, April 1978. 59. T. Ambridge, J.L. Stevenson and R.M. Redstall, “Applications of Electrochemical Methods for Semiconductor Characterization: I. Highly Reproducible Carrier Concentration Profiling of VPE “HiLo” nGaAs,” J. Electrochem. Soc. 127, 222–228, Jan. 1980; A.C. Seabaugh, W.R. Frensley, R.J. Matyi and G.E. Cabaniss, “Electrochemical C –V Profiling of Heterojunction Device Structures,” IEEE Trans. Electron Dev. ED36, 309–313, Feb. 1989. 60. C.D. Sharpe and P. Lilley, “The ElectrolyteSilicon Interface; Anodic Dissolution and Carrier Concentration Profiling,” J. Electrochem. Soc. 127, 1918–1922, Sept. 1980. 61. W.Y. Leong, R.A.A. Kubiak and E.H.C. Parker, “Dopant Profiling of SiMBE Material Using the Electrochemical CV Technique,” in Proc. First Int. Symp. on Silicon MBE, Electrochem. Soc., Pennington, NJ, 1985, pp. 140–148. 62. M. Pawlik, R.D. Groves, R.A. Kubiak, W.Y. Leong and E.H.C. Parker, “A Comparative Study of Carrier Concentration Profiling Techniques in Silicon: Spreading Resistance and Electrochemical CV,” in Emerging Semiconductor Technology (D.C. Gupta and R.P. Langer, eds.), STP 960, Am. Soc. Test. Mat., Philadelphia, 1987, 558–572. 63. A.C. Seabaugh, W.R. Frensley, R.J. Matyi, G.E. Cabaniss, “Electrochemical C –V Profiling of Heterojunction Device Structures,” IEEE Trans. Electron Dev. 36 309–313, Feb. 1989. 64. E. Peiner, A. Schlachetzki, and D. Kr¨uger, “Doping Profile Analysis in Si by Electrochemical CapacitanceVoltage Measurements,” J. Electrochem. Soc. 142, 576–580, Feb. 1995. 65. I. Mayes, “Accuracy and Reproducibility of the Electrochemical Profiler,” Mat. Sci. Eng. B80, 160–163, March 2001. 66. J.M. Shannon, “DC Measurement of the Space Charge Capacitance and Impurity Profile Beneath the Gate of an MOST,” SolidState Electron. 14, 1099–1106, Nov. 1971. 67. M.G. Buehler, “The DC MOSFET Dopant Profile Method,” J. Electrochem. Soc. 127, 701–704, March 1980; M.G. Buehler, “Effect of the DrainSource Voltage on Dopant Profiles Obtained from the DC MOSFET Profile Method,” IEEE Trans. Electron Dev. ED27, 2273–2277, Dec. 1980. 68. H.G. Lee, S.Y. Oh, and G. Fuller, “A Simple and Accurate Method to Measure the Threshold Voltage of an EnhancementMode MOSFET,” IEEE Trans. Electron Dev. ED29, 346–348, Feb. 1982.
REFERENCES
113
69. H.J. Mattausch, M. Suetake, D. Kitamaru, M. MiuraMattausch, S. Kumashiro, N. Shigyo, S. Odanaka, and N. Nakayama, “Simple Nondestructive Extraction of the Vertical ChannelImpurity Profile of SmallSize Metal–Oxide–Semiconductor FieldEffect Transistors,” Appl. Phys. Lett. 80, 2994–2996, April 2002. 70. M. Chi and C. Hu, “Errors in ThresholdVoltage Measurements of MOS Transistors for DopantProfile Determinations,” SolidState Electron. 24, 313–316, April 1981. 71. G.S. Gildenblat, “On the Accuracy of a Particular Implementation of the ShannonBuehler Method,” IEEE Trans. Electron Dev. 36, 1857–1858, Sept. 1989. 72. G.P. Carver, “Influence of ShortChannel Effects on Dopant Profiles Obtained from the DC MOSFET Profile Method,” IEEE Trans. Electron Dev. ED30, 948–954, Aug. 1983. 73. D.W. Feldbaumer and D.K. Schroder, “MOSFET Doping Profiling,” IEEE Trans. Electron Dev. 38, 135–140, Jan. 1991. 74. D.S. Wu, “Extraction of Average Doping Density and Junction Depth in an IonImplanted DeepDepletion Transistor,” IEEE Trans. Electron Dev. ED27, 995–997, May 1980. 75. R.A. Burghard and Y.A. ElMansy, “Depletion Transistor Threshold Voltage as a Process Monitor,” IEEE Trans. Electron Dev. ED34, 940–942, April 1987. 76. H. Jorke and H.J. Herzog, “Carrier Spilling in Spreading Resistance Analysis of Si Layers Grown by MolecularBeam Epitaxy,” J. Appl. Phys. 60, 1735–1739, Sept. 1986. 77. H. Maes, W. Vandervorst and R. Van Overstraeten, “Impurity Profile of Implanted Ions in Silicon,” in Impurity Doping Processes in Silicon (F.F.Y. Wang, ed.) NorthHolland, Amsterdam, 1981, 443–638. 78. E.F. Schubert, J.M. Kuo, and R.F. Kopf, “Theory and Experiment of CapacitanceVoltage Profiling on Semiconductors with Quantum Confinement,” J. Electron. Mat. 19, 521–531, June 1990. 79. A.M. Goodman, “MetalSemiconductor Barrier Height Measurement by the Differential Capacitance Method—One Carrier System,” J. Appl. Phys. 34, 329–338, Feb. 1963. 80. K. Mallik, R.J. Falster, and P.R. Wilshaw, “Schottky Diode Back Contacts for High Frequency Capacitance Studies on Semiconductors,” SolidState Electron. 48, 231–238, Feb. 2004. 81. J.D. Wiley and G.L. Miller, “Series Resistance Effects in Semiconductor CV Profiling,” IEEE Trans. Electron Dev. ED22, 265–272, May 1975. 82. J.D. Wiley, “C –V Profiling of GaAs FET Films,” IEEE Trans. Electron Dev. ED25, 1317–1324, Nov. 1978. 83. S.T. Lin and J. Reuter, “The Complete Doping Profile Using MOS CV Technique,” SolidState Electron. 26, 343–351, April 1983. 84. D.K. Schroder and P. Rai Choudhury, “SilicononSapphire with Microsecond Carrier Lifetimes,” Appl. Phys. Lett. 22, 455–457, May 1973. 85. J.R. Brews, “Correcting InterfaceState Errors in MOS Doping Profile Determinations,” J. Appl. Phys. 44, 3228–3231, July 1973; Y. Zohta, “Frequency Dependence of V /(C −2 ) of MOS Capacitors,” SolidState Electron. 17, 1299–1309, Dec. 1974. 86. B.L. Smith and E.H. Rhoderick, “Possible Sources of Error in the Deduction of Semiconductor Impurity Concentrations from SchottkyBarrier (C, V) Characteristics,” Brit. J. Appl. Phys. D2, 465–467, March 1969. 87. J.A. Copeland, “Diode Edge Effect on DopingProfile Measurements,” IEEE Trans. Electron. Dev. ED17, 404–407, May 1970; W. Tantraporn and G.H. Glover, “Extension of the C –V Doping Profile Technique to Study the Movements of Alloyed Junction and Substrate OutDiffusion, the Separation of Junctions, and Device Area Trimming,” IEEE Trans. Electron Dev. ED35, 525–529, April 1988. 88. E. Simoen, C. Claeys, A. Czerwinski, and J. Katcki, “Accurate Extraction of the Diffusion Current in Silicon pn Junction Diodes,” Appl. Phys. Lett. 72, 1054–1056, March 1998.
114
CARRIER AND DOPING DENSITY
89. P. Kramer, C. deVries and L.J. van Ruyven, “The Influence of Leakage Current on Concentration Profile Measurements,” J. Electrochem. Soc. 122, 314–316, Feb. 1975. 90. D.K. Schroder, T.T. Braggins, and H.M. Hobgood, “The Doping Concentrations of IndiumDoped Silicon Measured by Hall, C –V , and Junction Breakdown Techniques,” J. Appl. Phys. 49, 5256–5259, Oct. 1978. 91. L.C. Kimerling, “Influence of Deep Traps on the Measurement of FreeCarrier Distributions in Semiconductors by Junction Capacitance Techniques,” J. Appl. Phys. 45, 1839–1845, April 1974. 92. G. Goto, S. Yanagisawa, O. Wada and H. Takanashi, “An Improved Method of Determining Deep Impurity Levels and Profiles in Semiconductors,” Japan. J. Appl. Phys. 13, 1127–1133, July 1974. 93. K. Lehovec, “C –V Analysis of a Partially Depleted Semiconducting Channel,” Appl. Phys. Lett. 26, 82–84, Feb. 1975. 94. I. Amron, “Errors in Dopant Concentration Profiles Determined by Differential Capacitance Measurements,” Electrochem. Technol. 5, 94–97, March/April 1967. 95. R.A. Smith, Semiconductors, Cambridge University Press, Cambridge, 1959, Ch. 5. 96. D.L. Rode, C.M. Wolfe and G.E. Stillman, “MagneticField Dependence of the Hall Factor of Gallium Arsenide,” in GaAs and Related Compounds (G.E. Stillman, ed.) Conf. Ser. No. 65, Inst. Phys., Bristol, 1983, pp. 569–572. 97. A. Chandra, C.E.C. Wood, D.W. Woodard and L.F. Eastman, “Surface and Interface Depletion Corrections to Free CarrierDensity Determinations by Hall Measurements,” SolidState Electron. 22, 645–650, July 1979. 98. T.R. Lepkowski, R.Y. DeJule, N.C. Tien, M.H. Kim and G.E. Stillman, “Depletion Corrections in Variable Temperature Hall Measurements,” J. Appl. Phys. 61, 4808–4811, May 1987. 99. E.H. Putley, The Hall Effect and Related Phenomena, Butterworths, London, 1960, p. 106. 100. G.E. Stillman and C.M. Wolfe, “Electrical Characterization of Epitaxial Layers,” Thin Solid Films 31, 69–88, Jan. 1976. 101. T.T. Braggins, H.M. Hobgood, J.C. Swartz and R.N. Thomas, “High Infrared Responsivity IndiumDoped Silicon Detector Material Compensated by Neutron Transmutation,” IEEE Trans. Electron Dev. ED27, 2–10, Jan. 1980. 102. N.D. Young and M.J. Hight, “Automated Hall Effect Profiler for Electrical Characterisation of Semiconductors,” Electron. Lett. 21, 1044–1046, Oct. 1985. 103. R. Baron, G.A. Shifrin, O.J. Marsh, and J.W. Mayer, “Electrical Behavior of Group III and V Implanted Dopants in Silicon,” J. Appl. Phys. 40, 3702–3719, Aug. 1969. 104. R.D. Larrabee and W.R. Thurber, “Theory and Application of a TwoLayer Hall Technique,” IEEE Trans. Electron Dev. ED27, 32–36, Jan. 1980. 105. L.F. Lou and W.H. Frye, “Hall Effect and Resistivity in LiquidPhaseEpitaxial Layers of HgCdTe,” J. Appl. Phys. 56, 2253–2267, Oct. 1984. 106. R.L. Petritz, “Theory of an Experiment for Measuring the Mobility and Density of Carriers in the SpaceCharge Region of a Semiconductor Surface,” Phys. Rev. 110, 1254–1262, June 1958. 107. T.S. Moss, G.J. Burrell and B. Ellis, Semiconductor OptoElectronics, Wiley, New York, 1973, 42–46. 108. ASTM Standard F39882, “Standard Method for Majority Carrier Concentration in Semiconductors by Measurement of Wavelength of the Plasma Resonance Minimum,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 109. T. Abe and Y. Nishi, “NonDestructive Measurement of Surface Concentrations and Junction Depths of Diffused Semiconductor Layers,” Japan. J. Appl. Phys. 7, 397–403, April 1968.
REFERENCES
115
110. A.H. Tong, P.A. Schumann, Jr. and W.A. Keenan, “Epitaxial Substrate Carrier Concentration Measurement by the Infrared Interference Envelope (IRIE) Technique,” J. Electrochem. Soc. 119, 1381–1384, Oct. 1972. 111. P.A. Schumann, Jr., W.A. Keenan, A.H. Tong, H.H. Gegenwarth and C.P. Schneider, “Silicon Optical Constants in the Infrared,” J. Electrochem. Soc. 118, 145–148, Jan. 1971 and references therein; D.K. Schroder, R.N. Thomas and J.C. Swartz, “Free Carrier Absorption in Silicon,” IEEE Trans. Electron Dev. ED25, 254–261, Feb. 1978. 112. J. Isenberg and W. Warta, “Free Carrier Absorption in HeavilyDoped Silicon Layers,” Appl. Phys. Lett. 84, 2265–2267, March 2004. 113. D.C. Look, D.C. Walters, M.G. Mier, and J.R. Sizelove, “Nondestructive Mapping of Carrier Concentration and Dislocation Density in n+ type GaAs,” Appl. Phys. Lett. 65, 2188–2190, Oct. 1994. 114. J.L. Boone, M.D. Shaw, G. Cantwell and W.C. Harsh, “Free Carrier Density Profiling by Scanning Infrared Absorption,” Rev. Sci. Instrum. 59, 591–595, April 1988. 115. E. Burstein, G. Picus, B. Henvis and R. Wallis, “Absorption Spectra of Impurities in Silicon; I. Group III Acceptors,” J. Phys. Chem Solids 1, 65–74, Sept/Oct. 1956; G. Picus, E. Burstein and B. Henvis, “Absorption Spectra of Impurities in Silicon; II. Group V Donors,” J. Phys. Chem Solids 1, 75–81, Sept/Oct. 1956. 116. H.J. Hrostowski and R.H. Kaiser, “Infrared Spectra of Group III Acceptors in Silicon,” J. Phys. Chem. Solids 4, 148–153, 1958. 117. S.C. Baber, “Net and Total Shallow Impurity Analysis of Silicon by Low Temperature Fourier Transform Infrared Spectroscopy,” Thin Solid Films 72, 201–210, Sept. 1980; ASTM Standard F163095, “Standard Test Method for Low Temperature FTIR Analysis of Single Crystal Silicon for III–V Impurities,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., West Conshohocken, PA, 1996. 118. T.S. Low, M.H. Kim, B. Lee, B.J. Skromme, T.R. Lepkowski and G.E. Stillman, “Neutron Transmutation Doping of High Purity GaAs,” J. Electron. Mat. 14, 477–511, Sept. 1985. 119. J.J. White, “Effects of External and Internal Electric Fields on the Boron Acceptor States in Silicon,” Can. J. Phys. 45, 2695–2718, Aug. 1967; “AbsorptionLine Broadening in BoronDoped Silicon,” Can. J. Phys. 45, 2797–2804, Aug. 1967. 120. B.O. Kolbesen, “Simultaneous Determination of the Total Content of Boron and Phosphorus in HighResistivity Silicon by IR Spectroscopy at Low Temperatures,” Appl. Phys. Lett. 27, 353–355, Sept. 1975. 121. G.E. Stillman, C.M. Wolfe and J.O. Dimmock, “Far Infrared Photoconductivity in High Purity GaAs,” in Semiconductors and Semimetals (R.K. Willardson and A.C. Beer, eds.) Academic Press, New York, 12, 169–290, 1977. 122. M.J.H. van de Steeg, H.W.H.M. Jongbloets, J.W. Gerritsen and P. Wyder, “Far Infrared Photothermal Ionization Spectroscopy of Semiconductors in the Presence of Intrinsic Light,” J. Appl. Phys. 54, 3464–3474, June 1983. 123. E.E. Haller, “Semiconductor Physics in UltraPure Germanium,” in Festk¨orperprobleme 26 (P. Grosse, ed.), Vieweg, Braunschweig, 1986, 203–229. 124. S.M. Kogan and T.M. Lifshits, “Photoelectric Spectroscopy—A New Method of Analysis of Impurities in Semiconductors,” Phys. Stat. Sol. (a) 39, 11–39, Jan. 1977. 125. K.K. Smith, “Photoluminescence of Semiconductor Materials,” Thin Solid Films 84, 171–182, Oct. 1981. 126. M. Tajima, “Determination of Boron and Phosphorus Concentration in Silicon by Photoluminescence Analysis,” Appl. Phys. Lett. 32, 719–721, June 1978.
116
CARRIER AND DOPING DENSITY
127. G. Pickering, P.R. Tapster, P.J. Dean and D.J. Ashen, “Determination of Impurity Concentration in nType InP by a Photoluminescence Technique,” in GaAs and Related Compounds (G.E. Stillman, ed.) Conf. Ser. No. 65, Inst. Phys., Bristol, 1983, 469–476. 128. M. Tajima, T. Masui, T. Abe and T. Iizuka, “Photoluminescence Analysis of Silicon Crystals,” in Semiconductor Silicon 1981 (H.R. Huff, R.J. Kriegler and Y. Takeishi, eds.) Electrochem. Soc., Pennington, NJ, 1981, 72–89. 129. M. Pawlik, “Dopant Profiling in Silicon,” in Semiconductor Processing, ASTM STP 850 (D.C. Gupta, ed.) Am. Soc. Test. Mat., Philadelphia, PA, 1984, 391–408. 130. S.B. Felch, R. Brennan, S.F. Corcoran, and G. Webster, “A Comparison of Three Techniques for Profiling Ultrashallow p+ n Junctions,” Solid State Technol. 36, 45–51, Jan. 1993. 131. E. Ishida and S.B. Felch, “Study of Electrical Measurement Techniques for UltraShallow Dopant Profiling,” J. Vac. Sci. Technol. B14, 397–403, Jan./Feb. 1996; S.B. Felch, D.L. Chapek, S.M. Malik, P. Maillot, E. Ishida, and C.W. Mageee, “Comparison of Different Analytical Techniques in Measuring the Surface Region of Ultrashallow Doping Profiles,” J. Vac. Sci. Technol. B14, 336–340, Jan./Feb.1996. 132. E.J.H. Collart, K. Weemers, D.J. Gravesteijn, and J.G.M. van Berkum, “Characterization of Lowenergy (100 eV–10 keV) Boron Ion Implantation,” J. Vac. Sci. Technol. B16, 280–285, Jan./Feb. 1998. 133. W. Vandervorst and T. Clarysse, “On the Determination of Dopant/Carrier Distributions,” J. Vac. Sci. Technol. B10, 302–315, Jan./Feb. 1992. 134. H. Norstr¨om, K. Maex, J. Vanhellemont, G. Brijs, W. Vandervorst, and U. Smith, “Simultaneous Formation of Contacts and Diffusion Barriers for VLSI by Rapid Thermal Silicidation of TiW,” Appl. Phys., A51, 459–466, Dec. 1990. 135. R. Subrahmanyan and M. Duane, “Issues in TwoDimensional Dopant Profiling,” in Diagnostic Techniques for Semiconductor Materials and Devices 1994 (D.K. Schroder, J.L. Benton, and P. RaiChoudhury, eds.), Electrochem. Soc., Pennington, NJ, 1994, 65–77. 136. R. Subrahmanyan, “Methods for the Measurement of TwoDimensional Doping Profiles,” J. Vac. Sci. Technol. B10, 358–368, Jan./Feb. 1992. 137. A.C. Diebold, M.R. Kump, J.J. Kopanski, and D.G. Seiler, “Characterization of TwoDimensional Dopant Profiles: Status and Review,” J. Vac. Sci. Technol. B14, 196–201, Jan./Feb.1996. 138. M. Barrett, M. Dennis, D. Tiffin, Y. Li, and C.K. Shih, “TwoDimensional Dopant Profiling of Very Large Scale Integrated Devices Using Selective Etching and Atomic Force Microscopy,” J. Vac. Sci. Technol. B14, 447–451, Jan./Feb.1996. 139. W. Vandervorst, T. Clarysse, P. De Wolf, L. Hellemans, J. Snauwaert, V. Privitera, and V. Raineri, “On the Determination of TwoDimensional Carrier Distributions,” Nucl. Instrum. Meth. B96, 123–132, March 1995. 140. C.C. Williams, TwoDimensional Dopant Profiling by Scanning Capacitance Microscopy,” Annu. Rev. Mater. Sci. 29, 471–504, 1999. 141. W. Vandervorst, P. Eyben, S. Callewaert, T. Hantschel, N. Duhayon, M. Xu, T. Trenkler and T. Clarysse, “Towards Routine, Quantitative Twodimensional Carrier Profiling with Scanning Spreading Resistance Microscopy,” in Characterization and Metrology for ULSI Technology, (D.G. Seiler, A.C. Diebold, T.J. Shaffner, R. McDonald, W.M. Bullis, P.J. Smith, and E.M. Secula, eds.), Am. Inst. Phys. 550, 613–619, 2000. 142. G. Neubauer, A. Erickson, C.C. Williams, J.J. Kopanski, M. Rodgers, and D. Adderton, “TwoDimensional Scanning Capacitance Microscopy Measurements of CrossSectioned Very Large Scale Integration Test Structures,” J. Vac. Sci. Technol. B14, 426–432, Jan./Feb.1996; J.S. McMurray, J. Kim, and C.C. Williams, “Quantitative Measurement of Twodimensional Dopant Profile by Crosssectional Scanning Capacitance Microscopy,” J. Vac. Sci. Technol. B15, 1011–1014, July/Aug. 1997.
PROBLEMS
117
PROBLEMS The C –V curve of a Schottky diode on a ptype Si substrate is shown in Fig. P2.1(a) and (b). The C –V data are also given in tabular form. Determine the p(x) versus x profile for this device; plot as log[p(x)] in cm−3 versus W in µm. Ks = 11.7, A = 10−3 cm2 . V (V )
C (F )
V (V )
C (F )
V (V )
C (F )
0 0.94 2.16 3.52 4.93 6.34 7.69 8.96 10.14 11.21 12.18 13.05 13.81 14.49
8.39e11 4.63e11 3.20e11 2.44e11 1.97e11 1.66e11 1.43e11 1.26e11 1.12e11 1.01e11 9.22e12 8.47e12 7.83e12 7.28e12
15.09 15.62 16.07 16.47 16.81 17.36 17.84 18.17 18.39 19.06 20.31 21.60 23.11 24.65
6.80e12 6.38e12 6.01e12 5.68e12 5.38e12 4.88e12 4.36e12 3.95e12 3.60e12 3.32e12 3.07e12 2.86e12 2.67e12 2.51e12
26.29 28.03 29.86 31.79 33.82 35.94 38.16 40.48 42.89 45.40 48.01 50.71
2.37e12 2.24e12 2.12e12 2.02e12 1.93e12 1.84e12 1.76e12 1.69e12 1.62e12 1.56e12 1.51e12 1.45e12
8 × 10−11
C(F)
6 × 10−11 4 × 10−11 2 × 10−11
0
0
10
20 V(V)
30
40
30
40
(a) 2 × 10−11
C(F)
2.1
1 × 10−11
0
0
10
20 V(V) (b)
Fig. P2.1
118
The C –V curves and data of the devices in Fig. P2.2 are given. C is the total capacitance. Determine distance d (in cm), doping density NA (in cm−3 ), and builtin potential Vbi (in V ). Ks = 11.7, Kair = 1, A = 10−3 cm2 . The semiconductor capacitance is given by qKs εo NA . Cs = A 2(Vbi + V ) V (V )
C (F )
V (V )
C (F )
V (V )
C (F )
V (V )
C (F )
0 0.2 0.4 0.6 0.8 1 1.2 1.4 1.6 1.8 2 2.2 2.4 2.6
2.276E11 2.036E11 1.858E11 1.720E11 1.609E11 1.517E11 1.439E11 1.372E11 1.314E11 1.262E11 1.217E11 1.175E11 1.138E11 1.104E11
2.8 3 3.2 3.4 3.6 3.8 4 4.4 4.8 5.2 5.6 6.0 6.4 6.8
1.073E11 1.044E11 1.018E11 9.933E12 9.704E12 9.491E12 9.291E12 8.927E12 8.602E12 8.310E12 8.046E12 7.806E12 7.586E12 7.384E12
0.000 0.430 0.820 1.183 1.527 1.857 2.175 2.485 2.787 3.083 3.374 3.660 3.942 4.221
9.959E12 9.470E12 9.067E12 8.726E12 8.431E12 8.171E12 7.940E12 7.732E12 7.543E12 7.370E12 7.211E12 7.064E12 6.928E12 6.800E12
4.496 4.769 5.039 5.307 5.573 5.837 6.099 6.359 6.618 6.876 7.132 7.387 7.640 4.496
6.681E12 6.569E12 6.463E12 6.363E12 6.269E12 6.179E12 6.094E12 6.013E12 5.935E12 5.861E12 5.790E12 5.721E12 5.656E12 6.681E12
V V d
NA
NA
(a)
(b)
2 × 10−11 C (F)
2.2
CARRIER AND DOPING DENSITY
(a)
1 × 10−11
(b) 0 × 100
0
2
4
6 V (V)
Fig. P2.2
8
10
119
PROBLEMS
2.3
For a ptype Si MIS capacitor, Cinv /Cins = 0.32 and tins = 30 nm; “ins” stands for the insulator, which is not SiO2 in this case. (a) Determine the doping density for this device using Kins = 8, Ks = 11.7, ni = 1010 cm−3 , A = 10−3 cm2 , and T = 27◦ C. (b) Determine Cinv /Cins when NA = 1016 cm−3 . Use the approach that leads to Eq. (2.18) in the textbook for this problem. (c) Use Eq. (2.19) to determine NA instead of Eq. (2.18).
2.4
The C –V and 1/C 2 –V curves of a Schottky diode on a uniformlydoped substrate, doped to NA , are shown in Fig. P2.4. Draw the C –V and 1/C 2 –V curves on the same figures for the case of a ptype layer (doped to NA ) grown on a ptype substrate (doped to NA1 ) for (a) NA > NA1 and (b) NA < NA1 . The voltage required to deplete the player is shown by the vertical dashed line.
NA NA1 1/C2
C
V
V
Fig. P2.4
2.5
For a ptype Si MIS capacitor, Cinv /Cins = 0.116 and tins = 100 nm; “ins” stands for the insulator, which is not SiO2 in this case. (a) Determine the doping density NA (in cm−3 ) for this device. Use the approach that leads to Eq. (2.18) in the textbook for this problem. NA =
2 2 1 − Cinv 4φF 4φF R 2 Cox = . qKs εo A2 (1 − Cinv /Cox )2 qKs εo A2 (1 − R)2
(2.18)
(b) Use Eq. (2.19) to determine NA instead of Eq. (2.18). log(NA ) = 30.38759 + 1.68278 log(C1 ) − 0.03177[log(C1 )]2 .
(2.19)
(c) Determine Cinv /Cins when NA = 1016 cm−3 for tins = 100 nm. Use: Kins = 15, Ks = 11.7, ni = 1010 cm−3 , A = 10−3 cm2 , and T = 300 K. 2.6
The capacitance and conductance of semiconductor junction devices are usually measured using the device in Fig. P2.6(a) and its equivalent circuit in Fig. P2.6(b). A capacitance meter assumes the device is represented by the equivalent circuit in Fig. P2.6(c). Such a device can cause measurement problems due to series resistance at the bottom surface, i.e., where the wafer touches the probe station wafer holder,
120
CARRIER AND DOPING DENSITY
G
C
Gm
Cm
rs (a)
(c)
(b)
G
C
Gm
Cm
rs Cb (d)
(e)
(f)
Fig. P2.6
especially if the wafer is not metallized on the back. Such problems can be alleviated by making a capacitive, rather than a resistive contact, as shown in Fig. P2.6(d). (a) Derive expressions for Gm and Cm in Fig. P2.6(f) in terms of G, C, rs , and Cb in P2.6(e). (b) Find the minimum back capacitance Cb for this capacitance not to influence the measured capacitance and conductance, i.e., introduce an error of not more than 1%. (c) What area must be used for Cb if it is an oxide capacitance having an oxide thickness of 100 nm? Kox = 3.9. Use C = 100 pF, G = 10−6 S, f = 1 MHz, rs = 100 . The C –VG curve of an MOS capacitor (for positive VG only) with uniformly doped substrate is shown in Fig. P2.7. Determine the doping density NA using: (i) Eq. (2.5); (ii) Eq. (2.18); (iii) Eq. (2.19). A = 5 × 10−4 cm2 , Ks = 11.7, Kox = 3.9, ni = 1010 cm−3 , VF B = 0. 75 Cox = 98.7 pF
50 C (pF)
2.7
25
0
23.9 pF
0
0.5
1 VG (V)
Fig. P2.7
1.5
2
PROBLEMS
The capacitance—voltage plot of a Schottky diode on a ptype substrate is shown in P2.8.
Capacitance
2.8
121
Voltage Fig. P2.8
(a) Plot 1/C 2 –V and NA x for this device qualitatively. (b) Next plot, again qualitatively, the C –V curve and the 1/C 2 –V curve for another Schottky diode on a ptype substrate with layers 1, 2, and 3 having doping densities NA1 > NA2 , NA2 < NA3 , NA1 < NA3 . 2.9
The C –VG curve in Problem 2.7 was obtained with a structure of the type shown in Fig. P2.9(a). What would the curve look like for structure in P2.9(b)? Explain. The bottom area ≫ top area. Metal SiO2 Ohmic Contact
Identical Oxide Thickness
Si
(a)
(b) Fig. P2.9
2.10 The threshold voltage VT of an nchannel MOSFET is given as a function of body or back bias voltage VBS . Determine the doping density NA and the flatband voltage VF B . tox = 25 nm, Kox = 3.9, Ks = 11.7, ni = 1010 cm−3 , T = 300 K. VBS (V )
0
−2
−4
−6
−8
−10
−12
−14
−16
−18
−20
VT (V )
0.61
1.17
1.55
1.85
2.11
2.34
2.55
2.75
2.93
3.1
3.26
122
CARRIER AND DOPING DENSITY
2.11 The capacitance of a semiconductor device with series resistance is measured as Cm . The data are shown in Fig. P2.11. Determine the true capacitance C and the series resistance rs of this device. 103
Cm (pF)
102
101
100 3 10
104
105 Frequency (Hz)
106
107
Fig. P2.11
2.12 Someone wants to measure the majority carrier profiles of the structures shown in Fig. P2.12 by C –V profiling. The voltages during the C –V measurements are such that the spacecharge region width is confined to the pregion in each case. Comment on the validity of the conventional approach to C –V measurements, i.e., will the correct profile be obtained in each case? Explain why or why not. The spacecharge region width is contained within the ptype layer in each case and series resistance is negligible.
ptype ptype p+type (a)
(b)
ptype
ptype
p−type
ntype
(c)
(d)
Fig. P2.12
PROBLEMS
123
2.13 (a) Calculate and plot C vs. V and 1/C 2 vs. V for the Schottky barrier diode in Fig. P2.13 from 0 to 50 V for NA1 = 1015 cm−3 and (i) NA2 = 1014 cm−3 , (ii) NA2 = 1015 cm−3 , (iii) NA2 = 1016 cm−3 . Draw all three curves on the same figure. (b) Calculate VBD , the avalanchelimited breakdown voltage, for each case. Electric field at avalanche breakdown = 3 × 105 V/cm, A = 10−3 cm2 , Ks = 11.7, Vbi = 0.4 V. V
NA2
NA1 3 µm
Fig. P2.13
Hint: Starting with Poisson’s equation, find a relationship between the spacecharge region width W and the applied voltage V using the depletion approximation. Then C = Ks ε0 A/W . 2.14 Calculate and plot C vs. V and 1/C 2 vs. V for the Schottky barrier diode in Fig. P2.13 with the NA1 layer thickness of 1 µm from V = 0 to 28 V for NA1 (x) = 2 × 1016 exp(−kx) cm−3 and NA2 = 1014 cm−3 . k = 104 cm−1 , A = 10−3 cm2 , Ks = 11.7, Vbi = 0.5 V. Hint: Starting with Poisson’s equation, find a relationship between the spacecharge region width W and the applied voltage V using the depletion approximation. Then C = Ks ε0 A/W . 2.15 The error ε in the determination of the doping density NA by the C –V profiling technique is given by 1.4p ε= C/C where p is the measurement precision. (a) Derive and plot log(ε) versus log(W ), where W is the spacecharge region width in microns and ε is in %, for: (a) C = 10−14 F = constant, (b) W = 10−5 cm = constant, (c) V = 0.015 V = constant. (b) If you had a choice, which of these three approaches would you use for best accuracy? (c) In your opinion, which one of these three approaches is easiest to implement? Use p = 0.1%, NA = 1015 cm−3 , Ks = 11.7, A = 10−3 cm2 . The following relationships may be useful: C= Use 1 µm ≤ W ≤ 10 µm.
2Ks εo V Ks εo A ; W2 = W qNA
124
CARRIER AND DOPING DENSITY
10−9
10−2
10−10
10−3
10−11 106
Frequency (Hz)
Conductance (S)
Capacitance (F)
2.16 The capacitance and conductance of an MOS capacitor were measured and are shown in Fig. P2.16. Determine the true capacitance C, the true conductance G and the series resistance rs .
10−4 107
Fig. P2.16
2.17 In the MOSFET threshold voltage doping profiling method, the threshold voltage VT was measured as function of the substrate bias voltage VBS . The data are: VBS (V )
VT (V )
0 −1 −2 −3 −4 −5 −6 −7 −8 −9 −10
2.40 2.84 3.17 3.42 3.64 3.85 4.05 4.22 4.36 4.54 4.70
Determine the doping density profile and the flatband voltage VF B . tox = 20 nm, Kox = 3.9, Ks = 11.7, ni = 1010 cm−3 , T = 300 K. REVIEW QUESTIONS • How is the capacitance measured?
• Why is 1/C 2 –V preferred over C –V ?
• What is important in contactless C –V ?
• What is measured in most profiling techniques, i.e., doping density or majority carrier
density?
• What is the Debye length?
• What is measured in the “equilibrium” MOSC C –VG method?
REVIEW QUESTIONS
• What does series resistance do to capacitance measurements?
• What advantage does the electrochemical profiling technique have? • How does the threshold voltage technique work? • What determines the profiling limits?
• What is the Hall effect and how does it work? • What is secondary ion mass spectrometry?
• How does spreading resistance profiling work?
125
3 CONTACT RESISTANCE AND SCHOTTKY BARRIERS
3.1
INTRODUCTION
Since all semiconductor devices have contacts and all contacts have contact resistance, it is important to characterize such contacts. Contacts are generally metalsemiconductor contacts, but they may be semiconductorsemiconductor contacts, where both semiconductors can be single crystal, polycrystalline, or amorphous. In the conceptual discussion of ohmic contacts and contact resistance we will be mainly concerned with metalsemiconductor contacts because they are most common. For the discussion of the measurement techniques the type of contact is unimportant, but the resistance of the contact material is important. The metalsemiconductor contact, discovered by Braun in 1874, forms the basis of one of the oldest semiconductor devices.1 The first acceptable theory was developed by Schottky in the 1930s.2 In his honor metalsemiconductor devices are frequently referred to as Schottky barrier devices. Usually this name denotes the use of these devices as rectifiers with distinctly nonlinear currentvoltage characteristics. A good discussion of the history of metalsemiconductor devices is given by Henisch3 with a more recent review by Tung.4 Ohmic contacts have linear or quasilinear currentvoltage characteristics. It is not necessary, however, that ohmic contacts have linear I –V characteristics. The contacts must be able to supply the necessary device current, and the voltage drop across the contact should be small compared to the voltage drops across the active device regions. An ohmic contact should not degrade the device to any significant extent, and it should not inject minority carriers. Appendix 3.2 lists various metalsemiconductor contacts. The first comprehensive publication on ohmic contacts was the result of a conference devoted to this topic.5 The theory of metalsemiconductor contacts with emphasis Semiconductor Material and Device Characterization, Third Edition, by Dieter K. Schroder Copyright 2006 John Wiley & Sons, Inc.
127
128
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
on ohmic contacts was presented by Rideout.6 Ohmic contacts to III–V devices were reviewed by Braslau7 and Piotrowska et al.,8 and ohmic contacts to solar cells were discussed by Schroder and Meier.9 Yu and Cohen have presented discussions of contact resistance.10 – 11 Additional information can be found in the books by Milnes and Feucht,12 Sharma and Purohit,13 and Rhoderick.14 Cohen and Gildenblat give a very good discussion.15
3.2
METALSEMICONDUCTOR CONTACTS
The Schottky model of the metalsemiconductor barrier is shown in Fig. 3.1. The energy bands are shown before contact in the upper part of the figure and after contact in the lower part. We assume intimate contact between the metal and the semiconductor with no interfacial layer. The work function of a solid is defined as the energy difference between the vacuum level and the Fermi level. Work functions for the metal and the semiconductor are shown in Fig. 3.1, with the metal work function M being less than the semiconductor work function S in Fig. 3.1(a). The work function is given as the energy M related to the potential φM by φM = M /q. In Fig. 3.1(b) φM = φS , and in Fig. 3.1(c) φM > φS . The ideal barrier height after contact for this model is given by2, 16 φB = φM − χ
(3.1)
where χ is the electron affinity of the semiconductor, defined as the potential difference between the bottom of the conduction band and the vacuum level at the semiconductor surface. According to the Schottky theory, the barrier height depends only on the metal work function and on the semiconductor electron affinity and is independent of the semiconductor doping density. This should make it easy to vary the barrier height by merely using metals of the appropriate work function to implement any one of the three barrier types of Fig. 3.1. We have named them accumulation, neutral, and depletion contacts
FM
c
FS EC EF
EF
EV
fB
Vbi Accumulation (a)
Neutral (b)
W Depletion (c)
Fig. 3.1 Metalsemiconductor contacts according to the simple Schottky model. The upper and lower parts of the figure show the metalsemiconductor system before and after contact, respectively.
METALSEMICONDUCTOR CONTACTS
qfB
EC EF EV
qfB nType Fig. 3.2
129
pType
Depletiontype contacts on n and ptype substrates.
because the majority carriers are accumulated, unchanged (neutral), or depleted compared to their density in the neutral substrate. As is evident from Fig. 3.1 an accumulationtype contact is the preferred ohmic contact because electrons in the metal encounter the least barrier to their flow into or out of the semiconductor. In practice it is difficult to alter the barrier height by using metals of varying work functions. It is experimentally observed that the barrier height for the common semiconductors Ge, Si, GaAs, and other III–V materials is relatively independent of the work function of the metal.17 A depletion contact is generally formed on both ntype and ptype substrates, as shown in Fig. 3.2. For nsubstrates φB ≈ 2Eg /3 and for psubstrates φB ≈ EG /3.18 The relative constancy of the barrier height with various work function metals is sometimes attributed to Fermi level pinning, where the Fermi level in the semiconductor is pinned at some energy in the band gap to create a depletiontype contact. The details of Schottky barrier formation are not fully understood. It appears, however, that imperfections at the semiconductor surface play an important role during contact formation. Bardeen pointed out the importance of surface states in determining the barrier height.19 Such surface states may be dangling bonds at the surface or some other types of defects.17, 20 There is, however, still disagreement between the various proposed mechanisms causing Fermi level pinning.21 – 23 Whatever the mechanisms that cause barrier heights to be relatively independent of the metal work function, it is difficult to engineer an accumulationtype contact. Barrier height engineering being impractical, we must look to other means of implementing ohmic contacts. Ohmic contacts are frequently defined as regions of high recombination rates. This implies that highly damaged regions should serve as good ohmic contacts. Such fabrication methods are not practical because damage is usually the last thing one wants in a semiconductor device. Damageinduced ohmic contacts are also not reproducible. This leaves the semiconductor doping density as the only alternative to engineer contacts.24 As stated earlier, the barrier height is relatively independent of the doping density, but the barrier width does depend on the doping density. The barrier height does actually depend weakly on doping density through image force barrier lowering. Heavily doped semiconductors have narrow spacecharge region (scr) width W (W ∼ ND −1/2 ). For metalsemiconductor contacts with narrow scr widths, electrons can tunnel from the metal to the semiconductor and from the semiconductor to the metal. Holes tunnel for ptype semiconductors. Some readers may be uncomfortable with the concept of holes tunneling from a metal to a semiconductor. It may be helpful to think of hole tunneling from the metal to the semiconductor as electron tunneling from the semiconductor valence band to the metal.
130
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
Low ND Thermionic Emission
Intermediate ND Thermionic/Field Emission
High ND Field Emission
(a)
(b)
(c)
Fig. 3.3 Depletiontype contacts to ntype substrates with increasing doping concentrations. The electron flow is schematically indicated by the electrons and their arrows.
The conduction mechanisms for a metalntype semiconductor are illustrated in Fig. 3.3. For lightlydoped semiconductors the current flows as a result of thermionic emission (TE) shown in Fig. 3.3(a) with electrons thermally excited over the barrier.25 In the intermediate doping range thermionicfield emission (TFE) dominates with carriers thermally excited to an energy where the barrier is sufficiently narrow for tunneling to take place.26 – 27 For high doping densities the barrier is sufficiently narrow at or near the bottom of the conduction band for the electrons to tunnel directly, known as field emission (FE). The three regimes can be differentiated by considering the characteristic energy E00 defined by26
E00
qh = 4π
N = 1.86 × 10−11 Ks εo m∗tun
N(cm−3 ) [eV] Ks (m∗tun /m)
(3.2)
where N is the doping density, m∗ tun is the tunneling effective mass, and m the free electron mass. Equation (3.2) is plotted in Fig. 3.4. A comparison of E00 to the thermal energy kT shows thermionic emission to dominate for kT ≫ E00 , for thermionicfield emission kT ≈ E00 and for field emission kT ≪ E00 . For simplicity we have chosen the demarcation points on Fig. 3.4 as: for TE: E00 ≤ 0.5 kT, for TFE: 0.5 kT < E00 < 5 kT, and for FE: E00 ≥ 5 kT. For Si with a tunneling effective mass of 0.3 m,28 this corresponds
E00, kT (eV)
100
10−1
TE
FE
TFE kT
10−2
E00 10−3 1016
1017
1018
1019
Doping Density
Fig. 3.4
1020
1021
(cm−3)
E00 and kT as a function of doping density for Si with m∗ tun /m = 0.3. T = 300 K.
CONTACT RESISTANCE
n+
Fig. 3.5
131
nType
A metaln+ n semiconductor contact band diagram.
approximately to TE for N ≤ 3 × 1017 cm−3 , TFE for 3 × 1017 < N < 2 × 1020 cm−3 , and FE for N ≥ 2 × 1020 cm−3 . The tunneling effective mass differs for nSi and pSi and also depends on doping density. The structure of Fig. 3.3(c) is not realized in most real contacts. Generally only the semiconductor directly under the contact is heavily doped; the region farther from the contact being less heavily doped as illustrated in Fig. 3.5. The contact resistance becomes the sum of the metalsemiconductor contact resistance and the n+ n junction resistance. Such a structure has a contact resistance similar to a uniformly doped structure if the metalsemiconductor junction resistance dominates.29 However, the contact resistance dependence on doping density is expected to be different when the n+ n junction dominates over the metalsemiconductor junction. The inverse dependence of contact resistance on doping density has been attributed to the resistance of the highlow junction.30 – 31
3.3
CONTACT RESISTANCE
Metalsemiconductor contacts fall into two basic categories, illustrated in Fig. 3.6. The current flows either vertically or horizontally into the contact. Vertical and horizontal or lateral contacts can behave quite differently, because the effective contact area may differ from the true contact area. Let us consider the resistance between points A and B of the sample having metallic conductors lying on an insulator and making ohmic contacts to an ntype layer in a ptype substrate in Fig. 3.7. We divide the total resistance RT between points A and B into three components: (1) the resistance of the metallic conductor Rm , (2) the contact resistances Rc , and (3) the semiconductor resistance Rsemi . The total resistance is (3.3) RT = 2Rm + 2Rc + Rsemi
n I
(a)
Fig. 3.6
n
I p
p
(b)
(a) “Vertical” and (b) “horizontal” contact.
132
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
Rm
Rm
A
B Rsemi Rc
n Rc p
Fig. 3.7 A schematic diagram showing two contacts to a diffused semiconductor layer, with the metal resistance, the contact resistances and the semiconductor resistance indicated.
The semiconductor resistance is determined by the sheet resistance of the nlayer. The contact resistance is less clearly defined. It certainly includes the resistance of the metalsemiconductor contact, sometimes called the specific interfacial resistivity ρi .10 But it also includes a portion of the metal immediately above the metalsemiconductor interface, a part of the semiconductor below that interface, current crowding effects, and any interfacial oxide or other layer that may be present between the metal and the semiconductor. How then do we define contact resistance? The current density J of a metalsemiconductor contact depends on the applied voltage V , the barrier height φB and the doping density ND in a manner that varies for each of the three conduction mechanisms in Fig. 3.3. We write that dependence as J = f (V , φB , ND )
(3.4)
The contact resistance is characterized by two quantities: the contact resistance (ohms) and the specific contact resistivity, ρc (ohm·cm2 ), sometimes referred to as contact resistivity or specific contact resistance. The specific contact resistivity includes not only the actual interface but the regions immediately above and below the interface. We define a specific interfacial resistivity ρi (ohm·cm2 ) by
ρi =
∂V ∂J V =0
(3.5a)
As we will see later, the contact area also plays a role in the behavior of the contact. Hence ρi is also defined as ∂V ρi = (3.5b) ∂J A→0
where A is the contact area. This specific interfacial resistivity is a theoretical quantity referring to the metalsemiconductor interface only. It is not actually measurable because of the effects referred to above. The parameter that is determined from measured contact resistance is the specific contact resistivity. It is a very useful term for ohmic contacts because it is independent of contact area and is a convenient parameter when comparing contacts of various sizes. We will use ρi only when deriving theoretical expressions of metalsemiconductor contacts. Thereafter we use ρc when discussing real contacts, their measurements, and measurement interpretations.
CONTACT RESISTANCE
133
The current density of a metalsemiconductor contact, dominated by thermionic emission, is given in its simplest form by14 J = A∗ T 2 e−qφB /kT (eqV /kT − 1)
(3.6)
where A∗ = 4πqk 2 m∗ /h3 = 120(m∗ /m) A/cm2 ·K2 is Richardson’s constant, m is the free electron mass, m∗ the effective electron mass, and T the absolute temperature. With Eq. (3.5a) we find the specific interfacial resistivity for thermionic emission to be ρi (T E) = ρ1 eqφB /kT ; ρ1 =
k qA∗ T
(3.7)
For thermionicfield emission ρi is given by9 ρi (TFE ) = C1 ρ1 eqφB /E0
(3.8)
ρi (F E) = C2 ρ1 eqφB /E00
(3.9)
and for field emission it is9
C1 and C2 are functions of ND , T , and φB . E0 in Eq. (3.8) is related to E00 by26 E0 = E00 coth (E00 /kT )
(3.10)
Substituting for E00 in Eq. (3.9) leads to √ ρi (F E) ∼ exp(C3 / N)
(3.11)
where C3 is a constant and N the doping density under the contact. The actual expression for ρi (F E) is more complex.28 We give merely the very simplest forms here to indicate the dependence of ρi on doping density and barrier height. As Eq. (3.11) indicates, ρi (F E) is very sensitive to the doping density under the contact. N should be as high as possible for lowest specific interfacial resistivity. We have given the specific interfacial resistivity by these simple expressions in order not to obscure the main points in this discussion. More complex relations are available for the interested reader.28, 32 – 34 The detailed expressions for the various conduction mechanisms are rather complicated and a calculation of the specific interfacial resistivity for each of the three regions is difficult. Various approximations have been proposed and theoretical curves of ρi versus NA or ND have been generated.28, 32 – 34 These curves depend on the effective masses, the barrier height, and various other parameters. The barrier height depends also on the contact metal, and it is therefore impossible to derive “universal” ρi versus NA or ρi versus ND curves. Those that have been derived do not always agree with experimental data. We show in Figs. 3.8 experimental ρc versus ND and NA data for Si. There is considerable scatter, but a definite trend of lower specific contact resistivity with higher doping densities, predicted by Eq. (3.11), is obvious in the data. Data for GaAs can be found in ref. 37 and 38. The temperature dependence of the specific contact resistivity for tungsten contacts to nSi and pSi, normalized to T = 305 K, is shown in Fig. 3.9, showing that there is not a simple ρc –T relationship.39 The temperature behavior of ρc is very much dependent on the doping density. For surface doping densities around 1020 cm−3 , there is almost
134
10−3
10−3
10−4
10−4
rc (Ωcm2)
rc (Ωcm2)
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
10−5
10−6
10−7
10−5
10−6
10−7
pSi
nSi 10−8 1016
1017
1018
1019
1020
10−8 1016
1021
1017
ND (cm−3)
1018
1019
1020
1021
NA (cm−3)
Fig. 3.8 Specific contact resistivity as a function of doping density for Si. The references for nSi are given in ref. 35 and for pSi in ref. 36. 10 Si:B rc(T)/rc(305 K)
NA = 5 ×
1018
cm−3
2.5 × 1019 1
6.9 × 1019
100
1.8 × 1020 200
300
400
Temperature (K) (a) 10
rc(T)/rc(305 K)
9 × 1018 1.2 ×
ND = 5 × 1018 cm−3
1019
2.4 × 1019 1
8.2 × 1019 2.3 × 1020
Theory for 2.3 × 1020 Si:P
0.1 100
200
300
400
Temperature (K) (b)
Fig. 3.9 The specific contact resistivity, normalized to T = 305 K, as a function of temperature for (a) pSi and (b) nSi. The data for ND = 2 × 1018 cm−3 extend from T = 305 to 400 K only. The metal is tungsten. Reprinted after ref. 39 by permission of IEEE ( 1986, IEEE).
MEASUREMENT TECHNIQUES
135
no temperature dependence whereas for densities above and below that value, there are significant variations of ρc with temperature. 3.4
MEASUREMENT TECHNIQUES
Contact resistance measurement techniques fall into four main categories: twocontact twoterminal, multiplecontact twoterminal, fourterminal, and sixterminal methods. None of these methods is capable of determining the specific interfacial resistivity ρi . Instead they determine the specific contact resistivity ρc which is not the resistance of the metalsemiconductor interface alone, but it is a practical quantity describing the real contact. It is, therefore, difficult to compare theory with experiment because theory cannot predict ρc accurately and experiment cannot determine ρi accurately. At times it is even difficult to measure ρc unambiguously. We limit ourselves to discussions of measurement techniques. Contact formation and the impact of contact resistance on device behavior can be found in numerous references of which 7,12, 14 and 40 are a few. 3.4.1
TwoContact TwoTerminal Method
The twoterminal contact resistance measurement method is the earliest method.41 It is also of questionable accuracy if not properly executed. The simplest implementation is shown in Fig. 3.10. For a homogeneous semiconductor of resistivity ρ and thickness t with two contacts as shown in Fig. 3.10(a), the total resistance RT = V /I , measured by passing a current I through the sample and measuring the voltage V across the two contacts, is (3.12a) RT = Rc + Rsp + Rcb + Rp For Fig. 3.10(b) with both contacts on the top surface RT = 2Rc + 2Rsp + 2Rp
(3.12b)
I r t
r
V
(a) I
V
r r (b)
Fig. 3.10 (a) A vertical twoterminal contact resistance structure, (b) a lateral twoterminal contact resistance structure.
136
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
where Rc is the contact resistance of the top contact, Rsp the spreading resistance in the semiconductor directly under the contact, Rcb the contact resistance of the bottom contact, and Rp the probe or wire resistance. The bottom contact usually has a large contact area with a concomitant small resistance. Consequently, Rcb is often neglected. Similarly, the probe resistance is usually negligible. The spreading resistance of a flat, non indenting circular top contact of radius r on the surface of a semiconductor of resistivity ρ, thickness t, and a large bottom contact can be approximated by42 ρ arctan (2t/r) (3.13) Rsp = 2πr More exact expressions for the spreading resistance have been derived.43 For 2t ≫ r, Eq. (3.13) can be expressed as ρ (3.14) Rsp = C 4r where C is a correction factor that depends on ρ, r, and on the current distribution. For widely separated contacts for the structure in Fig. 3.10(b), on a uniformlydoped, semiinfinite substrate the correction factor C = 1. With the current flowing vertically into the top contact as in Fig. 3.10(a), the contact resistance is Rc =
ρc ρc = Ac πr 2
(3.15)
For small Rcb , Eq. (3.12) shows the contact resistance to be the difference between the total resistance and the spreading resistance. The spreading resistance cannot be measured independently and small errors in Rsp can lead to large errors in Rc . The twoterminal method, therefore, works best when Rsp ≪ Rc , approximated by using smallradius contacts.42, 44 – 47 A variation on the twoterminal contact resistance measurement technique is the use of top contacts of varying diameters. Then one measures and plots Rc , calculated from Eq. (3.12) using experimental RT data, as a function of 1/Ac and determines ρc from the slope of this plot.48 Alternately, the total resistance can be plotted against 1/r with Eq. (3.12) fitted to this curve.46 By using various diameters one can see from the shape of the curve whether the data are anomalous. The twoterminal method is more commonly implemented with the lateral structure of Fig. 3.11. This test structure differs from Fig. 3.10(b) by confining the current to the nisland. The test structure consists of two contacts separated by the spacing d. To confine the current flow, the region on which the contact is located must be isolated from the remainder of the substrate, by either confining the implanted or diffused region (ntype on ptype substrate in Fig. 3.11 or ponn) by planar techniques or by etching the region surrounding the island, leaving it as a mesa. The ntype island in this example has width W and ideally the contacts should also be W wide. That is difficult to implement and the contact width Z generally differs from W . The analysis becomes more difficult due to lateral current flow, current crowding at the contacts, and sample geometry.49 For the geometry of Fig. 3.11, the total resistance is RT = Rsh d/W + Rd + Rw + 2Rc
(3.16)
where Rsh is the sheet resistance of the nlayer, Rd the resistance due to current crowding under the contacts, Rw a contact width correction if Z < W , and Rc the contact resistance
MEASUREMENT TECHNIQUES
137
V
I
nType; Rsh (Ω/square) pType
W
Z
nType
pType
d
Fig. 3.11
A lateral twoterminal contact resistance structure in cross section and top view.
Rm
Rm Rsemi
Rc
Rc
V I
n p
n I
Fig. 3.12
V p
A contact string test structure; cross section and top view.
assumed to be identical for the two contacts. Expressions for these resistances are given in ref. 6. The contact chain or contact string in Fig. 3.12 is commonly used for process control, incorporating many contacts (hundreds, thousands, or as many as a million) of the type shown in Fig. 3.11. The total resistance between any two contacts is the sum of the semiconductor resistance, the contact resistance, and the metal resistance. The semiconductor resistance is calculated knowing the sheet resistance and the string geometry. By subtracting the semiconductor resistance from the total resistance one obtains the total contact resistance. The contact resistance for each contact is obtained by dividing by twice the number of contacts. A refined contact string divides the string into sections with intermediate contact pads.50
138
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
For a contact string consisting of N islands and 2N contacts, with contacts separated from each other by spacing d and width W , the total resistance is given by RT =
NRsh d + 2NRc W
(3.17)
neglecting the metal resistance. The contact string technique is considered to be a coarse measurement method that is not very useful for detailed evaluations of contact resistance. It is, however, extensively used as a process monitor. If the measured resistance is higher than the norm, it is difficult to know whether all contacts are poor or whether one particular contact is poor unless intermediate probe pads are provided. Frequently the contact string is only accessible at the ends with no intermediate contacts.
Exercise 3.1 Problem: What effect do the np junctions of the contact string have on the measured results? Solution: The contact string of Fig. 3.12 can be represented by Fig. E3.1. Let us consider the substrate grounded. Suppose R = Rm + 2R c + Rsemi = 50 and I = 1 mA. For 250 islands, we find V = 12.5 V. Assume the junctions have a breakdown voltage of 15 V. Clearly, there is no problem in measuring R. What happens if in one process run Rc increases such that R = 75 . Now V = I R = 18.8 V, but the junctions can only withstand 15 V. Since the total voltage cannot exceed 15 V, dictated by the breakdown voltage of the last np junction, an erroneous resistance will be measured. The situation is better if the substrate is not grounded, because now the voltage is divided among the many np junctions. The message here is to be cautious of the layout and measurement connection when making contact string measurements.
3.4.2
MultipleContact TwoTerminal Methods
The multiplecontact, twoterminal contact resistance measurement technique, shown in Fig. 3.13, was developed to overcome the deficiencies of the twocontact, twoterminal V n
I
p Rm
V1
V2 V
I
Rc
Rsemi
Grounded ?
Fig. E3.1
MEASUREMENT TECHNIQUES
I
1
I
2
139
3
nType; Rsh (Ω/square) pType
RT1
nType
RT2
W
Z
d2
d1
Fig. 3.13 Multiplecontact, twoterminal contact resistance test structure. The contact width and length are Z and L and the diffusion width is W .
method. Three identical contacts are made to the semiconductor with contact spacings d1 and d2 . Assuming identical contact resistances for each of the three contacts allows the total resistance to be written as Rsh di + 2Rc W
(3.18)
(RT 2 d1 − RT 1 d2 ) 2 (d1 − d2 )
(3.19)
RT i = where i = 1 or 2. Solving for Rc gives Rc =
This structure does not have the ambiguities of the simpler twoterminal structure, because neither the bulk resistance nor the layer sheet resistance need be known. The assumption of identical contact resistance for all three contacts is somewhat questionable but is reasonable for a sample that is not too large. The contact resistance is obtained by taking the difference of two large numbers. This can present difficulties and is especially troublesome for low resistance contacts. The determination of lengths d1 and d2 is a further source of inaccuracy. Occasionally negative contact resistances are obtained by this method. The structure of Fig. 3.13 only allows the contact resistance to be determined. The specific contact resistivity cannot be directly extracted from the two resistance measurements. To find ρc requires a more detailed evaluation of the nature of the current flow into and out of the lateral contacts. An early twodimensional current flow analysis by Kennedy and Murley in diffused semiconductor resistors revealed current crowding at the contacts.51 The analysis, based on zero contact resistance, showed that only a fraction of the total contact length was active during the transfer of current from the metal to the semiconductor and from the semiconductor to the metal. This fraction was found to be approximately equal to the thickness of the diffused semiconductor sheet. To take current crowding into account and to be able to extract the specific contact resistivity, a detailed theoretical investigation was undertaken. Murrmann and Widmann used a simple transmission line model (TLM) considering both the semiconductor sheet
140
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
resistance and the contact resistance.52 They also described a structure to determine the contact resistance using linear and concentric contacts.53 Berger extended the transmission line method.54 In contrast to the KennedyMurley model, in which the contact resistance is assumed to be zero, in the TLM the contact resistance is nonzero. However, the semiconductor sheet thickness is assumed to be zero in the TLM, with the layer retaining its sheet resistance Rsh . This assumption allows onedimensional current flow only. The “zero sheet thickness” restriction was relaxed by Berger in his extended TLM where he allowed nonzero sheet thickness, but with the current still restricted to onedimensional flow.54 The TLM model was later extended to two dimensions by the duallevel transmission line model with the current allowed to flow perpendicularly to the contact interface. A comparison between the simple and the revised TLM shows a maximum contact resistance deviation of 12%.55 When current flows from the semiconductor to the metal, it encounters the resistances ρc and Rsh in Fig. 3.14, choosing the path of least resistance. The potential distribution under the contact is determined by both ρc and Rsh according to54 √ I Rsh ρc cosh[(L − x)/LT ] V (x) = Z sinh(L/LT )
(3.20)
where L is the contact length, Z the contact width, and I the current flowing into the contact. Equation (3.20) is plotted in Fig. 3.15 with the potential under the contact normalized to unity at x = 0. The voltage is highest near the contact edge x = 0 and drops nearly exponentially with distance. The “1/e” distance of the voltage curve is defined as the transfer length LT LT = ρc /Rsh (3.21)
The transfer length can be thought of as that distance over which most of the current transfers from the semiconductor into the metal or from the metal into the semiconductor. LT is plotted in Fig. 3.16 against the specific contact resistivity as a function of the sheet resistance. Typical specific contact resistivities are ρc ≤ 10−6 ·cm2 for good contacts. The transfer length is on the order of 1 µm or less for such contacts. Contacts for contact
nType
I pType
I
ρc
Rsh
0
L
x
Fig. 3.14 Current transfer from semiconductor to metal represented by the arrows. The semiconductor/metal contact is represented by the ρc Rsh equivalent circuit with the current choosing the path of least resistance.
MEASUREMENT TECHNIQUES
141
1 rc = 10−5 Ωcm2
0.8
V(x)
0.6 0.4
10−6
0.2
10−7 10−8
0
0
2
4
6
8
10
x (µm)
Fig. 3.15 Normalized potential under a contact versus x as function of ρc , where x = 0 is the contact edge. L = 10 µm, Z = 50 µm, Rsh = 10 /square.
30 100 300
10−2 Rsh = 10 Ω/square
LT (cm)
10−3 1000 10−4 10−5 10−6 10−8
10−7
10−6 rc
10−5
10−4
10−3
10−2
(Ωcm2)
Fig. 3.16 Transfer length as a function of specific contact resistivity and semiconductor sheet resistance.
resistance measurements are often longer than 1 µm. For such contacts, some of the contact is inactive during current transfer. We will now consider the three contact configurations in Fig. 3.17, with the current flowing from contact 1 to contact 2. In the transmission line method test structure (TLM) in Fig. 3.17(a), also referred to as the contact front resistance test structure (CFR), the voltage is measured across the same contacts as the current. In the contact end resistance test structure (CER) in Fig. 3.17(b) the voltage is measured between contacts 2 and 3. In the cross bridge Kelvin resistance test structure (CBKR) (Fig. 3.17(c)), the voltage is measured at right angles to the current. With V measured between contacts 1 and 2 at x = 0, Eq. (3.20) gives the contact front resistance as
Rcf =
V = I
√
ρc Rsh ρc coth(L/LT ) = coth(L/LT ) Z LT Z
(3.22)
142
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
V I
1
δ
I
Z
2
W
3
V
1
2
3
L (a)
(b) I V 1
2
3 (c)
Fig. 3.17 (a) Conventional contact resistance test structure, (b) contact end resistance test structure, and (c) cross bridge Kelvin resistance test structure.
provided Z = W . Eq. (3.22) is only an approximation when the sample is wider than Z, because this equation does not consider the current flow around the contacts. The expression Rcf is usually referred to simply as the contact resistance Rc . We will do so here also. Two cases lead to simplifications of Eq. (3.22). For L ≤ 0.5 LT , coth(L/LT ) ≈ LT /L and ρc (3.23a) Rc ≈ LZ and for L ≥ 1.5 LT , coth(L/LT ) ≈ 1 and Rc ≈
ρc LT Z
(3.23b)
The effective contact area is the actual contact area Ac = LZ for the first case. But in the second case the effective contact area is Ac,eff = LT Z. In other words, the effective contact area can be smaller than the actual contact area. This can have important consequences. For example, consider a structure with Rsh = 20 /square and ρc = 10−7 ·cm2 . The transfer length LT = 0.7 µm. For a contact length of L = 10 µm and width Z = 50 µm, the actual contact area is LZ = 5 × 10−6 cm2 . However, the effective contact area is only LT Z = 3.5 × 10−7 cm2 . The current density flowing across the contact is 5 × 10−6 /3.5 × 10−7 = 14 times higher than if the entire contact were active. This higher current density can cause reliability problems by degrading the contact. The reduced contact area can burn out in extreme cases shifting the effective area along the contact until the entire contact is destroyed. The effect of contact length on contact resistance is illustrated in Fig. 3.18. It is a plot of the front contact resistance given by Eq. (3.22) multiplied by the contact width Z, for
MEASUREMENT TECHNIQUES
143
101 rc = 10−4 Ωcm2 RcZ (Ωcm)
100 10−5 10−1 10−6 10−2 10−7 10
−3
10−4 10−5
10−8 10−4
10−3
10−2
10−1
L (cm)
Fig. 3.18 Front contact resistance–contact width product as a function of contact length and specific contact resistivity for Rsh = 20 /square and Rsm = 0.
normalization purposes, against the contact length as a function of the specific contact resistivity. Note the initial Rc decrease with contact length. However, Rc Z reaches a minimum at L ≈ LT from which it departs no further no matter how long the contact. The metal/semiconductor representation of Fig. 3.14 may be too simple for certain contacts. For example, alloyed contacts typically made on GaAs consist of a metal, an alloyed region, and the underlying semiconductor. Similarly contacts formed by depositing a metal on a thin layer of a low band gap material on a higher band gap material fall into this category. This calls for a more complex transmission line model—the trilayer transmission line model. The equations, although similar to the TLM equations, become significantly more complex.56 When the voltage is measured between contacts 2 and 3 with the current flowing from 1 to 2, shown in Fig. 3.17(b), the structure is known as the contact end resistor. The voltage is now measured at x = L and Eq. (3.20) leads to the contact end resistance Rce =
V = I
√
ρc Rsh ρc 1 1 = Z sinh(L/LT ) LT Z sinh(L/LT )
(3.24)
The contact end resistance measurement can be used to determine ρc by measuring Rce and using an iteration of Eq. (3.24).57 For short contacts, Rce is sensitive to contact length variations with the error in determining L limiting the accuracy of the method. For long contacts, Rce becomes very small and the accuracy is limited by instrumentation, seen by looking at the ratio 1 Rce = (3.25) Rcf cosh(L/LT ) which obviously becomes very small for L ≫ LT . For the crossbridge Kelvin resistance test structure in Fig. 3.17(c), the voltage contact 3 is located at the side of contact 2. The measured voltage is thus the linear average of the potential over the contact length L. Integrating Eq. (3.20) as V =
1 L
0
L
V (x) dx
(3.26)
144
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
gives the contact resistance as Rc =
ρc V = I LZ
(3.27)
Equation (3.24) assumes the contact width Z to be identical to the sheet width W . This is rarely realized in practice. Usually Z < W . Experiments with Z = 5 µm and W ranging from 10 µm to 60 µm showed the contact end resistance to give erroneously high ρc . The error increased as ρc decreased or as Rsh increased.58 The error arises from the potential difference between the front edge and the rear edge of the contact allowing current to flow around the contact edges. The measured resistance is proportional to the sheet resistance and is insensitive to the contact resistance for large δ. For the simple onedimensional theory to hold, the test structure should meet the conditions: L ≤ LT , Z ≫ L and δ ≪ Z. The onedimensional analysis is not valid if these conditions are not met. Accurate extraction of ρc , however, is possible by fitting numerical simulations to measured data. The problem of W = Z can be avoided with circular test structures, consisting of a conducting circular inner region of radius L, a gap of width d, and a conducting outer region.59 The conducting regions are usually metallic and the gap typically varies form a few microns to tens of microns. For equal sheet resistances under the metal and in the gap, and for the geometry of the circular contact resistance structure in Fig. 3.19(a), the total resistance between the internal and the external contacts is60 LT K0 (L/LT ) d Rsh LT I0 (L/LT ) + + ln 1 + (3.28) RT = 2π L I1 (L/LT ) L + d K1 (L/LT ) L where I and K denote the modified Bessel functions of the first order. For L ≫ 4LT , the Bessel function ratios I0 /I1 and K0 /K1 tend to unity and RT becomes Rsh LT LT d + + ln 1 + (3.29) RT = 2π L L+d L In the circular transmission line test structure in Fig. 3.19(b), for L ≫ d, Eq. (3.29) simplifies to Rsh (d + 2LT )C RT = (3.30) 2πL where C is the correction factor61 C=
d L ln 1 + d L
(3.31)
L d
(a)
(b)
Fig. 3.19 Circular contact resistance test structure. The dark regions represent metallic regions. Spacing d and radius L are shown in (a).
MEASUREMENT TECHNIQUES
145
shown in Fig. 3.20(a). For d/L ≪ 1, Eq. (3.30) becomes RT =
Rsh (d + 2LT ) 2πL
(3.32)
For practical radii up to about 200 µm and gap spacings of 5–50 µm, the correction factor is necessary to compensate for the difference between the linear transfer length method and the circular TLM layouts to obtain a linear fit to the experimental data. Without the correction factor, the specific contact resistance is underestimated. The total resistance before and after data correction is shown in Fig. 3.20(b) as a function of gap spacing d. Similar to the linear TLM structure, the corrected circular TLM data are linear and yield the contact resistance and the transfer length, from which the specific contact resistivity can be determined. The circular test structure has one main advantage. It is not necessary to isolate the layer to be measured, because current can only flow from the central contact to the surrounding contact. In the linear TLM test structure, current can flow from contact to
Correction Factor, C
1 0.9 0.8 0.7 0.6 0.5
0
0.4
0.8
1.2
1.6
2
d/L (a) 20
15 RT (Ω)
Corrected data 10 Original data 5
2LT 2Rc
0 −10
0
10
20
30
40
50
d (µm) (b)
Fig. 3.20 (a) Correction factor C versus d/L ratio for the circular transmission line method test structure, (b) total resistance for the circular TLM test structure before and after data correction. RC = 0.75 ohms, LT = 2 µm, ρc = 4 × 10−6 ohmcm2 , Rsh = 110 ohms/square. Data courtesy of J.H. Klootwijk and C.E. Timmering, Philips Research Labs.
146
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
contact through the region beyond the test structure if it is not isolated. The circular test structure with four metal contacts is very similar to the crossbridge Kelvin resistor discussed in Section 3.4.3.62 Equations (3.22) and (3.24) are derived under the assumption that ρc > 0.2Rsh t 2 , where t is the layer thickness. For Rsh = 20 ohms/square and t = 1 µm, this constraint leads to ρc > 4 × 10−8 ohm·cm2 . The TLM method must be modified if that condition is not satisfied, as verified by experiments and by modeling.63 Most specific contact resistivities are above 4 × 10−8 ohm·cm2 and the TLM method is valid. The difficulty of deciding where to measure the voltage in the configuration of Fig. 3.17 has led to a test structure shown in Fig. 3.21(a) and a measurement technique known as the transfer length method originally proposed by Shockley.64 Unfortunately it is also abbreviated as TLM. The TLM test structure is very much like that of Fig. 3.13, but consists of more than three contacts. Two contacts at the ends of the test structure served as entry and exit point for the current in the original ladder structure and the voltage was measured between one of the large contacts and each of the successive narrow contacts in Fig. 3.21(a). Later the test structure had unequal spacing between contacts as in Fig. 3.21(b), with the voltage measured between adjacent contacts. The structure in Fig. 3.21(b) has certain advantages over that of Fig. 3.21(a). When the voltage is measured in the ladder structure between contacts 1 and 4, for example, the current flow may be perturbed by contacts 2 and 3. The effect of contacts 2 and 3 depends on the transfer length LT and the contact length L. For L ≪ LT , the current does not penetrate appreciably into the contact metal and, to first order, contacts 2 and 3 have no effect on the measurement. For L ≫ LT , the current does flow into the metal and the contact can be thought of as two contacts, each of length LT joined by a metallic conductor.65 The shunting of the current by the metal strips obviously influences the measured voltage or resistance. It is for this reason that the structure in Fig. 3.21(b) is preferred, because there is only bare semiconductor between any two contacts. For contacts with L ≥ 1.5 LT and for a front contact resistance measurement of the structure in Fig. 3.21(b), the total resistance between any two contacts is RT =
Rsh d Rsh + 2Rc ≈ (d + 2LT ) Z Z
(3.33)
where we have used the approximation leading from Eq. (3.22) to Eq. (3.23b). Eq. (3.33) is similar to Eq. (3.32) with the contact peripheral length 2πL replaced by the contact width Z.
Z 1
2
3
W 9
4 (a)
1
2
3
4 (b)
Fig. 3.21
Transfer length method test structures.
5
MEASUREMENT TECHNIQUES
147
δ
Z L d1
d2
d3
W
d4
RT Slope = Rsh/Z 2LT 2Rc 0
d
Fig. 3.22 A transfer length method test structure and a plot of total resistance as a function of contact spacing, d. Typical values might be: L = 50 µm, W = 100 µm, ZW = 5 µm (should be as small as possible), d ≈ 5 to 50 µm.
The total resistance is measured for various contact spacings and plotted versus d as illustrated in Fig. 3.22. Three parameters can be extracted from such a plot. The slope
(RT )/ (d) = Rsh /Z leads to the sheet resistance with the contact width Z independently measured. The intercept at d = 0 is RT = 2Rc giving the contact resistance. The intercept at RT = 0 gives −d = 2LT , which leads to the specific contact resistivity with Rsh known from the slope of the plot. The transfer length method gives a complete characterization of the contact by providing the sheet resistance, the contact resistance, and the specific contact resistivity. The transfer length method is commonly used, but it has its own problems. The intercept at RT = 0 giving LT is sometimes not very distinct, leading to incorrect ρc values. Perhaps a more serious problem is the uncertainty of the sheet resistance under the contacts. Eq. (3.33) assumes the sheet resistance to be identical under the contacts and between contacts. But the sheet resistance under the contacts may differ from the sheet resistance between contacts due to the effects of contact formation. This would be true for alloyed and silicided contacts where the region under the contact is modified during contact fabrication, leading to the modified expression for the front contact and total resistance,66 ρc coth (L/LT k ) Rcf = (3.34) LT k Z and RT =
2Rsk LT k Rsh Rsh d Rsh d + 2Rc ≈ + = [d + 2(Rsk /Rsh )LT k ] Z Z Z Z
(3.35)
where Rsk is the sheet resistance under the contact and LT k = (ρc /Rsk )1/2 . The slope of the RT versus d plot still gives Rsh /Z and the intercept at d = 0 gives 2Rc . However, the intercept at RT = 0 now yields 2LT k (Rsk /Rsh ) and it is no longer possible to determine ρc since Rsk is unknown. Nevertheless, by determining Rcf from the transfer length method and Rce from the end resistance method, where √ ρc Rce 1 Rsk ρc Rce = = ; (3.36) = Z sinh(L/LT k ) ZLT k sinh(L/LT k ) Rcf cosh(L/LT k )
148
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
one can determine LT k and ρc . In this way it is possible to find the contact resistance and the specific contact resistivity in addition to the sheet resistance between and under the contacts. One can also separate Rsh from Rsk by etching the semiconductor between the contacts. Extraction of electrical contact parameters by the TLM method is based on the assumption of constant electrical and geometrical contact parameters across the sample. However, such parameters typically exhibit scatter across a wafer. Statistical modeling has shown that the usual data extraction procedure can lead to errors in the extracted contact parameters even if there is no error in the measured electrical and geometrical parameters.67 For short contacts (L < LT ), ρc can be determined accurately regardless of the scatter in other parameters, while Rsh and Rsk are in error only if ρc exhibits scatter over the wafer. For long contacts, the extracted ρc and Rsk are in error only if Rsk or resistance measurements are in error. Best results are obtained for L ≥ 2LT . When a wafer exhibits nonuniformities of the electrical parameters of 10–30%, the error in ρc and Rsk can be as high as 100–1000%. Redundancy through the use of more than one test structure allows the errors to be reduced. We have so far considered the specific contact resistivity and sheet resistance of the semiconductor, but have neglected the resistance of the metal. This generally introduces little error although at times the metal resistance increases with aging and can no longer be neglected. The resistance of silicides is higher than that of pure metals and may not always be negligible. A more serious limitation arises when polysilicon conductors are used instead of metals. Their resistance is significantly higher than that of metals and may need to be considered for proper interpretation of the experimental results. For nonnegligible metal resistance, the contact resistance of Eq. (3.22) becomes68 – 69 L ρc 2 2 + (3.37) (1 + α )coth(L/LT m ) + α Rcf = LT m Z(1 + α)2 sinh(L/LT m ) LT m where α = Rsm /Rsk , Rsm is the metal sheet resistance, and LT m = [ρc /(Rsm + Rsk )]1/2 = LT k /(1 + α)1/2 . Equation (3.37) reduces to Eq. (3.34) for Rsm = 0 and to Eq. (3.22) for Rsk = Rsh and Rsm = 0. The contact front resistance from Eq. (3.37), normalized by multiplying by Z, is plotted in Fig. 3.23 against the contact length as a function of the specific contact resistivity. The main difference between Fig. 3.18 and 3.23 is the 101
RcZ (Ωcm)
100
rc = 10−4 Ωcm2 10−5
10−1 10−6 10
−2
10
−3
10−7
10−4 10−5
10−8 10−4
10−3
10−2
10−1
L (cm)
Fig. 3.23 Front contact resistance–contact width product as a function of contact length and specific contact resistivity for Rsk = 20 /square and Rsm = 50 /square.
MEASUREMENT TECHNIQUES
149
minimum in Fig. 3.23, which is absent when Rsm = 0. For each combination of ρc , Rsk , and Rsm there is an optimum contact length for minimum contact resistance. For lengths above and below this optimum value, the contact resistance increases. Further discussions of the effects of finiteresistance metal conductors can be found in ref. 70. We need to consider one more correction. So far we assumed the gap δ in Fig. 3.22 to be zero. The fact that δ = 0, can lead to incorrect intercepts of the RT − d plot. Various corrections have been proposed.49, 71 We follow the suggestions of ref. 72, where the δ region between the contacts is represented by parallel resistances. As shown in Appendix 3.1, instead of plotting RT versus d, one plots R ′ versus d, where R ′ = 2Rce +
(RT (δ = 0) − 2Rce )Rp Rp − RT (δ = 0) − 2Rce
(3.38)
where Rce is the contact end resistance, RT the measured resistance, and Rp the parallel “strip” resistance. The derivation of Eq. (3.38) and a method to determine Rp are given in Appendix 3.1. Figure 3.24 shows uncorrected and corrected TLM curves for one particular contact area. It clearly shows the different intercepts for the uncorrected lines (solid lines) leading to incorrect contact resistance, transfer length, and specific contact resistivity, but one common intercept for the corrected data (dashed line). 3.4.3
FourTerminal Contact Resistance Method
The specific contact resistivity measurement techniques discussed so far require the semiconductor bulk resistivity or the semiconductor sheet resistance to be known. However, it is desirable to measure Rc and ρc by minimizing or eliminating, if possible, the contribution from bulk or sheet resistance. The measurement technique that comes closest to this goal is the fourterminal Kelvin test structure also known as the crossbridge Kelvin resistance (CBKR). It appears to have been first used for evaluating metalsemiconductor contacts in 197273 but it was only in the early 1980s that it was evaluated seriously.74 – 76 In principle, this method allows the specific contact resistivity to be measured without being affected by the underlying semiconductor or the contacting metal conductor.
40 δ = 1, 2, 5 µm
RT (Ω)
30
δ = 5 µm δ = 2 µm
20 δ = 1 µm 10
L = 10 µm Z = 20 µm
0 −10
0
10
20
30
40
d (µm)
Fig. 3.24 Uncorrected (solid points and lines) and corrected (open points and dashed line) total resistance versus spacing d for Au/Ni/AuGe/nGaAs contacts annealed at 400◦ C for 20 s. Reprinted after ref. 72 by permission of IEEE ( 2002, IEEE).
150
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
3
I
I
1
2 nType
V 4
pType (a)
δ
3
1 A
2 A
nType δ
(b)
4
Fig. 3.25 A fourterminal or Kelvin contact resistance test structure. (a) Cross section through section A–A, (b) top view of the structure.
The principle is illustrated in Fig. 3.25. Current is forced between contacts 1 and 2 and the voltage is measured between contacts 3 and 4. There are three voltage drops between pad 1 and pad 2. The first is between pad 1 and the semiconductor nlayer, the second along the semiconductor sheet, and the third between the nlayer and the pad 2/3. A high input impedance voltmeter, for measuring the voltage V34 = V3 –V4 , allows very little current flow between pads 3 and 4. Hence, the potential at pad 4 is essentially the same as the potential in the nregion directly under contact 2/3, as illustrated in Fig. 3.25(a) by connection 4 under the contact. V34 is solely due to the voltage drop across the contact metalsemiconductor interface. The name “Kelvin Test Structure” refers to the fact that a voltage is measured with little current flow as in fourpoint probe resistance measurements. The contact resistance is V34 Rc = (3.39) I which is simply the ratio of the voltage to the current. The specific contact resistivity is ρc = Rc Ac
(3.40)
where Ac is the contact area. Equation (3.40) does not always agree with experimental data. The specific contact resistivity calculated with Eq. (3.40) is an apparent specific contact resistivity differing from the true specific contact resistivity by lateral current crowding for contact windows smaller than the diffusion tap, shown as δ > 0 in Fig. 3.25.77 Contact window to diffused layer misalignment and lateral dopant diffusion account for δ > 0. In the ideal case, δ = 0 as illustrated in Fig. 3.26(a). In an actual contact, some of the current, indicated by the arrows in Fig. 3.26(b), flows around the metal contact. In the ideal case with δ = 0, the voltage drop is V34 = I R c . For δ > 0, the lateral current flow gives an additional voltage
MEASUREMENT TECHNIQUES
I
I
d
L
L
W
W
(a)
151
d
(b)
Fig. 3.26 Fourterminal contact resistance test structures. (a) Ideal with only lateral current flow, (b) showing current flowing into and around the contact. The black area is the contact area.
RkxContact Area (Ωcm2)
drop that is included in V34 , leading to a higher voltage. Therefore, according to Eq. (3.39) Rc is higher and is usually designated Rk . According to Eq. (3.40) ρc is also higher if the actual contact area Ac is used. The ρc so extracted is known as the effective or apparent specific contact resistivity. The error introduced by this geometrical factor is highest for low ρc and/or high Rsh and lowest for high ρc and/or low Rsh .78 The vertical voltage drop in the semiconductor normal to the contact plane, usually neglected, leads to an additional correction.79 The effect of contact misalignment is shown in Fig. 3.27.80 Larger δ leads to higher measured resistance. Clearly, for large misalignment, the measured resistance is seriously in error. The true resistance is obtained by extrapolating to δ = 0. The effect of asymmetrical misalignment is illustrated in Fig. 3.28, where the apparent contact resistance is plotted versus misalignments L1 and L2 . This figure clearly shows the effect of parasitic current paths. In one case Rk increases, in the other it decreases. It is difficult to fabricate test structures with δ = 0. However, a solution is illustrated in Fig. 3.29(a). Here the semiconductor voltage tap consists of individual “strips”.80 The measured voltage for the three taps is shown in Fig. 3.29(b). By extrapolating the data to zero voltage tap spacing, the true resistance is obtained.
rc = 5 × 10−7 Ωcm2
10−5
Ac = 10 × 10 7×7 5×5 3×3 2×2 1.5 × 1.5
10−6 0
2
4 6 8 Misalignment d (µm)
10
Fig. 3.27 Apparent contact resistance multiplied by the contact area versus misalignment δ. The contact areas are given on the right side of the figure. Under the contact: Arsenic implant, 2 × 1015 cm−2 , 50 keV, annealed at 1000◦ C, 30 s. Contact metal: Ti/TiN/Al/Si/Cu. Adapted from ref. 80.
152
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
L1 varies
102
L2 = 1 µm Rk (Ω)
L L2
L L1
101
L1 = 1 µm L2 varies
Contact: 2 × 2 µm2 100
0
10 20 30 40 Alignment Margin, L1, L2 (µm)
50
Fig. 3.28 Dependence of contact resistance on misalignment dimensions L1 and L2 . Under the contact: Arsenic implant, 2 × 1015 cm−2 , 50 keV, annealed at 1000◦ C, 30 s. Contact metal: Ti/TiN/Al/Si/Cu. Adapted from ref. 80.
Metal voltage terminal
Contact Via Metal current terminal
Silicon current terminal
10 µm
0.5 µm
500 µm 22 µm 32 µm
4 µm
12
Silicon voltage terminal
(a) 180 160
RT (Ohms)
140 120 100 80 60 40 20 0
L = 25 µm 0
5
10
15
20
25
30
35
Tap Spacing (µm) (b)
Fig. 3.29 (a) Modified Kelvin contact resistance “tapped” test structure and (b) resistance versus tap spacing. After ref. 80.
MEASUREMENT TECHNIQUES
153
A simplified twodimensional approach gives the contact resistance Rk as80 Rk =
ρc +
√
ρc Rsh L1 coth(L/LT ) + 0.5 Rsh L21 + (L + L1 + L2 )W
√
ρc Rsh L2 /sinh(L/LT )
(3.41)
with the various dimensions shown on Fig. 3.28. Curves calculated with Eq. (3.41) agree qualitatively with the data in Fig. 3.27. Lateral current flow around the contact accounts for the additional resistance. The resistance increase gets worse the lower the specific contact resistivity, further aggravated for higher sheet resistances. Unfortunately, the trend in the technology of today’s highdensity integrated circuits is toward lower ρc and higher Rsh due to shallower junctions. Both are in the direction of complicating the interpretation of fourterminal contact resistance test structure measurements. Simple onedimensional interpretations must be carefully evaluated for their accuracy. Figure 3.30 shows calculated curves for the apparent and the actual values of specific contact resistivity for the structure of Fig. 3.31.79 For the ideal case of L/W = 1 or δ = 0 the two are identical indicated by the 45◦ line for twodimensional calculations. However, for the more realistic threedimensional calculations the two are not identical even for δ = 0. As ρc decreases the contact resistance voltage decreases and the lateral voltage becomes more important until the contact resistance voltage becomes negligible and ρc,apparent is independent of the true ρc . Universal error corrections curves from threedimensional modeling, including the finite depth of the semiconducting are shown in Fig. 3.31. In these calculations the semiconductor sheet resistance under the contact is assumed identical to the sheet resistance beyond the contacts. Rk in these curves is the contact resistance including parasitic resistances. Twodimensional models of the transmission line, the contact end resistance, and the crossbridge Kelvin resistance structures have been used to calculate and plot the contact resistance normalized by the sheet resistance against the contact length normalized by δ.81 Deviations from the simple onedimensional analysis are predicted for all three cases. The TLM has the least sensitivity to δ because it detects the front contact potential, which is only weakly perturbed by peripheral current flow. However, the TLM method relies on extrapolation of experimental data to determine ρc . That has a potential error especially if the data points do not lie on a welldefined straight line. Both the CER and the CBKR
rc,apparent (Ωcm2)
10−7
δ = 0.5 µm
0.2 µm
0.1 µm
10−8
10−9 10−10
δ=0
10−9 rc,true
10−8
10−7
(Ωcm2)
Fig. 3.30 Twodimensional (dashed) and threedimensional (solid lines) simulated apparent versus true specific contact resistivity for various tap spacings δ. Reprinted after ref. 79 by permission of IEEE ( 2004, IEEE).
154
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
d L W
R sh
r
t
104
Rk /Rsh
t/W = 0.5
LT/δ = 9 4.5
103
2.25
102
1.125 0.563
101 100 10−1
0.281
0.14
0.07
0.1
1
10
L/ d
Fig. 3.31 Threedimensional universal correction curves for CKR structures of Rk /Rsh versus L/δ as a function of LT /δ for tap depth/width ratios of t/L = 0.5. Reprinted after ref. 79 by permission of IEEE ( 2004, IEEE).
structures show significant deviations due to peripheral current flow. The contact resistances determined by the CER method are generally low, Rce (CER) < Rc (CBKR), making the measurement more difficult. Contact misalignment introduces further departures from onedimensional behavior.82 Selfaligned contacts solve the misalignment problem but not the lateral diffusion problem.83 Other models of contact resistance calculations are given in refs. 84 and 85. Contact resistance test structures can also be implemented with a modified MOSFET consisting of three n+ regions and two gates as illustrated in Fig. 3.32.86 The “sheet” between contacts 1 and 2 and between contacts 3 and 4 is due to a channel formed by biasing the two MOSFET sections into conduction. This structure is compatible with standard silicide processes. It can be implemented in the CFR, the CER, or in the CKBR configuration.
1 n+
2
3 n+
n+
pType
Fig. 3.32
A MOSFET contact resistance test structure.
MEASUREMENT TECHNIQUES
1
3
5
I
4
155
2
n+ p nType n+
6 Fig. 3.33
Vertical contact resistance Kelvin test structure.
The vertical Kelvin test structure in Fig. 3.33 was developed to overcome the lateral current flow problems of the conventional Kelvin structure.87 The device requires one additional mask level during its fabrication compared to conventional Kelvin structures. The metal/semiconductor contact is made to a diffused or ionimplanted layer (n+ layer in Fig. 3.33). Current I confined to the contact area by the oxide window and the isolating np junction, is forced between contact 5 and substrate contact 6. Voltage V24 is measured between contacts 2 and 4. V4 is the voltage of the metal and V2 is the voltage of the semiconductor layer just below the metal, even though V2 is measured at some distance from the contact. Just as in a conventional Kelvin structure, there is very little lateral voltage drop along the n+ layer during the voltage measurement because essentially no current is drawn. The contact resistance and the specific contact resistivity are given by Rc = V24 /I and ρc = Rc Ac . Lateral effects, so important in all methods that rely on lateral current flow, also play a role in this vertical structure. This comes about not because the current flows laterally to reach a collecting contact, but because of current spreading. The current does not flow strictly vertically. It has a small lateral, spreading component, shown in Fig. 3.33, making the voltage at the sensing contact (contact 2) not exactly equal to the voltage under the metal. The additional spreading resistance causes the measured contact resistance to be higher than the true contact resistance.88 An additional complication arises when the contact is smaller than the contact opening. The specific contact resistivity is then given approximately as87 ρc,eff ≈ ρc + Rsh xj /2 (3.42) where Rsh is the sheet resistance and xj the junction depth of the upper n+ layer in Fig. 3.33. Equation (3.42) is valid for L ≥ 10xj . The vertical test structure works well the smaller the contact area and the shallower the upper n+ layer is. Additional contacts are provided in Fig. 3.33. V13 can be used to average the voltage reading with V24 to reduce experimental errors. Furthermore, conventional lateral sixterminal measurements can be made to obtain the end resistance Rce , the front resistance Rcf , and the sheet resistance Rsh . A detailed study of various nonidealities in the vertical test structure has shown the current spreading effect to be small compared to lateral current crowding in horizontal Kelvin test structures.89 Misalignment between the isolation junction and the metal contact can produce more severe errors, but these can be minimized by averaging the voltage readings on the left and the right arms.
156
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
3.4.4
SixTerminal Contact Resistance Method
The sixterminal contact resistance structure in Fig. 3.34 is related to the fourterminal Kelvin structure with two more contacts for additional measurement options not available with the conventional Kelvin structure.75 The structure allows the contact resistance, the specific contact resistivity, the contact end resistance, the contact front resistance, and the sheet resistance under the contact to be determined. For the conventional Kelvin structure contact resistance measurement the current is forced between contacts 1 and 3 in Fig. 3.34 and the voltage is measured between contacts 2 and 4. The analysis is that of Eqs. (3.39) and (3.40) for the onedimensional case, where Rc = V24 /I and ρc = Rc Ac . All the twodimensional complications, not reflected in Eqs. (3.39) and (3.40), manifest themselves in the sixterminal structure also. To measure the contact end resistance Rce = V54 /I , current is forced between contacts 1 and 3 and the voltage is sensed across contacts 5 and 4. With the contact resistance and the specific contact resistivity determined from the Kelvin part of this structure, the sheet resistance under the contact can be determined from the end resistance using Eq. (3.36) and the contact front resistance, given by Rcf in Eqs. (3.22) and (3.36) can be calculated with Eq. (3.36). 3.4.5
NonPlanar Contacts
Thus far we have only concerned ourselves with deviations from simple theory due to twodimensional current flow. We have assumed the contact itself to be a smooth, intimate contact between the metal and the semiconductor. Real contacts are not this perfect introducing further complications. Contact history in Si integrated circuits is depicted in Fig. 3.35. Initially Al was deposited directly onto Si (Fig. 3.35(a)). For aluminumsilicon contacts, there is a tendency for the silicon to migrate into the aluminum, leaving voids in the silicon.90 Aluminum can subsequently migrate into these voids creating spiking. Under extreme conditions this can lead to junction shorts. Addition of 1 to 3 wt% Si to the Al reduces spiking considerably but creates other problems. For example, it is possible for the Si to precipitate and to grow epitaxially between the original Si surface and the Al film (Fig. 3.35(b)). The epitaxially regrown layer is p + type because it contains a high density of aluminum, a ptype dopant in Si, creating a pn junction at the regrown epi/n+ interface. It has been observed that the propensity for such epitaxial films to form is higher for (100) than for (111)oriented substrates.91 This can be a severe problem for small contact areas where the contact resistance for (100)oriented substrates increases over similar (111) surfaces.91
1
2
6 I 3
4 5
V
V
Fig. 3.34
Sixterminal Kelvin structure for the determination of Rc , Rce , Rcf , and Rsk .
157
SCHOTTKY BARRIER HEIGHT
Al
Al/1−2% Si n+
Spiking
p+
p (a)
(b)
Silicide
Silicide (c)
Barrier (d)
Fig. 3.35 Historic progression of ohmic contacts in Si technology; (a) Al/Si, (b) Al/12% Si, (c) Al/silicide/Si, and (d) Al/barrier layer/silicide/Si.
Silicides solved this problem (Fig. 3.35(c)). A silicide is formed by depositing a metal onto Si and heating the sample to form the silicide. Commonly used metals are Ti, Co, and Ni but many other metals form silicides. Silicides penetrate into the Si sample. There is also a chance that Al above the silicide can migrate through the silicide along grain boundaries and form Al/Si contacts. Hence, recent contacts consist of a silicide, a barrier layer (e.g., W plug), and Al or Cu as shown in Fig. 3.35(d). This can give the required low contact resistance and still be chemically stable. Unless the semiconductor is carefully cleaned, there can be interfacial layers between the metal and the semiconductor. These can consist of oxides forming prior to metal deposition. But interfacial layers can also be due to poor substrate cleaning or even due to poor vacuum during metal deposition.92 Contacts to GaAs are typically formed by alloying. A Gecontaining alloy is deposited on the device and heated until alloying occurs. The metalsemiconductor interface after contact formation can be very nonplanar. It has been suggested that the current in such alloyed contacts flows through Gerich islands with the contact resistance largely determined by the spreading resistance under the Gerich regions.93 The effective contact area is likely to be very different from the actual contact area for that model. Very smooth metalGaAs interfaces can be formed by evaporating Ge, Au, and Cr layers separately and keeping the annealing temperature below the AuGe eutectic temperature.94 All of these “technological” imperfections make contact resistance measurement interpretation yet more difficult. 3.5
SCHOTTKY BARRIER HEIGHT
The band diagram of a Schottky barrier diode on an ntype substrate is shown in Fig. 3.36. The ideal barrier height of φB0 is approached only when the diode is strongly forward biased. The actual barrier height φB is less than φB0 due to image force barrier lowering and other factors. Vbi is the builtin potential and Vo is the potential of the semiconductor Fermi level with respect to the conduction band. The thermionic currentvoltage relationship of a Schottky barrier diode, neglecting series and shunt resistance, is given by I = AA∗ T 2 e−qφB /kT (eqV /nkT − 1) = Is1 e−qφB /kT (eqV /nkT − 1) = Is (eqV /nkT − 1) (3.43)
158
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
fB0
Vbi
fB
Vo
EC /q EF /q
EV /q
Fig. 3.36 TABLE 3.1
Experimental A∗ Values.
Semiconductor nSi pSi nGaAs nGaAs pGaAs nInP
Schottky barrier potential band diagram.
A∗ (A/cm2 · K2 )
Ref.
112 (±6) 32 (±2) 4–8 0.41 (±0.15) 7 (±1.5) 10.7
95 95 96 97 97 109
where Is is the saturation current, A the diode area, A∗ = 4πqk 2 m∗ / h3 = 120(m∗ /m) A/cm2 ·K2 Richardson’s constant, φB the effective barrier height, and n the ideality factor. Published values of A∗ are given in Table 3.1. Measurements in ref. 97 were made on almost ideal Al/nGaAs devices with the Al deposited epitaxially by molecular beam epitaxy in ultrahigh vacuum. The ideality factor n incorporates all those unknown effects that make the device non ideal. A Schottky diode is unlikely to be uniform over its entire area. Barrier height patchiness leads to n > 1 and also explains other effects such as n decreasing with temperature and with increasing reverse bias.99 Equation (3.43) is sometimes expressed as (see Appendix 4.1) (3.44) I = Is eqV /nkT (1 − e−qV /kT ) Data plotted according to Eq. (3.43) as semilog I versus V are linear only for V ≫ kT /q as shown in Fig. 3.37. When plotting log[I /(1 − exp(−qV /kT ))] versus V using Eq. (3.44), the data are linear all the way to V = 0, also shown in Fig. 3.37. 3.5.1
CurrentVoltage
Among the currentvoltage methods, the barrier height is most commonly calculated from the current Is , determined by extrapolating the semilog I versus V curve to V = 0. The barrier height φB is calculated from Is in Eq. (3.43) according to kT AA∗ T 2 ln (3.45) φB = q Is The barrier height so determined is φB for zero bias. The most uncertain of the parameters in Eq. (3.45) is A∗ , rendering this method only as accurate as a knowledge of A∗ .
SCHOTTKY BARRIER HEIGHT
159
I, I/(1 − e−qV/kT) (A)
10−6 10−7 10−8
I/(1 − e−qV/kT)
10−9
slope = of/1/2.3nkT/q
10−10 10
Is I
−11
10−12
kT/q 0
0.05
0.1
0.15
0.2
Diode Voltage (V)
Fig. 3.37 Two ways of plotting currentvoltage for a Schottky diode. Reprinted with permission from Journal of Applied Physics, 69, 7142–7145, May 1991. Copyright American Institute of Physics.
Fortunately, A∗ appears in the “ln” term and an error of two in A∗ gives rise to an error of only 0.7 kT /q in φB . Nonetheless, errors do occur due to this uncertainty. An experimental semilog I versus V plot for a Cr/nSi diode is shown in Fig. 3.38(a). The current deviates from linearity for V > 0.2 V due to series resistance (discussed in
Forward Current (A)
100 rs = 0
10−1 10−2
No Anneal
10−3 460°C Anneal
10−4 10−5 10−6
A = 3.1 × 10−3 cm2 0
0.1
0.2
0.3
0.4
Forward Voltage (V) (a) 10−2
Current (A)
10−3
Slope = 15.8
10−4 10−5 10−6
0
0.05
0.1
0.15
0.2
Voltage (V) (b)
Fig. 3.38 (a) Currentvoltage characteristics of a Cr/nSi diode as deposited and annealed at 460◦ C measured at room temperature, (b) enlarged portion of (a). Courtesy of F. Hossain, Arizona State University.
160
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
Sections 4.2 and 4.3). The Schottky barrier diode with area 3.1 × 10−3 cm2 was fabricated on nSi.98 The device contains a p + guard ring around the periphery of the Schottky junction area to reduce the edge termination leakage current and it uses chromium (Cr) as the Schottky contact as well as titanium tungsten (TiW) as the diffusion barrier metal and nickel vanadium (NiV)gold (Au) as the metal overlayer and chromiumnickelgold as the back ohmic contact. The front and back metal were sputtered and evaporated, respectively. When the device is annealed at T = 460◦ C the barrier height increases and the current decreases. The expanded I –V curve in Fig. 3.38(b) allows the slope to be determined from which n = 1.05 and from the V = 0 intercept of Is = 5 × 10−6 A, the barrier height, calculated from Eq. (3.45), is φB (I –V ) = 0.58 V for A∗ = 110 A/cm2 K2 for nSi. 3.5.2
Current—Temperature
For V ≫ kT /q Eq. (3.43) can be written as ln(I /T 2 ) = ln(AA∗ ) − q(φB − V /n)/kT
(3.46)
A plot of ln(I /T 2 ) versus 1/T at a constant forward bias voltage V = V1 , sometimes called a Richardson plot, has a slope of −q(φB − V1 /n)/k and an intercept ln(AA∗ ) on the vertical axis. A Richardson plot for the diode of Fig. 3.38 is shown in Fig. 3.39. The slope is usually well defined, but the extraction of A∗ from the intercept is prone to error. Generally the 1000/T axis covers only a narrow range, 2.6 to about 3.4 in this example. Extrapolating the data from that narrow range to 1/T = 0 involves extrapolation over a long distance and any uncertainty in the data can produce a large uncertainty in A∗ . In Fig. 3.39 the intercept is given by log(AA∗ ) from which A∗ = 114 A/cm2 ·K2 . The barrier height is given by φB =
k d[ln(I /T 2 )] V1 2.3k d[log(I /T 2 )] V1 − = − n q d(1/T ) n q d(1/T )
(3.47)
The barrier height is obtained from the slope for a known forward bias voltage, but n must be determined independently. For the data of Fig. 3.39 with n = 1.05 determined
I/T 2 (A/K2)
10−5
10−6
V = 0.2 V 10−7 2.2
2.4
2.6
2.8
3
3.2
3.4
1000/T (K−1)
Fig. 3.39
Richardson plot of the “No Anneal” diode in Fig. 3.38 measured at V = 0.2 V.
SCHOTTKY BARRIER HEIGHT
161
from Fig. 3.38, V1 = 0.2 V, and the slope d[log(I /T 2 )]/d(1000/T ) = −1.97 we find φB (I − 1/T ) = 0.59 V, very close to φB (I –V ) = 0.58 V from the semilog I versus V plot. Sometimes ln(Is /T 2 ) is plotted against 1/T , with Is obtained from the intercept of semilog I versus V plots. The current I in Eq. (3.47) should then be replaced by Is and V1 = 0. An implicit assumption in the barrier height determination by the Richardson plot method is a temperatureindependent barrier height. Should it be temperature dependent, we can write φB as φB (T ) = φB (0) − ξ T (3.48) With this temperature dependence, Eq. (3.46) becomes ln(I /T 2 ) = ln(AA∗ ) + qξ/k − q(φB (0) − V /n)/kT
(3.49)
A Richardson plot now gives the “zero Kelvin” barrier height φB (0), and the intercept is ln(AA∗ ) + qξ/k. Now A∗ can no longer be determined. Nonlinearities are sometimes observed in Richardson plots at low temperatures. These may be due to current mechanisms other than thermionic emission current, usually manifesting themselves as n > 1.1. Nonlinear Richardson plots are also observed when both the barrier height and the ideality factor are temperature dependent. Accurate extraction of φB and A∗ becomes impossible, but linearity can be restored if nln(I /T 2 ) is plotted against 1/T .100 3.5.3
CapacitanceVoltage
The capacitance per unit area of a Schottky diode is given by101 C = A
±qKs εo (NA − ND ) 2(±Vbi ± V − kT /q)
(3.50)
where the “+” sign applies to ptype (NA > ND ) and the “−” sign to ntype (ND > NA ) substrates and V is the reversebias voltage. For ntype substrates ND > NA , Vbi < 0, and V < 0, whereas for ptype substrates ND < NA , Vbi > 0, and V > 0. The kT /q in the denominator accounts for the majority carrier tail in the spacecharge region which is omitted in the depletion approximation. The builtin potential is related to the barrier height by the relationship (3.51) φB = Vbi + Vo as seen in Fig. 3.36. Vo = (kT /q) ln(Nc /ND ), where Nc is the effective density of states in the conduction band. Plotting 1/(C/A)2 versus V gives a curve with the slope 2/[qKs εo (NA –ND )], and with the intercept on the V axis, Vi = −Vbi + kT /q. The barrier height is determined from the intercept voltage by φB = −Vi + Vo + kT /q
(3.52)
The doping density can be determined from the slope as discussed in Chapter 2. φB (C –V ) is approximately the flatband barrier height because it is determined from the 1/C 2 –V curve for 1/C 2 → 0 or C → ∞ indicating sufficient forward bias to cause flatband conditions in the semiconductor. A (C/A)−2 versus V plot of the diode of Fig. 3.38 is shown in Fig. 3.40. From the slope we find NA = 2 × 1016 cm−3 , and from Eq. (3.52)
162
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
7 × 1020
1/C 2 (cm4/F2)
6 × 1020 5 × 1020 4 × 1020 3 × 1020 2 × 1020 1 × 1020
−0.53 V
0 × 100 −1
1
3
5
7
9
Reverse Voltage (V)
Fig. 3.40 Reversebias 1/C 2 versus voltage of the “No Anneal” diode in Fig. 3.38 measured at room temperature.
the barrier height is φB (C –V ) = 0.74 V using the intercept voltage Vi = −0.53 V and the room temperature ni = 1010 cm−3 for Si. 3.5.4
Photocurrent
When a Schottky diode is irradiated with photons of sub band gap energy (hν < EG ), it is possible to excite carriers from the metal into the semiconductor as shown in Fig. 3.41(a). For hν > φB , electrons excited from the metal over the barrier into the semiconductor, are
hn
Iph
5
5
4
4
3
3 2
2 1 0 0.25
Pt/pSi T = 50 K NA = 8 × 1015 cm−3 0.3 0.35 Photon Energy (eV)
1
(Yhn)1/2 (arb. units)
Y1/2 (arb. units)
(a)
0 0.4
(b)
Fig. 3.41
Photoemission yields of a Pt/pSi Schottky diode. Data adapted from ref. 107.
COMPARISON OF METHODS
163
detected as photocurrent Iph . The light can be incident from the metal or the semiconductor side, since the semiconductor is transparent for these photon energies. The metal must be sufficiently thin for light penetration. The yield Y , defined as the ratio of the photocurrent to the absorbed photon flux, is given by102 Y = B(hν − qφB )2
(3.53)
where B is a constant. Y 1/2 is plotted versus hν, and an extrapolation of the linear portion of this curve, sometimes called a Fowler plot, to Y 1/2 = 0 gives the barrier height. The yield is also given as103 (hν − qφB )2 (3.54) Y =C hν where C is another constant. Example plots are shown in Fig. 3.41(b). The “toe” below 0.29 eV is due photonassisted thermionic emission. A Fowler plot is not always linear as predicted by the theory. When it is nonlinear it is difficult to determine φB . By differentiating Eq. (3.53) the deviation from linearity is much smaller than it is in the conventional Fowler plot, because the extended tail of the Fowler plot in the vicinity of the barrier height is removed by the differentiation.105 Moreover, the derivative plot is more sensitive to contact nonuniformities and has been used to detect such nonuniformities.105 The photocurrent technique relies only on photoexcited current flow and is little influenced by tunnel currents, especially if φB is obtained by extrapolating from hν ≫ φB , where only those electrons well above the barrier height contribute to the photocurrent. 3.5.5
Ballistic Electron Emission Microscopy (BEEM)
Ballistic Electron Emission Microscopy, based on scanning tunneling microscopy is a powerful lowenergy tool for nondestructive local characterization of semiconductor heterostructures, such as Schottky diodes and is discussed in more detail in Chapter 9. It can provide information on the homogeneity of the interface electronic structure with extremely high lateral resolution and can yield energyresolved information on hotelectron transport in the metal film, at the interface, and in the semiconductor.106 3.6
COMPARISON OF METHODS
A number of studies have been undertaken to compare barrier heights determined by the currentvoltage (I –V ), currenttemperature (I –T ), capacitancevoltage (C –V ), and photocurrent (P C) techniques. In one study the barrier height of evaporated Pt films on GaAs substrates was determined as φB (I –V ) = 0.81 V, φB (C –V ) = 0.98 V, and φB (P C) = 0.905 V.107 Which is the most reliable value? Any damage at the interface affects the I –V behavior because defects may act as recombination centers or as intermediate states for trapassisted tunnel currents. Either one of these mechanisms raises n and lowers φB . C –V measurements are less prone to such defects. However, defects can alter the spacecharge region width and hence the intercept voltage. Photocurrent measurements are less sensitive to such defects, and this method is judged to be the most reliable. Nevertheless, Fowler plots are not always linear. The first derivative plot usually does have a straightline portion, making φB extraction more reliable. The sequence φB (I –V ) < φB (P C) < φB (C –V ) was also observed for a variety of metals deposited on nGaAs and pGaAs.108 Barrier height measurements of Schottky
164
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
barriers on ptype InP gave φB (I –T ) < φB (C –V ).109 The difference was attributed to patchiness of barrier heights across the contact. When two Schottky diodes of different barrier height are connected in parallel, the lower barrier height dominates the I –V behavior, but the barrier height with the largest contact area dominates the C –V behavior.110 In the parallel conduction model, regions with different local barrier heights are assumed to be electrically independent and the total current is simply the sum of the currents flowing through all individual areas. This concept was extended theoretically to mixedphase contacts of varying dimensions but fixed area ratios, predicting that generally φB (C –V ) > φB (I –V ).111 For large contact regions results similar to those in ref. 110 were obtained. For smaller contact regions, however, the low barrier height regions were found to be pinched off by the high barrier height regions. The barrier height patchiness invoked to explain the differing barrier heights also predicts varying Richardson constants. It is frequently observed that A∗ varies with processing conditions such as annealing. It may well be that annealing causes the patchiness to vary and therefore A∗ to change. This would rule against using those methods that rely on a knowledge of A∗ for φB determination, favoring C –V and photocurrent measurements over I –V and I –T measurements. For the C –V method it is important that C −2 versus V plots be linear and independent of frequency. Photocurrent probes the device from outside the semiconductor, that is, photo emission is from the metal to the semiconductor. The I –V and C –V methods probe the device from the semiconductor side. It is for this reason that the latter two methods are more sensitive to spatial inhomogeneities, insulating layers between the metal and the semiconductor, doping inhomogeneities, surface damage, and tunneling. The P C technique is least influenced by these parameters and is therefore likely to yield the most reliable value of barrier height. For wellbehaved contacts with few of these degradation factors, all methods give values that agree reasonably well with one another.
3.7
STRENGTHS AND WEAKNESSES
TwoTerminal Methods: The twocontact, twoterminal contact resistance measurement technique is simple but the least detailed. The contact resistance data are corrupted by either the semiconductor bulk or sheet resistance. The method is only infrequently used today. The twoterminal contact string is used mainly as a process monitor. It does not give detailed contact resistance information nor can the specific contact resistivity be reliably extracted. The multiplecontact, twoterminal technique is usually employed in its transfer length method implementation, where the effect of the semiconductor sheet resistance is separated from the contact resistance and both contact resistance as well as specific contact resistivity can be determined. This method allows both front and end contact resistance measurements to be made. Complications in the interpretation of the experimental data arise due to three main effects: (1) the extrapolation of experimental data to obtain intercepts, (2) lateral current flow around the contact, and (3) the sheet resistance under the contact differing from the sheet resistance outside the contact window. Current flows laterally around the contact window whenever the contact window is narrower than the diffusion tap leading to erroneous contact resistances if the experimental data are analyzed by the conventional onedimensional theory. For the most reliable measurements the test structure should be configured to satisfy the following requirements: L > LT , Z ≫ L, δ = W − Z ≪ W as defined in Fig. 3.22.
165
APPENDIX 3.1
FourTerminal Method: The fourterminal or Kelvin structure is preferred over the two and threeterminal structures for several reasons. (1) There is only one metalsemiconductor contact and the contact resistance is measured directly as the ratio of a voltage to a current. Rc can therefore be very small. (2) Neither metal nor semiconductor sheet resistance enter into the Rc determination. Hence there is no practical limit to the value of Rc that can be measured. (3) The contact area can be made small to be consistent with contact areas used in highdensity ICs. This makes the method very simple and attractive. However, any lateral current flow obscures the interpretation. Modeling has shown two and threedimensional effects to be important, especially for appreciable gaps between the contact window and the diffusion edge. SixTerminal Method: The sixterminal method is very similar to the fourterminal technique. It incorporates the Kelvin structure, but additionally allows measurements of the front and end contact resistance as well as the contact sheet resistance. It is only slightly more complex than the fourterminal structure but does not require additional masking operations. For any of the contact resistance measurement methods it is difficult to determine absolute values of ρc . Simple onedimensional interpretations of the experimental data frequently give incorrect values of specific contact resistivity. Proper interpretation of the experimental data requires more exact modeling. This makes many of the data, determined in the past by simple onedimensional interpretation, suspect. Nevertheless, ρc can be used as a figure of merit but the experimental conditions under which they were obtained should be carefully specified. The contact resistance can be measured directly, but the measured resistance may not be the true contact resistance. Schottky Barrier Height: Strengths and weaknesses of Schottky barrier height measurements are discussed in Section 3.6. APPENDIX 3.1 Effect of Parasitic Resistance This discussion follows ref. 72. Equations (3.22) and (3.24) suggest the simple equivalent circuit in Fig. A3.1. When the current I flows as indicated, the resistance between A and ground is Rcf and between B and ground it is Rce as required. For the configuration of Fig. A3.2, the equivalent circuit is shown in Fig. A3.3. Rce , the end resistance, is similar to that in Fig. A3.1. The remainder of the contact has the resistance Rcf − Rce , making the contact resistance Rcf . The semiconductor region between the contacts of width Z is characterized by the resistance Rsh d/Z, where Rsh is the sheet resistance, leaving the small overlap regions of length d and width δ, characterized by the parallel resistance RP . The total resistance between the contacts is then RT (δ = 0) = 2Rce + [2(Rcf − Rce ) + Rsh d/Z]//RP /2
(A3.1)
where “//” denotes the parallel resistance combination. For δ = 0 RT (δ = 0) = 2Rcf + Rsh d/Z
(A3.2)
Multiplying the various terms in Eq. (A3.1) and solving for 2R cf + Rs d/Z, leads to 2Rcf + Rsh d/Z = 2Rce +
(RT (δ = 0) − 2Rce )RP = R′ RP /2 − RT (δ = 0) + 2Rce
(A3.3)
166
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
Rce I B
A Rcf − Rce
Fig. A3.1
Rcf − Rce
Equivalent circuit of a single contact showing the contact front and end resistances. d
Rs
Z
d
L
Fig. A3.2
TLM contact structure.
Rp
Rce Rshd/Z
Rcf − Rce
Rce Rcf − Rce
Rp
Fig. A3.3 Equivalent circuit of the TLM structure of Fig. A3.2, including the parallel resistances Rp .
RT (δ = 0) is the measured total resistance between two contacts and R ′ is the resistance corrected by including the two parallel resistances. The parallel resistance in Eq. (A3.1) is given by Rp = 2F Rsh
(A3.4)
F = K(k0 )/K(k1 )
(A3.5)
where F is the correction factor
and K is the complete elliptic integral K(k) =
0
π/2
dφ 1 − (k sin φ)2
(A3.6)
APPENDIX 3.2
12
d = 3 µm
10
4 µm
F
8
5 µm 6 µm 8 µm 10 µm
6 4 10 8
2 0
167
0
10
L = 25 µm 20
30 40 d (µm)
50
60
70
Fig. A3.4 Corrections factor versus d as a function of gap spacing δ for L = 25 µm. Reprinted after ref. 72 by permission of IEEE ( 2002, IEEE).
and k0 and k1 are given by k0 =
tanh(πd/4δ) ; k1 = tanh(π(d + 4L)/4δ)
1 − k02
(A3.7)
L is the contact length, d the contact spacing, and δ the gap, all shown on Fig. A3.2. The correction factor F is plotted in Fig. A3.4 versus contact spacing d as a function of gap spacing δ. APPENDIX 3.2 Alloys for Contacts to Semiconductors Material nSi pSi nSi pSi nGaAs nGaAs pGaAs pGaAs nGaInP nInP nInP pInP nAlGaAs∗ pAlGaAs∗ GaAs (n or p type) GaAs (n or p type) GaAs (n or p type) InP (n or p type) InP (n or p type)
Alloy
Contact Type
AuSb AuGa Al Al AuGe Sn AuZn In AuSn Ni/AuGe/Ni AuSn AuZn Ni/AuGe/Ni InSn Ni Al AuTi Au AuTi
ohmic ohmic ohmic Schottky ohmic ohmic ohmic ohmic ohmic ohmic ohmic ohmic ohmic ohmic Schottky Schottky Schottky Schottky Schottky
Source: BioRad. Ref. 112. ∗ with GaAs capping layer
168
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
REFERENCES 1. F. Braun “On the Current Transport in Metal Sulfides (in German),” Annal. Phys. Chem. 153, 556–563, 1874. 2. W. Schottky, “Semiconductor Theory of the Blocking Layer (in German),” Naturwissenschaften 26, 843, Dec. 1938; “On the Semiconductor Theory of Blocking and Point Contact Rectifiers (in German),” Z. Phys. 113, 367–414, July 1939; “Simplified and Expanded Theory of Boundary Layer Rectifiers (in German),” Z. Phys. 118, 539–592, Feb. 1942. 3. H.K. Henisch, Rectifying SemiConductor Contacts, Clarendon Press, Oxford, 1957. 4. R.T. Tung, “Recent Advances in Schottky Barrier Concepts,” Mat. Sci. Eng. R35, 1–138, 2001. 5. B. Schwartz (ed.), Ohmic Contacts to Semiconductors, Electrochem. Soc., New York, 1969. 6. V.L. Rideout, “A Review of the Theory and Technology for Ohmic Contacts to Group III–V Compound Semiconductors,” SolidState Electron. 18, 541–550, June 1975. 7. N. Braslau, “Alloyed Ohmic Contacts to GaAs,” J. Vac. Sci. Technol. 19, 803–807, Sept./Oct. 1981. 8. A. Piotrowska, A. Guivarch, and G. Pelous, “Ohmic Contacts to III–V Compound Semiconductors: A Review of Fabrication Techniques,” SolidState Electron. 26, 179–197, March 1983. 9. D.K. Schroder and D.L. Meier, “Solar Cell Contact Resistance—A Review,” IEEE Trans. Electron Devices ED31, 637–647, May 1984. 10. A.Y.C. Yu, “Electron Tunneling and Contact Resistance of MetalSilicon Contact Barriers,” SolidState Electron. 13, 239–247, Feb. 1970. 11. S.S. Cohen, “Contact Resistance and Methods for Its Determination,” Thin Solid Films 104, 361–379, June 1983. 12. A.G. Milnes and D.L. Feucht, Heterojunction and MetalSemiconductor Junctions, Academic Press, New York, 1972. 13. B.L. Sharma and R.K. Purohit, Semiconductor Heterojunctions, Pergamon, London, 1974; B.L. Sharma, “Ohmic Contacts to III–V Compound Semiconductors,” in Semiconductors and Semimetals, (R.K. Willardson and A.C. Beer, eds.), 15, 1–38, Academic Press, New York, 1981. 14. E.H. Rhoderick and R.H. Williams, MetalSemiconductor Contacts, 2nd ed., Clarendon, Oxford, 1988. 15. S.S. Cohen and G.S. Gildenblat, MetalSemiconductor Contacts and Devices, Academic Press, Orlando, FL, 1986. 16. N.F. Mott, “Note on the Contact Between a Metal and an Insulator or Semiconductor,” Proc. Camb. Phil. Soc. 34, 568–572, 1938. 17. W.E Spicer, I. Lindau, P.R. Skeath and C.Y. Su, “The Unified Model for Schottky Barrier Formation and MOS Interface States in 3–5 Compounds,” Appl. Surf. Sci. 9, 83–91, Sept. 1981; W. M¨onch, “On the Physics of MetalSemiconductor Interfaces,” Rep. Progr. Phys. 53, 221–278, March 1990; L.J. Brillson, “Advances in Understanding MetalSemiconductor Interfaces by Surface Science Techniques,” J. Phys. Chem. Solids 44, 703–733, 1983. 18. C.A. Mead, “Physics of Interfaces,” in Ohmic Contacts to Semiconductors (B. Schwartz, ed.), Electrochem. Soc., New York, 1969, 3–16. 19. J. Bardeen, “Surface States and Rectification at MetalSemiconductor Contact,” Phys. Rev. 71, 717–727, May 1947. 20. R.H. Williams, “The Schottky Barrier Problem,” Contemp. Phys. 23, 329–351, July/Aug. 1982. 21. L.J. Brillson, “Surface Photovoltage Measurements and Fermi Level Pinning: Comment on ’Development and Confirmation of the Unified Model for Schottky Barrier Formation and MOS Interface States on III–V Compounds’,” Thin Solid Films 89, L27–L33, March 1982. 22. J. Tersoff, “Recent Models of Schottky Barrier Formation,” J. Vac. Sci. Technol. B3, 1157–1161, July/Aug. 1985.
REFERENCES
169
23. I. Lindau and T. Kendelewicz, “Schottky Barrier Formation on III–V Semiconductor Surfaces: A Critical Evaluation,” CRC Crit. Rev. in Solid State and Mat. Sci. 13, 27–55, Jan. 1986. 24. F.A. Kroger, G. Diemer and H.A. Klasens, “Nature of Ohmic MetalSemiconductor Contacts,” Phys. Rev. 103, 279, July 1956. 25. S.M. Sze, Physics of Semiconductor Devices, 2nd ed., Wiley, New York, 1981, 255–258. 26. F.A. Padovani and R. Stratton, “Field and ThermionicField Emission in Schottky Barriers,” SolidState Electron. 9, 695–707, July 1966; F.A. Padovani, “The CurrentVoltage Characteristics of MetalSemiconductor Contacts,” in Semiconductors and Semimetals (R.K. Willardson and A.C. Beer, eds.), Academic Press, New York, 7A, 1971, 75–146. 27. C.R. Crowell and V.L. Rideout, “Normalized ThermionicField (TF) Emission in MetalSemiconductor (Schottky) Barriers,” SolidState Electron. 12, 89–105, Feb. 1969; “ThermionicField Resistance Maxima in MetalSemiconductor (Schottky) Barriers,” Appl. Phys. Lett. 14, 85–88, Feb. 1969. 28. K.K. Ng and R. Liu, “On the Calculation of Specific Contact Resistivity on (100) Si,” IEEE Trans. Electron Dev. 37, 1535–1537, June 1990. 29. R.S. Popovic, “MetalNType Semiconductor Ohmic Contact with a Shallow N + Surface Layer,” SolidState Electron. 21, 1133–1138, Sept. 1978. 30. D.F. Wu, D. Wang and K. Heime, “An Improved Model to Explain Ohmic Contact Resistance of nGaAs and Other Semiconductors,” SolidState Electron. 29, 489–494, May 1986. 31. G. Brezeanu, C. Cabuz, D. Dascalu and P.A. Dan, “A Computer Method for the Characterization of SurfaceLayer Ohmic Contacts,” SolidState Electron. 30, 527–532, May 1987. 32. C.Y. Chang and S.M. Sze, “Carrier Transport Across MetalSemiconductor Barriers,” SolidState Electron. 13, 727–740, June 1970. 33. C.Y. Chang, Y.K. Fang and S.M. Sze, “Specific Contact Resistance of MetalSemiconductor Barriers,” SolidState Electron. 14, 541–550, July 1971. 34. W.J. Boudville and T.C. McGill, “Resistance Fluctuations in Ohmic Contacts due to Discreteness of Dopants,” Appl. Phys. Lett. 48, 791–793, March 1986. 35. Data for nSi were taken from: 9, 32, 39, 43, 44, 45, 49, 55, 58, 69; S.S. Cohen, P.A. Piacente, G. Gildenblat and D.M. Brown, “Platinum Silicide Ohmic Contacts to Shallow Junctions in Silicon,” J. Appl. Phys. 53, 8856–8862, Dec. 1982; S. Swirhun, K.C. Saraswat and R.M. Swanson, “Contact Resistance of LPCVD W/Al and PtSi/Al Metallization,” IEEE Electron Dev. Lett. EDL5, 209–211, June 1984; S.S. Cohen and G.S. Gildenblat, “Mo/Al Metallization for VLSI Applications,” IEEE Trans. Electron Dev. ED34, 746–752, April 1987. 36. Data for pSi were taken from: 39, 43, 44, 49, 55, 69; S.S. Cohen, P.A. Piacente, G. Gildenblat and D.M. Brown, “Platinum Silicide Ohmic Contacts to Shallow Junctions in Silicon,” J. Appl. Phys. 53, 8856–8862, Dec. 1982; S. Swirhun, K.C. Saraswat and R.M. Swanson, “Contact Resistance of LPCVD W/Al and PtSi/Al Metallization,” IEEE Electron Dev. Lett. EDL5, 209–211, June 1984; S.S. Cohen and G.S. Gildenblat, “Mo/Al Metallization for VLSI Applications,” IEEE Trans. Electron Dev. ED34, 746–752, April 1987; G.P. Carver, J.J. Kopanski, D.B. Novotny and R.A. Forman, “Specific Contact Resistivity of MetalSemiconductor Contacts—A New, Accurate Method Linked to Spreading Resistance,” IEEE Trans. Electron Dev. ED35, 489–497, April 1988. 37. Data for nGaAs can be found in ref. 6 and references therein. 38. Data for pGaAs can be found in: 6, C.J. Nuese and J.J. Gannon, “SilverManganese Evaporated Ohmic Contacts to ptype GaAs,” J. Electrochem. Soc. 115, 327–328, March 1968; K.L. Klohn and L. Wandinger, “Variation of Contact Resistance of MetalGaAs Contacts with Impurity Concentration and Its Device Implications,” J. Electrochem. Soc. 116, 507–508, April 1969; H. Matino and M. Tokunaga, “Contact Resistances of Several Metals and Alloys to GaAs,” J. Electrochem. Soc. 116, 709–711, May 1969; H.J. Gopen and A.Y.C. Yu, “Ohmic Contacts to Epitaxial GaAs,” SolidState Electron. 14, 515–517, June 1971; O. Ishihara, K.Nishitani, H.Sawano and S.Mitsue, “Ohmic Contacts to PType GaAs,” Japan. J. Appl.
170
39. 40.
41. 42. 43. 44. 45. 46. 47.
48. 49. 50. 51. 52. 53.
54.
55. 56.
57.
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
Phys. 15, 1411–1412, July 1976; C.Y. Su and C. Stolte, “Low Contact Resistance Non Alloyed Ohmic Contacts to Zn Implanted GaAs,” Electron. Lett. 19, 891–892, Oct. 1983; R.C. Brooks, C.L. Chen, A. Chu, L.J. Mahoney, J.G. Mavroides, M.J. Manfra and M.C. Finn, “LowResistance Ohmic Contacts to pType GaAs Using Zn/Pd/Au Metallization,” IEEE Electron Dev. Lett. EDL6, 525–527, Oct. 1985. S.E. Swirhun and R.M. Swanson, “Temperature Dependence of Specific Contact Resistivity,” IEEE Electron Dev. Lett. EDL7, 155–157, March 1986. D.M. Brown, M. Ghezzo and J.M. Pimbley, “Trends in Advanced Process Technology—Submicrometer CMOS Device Design and Process Requirements,” Proc. IEEE, 74, 1678–1702, Dec. 1986. M.V. Sullivan and J.H. Eigler, “Five Metal Hydrides as Alloying Agents on Silicon,” J. Electrochem. Soc. 103, 218–220, April 1956. R.H. Cox and H. Strack, “Ohmic Contacts for GaAs Devices,” SolidState Electron. 10, 1213–1218, Dec. 1967. R.D. Brookes and H.G. Mathes, “Spreading Resistance Between Constant Potential Surfaces,” Bell Syst. Tech. J. 50, 775–784, March 1971. H. Muta, “Electrical Properties of PlatinumSilicon Contact Annealed in an H2 Ambient,” Japan. J. Appl. Phys. 17, 1089–1098, June 1978. A.K. Sinha, “Electrical Characteristics and Thermal Stability of Platinum SilicidetoSilicon Ohmic Contacts Metallized with Tungsten,” J. Electrochem. Soc. 120, 1767–1771, Dec. 1973. G.Y. Robinson, “Metallurgical and Electrical Properties of Alloyed Ni/AuGe Films on nType GaAs,” SolidState Electron. 18, 331–342, April 1975. G.P. Carver, J.J. Kopanski, D.B. Novotny, and R.A. Forman, “Specific Contact Resistivity of MetalSemiconductor Contacts—A New, Accurate Method Linked to Spreading Resistance,” IEEE Trans. Electron Dev. 35, 489–497, April 1988. A. Shepela, “The Specific Contact Resistance of P d2 Si Contacts on n and pSi,” SolidState Electron. 16, 477–481, April 1973. C.Y. Ting and C.Y. Chen, “A Study of the Contacts of a Diffused Resistor,” Solid State Electron. 14, 433–438, June 1971. J.M. Andrews, “A Lithographic Mask System for MOS FineLine Process Development.” Bell Syst. Tech. J. 62, 1107–1160, April 1983. D.P. Kennedy and P.C. Murley, “A TwoDimensional Mathematical Analysis of the Diffused Semiconductor Resistor,” IBM J. Res. Dev. 12, 242–250, May 1968. H. Murrmann and D. Widmann, “Current Crowding on Metal Contacts to Planar Devices,” IEEE Trans. Electron Dev. ED16, 1022–1024, Dec. 1969. H. Murrmann and D. Widmann, “Measurement of the Contact Resistance Between Metal and Diffused Layer in Si Planar Devices (in German),” SolidState Electron. 12, 879–886, Dec. 1969. H.H. Berger, “Models for Contacts to Planar Devices,” SolidState Electron. 15, 145–158, Feb. 1972; H.H. Berger, “Contact Resistance and Contact Resistivity,” J. Electrochem. Soc. 119, 507–514, April 1972. J.M. Pimbley, “DualLevel Transmission Line Model for Current Flow in MetalSemiconductor Contacts,” IEEE Trans. Electron Dev. ED33, 1795–1800, Nov. 1986. G.K. Reeves, P.W. Leech, and H.B. Harrison, “Understanding the Sheet Resistance Parameter of Alloyed Ohmic Contacts Using a Transmission Line Model,” SolidState Electron. 38, 745–751, April 1995; G.K. Reeves and H.B. Harrison, “An Analytical Model for Alloyed Ohmic Contacts Using a Trilayer Transmission Line Model.” IEEE Trans. Electron Dev. 42, 1536–1547, Aug. 1995. J.G.J. Chern and W.G. Oldham, “Determining Specific Contact Resistivity from Contact End Resistance Measurements,” IEEE Electron Dev. Lett. EDL5, 178–180, May 1984.
REFERENCES
58.
59.
60.
61. 62. 63. 64.
65. 66. 67.
68.
69.
70. 71.
72.
171
Comments on this Paper are: J.A. Mazer and L.W. Linholm, “Comments on ’Determining Specific Contact Resistivity from Contact End Resistance Measurements’,” IEEE Electron Dev. Lett. EDL5, 347–348, Sept. 1984; J. Chern and W.G. Oldham, “Reply to ’Comments on Determining Specific Contact Resistivity from Contact End Resistance Measurements’,” IEEE Electron Dev. Lett. EDL5, 349, Sept. 1984; M. Finetti, A. Scorzoni and G. Soncini, “A Further Comment on ’Determining Specific Contact Resistivity from Contact End Resistance Measurements’,” IEEE Electron Dev. Lett. EDL6, 184–185, April 1985. S.E. Swirhun, W.M. Loh, R.M. Swanson and K.C. Saraswat, “Current Crowding Effects and Determination of Specific Contact Resistivity from Contact End Resistance (CER) Measurements,” IEEE Electron Dev. Lett. EDL6, 639–641, Dec. 1985. G.K. Reeves, “Specific Contact Resistance Using a Circular Transmission Line Model,” SolidState Electron. 23, 487–490, May 1980; A.J. Willis and A.P. Botha, “Investigation of Ring Structures for MetalSemiconductor Contact Resistance Determination,” Thin Solid Films 146, 15–20, Jan. 1987. S.S. Cohen and G.Sh. Gildenblat, VLSI Electronics, 13, MetalSemiconductor Contacts and Devices, Academic Press, Orlando, FL, 1986, p. 115; G.S. Marlow and M.B. Das, “The Effects of Contact Size and NonZero Metal Resistance on the Determination of Specific Contact Resistance,” SolidState Electron. 25, 91–94, Feb. 1982; M. Ahmad and B.M. Arora, “Investigation of AuGeNi Contacts Using Rectangular and Circular Transmission Line Model,” SolidState Electron. 35, 1441–1445, Oct. 1992. J. Klootwijk, Philips Research Labs., private communication. A. Scorzoni, M. Vanzi, and A. Querz`e, “The Circular Resistor (CR)—A Novel Structure for the Analysis of VLSI Contacts,” IEEE Trans. Electron Dev. 37, 1750–1757, July 1990. E.G. Woelk, H. Kr¨autle and H. Beneking, “Measurement of Low Resistive Ohmic Contacts on Semiconductors,” IEEE Trans. Electron Dev. ED33, 19–22, Jan. 1986. W. Shockley in A. Goetzberger and R.M. Scarlett, “Research and Investigation of Inverse Epitaxial UHF Power Transistors,” Rep. No. AFALTDR64207, Air Force Avionics Lab., WrightPatterson Air Force Base, OH, Sept. 1964. L.K. Mak, C.M. Rogers, and D.C. Northrop, “Specific Contact Resistance Measurements on Semiconductors,” J. Phys. E: Sci. Instr. 22, 317–321, May 1989. G.K. Reeves and H.B. Harrison “Obtaining the Specific Contact Resistance from Transmission Line Model Measurements,” IEEE Electron Dev. Lett. EDL3, 111–113, May 1982. L. Gutai, “Statistical Modeling of Transmission Line Model Test Structures—Part I: The Effect of Inhomogeneities on the Extracted Contact Parameters,” “Part II: TLM Test Structure with Four or More Terminals: A Novel Method to Characterize Nonideal Planar Contacts in Presence of Inhomogeneities,” IEEE Trans. Electron Dev. 37, 2350–2360, 2361–2380, Nov. 1990. D.B. Scott, W.R. Hunter and H. Shichijo, “A Transmission Line Model for Silicided Diffusions: Impact on the Performance of VLSI Circuits,” IEEE Trans. Electron Dev. ED29, 651–661, April 1982. G.K. Reeves and H.B. Harrison, “Contact Resistance of PolysiliconSilicon Interconnections,” Electron. Lett. 18, 1083–1085, Dec. 1982; G. Reeves and H.B. Harrison, “Determination of Contact Parameters of Interconnecting Layers in VLSI Circuits,” IEEE Trans. Electron Dev. ED33, 328–334, March 1986. B. Kovacs and I. Mojzes, “Influence of Finite Metal Overlayer Resistance on the Evaluation of Contact Resistivity,” IEEE Trans. Electron Dev. ED33, 1401–1403, Sept. 1986. I.F. Chang, “Contact Resistance in Diffused Resistors,” J. Electrochem. Soc. 117, 368–372, Feb. 1970; A. Scorzoni and U. Lieneweg, “Comparison Between Analytical Methods and FiniteDifference in TransmissionLine Tap Resistors and LType CrossKelvin Resistors,” IEEE Trans. Electron Dev. ED37, 1099–1103, June 1990. E.F. Chor and J. Lerdworatawee, “QuasiTwoDimensional Transmission Line Model (QTDTLM) for Planar Ohmic Contact Studies,” IEEE Trans. Electron Dev. 49, 105–111, Jan. 2002.
172
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
73. K.K. Shih and J.M. Blum, “Contact Resistances of AuGeNi, AuZn and Al to III–V Compounds,” SolidState Electron. 15, 1177–1180, Nov. 1972. 74. S.S. Cohen, G. Gildenblat, M. Ghezzo and D.M. Brown, “Al0.9%Si/Si Ohmic Contacts to Shallow Junctions,” J. Electrochem. Soc. 129, 1335–1338, June 1982. 75. S.J. Proctor and L.W. Linholm, “A Direct Measurement of Interfacial Contact Resistance,” IEEE Electron Dev. Lett. EDL3, 294–296, Oct. 1982; S.J. Proctor, L.W. Linholm and J.A. Mazer, “Direct Measurements of Interfacial Contact Resistance, End Resistance, and Interfacial Contact Layer Uniformity,” IEEE Trans. Electron Dev. ED30, 1535–1542, Nov. 1983. 76. J.A. Mazer, L.W. Linholm and A.N. Saxena, “An Improved Test Structure and KelvinMeasurement Method for the Determination of Integrated Circuit Front Contact Resistance,” J. Electrochem. Soc. 132, 440–443, Feb. 1985. 77. A.A. Naem and D.A. Smith, “Accuracy of the FourTerminal Measurement Techniques for Determining Contact Resistance,” J. Electrochem. Soc. 133, 2377–2380, Nov. 1986. 78. M. Finetti, A. Scorzoni and G. Soncini, “Lateral Current Crowding Effects on Contact Resistance Measurements in Four Terminal Resistor Test Patterns,” IEEE Electron Dev. Lett. EDL5, 524–526, Dec. 1984. 79. A.S. Holland, G.K. Reeves, and P.W. Leech, “Universal Error Corrections for Finite Semiconductor Resistivity in CrossKelvin Resistor Test Structures,” IEEE Trans. Electron Dev. 51, 914–919, June 2004. 80. M. Ono, A. Nishiyama, and A. Toriumi, “A Simple Approach to Understanding Errors in the CrossBridge Kelvin Resistor and a New Pattern for Measurements of Specific Contact Resistivity,” SolidState Electron. 46, 1325–1331, Sept. 2002. 81. W.M. Loh, S.E. Swirhun, T.A. Schreyer, R.M. Swanson and K.C. Saraswat, “Modeling and Measurement of Contact Resistances,” IEEE Trans. Electron Dev. ED34, 512–524, March 1987. 82. A. Scorzoni, M. Finetti, K. Grahn, I. Suni and P. Cappelletti, “Current Crowding and Misalignment Effects as Sources of Error in Contact Resistivity Measurements—Part I: Computer Simulation of Conventional CER and CKR Structures,” IEEE Trans. Electron. Dev. ED34, 525–531, March 1987. 83. P. Cappelletti, M. Finetti, A. Scorzoni, I. Suni, N. Cirelli and G.D. Libera, “Current Crowding and Misalignment Effects as Sources of Error in Contact Resistivity Measurements—Part II: Experimental Results and Computer Simulation of SelfAligned Test Structures,” IEEE Trans. Electron. Dev. ED34, 532–536, March 1987. 84. U. Lieneweg and D.J. Hannaman, “New Flange Correction Formula Applied to Interfacial Resistance Measurements of Ohmic Contacts to GaAs,” IEEE Electron Dev. Lett. EDL8, 202–204, May 1987. 85. S.A. Chalmers and B.G. Streetman, “Lateral Diffusion Contributions to Contact Mismatch in Kelvin Resistor Structures,” IEEE Trans. Electron Dev. ED34, 2023–2024, Sept. 1987. 86. W.T. Lynch and K.K. Ng, “A Tester for the Contact Resistivity of SelfAligned Silicides,” IEEE Int. Electron Dev. Meet. Digest, San Francisco, 1988, 352–355. 87. T.F. Lei, L.Y. Leu and C.L. Lee, “Specific Contact Resistivity Measurement by a Vertical Kelvin Test Structure,” IEEE Trans. Electron Dev. ED34, 1390–1395, June 1987; W.L. Yang, T.F. Lei, and C.L. Lee, “Contact Resistivities of Al and Ti on Si Measured by a SelfAligned Vertical Kelvin Test Resistor Structure,” SolidState Electron. 32, 997–1001, Nov. 1989. 88. C.L. Lee, W.L. Yang and T.F. Lei, “The Spreading Resistance Error in the Vertical Kelvin Test Resistor Structure for the Specific Contact Resistivity,” IEEE Trans. Electron Dev. ED35, 521–523, April 1988. 89. L.Y. Leu, C.L. Lee, T.F. Lei, and W.L. Yang, “Numerical Simulation of the Vertical Kelvin Test Structure for Specific Contact Resistivity,” SolidState Electron. 33, 177–188, Feb. 1990.
REFERENCES
173
90. J.G.J. Chern, W.G. Oldham and N. Cheung, “ContactElectromigrationInduced Leakage Failure in AluminumSilicon to Silicon Contacts,” IEEE Trans. Electron Dev. ED32, 1341–1346, July 1985. 91. H. Onoda, “Dependence of AlSi/Al Contact Resistance on Substrate Surface Orientation,” IEEE Electron Dev. Lett. EDL9, 613–615, Nov. 1988. 92. T.J. Faith, R.S. Iven, L.H. Reed, J.J. O’Neill Jr., M.C. Jones and B.B. Levin, “Contact Resistance Monitor for Si ICs,” J. Vac. Sci. Technol. B2, 54–57, Jan./March 1984. 93. N. Braslau, “Alloyed Ohmic Contacts to GaAs,” J. Vac. Sci. Technol. 19, 803–807, Sept./Oct. 1981; “Ohmic Contacts to GaAs,” Thin Solid Films 104, 391–397, June 1983. 94. J. Willer, D. Ristow, W. Kellner and H. Oppolzer, “Very Stable Ge/Au/Cr/Au Ohmic Contacts to GaAs,” J. Electrochem. Soc. 135, 179–181, Jan. 1988. 95. J.M. Andrews and M.P. Lepselter, “Reverse CurrentVoltage Characteristics of MetalSilicide Schottky Diodes,” SolidState Electron. 13, 1011–1023, July 1970. 96. A.K. Srivastava, B.M. Arora, and S. Guha, “Measurement of Richardson Constant of GaAs Schottky Barriers,” SolidState Electron. 24, 185–191, Feb. 1981, and references therein. 97. M. Missous and E.H. Rhoderick, “On the Richardson Constant for Aluminum/Gallium Arsenide Schottky Diodes,” J. Appl. Phys. 69, 7142–7145, May 1991. 98. F. Hossain, Arizona State University. 99. R.T. Tung, “Electron Transport of Inhomogeneous Schottky Barriers,” Appl. Phys. Lett. 58, 2821–2823, June 1991. 100. A.S. Bhuiyan, A. Martinez and D. Esteve, “A New Richardson Plot for NonIdeal Schottky Diodes,” Thin Solid Films 161, 93–100, July 1988. 101. A.M. Goodman, “MetalSemiconductor Barrier Height Measurement by the Differential Capacitance Method—One Carrier System,” J. Appl. Phys. 34, 329–338, Feb. 1963. 102. R.H. Fowler, “The Analysis of Photoelectric Sensitivity Curves for Clean Metals at Various Temperatures,” Phys. Rev. 38, 45–56, July 1931. 103. W. M¨onch, Electronic Properties of Semiconductor Interfaces, Springer, Berlin, 2004, 63–67. 104. R. Turan, N. Akman, O. Nur, M.Y.A. Yousif, and M. Willander, “Observation of Strain Relaxation in Si1−x Gex layers by Optical and Electrical Characterisation of a Schottky Junction,” Appl. Phys. A72, 587–593, May 2001. 105. T. Okumura and K.N. Tu, “Analysis of Parallel Schottky Contacts by Differential Internal Photoemission Spectroscopy,” J. Appl. Phys. 54, 922–927, Feb. 1983. 106. L.D. Bell and W.J. Kaiser, “Ballistic Electron Emission Microscopy: A NanometerScale Probe of Interfaces and Carrier Transport,” Annu. Rev. Mat. Sci. 26, 189–222, 1996. 107. C. Fontaine, T. Okumura and K.N. Tu, “Interfacial Reaction and Schottky Barrier Between Pt and GaAs,” J. Appl. Phys. 54, 1404–1412, March 1983. 108. T. Okumura and K.N. Tu, “Electrical Characterization of Schottky Contacts of Au, Al, Gd and Pt on nType and pType GaAs,” J. Appl. Phys. 61, 2955–2961, April 1987. 109. Y.P. Song, R.L. Van Meirhaeghe, W.H. Lafl`ere and F. Cardon, “On the Difference in Apparent Barrier Height as Obtained from CapacitanceVoltage and CurrentVoltageTemperature Measurements on Al/pInP Schottky Barriers,” SolidState Electron. 29, 633–638, June 1986. 110. I. Ohdomari and K.N. Tu, “Parallel Silicide Contacts,” J. Appl. Phys. 51, 3735–3739, July 1980. 111. J.L. Freeouf, T.N. Jackson, S.E. Laux and J.M. Woodall, “Size Dependence of “Effective” Barrier Heights of MixedPhase Contacts,” J. Vac. Sci. Technol. 21, 570–574, July/Aug. 1982. 112. BioRad, Semiconductor Newsletter, Winter 1988.
174
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
PROBLEMS 3.1
The I –V data of a forwardbiased pn junction are given in the following table. Determine the temperature T and the series resistance Rs for this device. V (V ) 0.0000 0.025000 0.050000 0.075000 0.10000 0.12500 0.15000 0.17500 0.20000 0.22500 0.25000 0.27500 0.30000 0.32500
3.2
I (A) 0.0000 1.2910e12 4.2480e12 1.1020e11 2.6540e11 6.2090e11 1.4350e10 3.3010e10 7.5760e10 1.7370e09 3.9800e09 9.1190e09 2.0890e08 4.7860e08
V (V ) 0.35000 0.37500 0.40000 0.42500 0.45000 0.47500 0.50000 0.52500 0.55000 0.57500 0.60000 0.62500 0.65000 0.67500
I (A) 1.0960e07 2.5120e07 5.7540e07 1.3180e06 3.0190e06 6.9130e06 1.5820e05 3.6180e05 8.2520e05 0.00018720 0.00041910 0.00091340 0.0018820 0.0035060
V (V ) 0.70000 0.72500 0.75000 0.77500 0.80000 0.82500 0.85000 0.87500 0.90000 0.92500 0.95000 0.97500 1.0000
I (A) 0.0062910 0.010050 0.014290 0.019610 0.025430 0.031850 0.038330 0.045040 0.051940 0.058990 0.066160 0.073440 0.080800
A portion of a semiconductor test structure is shown in Fig. P3.2. It incorporates a TLM test structure, a oneelement contact string and a circular Schottky diode. Several measurements were made. Simple Contact String
TLM Test Structure
L
d1 d2
d3
Schottky Diode B
A d5 d6 d5
d4
D 0 xj
p+
t
x
0.4 6.71 × 10−4
0.5 0.0148
ntype (ND)
Fig. P3.2
(a) Schottky Diode I –V : V (V ) I (A)
0.1 5.59 × 10−8
0.2 1.36 × 10−6
0.3 3.04 × 10−5
Determine the barrier height φB (in V ) and the ideality factor n. (b) p+ Layer: The p + majority carrier profile is approximated by p(x) ≈ NA (x) = 8 × 1019 exp(−x/5 × 10−6 ), with x in cm. Determine the junction depth xj (in cm), and the sheet resistance Rsh (in /square) of the p + layer; neglect the contribution of the electrons in the p + layer.
PROBLEMS
175
(c) TLM Test Structure: The TLM test structure gave the following values: d (µm) RT ()
d1 = 1 8.2
d2 = 3 13.41
d3 = 7 23.83
d4 = 10 31.65
Determine the sheet resistance Rsh , the contact resistance Rc (), and the specific contact resistance ρc (cm2 ). (d) One Element Contact String: Determine the resistance between points A and B (in ). Neglect the metal resistance. (e) Resistance Through the Wafer: Suppose two circular contacts of diameter 1 cm are formed on opposite sides of the ntype wafer and that the current flow from top to bottom is confined to this area as it flows through the wafer. Determine the resistance between these two contacts using ρc = (∂J /∂V )−1 evaluated at V = 0 assuming current flow is due to thermionic emission. Z (width of the p+ layer) = 100 µm, d5 = 50 µm, d6 = 500 µm, L = 25 µm, D = 1 mm, A∗∗ = 110 A/cm2 · K, substrate ρ = 0.1 cm (to convert to doping density, use Fig. A1.1), t = 750 µm, T = 300 K, Ks = 11.7, use µp = 60 cm2 /V s. Neglect the spacecharge region width of the p + n junction in these calculations, i.e., assume it to be zero. The I–V and C –V curves of two Schottky diodes were measured. These diodes are fabricated on identical ntype substrates. One diode (device 1) has barrier height φB1 and area A and the other consists of a diode with barrier height φB1 over half the area and φB2 over the other half area. The total area is the same for both devices. The Schottky diode equations are I = AA∗ T 2 e−qφB /kT (eq(V −I r s )/nkT − 1) = Io (eq(V −I r s )/nkT − 1) and Ks εo qN D C=A 2(Vbi − V ) Io is the saturation current. The I –V curve of device 1 is shown in Fig. P3.3. 10−1 10−2 10−3 I (A)
3.3
10−4 10−5 10−6 10−7 10−8
T = 300 K 0
0.1
0.2
0.3 V (V)
Fig. P3.3
0.4
0.5
0.6
176
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
The saturation currents as a function of temperature are: Device 1:
T (K) 300 350 400
Io1 (A) 1.57 × 10−8 1.02 × 10−6 2.42 × 10−5
Device 2:
T (K) 300 350 400
Io2 (A) 3.83 × 10−7 1.46 × 10−5 2.33 × 10−4
The roomtemperature, zerobiased capacitance is: C1 (0V ) = 4.092 × 10−11 F ; C2 (0V ) = 4.335 × 10−11 F . Ks = 11.7, εo = 8.854 × 10−14 F/cm, k = 8.617 × 10−5 eV/K, A = 10−3 cm2 , ND = 1016 cm−3 , ni = 1010 cm−3 , Ei = EG /2 = 0.56 eV. Determine A∗ , n, rs , φB1 , and φB2 . 3.4
Consider a Schottky diode whose barrier height is not constant over the diode area. Determine the effective barrier height φB,eff , from (a) log(I)—V plot (b) (A/C)2 —V plot where the barrier heights and areas are: φB1 = 0.6 V, A1 = 0.2 A and φB2 = 0.7 V, A2 = 0.8 A, where A is the area given below. Use A∗ = 100 A/cm2 · K 2 , A = 10−3 cm2 , n = 1, T = 300 K, Ks = 11.7, ND = 1015 cm−3 , and NC = 2.5 × 1019 cm−3 . The effective barrier height is defined by the equations I = AA∗ T 2 e−qφB,eff /kT (eqV /nkT − 1) for the I–V plot, and by kT Nc ln for the (A/C)2 —V plot. Vbi = φB,eff + V0 = φB,eff + q ND Neglect the “kT/q” term in the capacitance equation in the book.
3.5
The transfer length contact resistance test structure is used to measure various electrical parameters. The sheet resistance between contacts Rsh is different from the sheet resistance under the contacts Rsk in this case. (a) For negligible metal resistance, the following data were obtained: d (µm) V (mV)
3 43.6
5 49.6
10 64.6
20 94.6
30 124.6
50 184.6
L = 12 µm, Z = 100 µm, I = 10 mA. The end resistance for this test structure is Re = 3.4 × 10−3 . Determine Rsh , Rsk , Rc , ρc , and LT c . (b) One day when these measurements were made, it was found that the contact resistance had increased to Rc = 5.18 . It is suspected that the metal resistance has increased due to a problem with the metal deposition system. All other parameters are unchanged. Determine the metal sheet resistance Rsm . 3.6
The I –V curves of a Schottky diode are shown as a function of temperature in Fig. P3.6. The diode has a circular area of 1 mm diameter. The current is given by I = AA∗ T 2 e−qφB /kT (eqV /nkT − 1). Determine A∗ , n, and φB .
PROBLEMS
177
100
I (A)
10−2 10−4
T = 250 K T = 300 K T = 350 K T = 400 K T = 450 K T = 500 K
10−6 10−8
0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
V (V)
Fig. P3.6
3.7
The I–V curves of a forwardbiased pn junction is shown in Fig. P3.7. Determine the temperature T for the “T =?” curve and the series resistance rs for the “T = 300 K” curve. 100 10−1 10−2 T=?
I (A)
10−3 10−4
T = 300 K
10−5 10−6 10−7 10−8
0
0.2
0.4
0.6
0.8
1
V (V)
Fig. P3.7
3.8
The pn junction diode I –V equation at high injection levels, neglecting series resistance, is: I = I01 (eqV /2kT − 1) With series resistance, but no high injection level effects, the I –V equation is: I = I02 (eq(V −I r s )/kT − 1) Discuss how one can determine which equation applies for experimental I –V data that fall in that region of the I –V curve where either one of these equations could be valid.
178
3.9
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
The doping density versus depth for the nlayer is shown for two cases in Fig. P3.9. Discuss the sheet resistances and the specific contact resistivities for these two cases, i.e., are they the same or not and why or why not. ND n
(a) (b)
p
x
Fig. P3.9
3.10 The contact resistance of contact A is RcA in Fig. P3.10. It is measured between points A–C and between points A–B. For both contacts A and B, we have LT < L, where LT is the transfer length and L is the contact length. Choose one answer from the following list and explain it briefly. RcA (A–C) > RcA (A–B) RcA (A–C) = RcA (A–B) RcA (A–C) < RcA (A–B) B
A L
C
Fig. P3.10
3.11 In the TLM test structure the resistance between adjacent contacts is measured and displayed in Fig. P3.11 as an RT vs. d plot. What parameters are determined with this test structure? One day something goes wrong during processing and a thin oxide film remains on the nlayer before the metal contacts are deposited. Show on the RT vs. d plot in Fig. P3.11 the data points that would be measured for this case. Contact spacing and size and the nlayer are the same as before. The oxide film is thin enough that current can tunnel through it and can be thought of as a resistive layer. d RT n p
d
Fig. P3.11
PROBLEMS
179
3.12 Two metallic contacts are made on an ntype semiconductor wafer. The I –V curve in Fig. P3.12 is for the case: contact A is a Schottky contact, contact B is an ohmic contact. Draw on the same figure the I –V curve when both contacts are Schottky contacts. V
+I
I
A
ntype
+V B
Fig. P3.12
3.13 The I –V curves of two Schottky diodes are shown in Fig. P3.13 for the same temperature T . The relevant equation for the current is I = AA∗ T 2 exp(−qφB /kT )(exp(qV /nkT ) − 1) The device parameter that has changed in going from curve (A) to curve (B) is: A∗
φB
n
Choose one answer and explain. 10−5 10−6 (A)
I (A)
10−7
(B)
10−8 10−9 10−10 10−11
0
0.1
0.2
0.3
V (V)
Fig. P3.13
3.14 A Schottky barrier diode is formed on both n and ptype semiconductor regions as shown in Fig. P3.14. (a) Draw the I –V curve for this device.
180
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
(b) Draw the band diagrams at the surface (x = 0) and at x = x1 for V = 0. The doping densities and the barrier heights and A* are the same for both semiconductor types and the areas on the two semiconductor types are identical.
V I 0 Schottky Contact x1
n Type
pType
Ohmic Contact
x
Fig. P3.14
3.15 The I —V and C —V plots of a Schottky diode on a Si substrate are shown in Fig. P3.15. From the I —V curve determine φB , A∗, rs , T ; from the C —V curve determine φB , ND . Use Ks = 11.7, k = 8.617 × 10−5 eV/K, εo = 8.854 × 10−14 F /cm, diode ideality factor n = 1, Area A = 10−3 cm2 , EG = 1.12 eV, ni = 9.15 × 1019 (T/300)2 exp(−6880/T)cm−3 . The saturation current is given at various temperatures as: T (K) 250 275 300 325 350 375 400
Is (A) 5.01 × 10−9 7.63 × 10−8 7.49 × 10−7 5.34 × 10−6 2.81 × 10−5 1.21 × 10−4 4.41 × 10−4
3.16 The resistance of a 100element (N = 100) contact chain RT is given by ρc L coth . RT = N(2Rc + Rs ) where Rc = LT Z LT Two elements of this chain are shown in Fig. P3.16. Determine and plot RT versus ρc for ρc = 10−8 to 10−5 cm2 as a loglog plot. Use a sufficient number of points for a smooth curve. L = 3 µm, d = 10 µm, Z(n+ layer width) = 10 µm, Rsh = 50 /square. Neglect the metal resistance. 3.17 The TLM test structure in Fig. P3.17 gave the RT values in the graph. The doping density ND in the n+ layer is uniform. (a) Determine the sheet resistance Rsh (ohms/square), the contact resistance Rc (ohms), the specific contact resistance ρc (ohmscm2 ), and the doping density ND (cm−3 ). Z(n+ layer width) = 100 µm, L = 25 µm, t = 2.5 × 10−4 cm, µn = 50 cm2 /V s. (b) Plot a new line for the same parameters as in (i), except ρc = 10−7 ohmscm2 .
181
10−1
10−1
10−3
10−2 I (A)
I (A)
PROBLEMS
10−5 10−7 10−9
10−3 10−4
0
0.1
0.2 V (V)
0.3
10−5 0.1
0.4
0.2
0.3 0.4 V (V)
0.5
0.6
1 × 10−11
C (F)
8 × 10−12 6 × 10−12 4 × 10−12 2 × 10−12 −5
−4
−3 −2 V (V)
−1
0
Fig. P3.15
n+ L d p
Fig. P3.16
1 L
d n+
0.6 0.4 p (NA) 0.2 10 × 10−3
8 × 10−4
6 × 10−4
4 × 10−4
2 × 10−4
0 0 × 100
RT (ohms)
0.8
d (cm)
Fig. P3.17
t
182
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
3.18 A transfer length method test structure is shown in P3.18. The n layer is 1 µm thick with resistivity ρ = 0.001 ohmcm. The specific contact resistivity is ρc = 10−6 ohmcm2 . Calculate and plot RT versus d for d = 2, 4, 6, 10 µm. Z = 20 µm, L = 10 µm. RT = 2Rc + Rs =
Rsh d 2ρc L coth . + LT Z LT Z
n
L d1 L
d2
L
d3
Z
L
d4
L
Fig. P3.18
3.19 In the Kelvin contact resistance test structure in Fig. P3.19, it is usually assumed that the voltmeter has very high input resistance and there is negligible voltage drop along the voltage measurement arm. Now suppose the input resistance Rin of the voltmeter is finite. For I = 10−3 A, Rarm = 100 , and Rc = 10 , determine Rin for a 10% error in Rc . I
I
Rarm
Rin Voltmeter
Fig. P3.19
3.20 (a) All contacts in Fig. P3.20 have identical specific contact resistance ρc . Is the contact resistance Rc of the three top contacts the same? Discuss. L ≫ LT , where LT is the transfer length.
PROBLEMS
I
L
I
I
L
p+
183
L
p+
ntype
ntype
Fig. P3.20
3.21 MOSFETs with different channel lengths, shown in Fig. P3.21, are used to determine the channel length and series resistance RSD . Can such transistors be used to determine the contact resistance Rc and the specific contact resistivity ρc ? Discuss.
n
n
n
n
p
Fig. P3.21
3.22 RT versus d data points of a transfer length method contact resistance measurement are shown in Fig. P3.22 for a uniformlydoped ntype layer on a ptype substrate. The ntype resistivity is ρ, the contact length is L, and the contact width is Z. (a) Indicate on the figure three parameters that can be determined from these data. (b) Draw the data points when the nlayer thickness is increased; all other parameters remain unchanged.
d ntype
RT
ptype d
Fig. P3.22
3.23 RT versus d data points of a transfer length method contact resistance measurement are shown in Fig. P3.23 for a uniformlydoped ntype layer on a ptype substrate. The ntype resistivity is ρ, the contact length is L, and the contact width is Z. (a) Indicate on the figure three parameters that can be determined from these data.
184
CONTACT RESISTANCE AND SCHOTTKY BARRIERS
d ntype
RT
ptype d
Fig. P3.23
(b) Draw the data points when the nlayer resistivity is increased; all other parameters remain unchanged.
REVIEW QUESTIONS • What is the most important parameter to give low contact resistance? • What are the three metalsemiconductor conduction mechanisms? • What is Fermi level pinning?
• What is the specific contact resistivity and what are its units?
• Does the contact chain give detailed contact characterization? Why or why not? • What is the transfer length method?
• Why is the Kelvin contact test structure best?
• What is the effect of lateral current flow on Kelvin contact resistance measurement? • How is the barrier height of Schottky diodes determined? • How can the Richardson constant be measured?
4 SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
4.1
INTRODUCTION
Semiconductor device and circuit performance is generally degraded by series resistance that depends on the series and shunt resistance, on the device, on the current flowing through the device, and on a number of other parameters. The series resistance rs depends on the semiconductor resistivity, on the contact resistance, and sometimes on geometrical factors. Series resistance may be very large before causing device degradation. For example, in a reversebiased photodiode with a photocurrent in the nanoamperes range, series resistance is a minor consideration. However, series resistances of a few ohms are detrimental for solar cells and power devices. The effect of rs on capacitance and carrier concentration profiling measurements is discussed in Chapter 2. The aim of the device designer should be a design in which series resistance is negligibly small for that device. However, since rs cannot be zero, it is important to be able to measure it. The effective channel length and width of a MOSFET are important device parameters because they are required for modeling and they usually differ from the maskdefined and the physical dimensions and the threshold voltage is one of the most important MOSFET parameters. Methods to determine these are discussed.
4.2 4.2.1
PN JUNCTION DIODES CurrentVoltage
The current of a pn junction is often written as a function of the diode voltage Vd as I = Io (eqV d /nkT − 1)
(4.1)
Semiconductor Material and Device Characterization, Third Edition, by Dieter K. Schroder Copyright 2006 John Wiley & Sons, Inc.
185
186
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
rs
I
+
+
Vd
V
−
−
Fig. 4.1
Equivalent circuit of a diode.
where Io is the saturation current and n the diode ideality factor. The diode voltage Vd is the voltage across the spacecharge region and excludes any voltage drops across the p and n quasineutral regions. If both Io and n are constant, then a plot of log(I ) versus Vd yields a straight line for Vd > nkT /q. A semiconductor diode can be represented by the equivalent circuit of Fig. 4.1, consisting of an ideal diode in series with resistance rs . When current flows through the device, the diode terminal voltage V is V = Vd + I R s
(4.2)
With series resistance Eq. (4.1) becomes I = Io (eq(V −I rs )/nkT − 1)
(4.3)
The current in pn junction diodes is due to two components: spacecharge region (scr) recombination/generation and quasineutral region (qnr) recombination/generation, leading to the I –V relationship I = Io,scr (eq(V −I rs )/nkT − 1) + Io,qnr (eq(V −I rs )/nkT − 1)
(4.4)
Equation (4.4) is plotted in Fig. 4.2 for forward bias. There are four distinct regions in the figure. For I rs ≪ V ≪ nkT /q, the current depends linearly on voltage (eqV /nkT − 1 ≈ qV /nkT ), giving a nonlinear curve on the semilog plot. For V ≫ nkT /q, the current is dominated by scr recombination at low current and by qnr recombination at higher current. The breakpoint between the two current components occurs at V = 0.3 V in this example. The I –V curve deviates from linearity at high current due to series resistance rs . Extrapolating the two linear regions to V = 0 gives Io,scr and Io,qnr . The slope is given by d log I (4.5) m= dV Knowing the slope and sample temperature allows the ideality factor to be determined from the relationship q q = (4.6) n= ln(10)mkT 2.3mkT We will generally use the logarithm to base 10, written as “log”, instead of the logarithm to base e, written as “ln”, because experimental data are usually plotted on “log”, not “ln”, scales.
PN JUNCTION DIODES
187
100 ∆V = Irs
Current (A)
10−2 10−4
qnr
10−6
Slope m = q/2.3nkT
10−8
scr Io,scr
10−10
Io,qnr 10−12
Fig. 4.2
0
0.2
0.4 0.6 Voltage (V)
0.8
1
Current versus voltage for a diode with series resistance. Upper dashed line is for rs = 0.
The deviation of the log(I )–V curve from linearity at high currents is V = I rs , allowing rs to be determined according to rs =
V I
(4.7)
Since the Schottky diode currentvoltage behavior is similar to pn junctions, we will use Fig. 3.38 for the rs extraction. Figure 4.3(a) gives that part of the I –V curve where rs is negligible and n = 1.1 from the slope. Figure 4.3(b) shows the part of the rs dominated curve. The deviation from linearity, according to Eq. (4.7), gives rs = 0.8 . The resistance can also be obtained from the diode conductance gd = dI /dV . In the region where rs is important, qnr recombination dominates and the current I ≈ Io,qnr eq(V −Irs )/nkT
(4.8)
gives gd =
qI (1 − rs gd ) nkT
(4.9)
We can write Eq. (4.9) as1 nkT 1 = + I rs gd q
(4.10)
suggesting a plot of I /gd versus I . Such a plot has an I = 0 intercept of nkT /q and slope rs , as shown in Fig. 4.4(a). Equation (4.9) can also be written as q(1 − rs gd ) gd = I nkT
(4.11)
Plotting gd /I versus gd , the gd = 0 intercept is q/nkT , the gd /I = 0 intercept is 1/rs and the slope is qrs /nkT , as shown in Fig. 4.4(b). Careful measurements have revealed the approach of Eq. (4.11) to give the most reliable results,2 although Fig. 4.4 shows the scatter in (b) to be more severe than in (a) because both axes require a differentiation of the data. Comparing Figs. 4.3 and 4.4 for rs extraction brings out an important point. A slope method is generally more accurate than a single point method to determine an
188
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
10−2
Current (A)
10−3
Slope = 15.8
10−4
10−5 10−6
0
0.05
0.1 Voltage (V)
0.15
0.2
(a) 100
Current (A)
10−1
∆V = 0.12 V
I = 0.15 A
10−2 10−3
10−4 0.1
0.2
0.3
0.4
Voltage (V) (b)
Fig. 4.3 Current versus voltage for the diode in Fig. 3.38. (a) low voltage where rs can be neglected, (b) highvoltage where rs dominates.
unknown quantity. Since experimental data exhibit small errors, slope methods allow smoothing of the data, whereas single point measurements incorporate any experimental uncertainties in the parameter determination. The diode conductance can be measured by superimposing a small ac voltage δV on the dc voltage V and measuring the inphase component δI with a lockin amplifier to obtain gd = δI /δV .3 Because of the exponential dependence of current on voltage, δV should be kept as low as possible. Alternately, one can differentiate the I –V curve. Again, because of the exponential nature of the curve, dc voltage steps should be less than 1 mV. Using the semilog plot, where gd = Id [ln (I )]/dV , voltage steps as high as 10 mV are permissible.2 4.2.2
OpenCircuit Voltage Decay (OCVD)
Opencircuit voltage decay is a method to determine the minority carrier lifetime of pn junctions as discussed in Chapter 7 and can also be used to determine the diode series resistance, as illustrated in Fig. 4.5. The diode is forward biased. At t = 0 switch S is opened, and the opencircuit diode voltage is monitored as a function of time. The lifetime
PN JUNCTION DIODES
189
0.15
I/gd (V)
0.1
Slope = rs 0.05 Intercept = nkT/q 0
0
0.05 0.1 Current (A) (a)
0.15
50 Intercept = q/nkT
gd /I (V−1)
40 30 Intercept = 1/rs
20 Slope = qrs/nkT 10 0
0
0.25
0.5 0.75 gd (S)
1
1.25
(b)
Fig. 4.4
(a) I /gd versus I, (b) gd /I versus gd for the device of Fig. 4.3. Voc(t) I
S
V rs Voc(0−) ∆V Voc(0+) Voc(t) 0
Fig. 4.5
t
Opencircuit voltage decay of a pn junction showing the voltage discontinuity at t = 0.
is determined from the slope of the Voc − t curve. The series resistance is obtained from the voltage discontinuity V at t = 0.3 The voltage drop across the diode just before opening the switch Voc (0− ) consists of the diode voltage Vd and the voltage drop across any device resistances Voc (0− ) = Vd + I rs
(4.12)
190
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
When switch S is opened and the current drops to zero, the voltage drops abruptly and Voc (0+ ) = Vd . With the measured voltage drop given by V = Voc (0− ) − Voc (0+ ) = I rs and I measured independently, it is a simple matter to calculate the series resistance rs = V /I . This absolute measure does not rely on slopes or intercepts and is suitable for low rs measurements. Diode series resistances as low as 10 to 20 m have been determined this way. 4.2.3
CapacitanceVoltage (C –V )
We show the effect of series resistance on capacitance in Chapter 2. For the parallel equivalent circuit configuration, the measured capacitance Cm of a junction device is related to the true capacitance C by Cm =
C (1 + rs G)2 + (2πf rs C)2
(4.13)
where G is the conductance and f the frequency. For reasonably good junction devices, the condition rs G ≪ 1 is generally satisfied, and Eq. (4.13) simplifies to Cm ≈
C 1 + (2πf rs C)2
(4.14)
Lowering the frequency reduces the second term in the denominator to less than unity and the true capacitance is determined. Then the frequency is raised until the second term dominates, and rs can be calculated with all other quantities known. This method is only effective when rs ≫ 1/2πf C. It can also be used when dc current techniques are unable to determine the series resistance, e.g., for an MOS capacitor with no dc current flow. 4.3 4.3.1
SCHOTTKY BARRIER DIODES Series Resistance
The currentvoltage characteristic of a Schottky barrier diode without series resistance is discussed in Section 3.5. The thermionic currentvoltage expression of a Schottky barrier diode with series resistance is given by I = Is (eq(V −I rs )/nkT − 1)
(4.15)
where Is is the saturation current Is = AA∗ T 2 e−qφB /kT = Is1 e−qφB /kT
(4.16)
where A is the diode area, A∗ = 4πqk 2 m∗ / h3 = 120 (m∗ /m) A/cm2 K2 is Richardson’s constant4 , φB the effective barrier height, and n the ideality factor. Equation (4.15) is sometimes expressed as (see Appendix 4.1) qV qV 1 − exp − (4.17) I = Is exp nkT kT valid for I rs ≪ V . Data plotted according to Eq. (4.15) are linear only for V ≫ kT /q. When plotting log[I /(1 − exp(−qV /kT ))] versus V , using Eq. (4.17), the data are linear to V = 0.
SCHOTTKY BARRIER DIODES
191
The method of extracting rs , given in Section 4.2.1, can also be used for Schottky diodes. Another method defines the Norde function F as5 kT V I − ln (4.18) F = 2 q Is1 With Eqs. (4.15) and (4.16), Eq. (4.18) becomes I rs 1 1 F = V + − + φB 2 n n
(4.19)
Why is this rather peculiarly defined F function used? When F is plotted against V , it exhibits a minimum which is used to determine rs and φB . To see the dependence of F on V , we consider the low and high voltage limits. At low applied voltages, where I rs ≪ V , Eq. (4.19) gives dF /dV = 1/2 − 1/n ≈ −1/2 for n ≈ 1. At high voltages, where I rs ≫ V , dF /dV = 1/2. Hence, F has a minimum lying between these two limits. The voltage at the minimum is Vmin and the corresponding current is Imin . From dF /dV = 0 at the minimum, the series resistance is rs =
2 − n kT Imin q
The minimum F value, found by substituting Eq. (4.20) into Eq. (4.19), is 1 2 − n kT 1 − + φB Vmin + F = 2 n n q
(4.20)
(4.21)
The series resistance of the Schottky diode is calculated from the ideality factor n and from Imin . The ideality factor is obtained from the slope of the log(I ) versus V plot, and Imin is the current at V = Vmin . For this method, Is1 , and therefore A∗ , must be known. This is a disadvantage of this technique, since A∗ is not necessarily known. In the absence of an experimentally determined A∗ , one must use published values for A∗ . That is not always a good assumption since A∗ depends on the contact preparation, including the surface cleaning procedure6 and sample annealing temperature; it even appears to depend on the metal thickness and on the metal deposition method.7 The original Norde method of plotting F versus V assumes the ideality factor n = 1, and the statistical error is increased by using only a few data points near the minimum of the F versus V curve. A modified Norde increases the accuracy, allowing rs , n, and φB to be extracted from an experimental log(I ) versus V plot.8 Alternately, rs , n, and φB can be determined from the I –V curves at two different temperatures.9 Barrier height measurements in the absence of series resistance are discussed in Section 3.5. The barrier height is commonly calculated from the saturation current Is determined by an extrapolation of the log(I ) versus V curve to V = 0. Series resistance is not important in this extrapolation because the current Is is very low. The barrier height φB is calculated from Is in Eq. (4.16) according to φB =
kT AA∗ T 2 ln q Is
(4.22)
The barrier height so determined is φB at zero bias. The most uncertain of the parameters in Eq. (4.22) is A∗ , rendering this method only as accurate as A∗ is known. Fortunately,
192
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
A∗ appears in the “ln” term. For example, an error of two in A∗ gives rise to an error of 0.69 kT/q in φB . Several variations of the Norde plot have been proposed to overcome its limitations. In one of these, an H function is defined as10 nkT I ln = I rs + nφB (4.23) H =V − q Is1 A plot of H versus I has a slope of rs and an H axis intercept of nφB . Like the F plot, the H plot also requires a knowledge of A∗ . An approach, not requiring a knowledge of A∗ , is the modified Norde plot11 qV I (4.24) − ln F1 = 2kT T2 F 1 is plotted versus V for several different temperatures. Each of these plots exhibits a minimum and each minimum defines an F 1min , a voltage Vmin , and a current Imin . With Eqs. (4.15), (4.16) and (4.20) and V ≫ kT /q, qnφB Imin (4.25) = 2 − n(ln(AA∗ ) + 1) + 2F 1min + (2 − n) ln 2 T kT When the left side of Eq. (4.25) is plotted against q/kT , a straight line results with slope nφB and yaxis intercept {2 − n[ln(AA∗ ) + 1]}. With n independently determined, it is possible to extract both φB and A∗ , provided the area A is known. The function F (V ) = V − Va ln(I ) (4.26) was also used to determine, Is , and rs . One determines the minimum of F (V ) for different Va , where Va is an independent voltage.12 Using Eq. (4.26), but with the current I as the dependent variable, and finding the minimum is the basis of yet another method.13 Methods with different assumed functions but requiring solutions to simultaneous equations have also been proposed.14 Occasionally it is impossible to extract barrier height and series resistance from I –V measurements using the thermionic emission equation. It may then be necessary to include spacecharge region recombination and tunnel currents.15 When the barrier height is voltage dependent, the extraction of device parameters saturation current, barrier height, diode ideality factor, and series resistance becomes more difficult. One solution to this problem is provided in ref. 16.
4.4
SOLAR CELLS
Solar cells are particularly prone to series resistance, because it reduces the maximum available power. The series resistance should be approximately rs < (0.8/X) for 1 cm2 area cells, where X is the solar concentration.17 Here X = 1 for nonconcentrator cells, whereas for concentrator cells X can be several hundred. For X = 100, rs < 8 × 10−3 . Under “onesun” conditions 10–20% of the maximum power available from a solar cell can be lost due to a series resistance of 1 . Although solar cells are pn junction diodes, their I –V characteristics are often not suitable for the types of measurements of conventional diodes. Since the operation of solar cells in the presence of sunlight
SOLAR CELLS
193
rs I + Iph
rsh
V
RL
−
Fig. 4.6
Solar cell equivalent circuit.
may alter the series resistance, rs should be determined under operating conditions. Shunt resistance is also important for solar cells. Several methods have been used to determine rs . They are generally neither simple to implement nor to interpret. A solar cell, represented by the equivalent circuit of Fig. 4.6, consists of a photon or lightinduced current generator Iph , a diode, a series resistor rs , and a shunt resistor rsh . The part of the circuit to the left of the two points is the cell and the part to the right is the load, characterized by the load resistor RL . Frequently rs and rsh are assumed to be constant, but they may depend on the cell current. The current I flows through the load resistor and develops a voltage V across it. The current is given by V + I rs q(V + I rs ) −1 − I = Iph − Io exp nkT rsh
(4.27)
This equation does not take into account that both Io , and n are not constant over the entire I –V curve. At low voltage, spacecharge region (scr) recombination generally dominates, but at higher voltage quasineutral region (qnr) recombination is dominant. Equation (4.27) is used for most solar cell analyses in spite of its simplifications, although scr and qnr recombination are occasionally considered separately. The currentvoltage characteristic is measured with conventional I –V techniques or with the quasisteadystate (Qss ) photoconductance technique, where a flash lamp produces slowly varying illumination and the resulting time dependence of the excess photoconductance of the sample is measured.18 The Qss approach can measure the opencircuit voltage of solar cells as a function of the incident light intensity. Monotonically varying illumination produces a voltage versus illumination curve in a fraction of a second. This quasisteadystate opencircuit voltage method has important advantages over the classic Isc − Voc technique to measure the characteristics of the solar cell free from series resistance effects. An example light intensityopen circuit voltage curve is shown in Fig. 4.7. Care should be exercised when using this technique on high sheet resistance cells, e.g., amorphous solar cells, due to shadows cast by the probe needle, for example.19 Such shadowing distorts the experimental data. A currentvoltage curve of a solar cell is shown in Fig. 4.8. The opencircuit voltage Voc , the shortcircuit current Isc , and the maximum power point Vmax and Imax are also shown. The quantities rso and rsho are the resistances defined by the slopes of the I –V curve at I = 0 and at V = 0, respectively. The effects of series and shunt resistances are shown on the I –V characteristics in Fig. 4.9 calculated from Eq. (4.27). Series resistances of a few ohms or less degrade the device performance, as do shunt resistances of several hundred ohms. Small I –V degradation has a significant effect on cell efficiency. The maximum power points are shown by the points on Fig. 4.8 and 4.9.
194
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
Illumination Intensity (Suns)
102 101 100 10−1 10−2 10−3 0.4
Fig. 4.7
0.5 0.6 0.7 Open Circuit Voltage (V)
0.8
Light intensity versus open circuit voltage. After ref. 18.
Isc
rsho = −(dV/dI) @ V = 0
Imax rso = −(dV/dI) @I = 0
Current
Max. Power Point
VmaxVoc Voltage
Fig. 4.8
Currentvoltage characteristic of a solar cell.
60 (a) Current (mA)
(b) 40
20
0
0
0.2
0.4
0.6
0.8
Voltage (V)
Fig. 4.9 Currentvoltage curve of a solar cell with Iph = 55 mA, Io = 10−13 A, n = 1, T = 300 K. The series and shunt resistances are: (a) rs = 0, rsh = ∞, (b) rs = 0.5 , rsh = 500 .
SOLAR CELLS
4.4.1
195
Series Resistance—Multiple Light Intensities
An early method to determine rs is based on the measurement of the I –V curves at two different light intensities giving the shortcircuit currents Isc1 and Isc2 , respectively. A current δI below Isc , I = Isc − δI , is picked on both I –V curves. The currents I1 = Isc1 − δI and I2 = Isc2 − δI correspond to voltages V1 and V2 . The series resistance is then20 V1 − V2 V1 − V2 = (4.28) rs = I2 − I1 Isc2 − Isc1 By using more than two light intensities more than two points are generated. Drawing a line through all of the points gives the series resistance by the slope of this line, I /V , as V (4.29) rs = I The method is illustrated in Fig. 4.10. The slope method lends itself to rs determination at any current with no limiting approximations and is generally considered to give good results. It is also independent of Io , n, and rsh , provided they do not change with the operating point. This is an important consideration. Those techniques that require a knowledge of Io , n, and rsh , and even Iph in some cases, are at a disadvantage because these parameters may not be accurately known. It is important that the temperature of the cell be constant during the measurements at different light intensities, as temperature variations can alter the series resistance. Comparison of experimental I –V curves with a theoretical curves (rs = 0) has also been used to determine rs . The shift of the maximum power point from its theoretical value, Vmax = Vmax (theory) − Vmax (exp), is given by22 rs =
Vmax Imax
(4.30)
A weakness of this method is the assumption that parameters like Io and n are known. If unknown, they must be determined by other means, for they are required to calculate the theoretical I –V curve. 0.08 δI
Current (A)
0.06
0.04
0.02 rs = ∆V/∆I = 0.5 Ω 0
0
0.2
0.4
0.6
0.8
Voltage (V)
Fig. 4.10
Series resistance determination of a solar cell.
196
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
Under shortcircuit conditions, where I = Isc and V = 0, Eq. (4.27) becomes qIsc rs Iph − Isc (4.31) = ln Io nkT A plot of ln[(Iph − Isc )/Io ] versus Isc has a slope of qrs /nkT .23 The series resistance is calculated from the slope, provided n and Iph are known. Another method relies on a dark I –V curve, the opencircuit voltage, and the shortcircuit current. From Eq. (4.27) with rsh very large, the dark voltage is Vdk =
nkT Idk ln − Idk rs q Io
(4.32)
The opencircuit voltage is given by Voc =
Iph nkT ln q Io
(4.33)
Voc is independent of rs since there is no current during an open circuit voltage measurement. Hence, by comparing Voc with Vdk at a given current Idk , it is possible to determine rs at that current. To reduce any error, one should choose that point on the Idk − Vdk curve where the diode parameters are the same as those of the opencircuit condition.24 That corresponds to Idk = Iph and since generally Iph ≈ Isc , rs ≈
Vdk (Isc ) − Voc Isc
(4.34)
Idk = Isc ensures that the upper limit of the series resistance for a given light intensity is obtained.24 4.4.2
Series Resistance—Constant Light Intensity
The series resistance can be determined by the area under the I –V curve,25 given by the power P1 , Isc P1 = V (I ) dI (4.35) 0
The series resistance, obtained from Eqs. (4.27) and (4.35), is25 P1 nkT Voc rs = 2 − 2 − Isc Isc qIsc
(4.36)
This method has been used to measure the very low resistances of concentrator solar cells of rs = 5 to 6 × 10−3 . Such cells, because they are operated under solar concentrations with high photocurrents, are particularly prone to series resistance degradation. Series resistances determined by the “area” method have been compared to values determined by the “slope” methods. Such comparisons have shown the “area” method to overestimate rs at “onesun” and lower illuminations,26 because n must be known accurately in Eq. (4.36) and rsh may not be negligible. The results of the two methods at high illumination are in reasonably good agreement.
SOLAR CELLS
197
Various analytical techniques have also been used to determine rs . Some are based on complete curve fitting of the solar equation to experimental I –V curves. Others use several points on the experimental I –V curve to determine the key parameters. In the five point method the parameters Iph , Io , n, rs , and rsh are calculated from the experimental Voc , Isc , Vm , Im , rso , and rsho shown in Fig. 4.8.27 Later simplifications in the equations make the analysis more tractable.28 A comparison of the five parameters determined by the exact five point, by the approximate five point, and by numerical techniques gave very good agreement for Iph , Io , and n. The main differences were found for rs and rsh at low light intensities. In the three point method , Iph , Io , n, rs , and rsh are determined from the opencircuit voltage, the short circuit current, and the maximum power point. Both fivepoint and threepoint methods give comparable results.29 – 30 Because scr and qnr recombination take place in a solar cell, parameters describing both of these processes should be determined for complete solar cell modeling. Applying small current steps to a solar cell in both the forward and reverse current directions and measuring the resulting voltage, allows Io (scr), Io (qnr), n(scr), n(qnr), rs , and rsh to be determined.31 A technique especially suitable for concentrator solar cells with low series resistances is based on high intensity flash illumination.32 Neglecting the shunt resistance in the circuit in Fig. 4.6, for very high light intensities the output current I approaches but cannot exceed Voc /(RL + rs ). In order to keep the cell temperature as constant as possible during the measurement, it is best to flash the illumination. Approximating the voltage by Voc ≈ I (RL + rs ) and varying the load resistance at constant light intensity rs ≈
I2 RL2 − I1 RL1 I1 − I2
(4.37)
where I1 and I2 are the currents for load resistances RL1 and RL2 . Series resistances as low as 7 to 9 m have been determined with this method for GaAs concentrator solar cells at light intensities approaching 9000 suns with 1 ms light pulses.32 The value of the load resistance should be on the order of the series resistance. 4.4.3
Shunt Resistance
The shunt resistance rsh can be determined by some of the curvefitting approaches discussed in the previous section, or it can be determined independently. It is sometimes found from the slope of the reversebiased currentvoltage characteristic before breakdown. Most solar cells, however, exhibit large reverse currents at voltages well below breakdown because solar cells are not designed to operate under high reverse voltages. This makes it difficult to obtain reasonable value for rsh by this method. Furthermore, a solar cell in the dark under reverse bias is a poor representation of a solar cell operating in the light under forward bias. An alternate method is to rewrite Eq. (4.27) in terms of Voc and Isc as rs Voc qIsc rs qV oc − − exp (4.38) Isc 1 + = Io exp rsh rsh nkT nkT This equation can be simplified for the usual condition of rs ≪ rsh . If the measurement is made under low light intensities where Isc rs ≪ nkT /q, then Eq. (4.38) becomes Voc qV oc −1 = (4.39) Isc − Io exp nkT rsh
198
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
This approximation is valid for Isc ≤ 3 mA for series resistances on the order of 0.1 . When measurements of rsh were made under these conditions, rsh was found to be highly sensitive to Io and n, that may not be known accurately.33 This problem was alleviated by making the measurements at very low light intensities, allowing the second term on the left side of Eq. (4.39) to be neglected and then Isc ≈
Voc rsh
(4.40)
The Isc − Voc plot has a linear region of slope 1/rsh . The curve becomes nonlinear at higher light intensities, and the method becomes invalid. Measurements showed that for Isc in the 0 to 200 µA and Voc in the 0 to 50 mV range, the shunt resistances were 65 to 1170 .33 Example Jsc − Voc plots are shown in Fig. 4.11. 4.5
BIPOLAR JUNCTION TRANSISTORS
An integratedcircuit bipolar junction transistor (BJT) with parasitic series resistances is shown in Fig. 4.12. The n+ emitter and the pbase are formed in an ncollector layer on a psubstrate. The transistor is decoupled from adjacent transistors by oxide isolation regions not shown. The parasitic resistances and their measurement are relevant for our purpose. The emitter resistance RE is primarily determined by the emitter contact resistance. The base resistance RB is composed of the intrinsic base resistance RBi , under the emitter, and the extrinsic base resistance RBx , from the emitter to the base contact including the base contact resistance. The collector resistance RC is comprised of two components: RC1 and RC2 . The resistances are generally functions of the device operating point. A common method to display the base and collector current is a semilog plot of the logarithm of the current plotted against the emitterbase voltage, shown in Fig. 4.13 and known as a Gummel plot.34 The two currents are expressed as a function of the baseemitter voltage VBE by q(VBE − IB RB − IE RE (4.41) IB = IB0 exp nkT
Short Circuit Current Density (A/cm2)
4 × 10−4
3 × 10−4
2 × 10−4
1 × 10−4
0 × 100 0
Fig. 4.11 ref. 21.
30 ohmcm2 370 ohmcm2
0.03 0.01 0.02 Open Circuit Voltage (V)
0.04
Short circuit current density versus open circuit voltage for two solar cells. Adapted from
BIPOLAR JUNCTION TRANSISTORS
B1 IB
IB
IE
PolySi
C
B2
E
n+
199
IC
p+ PolySi n+ PolySi
p+
p+ n−
n+
n+ RC1
p RC2
n+ p Substrate
B2
E
n+
Re RBx
p RBi n−
Fig. 4.12
An npn bipolar junction transistor and its parasitic resistances. 100
∆VBE
10−2
Current (A)
n=1 10−4
n=1 IC IB
10−6
n = 1.52
10−8
ICB0 10−10
0
0.2 0.4 0.6 BaseEmitter Voltage (V)
0.8
Fig. 4.13 Gummel plots showing the effects of emitterbase spacecharge region recombination (n ≈ 1.5–2), quasineutral region recombination (n ≈ 1), and series resistance.
200
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
q(VBE − IB RB − IE RE IC = IC0 exp kT
(4.42)
IB0 depends on whether the dominant recombination mechanism is spacecharge region (scr) or quasineutral region recombination. The collector current Gummel plot is linear with slope of q/ ln(10)kT over most of its range. It saturates at the collectorbase junction leakage current ICB0 at low voltages and deviates from linearity at high voltages due to series resistances. For simplicity, additional deviations from linearity at high voltages due to highlevel injection are not shown. The base current generally exhibits two linear regions. At low voltages the current is dominated by emitterbase spacecharge region recombination with a slope of q/ ln(10)nkT , where n ≈ 1.5 to 2. At intermediate voltages the slope is q/ ln(10)kT just as it is for the collector current due to quasineutral region recombination, and at higher voltages the curve deviates from linearity due to series resistances. Highlevel injection effects are again not shown, for clarity. The external voltage drop between the base and the emitter terminals VBE is ′ ′ VBE = VBE + IB RB + IE RE = VBE + (RB + (β + 1)RE )IB
(4.43)
and the voltage drop across the parasitic resistances is VBE = IB RB + IE RE = (RB + (β + 1)RE )IB
(4.44)
where β is the common emitter current gain, IC = βIB , IE = IC + IB = (β + 1)IB , and VBE is the potential drop across the baseemitter junction. Although RE is generally small, the (β + 1) multiplier can make (β + 1)RE appreciable. The emitter and base resistances depress the currents below their ideal values, shown by the curves below the extrapolated dashed lines in Fig. 4.13. BJT resistance measurement techniques fall into two main categories: dc methods and ac methods. The dc methods are generally fast and easy to implement and can be further subdivided into methods relying on determining the series resistance from I –V curves or from open circuit voltage measurements. The ac techniques require measurement frequencies of typically 50 MHz to several GHz, necessitating a careful consideration of device and measurement circuit parasitics and of the distributed nature of BJT parameters. 4.5.1
Emitter Resistance
The emitter resistance in discrete BJTs is around 1 and for smallarea IC transistors it is around 5 to 100 . One method to determine RE is based on a measure of the collectoremitter voltage VCE 35 – 36 kT IB + IC (1 − αR ) ln + RE (IB + IC ) + RC IC VCE = (4.45) q αR (IB − IC (1 − αR )/αF neglecting the small reverse saturation current. Here αF = βF /(1 + βF ) and αR = βR / (1 + βR ) are the largesignal forward and reverse common base current gains. With the collector open circuited, IC = 0 and Eq. (4.45) becomes kT kT 1 1 + βR ln ln + RE IB = + R E IB (4.46) VCE = q αR q βR
BIPOLAR JUNCTION TRANSISTORS
201
RB VCE IB
IB Slope = 1/RE
RE
VCE
Fig. 4.14
Emitter resistance measurement setup and IB − VCE plot.
A plot of IB versus VCE and the measurement setup are shown in Fig. 4.14. The curve is linear with a VCE axis intercept of (kT /q) ln(1/αR ) and a slope of 1/RE . This behavior is indeed observed for discrete transistors.36 – 37 The base current should not be too small for unambiguous measurements. For example, base currents around 10 mA are suitable for RE ≈ 1 , and it is important to ensure that zero or very low collector currents are drawn during the measurement. A suitable connection is: BJT base connected to the collector terminal, BJT emitter connected to the emitter terminal, and BJT collector connected to the base terminal of the curve tracer.38 Departures of the IB − VCE curve from linearity occur when αR is current dependent. This generally happens at low and high currents. Hence an RE determination may not yield one unique value. The slope of the curve increases at high base currents.38 – 39 Intermediate base currents usually give good linearity. Additional complications can arise for integrated circuit transistors where part of the buried layer resistance can add to the emitter resistance due to internally circulating currents even for zero external collector current. The accuracy of this method is also dependent on the sensitivity of the base charge with respect to base current.40 A method to improve the original open collector measurement, requiring a measurement of forward/reverse current gains and the intrinsic base sheet resistance, allows the IB − VCE plot to be linearized, making the unambiguous extraction of RE easier.41 A different approach uses two base contacts in Fig. 4.12, by biasing the device in the forward active region with base current supplied through base contact B1 and no current flowing through contact B2 . The baseemitter voltage VBE 2 is VBE 2 = VBE 0 + RE IE
(4.47)
where VBE 0 is the baseemitter voltage at the edge closest to B2 .42 The emitter resistance is RE =
VBE 2 − VBEeff IE
(4.48)
where VBEeff is determined from the base current expression42 IB1 =
IC0 β
exp
qV BEeff nkT
−1
(4.49)
The same method can also be used for base resistance extraction.42 Yet another method uses the null in thirdorder intermodulation as a function of emitter current in a bipolar transistor to find the emitter resistance and the thermal resistance.43
202
4.5.2
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
Collector Resistance
A problem with collector resistance measurements is the strong dependence of collector resistance on the device operating point. The collector resistance can be determined by the same IB − VCE method of Section 4.5.1 by interchanging the collector and emitter terminals. With E → C and C → E, the IB − VCE curve has a VCE axis intercept of (kT /q) ln(1/αF ) and a slope of 1/RC . Another method uses the parasitic substrate pnp transistor that exists in the structure of Fig. 4.12 and the reverse transistors associated with the npn transistor to determine the internal voltages of the npn BJT, allowing RC to be determined.44 Another method uses the transistor output characteristics. Typical output IC − VCE curves are shown in Fig. 4.15. The two dashed lines 1/RCnorm and 1/RCsat represent the two limiting values of RC . The 1/RCnorm line is drawn through the knee of each curve, where the output curves tend to horizontal. The collector resistance obtains for the device in its normal, active mode of operation. The 1/RCsat line gives the appropriate collector resistance for the transistor in saturation. A good discussion of this measurement technique using a curve tracer is given in Getreu.38 The collector resistance can also be determined by measuring the substrate current of the parasitic pnp vertical transistor linked with the npn transistor.45 The pnp device is operated with either the bottom substratecollector or the top basecollector pn junction forward biased, allowing the separation of the various RC components. 4.5.3
Base Resistance
The base resistance is difficult to determine accurately because it depends on the device operating point and because its measurement is influenced by the emitter resistance through the term (β + 1)RE . The base current flows laterally in BJTs, giving lateral voltage drops in the base, causing VBE to be a function of position. Small VBE variations give rise to large current variations since IC and IB depend exponentially on VBE . Most of the emitter current flows at the emitter edge nearest the base contact, referred to as emitter crowding, reducing the distance for base current flow with increased emitter current, thereby decreasing RBi with current.
Slope = 1/RCsat Slope = 1/RCnorm
Saturation IC
VCE
Fig. 4.15
Common emitter output characteristics. The two lines show the limiting values of RC .
BIPOLAR JUNCTION TRANSISTORS
203
A simple method to determine the total series resistance between emitter and base is shown in Fig. 4.13. The experimental base current deviates from the extrapolated straight line by the voltage drop (4.50) VBE = (RB + (β + 1)RE )IB A plot of VBE /IB versus β has a slope of RE and an intercept on the VBE /IB axis of RB + RE . To vary the current gain β one chooses a device with varying β over some operating range, or use different devices from the same lot. The first method ensures that only one device is measured, but conductivity modulation and other secondorder effects may distort the measurement since the current must be changed to vary β. In order to avoid conductivity modulation and other secondorder effects, one should make the measurement at a constant emitter current. But, of course, a constant IE implies constant β. In that case one must use different devices from the same lot whose βs vary over some appropriate range, assuming the resistances to be the same for all devices from that lot.46 A variation on this method is based on rewriting Eqs. (4.41) and (4.42) as39 RE + RBx RBi nkT IB1 ln + = RE + qIC IB β β
(4.51)
where RB = RBi + RBx and IB1 = IB0 exp(qV BE /nkT ). Then RBi /β is constant if RBi is proportional to β.47 The requirement of RBi ∼ β at all IE is a weakness in this method; it may not always be satisfied. A plot of (kT /qIC ) ln(IB1 /IB ) versus 1/β, for n = 1, has a slope of RE + RBx and an intercept on the (kT /qIC ) ln(IB1 /IB )axis of RE + RBi /β, as shown in Fig. 4.16. The intrinsic base resistance must be calculated in this technique. For a rectangular emitter of width WE and length LE with a base contact on one side RBi = WR shi /3L, where Rshi is the intrinsic base sheet resistance. For a rectangular emitter with two base contacts, RBi = WR shi /12L. For square emitters with contacts on all sides, RBi = Rshi /32, and for circular emitters with a base contact all around RBi = Rshi /8π.39 The method based on Eq. (4.51) does not take into account lateral voltage drops along the intrinsic base current path. This condition is satisfied for collector currents of less than 10
(nkT/qIC)ln(IB1/IB) (Ω)
12
Slope = RE + RBx 11 Intercept = RE + RBi/β
10
0
0.005
0.01
0.015
0.02
0.025
β−1
Fig. 4.16 Measured device characteristics according to Eq. (4.51) for a selfaligned, highspeed digital BJT. Reprinted after Ning and Tang39 by permission of IEEE ( 1984, IEEE).
204
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
B1
B2
E VB1E
IB
VB2E IE
RBx
RBi
Fig. 4.17
RBx
RE
RBi
Equivalent emitterbase portion of the “twobase contact” BJT.
to 20 mA for scaled digital BJTs.39 Current crowding makes the results unreliable, unless such crowding is insignificant, e.g., in very narrow emitter transistors. The method of Eq. (4.51) must be used with caution for polysilicon emitter contacts when a thin insulating barrier exists between the polysilicon and the single crystal emitter. This can cause the (kT /qIC ) ln(IB1 /IB ) versus 1/β curve to be nonlinear for low 1/β values. The slope of this plot can even become negative. This behavior cannot be explained by a resistive drop, but is attributable to an interfacial layer between the polysilicon contact and the single crystal emitter.48 A quite different approach makes use of the BJT in Fig. 4.12 with two independent base contacts, B1 and B2 . The BJT emitterbase junction is forward biased using base contact B1 . The voltage is measured between B1 and the emitter, VB1E , and between B2 and the emitter, VB2E . For the equivalent circuit of Fig. 4.17, base current flows from B1 only. For the Kelvin voltage measurement of VB2E , almost no current flows through the right half of the base. The resulting voltages are
and
VB1E = (RBx + RBi )IB + RE IE ; VB2E = RE IE
(4.52)
VBE VB1E − VB2E = = RBx + RBi IB IB
(4.53)
To separate the base resistance into its components, RB can be written as RB = RBx + RBi = RBx +
Rshi (WE − 2d) 3LE
(4.54)
where WE and LE are the emitter window width and length, and d describes the deviation between the emitter window and the effective internal base region.49 The second term on the right side of Eq. (4.54) is discussed earlier with respect to Eq. (4.51). Both RBx and RBi can be determined by measuring RB as a function of WE for transistors with identical LE but varying WE . Such a plot is shown in Fig. 4.18. The sheet resistance Rshi is varied by changing the baseemitter bias voltage, due to base conductivity modulation. VBE , however, should not be too high or excessive current crowding will result, but it should be sufficiently high to avoid uncertainties in the potential measurement. The intersection point gives RBx and 2d. A further refinement of this Kelvin method is given in ref. 50, where more detailed modeling further elucidates the various resistive components.
BIPOLAR JUNCTION TRANSISTORS
205
250 0.92 V
RB (Ω)
200
VBE = 0.9 V
150
0.96 V
100
1.02 V
2d
50 0
RBx 0
1
2 WE (µm)
VBC = 0 3
4
Fig. 4.18 Measured base resistance versus emitter window width as a function of baseemitter voltage. Reprinted after Weng et al.49 by permission of IEEE ( 1992, IEEE).
Several techniques to measure RB are based on frequency measurements. In the input impedance circle method, the emitterbase input impedance is measured as a function of frequency and is plotted on the complex impedance plane for zero ac collector voltage.51 The locus of this plot is a semicircle whose real axis intersections at low and high frequencies are Rin,lf = Rπ + RB + (1 + β)RE ; Rin,hf = Rπ + RB
(4.55)
Resistance Rπ can be calculated from the relationships Rπ = β/gm with gm = qIC /nkT . This method allows both RB and RE to be determined. The effect of Rπ on the measurement of RB can be reduced by measuring at low temperatures, where Rπ is reduced according to the relationships Rπ = nkT β/qIC .52 The semicircle is sometimes distorted due to parasitic capacitances making the interpretation more difficult. Furthermore, the measurement is very timeconsuming and loses accuracy at low collector current when the circle diameter is large. The method is more accurate for RB > 40 and I ≥ 1 mA.53 A variation of this technique is the phase cancellation method in which a common base transistor is connected to an impedance bridge, and the input impedance is measured as a function of collector current at a constant frequency of a few MHz. The collector current is varied until the input capacitance becomes zero, and the input impedance is purely resistive at collector current IC1 . The input impedance is Zi = RB + RE and the base resistance is given by51 nkT RB = (4.56) qIC1 The phase cancellation method does not lend itself to BJTs with β < 10 commonly found in lateral pnp transistors, and the base resistance in this method obtains for one value of collector current only. However, the method is fast and relatively unaffected by the emitter resistance, since RE appears in the input impedance as RE directly, not as (β + 1)RE .
206
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
In another method the frequency response of β(f ) and yf b (f ), the forward transfer admittance of the BJT in the common base configuration, are measured. The base resistance is54 β(0)fβ (4.57) RB = yf b (0)fy where β(0) is the low frequency β, yf b (0) the low frequency yf b , fβ the 3 dB frequency of β, and fy the 3 dB frequency of yf b . The 3 dB frequency is the frequency at which the respective quantity has decreased to 0.7 of its low frequency value. The advantage of this technique is that Eq. (4.57) is relatively unaffected by collector and emitter resistances and that the measurement of yf b is relatively insensitive to stray capacitance. However, it does require measurements of β and yf b over a wide frequency range. In a variation on one of the ac methods, the input impedance of common emitter BJTs is measured at 10 to 50 MHz and RBi , RBx , and RE are extracted from the measurement.55 The method is suitable for low baseemitter voltages with negligible high current effects. A further variation using a single frequency but varying the emitterbase voltage allows not only the base and emitter resistances but also the baseemitter and the basecollector capacitances to be determined.56 The base resistance can also be determined from a pulse measurement similar to the method shown in Fig. 4.5. The base current of a common emitter BJT is pulsed to zero, and the resulting VBE is determined.57 The base resistance is determined from the sudden drop of the emitterbase voltage VBE = RB IB . A cautionary note: extraction of resistances using methods involving kT /q will be in error if self heating causes temperature variations in the device, even with temperaturecontrolled probe stations.
4.6 4.6.1
MOSFETS Series Resistance and Channel Length–CurrentVoltage
The MOSFET source/drain series resistance and the effective channel length or width are frequently determined with one measurement technique. The resistance between source and drain consists of source resistance, channel resistance, drain resistance, and contact resistances. The source resistance RS and drain resistance RD are shown in Fig. 4.19. They are due to the source and drain contact resistance, the sheet resistance of the source and drain, the spreading resistance at the transition from the source diffusion to the channel, and any additional “wire” resistance. The channel resistance is contained in the MOSFET symbol and is not explicitly shown. Current crowding in the source in the vicinity of the channel gives rise to the spreading resistance Rsp . A firstorder expression for Rsp for a source of constant resistivity is given by ξ xj 0.64ρ ln (4.58) Rsp = W xch where W is the channel width, ρ the source resistivity, xj the junction depth, xch the channel thickness, and ξ is a factor that has been given as 0.37,58 0.58,59 , 0.75,60 and 0.9.61 Its exact value is not that important since it appears in the “ln” term. More realistic expressions for Rsp have been derived for junctions with nonuniform dopant profiles.58 The effective channel length differs from the maskdefined gate length and even from the physical device gate length due to source and drain junction encroachment under the
MOSFETs
207
G VGS
V ′GS RS
ID
RD
D
S V′DS V′BS
VDS
VBS B (a)
L
n+
n+
p dL ∆L = 2dL
dL
(b)
Fig. 4.19 (a) A MOSFET with source and drain resistances, (b) device cross section showing the actual gate length L and Leff = L − L with L = 2δL. The substrate resistance is not shown. Lm
L
n+
Lmet p
n+
Leff
Fig. 4.20 Various MOSFET gate lengths: mask length, physical gate length, metallurgical, and effective channel lengths.
gate, as shown in Fig. 4.20, where Lm is the maskdefined gate length, L the physical gate length, Lmet the metallurgical channel length (distance between source and drain), and Leff the effective channel length. The effective or electrical channel length is often thought to be the distance between source and drain, i.e., Leff = Lmet . That is not always
208
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
the case. For highly doped source and drain with steep doping density gradients, the effective length is approximately equal to the physical length between source and drain. However, for lightlydoped drain (LDD) structures, the effective length can be larger than the source/drain spacing, because the channel can extend into the lightlydoped source and drain, especially for high gate voltages. Leff can be thought of as that channel length that gives good agreement between theory and experiment when it is substituted into appropriate model equations. Neglecting the body effect of the ionized bulk charge in the MOSFET spacecharge region, the MOSFET currentvoltage equation, valid for low drain voltage, is ′ ′ ′ − VT − 0.5VDS )VDS ID = k(VGS
(4.59)
where k = Weff µeff Cox /Leff , Weff = W − W , Leff = L − L, VT is the threshold volt′ ′ and VDS are defined in Fig. 4.19(a), W is the gate width, L the gate length, Cox age, VGS the oxide capacitance/unit area, and µeff the effective mobility. W and L usually refer to the mask dimensions. ′ ′ + ID RS and VDS = VDS + ID (RS + RD ), Eq. (4.59) becomes With VGS = VGS ID = k(VGS − VT − 0.5VDS )(VDS − ID RSD )
(4.60)
if RS = RD = RSD /2, where RSD = RS + RD . For these measurements the drain voltage is usually low (VDS ≈ 50–100 mV) ensuring device operation in the linear region. For the device in strong inversion, with (VGS − VT ) ≫ 0.5VDS , Eq. (4.60) becomes ID = k(VGS − VT )(VDS − ID RSD )
(4.61)
Weff µeff Cox (VGS − VT )VDS (L − L) + Weff µeff Cox (VGS − VT )RSD
(4.62)
which can be written as
ID =
Equation (4.62) is the basis for most techniques to determine RSD , µeff , Leff , and Weff . We will discuss the most relevant methods here. The techniques usually require at least two devices of different channel lengths. Comparisons of the various techniques are given by Ng and Brews62 , McAndrew and Layman63 , and Taur.64 We should make a comment here regarding the threshold voltage VT which is used in many of the following techniques. As shown later in Section 4.8, one method to determine VT is the linear extrapolation method. In this technique, VT = VGSi − VDS /2, but the VDS /2 term is neglected in Eq. (4.62), leading to some error. An early method is due to Terada and Muta,65 and Chern et al.,66 with Rm = VDS /ID Rm = Rch + RSD =
L − L + RSD Weff µeff Cox (VGS − VT )
(4.63)
where Rch is the channel resistance, i.e., the intrinsic resistance of the MOSFET. Equation (4.63) gives Rm = RSD for L = L. A plot of Rm versus L for devices with differing L and for varying gate voltages in Fig. 4.21, has lines intersecting at one point giving both RSD and L. Which gate lengths should be used in these plots? Should it
MOSFETs
209
1000 VGS = 3 V
Rm (Ω)
750
4V
5V
500
∆L
250
RSD 0
0
2
4
6
8
10
L (µm)
Fig. 4.21
Rm versus L as a function of gate voltage.
be the maskdefined gate lengths or the physical gate lengths? It does not matter. These methods give a L such that Leff will be the correct value, regardless which L is used. If the Rm versus L lines fail to intersect at a common point, one can carry this technique one step further by writing Eq. (4.63) as Rm = RSD + ALeff = (RSD − AL) + AL = B + AL
(4.64)
The parameters A and B are determined from slope and intercept of Rm versus L plots for different gate voltages. L and RSD are obtained from the slope and intercept, respectively, of a B versus A plot.67 A and B depend implicitly on (VGS − VT ) and they can be fitted for various gate voltages with a least squares technique. Such a linear regression can be used to extract both RSD and L, with no requirement for a common intersection point.68 It is, however, assumed that both L and RSD and are only weakly VGS dependent, required for a linear equation. Since neither L nor RSD are fully gate voltage independent, the linear regression will give only approximate results. The difference between L and Leff is particularly important for shortchannel devices. But shortchannel devices also have a channel lengthdependent threshold voltages, so that each threshold voltage must be determined independently. Furthermore, both the series resistance and the effective channel length may be gate voltage dependent.69 The effective channel length increases and the series resistance decreases with increasing gate voltage, due to channel broadening in which Leff is modulated by the gate voltage. The effective channel is considered to lie between the transitional points where the current flows from the lateral spread of the source and the drain diffusion to the inversion layer. The end of the channel is where the conductivity of the diffusion resistance is approximately equal to the incremental inversion layer conductivity. Since the inversion layer conductivity increases with gate voltage, it follows that Leff increases and the series resistance decreases with increasing gate voltage. The dependence of Leff and RSD on gate voltage is particularly acute for LDD devices, containing lightlydoped regions between the source and the channel and between the drain and the channel.70 The effect of gate voltagedependent Leff and RSD is one reason for the failure of the Rm versus L lines of Fig. 4.21 to intersect at a common point. As a result no unique value of these two parameters can be obtained. A suggested method to
210
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
ensure that the lines intersect at one point is to vary VT in Eq. (4.63) instead of varying VGS .71 This is most conveniently done by varying the substrate bias VBS , maintaining the gate voltage constant at VGS ≈ 1 to 2 V. Another approach is to confine the gate voltages to small variations from each other. For example, instead of varying VGS by 1 V as in Fig. 4.21, one might vary VGS by 0.1 V. This brings the several intersection points close to one common point. For LDD devices, RSD and Leff also depend on drain voltage, because the drain spacecharge region width varies with VDS .72 This is usually considered to be a minor effect and is frequently neglected. The substrate bias technique has yielded unreliable data because substrate bias changes the threshold voltage of MOSFETs of different channel lengths by different amounts. A more serious error is introduced by assuming dLeff /dVBS = 0. It has been shown that Leff is reduced by VBS and is no longer clearly defined.62 An improved method is a combination substrate/gate bias technique.73 The gate voltage of the longest channel device is held constant while its threshold voltage is changed by substrate bias modulation. When measuring the resistance of shorterchannel devices, the gate voltage is reduced by the amount the threshold voltage has decreased from the longchannel value, ensuring constant gate drive for all devices. Yet another variation on the Rm versus L method uses a “paired gate voltage” approach.74 Two Rm versus L lines are determined for two gate voltages, one being typically 0.5 V lower than the other. The intersection of these two lines gives a good approximation of RSD and Leff . The gate voltage dependence of RSD and Leff can be found using various VGS pairs. In a variation of the paired gate voltage method, L is determined for a given VT using one short and one longchannel device. A new L is found for a VT that differs by about 0.1–0.2 V from the original. This is repeated a number of times and L is plotted against VT . The intercept on the L axis yields the metallurgical channel length Lmet .75 A different representation of Eq. (4.62) is to define the parameter E as76 E = Rm (VGS − VT ) =
L − L + RSD (VGS − VT ) Weff µeff Cox
(4.65)
There are a number of mobility expressions. One of the simplest and one that is frequently used to interpret channel length and width measurements, is µeff =
µo µo µo ≈ = ′ 1 + θ (VGS 1 + θ (VGS − ID RS − VT ) 1 + θ (VGS − VT ) − VT )
(4.66)
The approximation in Eq. (4.66) is valid for (VGS − VT ) ≫ ID RS . Substituting Eq. (4.66) into Eq. (4.65) gives E=
(L − L)[1 + θ (VGS − VT )] + RSD (VGS − VT ) Weff µo Cox
(4.67)
From Eq. (4.65) we find the intercept Eint and slope m of E versus (VGS − VT ) plots to be dE (L − L)θ (L − L) ;m = = + RSD (4.68) Eint = Weff µo Cox dVGS Weff µo Cox E is plotted against (VGS − VT ) as a function of channel length. The slopes of these plots are m = (L − L)θ/Weff µo Cox + RSD and the intercepts on the Eaxis are
MOSFETs
211
Ei = (L − L)/Weff µo Cox . Ei varies since devices with varying channel lengths are used. Plots of Ei and m versus L give L and RSD from the intercepts and µo and θ from the slopes. A method related to the method of Eq. (4.65), allowing L, RSD , µo and θ to be extracted, is that due to De La Moneda et al., based on writing Eq. (4.63) as77 Rm =
θ (L − L) L − L + + RSD Weff µo Cox (VGS − VT ) Weff µo Cox
(4.69)
with the effective mobility of Eq. (4.66). First Rm is plotted against 1/(VGS − VT ) as shown in Fig. 4.22(a). The slope of this plot is m = (L − L)/Weff µo Cox and the intercept on the Rm axis is Rmi = [RSD + θ (L − L)/Weff µo Cox ] = RSD + θ m. Next m is plotted against L (Fig. 4.22(b)). This plot has a slope of 1/Weff µo Cox and an intercept on the L axis of L, allowing µo and L to be determined. Lastly, Rmi is plotted against m (Fig. 4.22(c)), giving θ from the slope and RSD from the intercept on the Rmi axis. Two devices suffice for these measurements. The channel lengths of the device pair should be selected to minimize the error in L associated with the extrapolation of the m versus L plot because errors in m are magnified by extrapolation. Errors in L are minimized by choosing channel lengths that differ by about a factor of ten. Furthermore, (VGS − VT ) should be chosen to cover a wide range. One bias point should be for low (VGS − VT ) (about 1 V) where µo Cox is dominant. A second bias point should be for high (VGS − VT ) (about 3–5 V), where θ and RSD dominate. As mentioned earlier, RSD is gate voltage dependent for LDD devices. To find this dependence, one can determine L, plot Rm versus L for various VGS − VT and determine various RSD at L = L. These RSD can then be plotted as a function of VGS − VT to illustrate this gate voltage dependence.78 A variation of the de la Moneda method is a combination of Eq. (4.60) and (4.66) to give79 ID =
ko (VGS − VT )(VDS − ID RSD ) = ko (VGS − VT )(VDS − ID R ′ ) 1 + θ (VGS − VT )
where ko =
Weff µo Cox ′ θ ; R = RSD + Leff ko
(4.70)
(4.71)
Differentiating Eq. (4.70) and using the definition for the transconductance gives gm =
ko (VDS − ID R ′ ) ∂ID VDS =constant = ∂VGS 1 + ko R ′ (VGS − VT )
(4.72)
When combined with Eq. (4.70), we obtain ID = ko VDS (VGS − VT ) √ gm
(4.73)
To determine the various device parameters, we plot ID /gm 1/2 versus VGS . The intercept yields the threshold voltage VT and the slope gives ko . The relationship L − L 1 = ko Weff µo Cox
(4.74)
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
1000 L = 4 µm
Rm (Ω)
750 Slope = m
500
2 µm
250
1 µm
Rmi 0 0
0.2
0.4
0.6
0.8
1
1/(VGS −VT) (V −1) (a) 1000
m (V·Ω)
750
500
250
0
Slope ~ µo
∆L
0
1
2 L (µm)
3
4
750
1000
(b) 200
150 Slope ~ θ Rmi (Ω)
212
100
RSD
50
0
Fig. 4.22
0
250
500 m (V·Ω) (c)
(a) Rm versus 1/(VGS − VT ); (b) slope m versus L, and (c) Rmi versus m.
MOSFETs
213
suggest a plot of 1/ko versus L. Such a plot has the intercept L = L. R ′ is obtained from Eq. (4.71). A subsequent plot of R ′ versus 1/ko yields RSD from the intercept and θ from the slope. A further variation of Eq. (4.61) for devices with two different channel lengths is the drain current ratio80 (ID1 − ID2 )RSD k1 ID1 1− (4.75) = ID2 k2 VDS for VDS1 ≫ ID1 RSD and VDS2 ≫ ID2 RSD and equal mobilities and equal threshold voltages for the two devices. A plot of ID1 /ID2 versus (ID1 − ID2 ) has a slope of k1 RSD /k2 VDS and an intercept on the ID1 /ID2 axis of k1 /k2 . This method does not work if the conditions VDS1 ≫ ID1 RSD and VDS2 ≫ ID2 RSD are not satisfied. In case these conditions are not satisfied, a modification consists of a plot of (VDS2 /ID2 − VDS1 /ID1 ) versus VDS1 /ID1 ,81 which is linear with an intercept on the VDS1 /ID1 axis of RSD and a slope (L2 − L1 )/(L1 − L) yielding L. The transconductance is also used in the transresistance method.82 – 83 The transconductance gm and the drain conductance gd = ∂ID /∂VDS are measured in the linear MOSFET region at drain voltages of 25 to 50 mV. The transresistance r is defined by r=
gm gd2
(4.76)
Two devices are required for the measurement. One is a longchannel device and the other is a shortchannel device with known channel length L. The transresistance is determined for each device and a parameter λ is calculated from the two channel lengths and the two transresistances as Lrref − Lref r (4.77) λ = rref − r where λ is plotted against (VGS − VT ) and the extrapolated intercept on the λ axis is L. The series resistance depends on the channel lengths and the drain conductances as RSD =
(Lref − L)/gd − (L − L)/gdref Lref − L
(4.78)
A comment about techniques that require differentiation: As is well known, differentiation is a noiseproducing process, by accentuating small variations in the data. Hence such techniques, e.g., those that require gd or gm , tend to be noisier than those not requiring differentiation. A technique in which the mobility can be any function of gate voltage, and for any RSD , is the shift and ratio (S/R) method.84 It uses one large device and several small devices (varying channel lengths, constant channel width) and starts with Eq. (4.63) rewritten as Rm = RSD + Lf (VGS − VT )
(4.79)
where f is a general function of gate overdrive, VGS − VT , common to all devices. Equation (4.79) is differentiated with respect to VGS . The resistance RSD is usually a weak function of gate voltage and its derivative is neglected. Equation (4.79) becomes S=
d[f (VGS − VT )] dRm =L dVGS dVGS
(4.80)
214
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
S is plotted versus VGS for the large and one small device. To solve for L and VT , one curve is shifted horizontally by a varying amount δ and the ratio r = S(VGS )/S(VGS − δ) between the two devices is computed as a function of VGS . When S is shifted by a voltage equal to the threshold voltage difference between the two devices, r is nearly constant, which is the key in this measurement. With constant gate overdrive, the mobility is identical or nearly identical, allowing r to be written as r=
L0 S(VGS ) = S(VGS − δ) L
(4.81)
where Lo and L are the channel lengths of the large and small device, respectively. Plotting the L so obtained versus Lm for several devices gives a line with intercept L on the Lm axis. The method has been successfully used for MOSFETs with channel lengths below 0.2 µm. The best range for VGS is from slightly above VT to about 1 V above VT . For LDD devices one should use low gate overdrives to ensure high S allowing dRSD /dVGS to be neglected.85 Once L is found, RSD can be calculated from Eq. (4.79). A detailed analysis of various Leff and RSD extraction techniques showed the S/R method to provide the lowest variance and the best accuracy.85 It is very important, however, to choose a properly optimized gate voltage range in order to satisfy the basic assumption that RSD is VGS independent. It is well known that RSD does depend on VGS , especially near the threshold voltage and in LDD devices. More precise L and VT extraction is achieved by assuming that dRSD /dVGS = 0 only at high gate voltages where L is maximized.86 A comprehensive study of the various mechanisms limiting the accuracy of channel length extraction techniques especially for lightly doped drain MOSFETs has shown that low gate overdrives and consistent threshold voltage measurements are very important for reliable channel length extraction.87 Other methods of determining the series resistance are based on fitting the currentvoltage characteristics using one of several methods. In the least squares method both nonlinear and multivariable least square methods have been used. Twodimensional device simulators have also been used. A detailed comparison of many of the techniques showed that the various plots, which according to simple theory should be linear, are frequently nonlinear.63 As a result, there are no unique slopes and intercepts rendering the results unreliable. Furthermore, measurement noise can substantially affect intercepts. Experimental noise can sometimes be reduced by using longer integration times during current and voltage measurements. A nonlinear optimization procedure gave significantly more accurate and robust results than some of the methods above.63 A robust method to extract VT , RSD , L, and W based on optimization using an iterative linear regression procedure has been developed.88 The parameters are extracted from analytical expressions to a linear set of equations, avoiding differentiations. The method is especially suited to process characterization. In all methods where series resistance is extracted, it is always RSD that is determined. It is usually assumed that RS = RD . That may not be always true, especially if a device has been stressed to cause hot electron damage. It is possible to determine the asymmetry between RS and RD by measuring the transconductance in the usual MOSFET configuration, i.e., drain is drain and source is source, and in the inverted configuration in which source and drain are interchanged. Combining this measurement with substrate bias and external resistances, allows the asymmetry to be determined.89 The conventional currentvoltage methods reach their limit when Leff approaches 0.1 µm, because Rch is no longer a linear function of Leff due to short channel effects.
MOSFETs
215
Hence, the key assumption of these methods is no longer satisfied. A method based on an entirely different principle is the draininduced barrier lowering (DIBL) method.90 DIBL, one manifestation of short channel effects, is the threshold voltage reduction with drain voltage, because the drain voltage affects the barrier at the sourcesubstrate junction. In the subthreshold region, the drain current becomes ID = I0 exp
qλVDS q(VGS − VT ) q(VGS − VT′ ) exp = I0 exp nkT kT nkT
(4.82)
where λ is the DIBL coefficient and VT′ = VT − nλVDS ⇒ VT = VT′ − VT = −nλVDS
(4.83)
The effect of DIBL on drain current is shown in Fig. 4.23(a), showing both increased off current (ID at VGS = 0) and reduced threshold voltage. The DIBL coefficient is
Drain Current (A)
10−3 10−4
L = 0.4 µm
10−5
tox = 9 nm VDS = 3 V
10−6 2V
10−7
1V
10−8 10−9
0.1 V
10−10 10−11
0
0.2
0.4 0.6 Gate Voltage (V) (a)
0.8
1
0
∆VT(V)
−0.05 l = 0.037 −0.1
L = 0.4 µm −0.15
0
1
2 3 Drain Voltage (V) (b)
4
5
Fig. 4.23 (a) Drain current versus gate voltage as a function of drain voltage illustrating DIBL (b) threshold voltage shift versus drain voltage; the slope gives λ.
216
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
determined from the slope of a VT versus VDS plot, illustrated in Fig. 4.23(b) taking VT = 0 for VDS = 0.1 V. Draininduced barrier lowering also depends on the channel length. The shorter the channel the more the drain voltage modulates the sourcesubstrate barrier, suggesting the use of DIBL for effective channel length measurement. The VT dependence on channel length is90 Leff (4.84) VT = α + β exp − 2Lc where α, β and Lc are constants. The key issue of Leff extraction is to determine these constants. α = VT for devices with channel length in the range of 1 µm > Leff > 0.4 µm. β is determined from the junction builtin and Fermi potentials that depend on the doping density according to (4.85) β = 2 (Vbi − 2φF )(Vbi − 2φF + VDS ) with β between 0.4 and 0.8 V. The length Lc is determined from Lc =
LDdes1 − LDdes2 2[ln(VT 1 − α) − ln(VT 2 − α)]
(4.86)
where LDdes are the design channel lengths of two devices with slightly different channel lengths which should lie between 0.1 and 0.2 µm. The method has been applied for Leff as low as 40 nm. 4.6.2
Channel Length—CapacitanceVoltage
The currentvoltage methods of Section 4.6.1 are the most common methods to determine series resistance and effective channel length, largely because of their measurement simplicity. But they do have some limitations, as discussed above. Hence, capacitance techniques are also used to determine Leff . While series resistance cannot be determined by C –V techniques, the measurement is free of ambiguities introduced by series resistance and gate voltagedependent mobility. We discuss capacitance measurements with reference to the MOSFET in Fig. 4.24. The capacitance is measured between the gate and the source/drain connected together for devices with varying channel length and wide constant width gates.91 The substrate is grounded (connected to the shield of the C –V meter cables) to shunt the drainsubstrate and sourcesubstrate capacitances from the C –V meter. For VG < VT , the surface under the gate is accumulated and the capacitance meter reads the two overlap capacitances (Fig. 4.24(a)). For VG > VT , the surface under the gate is inverted and the capacitance meter reads the two overlap capacitances and the channel capacitance (Fig. 4.24(b)). The effective gate length in this measurement is considered to be the metallurgical channel length Lmet . Cov and Cinv are given by Cov =
Kox εo LW Kox εo LW ; Cinv = tox tox
(4.87)
Rearranging Eq. (4.87) yields Lmet as Cov Lmet = L − L = L 1 − Cinv
(4.88)
217
MOSFETs
VGS < VT
VGS > VT
Cov/2
Cov/2
Cov/2
Cch
Cov/2
L
(a)
(b)
5 × 10−15 L = 1.2 µm
CGC (pF)
4 × 10−15
1 µm 0.8 µm
3 × 10−15
0.6 µm 2 × 10−15 Cov
1 × 10−15
VGS,ov 0 −4
−3
−2
−1
0 1 VGS (V)
2
3
4
(c)
Fig. 4.24 MOSFET for (a) VGS < VT , (b) VGS > VT , and (c) CGC − VGS curves; W = 10 µm, tox = 10 nm, NA = 1.6 × 1017 cm−3 .
One can either make a measurement on a single device and use Eq. (4.88) or plot (Cinv − Cov ) versus L, with slope Kox εo W/tox and intercept L on the L axis. A modified C –V method is given in ref. 92. It has also been applied to DMOSFETs.93 At what gate voltage should Cov be measured? Extensive modeling and experimental results place the gate voltage corresponding to Cov at the point where the surface just begins to invert, i.e., VGS = VGS ,ov which is near VT . To determine VGS ,ov one measures the capacitance of several devices with different channel lengths. Such curves are shown in Fig. 4.24(c). Then VGS ,ov is that gate voltage where the capacitancegate voltage curves begin to diverge. Figure 4.24(c) shows a single curve in accumulation. Detailed measurements show the curves in accumulation to depend weakly on gate length due to stray capacitances.94 Cov in the “off” state may differ from that in the “on” state. If it is taken as the capacitance just below the threshold voltage, it contains an unwanted inner fringe term that is absent when the conducting channel is formed. If taken at a negative gate voltage for nMOSFETs to accumulate the substrate and eliminate the inner fringe component, the overlapped sourcedrain region can be depleted. Such errors translate into a large error in L for shortchannel devices with low intrinsic capacitances. For smallarea MOSFETs the capacitance is very small and the overlap capacitance is still smaller, making for difficult measurements. This problem can be alleviated by connecting many devices in parallel, thereby making the effective area much larger. In
218
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
one design, 3200 transistors were connected in parallel.95 A multifinger gate device for sufficiently high capacitance, may have an offset to the MOSFET device used for I –V characterization due to lithographic proximity effects. For sub100 nm MOSFETs, the gate oxides are so thin for tunnel currents to be significant, affecting the capacitance measurement. Once Lmet is known and if one measures µeff on a large MOSFET, it is then possible to determine RSD by comparing an ideal with a real device. In this comparison one assumes Lmet ≈ Leff . If we use ID for the drain current of Eq. (4.60) and ID0 as the drain current when RSD = 0, then by simply taking the ratio ζ = ID /ID0 , RSD is RSD =
(1 − ς)VDS ID
(4.89)
In this manner, one can easily generate an RSD versus VGS curve showing the gate voltage dependence of the series resistance.91 4.6.3
Channel Width
The methods to determine the channel width W are similar to those for channel length. Several devices with varying gate width and constant gate length are used. An early technique used a plot of the MOSFET drain conductance as a function of W for devices with constant channel length.96 If source and drain resistances are neglected, then from Eq. (4.60) the drain conductance is gd =
(W − W )µeff Cox (VGS − VT ) ∂ID V =constant = ∂VDS GS Leff
(4.90)
A plot of gd against W has an intercept on the W axis of W at gd = 0. This method neglects the source and drain resistances, which is more problematic than it is for channel length measurements. Although it is a reasonably good assumption to take RS and RD as constants for devices with varying channel lengths, this is no longer true for devices with varying channel widths. Both source and drain resistances depend on channel width. When the drain conductance in Eq. (4.90) is used to extract Weff , it is possible for the intersection point to occur at negative gd . This can be due to a resistance in parallel with the intrinsic MOSFET due to a leakage path between source and drain at the device periphery. The intersection point yields both Weff and GP , the parallel conductance.97 The drain current can be written as (see Eq. (4.62)) ID =
(W − W )µeff Cox (VGS − VT )VDS Leff + (W − W )µeff Cox (VGS − VT )RSD
(4.91)
Plotting ID versus W gives W = W for ID = 0. This has been used to determine Weff .98 The measured drain resistance is [see Eq. (4.63)] Rm = Rch + RSD =
Leff + RSD (W − W )µeff Cox (VGS − VT )
(4.92)
The slope of Rm versus 1/(VGS − VT ) is m = Leff /(W − W )µeff Cox . An mW versus m plot has the slope W .99 Even if RSD varies with W , it does not vary with L, and
MESFETs AND MODFETs
219
differentiating Eq. (4.92) with respect to L gives m=
1 = (W − W )µeff Cox (VGS − VT ) dRm /dL
(4.93)
Plotting m versus W gives the intercept W = W at m = 0. Both methods require devices of varying gate widths with constant gate length. By varying the gate voltage, it is possible to generate data for Weff as a function of VGS . A technique using nonlinear optimization, similar to that for Leff determination in ref. 63, can also be used for Weff extraction.100 The drain current is measured for devices with varying widths and constant length and varying lengths and constant width. A nonlinear optimization model is fit to the data accounting for the widthdependent VT , RSD , and Weff . The method is robust, does not assume a linear model, and does not suffer from extrapolation errors in the presence of nonlinear or noisy data. A method that does not rely on currentvoltage measurements, not affected by series resistance, is the capacitance method. The oxide capacitance of a MOSFET is given by Cox =
Kox εo Leff (W − W ) tox
(4.94)
A plot of Cox as a function of W for transistors with identical gate lengths but varying widths gives a straight line with slope Kox εo Leff /tox and intercept on the W axis at W = W .101 4.7
MESFETS AND MODFETS
A MESFET (metalsemiconductor fieldeffect transistor) consists of a source, channel, drain, and gate. Majority carriers flow from source to drain in response to a drain voltage. The drain current is modulated by a reverse bias on the metalsemiconductor junction gate. With sufficient reverse bias, the spacecharge region of the metalsemiconductor contact extends to the insulating substrate and the channel is pinched off. The output currentvoltage characteristics resemble those of depletionmode MOSFETs. However, in contrast to MOSFETs, the MESFET metalsemiconductor junction can be forward biased, leading to high input currents. A MODFET (modulationdoped FET), shown in Fig. 4.25, is similar to a MESFET, with a wide band gap semiconductor interposed between the
G Wide Band Gap Semiconductor RS
RG
Rch/2
RD
S n+
D nChannel
n+
Semi Insulating Substrate
Fig. 4.25 Crosssection of a MODFET showing the various resistances. RG is the resistance of the wide band gap semiconductor.
220
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
nchannel and the gate; in a MESFET the gate is placed directly on the nchannel. We will not distinguish between these two structures. The ability to forward bias the gate of a MESFET allows additional measurements that are not possible with a MOSFET. With the gate forward biased, the drainsource voltage is (4.95) VDS = (Rch + RS + RD )ID + (αRch + RS )IG where α accounts for the fact that the gate current flows only through a portion of the channel resistance from the gate to the source; α ≈ 0.5. The gatesource voltage is VGS
nkT IG ln + RS (ID + IG ) = q Is
(4.96)
where IG = Is exp(qV GS /nkT ) is the forwardbiased gate Schottky diode current with zero resistance. ID versus VDS as a function of IG has a slope of 1/(Rch + RS + RD ), and VDS /IG gives (αRch + RS ) for ID = 0. Furthermore, from the forwardbiased IG − VGS curves as a function of ID , VGS /ID = RS for IG = constant, allowing RS , RD , and Rch to be determined. When the gate resistance RG is included, it is determined from the gate current with a voltage between gate and source. However, log(IG ) is plotted against VGD , not VGS , with the drain open circuited. A deviation of this semilog plot from a straight line is caused by the gate resistance. Another method relies on a measure of the gate current as a function of the drainsource voltage. The source is grounded and the gate current flows from the gate to the source. The gate current flowing through the source resistance and through a portion of the channel resistance rch creates a voltage drop. The drain acts as a voltage probe of this voltage drop. The “end” resistance is defined as Rend =
∂VDS ∂IG
(4.97)
From Eq. (4.97) the “end” resistance is approximately Rend = αRch + RS
(4.98)
In one “end” resistance measurement method, the drain current is zero and the drain contact floats electrically. This gives α ≈ 0.5. In another version, drain current does flow, but it is constant during the measurement, and the drain does not float. For IG ≪ ID ,102 Rend = RS +
nkT qID
(4.99)
A plot of Rend versus 1/ID has a slope nkT /q and an intercept RS on the Rend axis. This plot has a rather limited straightline portion. Deviation from a straight line at high ID is the result of the drain current being not much lower than the saturation drain current. At low ID there is a deviation due to a violation of the IG ≪ ID requirement, rendering the method of rather limited usefulness. A refinement of this method is given in Chaudhuri and Das.103 The transmission line method, discussed in detail in Chapter 3, has also been used for RS measurement. The technique yields the sheet resistance of the nchannel, from which
MESFETs AND MODFETs
221
the source resistance can be calculated, knowing the device dimensions. A disadvantage of this method is the absence of the gate on the TLM structure. Consequently, spreading resistance due to current crowding at the source end cannot be accurately measured. In another technique, devices with varying channel lengths are used with the devices operated in their linear region.104 Currentvoltage measurements are made with one of the contacts floating. With the gate floating electrically, the various resistances are RGS (fg) = RS + Rch /2; RGD (fg) = RD + Rch /2; RSD (fg) = RS + RD + Rch (4.100) A small current is forced from source to drain and the voltage drop between the floating gate and the source is measured with a highimpedance voltmeter to give RGS . Similarly for the other resistances. With the source floating, RGS (f s) = RG We define Rch = RLG ; RG =
(4.101)
1 GLG
(4.102)
where R represents the channel resistance per unit length of channel and G represents the gatetochannel conductance/unit length of channel. Substituting Eq. (4.102) into (4.100) and (4.101) gives RGS (fg) = RS +
R
; RGD (fg) = RD +
2GRGS (f s) R RSD (fg) = RS + RD + GRGS (f s)
R 2GRGS (f s)
; (4.103)
Plots of RGS (fg), RGD (fg), and RSD (fg) versus 1/RGS (f s) are linear with intercepts on the vertical axes of RS , RD , and RS + RD . Examples of such plots are shown in Fig. 4.26. The method can be checked by plotting 1/RSD (f s) versus Lm , the maskdefined or drawn channel length. Such a plot should yield a straight line with an intercept 400 RSD(fg) RS + RD = 157.9 Ω
Resistance (Ω)
300
200
RGD(fg) RD = 78.5 Ω RGS(fg)
100 RS = 77.9 Ω 0
0
0.5
1
1.5
2
1/RGS(fs) (Ω−1)
Fig. 4.26 Plots of RGS (fg), RGD (fg), and RSD (fg) versus 1/RGS (f s). Reprinted after Azzam et al.104 by permission of IEEE ( 1990, IEEE).
222
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
at Lm = 0. Another method uses two drain currents at constant gate current with the gate forward biased. The shift in the IG − VGS curves corresponding to these two conditions is related to the source resistance.105 A technique, related to the end contact resistance method, uses the gate electrode instead of the source and drain contacts to measure the source and drain resistances.106 4.8
THRESHOLD VOLTAGE
Before discussing threshold voltage measurement techniques, we briefly discuss the concept of threshold voltage. A good overview of threshold voltage measurement techniques is given in ref. 107. The threshold voltage VT is an important MOSFET parameter required for the channel length/width and series resistance measurements of this chapter. However, VT is not uniquely defined. Various definitions exist and the reason for this can be found in the ID − VGS curves of Fig. 4.27. Fig. 4.27(a) shows the ID − VGS curve of a MOSFET, illustrating the nonlinear nature of this curve. Figure 4.27(b) gives an expanded view
Drain Current (A)
4 × 10−6 3 × 10−6 2 × 10−6 1 × 10−6 0
0
0.5
1 1.5 Gate Voltage (V) (a)
2
1 × 10−6
Drain Current (A)
8 × 10−7 6 × 10−7 VT,extrapol.
4 × 10−7 2 × 10−7 0 0.5
VT,2φ
0.6
F
0.7 0.8 Gate Voltage (V) (b)
0.9
1
Fig. 4.27 ID − VGS curve of a MOSFET near the threshold voltage; (b) is an enlarged portion of (a). Modeled using Leff = 1.5 µm, tox = 25 nm, VT ,start = 0.7 V, VD = 0.1 V.
THRESHOLD VOLTAGE
223
showing the curve near the threshold voltage. There is clearly no unique gate voltage at which drain current begins to flow. A commonly used definition of threshold voltage is that gate voltage for which the surface potential, φs , in the semiconductor below the gate oxide is given by φs = 2φF =
2kT 2kT p NA ln ln ≈ q ni q ni
(4.104)
for an nchannel MOSFET. This definition, first proposed in 1953,108 is based on equating the surface minority carrier density to the majority carrier density in the neutral bulk, i.e., n(surface) = p(bulk) and is shown as VT ,2 φF in Fig. 4.27(b). Clearly, it is well below the extrapolated threshold voltage, VT ,extrapol . The threshold voltage for largegeometry, nchannel devices on uniformly doped substrates with no short or narrowchannel effects, when measured from gate to source and the φs = 2φF definition, is VT = VF B + 2φF +
√
2qKs εo NA (2φF − VBS ) Cox
(4.105)
where VBS is the substratesource voltage and VF B is the flatband voltage. The threshold voltage for nonuniformly doped, ionimplanted devices depends on the implant dose as well. Additional corrections obtain for short and narrowchannel devices. 4.8.1
Linear Extrapolation
A common threshold voltage measurement technique is the linear extrapolation method with the drain current measured as a function of gate voltage at a low drain voltage of typically 50–100 mV to ensure operation in the linear MOSFET region.109 – 111 According to Eq. (4.60) the drain current is zero for VGS = VT + 0.5VDS . But Eq. (4.60) is valid only above threshold. The drain current is not zero below threshold and approaches zero only asymptotically. Hence the ID versus VGS curve is extrapolated to ID = 0, and the threshold voltage is determined from the extrapolated or intercept gate voltage VGSi by VT = VGSi − VDS /2
(4.106)
Equation (4.106) is strictly only valid for negligible series resistance.112 Fortunately series resistance is usually negligible at the low drain currents where threshold voltage measurements are made, but it can be appreciable in LDD devices. The linear extrapolation technique can also be used for threshold voltage measurements of depletionmode or buried channel MOSFETs.113 The ID − VGS curve deviates from a straight line at gate voltages below VT due to subthreshold currents and above VT due to series resistance and mobility degradation effects. It is common practice to find the point of maximum slope on the ID − VGS curve by a maximum in the transconductance, fit a straight line to the ID − VGS curve at that point and extrapolate to ID = 0, as illustrated in Fig. 4.28. According to Eq. (4.106), VT = 0.9 V for this device. The linear extrapolation method is sensitive to series resistance and mobility degradation.87, 112, 114
224
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
2.5 × 10−4
2 × 10−4 ID
Drain Current (A)
1.5 ×
2 × 10−4 1.5 × 10−4
−4
1 × 10
1 × 10−4 VGSi = 0.95 V
5 × 10−5
5 × 10−5
Transconductance (S)
gm 10−4
VDS = 0.1 V 0 × 100
0
0.5
1 1.5 Gate Voltage (V)
2
0 × 100
Fig. 4.28 Threshold voltage determination by the linear extrapolation technique. VDS = 0.1 V, tox = 17 nm, W/L = 20 µm/0.8 µm. Data courtesy of M. Stuhl, Medtronic Corp.
Exercise 4.1 Problem: Does the linearly extrapolated threshold voltage depend on series resistance RSD ? Assume µeff to be independent of VGS . Solution: First consider the case for RSD = 0. As in the linear extrapolation method, the maximum slope of the ID − VGS curve, the transconductance gm,max is determined. From Fig. E4.1 VGSi = VGS,max −
ID,max , where gm,max
ID,max = k(VGS,max − VT − VDS /2)VDS and gm,max = kVDS ; k =
Weff µeff Cox Leff
Substituting ID,max and gm,max into the first equation, and solving for VT gives VT = VGsi − VDS /2, identical to Eq. (4.106). From Eq. (4.60) with RSD = 0; 2 × 10−5
4 × 10−5 3 × 10−5
gm
2 × 10−5
ID
1 × 10−5
VGS,max 1 × 10−5 0
VGSi 0
ID,max 0.5
1 1.5 Gate Voltage (V)
Fig. E4.1
2
0
Transconductance (S)
Drain Current(A)
gm,max
225
THRESHOLD VOLTAGE
ID,max = k(VGS,max − VT − VDS /2)(VDS − ID,max RSD ) =
k(VGS,max − VT − VDS /2)VDS 1 + kRSD (VGS,max − VT − VDS /2)
and gm,max =
kVDS [1 + kRSD (VGS,max − VT − VDS /2)]2
Substituting ID,max and gm,max into the VGsi equation above gives VGSi = VT + VDS /2 − kRSD (VGS,max − VT − VDS /2)2 Solving for the threshold voltage gives 1− VDS + VT = VGS,max − 2 Expanding this expression, using
√
1 + 4kRSD (VGS,max − VGSi ) 2kRSD
1+x ≈ 1+
x x2 3x 3 − + gives 2 8 48
VT ≈ VGSi − VDS /2 + kRSD (VGS,max − VGSi )2 − 2(kRSD )2 (VGS,max − VGSi )3
The threshold voltage can also be determined in the MOSFET saturation regime. The drain current in saturation for mobilitydominated MOSFETs is ID,sat =
mW µeff Cox (VGS − VT )2 L
(4.107)
where m is a function of doping density; it approaches 0.5 for low doping densities. VT is determined by plotting ID 1/2 versus VGS and extrapolating the curve to zero drain current, illustrated in Fig. 4.29(a).115 – 116 Since ID is dependent on mobility degradation and series resistance, we again extrapolate at the point of maximum slope. Setting VGS = VDS ensures operation in the saturation region. For shortchannel MOSFETs, where the drain current is velocity saturation limited, the saturated drain current is ID = W Cox (VGS − VT )vsat
(4.108)
where vsat is the saturationlimited velocity. The drain current in Eq. (4.108) is linear in VGS − VT as shown in Fig. 4.29(b). The threshold voltage now is simply the extrapolated gate voltage. 4.8.2
Constant Drain Current
It is obvious from Fig. 4.27 that the drain current at the threshold voltage is higher than zero. This is utilized in the constant drain current method where the gate voltage at a specified threshold drain current, IT , is taken to be the threshold voltage. This measurement is simple with only one voltage measurement necessary and it can be implemented with the circuit of Fig. 4.30(a) or by digital means.115 It lends itself readily to threshold voltage mapping. The threshold current IT is forced at the MOSFET source terminal and the opamp adjusts its output voltage to equal the gate voltage consistent with that IT .
226
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
1 × 10−3
0.03
ID1/2
0.02 ID1/2 (A1/2)
Drain Current (A)
8 × 10−4 6 × 10−4 ID 4 × 10−4 0.01 VT = 0.83 V
2 × 10−4
VDS = 2 V 0 × 100
0
0.5
1 Gate Voltage (V) (a)
1.5
2
0
1 × 10−2
Drain Current (A)
tox = 14 nm 8×
10−3
6×
10−3
W = 20 µm L = 0.6 µm
4 × 10−3 VT = 1 V 2 × 10−3 VDS = 5 V 0 × 100
0
1
2 3 Gate Voltage (V) (b)
4
5
Fig. 4.29 Threshold voltage determination by the saturation extrapolation technique. (a) VDS = 2 V, tox = 17 nm, W/L = 20 µm/0.8 µm. (b) saturation limited velocity case. Data courtesy of M. Stuhl, Medtronic Corp.
In order to make IT independent of device geometry, IT = ID /(Weff /Leff ) is sometimes specified at a current around 10 to 50 nA but other values have been used.114 – 115 VT for ID = 1 µA, often used in this type of measurement, is shown in Fig. 4.30(b). Also shown is the “linear extrapolation” VT . The method has found wide application, provided a consistent drain current is chosen. 4.8.3
Subthreshold Drain Current
In the subthreshold method the drain current is measured as a function of gate voltage below threshold and plotted as log(ID ) versus VGS . The subthreshold current depends
THRESHOLD VOLTAGE
227
VDS VBS
− +
VT
IT
(a) 10−4
2 × 10−4
Drain Current (A)
10−5
VT (Subthreshold)
10−6
1.5 × 10−4
10−7 10−8
1 × 10−4
10−9 VT (1 µA)
10−10 10−11 10−12
0
0.5
1 Gate Voltage (V) (b)
VT
5 × 10−5
Drain Current (A)
VDS = 0.1 V
(linear)
1.5
2
0 × 100
Fig. 4.30 Threshold voltage determination by the subthreshold and the threshold drain current technique. (a) Measurement circuit, (b) experimental data. tox = 17 nm, W/L = 20 µm/0.8 µm. Data courtesy of M. Stuhl, Medtronic Corp.
linearly on gate voltage in such a semilog plot. The gate voltage at which the plot departs from linearity is sometimes taken as the threshold voltage. However, for the data of Fig. 4.30(b) this point yields a threshold voltage of VT = 0.87 V, somewhat lower than that determined by the linear extrapolation method (VT = 0.95 V). 4.8.4
Transconductance
The transconductance method uses a linear extrapolation of the gm − VGS characteristic at its maximum first derivative point.117 In weak inversion, the transconductance depends exponentially on gate bias, but in strong inversion, if series resistance and mobility degradation are negligible, the transconductance tends to a constant value. In the transition region between weak and strong inversion, the transconductance depends linearly on gate bias. Fig. 4.31 shows an example of this technique with VT = 0.83 V, lower than the previous techniques.
228
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
Transconductance (S)
2.5 × 10−4 2 × 10−4 1.5 × 10−4 1 × 10−4 VT = 0.83 V 5 × 10−5 VDS = 0.1 V 0 × 100
0
0.5
1 1.5 Gate Voltage (V)
2
Fig. 4.31 Threshold voltage determination by the transconductance technique. tox = 17 nm, W/L = 20 µm/0.8 µm. Data courtesy of M. Stuhl, Medtronic Corp.
4.8.5
Transconductance Derivative
The derivative of the transconductance with gate voltage ∂gm /∂VGS is determined at low drain voltage and plotted versus gate voltage in the transconductance derivative method. The origin of this method can be understood by considering an ideal MOSFET, where ID = 0 for VGS < VT and ID ∼ VGS for VGS > VT . Hence the first derivative dID /dVGS is a step function and the second derivative d 2 ID = dVGS 2 will tend to infinity at VGS = VT . In a real device the second derivative is not infinite, but exhibits a maximum. An example plot is shown in Fig. 4.32 for the device of Fig. 4.28. The threshold voltage is about the same as for the method in Figs. 4.28. The method is not affected by series resistance and mobility degradation.112 4.8.6
Drain Current Ratio
The drain current ratio method was developed to avoid the dependence of the extracted VT on mobility degradation and parasitic series resistance.114 The drain current, given in Eq. (4.62), is reproduced here 1 × 10−3 VGS = 0.1 V dgm/dVGS (S/V)
8 × 10−4 6 × 10−4 4 × 10−4 VT = 0.98 V
2 × 10−4 0v104
0
0.5
1 1.5 Gate Voltage (V)
2
Fig. 4.32 Threshold voltage determination by the transconductance change technique. tox = 17 nm, W/L = 20 µm/0.8 µm. Data courtesy of M. Stuhl, Medtronic Corp.
THRESHOLD VOLTAGE
ID =
Weff µeff Cox (VGS − VT )VDS (L − L) + Weff µeff Cox (VGS − VT )RSD
Using
229
(4.109)
µo 1 + θ (VGS − VT )
(4.110)
W Cox µo (VGS − VT )VDS L 1 + θeff (VGS − VT )
(4.111)
µeff = allows Eq. (4.109) to be written as ID = where
θeff = θ + (W/L)µo Cox RSD
(4.112)
The transconductance is given by gm =
∂ID W Cox µo = VDS ∂VGS L [1 + θeff (VGS − VT )]2
The ID /gm 1/2 ratio ID = √ gm
W Cox µo VDS (VGS − VT ) L
(4.113)
is a linear function of gate voltage, whose intercept on the gatevoltage axis is the threshold voltage. This method is valid provided the gate voltage is confined to small variations near VT and the assumptions VDS /2 ≪ (VGS − VT ) and ∂RSD /∂VGS ≈ 0 are satisfied. The plot is shown in Fig. 4.33 giving VT = 0.97 V. The lowfield mobility µo can be determined from the slope of the ID − gm 1/2 versus VGS − VT plot and the mobility degradation factor is ID − gm (VGS − VT ) (4.114) θeff = gm (VGS − VT )2 from which θ can de determined provided RSD is known.
ID/gm1/2 (A1/2V1/2)
0.02
0.015
0.01 VT = 0.97 V
0.005
VDS = 0.1 V 0
0
0.5
1 1.5 Gate Voltage (V)
2
Fig. 4.33 Threshold voltage determination by the drain current/transconductance technique. tox = 17 nm, W/L = 20 µm/0.8 µm. Data courtesy of M. Stuhl, Medtronic Corp.
230
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
A comparison of several methods was carried out as a function of channel length.118 The results are shown in Fig. 4.34. It is clear from this plot, as it is from the data in this section, that the threshold voltage can vary widely depending on how it is measured. In all threshold voltage measurements it is important to state the sample measurement temperature since VT does depend on temperature. A typical VT temperature coefficient is −2 mV/◦ C, but it can be higher.119 4.9
PSEUDO MOSFET
The pseudo MOSFET is a simple test structure to characterize the Si layer of silicononinsulator (SOI) wafers without having to fabricate test devices.120 The original implementation is illustrated in Fig. 4.35(a), with the bulk Si substrate the “gate”, the buried oxide (BOX) the “gate” oxide, and the Si film the transistor “body”. Mechanical probes on the film surface form the source and drain. Biasing the gate drives the Si at the bottom interface into inversion, depletion, or accumulation, allowing both electron and hole conduction to be characterized. Drain currentgate voltage and drain currenttime measurements yield the effective electron and hole mobilities, threshold voltage, dopant type, dopant density, interface and oxide charge densities, series resistance, and layer defects. To reduce the effect of BOX leakage due to BOX defects, it is advantageous to etch the Si layer into islands. A more recent implementation is the mercury probe HgFET in Fig. 4.35(b), with Hg the source S, the concentric drain D, and the concentric guard ring GR.121 While changing the probe configuration from Fig. 4.35(a) to Fig. 4.35(b) may appear to be trivial, this change is actually quite profound. In the twoprobe configuration, the probe contact resistance and contact area depend on the probe pressure that may be difficult to control. The Hg probe configuration has welldefined source and drain areas, as well as a guard ring to suppress surface leakage currents. However, the HgFET relies on HgSi interfaces, i.e., Schottky barrier source and drain. It turns out that the HgSi interface is
Threshold Voltage (V)
1
7 6 5 4 3 2
0.9 0.8 0.7
1 0.6 0.5
0
0.5
1 1.5 Channel Length (µm)
2
Fig. 4.34 Threshold voltage versus channel length determined by various methods: 1: constant current for ID = 1 nA/(W/L), 2: transconductance, 3: saturation drain current extrapolation, 4: VGS where d 2 log ID /dVGS 2 is a minimum, 5: drain current linear extrapolation, 6: transconductance derivative, 7: linear extrapolation corrected for mobility. From ref. 118.
APPENDIX 4.1
S
231
D
D
GR S
Gate
Si Film Gate O xide
Oxide
Gate
Gate
(a)
Fig. 4.35
(b)
Pseudo MOSFETs (a) probe and (b) Hg contact configurations.
very sensitive to surface treatment and this interface is extremely important during HgFET measurements. A common method to control the HgSi barrier, is to rinse the Si sample in dilute HF (e.g., 1 HF:20 H2 O). This gives a low electron barrier height.122 With time, as the surface conditions change, the electron barrier height increases and the hole barrier height decreases.123 4.10 STRENGTHS AND WEAKNESSES This chapter covers such a variety of characterization techniques that it is difficult to summarize the strengths and weaknesses of each method here. Instead, we have chosen to mention the strengths and weaknesses throughout the chapter. APPENDIX 4.1 Schottky Diode CurrentVoltage Equation The currentvoltage equation of a Schottky diode with series resistance is I = AA∗ T 2 e−qφB /kT (eq(V −I rs )/nkT − 1)
(A4.1)
It has been suggested that Eq. (A4.1) is incorrect because it predicts the nonideality, included through the parameter n, to affect only the current flow from the semiconductor to the metal but not from the metal to the semiconductor,124 as is obvious from Eq. (A4.1). For high forward bias only the first term in the “exp” bracket is important and it contains the factor n. For reverse bias the second term is important and it does not contain n. To overcome this problem, consider the voltage dependence of the barrier height. The barrier height φB depends on voltage due to image force barrier lowering, due to voltage drops across any interfacial layers between the metal and the semiconductor, and other possible effects. Assuming the barrier height depends linearly on voltage according to φB (V ) = φB0 + γ (V − I rs )
(A4.2)
where γ > 0 because the barrier height increases with increased forward bias, Eq. (A4.1) becomes (A4.3) I = AA∗ T 2 e−qφB0 /kT e−qγ (V −I rs )/kT (eq(V −I rs )/kT − 1)
232
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
Defining the diode ideality factor n by ∂φB 1 = 1−γ =1− n ∂V
(A4.4)
allows Eq. (A4.3) to be written as I = AA∗ T 2 e−qφB0 /kT eq(V −I rs )/nkT (1 − e−q(V −I rs )/kT )
(A4.5)
To determine n, it is common practice to use that range of the log(I )–V plot where series resistance is negligible (V ≪ I rs ). Under those restrictions Eq. (A4.5) becomes I = AA∗ T 2 e−qφB0 /kT eqV /nkT (1 − e−qV /kT )
(A4.6)
Instead of plotting log(I ) versus V , Eq. (A4.6) predicts that log[I /(1 − exp(−qV / kT ))] versus V should be plotted. Such a plot exhibits a straight line all the way to V = 0, giving a wider range of the curve from which n is determined.125 The ideality factor is near unity for wellbehaved Schottky diodes. However, it can deviate from unity as a result of current flow due to mechanisms other than thermionic emission, e.g., thermionicfield emission current, interface damage, and interfacial layers all tend to raise n above unity.
REFERENCES 1. J.S. Escher, H.M. Berg, G.L. Lewis, C.D. Moyer, T.U. Robertson and H.A. Wey, “JunctionCurrentConfinement Planar LightEmitting Diodes and Optical Coupling into LargeCore Diameter Fibers Using Lenses,” IEEE Trans. Electron Dev. ED29, 1463–1469, Sept. 1982. 2. J.H. Werner, “Schottky Barrier and pnJunction I/V Plots—Small Signal Evaluation,” Appl. Phys. A47, 291–300, Nov. 1988. 3. K. Schuster and E. Spenke, “The Voltage Step at the Switching of Alloyed pin Rectifiers,” SolidState Electron. 8, 881–882, Nov. 1965. 4. S.M. Sze, Physics of Semiconductor Devices, 2nd ed., Wiley, New York, 1981, 256–263. 5. H. Norde, “A Modified Forward I–V Plot for Schottky Diodes with High Series Resistance,” J. Appl. Phys. 50, 5052–5053, July 1979. 6. N.T. Tam and T. Chot, “Experimental Richardson Constant of MetalSemiconductor Schottky Barrier Contacts,” Phys. Stat. Sol. 93a, K91–K95, Jan. 1986. 7. N. Toyama, “Variation in the Effective Richardson Constant of a MetalSilicon Contact Due to Metal Film Thickness,” J. Appl. Phys. 63, 2720–2724, April 1988. 8. C.D. Lien, F.C.T. So and M.A. Nicolet, “An Improved Forward I–V Method for NonIdeal Schottky Diodes with High Series Resistance,” IEEE Trans. Electron Dev. ED31, 1502–1503, Oct. 1984. 9. K. Sato and Y. Yasumura, “Study of the Forward I–V Plot for Schottky Diodes with High Series Resistance,” J. Appl. Phys. 58, 3655–3657, Nov. 1985. 10. S.K. Cheung and N.W. Cheung, “Extraction of Schottky Diode Parameters from Forward CurrentVoltage Characteristics,” Appl. Phys. Lett. 49, 85–87, July 1986. 11. T. Chot, “A Modified Forward IU Plot for Schottky Diodes with High Series Resistance,” Phys. Stat. Sol. 66a, K43–K45, July 1981. 12. R.M. Cibils and R.H. Buitrago, “Forward I–V Plot for Nonideal Schottky Diodes With High Series Resistance,” J. Appl. Phys. 58, 1075–1077, July 1985.
REFERENCES
233
13. T.C. Lee, S. Fung, C.D. Beling, and H.L. Au, “A Systematic Approach to the Measurement of Ideality Factor, Series Resistance, and Barrier Height for Schottky Diodes,” J. Appl. Phys. 72, 4739–4742, Nov. 1992. 14. K.E. Bohlin, “Generalized Norde Plot Including Determination of the Ideality Factor,” J. Appl. Phys. 60, 1223–1224, Aug. 1986; J.C. Manifacier, N. Brortyp, R. Ardebili, and J.P. Charles, “Schottky Diode: Comments Concerning Diode Parameter Determination from the Forward I–V Plot,” J. Appl. Phys. 64, 2502–2504, Sept. 1988. 15. D. Donoval, M. Barus, and M. Zdimal, “Analysis of I–V Measurements on PtSiSi Schottky Structures in a Wide Temperature Range,” SolidState Electron. 34, 1365–1373, Dec. 1991. 16. V. Mikhelashvili, G. Eisenstein, and R. Uzdin, “Extraction of Schottky Diode Parameters with a Bias Dependent Barrier Height,” SolidState Electron. 45, 143–148, Jan. 2001. 17. D.K. Schroder and D.L. Meier, “Solar Cell Contact Resistance—A Review,” IEEE Trans. Electron Dev. ED31, 637–647, May 1984. 18. M.J. Kerr, A. Cuevas, and R.A. Sinton, “Generalized Analysis of QuasiSteadyState and Transient Decay Open Circuit Voltage Measurements,” J. Appl. Phys. 91, 399–404, Jan. 2002. 19. N.P. Harder, A.B. Sproul, T. Brammer, and A.G. Aberle, “Effects of Sheet resistance and Contact Shading on the Characterization of Solar Cells by OpenCircuit Voltage Measurements,” J. Appl. Phys. 94, 2473–2479, Aug. 2003. 20. M. Wolf and H. Rauschenbach, “Series Resistance Effects on Solar Cell Measurements,” Adv. Energy Conv. 3, 455–479, Apr./June 1963. 21. D.H. Neuhaus, N.P. Harder, S. Oelting, R. Bardos, A.B. Sproul, P. Widenborg, and A.G. Aberle, “Dependence of the Recombination in ThinFilm Si Solar Cells Grown by IonAssisted Deposition on the Crystallographic Orientation of the Substrate,” Solar Energy Mat. and Solar Cells, 74, 225–232, Oct. 2002. 22. G.M. Smirnov and J.E. Mahan, “Distributed Series Resistance in Photovoltaic Devices; Intensity and Loading Effects,” SolidState Electron. 23, 1055–1058, Oct. 1980. 23. S.K. Agarwal, R. Muralidharan, A. Agarwala, V.K. Tewary and S.C. Jain, “A New Method for the Measurement of Series Resistance of Solar Cells,” J. Phys. D. 14, 1643–1646, Sept. 1981. 24. K. Rajkanan and J. Shewchun, “A Better Approach to the Evaluation of the Series Resistance of Solar Cells,” SolidState Electron. 22, 193–197, Feb. 1979. 25. G.L. Araujo and E. Sanchez, “A New Method for Experimental Determination of the Series Resistance of a Solar Cell,” IEEE Trans. Electron Dev. ED29, 1511–1513, Oct. 1982. 26. J.C.H. Phang, D.S.H. Chan and Y.K. Wong, “Comments on the Experimental Determination of Series Resistance in Solar Cells,” IEEE Trans. Electron Dev. ED31, 717–718, May 1984. 27. K.L. Kennerud, “Analysis of Performance Degradation in CdS Solar Cells,” IEEE Trans. Aerosp. Electr. Syst. AES5, 912–917, Nov. 1969. 28. D.S.H. Chan, J.R. Phillips and J.C.H. Phang, “A Comparative Study of Extraction Methods for Solar Cell Model Parameters,” SolidState Electron. 29, 329–337, March 1986. 29. J.P. Charles, M. Abdelkrim, Y.H. Muoy and P. Mialhe, “A Practical Method for Analysis of the I–V Characteristics of Solar Cells,” Solar Cells 4, 169–178, Sept. 1981. 30. P. Mialhe, A. Khoury and J.P. Charles, “A Review of Techniques to Determine the Series Resistance of Solar Cells,” Phys. Stat. Sol. 83a, 403–409, May 1984. 31. D. Fuchs and H. Sigmund, “Analysis of the CurrentVoltage Characteristic of Solar Cells,” SolidState Electron. 29, 791–795, Aug. 1986. 32. J.E. Cape, J.R. Oliver and R.J. Chaffin, “A Simplified Flashlamp Technique for Solar Cell Series Resistance Measurements,” Solar Cells 3, 215–219, May 1981. 33. D.S. Chan and J.C.H. Phang, “A Method for the Direct Measurement of Solar Cell Shunt Resistance,” IEEE Trans. Electron Dev. ED31, 381–383, March 1984.
234
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
34. H.K. Gummel, “Measurement of the Number of Impurities in the Base Layer of a Transistor,” Proc. IRE, 49, 834, April 1961. 35. J.J. Ebers and J.L. Moll, “Large Signal Behavior of Junction Transistors,” Proc. IRE, 42, 1761–1772, Dec. 1954. 36. W. Filensky and H. Beneking, “New Technique for Determination of Static Emitter and Collector Series Resistances of Bipolar Transistors,” Electron. Lett. 17, 503–504, July 1981. 37. L.J. Giacoletto, “Measurement of Emitter and Collector Series Resistances,” IEEE Trans. Electron Dev. ED19, 692–693, May 1972. 38. I. Getreu, Modeling the Bipolar Transistor, Tektronix, Beaverton, OR, 1976. This book provides a very good discussion of BJT characterization methods, especially for using curve tracers. 39. T.H. Ning and D.D. Tang, “Method for Determining the Emitter and Base Series Resistances of Bipolar Transistors,” IEEE Trans. Electron Dev. ED31, 409–412, April 1984. 40. J. Choma, Jr., “Error Minimization in the Measurement of Bipolar Collector and Emitter Resistances,” IEEE J. SolidState Circ. SC11, 318–322, April 1976. 41. K. Morizuka, O. Hidaka, and H. Mochizuki, “Precise Extraction of Emitter Resistance from an Improved Floating Collector Measurement,” IEEE Trans. Electron Dev. 42, 266–273, Feb. 1995. ¨ 42. M. Linder, F. Ingvarson K.O. Jeppson, J.V. Grahn SL Zhang, and M. Ostling, “Extraction of Emitter and Base Series Resistances of Bipolar Transistors from a Single DC Measurement,” IEEE Trans. Semicond. Manufact. 13, 119–126, May 2000. 43. J.B. Scott, “New Method to Measure Emitter Resistance of Heterojunction Bipolar Transistors,” IEEE Trans. Electron Dev. 50, 1970–1973, Sept. 2003. 44. W.D. Mack and M. Horowitz, “Measurement of Series Collector Resistance in Bipolar Transistors,” IEEE J. SolidState Circ. SC17, 767–773, Aug. 1982. 45. J.S. Park, A. Neugroschel, V. de la Torre, and P.J. Zdebel, “Measurement of Collector and Emitter Resistances in Bipolar Transistors,” IEEE Trans. Electron Dev. 38, 365–372, Feb. 1991. 46. J. Logan, “Characterization and Modeling for Statistical Design,” Bell Syst. Tech. J. 50, 1105–1147, April 1971. 47. D.D. Tang, “Heavy Doping Effects in pnp Bipolar Transistors,” IEEE Trans. Electron Dev. ED27, 563–570, March 1980. 48. B. Ricco, J.M.C. Stork and M. Arienzo, “Characterization of NonOhmic Behavior of Emitter Contacts of Bipolar Transistors,” IEEE Electron Dev. Lett. EDL5, 221–223, July 1984. 49. J. Weng, J. Holz, and T.F. Meister, “New Method to Determine the Base Resistance of Bipolar Transistors,” IEEE Electron Dev. Lett. 13, 158–160, March 1992. 50. R.C. Taft and J.C. Plummer, “An EightTerminal KelvinTapped Bipolar Transistor for Extracting Parasitic Series Resistance,” IEEE Trans. Electron Dev. 38, 2139–2154, Sept. 1991. 51. W.M.C. Sansen and R.G. Meyer, “Characterization and Measurement of the Base and Emitter Resistances of Bipolar Transistors,” IEEE J. SolidState Circ. SC7, 492–498, Dec. 1972. 52. T.E. Wade, A. van der Ziel, E.R. Chenette and G. Roig, “Base Resistance Measurements on Bipolar Junction Transistors Via Low Temperature Bridge Techniques,” SolidState Electron. 19, 385–388, May 1976. 53. R.T. Unwin and K.F. Knott, “Comparison of Methods Used for Determining Base Spreading Resistance,” Proc. IEE Pt.I 127, 53–61, April 1980. 54. G.C.M. Meijer and H.J.A. de Ronde, “Measurement of the Base Resistance of Bipolar Transistors,” Electron. Lett. 11, 249–250, June 1975. 55. A. Neugroschel, “Measurement of the LowCurrent Base and Emitter Resistances of Bipolar Transistors,” IEEE Trans. Electron Dev. ED34, 817–822, April 1987; “Corrections to “Measurement of the LowCurrent Base and Emitter Resistances of Bipolar Transistors”,” IEEE Trans. Electron Dev. ED34, 2568–2569, Dec. 1987.
REFERENCES
235
56. J.S. Park and A. Neugroschel, “Parameter Extraction for Bipolar Transistors,” IEEE Trans. Electron Dev. ED36, 88–95, Jan. 1989. 57. P. Spiegel, “Transistor Base Resistance and Its Effect on High Speed Switching,” Solid State Design 15–18, Dec. 1965. 58. K.K. Ng and W.T. Lynch, “Analysis of the GateVoltageDependent Series Resistance of MOSFET’s,” IEEE Trans. Electron Dev. ED33, 965–972, July 1986. 59. K.K. Ng, R.J. Bayruns and S.C. Fang, “The Spreading Resistance of MOSFET’s,” IEEE Electron Dev. Lett. EDL6, 195–198, April 1985. 60. G. Baccarani and G.A. SaiHalasz, “Spreading Resistance in Submicron MOSFET’s,” IEEE Electron Dev. Lett. EDL4, 27–29, Feb. 1983. 61. J.M. Pimbley, “TwoDimensional Current Flow in the MOSFET SourceDrain,” IEEE Trans. Electron Dev. ED33, 986–996, July 1986. 62. K.K. Ng and J.R. Brews, “Measuring the Effective Channel Length of MOSFETs,” IEEE Circ. Dev. 6, 33–38, Nov. 1990. 63. C.C. McAndrew and P.A. Layman, “MOSFET Effective Channel Length, Threshold Voltage, and Series Resistance Determination by Robust Optimization,” IEEE Trans. Electron Dev. 39, 2298–2311, Oct. 1992. 64. Y. Taur, “MOSFET Channel Length: Extraction and Interpretation,” IEEE Trans. Electron Dev. 47, 160–170, Jan. 2000. 65. K. Terada and H. Muta, “A New Method to Determine Effective MOSFET Channel Length,” Japan. J. Appl. Phys. 18, 953–959, May 1979. 66. J.G.J. Chern, P. Chang, R.F. Motta and N. Godinho, “A New Method to Determine MOSFET Channel Length,” IEEE Electron Dev. Lett. EDL1, 170–173, Sept. 1980. 67. D.J. Mountain, “Application of Electrical Effective Channel Length and External Resistance Measurement Techniques to a Submicrometer CMOS Process,” IEEE Trans. Electron Dev. ED36, 2499–2505, Nov. 1989. 68. S.E. Laux, “Accuracy of an Effective Channel Length/External Resistance Extraction Algorithm for MOSFET’s,” IEEE Trans. Electron Dev. ED31, 1245–1251, Sept. 1984. 69. K.L. Peng, S.Y. Oh, M.A. Afromowitz and J.L. Moll, “Basic Parameter Measurement and Channel Broadening Effect in the Submicrometer MOSFET,” IEEE Electron Dev. Lett. EDL5, 473–475, Nov. 1984. 70. S. Ogura, P.J. Tsang, W.W. Walker, D.L. Critchlow and J.F. Shepard, “Design and Characteristics of the Lightly Doped DrainSource (LDD) Insulated Gate FieldEffect Transistor,” IEEE J. SolidState Circ. SC15, 424–432, Aug. 1980. 71. B.J. Sheu, C. Hu, P. Ko and F.C. Hsu, “SourceandDrain Series Resistance of LDD MOSFET’s,” IEEE Electron Dev. Lett. EDL5, 365–367, Sept. 1984; C. Duvvury, D.A.G. Baglee and M.P. Duane, “Comments on ‘SourceandDrain Series Resistance of LDD MOSFET’s’,” IEEE Electron Dev. Lett. EDL5, 533–534, Dec. 1984; B.J. Sheu, C. Hu, P. Ko and F.C. Hsu, “Reply to ‘Comments on “SourceandDrain Series Resistance of LDD MOSFET’s”’,” IEEE Electron Dev. Lett. EDL5, 535, Dec. 1984. 72. S.L. Chen and J. Gong, “Influence of Drain Bias Voltage on Determining the Effective Channel Length and Series Resistance of DrainEngineered MOSFETs Below Saturation,” SolidState Electron. 35, 643–649, May 1992. 73. M.R. Wordeman, J.Y.C. Sun and S.E. Laux, “Geometry Effects in MOSFET Channel Length Extraction Algorithms,” IEEE Electron Dev. Lett. EDL6, 186–188, April 1985. 74. G.J. Hu, C. Chang, and Y.T. Chia, “GateVoltage Dependent Effective Channel Length and Series Resistance of LDD MOSFET’s,” IEEE Trans. Electron Dev. ED34, 2469–2475, Dec. 1987. 75. S. Hong and K. Lee, “Extraction of Metallurgical Channel Length in LDD MOSFET’s,” IEEE Trans. Electron Dev. 42, 1461–1466, Aug. 1995.
236
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
76. P.I. Suciu and R.L. Johnston, “Experimental Derivation of the Source and Drain Resistance of MOS Transistors,” IEEE Trans. Electron Dev. ED27, 1846–1848, Sept. 1980. 77. F.H. De La Moneda, H.N. Kotecha and M. Shatzkes, “Measurement of MOSFET Constants,” IEEE Electron Dev. Lett. EDL3, 10–12, Jan. 1982. 78. S.S. Chung and J.S. Lee, “A New Approach to Determine the DrainandSource Series Resistance of LDD MOSFET’s,” IEEE Trans. Electron Dev. 40, 1709–1711, Sept. 1993. 79. M. Sasaki, H. Ito, and T. Horiuchi, “A New Method to Determine Effective Channel Length, Series Resistance, and Threshold Voltage,” Proc. IEEE Int. Conf. Microelectr. Test Struct. 1996, 139–144. 80. K.L. Peng and M.A. Afromowitz, “An Improved Method to Determine MOSFET Channel Length,” IEEE Electron Dev. Lett. EDL3, 360–362, Dec. 1982. 81. J.D. Whitfield, “A Modification on ‘An Improved Method to Determine MOSFET Channel Length’,” IEEE Electron Dev. Lett. EDL6, 109–110, March 1985. 82. S. Jain, “A New Method for Measurement of MOSFET Channel Length,” Japan. J. Appl. Phys. 27, L1559–L1561, Aug. 1988; “Generalized Transconductance and Transresistance Methods for MOSFET Characterization,” SolidState Electron. 32, 77–86, Jan. 1989. 83. S. Jain, “Equivalence and Accuracy of MOSFET Channel Length Measurement Techniques,” Japan. J. Appl. Phys. 28, 160–166, Feb. 1989. 84. Y. Taur, D.S. Zicherman, D.R. Lombardi, P.R. Restle, C.H. Hsu, H.I. Hanafi, M.R. Wordeman, B. Davari, and G.G. Shahidi, “A New “Shift and Ratio” Method for MOSFET ChannelLength Extraction,” IEEE Electron Dev. Lett. 13, 267–269, May 1992. 85. S. Biesemans, M. Hendriks, S. Kubicek, and K.D. Meyer, “Practical Accuracy Analysis of Some Existing Effective Channel Length and Series Resistance Extraction Method for MOSFET’s,” IEEE Trans. Electron Dev. 45, 1310–1316, June 1998. 86. G. Niu, S.J. Mathew, J.D. Cressler, and S. Subbanna, “A Novel Channel Resistance Ratio Method for Effective Channel Length and Series Resistance Extraction in MOSFETs,” SolidState Electron. 44, 1187–1189, July 2000. 87. J.Y.C. Sun, M.R. Wordeman and S.E. Laux, “On the Accuracy of Channel Length Characterization of LDD MOSFET’s,” IEEE Trans. Electron Dev. ED33, 1556–1562, Oct. 1986. 88. P.R. Karlsson and K.O. Jeppson, “An Efficient Method for Determining Threshold Voltage, Series Resistance and Effective Geometry of MOS Transistors,” IEEE Trans. Semic. Manufact. 9, 215–222, May 1996. 89. A. Raychoudhuri, M.J. Deen, M.I.H. King, and J. Kolk, “Finding the Asymmetric Parasitic Source and Drain Resistances from the ac Conductances of a Single MOS Transistor,” SolidState Electron. 39, 900–913, June 1996. 90. Q. Ye and S. Biesemans, “Leff Extraction for Sub100 nm MOSFET Devices,” SolidState Electron. 48, 163–166, Jan. 2004. 91. S.W. Lee, “A CapacitanceBased Method for Experimental Determination of Metallurgical Channel Length of Submicron LDD MOSFET’s,” IEEE Trans. Electron Dev. 41, 403–412, March 1994; J.C. Guo, S.S. Chung, and C.H. Hsu, “A New Approach to Determine the Effective Channel Length and the DrainandSource Series Resistance of Miniaturized MOSFET’s,” IEEE Trans. Electron Dev. 41, 1811–1818, Oct. 1994. 92. H.S. Huang, J.S. Shiu, S.J. Lin, J.W. Chou, R. Lee, C. Chen, and G. Hong, “A Modified CapacitanceVoltage Method Used for Leff Extraction and Process Monitoring in Advanced 0.15 µm Complementary MetalOxideSemiconductor Technology and Beyond,” Japan. J. Appl. Phys. 40, 1222–1226, March 2001; H.S. Huang, S.J. Lin, Y.J. Chen, I.K. Chen, R. Lee, J.W. Chou, and G. Hong, “A Capacitance Ratio Method Used for Leff Extraction of an Advanced MetalOxideSemiconductor Device With Halo Implant,” Japan. J. Appl. Phys. 40, 3992–3995, June 2001.
REFERENCES
237
93. R. Valtonen, J. Olsson, and P. De Wolf, “Channel Length Extraction for DMOS Transistors Using CapacitanceVoltage Measurements,” IEEE Trans. Electron Dev. 48, 1454–1459, July 2001. 94. C.H. Wang, “Identification and Measurement of ScalingDependent Parasitic Capacitances of SmallGeometry MOSFET’s,” IEEE Trans. Electron Dev. 43, 965–972, June 1996. 95. P. Vitanov, U. Schwabe and I. Eisele, “Electrical Characterization of Feature Sizes and Parasitic Capacitances Using a Single Test Structure,” IEEE Trans. Electron Dev. ED31, 96–100, Jan. 1984. 96. Y.R. Ma and K.L. Wang, “A New Method to Electrically Determine Effective MOSFET Channel Width,” IEEE Trans. Electron Dev. ED29, 1825–1827, Dec. 1982. 97. M.J. Deen and Z.P. Zuo, “Edge Effects in NarrowWidth MOSFET’s,” IEEE Trans. Electron Dev. 38, 1815–1819, Aug. 1991. 98. Y.T. Chia and G.J. Hu, “A Method to Extract GateBiasDependent MOSFET’s Effective Channel Width,” IEEE Trans. Electron Dev. 38, 424–437, Feb. 1991. 99. N.D. Arora, L.A. Bair, and L.M. Richardson, “A New Method to Determine the MOSFET Effective Channel Width,” IEEE Trans. Electron Dev. 37, 811–814, March 1990. 100. C.C. McAndrew, P.A. Layman, and R.A. Ashton, “MOSFET Effective Channel Width Determination by Nonlinear Optimization,” SolidState Electron. 36, 1717–1723, Dec. 1993. 101. B.J. Sheu and P.K. Ko, “A Simple Method to Determine Channel Widths for Conventional and LDD MOSFET’s,” IEEE Electron Dev. Lett. EDL5, 485–486, Nov. 1984. 102. K. Lee, M.S. Shur, A.J. Valois, G.Y. Robinson, X.C. Zhu and A. van der Ziel, “A New Technique for Characterization of the “End” Resistance in ModulationDoped FET’s,” IEEE Trans. Electron Dev. ED31, 1394–1398, Oct. 1984. 103. S. Chaudhuri and M.B. Das, “On the Determination of Source and Drain Series Resistances of MESFET’s,” IEEE Electron Dev. Lett. EDL5, 244–246, July 1984. 104. W.A. Azzam and J.A. Del Alamo, “An AllElectrical FloatingGate Transmission Line Model Technique for Measuring Source Resistance in Heterostructure FieldEffect Transistors,” IEEE Trans. Electron Dev. 37, 2105–2107, Sept. 1990. 105. L. Yang and S.I. Long, “New Method to Measure the Source and Drain Resistance of the GaAs MESFET,” IEEE Electron Dev. Lett. EDL7, 75–77, Feb. 1986. 106. R.P. Holmstrom, W.L. Bloss and J.Y. Chi, “A Gate Probe Method of Determining Parasitic Resistance in MESFET’s,” IEEE Electron Dev. Lett. EDL7, 410–412, July 1986. 107. A. OrtizConde, F.J. Garcia Sanchez, J.J. Liou, A. Cerdeira, M. Estrada, and Y. Yue, “A Review of Recent MOSFET Threshold Voltage Extraction Methods,” Microelectr. Rel. 42, 583–596, AprilMay 2002. 108. W.L. Brown, “nType Surface Conductivity on pType Germanium,” Phys. Rev. 91, 518–537, Aug. 1953. 109. S.C. Sun and J.D. Plummer, “Electron Mobility in Inversion and Accumulation Layers on Thermally Oxidized Silicon Surfaces,” IEEE Trans. Electron Dev. ED27, 1497–1508, Aug. 1980. 110. R.V. Booth, M.H. White, H.S. Wong and T.J. Krutsick, “The Effect of Channel Implants on MOS Transistor Characterization,” IEEE Trans. Electron Dev. ED34, 2501–2509, Dec. 1987. 111. ASTM Standard F617M95, “Standard Method for Measuring MOSFET Linear Threshold Voltage,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., Conshohocken, PA, 1996. 112. H.S. Wong, M.H. White, T.J. Krutsick and R.V. Booth, “Modeling of Transconductance Degradation and Extraction of Threshold Voltage in Thin Oxide MOSFET’s,” SolidState Electron. 30, 953–968, Sept. 1987. 113. S.W. Tarasewicz and C.A.T. Salama, “Threshold Voltage Characteristics of IonImplanted Depletion MOSFETs,” SolidState Electron. 31, 1441–1446, Sept. 1988.
238
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
114. G. Ghibaudo, “New Method for the Extraction of MOSFET Parameters,” Electron. Lett. 24, 543–545, April 1988; S. Jain, “Measurement of Threshold Voltage and Channel Length of Submicron MOSFETs,” Proc. IEE Pt.I 135, 162–164, Dec. 1988. 115. H.G. Lee, S.Y. Oh and G. Fuller, “A Simple and Accurate Method to Measure the Threshold Voltage of an EnhancementMode MOSFET,” IEEE Trans. Electron Dev. ED29, 346–348, Feb. 1982. 116. ASTM Standard F1096, “Standard Method for Measuring MOSFET Saturated Threshold Voltage,” 1996 Annual Book of ASTM Standards, Am. Soc. Test. Mat., Conshohocken, PA, 1996. 117. M. Tsuno, M. Suga, M. Tanaka, K. Shibahara, M. MiuraMattausch, and M. Hirose, “PhysicallyBased Threshold Voltage Determination for MOSFET’s of All Gate Lengths,” IEEE Trans. Electron Dev. 46, 1429–1434, July 1999. 118. K. Terada, K. Nishiyama, and KI, Hatanaka, “Comparison of MOSFETThresholdVoltage Extraction Methods,” SolidState Electron. 45, 35–40, Jan. 2001. 119. F.M. Klaassen and W. Hes, “On the Temperature Coefficient of the MOSFET Threshold Voltage,” SolidState Electron. 29, 787–789, Aug. 1986. 120. S. Cristoloveanu, D. Munteanu, and M. Liu, “A Review of the PseudoMOS Transistor in SOI Wafers: Operation, Parameter Extraction, and Applications,” IEEE Trans. Electron Dev., 47, 1018–1027, May 2000. 121. H.J. Hovel, “Si Film Electrical Characterization in SOI Substrates by the HgFET Technique,” SolidState Electron. 47, 1311–1333, Aug. 2003. 122. Y.J. Liu and H.Z. Yu, “Effect of Organic Contamination on the Electrical Degradation of Hydrogen terminated Silicon upon Exposure to Air under Ambient Conditions,” J. Electrochem. Soc. 150, G861–G865, Dec. 2003. 123. J.Y. Choi, S. Ahmed, T. Dimitrova, J.T.C. Chen, and D.K. Schroder, “The Role of the MercurySi Schottky Barrier Height in PseudoMOSFETs,” IEEE Trans. Electron Dev. 51 1164–1168, July 2004. 124. E.H. Rhoderick, “MetalSemiconductor Contacts,” Proc. IEE Pt.I 129, 1–14, Feb. 1982; E.H. Rhoderick and R.H. Williams, MetalSemiconductor Contacts, 2nd ed., Clarendon Press, Oxford, 1988. 125. J.D. Waldrop, “SchottkyBarrier Height of Ideal Metal Contacts to GaAs,” Appl. Phys. Lett. 44, 1002–1004, March 1984.
PROBLEMS 4.1
The I –V data of a forwardbiased pn junction are shown. Determine the temperature T and the series resistance rs for this device. V (V ) 0.00 0.0250 0.0500 0.0750 0.100 0.125 0.150 0.175 0.200 0.225 0.250 0.275 0.300 0.325
I (A) 0.0000 1.291e12 4.248e12 1.102e11 2.654e11 6.209e11 1.435e10 3.301e10 7.576e10 1.737e09 3.980e09 9.119e09 2.089e08 4.786e08
V (V ) 0.350 0.375 0.400 0.425 0.450 0.475 0.500 0.525 0.550 0.575 0.600 0.625 0.650 0.675
I (A) 1.096e07 2.512e07 5.754e07 1.318e06 3.019e06 6.913e06 1.582e05 3.618e05 8.252e05 0.0001872 0.0004191 0.0009134 0.001882 0.003506
V (V ) 0.700 0.725 0.750 0.775 0.800 0.825 0.850 0.875 0.900 0.925 0.950 0.975 1.00
I (A) 0.006291 0.01005 0.01429 0.01961 0.02543 0.03185 0.03833 0.04504 0.05194 0.05899 0.06616 0.07344 0.08080
PROBLEMS
4.2
239
The I –V curves of a forwardbiased pn junction are shown in Fig. P4.2. Determine the temperature T for the “T = ?” curve and the series resistance rs for the “T = 300 K” curve. 100
I (A)
10−2
T=?
10−4
T = 300K
10−6
10−8
0
0.2
0.4
0.6
0.8
1
V (V)
Fig. P4.2
4.3
The current voltage relationship for a pn junction is q(V − I rs ) q(V − I rs ) − 1 + Io,qnr exp −1 . I = Io,scr exp nkT nkT
From the I –V curve in Fig. P4.3 or data determine Io,scr , Io,qnr , n in the scr, n in the qnr, and rs . T = 300 K. Determine rs and n also from I /gd versus I and gd /I versus gd plots.
10−2 10−4 I (A)
qnr 10−6 scr
10−8 10−10 0
0.2
0.4 V (V)
0.6
0.8
Fig. P4.3 V (V ) 0.0 0.01 0.02
I (A) 0.0 2.141e10 4.738e10
V 0.20 0.21 0.22
I 4.916e08 6.046e08 7.445e08
V 0.40 0.41 0.42
I 7.533e06 1.049e05 1.472e05
V 0.6 0.61 0.62
I 0.005193 0.006188 0.007770
240
4.4
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
V (V )
I (A)
V
I
V
I
V
I
0.03 0.04 0.05 0.06 0.07 0.08 0.09 0.10 0.11 0.12 0.13 0.14 0.15 0.16 0.17 0.18 0.19
7.890e10 1.172e09 1.637e09 2.201e09 2.887e09 3.721e09 4.734e09 5.966e09 7.466e09 9.291e09 1.151e08 1.422e08 1.753e08 2.157e08 2.651e08 3.257e08 4.001e08
0.23 0.24 0.25 0.26 0.27 0.28 0.29 0.30 0.31 0.32 0.33 0.34 0.35 0.36 0.37 0.38 0.39
9.183e08 1.135e07 1.408e07 1.751e07 2.187e07 2.745e07 3.464e07 4.398e07 5.623e07 7.243e07 9.406e07 1.232e06 1.629e06 2.173e06 2.925e06 3.975e06 5.449e06
0.43 0.44 0.45 0.46 0.47 0.48 0.49 0.50 0.51 0.52 0.53 0.54 0.55 0.56 0.57 0.58 0.59
2.079e05 2.952e05 4.211e05 6.029e05 8.657e05 0.0001245 0.0001792 0.0002575 0.0003691 0.0005260 0.0007432 0.001037 0.001421 0.001904 0.002479 0.003122 0.003792
0.63 0.64 0.65 0.66 0.67 0.68 0.69 0.70 0.71 0.72 0.73 0.74 0.75 0.76 0.77 0.78 0.79
0.009066 0.01073 0.01224 0.01402 0.01569 0.01757 0.01937 0.02112 0.02321 0.02506 0.02720 0.02912 0.03130 0.03327 0.03549 0.03765 0.03976
The current–voltage curves of a Schottky diode are shown in Fig. P4.4 for various temperatures. Determine n, φB , A∗ , and rs . A = 10−3 cm2 . 10−2 400K
I (A)
10−4
350K
10−6 300K 10−8 10−10 10−12
T = 250K 0
0.2
0.4
0.6
0.8
1
V (V)
Fig. P4.4
4.5
A solar cell obeys the “light” and “dark” equations q(V − I rs ) q(V + I rs ) − 1 ; Idk = Io exp −1 . I = IL − Io exp nkT nkT From the curves in Fig. P4.5 determine: Io , n and rs . T = 290 K. To determine rs use three methods: (i) the “light” curves only; (ii) the “dark” curve only; (iii) both curves.
4.6
Consider a resistor R placed externally in either the base lead or the emitter lead in the bipolar junction transistor in Fig. P4.6. Which placement has the largest effect on the collector IC ?
PROBLEMS
100 10−2
I (A)
10−4 10−6 10−8 10−10 10−12
0
0.2
0.4 V (V)
0.6
0.8
(a)
0.14 0.12
I (A)
0.10 0.08 0.06 0.04 0.02 0.00
0
0.1
0.2
0.3 V (V)
0.4
0.5
0.6
(b)
10−9
I (A)
10−10
10−11
10−12
0
0.02
0.04 0.06 V (V) (c) Fig. P4.5
0.08
0.1
241
242
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
100
I (A)
10−1
10−2
10−3 0.4
0.5
0.6 V (V)
0.7
0.8
(d)
Fig. P4.5 B
IE
(continued)
E
C
IB
IC n+
p+
n+
n
p Substrate
Fig. P4.6
4.7
Leff and RSD = RS + RD of a MOSFET can be obtained from a plot of the measured drain resistance Rm vs. L. Consider two Rm versus L curves of an LDD (lightlydoped drain) MOSFET for VGS1 and VGS2 , where VGS2 = VGS1 + V1 . Draw the two lines for VGS1 and VGS2 on an Rm versus L plot. On the same figure, draw the line for VGS3 = VGS1 + 2 , where V2 < V1 . Remember, in LDD devices, both Leff and RSD are gate voltage dependent. Give reasons for your answer.
4.8
Consider the two nchannel MOSFETs in Fig. P4.8. NA2 > NA1 . Discuss whether the threshold voltages and the drain currents for a given drain and gate voltage
n+
n+ NA1
NA1
(a)
NA2
(b)
Fig. P4.8
PROBLEMS
243
are the same for these devices. Justify your answers. Assume the source and substrate to be grounded. 4.9
Consider the four nchannel MOSFETs in Fig. P4.9. NA2 > NA1 . Discuss whether the threshold voltages and the drain currents for a given drain and gate voltage are the same for these devices. Justify your answers. Assume the source and substrate to be grounded.
n+
n+
NA1
NA1
(a)
n+
NA2
(b)
n+
NA2
NA2
(c)
NA1
(d)
Fig. P4.9
4.10 Consider two MOSFETs of the type shown in Fig. P4.10. G
D
n
n 0
L
x
p
Fig. P4.10
(a) Uniform gate oxide thickness tox = tox1 .
(b) Graded gate oxide thickness between source and drain, according to tox (x) = (tox1 − tox2 )(1 − x/L) + tox2 ; tox2 < tox1 . Are the threshold voltages for these two structures identical? Are the drain currents, measured at low drain voltage, identical for these two structures? Give reasons for your answers. VF B = 0.
244
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
4.11 The measured resistance of a MOSFET is shown in Fig. P4.11 for various gate lengths as a function of gate voltage. Choose one answer. VG1 > VG2 , VG1 = VG2 , VG1 < VG2 .
What is determined by point A? Draw on the same figure the lines for the same gate voltages when Rm = 0 and L = 0. All other parameters are unchanged. VG1
Rm
VG2 A
L
Fig. P4.11
4.12 Rm = VDS /ID is shown in Fig. P4.12 for the MOSFET on the left for gate voltages VG1 and VG2 . Draw the VG2 line for the LDD structure on the right. VG1 is that gate voltage at which a channel is formed between the two nregions without changing the conductivity of these regions.
n+
n+ p
Rm
n VG1
p
Rm VG1 VG2
RSD 2L1
L
L
Fig. P4.12
4.13 The currentvoltage relationship of a MOSFET in the presence of series resistance is (source and substrate are grounded): ID ≈
Weff Cox µo ′ , (VGS − VT − 0.5VDS )VDS Leff [1 + θ (VGS − VT )]
PROBLEMS
245
′ where VDS = VDS − ID (RS + RD ), Weff = W − W , and Leff = L − L. Using the ID − VGS data determine VT , µo , θ , L, and RSD = RS + RD ; assume W = 0. tox = 10 nm, W = 50 µm, VD = 50 mV. The drain current for various channel lengths and various gate voltages is listed in the following table:
VGS (V ) 0.725 1.025 1.325 1.625 1.925 2.225 2.525 2.825 3.125 3.425 3.725 4.025 4.325 4.625 4.925 5.225
L = 20 µm 4.935e07 6.176e06 1.145e05 1.636e05 2.094e05 2.523e05 2.924e05 3.301e05 3.656e05 3.991e05 4.307e05 4.606e05 4.889e05 5.157e05 5.412e05 5.655e05
ID (A) 12 µm
7 µm
1 µm
8.326e07 1.026e05 1.876e05 2.645e05 3.345e05 3.985e05 4.572e05 5.113e05 5.612e05 6.075e05 6.504e05 6.905e05 7.278e05 7.628e05 7.957e05 8.265e05
1.460e06 1.749e05 3.119e05 4.304e05 5.339e05 6.250e05 7.058e05 7.781e05 8.430e05 9.017e05 9.550e05 0.0001004 0.0001048 0.0001089 0.0001127 0.0001162
1.517e05 0.0001132 0.0001527 0.0001740 0.0001873 0.0001964 0.0002031 0.0002081 0.0002121 0.0002153 0.0002179 0.0002202 0.0002220 0.0002237 0.0002251 0.0002263
4.14 Draw ID − VDS for VGS = VGS1 > VT and ID − VGS for low VDS , with region [1]: (i) p + , (ii) n+ , as shown in Fig. P4.14. Draw both curves on the same figure in each case. What device characteristics are determined from ID − VDS curves? What device characteristics are determined from ID − VGS curves? VGS
VDS
n
n
[1] ptype
ID
ID
VDS
VGS
Fig. P4.14
246
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
4.15 The ID − VGS and ID − VDS plots of two MOSFETs with different gate lengths are shown in Fig. P4.15. Determine VT , RSD and L for each device. Determine the effective mobility for the L = 2 µm device at VGS = 2 V, using µeff =
gd Leff . W Cox (VGS − VT )
MOSFET1: tox = 5 nm, L = 0.5 µm, W = 10 µm, Kox = 3.9. MOSFET2: tox = 10 nm, L = 2 µm, W = 10 µm, Kox = 3.9. 2 × 10−5
4 × 10−5
2 × 10−5
1 × 10−5
L = 2 µm
1 × 10−5
Drain Current (A)
Drain Current (A)
L = 0.5 µm 3 × 10−5
VDS = 0.1 V 0 0.5
0.6 0.7 Gate Voltage (V) (a) 1 × 10−4
VGS = 1.9 V
Drain Current (A)
Drain Current (A)
0.0004
0 0.8
0.0002 1.4 V L = 0.5 µm tox = 5 nm
0 0
0.05 Drain Voltage (V) (b)
0.1
VGS = 2 V 5 × 10−5 1.5 V
0 × 10
L = 2 µm tox = 10 nm
0
0
0.05 Drain Voltage (V) (c)
0.1
Fig. P4.15
4.16 The ID − VGS and ID − VDS plots of two MOSFETs with different gate lengths are shown ion Fig. P4.16. Determine VT , RSD and L. Determine the effective mobility for the L = 2 µm device at VGS = 2 V, using µeff =
gd Leff . W Cox (VGS − VT )
MOSFET1: tox = 5 nm, L = 0.25 µm, W = 5 µm, Kox = 3.9. MOSFET2: tox = 5 nm, L = 2 µm, W = 5 µm, Kox = 3.9.
PROBLEMS
1 × 10−4
247
4 × 10−5
3 × 10−5 L = 2 µm 5 × 10−5
2 × 10−5
1 × 10−5
Drain Current (A)
Drain Current (A)
L = 0.25 µm
VDS = 0.1 V 0 × 100 0.3
0.4
0.5 0.6 Gate Voltage (V) (a) 1 × 10−4
VGS = 2 V
2 × 10−4
0 × 100
Drain Current (A)
Drain Current (A)
4 × 10−4
0 0.7
1.5 V L = 0.25 µm tox = 5 nm 0
0.05 Drain Voltage (V) (b)
0.1
VGS = 2 V
1.5 V
5 × 10−5
0 × 100
L = 2 µm tox = 5 nm 0
0.05 Drain Voltage (V) (c)
0.1
Fig. P4.16
4.17 Rm = VDS /ID versus 1/(VGS − VT ) curves are measured on MOSFETs with various gate lengths and shown in Fig. P4.17. Determine L(in µm), RSD , µo , and θ . W = 10 µm, tox = 5 nm, Kox = 3.9, VT = 0.4 V. Curve fitting gives: y = 198.7 + 50x; y = 200.6 + 112x; y = 203 + 173x; y = 207.3 + 263x. 400
Rm (Ω )
L = 1 µm
Slope = m
0.7 µm
0.5 µm
300 0.3 µm Rmi 200
0
0.5 1/(VGS − VT) (V−1)
Fig. P4.17
1
248
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
4.18 On Fig. P4.18, show the physical gate length and the metallurgical channel length. Can the effective channel length be larger than L1 ? Discuss.
Gate Gate Oxide n+
n+
L1
p
Fig. P4.18
4.19 Two Rm versus L lines for a MOSFET are shown in Fig. P4.19. Rm = VDS /ID . Determine the source and drain resistance RSD and L = L − Leff . Then, on the same figure, draw the two lines when the MOSFET oxide thickness tox is decreased. 250
Rm (Ohms)
200 150 100 50 VDS = 0.1 V 0
0
0.5
1 L (µm)
1.5
2
Fig. P4.19
4.20 The total resistance Rm defined as VDS /ID is shown in Fig. P4.20 for MOSFETs with different gate lengths.
VGS1 VGS2 Rm
L
Fig. P4.20
PROBLEMS
249
Choose one answer: VGS1 > VGS2 VGS1 = VGS2 VGS1 < VGS2 What parameters can be determined from this plot? Draw the two lines for the same gate voltages VGS1 and VGS2 when the oxide thickness is reduced. Assume the threshold voltage remains unchanged. 4.21 The total resistance Rm defined as VDS /ID is shown in Fig. P4.21 for MOSFETs with different gate lengths.
VGS1 VGS2 Rm
L
Fig. P4.21
Choose one answer: VGS1 > VGS2 VGS1 = VGS2 VGS1 < VGS2 What parameters can be determined from this plot? Draw the two lines for the same gate voltages VGS1 and VGS2 when the source and drain contact resistances are increased. 4.22 The Rm versus L plot of MOSFET (a) is shown in Fig. P 4.22.
n+
VGS2
n+ p Rm
(a) n+
n
n
VGS1
n+
p
L
(b)
Fig. P4.22
(a) What is L and Rm at the point of intersection? (b) VGS1 > VGS2 VGS1 = VGS2 VGS1 < VGS2 (c) Draw on the Rm versus L plot the two lines for the LDD MOSFET (b) for the same gate voltages. The gate overlap over the n+ source and drain in (a) is the
250
SERIES RESISTANCE, CHANNEL LENGTH AND WIDTH, AND THRESHOLD VOLTAGE
same as the overlap over the n regions in (b). For MOSFET (b): At the lower gate voltage, a channel exists between the two nregions; at the higher gate voltage, the nregions are accumulated by the gate voltage.
REVIEW QUESTIONS • Why is the I –V curve a straight line on a semilog plot? • Why does a Si diode log I –V curve have two slopes?
• How does series resistance affect the diode current?
• How is the barrier height of Schottky diodes determined?
• Why can the Schottky diode barrier heights be different when determined from
I –V or C –V data?
• Why are series and shunt resistance important in solar cells? • How are emitter and base resistances in BJT determined?
• Name three device/material parameters that influence the threshold voltage? • Why does the effective channel length differ from the physical gate length?
• Which effective channel length methods are useful for shortchannel MOSFETs?
• What is an advantage of the capacitancevoltage technique over currentvoltage
techniques for effective channel length determination?
• How is the threshold voltage measured?
5 DEFECTS
5.1
INTRODUCTION
All semiconductors contain defects. They may be foreign atoms (impurities) or crystalline defects. Impurities are intentionally introduced as dopant atoms (shallowlevel impurities), recombination centers (deeplevel impurities) to reduce the device lifetime, or deeplevel impurities to increase the substrate resistivity. Impurities are also unintentionally incorporated during crystal growth and device processing. Various types of defects are shown schematically in Fig. 5.1. The open circles represent the host atoms (e.g., silicon). The defects are: (1) foreign interstitial (e.g., oxygen in silicon), (2) foreign substitutional (e.g., dopant atom), (3) vacancy, (4) self interstitial, (5) stacking fault, (6) edge dislocation, and (7) precipitate. The corncob illustrates a vacancy and an interstitial and the saguaro cactus a stacking fault and edge dislocation. Today’s silicon is grown very pure with metallic densities on the order of 1010 cm−3 or less. Processing tends to introduce higher densities, but many of these impurities are gettered during subsequent processing with densities of typically 1010 –1012 cm−3 after processing. Metallic impurities affect various device parameters. We show in Fig. 5.2 some regions where metals cause problems. A major concern is metallic contamination at the semiconductor/oxide interface because it degrades the gate oxide integrity. Metals also degrade devices if located at high stress points and in junction spacecharge regions. The effect of iron and copper contamination in silicon is illustrated in Fig. 5.3. Fig. 5.3(a) shows the % failure versus oxide breakdown electric field as a function of iron contamination in Si wafers. Fig. 5.3(b) shows a similar plot for copper contamination. Typically metal contamination leads to more severe oxide breakdown degradation for thicker oxides, but as these figure show there is degradation even for 3 nm oxides. Thinner oxides show
Semiconductor Material and Device Characterization, Third Edition, by Dieter K. Schroder Copyright 2006 John Wiley & Sons, Inc.
251
252
DEFECTS (1)
(3)
(2)
(4) (5)
(6)
Fig. 5.1
(7)
Schematic representation of defects in semiconductors described in the text.
Stress Metal precipitate
Fig. 5.2
Spacecharge region
MOSFET regions sensitive to metal contamination.
less degradation due to the higher leakage currents through such thin oxides even in the absence of metal contamination. The characterization of shallowlevel or dopant impurities is discussed in Chapters 2, 10, and 11. Shallowlevel impurity densities are best measured electrically, but their energy levels are best determined optically. In this chapter we discuss predominantly the measurement of deeplevel impurities whose densities and energy
GENERATIONRECOMBINATION STATISTICS
253
99.99 99.9
tox = 3 nm
Fe
Failures (%)
99 95 90 80 70 50 30 20 10 5
NFe = 1.4 × 1012 cm−3 5.0 × 1011 No Fe
1 .1 .01 1 × 106
4 × 1010 4 × 106
7 × 106 −Eox, bd (V/cm)
1 × 107
1.3 × 107
(a) 99.99 99.9
Cu
tox = 3 nm
Failures (%)
99 95 90 80 70 50 30 20 10 5 1 .1 .01 8 × 106
10 ppm
No Cu
10 ppb
1 × 107
1.2 × 107 1.4 × 107 Eox, bd (V/cm)
1.6 × 107
(b)
Fig. 5.3 Oxide failure percentage versus oxide breakdown electric field as a function of metal contamination for (a) Fecontaminated Si and (b) Cucontaminated Si; the wafers were dipped in a 10 ppb or 10 ppm CuSO4 solution and annealed at 400◦ C. Data after ref. 1.
levels are best measured electrically. Milnes gives a good review of impurities in semiconductors.2 – 3 Jaros treats the theoretical aspects of deeplevel impurities.4
5.2 5.2.1
GENERATIONRECOMBINATION STATISTICS A Pictorial View
The band diagram of a perfect single crystal semiconductor consists of a valence band and a conduction band separated by the band gap, with no energy levels within the
254
DEFECTS
band gap. When the periodicity of the single crystal is perturbed by foreign atoms or crystal defects, discrete energy levels are introduced into the band gap, shown by the ET lines in Fig. 5.4. Each line represents one such defect. Such defects are commonly called generationrecombination (GR) centers or traps. GR centers lie deep in the band gap and are known as deep energy level impurities, or simply deeplevel impurities. They act as recombination centers when there are excess carriers in the semiconductor and as generation centers when the carrier density is below its equilibrium value as in the reversebiased spacecharge region (scr) of pn junctions or MOScapacitors, for example. For single crystal semiconductors like silicon, germanium, and gallium arsenide, deep level impurities are usually metallic impurities, but they can be crystal imperfections, such as dislocations, stacking faults, precipitates, vacancies, or interstitials. Usually they are undesirable, but occasionally they are deliberately introduced to alter a device characteristic, e.g., the switching time of bipolar devices. In some semiconductors like GaAs and InP, deeplevel impurities raise the substrate resistivity, creating semiinsulating substrates. For amorphous semiconductors, defects are mainly due to structural imperfections. Let us consider the deeplevel impurity in Fig. 5.4 with an energy ET and density NT impurities/cm3 . The energy ET is an effective energy discussed in Appendix 5.1. The semiconductor has n electrons/cm3 in the conduction band and p holes/cm3 in the valence band introduced by shallowlevel dopants, not shown on the figure. To follow the various capture and emission processes, let the center first capture an electron from the conduction band (Fig. 5.4(a)), characterized by the capture coefficient cn . After electron capture one of two events takes place. The center can either emit the electron back to the conduction band, called electron emission en (Fig. 5.4(b)), or it can capture a hole from the valence band, shown in Fig. 5.4(c) as cp . After either of these events, the GR center is occupied by a hole and again has two choices. Either it emits the hole back to the valence band ep in Fig. 5.4(d) or captures an electron (Fig. 5.4(a)). These are the only four possible events between the conduction band, the impurity energy level, and the valence band. Process (d) is sometimes viewed as electron emission from the valence band to the impurity shown by the dashed arrow. We will, however, use the hole emission process in (d) because it lends itself more readily to mathematical analysis. A recombination event is Fig. 5.4(a) followed by (c) and a generation event is (b) followed by (d). The impurity is a GR center and both the conduction and valence bands participate in recombination and generation. These mechanisms are the topic of
n
E
cn
Ec en ET
nT pT
cp
ep Ev
p (a)
(b)
(c)
(d)
x
Fig. 5.4 Electron energy band diagram for a semiconductor with deeplevel impurities. The capture and emission processes are described in the text.
GENERATIONRECOMBINATION STATISTICS
255
Chapter 7. A third event that is neither recombination nor generation, is the trapping event (a) followed by (b) or (c) followed by (d). In either case a carrier is captured and subsequently emitted back to the band from which it came. Only one of the two bands and the center participate and the impurity is a trap. Impurities are frequently referred to as traps, regardless of whether they act as recombination, generation, or trapping centers. The subscript “T ” in the following equations stands for trap. Whether an impurity acts as a trap or a GR center depends on ET , the location of the Fermi level in the band gap, the temperature, and the capture crosssections of the impurity. Generally those impurities with energies near the middle of the band gap behave as GR centers, whereas those near the band edges act as traps. Generally the electron emission rate for centers in the upper half of the band gap is higher than the hole emission rate. Similarly the hole emission rate is generally higher than the electron emission rate for centers in the lower half of the band gap. For most centers one emission rate dominates, and the other can frequently be neglected. 5.2.2
A Mathematical Description
A GR center can exist in one of two states. When occupied by an electron, it is in the nT state and when occupied by a hole, it is in the pT state (both shown in Fig. 5.4). If the GR center is a donor, nT is neutral and pT is positively charged. For an acceptor, nT is negatively charged and pT is neutral. The density of GR centers occupied by electrons nT and holes pT must equal the total density NT or NT = nT + pT . In other words, a center is either occupied by an electron or a hole. When electrons and holes recombine or are generated, the electron density in the conduction band n, the hole density in the valence band p, and the charge state of the center nT or pT are all functions of time. For that reason we will first address the question, “what is the time rate of change of n, p, and nT ?” We develop the appropriate equations for electrons. The equations for holes are analogous, and their derivation follows similar paths. A good discussion of the equations and their derivations is given by Sah et al.5 The electron density in the conduction band is diminished by electron capture (process (a) in Fig. 5.4) and increased by electron emission (process (b) in Fig. 5.4) and the electron time rate of change due to GR mechanisms is6 – 7 dn G−R = (b) − (a) = en nT − cn npT dt
(5.1)
The subscript “GR” signifies that we are only considering emission and capture processes through GR centers. We are not considering radiative or Auger processes. However, later in the chapter we address briefly optical emission as a mechanism to excite carriers into or out of GR centers. Electron emission depends on the density of GR centers occupied by electrons and the emission rate through the relation (b) = en nT . This relationship does not contain n because it is not necessary for there to be electrons in the conduction band during the emission process. But the GR centers must be occupied by electrons, for if there are no electrons on the centers, none can be emitted. The capture process is slightly more complicated because it depends on n, pT and the capture coefficient cn through the relation (a) = cn npT . The electron density n is important because, to capture electrons, there must be electrons in the conduction band. For holes we find the parallel expression dp G−R = (d) − (c) = ep pT − cp pnT dt
(5.2)
256
DEFECTS
The emission rate en represents the electrons emitted per second from electronoccupied GR centers. The capture rate cn n represents the density of electrons captured per second from the conduction band. The units are: en in 1/s and cn in cm3 /s. You may wonder how there can be more than one electron emitted from a GR center. After an electron has been emitted, the center finds itself in the pT state and subsequently emits a hole, returning it to the nT state. Then the cycle repeats. Where do the electrons and holes come from for this cycle to continue? Surely they cannot come from the center itself. It may be helpful to view hole emission from the GR center as electron emission from the valence band to the GR center, indicated by the dashed line in Fig. 5.4(d). In this picture the electronhole emission process is nothing more than an electron being excited from the valence band to the conduction band with an intermediate stop at the ET level. However, it is easier to deal with the equations if we consider hole and electron emission as shown by the solid lines in Fig. 5.4. The capture coefficient cn is defined by cn = σn vth
(5.3)
where vth is the electron thermal velocity and σn is the electron capture crosssection of the GR center. A physical explanation of cn can be gleaned from Eq. (5.3). We know that electrons move randomly at their thermal velocity and that GR centers remain immobile in the lattice. Nevertheless, it is helpful to change the frame of reference by letting the electrons be immobile and the GR centers move at velocity vth . The centers then sweep out a volume per unit time of σn vth . Those electrons that find themselves in that volume have a very high probability of being captured. Capture crosssections vary widely depending on whether the center is neutral, negatively, or positively charged. A center with a negative or repulsive charge has a smaller electron capture cross section than one that is neutral or attractively charged. Neutral capture crosssections are on the order of 10−15 cm2 —roughly the physical size of the atom. Whenever an electron or hole is captured or emitted, the center occupancy changes, and that rate of change is, from Eqs. (5.1) and (5.2), given by dn dp dnT G−R = − = (cn n + ep )(NT − nT ) − (cp p + en )nT dt dt dt
(5.4)
This equation is nonlinear, with n and p being timedependent variables. If the equation can be linearized, it can be solved easily. Two cases allow this simplification. (1) In a reversebiased spacecharge region both n and p are small and can, to first order, be neglected. (2) In the quasineutral regions n and p are reasonably constant. Solving Eq. (5.4) for condition (2) gives nT (t) as (ep + cn n)NT t t + 1 − exp − nT (t) = nT (0) exp − τ en + cn n + ep + cp p τ
(5.5)
where nT (0) is the density of GR centers occupied by electrons at t = 0 and τ = 1/(en + cn n + ep + cp p). The steadystate density as t → ∞ is nT =
ep + cn n NT en + cn n + ep + cp p
(5.6)
257
GENERATIONRECOMBINATION STATISTICS
This equation shows the steadystate occupancy of nT to be determined by the electron and hole densities as well as by the emission and capture rates. Equations (5.5) and (5.6) are the basis for most deeplevel impurity measurements. Equation (5.5) is difficult to solve because neither capture nor emission rates may be known. Furthermore, n and p vary with time and generally also with distance in a device. Certain experimental simplifications are usually made to allow data interpretation. We will show the results of those simplifications here and the experimental implementations later. For an ntype substrate where, to first order, p can be neglected, Equation (5.5) becomes (ep + cn n)NT t t + 1 − exp − (5.7) nT (t) = nT (0) exp − τ1 en + cn n + ep τ1 with τ1 = 1/(en + cn n + ep ). There are two cases of particular interest for the Schottky diode on an nsubstrate in Fig. 5.5. The diode is at zero bias in Fig. 5.5(a). With n mobile electrons, capture dominates emission, and the steadystate GR center density from Eq. (5.7) is nT ≈ NT . When the diode is pulsed from zero to reverse bias as shown in Fig. 5.5(b), with most GR centers initially occupied by electrons for t ≤ 0, electrons are emitted from the GR centers for t > 0. Emission dominates during this reversebias phase because the emitted electrons are swept out of the reversebiased spacecharge region very quickly, thereby reducing the chance of being recaptured. The electron sweepout or transit time is tt ≈ W/vn . For vn ≈ 107 cm/s and W being a few microns, tt is a few tens of picoseconds. This time is significantly shorter than typical capture times. However, near the edge of the scr the mobile electron density tails off into the scr from the quasineutral region even under reverse bias. This implies that the cn n term in Eq. (5.7) is
nT V=0 pT
+
ND
nType
+
+
−V1
−V1
+ W
W
+ + W
−V1
−V1 Ec ET Ev
(a)
(b)
(c)
C C (V = 0)
V −V1
C0
0
∆Ce
0
t
t
(d)
Fig. 5.5 A Schottky diode for (a) zero bias, (b) reverse bias at t = 0, (c) reverse bias as t → ∞. The applied voltage and resultant capacitance transient are shown in (d).
258
DEFECTS
not negligible in that part of the scr and electron emission competes with electron capture. With n not spatially homogeneous, τ is not constant, and the time dependence of n(t) can be nonexponential. Let us consider traps in the upper half of the band gap with en ≫ ep , allowing ep to be neglected in Eq. (5.7). During the initial emission period, the time dependence of nT simplifies to t t ≈ NT exp − (5.8) nT (t) = nT (0) exp − τe τe with τe = 1/en . Following electron emission from traps, holes remain and are subsequently emitted followed by electron emission, and so on. The steadystate trap density nT in the reversebiased scr is ep NT (5.9) nT = en + ep Some traps will be in the nT and some will be in the pT state. When the diode is pulsed from reverse bias to zero bias, electrons rush in to be captured by traps in the pT state. The time dependence of nT during the capture period is t (5.10) nT (t) = NT − (NT − nT (0)) exp − τc where τc = 1/cn n and nT (0) is the initial steadystate density given by Eq. (5.9). Similar equations to those in this section also hold for interface trapped charge. The relevant electron and hole densities are those at the surface, the traps are interface traps, and the capture and emission coefficients are those of the interface traps. The concepts, however, remain unchanged. 5.3
CAPACITANCE MEASUREMENTS
The equations in Section 5.2.2 describe the traps in terms of their densities and their emission and capture coefficients. With impurities being charged or neutral, and with electrons or holes emitted or captured, any measurement that detects charged species can be used for their characterization, i.e., capacitance, current, or charge measurements. We will first discuss capacitance measurements and later address the other two. The capacitance of the Schottky diode of Fig. 5.5 is qKs εo Nscr (5.11) C=A 2 Vbi − V where Nscr is the ionized impurity density in the spacecharge region. The ionized shallowlevel donors (dopant atoms) in the scr are positively charged and Nscr = ND + − n− T for deeplevel acceptor impurities that are negatively charged when occupied by electrons. When occupied by holes the deep level acceptors are neutral and Nscr = ND + . For shallowlevel donors and deeplevel donors occupied by electrons, Nscr = ND + . For deeplevel donors occupied by holes, Nscr = ND + + pT + . The timedependent capacitance reflects the time dependence of nT (t) or pT (t). Two chief methods are utilized to determine deeplevel impurities. In the first, the steadystate capacitance is measured at t = 0 and at t = ∞. In the second, the timevarying capacitance is monitored.
CAPACITANCE MEASUREMENTS
5.3.1
259
SteadyState Measurements
We saw in Chapter 2 that plots of 1/C 2 versus V yield the doping density. It is possible to determine NT from such plots. For shallowlevel donors and deeplevel acceptors 1/C 2 is given as 1 Vbi − V 1 = 2 (5.12) C2 K ND − nT (t) For the reversebiased diode of Fig. 5.5, nT (t) is negatively charged when occupied by electrons. With time, as electrons are emitted and the traps become neutral, (ND − nT (t)) increases and 1/C 2 decreases. In steadystate measurements the reversebiased capacitance at t = 0 is compared with the reversebiased capacitance as t → ∞. If we define a slope S(t) = −dV /d(1/C 2 ), then S(∞) − S(0) = K 2 [nT (0) − nT (∞)]
(5.13)
For nT (0) ≈ NT and nT (∞) ≈ 0, applicable for en ≫ ep , the difference of the two slopes gives the deeplevel impurity density. This method was used during early impurity measurements.8 A slightly more detailed analysis takes account of those traps with energy levels below the Fermi level.9 They do not emit and capture electrons as those levels above the Fermi level, perturbing the charge distributions somewhat, but is usually a minor effect. 5.3.2
Transient Measurements
Figure 5.5 shows the spacecharge region width W to change when electrons are emitted from traps. In transient measurements it is this timevarying W that is detected as a timevarying capacitance. From Eq. (5.11) nT (t) nT (t) qKs εo ND = C0 1 − 1− C=A 2(Vbi − V ) ND ND
(5.14)
where C0 is the capacitance of a device with no deeplevel impurities at reverse bias V . It is, of course, possible to measure C and analyze the data as C 2 to avoid taking the square root. We address that method at the end of this section. However, for the most common use of transient capacitance measurements, the deeplevel impurities form only a small fraction of the scr impurity density, i.e., NT ≪ ND . In other words, one is looking for trace amounts of impurities. Using a firstorder expansion of Eq. (5.14) gives nT (t) (5.15) C ≈ C0 1 − 2ND Emission—Majority Carriers: Carrier emission is most commonly measured. The junction device is initially zero biased, allowing impurities to capture majority carriers (Fig. 5.5(a)). The capacitance is the zerobiased value C(V = 0). Following a reverse bias pulse, majority carriers are emitted as a function of time (Fig. 5.5(b)). Equation (5.8) is the appropriate equation. When substituted into Eq. (5.15), we find t nT (0) exp − C = C0 1 − 2ND τe
(5.16)
260
DEFECTS
Equation (5.16) is shown in Fig. 5.5(d) for t > 0. The scr is widest and the capacitance is lowest immediately after the device is reverse biased. As majority carriers are emitted from the traps (Fig. 5.5(b)), W decreases and C increases until steady state is attained (Fig. 5.5(c)). In Fig. 5.5(c) holes remain on the traps. What happens, of course, is that after electrons are emitted, holes will be emitted, then electrons, and so forth. This is the leakage current of reversebiased diodes. Here we are only concerned with the initial electron emission to characterize the traps. The same time dependence of the capacitance is observed for deeplevel donor impurities in ntype substrates. In that case the impurities are neutral, when initially occupied by electrons, and the scr impurity density at t = 0+ is ND . As electrons are emitted, the traps become positively charged, and the final charge is q[ND + pT (∞)]. Both charge and capacitance increase with time. The capacitance increases with time regardless of whether the deeplevel impurities are donors or acceptors. Using the same arguments, it is straightforward to show that this is also true for ptype substrates with either donor or acceptor traps. The capacitance increases with time for majority carrier emission whether the substrate is n or ptype and whether the impurities are donors or acceptors. From the decay time constant of the Ct curve one derives τe and from the reversebiased capacitance change, one obtains nT (0). Defining Ce = C(t = ∞) − C(t = 0) we have nT (0) C0 (5.17) Ce = 2ND Plotting the capacitance difference t nT (0) C0 exp − C(∞) − C(t) = 2ND τe
(5.18)
as ln[C(∞) − C(t)] versus t, gives a curve with slope −1/τe and intercept on the lnaxis of ln[nT (0)C0 /2ND ]. The emission time constant contains parameters describing the trap. To bring these out, we have to return to the capture and emission coefficients. The capture and emission coefficients are related to each other through Eqs. (5.1) and (5.2). In equilibrium we invoke the principle of detailed balance, which states that under equilibrium conditions each fundamental process and its inverse must balance independent of any other process that may be occurring inside the material.10 – 11 This requires fundamental process (a) in Fig. 5.4 to selfbalance with its inverse process (b). Consequently dn/dt = 0 under equilibrium conditions and eno nT o = cno no pT o = cno no (NT − nT o )
(5.19)
where the subscript “o” stands for equilibrium. no and nT o are defined as10 no = ni exp((EF − Ei )/kT ); nT o =
NT 1 + exp((ET − EF )/kT )
(5.20)
Combining Eqs. (5.19) and (5.20) gives eno = cno ni exp((ET − Ei )/kT ) = cno n1 The derivation for holes gives an expression similar to Eq. (5.21).
(5.21)
CAPACITANCE MEASUREMENTS
261
Then a crucial assumption is made: the emission and capture coefficients remain equal to their equilibrium values under nonequilibrium conditions. This gives en = cn n1 ; ep = cp p1
(5.22)
n1 = ni exp((ET − Ei )/kT ); p1 = ni exp(−(ET − Ei )/kT )
(5.23)
where
The validity of the equilibrium assumption under nonequilibrium conditions is open to question. For small deviations from equilibrium, it may be assumed that the emission and capture coefficients do not deviate significantly from their equilibrium values.12 Certainly it is a poor approximation in the reversebiased junction scr where high electric fields exist, but that is precisely where most capacitance transient measurements are made. Capture crosssections determined from emission measurements generally do not give true crosssection values, as discussed in Appendix 5.1. The equilibrium assumption is nevertheless a common assumption, and any measured results are subject to this uncertainty. We show the electric field effect in Fig. 5.6. An electron energy diagram at zero electric field is shown by (1). An energy Ec − ET is required for electron emission from the trap to the conduction band. An applied electric field causes the bands to be slanted, as shown by (2), and the emission energy is reduced by the energy δE. PooleFrenkel emission over the lowered barrier is shown as (a).13 Even less energy is required for phononassisted tunneling, shown as (b), in which the electron is excited by phonons for only part of the energy barrier and then tunnels through the remaining barrier. As an example, the electric field dependence of the emission coefficient for the gold acceptor level in silicon is negligible for electric fields up to 104 V/cm, but for fields around 105 V/cm the emission coefficient increases by about a factor of two and continues to increase with higher fields.14 With en = 1/τe and cn = σn vth , the emission time constant is τe =
exp((Ec − ET )/kT ) exp((Ei − ET )/kT ) = σn vth ni σn vth Nc
(5.24)
(2) (1) EC
(a)
δE (b)
EC − ET
Fig. 5.6 Electron energy diagram in equilibrium (1) and in the presence of an electric field (2) showing fieldenhanced electron emission: (a) PooleFrenkel emission, (b) phononassisted tunneling.
262
DEFECTS
TABLE 5.1
Coefficients γn,p for Si and GaAs. γn,p (cm−2 s−1 K−2 )
Semiconductor
1.07 × 1021 1.78 × 1021 2.3 × 1020 1.7 × 1021
nSi pSi nGaAs pGaAs
A similar expression for holes is τe =
exp((ET − Ev )/kT ) exp((ET − Ei )/kT ) = σp vth ni σp vth Nc
(5.25)
where Nc and Nv are the effective conduction and valence band densities of state and the thermal velocities vth differ slightly for electrons and holes. The emission time constant τe depends on the energy ET and the capture crosssection σn . The emission time constants in Eqs. (5.24) and (5.25) are somewhat simplified. The energy differences Ec = (Ec − ET ) and Ev = (ET − Ev ) are actually Gibbs free energies G, that differ from E, discussed in Appendix 5.1. The electron thermal velocity is 3kT (5.26) vth = mn and the effective density of states in the conduction band is 2πmn kT 3/2 Nc = 2 h2
(5.27)
allowing the emission time constant to be written as τe T 2 =
exp((Ec − ET )/kT ) γn σn
(5.28)
with γn = (vth /T 1/2 )(Nc /T 3/2 ) = 3.25 × 1021 (mn /mo ) cm−2 s−1 K−2 , where mn is the electron densityofstates effective mass.15 – 16 The γ values for Si and GaAs17 are given in Table 5.1. Modified GaAs values γn = 1.9 × 1020 cm−2 s−1 K−2 and γp = 1.8 × 1021 cm−2 s−1 K−2 have been proposed, based on a critical evaluation of GaAs parameters.18
Exercise 5.1 Problem: What are typical emission times for impurities with energy levels in the semiconductor band gap? Solution: The emission time constant τe , given by Eq. (5.24), is plotted in Fig. E5.1, illustrating the large range of τe for a change in energy level E = Ec − ET .
CAPACITANCE MEASUREMENTS
263
105 T = 200 K
103
225 K
101 10−1 τe (s)
300 K
250 K 275 K
10−3 10−5 10−7 10−9 10−11
0
0.2
0.4
0.6
0.8
1
EC − E T (eV)
Fig. E5.1
Emission time constants for γn = 1.07 × 1021 cm−2 s−1 K−2 and σn = 10−15 cm2 .
108
τeT 2 (K 2·s)
107
Diode 4/Rh Diode 1/Au
106
105
104 0.004
Diode 5/Au Diode 4/Rh
0.006
0.008
0.01
1/T (K−1)
Fig. 5.7 τe T 2 versus 1/T plots for Si diodes containing Au and Rh. Reprinted with permission after Pals. Ref. 19.
A plot of ln(τe T 2 ) versus 1/T , has a slope of (Ec − ET )/k and an intercept on the ln(τe T 2 ) axis of ln[1/(γn σn )], leading to σn . Although this method of determining the capture crosssection is fairly common, the values so obtained should be viewed with caution. The crosssections are affected by the electric fields in the scr as well as by other effects discussed in Appendix 5.1. An example plot for Au and Rh in Si is shown in Fig. 5.7, whose ET and σ are shown in Table 5.2. The energy levels and the capture crosssections in Table 5.2 are determined from the intercept of the ln(τe T 2 ) versus 1/T lines and by another method—the filling pulse method that is described in the subsection “Capture—Majority Carriers”. Note the large discrepancy between the two methods, with the intercept method giving values at least ten times larger. There are various reasons for this large discrepancy. Electric field enhanced emission tends to give larger crosssections. As discussed in Appendix 5.1, the term (γn σn ) contains possible degeneracy factors and entropy terms, rendering the extrapolated crosssections questionable.
264
DEFECTS
TABLE 5.2 Energy Levels and Capture Cross Sections for the Diodes of Fig. 5.7. Diode
1 − p+ n 4 − p+ n 4 − p+ n 5 − n+ p
Ec − ET (eV)
Ec − ET (eV)
0.56 0.315 0.534 0.346
σn,p (intercept) (cm2 )
σn,p (filling pulse) (cm2 )
2.8 × 10−14 1.6 × 10−13 7.5 × 10−15 1.5 × 10−13
1.3 × 10−16 3.6 × 10−15 4 × 10−15 1.6 × 10−15
The time constant τe can also be determined by combining Eqs. (5.12), (5.13), and (5.8) as (5.29) S(∞) − S(t) = K 2 nT (t) = K 2 nT (0) exp(−t/τe ) and plotting ln[S(∞) − S(t)] versus t. This was one of the earliest approaches.9 However, the slope −dV /d(1/C 2 ) is more complex to measure with automatic equipment than just C, and the method of Eq. (5.29) is rarely used today. Yet, Eq. (5.29) does not entail a smallsignal expansion and is not subject to the limitation NT ≪ ND . Transient Ct data no longer follow a simple exponential time dependence when the emission rate is electric field dependent, when there are multiple exponentials due to several trapping levels with similar emission rates, and when the trap density is not negligibly small compared to the shallowlevel dopant density. The analysis becomes more complicated for the last case, and we do not derive the relevant equations. This problem has been treated elsewhere.20 – 23 Emission—Minority Carriers: The preceding section considered the capacitance response to majority carrier capture and emission when a Schottky diode is pulsed between zero and reverse bias. Similar results obtain when a pn junction is pulsed between zero and reverse bias. With the pn junction there is an additional option. Under forward bias, minority carriers are injected. Let us consider a p + n junction and neglect the p + region in this discussion. During the forwardbias phase, holes are injected into the nsubstrate and capture dominates emission. The steadystate GR center occupancy is from Eq. (5.6): nT =
cn n NT cn n + cp p
(5.30)
which depends on both capture coefficients and both carrier densities. The occupancy is difficult to predict, but the traps are no longer solely occupied by electrons as they are for the zero bias case; a certain fraction is occupied by holes. Schottky diodes do not inject minority carriers efficiently, and pn junctions should be used for electrical minority carrier injection. It is possible to inject minority carriers from highbarrierheight Schottky diodes with minority carrier storage at the inverted surface.24 – 25 For the sake of our discussion here, we assume cp ≫ cn and p ≈ n. Then most traps are occupied by holes and for the deeplevel acceptor impurities we have considered so far, the centers are neutral with nT ≈ 0 and Nscr ≈ ND at t = 0 after the junction has been forward biased. When pulsed to reverse bias, minority holes are emitted from the traps, their charge changes from neutral to negative, and Nscr ≈ (ND − nT ) for t → ∞. The total ionized scr density decreases, the scr width increases, and the capacitance decreases
CAPACITANCE MEASUREMENTS
265
C exp(−t/τe) = exp(−ent) Nscr = ND
exp(−t/τe) = exp(−ept) Nscr = ND
C0
Nscr = NDNT Nscr = ND − NT 0
Majority Carriers Minority Carriers
t
Fig. 5.8 The capacitancetime transients following majority carrier emission and minority carrier emission.
with time. This is shown in Fig. 5.8 and is opposite to majority carrier behavior. For simplicity, we assume in Fig. 5.8 all deeplevel impurities to be filled with electrons (majority carrier emission) or holes (minority carrier emission) at t = 0. The capacitance transient is still described by an expression of the type in Eq. (5.16), with the emission time constant now τe = 1/ep . Traps in the upper half of the band gap are generally detected with majority carrier pulses; those in the lower half of the band gap are observed with minority carrier pulses for ntype substrates. Traps with energies around the middle of the band gap can respond to either majority or minority carrier excitation. Minority carriers can also be injected optically as discussed later. Capture—Majority Carriers: Consider the Schottky diode of Fig. 5.5(c). It has been reverse biased sufficiently long that all majority carriers have been emitted and the traps are in the pT state. When the diode is pulsed from reverse bias (5.5(c)) to zero bias (5.5(a)), electrons rush into the scr to be captured by unoccupied traps. The density of traps able to capture majority carriers, for negligible emission, is given by nT (t) = NT − [NT − nT (0)] exp(−tf /τc )
(5.31)
where tf is the capture or “filling” time. If there is sufficient time, i.e., tf ≫ τc , essentially all traps capture electrons and nT (tf → ∞) ≈ NT . If the time available for electron capture is short, only a fraction of the traps will be occupied by electrons when the diode returns to reverse bias. In the limit of very short times, i.e., tf ≪ τc , very few electrons are captured and nT (tf → 0) ≈ 0. When the device is reverse biased, nT (0) in Eq. (5.16) is given by Eq. (5.31), with the initial density during the emission phase equal to the final density of the capture phase. The reversebias capacitance at t = 0 then depends on the filling pulse width, shown by substituting Eq. (5.31) into (5.16) to give NT − [NT − nT (0)] exp(−tf /τc ) t − tf C(t) = C0 1 − exp − 2ND τe Equation (5.32) is shown in Fig. 5.9(a).
(5.32)
266
DEFECTS
Capture 1 − exp(−t f /tc) (nT(0) = 0)
C
C
Emission Emission
C0
tf decreasing
C0
exp(−(t − t f )/te ) 0
tf
∆Cc t
(a)
t
tf (b)
Fig. 5.9 (a) Ct response showing the capture and initial part of the emission process, (b) the emission Ct response as a function of capture pulse width.
The capture time τc can be determined by varying tf , the filling pulse width. The capture time is usually much shorter than the emission time. We show the Ct curves during emission as a function of tf in Fig. 5.9(b). The capacitance at t = tf + is dependent on the capture time and is given by NT − [NT − nT (0)] exp(−tf /τc ) C(tf+ ) = C0 1 − 2ND
(5.33)
Equation (5.33) can be written as CC = C(tf ) − C(tf = ∞) =
tf NT − nT (0) C0 exp − 2ND τc
(5.34)
with Cc shown on Fig. 5.9(b). Then tf can be extracted from Eq. (5.34) by writing it as tf NT − nT (0) C0 − (5.35) ln(CC ) = ln 2ND τc A plot of ln(Cc ) versus tf has a slope of −1/τc = −σn vth n and an intercept on the ln(Cc ) axis of ln{[NT − nT (0)]C0 /2ND }, obtained by varying the capture pulse width during the capacitance transient measurement. In this manner the capture crosssection is determined from capture, not emission. Since capture times are much shorter than emission times, the instrumentation is more demanding. Modifications to capacitance meters to accommodate the necessary narrow pulses are given in ref. 26. Sometimes one obtains nonlinear ln(Cc ) versus tf plots due to slow capture from carrier tails extending into the scr. Models to derive σn from these curves are frequently too imprecise or involve complicated curve fitting routines, but are required for nonlinear experimental data.27 A variation on this method is not to measure the capacitance as a function of time, but instead to keep the capacitance constant during the measurement through a feedback circuit and measure the voltage required to keep the capacitance constant.28 – 29 The data analysis is similar and a plot of the voltage change V required to keep the capacitance constant shows the expected semilogarithmic behavior.
CURRENT MEASUREMENTS
267
Equation (5.31) gives the capture time as τc = (σn vth n)−1 . The actual trap filling process is more complicated because not all traps empty during the emission process. Those traps with energy levels below the Fermi level will tend to remain occupied by electrons during the emission transient29 and do not capture electrons during the filling pulse. This should be taken into account during the data analysis. Capture—Minority Carriers: There are several methods to determine the capture properties of minority carriers. One method is very similar to that of the previous section, except that during the filling pulse the diode is forward biased. Various pulse widths are used to determine the capture properties.26,30 – 31 Neglecting carrier emission, the capture time constant during the filling pulse is given by Eq. (5.5) as τc =
1 cn n + cp p
(5.36)
and the trap occupancy will be that of Eq. (5.30). It depends not only on n and p, but also on cn and cp . The injected minority carrier density is varied by changing the injection level, and both cn and cp can be determined.26 The narrow pulse widths (nanoseconds or lower) necessary to fill the centers partially are a decided disadvantage. A more fundamental limit is the turnon time of junction diodes, because they do not turn on instantly following a sharp pulse. The minority carrier density builds up in a time related to the minority carrier lifetime. For the narrow pulses required for the capture measurements, it is very likely that the minority carrier density does not reach its steadystate value. In an alternate method, the traps are populated with minority carriers not with constantamplitude, varyingwidth bias pulses, but with constantwidth, varyingamplitude pulses. The diode is forward biased with a long pulse, around 1 ms, and then reverse biased. The reversebias capacitance transient is observed. The minority carrier density is related to the injection current.26 One must pay attention that minority carrier recombination with majority carriers is not significant. It is also possible to inject minority carriers optically in pn junctions or Schottky diodes. We mention the method only briefly here and discuss it in more detail in Section 5.6.3. Consider a reversebiased pn junction or Schottky barrier diode. A light pulse with photon energy hν > EG is flashed on the device, creating electronhole pairs in the scr and in the quasineutral region. The minority carriers from the quasineutral region diffuse to the reversebiased spacecharge region to be captured by traps. With the light turned off, those captured minority carriers are emitted and detected as Ct or I t transients. From the transient one determines ET , σp , and NT .32
5.4
CURRENT MEASUREMENTS
The carriers emitted from traps can be detected as a capacitance, a charge, or a current.5,33 – 34 We saw earlier that the capacitance is given by Eq. (5.16). As the temperature changes, only the time constant changes; the initial capacitance step remains constant. For transient current measurements, the integral of the I t curve represents the total charge emitted by the traps. For high temperatures, the time constant is short, but the initial current is high. For low temperatures, the time constant increases and the current decreases, but the area under the I t curve remains constant. This makes current measurements difficult at low temperatures. By combining Ct measurements at the lower
268
DEFECTS
temperatures with I t measurements at the higher temperatures, it is possible to obtain time constant data over ten orders of magnitude.33 Current measurements are more complicated because the current consists of emission current Ie , displacement current Id , and junction leakage current I1 . The emission current is W dn dx (5.37) Ie = qA dt 0 The displacement current is5 Id = qA
0
W
dnT x dx dt W
(5.38)
The lower limit of the integral in Eqs. (5.37) and (5.38) should have been the zerobiased scr width. However, for simplicity we have set the lower limit to zero. With dn/dt ≈ en nT (Eq. (5.1)), dnT /dt ≈ −en nT (Eq. (5.4)), and electron emission dominating for the reversebiased diode of Fig. 5.4, we find I (t) =
qAW (t)en nT (t) qAW0 nT (t) + I1 = √ + I1 2 2τe 1 − nT (t)/ND
(5.39)
using W (t) =
2Ks εo (Vbi − V ) = q(ND − nT (t))
W0 2Ks εo (Vbi − V ) = √ qND (1 − nT (t)/ND ) 1 − nT (t)/ND
(5.40)
For nT ≪ ND and using Eq. (5.8), the current becomes I (t) =
nT (0) exp(−t/τe ) qAW0 + I1 2τe 1 − (nT (0)/2ND ) exp(−t/τe )
(5.41)
The interpretation of current measurements is more complex than capacitance measurements because the I t curve does not have a simple dependence on τe , i.e., τe appears in the numerator and the denominator of Eq. (5.41). If the second term in the denominator is small compared to unity for nT (0) ≪ 2ND and may be neglected, the current exhibits an exponential time dependence. The addition of the leakage current generally presents no problems since it is constant unless it is sufficiently high to mask the current transient. The instrumentation must be able to handle the large current transients during the pulse. The amplifier should be nonsaturable, or the large circuit transients must be eliminated from the current transient of interest. A circuit with these properties is described in ref. 26. Current transients do not allow a distinction between majority and minority carrier emission. Another feature of current measurements is a shift of the peak to higher temperatures relative to capacitance for the same rate window because the current is inversely proportional to the emission time constant (see Eq. (5.41)) while the capacitance is not. This property causes the current to increase very rapidly with temperature, effectively skewing the line shape toward higher temperatures. Current measurements are preferred when it is difficult to make capacitance measurements. For example, the low capacitance of smallgeometry MOSFETs or MESFETs is difficult to measure and the capacitance change is even smaller. In that case it is possible to detect the presence of deeplevel impurities by pulsing the gate voltage and monitoring
CHARGE MEASUREMENTS
269
ID
ID, CG
0.1 µA 10 fF
CG
0
150
300
T (K) Fig. 5.10 Drain current ID and gate capacitance CG transients of a 100 µm × 150 µm gate MESFET. Reprinted with permission after Hawkins and Peaker. Ref. 38.
the drain current as a function of time, known as conductance or current DLTS. Consider a MOSFET biased to some drain voltage and pulsed from accumulation to inversion, that is, from “off ” to “on”. Traps have captured majority carriers during the “off ” state. A spacecharge region is created when the device is turned “on” and drain current flows. As carriers are emitted from traps, the scr width and the threshold voltage change, causing a timedependent drain current.35 In constantresistance DLTS, the MOSFET conductance is applied as an input signal to a feedback circuit, providing the voltage to compensate for the charge loss from traps during emission.36 The mobility or transconductance need not be known. This technique is similar to the constant capacitance DLTS as it compensates for the emission of trapped carriers by adjusting the applied bias. Current measurements work best in devices in which the channel can be totally depleted. In a MESFET, for example, the gate is pulsed from zero to reverse bias, creating a deep spacecharge region. Electron or hole emission from traps changes the scr width and is measured as a drain current change that can be detected with the gate voltage held constant, or the gate voltage change can be detected with the current held constant through a feedback circuit.37 Examples of MESFET drain current and capacitance data are shown in Fig. 5.10.38 For these measurements it was necessary to use gate areas of 100 µm × 150 µm to obtain sufficiently large capacitances to be measurable. Drain current measurements are relatively simple to implement, but they are more difficult to interpret than capacitance measurements for trap density extraction because the current is a change in drain current brought about by a changing scr width. Interpretation of the data requires a knowledge of the mobility.39 This difficulty is circumvented by holding the drain current constant, changing the gate voltage, and converting gate voltage changes to current changes through the device transconductance.38
5.5
CHARGE MEASUREMENTS
Carriers emitted from traps can be detected directly as a charge with the circuit of Fig. 5.11. Switch S is closed to discharge the feedback capacitor CF . At t = 0 the diode is reverse biased, S is opened, and from Eq. (5.41), with the second term in the denominator
270
DEFECTS
S CF Diode Under Test
RF −
0
+
V o(t)
−V 1
Fig. 5.11
Circuit for charge transient measurements.
neglected, the current through the diode for t ≥ 0 is I (t) =
qAW0 nT (0) exp(−t/τe ) + I1 2τe
(5.42)
With the input current into the opamp approximately zero, the diode current must flow through the RF CF feedback circuit, giving the output voltage
V0 (t) =
t t t qAW0 RF nT (0) − exp − + I1 RF 1 − exp − exp − 2(tF − τe ) tF τe tF
(5.43) where tF = RF CF . Choosing the feedback network such that tF ≫ τe reduces Eq. (5.43) to t I1 t qAW0 nT (0) 1 − exp − + V0 (t) ≈ (5.44) 2CF τe CF Charge transient measurements have been implemented with the relatively simple circuit shown in Fig. 5.11.40 The integrator replaces the highspeed capacitance meter in Ct measurements or the highgain current amplifier in I t measurements. The output voltage depends only on the total charge released during the measurement and is independent of τe . Charge measurements can also be used for MOS capacitor characterization.41
5.6 5.6.1
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS) Conventional DLTS
The early Ct and I t measurements and methods were developed by Sah and his students.5,33 The initial implementation was timeconsuming and tedious because the measurements were singleshot measurements. The power of emission and capture transient analysis was only fully realized when automated data acquisition techniques were adopted. The first of these was Lang’s dualgated integrator or double boxcar approach named deeplevel transient spectroscopy (DLTS).42 – 43 Lang introduced the rate window concept to deep level impurity characterization. If the Ct curve from a transient capacitance experiment is processed so that a selected decay rate produces a maximum output, then a signal whose decay time changes monotonically
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
271
with time reaches a peak when the rate passes through the rate window of a boxcar averager or the frequency of a lockin amplifier. When observing a repetitive Ct transient through such a rate window while varying the decay time constant by varying the sample temperature, a peak appears in the capacitance versus temperature plot. Such a plot is a DLTS spectrum.44 – 45 The technique, which is merely a method to extract a maximum in a decaying waveform, applies to capacitance, current, and charge transients. We explain DLTS using capacitance transients. Assume the Ct transient follows the exponential time dependence t nT (0) exp − C(t) = C0 1 − 2ND τe
(5.45)
with τe depending on temperature as exp((Ec − ET )/kT ) γn σn T 2
τe =
(5.46)
T1
Temperature
Capacitance at Various Temperatures
The time constant τe decreases with increasing temperature, illustrated by the Ct curves in Fig. 5.12(a). The capacitance decay waveform is typically corrupted with noise, and the heart of DLTS is the extraction of the signal from the noise in an automated manner. The technique is a correlation technique, which is a signalprocessing method with the input signal multiplied by a reference signal, the weighting function w(t), and the product filtered
T
δCmax
0
t1
t2
Time (a)
δC = C(t1) − C(t2) (b)
Fig. 5.12 Implementation of the rate window concept with a double boxcar integrator. The output is the average difference of the capacitance amplitudes at sampling times t1 and t2 . Reprinted with permission after Miller et al.44
272
DEFECTS
(averaged) by a linear filter. The properties of such a correlator depend strongly on the weighting function and on the filtering method. The filter can be an integrator or a lowpass filter. The correlator output is δC =
1 T
0
T
f (t)w(t) dt =
C0 T
0
T
nT (0) t 1− w(t) dt exp − 2ND τe
(5.47)
where T is the period and we use Eq. (5.45) for f (t). Boxcar DLTS: Suppose that the Ct waveforms in Fig. 5.12(a) are sampled at times t = t1 and t = t2 and that the capacitance at t2 is subtracted from the capacitance at t1 , i.e., δC = C(t1 ) − C(t2 ). Such a difference signal is a standard output feature of a double boxcar instrument. The temperature is slowly scanned while the device is repetitively pulsed between zero and reverse bias. There is no difference between the capacitance at the two sampling times for very slow or for very fast transients, corresponding to low and high temperatures. A difference signal is generated when the time constant is on the order of the gate separation t2 − t1 , and the capacitance difference passes through a maximum as a function of temperature, as shown in Fig. 5.12(b). This is the DLTS peak. The capacitance difference, or DLTS signal, is obtained from Eq. (5.47), using the weighting function w(t) = δ(t − t1 ) − δ(t − t2 ), as t2 nT (0) t1 δC = C(t1 ) − C(t2 ) = C0 exp − − exp − (5.48) 2ND τe τe where T = t1 –t2 in Eq. (5.47). δC in Fig. 5.12(b) exhibits a maximum δCmax at temperature T1 . Differentiating Eq. (5.48) with respect to τe and setting the result equal to zero gives τe,max at δCmax as τe,max =
t2 − t1 ln(t2 /t1 )
(5.49)
Equation (5.49) is independent of the magnitude of the capacitance and the signal baseline need not be known. By generating a series of Ct curves at different temperatures for a given gate setting t1 and t2 , one value of τe corresponding to a particular temperature is generated, giving one datum point on a ln(τe T 2 ) versus 1/T plot. The measurement sequence is then repeated for another t1 and t2 gate setting for another point. In this manner, a series of points are obtained to generate an Arrhenius plot. δCt plots for t2 /t1 fixed, t1 and t2 varied are shown in Fig. 5.13. The effect of other t1 , t2 variations on δCt plots is discussed in Exercise 5.2. Example DLTS spectra of irondoped Si are shown in Fig. 5.14.46 As discussed in Chapter 7, iron forms FeB pairs in borondoped ptype Si with a DLTS peak at around T = 50 K. When the sample is heated at 180–200◦ C for a few minutes, the FeB pairs dissociate into interstitial iron and substitutional boron and the DLTS peak for the interstitial Fe occurs around T = 250 K. After a few days the interstitial iron again forms FeB pairs and the “T = 50 K” peak returns as shown in Fig. 5.14. Example DLTS spectra of Audoped Si samples are shown in Fig. 5.15 showing both majority and minority carrier peaks.47 The opposite polarity peaks correspond to the schematic diagrams in Fig. 5.8. The majority carrier peaks are measured with DLTS pulsed between zero and reverse bias. The minority carrier peaks are determined by optical minority carrier injection, where above band gap light, incident on the semitransparent Schottky diode, creates
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
273
0
δC (F)
−1 × 10−15 −2 × 10−15 −3 × 10
2 ms/4 ms 1 ms/2 ms
−15
t1 = 0.5 ms, t2 = 1 ms −4 × 10−15 200
250
350
300
400
Temperature (K)
Fig. 5.13 DLTS spectra for t2 /t1 fixed, t1 and t2 varied. Ec − ET 1 = 0.37 eV, σn1 = 10−15 cm2 , NT 1 = 5 × 1012 cm−3 , Ec − ET 2 = 0.6 eV, σn2 = 5 × 10−15 cm2 , NT 2 = 2 × 1012 cm−3 , C0 = 4.9 × 10−12 F , ND = 1015 cm−3 .
RT/5d
180°C/30s
−δC (f F )
60
40
Asis
20
180°C/30s Asis; RT/5d
0 50
100
150
200
250
300
Temperature (K)
Fig. 5.14 DLTS spectra for ironcontaminated Si wafer; “Asis”, after 180◦ C/30 s dissociation anneal, and room temperature storage for 5 days. Data after ref. 46.
DLTS Signal (a.u.)
0.4 0.2
Minority carrier peaks
0 Majority carrier peaks
−0.2 −0.4 100
150
200
250
Temperature (K)
Fig. 5.15 ref. 47.
Majority and minority carrier DLTS peaks for a Audoped Si sample. Adapted from
274
DEFECTS
electronhole pairs. The sampling or gate width should be relatively wide, because the signal/noise ratio is proportional to the square root of the gate width.45 Equation (5.49) then needs to be modified by changing t1 to (t1 + t) and t2 to (t2 + t) where t is the gate width.48
Exercise 5.2 Problem: What is the effect of varying the sampling times t1 and t2 ? Solution: The sampling times can be varied by: (1) t1 fixed, t2 varied (Fig. E5.2(a)); (2) t2 fixed, t1 varied (Fig. E5.2(b)); (3) t2 /t1 fixed, t1 and t2 varied (Fig. 5.14). Method (3) is best because the peaks shift with temperature with no curve shape change, making peak location easier. Additionally ln(t2 /t1 ) remains constant. For methods (1) and (2) the peaks change both in size and in shape. Alternatively, one can vary t2 t1 at a constant temperature with t2 /t1 constant. Then one would change the temperature and repeat to generate an Arrhenius plot from a single temperature scan. 0
δC (F)
−2 × 10 −15 −4 × 10 −15 0.5 ms/1 ms −6 × 10 −15 −8 × 10 −15
0.5 ms/2 ms t1 = 0.5 ms, t2 = 4 ms
−1 × 10 −14 200
250
300 350 Temperature (K)
400
(a) 0
δC (F)
−2 × 10 −15 −4 × 10 −15 −6 × 10 −15
2 ms/4 ms 1 ms/4 ms
−8 × 10 −15 −1 × 10
t1 = 0.5 ms, t2 = 4 ms
−14
200
250
300 350 Temperature (K)
400
(b)
Fig. E5.2 DLTS spectra for (a) t1 fixed, t2 varied, (b) t2 fixed, t1 varied. Ec − ET 1 = 0.37 eV, σn1 = 10−15 cm2 , NT 1 = 5 × 1012 cm−3 , Ec − ET 2 = 0.6 eV, σn2 = 5 × 10−15 cm2 , NT 2 = 2 × 1012 cm−3 , C0 = 4.9 × 10−12 F , ND = 1015 cm−3 .
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
275
The DLTS signal does not give the capacitance step Ce of Fig. 5.5 (δCmax < Ce ), and the impurity density cannot be determined from the DLTS signal using Eq. (5.17). The impurity density, derived from the maximum capacitance δCmax of the δCT curves, is given by NT =
δCmax 2r r/(r−1) δCmax 2ND exp{[r/(r − 1)] ln(r)} = ND C0 1−r C0 1−r
(5.50)
where r = t2 /t1 . Equation (5.50) is derived from Eqs. (5.48) and (5.49) with δCmax = δC, assuming nT (0) = NT . For r = 2, a common ratio, NT = −8ND δCmax /C0 , and for r = 10, NT = −2.87ND δCmax /Co . The minus sign accounts for the fact that δC < 0 for majority carrier traps. Wellmaintained DLTS systems can detect δCmax /C0 ≈ 10−5 to 10−4 , allowing trap densities on the order of (10−5 to 10−4 )ND to be determined. Highsensitivity bridges allow measurements as low as δCmax /C0 ≈ 10−6 .49 Capacitance meters often have response times of 1 to 10 ms and should be modified to allow faster transients to be measured. In addition, difficulties arise from overloads during device pulsing. Overload recovery delays are avoided by installing a fast relay that grounds the input of the amplifier during the pulse, deactivating the internal overload detection circuitry.50 Several refinements of the basic boxcar DLTS technique have been implemented. In the DoubleCorrelation DLTS (DDLTS) method, pulses of two different amplitudes are used instead of the oneamplitude pulse of the basic technique. However, DDLTS retains the conventional DLTS rate window concepts as shown in Fig. 5.16.51 The weighting function gives the signal [C ′ (t1 ) − C(t1 )] − [C ′ (t2 ) − C(t2 )] = C(t1 ) − C(t2 )
(5.51)
Capacitance
Bias Voltage
In the first correlation the transient capacitances after the two pulses are related to form the differences C(t1 ) and C(t2 ) at corresponding delay times after each pulse shown in Fig. 5.16. In a second step, the correlation [C(t1 ) − C(t2 )] is performed as in conventional DLTS to resolve the time constant spectrum during the temperature scan. The
C(t1)
C′(t1) C′(t2)
C(t2) Time
Fig. 5.16 Bias pulses and capacitance transients for double correlation DLTS. Reprinted with permission after Lef`evre and Schulz.51
276
DEFECTS
measurement requires either a fourchannel boxcar integrator or an external modification to a twochannel boxcar integrator.52 This added complexity sets an observation window within the spacecharge region, allowing the impurities within this spatial window to be detected. By setting the window well within the scr, away from the quasineutral region scr edge, all traps are well above the Fermi level, and the capacitance transient is due to emission only. Traps near the Fermi level are excluded from the measurement and all traps within the window experience approximately the same electric field. Trap density profiles are obtained by varying the observation window or by changing the pulse amplitudes or the dc reverse bias. Constant Capacitance DLTS: In Constant Capacitance DLTS (CCDLTS) the capacitance is held constant during the carrier emission measurement by dynamically varying the applied voltage during the transient through a feedback path.26,53 – 54 Miller pioneered the feedback method and applied it originally to carrier density profiling.55 Just as the transient capacitance contains the trap information in the constant voltage method, so the timevarying voltage contains the trap information in the constant capacitance method. The approximate capacitance transient expression in Eq. (5.15) is valid for NT ≪ ND . For NT > 0.1ND large changes occur in W and the Ct signal becomes nonexponential. Equation (5.14), which does not have this limitation, gives t qKs εo A N − n (0) exp − + Vbi (5.52) V =− D T 2C 2 τe valid for arbitrary NT because the scr width is held constant and the resulting voltage change is directly proportional to the change in scr charge. Equation (5.52) shows the V t response to be exponential in time. Sometimes a nonexponential portion to the V t curve occurs near t = 0, e.g., by carrier capture even during the emission phase of the measurement. The majority carrier density does not drop abruptly to zero at the scr edge but tails into the scr, and electron emission competes with electron capture in that tail region. Electron capture dominates at the scr edge and most of the traps remain filled with electrons, leading to a nonexponential V t curve.56 One of the limitations of CCDLTS is the slower circuit response due to the feedback circuits. An early implementation was limited to transients with time constants on the order of a second,57 that was reduced to about 10 ms for the same meter by using double feedback amplifiers.58 The response time was later further reduced and the sensitivity increased.59 However, feedback circuitry generally degrades the sensitivity of CCDLTS compared to Constant Voltage DLTS (CVDLTS). CCDLTS is well suited for trap density depth profiling.60 It has also been used for interface trapped charge measurements due to its highenergy resolution, and it permits more accurate DLTS measurements of defect profiles for high trap densities. Further refinements are possible by combining DDLTS with CCDLTS.61 Lockin Amplifier DLTS: Lockin amplifier DLTS is attractive because lockin amplifiers are more standard lab instruments than boxcar integrators,62 and they have a better signal/noise ratio than boxcar DLTS.63 Lockin amplifiers use a square wave weighting function whose period is set by the frequency of the lockin amplifier. A DLTS peak is observed when this frequency bears the proper relationship to the emission time constant. A lockin amplifier can be thought of as a onecomponent Fourier analyzer to analyze a repetitive signal. The weighting function resembles that of a boxcar integrator but is wider, increasing the signal/noise ratio but also posing an overload problem.
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
277
The device junction capacitance is very high during the forwardbiased phase and tends to overload the relatively slow (response time ∼1 ms unless modified) capacitance meter. A lockin amplifier is very sensitive to the meter transient and overloads easily since its square wave weighting function has unit amplitude at all times. The boxcar does not have this problem because the first sampling window is delayed past the initial transient. The lockin amplifier sensitivity to overloads can be reduced by preceding the weighting function by a narrowband filter. This leads to an approximate sinusoidal weighting function. A better solution is to gate off the first 1 to 2 ms of the capacitance meter output, eliminating the overloading problems.48,64 The analysis of the lockin amplifier signal must include this gateoff time. The gateoff time also affects the base line which may become nonzero after the signal is suppressed part of the time.65 The phase setting also affects the signal.66 Details of three basic modes of lockin DLTS operation and the relevant precautions to observe are discussed in ref. 48. Choosing a gateoff time that is always the same fraction of the repetition rate avoids problems of erroneous DLTS peaks.67 The details of a lockin amplifierbased DLTS system are given by Rohatgi et al.64 For the weighting function w(t) = 0 for 0 ≤ t < td , w(t) = 1 for td < t < T /2, w(t) = −1 for T /2 < t < (T − td ), and w(t) = 0 for (T − td ) < t < T , the output from the lockin amplifier is63 δC = −
T − 2td 2 td GC0 nT (0) τe 1 − exp − exp − ND T τe 2τe
(5.53)
where G is the lockin amplifier and capacitance meter gain, T is the pulse period, and the delay time td is the interval between the end of the bias pulse and the end of the holding interval. Equation (5.53) exhibits a maximum, similar to that of Eq. (5.48). Differentiating Eq. (5.53) with respect to τe and setting the result equal to zero allows τe,max to be determined from the transcendental equation 1+
td τe,max
T − 2td T − td exp − = 1+ τe,max 2τe,max
(5.54)
For a typical delay time of td = 0.1T , τe,max = 0.44T . A ln(τe T 2 ) versus 1/T plot is generated as described in the previous section once pairs of τe and T are known. The trap density, derived from Eqs. (5.53) and (5.54) for δC = δCmax under the assumption that nT (0) = NT and td = 0.1T , is given by NT =
8δCmax ND . C0 G
(5.55)
Instead of holding the lockin frequency constant and varying the sample temperature, it is also possible to keep the temperature constant and vary the frequency.68 Correlation DLTS: Correlation DLTS is based on optimum filter theory, which states that the optimum weighting function of an unknown signal corrupted by white noise has the form of the noisefree signal itself. This can be implemented in DLTS by multiplying the exponential capacitance or current waveforms by a repetitive decaying exponential generated with an RC function generator and integrating the product.63 Correlation DLTS has a higher signal/noise ratio than either boxcar or lockin DLTS.69 Since the small capacitance transient rides on a dc background, it is not sufficient to use a
278
DEFECTS
simple exponential because the weighting function and baseline restoration are required.70 The method has not found much application, but it has been used to study impurities in highpurity germanium.71 Isothermal DLTS: In the isothermal DLTS method, the sample temperature is held constant and the sampling time is varied.72 The technique is also based on Eq. (5.45), repeated here t nT (0) exp − (5.56) C(t) = C0 1 − 2ND τe Differentiating this expression and multiplying by time t, gives t
t nT (0) dC(t) t =− C0 exp − dt τe 2ND τe
(5.57)
The function t dC(t)/dt plotted versus t has a maximum value (nT (0)C0 /2ND )(1/e) at t = τe . Generating a series of t dC(t)/dt versus t plots at several constant temperatures allows an Arrhenius plot of ln(τe T 2 ) versus 1/T , similar to a conventional DLTS plot. The chief difference is the constancy of the temperature during the measurement, easing the requirements on the temperature control/measurement. Instead, the measurement difficulty shifts to the time domain, where C(t) measurements have to be made over a wide time range, requiring fast capacitance meters. Differentiating may introduce additional “noise” into the data. A plot of t dC(t)/dt versus t for the same data as Fig. 5.13, is shown in Fig. 5.17. Note the close correspondence between the temperature dependence and the time dependence of the capacitance signal. Computer DLTS: Computer DLTS refers to DLTS systems in which the capacitance waveform is digitized and stored electronically for further data management.73 One temperature sweep of the sample is sufficient since the entire Ct curve is obtained at each of a number of different temperatures. It is readily established whether the signal is exponential; this is not possible with the boxcar or lockin methods since those methods only
0
tdC/dt (F)
−1 × 10−15 −2 × 10−15 T = 325 K −3 × 10−15 −4 × 10−15
T = 300 K T = 275 K
−5 × 10−15 10−7 10−6 10−5 10−4 10−3 10−2 10−1 100 Time (s)
Fig. 5.17 DLTS spectra for T fixed, t varied. Ec − ET 1 = 0.37 eV, σn1 = 10−15 cm2 , NT 1 = 5 × 1012 cm−3 , Ec − ET 2 = 0.6 eV, σn2 = 5 × 10−15 cm2 , NT 2 = 2 × 1012 cm−3 , C0 = 4.9 × 10−12 F , ND = 1015 cm−3 .
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
279
give maxima at selected temperatures but lose the waveform itself. Various signal processing functions can be applied to the Ct data: fast Fourier transforms, the method of moments to analyze simple and multiple exponential decays,74 – 76 Laplace transform,77 spectroscopic line fitting,78 the covariance method of linear predictive modeling,79 linear regression,80 and an algorithm allowing the separation of closely spaced peaks.81 One implementation uses a pseudo logarithmic sample storage scheme allowing 11 different sampling rates and 3–5 decades of time constants to be taken, that can separate closely spaced deep levels, where conventional DLTS fails.82 Laplace DLTS: There are two broad DLTS categories: analog and digital signal processing. Analog signal processing is done in real time as the sample temperature is ramped, choosing only one or two decay components at a time with filters producing an output proportional to the signal within a particular time constant range, by multiplying the capacitance meter output signal by a timedependent weighting function. Digital schemes digitize the analog transient output of the capacitance meter and averaging many digitized transients to reduce the noise level. The time constant resolution of conventional DLTS is too poor for studying fine structure in the emission process due to the filter rather than thermal broadening. Even a perfect defect produces a broad line on the DLTS spectrum due to instrumental effects. Any emission time constant variation results in additional peak broadening. Some improvement in resolution is possible by changing the filter characteristic.77 A common approach to the quantitative description of nonexponential behavior in the capacitance transients is to assume that they are characterized by a spectrum of emission rates ∞ F (s)e−st ds (5.58) f (t) = 0
where f (t) is the recorded transient and F (s) is the spectral density function.77 For simplicity, this spectrum is sometimes represented by a Gaussian distribution overlaying the logarithmic emission rate scale. In this way it is possible to describe the nonexponential transient in terms of broadening of the emission activation energy. A mathematical representation of the capacitance transients given by Eq. (5.58) is the Laplace transform of the true spectral function F (s). To find a real spectrum of the emission rates in the transient it is necessary to use an algorithm that effectively performs an inverse Laplace transform for the function f (t), yielding a spectrum of deltalike peaks for multi, monoexponential transients, or a broad spectrum with no fine structure for continuous distribution. It is not necessary to make any a priori assumptions about the functional shape of the spectrum, except that all decays are exponential in the same direction. Laplace DLTS (LDLTS) gives an intensity output as a function of emission rate. The area under each peak is directly related to the initial trap concentration. The measurement is carried out at a fixed temperature, and several thousand capacitance transients are captured and averaged. LDLTS can provide an order of magnitude higher energy resolution than conventional DLTS techniques, provided a good signaltonoise ratio exists. In practice this limits the application to cases where the defect density is 5 × 10−4 to 5 × 10−2 of the shallow donor or acceptor density. Given these limitations, LDLTS enables a range of measurements which are not practical in other systems. It is very important to reduce all noise contributions. For example, it is very important to use very stable power supplies and pulse generators. An obvious application of LDLTS is to separate states with very similar emission rates. The poor resolution of conventional DLTS has resulted in considerable confusion over
Spectral Density Function
DEFECTS
DLTS Signal
280
200
240
280
320
Temperature (K) (a)
T = 260 K 1
10
100
Emission Rate
1000
(s−1)
(b)
Fig. 5.18 (a) DLTS and (b) Laplace DLTS spectra of hydrogenated silicon containing gold. The DLTS peak is attributed to electron emission from the gold acceptor and goldhydrogen levels. The Laplace spectrum clearly separates the goldacceptor level and the goldhydrogen. Adapted from Deixler et al.83
the “identity” of particular DLTS fingerprints. Using conventional DLTS, it is sometimes possible to separate states with very similar emission rates, provided they have different activation energies, by conducting the DLTS experiment over a very wide range of rate windows. An example is shown in Fig. 5.18. Figure 5.18(a) gives a conventional DLTS peak of gold in Si. This sample was hydrogen annealed and there should be a hydrogengold peak, which is not obvious, however. The LDLTS spectrum, which is a plot of spectral density function versus emission rate, in Fig. 5.18(b) clearly shows two distinct peaks.83 Knowing the emission rate allows the energy level to be determined. Laplace DLTS has been used for Ptdoped Si, EL2 in GaAs, and DX defects in AlGaAs, GaSb, GaAsP, and δdoped GaAs.84 In each case the standard DLTS gave featureless peaks while the Laplace DLTS spectra revealed the fine structure in the thermal emission process. 5.6.2
Interface Trapped Charge DLTS
The instrumentation for interface trapped charge DLTS is identical to that for bulk deeplevel DLTS. However, the data interpretation is different because interface traps are continuously distributed in energy through the band gap, whereas bulk traps have discrete energy levels. We illustrate the interface trapped charge majority carrier DLTS concept for the MOS capacitor (MOSC) in Fig. 5.19(a). For a positive gate voltage electrons are captured and most interface traps are occupied by majority electrons for nsubstrates (Fig. 5.19(b)). A negative gate voltage drives the device into deep depletion, and electrons are emitted from interface traps (Fig. 5.19(c)). The emitted electrons give rise to a capacitance, current, or charge transient. Although electrons are emitted over a broad energy spectrum, emission from interface traps in the upper half of the band gap dominates. DLTS is very sensitive, allowing interface trap density determination in the mid 109 cm−2 eV −1 range. Interface trap characterization by DLTS was first implemented with MOSFETs.85 MOSFETs, being threeterminal devices, have an advantage over MOS capacitors (MOSCs). By reverse biasing the source/drain and pulsing the gate, majority electrons are captured and emitted without interference from minority holes that are collected by the sourcedrain.
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
Ec
281
EF
Ev
(a)
V G2
V G1
(b)
Fig. 5.19
(c)
(a) Majority carrier capture and (b) majority carrier emission from interface traps.
This allows interface trap majority carrier characterization in the upper half of the band gap. With the sourcedrain forward biased, an inversion layer forms, allowing interface traps to be filled with minority holes. Minority carrier characterization is then possible and the lower half of the band gap can be explored. This is not possible with MOSCs because there is no minority carrier source. When an inversion layer does form through thermal ehp generation, especially at higher temperatures and at high ehp generation rates, it can interfere with majority carrier trap DLTS measurements. MOS capacitors are, nevertheless, used for interface trap characterization.53,86 – 87 Unlike the conductance technique discussed in Chapter 6, DLTS measurements are independent of surface potential fluctuations. The derivation of the capacitance expression is more complex for MOSCs than it is for diodes. We quote the main results whose derivations can be found in Johnson54 and Yamasaki et al.87 For q 2 Dit = Cit ≪ Cox and δC = Chf (t1 ) − Chf (t2 ) ≪ Chf δC =
3 Chf
Ks εo ND Cox
∞
−∞
where τe =
Dit (e−t2 /τe − e−t1 /τe ) dEit
e(Ec −Eit )/kT γn σn T 2
(5.59)
(5.60)
Eit is the energy of the interface traps. The maximum emission time is τe,max = (t2 − t1 )/ ln(t2 /t1 ) from Eq. (5.49). In conjunction with Eq. (5.60) where τe,max corresponds to Eit,max , we find, when the electron capture crosssection is not a strong function of energy, γn σn T 2 (t2 − t1 ) Eit,max = Ec − kT ln (5.61) ln(t2 /t1 )
282
DEFECTS
where Eit,max is sharply peaked. If Dit varies slowly in the energy range of several kT around Eit,max , it can be considered reasonably constant and can be taken outside the integral of Eq. (5.59). The remaining integral becomes
∞
−∞
(e−t2 /τe − e−t1 /τe ) dEit = −kT ln(t2 /t1 )
(5.62)
allowing Eq. (5.59) to be written as δC ≈
3 Chf
Ks εo ND Cox
kT Dit ln(t2 /t1 )
(5.63)
From Eq. (5.63) the interface trap density is Dit = −
Ks εo ND Cox δC 3 kT Chf ln(t2 /t1 )
(5.64)
determined from electrons emitted from interface traps in time (t2 − t1 ) in the energy interval E = kT ln(t2 /t1 ) at energy Eit,max . A plot of Dit versus Eit is constructed by varying t1 and t2 . For each t1 ,t2 combination, an Eit is obtained from Eq. (5.60) and a Dit from Eq. (5.64). If the sample contains bulk as well as interface traps, it is possible to differentiate bulk traps from interface traps by the shape and the peak temperature of the DLTS plot.87 For the constant capacitance DLTS technique an equation analogous to Eq. (5.64) is54 Dit =
Cox VG qkT A ln(t2 /t1 )
(5.65)
where A is the device area and VG is the gate voltage change required to keep the capacitance constant. Equation (5.65) is easier to use than (5.64) because neither the highfrequency capacitance nor the doping density need be known. Figure 5.20 shows the interface trap distribution for nSi, with Dit measured by the quasistatic and the
6 × 1010
D it (cm−2eV−1)
5 × 1010 4 × 1010 Quasistatic CV
3 × 1010 2 × 1010 1 × 1010 00
CCDLTS
0.1
0.2 0.3
0.4
0.5
0.6
0.7
0.8
E c−E (eV)
Fig. 5.20 Interface trapped charge density for nSi measured by the CCDLTS and quasistatic methods. Reprinted with permission after Johnson et al. Ref. 88.
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
283
CCDLTS technique.88 The discrepancy between the two curves may be due to the assumption of constant capture crosssections in the DLTS analysis. MOS capacitors can also be measured by the current DLTS method. Using the small pulse method,89 in which pulses of tens of millivolts are used, both interface trap density and capture crosssections can be measured.90 Small filling pulses are applied as the quiescent bias is scanned at constant temperature and constant rate window. As the Fermi level scans the band gap, a DLTS peak is observed when τe in a small energy region around the Fermi level matches the rate window. Varying the rate window or the temperature gives the interface trap distribution. 5.6.3
Optical and Scanning DLTS
Optical DLTS comes in various implementations. Light can be used (1) to determine optical properties of traps, such as optical capture crosssections, (2) to create electronhole pairs for minority carrier injection, and (3) to create ehps in semiinsulating materials, where electrical injection is difficult. Light does two basic things: it imparts energy to a trapped carrier, causing its emission from a trap to the conduction or to the valence band, and it changes n and/or p by creating ehps, thereby changing the capture properties of the center. An electron beam in a scanning electron microscope also creates ehps and can be used for DLTS measurements. Optical Emission: For conventional majority carrier emission, a Schottky diode on an ntype substrate is zero biased and traps are filled with electrons at low temperatures. Instead of raising the temperature and detecting the capacitance or current transient due to thermal emission, the sample is held at a sufficiently low temperature for negligible thermal emission. Light is shone on the sample provided with a transparent or semitransparent contact. For hν < (Ec − ET ) there is no band gap optical absorption. For hν > Ec − ET photons excite electrons from the traps into the conduction band. Equation (5.8) holds, but the emission rate en becomes en + en o , where en o is the optical emission rate en o = σn o , with σn o the optical capture crosssection and the photon flux density. The trap density is obtained from the capacitance step just as it is during thermal emission measurements. The light is used in these experiments to determine optical trap properties, such as the optical crosssection, using either capacitance or current transients.30,91 – 93 It is possible to determine the multiplicity of charge states by varying the energy of the incident light. For a center with two donor levels, for example, one increases the light energy to excite electrons from the upper level into the conduction band, detected by a capacitance change. Increasing the energy further leaves the capacitance unchanged, provided all electrons have been excited out of that level, until the energy is sufficient to excite electrons from the second level into the conduction band, giving a second capacitance rise. This has been used to determine the doubledonor nature of sulfur in silicon.94 In the twowavelength method, a steadystate, above band gap background light creates a steadystate population of holes on traps below the Fermi level and of electrons on traps above the Fermi level. A variableenergy probe light excites carriers from the traps into either of the bands while the junction is pulsed electrically,95 or ehps are generated optically by above bandgap light.96 Both electrons and holes can be captured by traps in the scr. When the light is turned off, the carriers are thermally emitted. In this method, the light merely generates ehps; the transient is due to thermal emission. Other optical techniques were mentioned earlier when we discussed the use of light to generate ehps for the measurement of the minority carrier capture crosssections.26,32
284
DEFECTS
Photoinduced Current Transient Spectroscopy: The optical techniques of the previous section supplement electrical measurements. Although the measurements can generally be done electrically, the optical input makes the measurement easier (minority carrier generation) or gives additional information (optical crosssection). But purely electrical measurements are difficult in highresistivity or semiinsulating substrates, e.g., GaAs and InP. Optical inputs can then be a decided advantage and in some cases are the only way to obtain information of deep level impurities. In the photoinduced current transient spectroscopy (PITS or PICTS) method the current is measured as a function of time. The sample is provided with a top semitransparent ohmic contact. Capacitance cannot be measured because the substrate resistance is too high. During the PITS measurement light is pulsed on the sample, and the photocurrent rises to a steadystate value. The light pulse can have above bandgap or below bandgap energy.97 The photocurrent transient at the end of the light pulse consists of a rapid drop followed by a slower decay. The initial rapid drop is due to ehp recombination and the slow decay is due to carrier emission. The slow current transient can be analyzed by DLTS rate window methods.98 It is sometimes possible to determine whether the level is an electron or a hole trap by measuring the peak height as the bias polarity is changed. However, this identification is not as simple as it is for capacitance transients. For electron traps and sufficient light intensity to saturate the photocurrent, the transient current is99 CNT δI = exp(−t/τe ) (5.66) τe where C is a constant [see Eq. (5.42)]. When plotted against temperature, δI exhibits a maximum for t = τe as determined by differentiating Eq. (5.66) with respect to temperature, KNT dτe d(δI ) = (5.67) (t − τe ) exp(−t/τe ) dT τe3 dT and setting Eq. (5.67) equal to zero. PITS is not well suited for trap density determination, and the reliability of information extracted from the data for trap identification falls off as the trap energy approaches the intrinsic Fermi level.108 Additional complications occur when carriers emitted from traps recombine. The recombination lifetime for semiinsulating materials is usually quite low. In addition, emitted carriers can be retrapped. All of these effects make the method difficult to use.100 Unfortunately, there are few techniques other than PITS to characterize such materials. Scanning DLTS: Scanning DLTS (SDLTS) uses a scanning electron microscope electron beam as the excitation source. The high spatial resolution—in the micron range—is its main advantage, but also one of its disadvantages because such a small sampling area produces very small DLTS signals. For conventional DLTS the diode diameter is typically in the 0.5 to 1 mm range, and the entire area is active during the measurement. For SDLTS the diode diameter is similar, giving rise to a large steadystate capacitance. But the emissionactive area, defined by the electron beam diameter, can be much smaller and gives very small capacitance changes. The original SDLTS used current DLTS because it can be more sensitive than capacitance DLTS.101 Equation (5.41) shows the current to be inversely proportional to the emission time constant. As T increases, τe decreases, and hence I increases. Later developments of an extremely sensitive capacitance meter with 10−6 pF sensitivity, consisting of a resonancetuned LC bridge at 28 MHz with
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
285
permanent slow automatic zero balance to ensure operation in a tuned state at all times, allowed capacitance DLTS measurements.102 Quantitative measurements are difficult to implement in SDLTS,103 but one can map a distribution of a particular impurity by scanning the device area, choosing an appropriate temperature and rate window. A few hundred impurity atoms per scanning point have been detected.104 5.6.4
Precautions
Leakage Current: Several measurement precautions have already been mentioned throughout this chapter. Here we point out a few more. Devices sometimes exhibit high reversebias leakage currents. During DLTS measurements of leaky MOS capacitors, the DLTS peak amplitude decreases much more strongly with slower rate windows than expected. This was attributed to competition between carrier capture due to leakage current and thermal emission. The thermal emission rate then becomes an apparent rate given by en,app = en + cn n
(5.68)
We can write the leakage current density as Jleak = qnv =
qnvcn qncn qnvcn = ≈ cn σn vth σn
(5.69)
assuming v ≈ vth . Substituting Eq. (5.69) into Eq. (5.68) gives en,app = en +
Jleak σn q
(5.70)
If we assume the leakage current to be of the form105 Jleak = qA∗ T 2 e−EA /kT
(5.71)
then Eq. (5.28) becomes τe T 2 =
exp((Ec − ET )/kT ) σn γn (1 − (A∗ /γn ) exp((Ec − ET − EA )/kT ))
(5.72)
If Eq. (5.72) applies, errors in the trap energy and capture crosssection extracted from an Arrhenius plot will result.105 For leaky diodes, an experimental system with two diodes, having similar C –V and I –V characteristics, is driven 180◦ out of phase.106 Series Resistance: Another device anomaly that can affect the DLTS response is the device series resistance and parallel conductance. A pn or Schottky diode consisting of junction capacitance C, junction conductance G, and series resistance rs in Fig. 5.21(a). Capacitance meters assume the device to be represented by either the parallel equivalent circuit in Fig. 5.21(b) or the series equivalent circuit in Fig. 5.21(c). CP and CS can be written as C C G 2 (5.73) ≈ ; CS = C 1 + CP = (1 + rs G)2 + (ωrs C)2 1 + (ωrs C)2 ωC
286
DEFECTS
G
C
GP
CS
CP
RS rs
(a)
(b)
(c)
Fig. 5.21 (a) Actual circuit, (b) parallel equivalent circuit, and (c) series equivalent circuit for a pn or Schottky diode.
where ω = 2πf and the “rs G” term in the denominator was neglected in the approximate expression. A DLTS measurement records the change in capacitance given by 2(ωrs C)2 C G 2 (5.74) 1− ; CS = C 1 − CP = 1 + (ωrs C)2 1 + (ωrs C)2 ωC where CP depends on rs and CS depends on G. For rs = 0 and G = 0, CP = CS = C. However, as rs increases, CP decreases. CP and the DLTS signal can become zero and even reverse sign and majority carrier traps can be mistaken for minority carrier traps.78,107 Similarly, as G increases, CS decreases and can also become negative. If series resistance is anticipated to be a problem, one can insert additional external resistance into the circuit and check for sign reversal.108 If sign reversal is not observed, there is a good chance that it has already taken place without any additional external resistance, and the measured data must be carefully evaluated. Occasionally an additional capacitance is introduced by an oxide layer at the back of the sample, which can also lead to DLTS signal reversal.109 Series resistance is not a particular problem for current DLTS because it is essentially a dc measurement, not requiring the high probe frequency of capacitance DLTS. Instrumentation Considerations: The temperature of the sample has to be precisely controlled and measured for precise energy level extraction. Temperature control and measurement to 0.1 K is desirable. That is not always easy to do, since the thermocouple or diode used for temperature measurements is usually located in a heat sink block away from the sample under test. The capacitance meter should be sufficiently fast to be able to follow the smallest transient of interest. For some instruments it is necessary to block the large capacitance during the filling pulse to prevent instrument overload. A good discussion of instrument considerations is given in ref. 43. Incomplete Trap Filling: We have assumed that all traps fill with majority carriers during the capture time and emit majority carriers during the emission time. That is only an assumption as illustrated with the band diagram in Fig. 5.22.110 For the zerobiased device in Fig. 5.22(a), traps within W1 do not fill because they are above the Fermi level;
DEEPLEVEL TRANSIENT SPECTROSCOPY (DLTS)
Ec ET
287
EF
Ev W1 (a)
−V1
(b)
−V1
l W2 (c)
Fig. 5.22 Band diagram for a Schottky diode on an nsubstrate. (a) Diode at zero bias during the filling phase, (b) immediately after the reverse bias pulse, (c) steadystate reverse bias.
those traps to the right of W1 , but near W1 , fill more slowly than those further to the right because the electron density tails off. Consequently, for narrow filling pulses, not all traps to the right of W1 become occupied by electrons. When the bias switches to reverse bias, Fig. 5.22(b), electrons are emitted. However, those traps within λ do not emit electrons because they are below the Fermi level (Fig. 5.22(c)), where W2 is the final scr width and λ is given by45 λ=
2Ks εo (EF − ET ) q 2 ND
(5.75)
Only those traps within (W W1 λ) participate during the DLTS measurement.111 W1 is almost always neglected; frequently λ is neglected too. When λ is not neglected, the capacitance step Ce of Eq. (5.17) becomes45,112 Ce =
nT (0) C0 f (W ) 2ND
(5.76)
288
DEFECTS
where f (W ) = 1 −
(2λ/W (V ))(1 − C(V )/C(0) 1 − [C(V )/C(0)]2
(5.77)
C(0) and C(V ) are the capacitances at voltages zero and V , respectively. If the edge region can be neglected, f (W ) becomes unity. However, with f (W ) < 1, neglecting the edge region can introduce appreciable error.113 Blackbody Radiation: The usual assumption is that the device is in the dark during DLTS measurements. This is true if the device is encapsulated with the case at the measurement temperature. If, however, the device is in wafer form and it “sees” a part of the dewar at a temperature higher than the measurement temperature, e.g., room temperature, it is possible for photons in the blackbody radiation spectrum to cause optical emission to add to thermal emission and give erroneous activation energies. If this is a concern, it is experienced at low temperatures and at low scanning rates.114
5.7
THERMALLY STIMULATED CAPACITANCE AND CURRENT
Thermally stimulated capacitance (TSCAP) and current (TSC) measurements were popular before DLTS. The techniques were originally used for insulators and later adapted to lower resistivity semiconductors when it was recognized that the reversebiased scr is a region of high resistance.115 During the measurement the device is cooled and the traps are filled with majority carriers at zero bias or traps can be filled with minority carriers by optical injection or by forward biasing a pn junction. Then the device is reverse biased, heated at a constant rate, and the steadystate capacitance or current is measured as a function of temperature. Capacitance steps or current peaks are observed as traps emit their carriers, shown in Fig. 5.23. The temperature of the TSC peak or the midpoint of the TSCAP step Tm is related to the activation energy E = Ec − ET or E = ET − Ev by116 γn σn kTm4 E = kTm ln β(E + 2kTm )
Minority Carrier Emission
(5.78)
Current
Capacitance
Majority Carrier Emission Tm1
Tm2
Tm1
Tm2
Temperature
Temperature
(a)
(b)
Fig. 5.23 Schematic of (a) TSCAP and (b) TSC for a sample with a majority carrier trap of density NT and a shallower minority carrier trap of density 2NT . The current increase at higher temperatures is due to thermally generated current. Reprinted with permission after Lang. Ref. 45.
POSITRON ANNIHILATION SPECTROSCOPY (PAS)
289
0.25
20
0.2 TSC 0.15
10 0.1 5
0
Current (nA)
Capacitance (fF)
DLTS 15
0.05
0
50
100
150
200
250
0 300
Temperature (K)
Fig. 5.24 DLTS and TSC data for high resistivity silicon. Reprinted from ref. 117 with kind permission from Elsevier ScienceNL, Burgerhartsraat 2S, 1055 KV Amsterdam, The Netherlands.
For ptype samples the subscript n should be replaced by p. The trap density is obtained from the area under the TSC curve or from the step height of the TSCAP curve. The equipment is simpler than that for DLTS, but the information obtained from TSC and TSCAP is more limited and more difficult to interpret. The thermally stimulated techniques allow a quick sweep of the sample to survey the entire range of traps in a sample and work well for NT ≥ 0.1ND and E ≥ 0.3 eV. The TSC peaks depend on the heating rate, but the TSCAP steps do not. TSC is influenced by leakage currents. TSCAP allows discrimination between minority and majority carrier traps by the sign of the capacitance change as indicated in Fig. 5.23(a); TSC does not. Thermally stimulated measurements have been largely replaced with DLTS. However, in highresistivity materials, where it is difficult to make DLTS measurements, TSC can be used. An example is shown in Fig. 5.24 where both DLTS and TSC were used to determine the energy levels in high resistivity Si.117 The defect energy levels extracted from the data agree quite well between the two methods.
5.8
POSITRON ANNIHILATION SPECTROSCOPY (PAS)
Positron annihilation spectroscopy (PAS) is the spectroscopy of gamma (γ ) rays emerging from the annihilation of positrons and electrons. It can be used to examine defects in semiconductors without any special test structures, is independent of the sample conductivity, and is nondestructive.118 Before discussing PAS, we will briefly describe positrons, since they are rarely mentioned in semiconductor books. A positron is similar to an electron. Its mass is the same as that of an electron and its charge is the same magnitude but of opposite sign to that of an electron. The positron was predicted by Dirac in 1928 and was observed experimentally in 1932 by Anderson during cosmic ray cloud chamber experiments. Positrons diffusing through matter may be captured at certain trapping sites and the character and the density of these lattice defects can be investigated. An excellent discussion of PAS is given by KrauseRehberg and Leipner.118 The energy and momentum conservation during the annihilation of electrons with positrons can be used to study solids because the annihilation parameters are sensitive to lattice imperfections. The positron may be trapped in crystal defects, based on the formation of an
290
DEFECTS
Na22 (Positron Source) g annihilation (511 keV± ∆E)
g birth (128 MeV) Positron
∆Eg : Doppler Broadening Positronelectron annihilation
∆t: Lifetime g annihilation ± (511 keV ∆E) ∆q: Angular Correlation
Fig. 5.25 Schematic illustration of positron annihilation showing positron creation, positronelectron annihilation, γ ray emission and the three main experimental techniques for PAS.
attractive potential at openvolume defects, such as vacancies, vacancy agglomerates, and dislocations. When a positron is trapped in an openvolume defect, the annihilation parameters are changed in a characteristic way. Its lifetime increases due to the lower electron density. Momentum conservation leads to a small angular spread of the collinear γ quanta or a Doppler shift of the annihilation energy. Most positron lifetimes for the important semiconductors and lifetimes for various vacancytype defects have been experimentally determined. Neutral and negative vacancytype defects, as well as negative ions, are the dominant positron traps in semiconductors. Temperaturedependent lifetime measurements may distinguish between both defect types. Positrons are most commonly produced during nuclear decay, when a proton of proton rich nuclei decays into a neutron with the emission of a positron and a neutrino. For example 11 Na 22 →10 Ne22 + positron + neutrino. The Na22 isotope has a half life of 2.6 years and emits a 1.27 MeV γ ray within 10 ps of emitting a positron. This γ ray is used in lifetime spectroscopy measurements. Radioactive decay positrons possess a wide energy range. To produce a monochromatic positron beam for PAS from such a broad spectrum, the positrons pass through a moderator, e.g., W , Ni, and Mo. The positron energy is typically kT ≈ 25 meV after moderation. A positron is a stable particle by itself, but when it is combined with an electron, the two annihilate each other with the mass of the positronelectron pair converted into energy, i.e., gamma rays, as illustrated in Fig. 5.25. The released energy is twice the electron rest mass energy 2mc2 = 2 × 8.19 × 10−14 J = 2 × 5.11 × 105 eV, where m is the electron rest mass and c the speed of light. The most probable decay is by the emission of two γ rays, moving in opposite directions. The energies, emission directions, and time of emission of these γ rays provide information about the behavior of positronelectron pairs and thus about the material where they annihilate. Energy and momentum conservation requires each γ ray to have one half the energy of the positronelectron system, i.e., 511 keV. The probability of annihilation depends on the density of available electrons. When annihilation occurs, the gamma rays have an energy and directional distribution which depends on the electron motion before annihilation. The angle between the two γ rays differs slightly from 180◦ , with the angular deviation θ depending on the component of electron momentum perpendicular to the emission direction, pperp . The energy of each γ ray, Eγ , depends on the component of electron momentum parallel to the emission direction, ppar θ =
pperp ppar c ppar c ; Eγ = mc2 + ; Eγ = Eγ − mc2 = mc 2 2
(5.79)
POSITRON ANNIHILATION SPECTROSCOPY (PAS)
291
The terms θ and Eγ provide information about the electron momentum components in a material. It is chiefly the electron momenta that determine θ and Eγ , since positrons have low energy before annihilation. Additional information about the state of the electron before annihilation can be obtained by measuring the positron lifetime t. The annihilation positron lifetime is in the low ns range, but is affected by processes that alter the local density of electrons, making the lifetime one measure of crystal perfection. The positron lifetime is inversely proportional to the electron density of the material sampled by the positron, making it a unique probe of open volume lattice defects. The lifetime is the time between the creation of the positron and the creation of the gamma rays. For pure Si it is 219 ps, for monovacancies in Si about 266 ps, and for divacancies in Si about 320 ps.119 Most defects produce two effects related to positron annihilation. Defects producing local region of negative charge, attract positrons and defects alter the electron density and momentum distribution near the trapped positron. This leads to changes in t, θ , and Eγ . The positron lifetime is measured with two fast γ ray detectors and a timing circuit. Many positron sources, including Na, emit gamma rays (γbirth in Fig. 5.25) within a few picoseconds of the positron emission. Detection of this γ ray signals the positron injection into the material under test. θ is measured with a positron angular correlation spectrometer. In angular correlation of annihilation radiation, one measures the angle between the directions of photons in two γ annihilations. Momentum conservation during annihilation of a positronelectron pair requires the γ rays to move in opposite directions if the pair is at rest. If the pair has a finite momentum, it causes a deviation of the angle between the gamma rays from 180◦ . The measurement consists of counting pairs of annihilating γ rays emitted at angles that differ slightly from 180◦ as illustrated in Fig. 5.25. Typical values for θ are on the order of 0.01 rad. An example of the positron lifetime after electron irradiation is shown in Fig. 5.26, where 2 MeV electron irradiation produced vacancies which were annealed and the lifetime is a measure of the vacancy density. The initial vacancy density was estimated to be 3 × 1017 cm−3 .118 The motion of the annihilating positronelectron pair causes a Doppler shift in the energy of the 511 keV γ rays. The energy Eγ is measured with a positron Doppler
280 Electronirrradiated FZ Si
Positron Lifetime (ps)
270 260 250 240 230 Bulk Lifetime
220 210
0
100
200
300
400
500
600
700
Annealing Temperature (K)
Fig. 5.26 Positron lifetime versus annealing temperature for floatzone Si. The sample was electron irradiated at 2 MeV, T = 4 K, and 1018 cm−2 dose. The bulk lifetime refers to a vacancyfree sample. Adapted from KrauseRehberg and Leipner.118
292
DEFECTS
broadening lineshape spectrometer. The shape of the 511 keV gamma ray line is broadened due to the electron momenta and is usually characterized by the “S parameter”. The S parameter is defined as the number of counts in the central region of the 511 keV peak, containing about half of the total area, divided by the total number of counts in the peak. Lifetime and Doppler broadening experiments are more commonly used than angular correlation. The latter requires more complex equipment. PAS exploits the high sensitivity of positrons to regions of lowerthanaverage electron density such as vacancies, vacancy clusters, voids, and other defects in semiconductors, e.g., dislocations, grain boundaries, and interfaces. Any process that produces vacancies is suitable for PAS, e.g., ion implantation, where small vacancy clusters, too small for electron microscope detection, can be detected. PAS has also been used to study radiation damage and the SiO2 Si interface.119 Doppler broadening reflects the momentum state of the electron annihilated by the positron. Positrons trapped at vacancies have a higher probability of annihilation with electrons having low momentum and consequently the S parameter increases with the presence of vacancies or vacancytype defects. Measuring the S parameter as a function of annealing allows ion implanted samples to be characterized in terms of vacancy creation during implantation and their subsequent destruction during the implant damage anneal.120 To study depthdependent defects, positron beams with 0.1–30 keV energies were implanted. However, there is a depth resolution limit, because the positron implantation profile is broadened with increasing positron energy and its full width half maximum is comparable to the mean implanted depth. The trap sites of the implanted positrons also depend on their thermal diffusion following implantation. Enhanced depth resolution was achieved by repeated chemical etching and positron measurement.121 The defect profile and annealing behavior in B and P ion implantations to Si showed that defects were induced beyond the implanted ion profile. Positron emission has also been applied to microscopy where positrons are used instead of electrons in a scanning electron microscope.122
5.9
STRENGTHS AND WEAKNESSES
DLTS is the most common deeplevel characterization technique today, having replaced thermally stimulated current and capacitance. It lends itself to a number of different implementations and equipment is commercially available. Although DLTS is spectroscopic in nature, giving trap energies, it is frequently not easy to assign a specific impurity to a particular DLTS spectrum. Identification of impurities is not always straightforward. Capacitance Transient Spectroscopy: Its strength lies in the ease of measurement. Most systems use commercial capacitance meters or bridges and add signalprocessing functions (lockin amplifiers, boxcar integrators, or computers). One can distinguish between majority and minority carrier traps, and its sensitivity is independent of the emission time constant. Its major weakness is the inability to characterize high resistivity substrates. The fact that its sensitivity is independent of a time constant can be a disadvantage because the sensitivity cannot be changed. Laplace DLTS produces very high resolution plots allowing trap with close lying energy levels to be distinguished. Current Transient Spectroscopy: Its strength lies in the ability to characterize conducting as well as semiinsulating substrates. The fact that the current depends inversely on the emission time constant allows the sensitivity of the method to be changed by
APPENDIX 5.1
293
changing the time constant. This has led to its use in scanning DLTS. Its weakness is its dependence on diode quality, where leakage current can interfere with the measurement. Optical DLTS: Its strength lies in the ability to create minority carriers without the need for pn junctions. This allows materials in which it is difficult to make pn junctions to be characterized. ODLTS is useful to determine impurity optical crosssections. Its major weakness lies in the requirement for light. The low temperature dewar must have transparent windows, and monochromators or pulsed light sources must be available. Positron Annihilation Spectroscopy: Its strength lies in the contactless, nondestructive characterization of defects in solids. It allows depthdependent defect characterization. Its weaknesses are that it is chiefly sensitive to voidlike defects such as vacancies and requires elaborate equipment that is not readily available to most researchers.
APPENDIX 5.1 Activation Energy and Capture CrossSection The relationship between the emission rate and the capture crosssection is often written as en = σn vth Nc exp((Ec − ET )/kT )
(A5.1)
This relationship is frequently used to determine ET and σn . However, when the capture crosssection is determined from the intercept of a ln(τe T 2 ) versus 1/T plot, considerable error can result. From thermodynamics we find the following definitions:123 G = H − T S; H = E + pV
(A5.2)
where G is the Gibbs free energy, H the enthalpy, E the internal energy, T the temperature, S the entropy, p the pressure and V the volume. The energy to excite an electron thermally from a trap into the conduction band is Gn .124 Equation (A5.1) then becomes en = σn vth Nc exp(−Gn /kT )
(A5.3)
From Eq. (A5.2), Gn = Hn − T Sn for constant T . When substituted into Eq. (A5.3), the emission rate is en = σn Xn vth Nc exp(−Hn /kT ) (A5.4) where Xn = exp(Sn /k) is an “entropy factor”, that accounts for the entropy change accompanying electron emission from a trap to the conduction band. The entropy change can be expressed as Sn = Sne + Sna , where Sne is the change due to electronic degeneracy and Sna is due to atomic vibrational changes. The electronic contribution may be expressed in terms of two degeneracy factors: g0 is the degeneracy of the trap unoccupied by an electron, and g1 is the degeneracy of the trap occupied by one electron, giving Xn = (g0 /g1 ) exp(Sna /k)
(A5.5)
294
DEFECTS
The degeneracy factors are not well known for deeplevel impurities. Using values from shallow levels and with Sna ≈ a few k, Xn can easily be 10–100. Equation (A5.4) states that the energy determined from a ln(τe T 2 ) or ln(T 2 /en ) versus 1/T plot is an enthalpy, and the prefactor can be written as σn,eff vth NC , with σn,eff = σn Xn . In other words, the effective capture crosssection differs from the true capture crosssection by Xn . If that distinction is not made, then obviously the extracted crosssection can be seriously in error. Effective crosssections larger by factors of 50 or more from true crosssections are not uncommon.15 Examples are shown in Table 5.2. Additional complications occur when σn is temperature dependent. Some crosssections follow the relationship (A5.6) σn = σ∞ exp(−Eb /kT ) where σ∞ is the crosssection as T → ∞ and Eb is the crosssection activation energy. Equation (A5.4) becomes Hn + Eb en = σn Xn vth Nc exp − kT
(A5.7)
Under these conditions the Arrhenius plot gives neither the trap energy level nor its extrapolated crosssection correctly. If in addition the capture crosssection is electricfield dependent, further inaccuracies arise. A good discussion of energy levels, enthalpies, entropies, capture crosssections, etc., can be found in the work of Lang et al.15 Further thermodynamic derivations can be found in the work by Thurmond and Van Vechten.125 – 126 A nonthermodynamic approach defines the energy ET = Ec − ET as being temperature dependent according to ET = ET 0 − αT . The degeneracy ratio in Eq. (A5.5) is written as gn .127 Equation (A5.1) becomes en = σn Xn vth Nc exp(−ET 0 /kT )
(A5.8)
where now Xn = gn exp(α/k). We find the energy as that as T → 0K and the crosssection is again σn Xn , although now Xn is defined differently.
APPENDIX 5.2 Time Constant Extraction The capacitance of a Schottky barrier or p + n junction containing impurities is from Eq. (5.11) ND − NT exp(−t/τe ) (A5.9) C=K Vbi − V where nT (0) = NT , if we confine ourselves to emission transients for simplicity. How is τe determined? One method to extract τe is to take dV /d(1/C 2 ) from Eq. (A5.9) 8 as dV dV t=∞ − t = K 2 NT exp(−t/τe ) (A5.10) d(1/C 2 ) d(1/C 2 )
APPENDIX 5.2
295
and to plot the ln(left side of Eq. (A5.10)) versus t. The slope of this plot gives τe , and the intercept at t = 0 is ln(K2 NT ). This method places no limitation on the magnitude of NT with respect to ND . Another method defines f (t) = C(t)2 − C0 2 = [−K 2 NT /(Vbi − V )] exp(−t/τe ), where C0 is the capacitance in Eq. (A5.9) for NT = 0. The measurement is made at constant temperature. Differentiating f (t) and multiplying by t gives t
K 2 NT t df = exp(−t/τe ) dt Vbi − V τe
(A5.11)
When plotted against t, tdf/dt has a maximum of K 2 NT /[e(Vbi − V )] at t = τ .72 Hence determining the maximum in the curve gives the time constant. For NT ≪ ND , we can write [see Eq. (5.16)] nT (0) NT C = C0 1 − exp(−t/τe ) = C0 1 − exp(−t/τe ) (A5.12) 2ND 2ND Equation (A5.12) has been used in a number of implementations to extract τe . In the twopoint method, the Ct exponential timevarying curve is sampled t = t1 and t = t2 .42 From Eq. (5.49) t2 − t1 (A5.13) τe,max = ln(t2 /t1 ) In the threepoint method, three points are measured on the Ct curve at a constant temperature, C = C1 at t = t1 , C = C2 at t = t2 , and C = C3 at t = t3 .128 From Eq. (A5.12) exp(t/τe ) − 1 C1 − C2 = C2 − C 3 1 − exp(t/τe )
(A5.14)
where t = t2 − t1 = t3 − t2 . A solution of Eq. (A5.14) for τe is τe =
t ln[(C1 − C2 )/(C2 − C3 )]
(A5.15)
A good choice for t is τe /2, but of course τe is not known a priori, although a firstorder value for it can be obtained from the “1/e point” on the capacitance decay curve. Another technique is based on a very different approach. Consider the function y1 = y(t) = A exp(−t/τ ) + B, i.e., an exponentially decaying function superimposed on a dc background. We define a second function y2 = y(t + t) = A exp[−(t + t)/τ ] + B. The second function is obtained from the first by simply adding a constant increment t to the time t. A plot of y2 versus y1 is a straight line with slope m = exp(−t/τ ) and intercept on the y2 axis of B(1 − m).129 Then τ is calculated from the slope and t and B are found from the intercept and the slope. t should be smaller than τ , but not much smaller, e.g., t ≈ 0.1 to 0.5τ . An excellent discussion of decay time extraction is given by Istratov and Vyvenko.130 For a single energy level impurity with a single exponential decay, the transient is characterized by f (t) = A exp(−λt) + B (A5.16) where A is the decay amplitude, B is a constant (the baseline offset), and λ is the decay rate, decay constant or rate constant, which is the inverse of the decay time constant τ
296
DEFECTS
(τ = 1/λ). If the decay consists of a sum of n exponentials of the form Eq. (A5.16), then n
Ai exp(−λi t) (A5.17) f (t) = i=1
neglecting the baseline offset B. This behavior is expected from more than one energy level. The goal of any multiexponential analysis is to determine the number of exponential components n, their amplitudes Ai , and decay rates λi . When the decay is due to a continuous distribution of emission rates given by a spectral function g(λ) rather than by a sum of discrete exponential transients f (t) =
∞
g(λ) exp(−λt) dλ
(A5.18)
0
where g(λ) is the spectral function. Such behavior is exhibited by interface traps with a continuous distribution of energy in the band gap at the SiO2 /Si interface, for example. The major goal of exponential analysis is to distinguish exponential components with close time constants in the experimentally measured decay. To achieve high resolution in exponential analysis, it is very important to record the transient until it decays completely. Since the ratio of amplitudes of two exponentials with close decay rates: exp(−λ1 t) and exp(−λ2 t) increases with the time as exp[((λ2 − λ1 )t], these exponentials always can, at least theoretically, be distinguished if the decay is monitored for a sufficiently long time. Since the exponential is a decaying function of time, the transient should be monitored as long as the signal amplitude exceeds the noise level. For a signaltonoise ratio, S/R = 100, the measurement time should be at least 4.6τ , for S/R = 1000 about 6.9τ , and for S/R = 104 at least 9.2τ .130 This is frequently ignored in experiments and numerical simulations. Consider the example in Fig. A5.1. Twentyfour data points were fitted by a double exponential f2 (t) = 2.202 exp(−4.45t) + 0.305 exp(−1.58t) and by a triple exponential f3 (t) = 0.0951 exp(−t) + 0.8607 exp(−3t) + 1.5576 exp(−5t) in Fig. A5.1(a). Lanczos showed that a sum of two exponentials could be reproduced to within two decimal places by a sum of three exponentials with entirely different time constants and amplitudes.131 However, a discrepancy is observed when the data are extended to longer times as shown in Fig. A5.1(b). However, the difference between the two curves does not exceed 0.001 of the decay amplitude, and can be detected only if the S/R exceeds 1000.
APPENDIX 5.3 Si and GaAs Data Arrhenius plots for Si and GaAs are shown in Figs. A5.2 and A5.3. In Fig. A5.2, (300/T )2 en and (300/T )2 ep are plotted instead of τnT 2 and τpT 2 , giving negative slopes. The deep level impurity metals are shown wherever possible, and the numbers listed below the elements are their energy levels calculated from the slopes. The superscripts are the references given in the review paper by Chen and Milnes.3 Table A5.1 lists typical trace contamination in Si most commonly produced during device processing or after 1MeV electron beam irradiation.132 The impurities were determined from transient capacitance spectroscopy. DLTS spectra have been correlated with metallic impurities, growthrelated defects, oxidation, heat treatments, electron and proton
APPENDIX 5.3
297
Amplitude (a.u.)
101 f2 f3 100
10−1 2 ms/4 ms 10−2
0
0.5
1
1.5
Time (h) (a) 101 f2 f3
Amplitude (a.u.)
100 10−1 10−2 10−3 10−4 10−5
0
1
2
3
4
5
6
Time (h) (b) Fig. A5.1 (a) Data points were fitted by a double exponential f2 (t) = 2.202 exp(−4.45t) + 0.305 exp(−1.58t) and by a triple exponential f3 (t) = 0.0951 exp(−t) + 0.8607 exp(−3t) + 1.5576 exp (−5t). The difference between f2 (t) and f3 (t) is less than the line width. (b) The curves separated after 2 h, but the absolute value of the separation is less than only 0.001 of the decay amplitude. Adapted from ref. 131.
irradiation, dislocationrelated states, electronically stimulated defects, and laser anneal. Established temperature regimes of defect and impurity reactions are indicated. An unknown DLTS peak can be compared with the data in Table A5.1 by two methods.132 First, an Arrhenius plot of τe T 2 versus 1/T can be constructed using the point given by the temperature of the known peak (T ) at a time constant of 1.8 ms (τ ) and the slope given by the activation energy (ET ) in the table. Alternatively, the temperature at which a signal from a listed defect should occur using any time constant of the analyzing instrument can be determined by iteration. A simple computer program sets the ratio R, τ1 T12 exp(−ET /kT1 ) (A5.16) R= τ2 T22 exp(−ET /kT2 )
298
DEFECTS 105
104
en (300/ T)2 s−1
103
102
101
100
10−1
10−2
10−3
2
3
4
5
6
7
8
9
10
11
12
13
14
15
16
11
12
13
14
15
16
1000/ T (K−1) (a) 105
104
ep (300/ T)2 s−1
103
102
101
100
10−1
10−2
10−3
2
3
4
5
6
7
8
9
10
1000/ T (K−1) (b)
Fig. A5.2 Arrhenius plots obtained from capacitance transient measurements: (a) electron traps, (b) hole traps in Si. The vertical axis is (300/T 2 )en,p instead of τn,p T 2 . Reprinted, with permission, from the Annual Review of Material Science, Vol. 10, 1980 by Annual Reviews Inc.
APPENDIX 5.3
299
107 106
T2/en (K2 − s)
105 104 103 102 101 100
2
3
4
5
7
6
8
9
10
11
12
1000/T (K−1) (a) 107 106
T2/ep (K2 − s)
105 104 103 102 101 100
2
3
4
5
6
7
8
9
1000/T (K−1) (b)
Fig. A5.3 Arrhenius plots obtained from capacitance transient measurements: (a) electron traps, (b) hole traps in GaAs. The vertical axis is T 2 /en,p instead of τn,p T 2 . Reprinted, with permission after Martin et al.17 and Mitonneau et al.17 Institution of Electrical Engineers.
where subscript 1 refers to the value of Table A5.1 and subscript 2 refers to the value for the particular measurement. For τ1 > τ2 the temperature T2 is increased; for τ1 < τ2 the temperature T2 is decreased until R = 1.
300
DEFECTS
TABLE A5.1 Defect Ag Au Cu Fe (FeB) (F ei )
Mn
Ni Pt
ODonor
Heat Treatment
Laser Donor
VacancyO VacancyVacancy
P Vacancy Cs − Ci Dislocation Point Defect Debris
Capacitance Transient Spectral Features for Silicon. T (K) 1.8 ms 286 184 288 173 112 242 181 59 267 208 299 184 170 168 237 220 68 216 81 257 88 114 174 87 Below Freezeout 58 59,60
ET (eV)
σmaj (cm2 )
(0.51) (0.38) (0.53) (0.35) (0.22) (0.41) (0.35) (0.10) (0.46) (0.21) (0.46) (0.23) (0.35) (0.30) (0.43) (0.47) (0.11) (0.41) (0.13) (0.43) (0.14) (0.22) (0.30) (0.22) (0.07)
10−16 — 2 × 10−16 > 10−15 > 6 × 10−14 8 × 10−14 6 × 10−15 > 4 × 10−15
E H E H H H E H H E E H E H H H E E H E E E E H E
E (0.15) E (0.15)
— — — — 5 × 10−15 — — — 10−15 > 2 × 10−15 5 × 10−16 10−16 > 4 × 10−15 ∼ 10−15 ∼ 10−15 — —
112 228 115 200 211 98 139
E (0.22) > 3 × 10−15 E (0.47) 2 × 10−16 E (0.19) 7 × 10−16 E (0.33–0.36) 5 × 10−16 H (0.36) 5 × 10−19 E (0.18) 5 × 10−16 E (0.23)
245 123 237 204 225 206 288
E (0.41) H (0.21) E (0.44) H (0.36) E (0.38) H (0.35) E (0.63–0.68)
— 10−14 2 × 10−16 4 × 10−15 2 × 10−16 > 10−16 8 × 10−17
Comments(a)
Anneal
In 400◦ C, out 600◦ C
Q, *, FZ Q, *, FZ Q, *, FZ Q, *, FZ Q, *, FZ Q, *, FZ Q, *, FZ Q, *, FZ Q, *, FZ S, FZ S, FZ S, FZ Q, CG Q, CG Q, CG Q, CG Q, FZ Q, FZ Q, FZ Q, *, FZ Q, *, FZ Q, *, FZ Q, *, FZ Q, *, FZ *, CG
In 400◦ C, out 600◦ C In 900◦ C
*, CG *, CG
In 900◦ C In 900◦ C Out 550◦ C Out 650◦ C
*, CG *, CG Q, FZ, CG Q, FZ, CG Q, *, FZ, CG 1 MeV, CG 1 MeV, CG, FZ
Out 150◦ C Out > 150◦ C In > 150◦ C, out > 200◦ C
Out 150◦ C
In −43◦ C, out 350◦ C Out 300◦ C Out 300◦ C Out 300◦ C Out 150◦ C In 43◦ C Out 800◦ C
1 1 1 1
MeV, CG, FZ MeV, CG, FZ MeV, CG, FZ MeV, CG, FZ FZ FZ FZ, cross slip
1.4 × 10−15 > 5 × 10−17 Source: Ref. 132. (a) Symbols: Q = quenched material, ∗ = diffused junction, S = slow cool, FZ = float zone growth, CG = crucible growth, and 1 MeV = electron bombardment.
REFERENCES
301
REFERENCES 1. B.D. Choi and D.K. Schroder, “Degradation of Ultrathin Oxides by Iron Contamination,” Appl. Phys. Lett. 79, 2645–2647, Oct. 2001; Y.H. Lin, Y.C. Chen, K.T. Chan, F.M. Pan, I.J. Hsieh, ˚ Gate Oxide Integrity Contaminated by Copper,” and A. Chin, “The Strong Degradation of 30 A J. Electrochem. Soc. 148, F73–F76, April 2001. 2. A.G. Milnes, Deep Impurities in Semiconductors, WileyInterscience, New York, 1973. 3. J.W. Chen and A.G. Milnes, “Energy Levels in Silicon,” in Annual Review of Material Science (R.A. Huggins, R.H. Bube and D.A. Vermilyea, eds.), Annual Reviews, Palo Alto, CA, 10, 157–228, 1980; A.G. Milnes, “Impurity and Defect Levels (Experimental) in Gallium Arsenide,” in Advances in Electronics and Electron Physics (P.W. Hawkes, ed.), Academic Press, Orlando, FL, 61, 63–160, 1983. 4. M. Jaros, Deep Levels in Semiconductors, A. Hilger, Bristol, 1982. 5. C.T. Sah, L. Forbes, L.L. Rosier and A.F. Tasch Jr., “Thermal and Optical Emission and Capture Rates and Cross Sections of Electrons and Holes at Imperfection Centers in Semiconductors from Photo and Dark Junction Current and Capacitance Experiments,” SolidState Electron. 13, 759–788, June 1970. 6. R.N. Hall, “ElectronHole Recombination in Germanium,” Phys. Rev. 87, 387, July 1952. 7. W. Shockley and W.T. Read, “Statistics of the Recombinations of Holes and Electrons,” Phys. Rev. 87, 835–842, Sept. 1952. 8. R. Williams, “Determination of Deep Centers in Conducting Gallium Arsenide,” J. Appl. Phys. 37, 3411–3416, Aug. 1966; R.R. Senechal and J. Basinski, “Capacitance of Junctions on GoldDoped Silicon,” J. Appl. Phys. 39, 3723–3731, July 1968; “Capacitance Measurements on AuGaAs Schottky Barriers,” J. Appl. Phys. 39, 4581–4589, Sept. 1968. 9. M. Bleicher and E. Lange, “SchottkyBarrier Capacitance Measurements for Deep Level Impurity Determination,” SolidState Electron. 16, 375–380, March 1973. 10. R.F. Pierret, Advanced Semiconductor Fundamentals, AddisonWesley, Reading, MA, 1987, 146–152. 11. W. Shockley, “Electrons, Holes, and Traps,” Proc. IRE 46, 973–990, June 1958. 12. C.T. Sah, “The Equivalent Circuit Model in SolidState Electronics—Part I: The Single Energy Level Defect Centers,” Proc. IEEE 55, 654–671, May 1967; “The Equivalent Circuit Model in SolidState Electronics—Part II: The Multiple Energy Level Impurity Centers,” Proc. IEEE 55, 672–684, May 1967. 13. P.A. Martin, B.G. Streetman and K. Hess, “Electric Field Enhanced Emission from NonCoulombic Traps in Semiconductors,” J. Appl. Phys. 52, 7409–7415, Dec. 1981. 14. A.F. Tasch, Jr. and C.T. Sah, “RecombinationGeneration and Optical Properties of Gold Acceptor in Silicon,” Phys. Rev. B1, 800–809, Jan. 1970. 15. D.V. Lang, H.G. Grimmeiss, E. Meijer and M. Jaros, “Complex Nature of GoldRelated Deep Levels in Silicon,” Phys. Rev. B22, 3917–3934, Oct. 1980. 16. H.D. Barber, “Effective Mass and Intrinsic Concentration in Silicon,” SolidState Electron. 10, 1039–1051, Nov. 1967. 17. G.M. Martin, A. Mitonneau and A Mircea, “Electron Traps in Bulk and Epitaxial GaAs Crystals,” Electron. Lett. 13, 191–193, March 1977; A. Mitonneau, G.M. Martin, and A Mircea, “Hole Traps in Bulk and Epitaxial GaAs Crystals,” Electron. Lett. 13, 666–668, Oct. 1977. 18. W.B. Leigh, J.S. Blakemore and R.Y. Koyama, “Interfacial Effects Related to Backgating in IonImplanted GaAs MESFET’s,” IEEE Trans. Electron Dev. ED32, 1835–1841, Sept. 1985. 19. J.A. Pals, “Properties of Au, Pt, Pd and Rh Levels in Silicon Measured with a Constant Capacitance Technique,” SolidState Electron. 17, 1139–1145, Nov. 1974. 20. H. Okushi and Y. Tokumaru, “A Modulated DLTS Method for Large Signal Analysis (C 2 – DLTS),” Japan. J. Appl. Phys. 20, L45–L47, Jan. 1981.
302
DEFECTS
21. W.E. Phillips and J.R. Lowney, “Analysis of Nonexponential Transient Capacitance in Silicon Diodes Heavily Doped with Platinum,” J. Appl. Phys. 54, 2786–2791, May 1983. 22. A.C. Wang and C.T. Sah, “Determination of Trapped Charge Emission Rates from Nonexponential Capacitance Transients Due to High Trap Densities in Semiconductors,” J. Appl. Phys. 55, 565–570, Jan. 1984. 23. D. Sti´evenard, M. Lannoo and J.C. Bourgoin, “Transient Capacitance Spectroscopy in Heavily Compensated Semiconductors,” SolidState Electron. 28, 485–492, May 1985. 24. F.D. Auret and M. Nel, “Detection of MinorityCarrier Defects by Deep Level Transient Spectroscopy Using Schottky Barrier Diodes,” J. Appl. Phys. 61, 2546–2549, April 1987. 25. L. Stolt and K. Bohlin, “DeepLevel Transient Spectroscopy Measurements Using High Schottky Barriers,” SolidState Electron. 28, 1215–1221, Dec. 1985. 26. C.H. Henry, H. Kukimoto, G.L. Miller and F.R. Merritt, “Photocapacitance Studies of the Oxygen Donor in GaP. II. Capture Cross Sections,” Phys. Rev. B7, 2499–2507, March 1973; A.C. Wang and C.T. Sah, “New Method for Complete Electrical Characterization of Recombination Properties of Traps in Semiconductors,” J. Appl. Phys. 57, 4645–4656, May 1985. 27. J.A. Borsuk and R.M. Swanson, “CaptureCrossSection Determination by TransientCurrent TrapFilling Experiments,” J. Appl. Phys. 52, 6704–6712, Nov. 1981. 28. S.D. Brotherton and J. Bicknell, “The Electron Capture Cross Section and Energy Level of the Gold Acceptor Center in Silicon,” J. Appl. Phys. 49, 667–671, Feb. 1978. 29. A. Zylbersztejn, “Trap Depth and Electron Capture Cross Section Determination by Trap Refilling Experiments in Schottky Diodes,” Appl. Phys. Lett. 33, 200–202, July 1978. 30. H. Kukimoto, C.H. Henry and F.R. Merritt, “Photocapacitance Studies of the Oxygen Donor in GaP. I. Optical Cross Sections, Energy Levels, and Concentration,” Phys. Rev. B7, 2486–2499, March 1973. 31. S.D. Brotherton and J. Bicknell, “Measurement of Minority Carrier Capture Cross Sections and Application to Gold and Platinum in Silicon,” J. Appl. Phys. 53, 1543–1553, March 1982. 32. B. Hamilton, A.R. Peaker and D.R. Wight, “DeepStateControlled MinorityCarrier Lifetime in nType Gallium Phosphide,” J. Appl. Phys. 50, 6373–6385, Oct. 1979; R. Brunwin, B. Hamilton, P. Jordan and A.R. Peaker, “Detection of MinorityCarrier Traps Using Transient Spectroscopy,” Electron. Lett. 15, 349–350, June 1979. 33. C.T. Sah, “Bulk and Interface Imperfections in Semiconductors,” SolidState Electron. 19, 975–990, Dec. 1976. 34. J.A. Borsuk and R.M. Swanson, “Current Transient Spectroscopy: A HighSensitivity DLTS System,” IEEE Trans. Electron Dev. ED27, 2217–2225, Dec. 1980. 35. P.K. McLarty, D.E. Ioannou and H.L. Hughes, “Deep States in SilicononInsulator Substrates Prepared by Oxygen Implantation Using Current Deep Level Transient Spectroscopy,” Appl. Phys. Lett. 53, 871–873, Sept. 1988. 36. P.V. Kolev and M.J. Deen, “ConstantResistance DeepLevel Transient Spectroscopy in Submicron MetalOxideSemiconductor FieldEffect Transistors,” J. Appl. Phys. 83, 820–825, Jan. 1998. 37. M.G. Collet, “An Experimental Method to Analyse Trapping Centres in Silicon at Very Low Concentrations,” SolidState Electron. 18, 1077–1083, Dec. 1975. 38. I.D. Hawkins and A.R. Peaker, “Capacitance and Conductance Deep Level Transient Spectroscopy in FieldEffect Transistors,” Appl. Phys. Lett. 48, 227–229, Jan. 1986. 39. J.M. Golio, R.J. Trew, G.N. Maracas and H. Lef`evre, “A Modeling Technique for Characterizing IonImplanted Material Using CV and DLTS Data,” SolidState Electron. 27, 367–373, April 1984.
REFERENCES
303
40. J.W. Farmer, C.D. Lamp and J.M. Meese, “Charge Transient Spectroscopy,” Appl. Phys. Lett. 41, 1063–1065, Dec. 1982. 41. K.I. Kirov and K.B. Radev, “A Simple ChargeBased DLTS Technique,” Phys. Stat. Sol. 63a, 711–716, Feb. 1981. 42. D.V. Lang, “DeepLevel Transient Spectroscopy: A New Method to Characterize Traps in Semiconductors,” J. Appl. Phys. 45, 3023–3032, July 1974; D.V. Lang, “Fast Capacitance Transient Apparatus: Application to ZnO and O Centers in GaP pn Junctions,” J. Appl. Phys. 45, 3014–3022, July 1974. 43. ASTM Standard F 97890, “Standard Test Method for Characterizing Semiconductor Deep Levels by Transient Capacitance,” 1996 Annual Book of ASTM Standards, Am. Soc. Test., Conshohocken, PA, 1996. 44. G.L. Miller, D.V. Lang and L.C. Kimerling, “Capacitance Transient Spectroscopy,” in Annual Review Material Science (R.A. Huggins, R.H. Bube and R.W. Roberts, eds.), Annual Reviews, Palo Alto, CA, 7, 377–448, 1977. 45. D.V. Lang, “SpaceCharge Spectroscopy in Semiconductors,” in Topics in Applied Physics, 37, Thermally Stimulated Relaxation in Solids (P. Br¨aunlich, ed.), Springer, Berlin, 1979, 93–133. 46. B.D. Choi, D.K. Schroder, S. Koveshnikov, and S. Mahajan, “Latent Iron in Silicon,” Japan. J. Appl. Phys. 40, L915–L917, Sept. 2001. 47. M.A. Gad and J.H. EvansFreeman, “High Resolution Minority Carrier Transient Spectroscopy of Si/SiGe/Si Quantum Wells,” J. Appl. Phys. 92, 5252–5258, Nov. 2002. 48. D.S. Day, M.Y. Tsai, B.G. Streetman and D.V. Lang, “DeepLevelTransient Spectroscopy: System Effects and Data Analysis,” J. Appl. Phys. 50, 5093–5098, Aug. 1979. 49. S. Misrachi, A.R. Peaker and B. Hamilton, “A High Sensitivity Bridge for the Measurement of Deep States in Semiconductors,” J. Phys. E: Sci. Instrum. 13, 1055–1061, Oct. 1980. 50. T.I. Chappell and C.M. Ransom, “Modifications to the Boonton 72BD Capacitance Meter for DeepLevel Transient Spectroscopy Applications,” Rev. Sci. Instrum. 55, 200–203, Feb. 1984. 51. H. Lef`evre and M. Schulz, “Double Correlation Technique (DDLTS) for the Analysis of Deep Level Profiles in Semiconductors,” Appl. Phys. 12, 45–53, Jan. 1977. 52. K. Kosai, “External Generation of Gate Delays in a Boxcar Integrator—Application to Deep Level Transient Spectroscopy,” Rev. Sci. Instrum. 53, 210–213, Feb. 1982. 53. G. Goto, S. Yanagisawa, O. Wada and H. Takanashi, “Determination of DeepLevel Energy and Density Profiles in Inhomogeneous Semiconductors,” Appl. Phys. Lett. 23, 150–151, Aug. 1973. 54. N.M. Johnson, “Measurement of SemiconductorInsulator Interface States by ConstantCapacitance, DeepLevel Transient Spectroscopy,” J. Vac. Sci. Technol. 21, 303–314, July/Aug. 1982. 55. G.L. Miller, “A Feedback Method for Investigating Carrier Distributions in Semiconductors,” IEEE Trans. Electron Dev. ED19, 1103–1108, Oct. 1972. 56. J.M. Noras, “Thermal Filling Effects on Constant Capacitance Transient Spectroscopy,” Phys. Stat. Sol. 69a, K209–K213, Feb. 1982. 57. M.F. Li and C.T. Sah, “New Techniques of CapacitanceVoltage Measurements of Semiconductor Junctions,” SolidState Electron. 25, 95–99, Feb. 1982. 58. R.Y. DeJule, M.A. Haase, D.S. Ruby and G.E. Stillman, “Constant Capacitance DLTS Circuit for Measuring High Purity Semiconductors,” SolidState Electron. 28, 639–641, June 1985. 59. P. Kolev, “An Improved Feedback Circuit for ConstantCapacitance Voltage Transient Measurements,” SolidState Electron. 35, 387–389, March 1992. 60. M.F. Li and C.T. Sah, “A New Method for the Determination of Dopant and Trap Concentration Profiles in Semiconductors,” IEEE Trans. Electron Dev. ED29, 306–315, Feb. 1982.
304
DEFECTS
61. N.M. Johnson, D.J. Bartelink, R.B. Gold, and J.F. Gibbons, “ConstantCapacitance DLTS Measurement of DefectDensity Profiles in Semiconductors,” J. Appl. Phys. 50, 4828–4833, July 1979. 62. L.C. Kimerling, “New Developments in Defect Studies in Semiconductors,” IEEE Trans. Nucl. Sci. NS23, 1497–1505, Dec. 1976. 63. G.L. Miller, J.V. Ramirez and D.A.H. Robinson, “A Correlation Method for Semiconductor Transient Signal Measurements,” J. Appl. Phys. 46, 2638–2644, June 1975. 64. A. Rohatgi, J.R. Davis, R.H. Hopkins and P.G. McMullin, “A Study of GrownIn Impurities in Silicon by DeepLevel Transient Spectroscopy,” SolidState Electron. 26, 1039–1051, Nov. 1983. 65. G. Couturier, A. Thabti and A.S. Barri`ere, “The Baseline Problem in DLTS Technique,” Rev. Phys. Appliqu´e 24, 243–249, Feb. 1989. 66. J.T. Schott, H.M. DeAngelis and P.J. Drevinsky, “Capacitance Transient Spectra of Processingand RadiationInduced Defects in Silicon Solar Cells,” J. Electron. Mat. 9, 419–434, March 1980. 67. G. Ferenczi and J. Kiss, “Principles of the Optimum LockIn Averaging in DLTS Measurement,” Acta Phys. Acad. Sci. Hung. 50, 285–290, 1981. 68. P.M. Henry, J.M. Meese, J.W. Farmer and C.D. Lamp, “FrequencyScanned DeepLevel Transient Spectroscopy,” J. Appl. Phys. 57, 628–630, Jan. 1985. 69. K. Dmowski and Z. Pi´oro, “Noise Properties of Analog Correlators with Exponentially Weighted Average,” Rev. Sci. Instrum. 58, 2185–2191, Nov. 1987. 70. M.S. Hodgart, “Optimum Correlation Method for Measurement of Noisy Transients in SolidState Physics Experiments,” Electron. Lett. 14, 388–390, June 1978; C.R. Crowell and S. Alipanahi, “Transient Distortion and nth Order Filtering in Deep Level Transient Spectroscopy (D n LT S),” SolidState Electron. 24, 25–36, Jan. 1981. 71. E.E. Haller, P.P. Li, G.S. Hubbard and W.L. Hansen, “Deep Level Transient Spectroscopy of High Purity Germanium Diodes/Detectors,” IEEE Trans. Nucl. Sci. NS26, 265–270, Feb. 1979. 72. H. Okushi and Y. Tokumaru, “Isothermal Capacitance Transient Spectroscopy for Determination of Deep Level Parameters,” Japan. J. Appl. Phys. 19, L335–L338, June 1980. 73. K. H¨olzlein, G. Pensl, M. Schulz and P. Stolz, “Fast ComputerControlled Deep Level Transient Spectroscopy System for Versatile Applications in Semiconductors” Rev. Sci. Instrum. 57, 1373–1377, July 1986. 74. P.D. Kirchner, W.J. Schaff, G.N. Maracas, L.F. Eastman, T.I. Chappell and C.M. Ransom, “The Analysis of Exponential and Nonexponential Transients in DeepLevel Transient Spectroscopy,” J. Appl. Phys. 52, 6462–6470, Nov. 1981. 75. K. Ikeda and H. Takaoka, “Deep Level Fourier Spectroscopy for Determination of Deep Level Parameters,” Japan. J. Appl. Phys. 21, 462–466, March 1982. 76. S. Weiss and R. Kassing, “Deep Level Transient Fourier Spectroscopy (DLTFS)—A Technique for the Analysis of Deep Level Properties,” SolidState Electron. 31, 1733–1742, Dec. 1988. 77. L. Dobaczewski, A.R. Peaker, and K. Bonde Nielsen, “Laplacetransform Deeplevel Spectroscopy: The Technique and Its Applications to the Study of Point Defects in Semiconductors,” J. Appl. Phys. 96, 4689–4728, Nov. 2004. 78. J.E. Stannard, H.M. Day, M.L. Bark and S.H. Lee, “Spectroscopic Line Fitting to DLTS Data,” SolidState Electron. 24, 1009–1013, Nov. 1981. 79. F.R. Shapiro, S.D. Senturia and D. Adler, “The Use of Linear Predictive Modeling for the Analysis of Transients from Experiments on Semiconductor Defects,” J. Appl. Phys. 55, 3453–3459, May 1984.
REFERENCES
305
80. M. Henini, B. Tuck and C.J. Paull, “A MicrocomputerBased Deep Level Transient Spectroscopy (DLTS) System,” J. Phys. E: Sci. Instrum. 18, 926–929, Nov. 1985. 81. R. Langfeld, “A New Method of Analysis of DLTSSpectra,” Appl. Phys. A44, 107–110, Oct. 1987. 82. W.A. Doolittle and A. Rohatgi, “A Novel Computer Based PseudoLogarithmic Capacitance/Conductance DLTS System Specifically Designed for Transient Analysis,” Rev. Sci. Instrum. 63, 5733–5741, Dec. 1992. 83. P. Deixler, J. Terry, I.D. Hawkins, J.H. EvansFreeman, A.R. Peaker, L. Rubaldo, D.K. Maude, J.C. Portal, L. Dobaczewski, K. Bonde Nielsen, A. Nylandsted Larsen, and A. Mesli, “Laplacetransform Deeplevel Transient Spectroscopy Studies of the G4 Gold–hydrogen Complex in Silicon,” Appl. Phys. Lett. 73, 3126–3128, Nov. 1998. 84. L. Dobaczewski, P. Kaczor, M. Missous, A.R. Peaker, and Z.R. Zytkiewicz “Evidence for SubstitutionalInterstitial Defect Motions Leading to DX Behavior by Donors in Alx Ga1−x As,” Phys. Rev. Lett. 68, 2508–2511, April 1992; L. Dobaczewski, P. Kaczor, I.D. Hawkins, and A.R. Peaker, “Laplace Transform Deeplevel Transient Spectroscopic Studies of Defects in Semiconductors,” J. Appl. Phys. 76, 194–198, July 1994. 85. K.L. Wang and A.O. Evwaraye, “Determination of Interface and BulkTrap States of IGFET’s Using Deep Level Transient Spectroscopy,” J. Appl. Phys. 47, 4574–4577, Oct. 1976; K.L. Wang, “Determination of ProcessingRelated Interface States and Their Correlation with Device Properties,” in Semiconductor Silicon 1977 (H.R. Huff and E. Sirtl, eds.), Electrochem. Soc., Princeton, NJ, 404–413; K.L. Wang, “MOS InterfaceState Density Measurements Using Transient Capacitance Spectroscopy,” IEEE Trans. Electron Dev. ED27, 2231–2239, Dec. 1980. 86. M. Schulz and N.M. Johnson, “Transient Capacitance Measurements of Hole Emission from Interface States in MOS Structures,” Appl. Phys. Lett. 31, 622–625, Nov. 1977; T.J. Tredwell and C.R. Viswanathan, “Determination of InterfaceState Parameters in a MOS Capacitor by DLTS,” SolidState Electron. 23, 1171–1178, Nov. 1980. 87. K. Yamasaki, M. Yoshida and T. Sugano, “Deep Level Transient Spectroscopy of Bulk Traps and Interface States in Si MOS Diodes,” Japan. J. Appl. Phys. 18, 113–122, Jan. 1979. 88. N.M. Johnson, D.J. Bartelink and M. Schulz, “Transient Capacitance Measurements of Electronic States at the SiSiO2 Interface,” in The Physics of SiO2 and Its Interfaces (S.T. Pantelides, ed.), Electrochem. Soc., Pergamon Press, New York, 1978, pp. 421–427. 89. T. Katsube, K. Kakimoto and T. Ikoma, “Temperature and Energy Dependences of Capture Cross Sections at Surface States in Si MetalOxideSemiconductor Diodes Measured by Deep Level Transient Spectroscopy,” J. Appl. Phys. 52, 3504–3508, May 1981. 90. W.D. Eades and R.M. Swanson, “Improvements in the Determination of Interface State Density Using Deep Level Transient Spectroscopy,” J. Appl. Phys. 56, 1744–1751, Sept. 1984; W.D. Eades and R.M. Swanson, “Determination of the Capture Cross Section and Degeneracy Factor of SiSiO2 Interface States,” Appl. Phys. Lett. 44, 988–990, May 1984. 91. B. Monemar and H.G. Grimmeiss, “Optical Characterization of Deep Energy Levels in Semiconductors,” Progr. Cryst. Growth Charact. 5, 47–88, Jan. 1982; H.G. Grimmeiss, “Deep Level Impurities in Semiconductors,” in Annual Review Material Science (R.A. Huggins, R.H. Bube and R.W. Roberts, eds.), Annual Reviews, Palo Alto, CA, 7, 341–376, 1977. 92. A. Chantre, G. Vincent and D. Bois, “DeepLevel Optical Spectroscopy in GaAs,” Phys. Rev. B23, 5335–5339, May 1981. 93. P.M. Mooney, “PhotoDeep Level Transient Spectroscopy: A Technique to Study Deep Levels in Heavily Compensated Semiconductors,” J. Appl. Phys. 54, 208–213, Jan. 1983. 94. C.T. Sah, L.L. Rosier and L. Forbes, “Direct Observation of the Multiplicity of Impurity Charge States in Semiconductors from LowTemperature HighFrequency PhotoCapacitance,” Appl. Phys. Lett. 15, 316–318, Nov. 1969.
306
DEFECTS
95. A.M. White, P.J. Dean and P. Porteous, “Photocapacitance Effects of Deep Traps in Epitaxial GaAs,” J. Appl. Phys. 47, 3230–3239, July 1976. 96. S. Dhar, P.K. Bhattacharya, F.Y. Juang, W.P. Hong and R.A. Sadler, “Dependence of DeepLevel Parameters in IonImplanted GaAs MESFET’s on Material Preparation,” IEEE Trans. Electron Dev. ED33, 111–118, Jan. 1986. 97. R.E. Kremer, M.C. Arikan, J.C. Abele and J.S. Blakemore, “Transient Photoconductivity Measurements in SemiInsulating GaAs. I. An Analog Approach,” J. Appl. Phys. 62, 2424–2431, Sept. 1987 and references therein; J.C. Abele, R.E. Kremer and J.S. Blakemore, “Transient Photoconductivity Measurements in SemiInsulating GaAs. II. A Digital Approach,” J. Appl. Phys. 62, 2432–2438, Sept. 1987. 98. D.C. Look, “The Electrical and Photoelectronic Properties of SemiInsulating GaAs,” in Semiconductors and Semimetals (R.K. Willardson and A.C. Beer, eds.) Academic Press, New York, 19, 75–170, 1983. 99. M.R. Burd and R. Braunstein, “Deep Levels in SemiInsulating Liquid Encapsulated CzochralskiGrown GaAs,” J. Phys. Chem. Sol. 49, 731–735, 1988. 100. J.C. Balland, J.P. Zielinger, C. Noguet and M. Tapiero, “Investigation of Deep Levels in HighResistivity Bulk Materials by PhotoInduced Current Transient Spectroscopy: I. Review and Analysis of Some Basic Problems,” J. Phys. D.: Appl. Phys. 19, 57–70, Jan. 1986; J.C. Balland, J.P. Zielinger, M. Tapiero, J.G. Gross and C. Noguet, “Investigation of Deep Levels in HighResistivity Bulk Materials by PhotoInduced Current Transient Spectroscopy: II. Evaluation of Various Signal Processing Methods,” J. Phys. D.: Appl. Phys. 19, 71–87, Jan. 1986. 101. P.M. Petroff and D.V. Lang, “A New Spectroscopic Technique for Imaging the Spatial Distribution of Nonradiative Defects in a Scanning Transmission Electron Microscope,” Appl. Phys. Lett. 31, 60–62, July 1977. 102. O. Breitenstein, “A Capacitance Meter of High Absolute Sensitivity Suitable for Scanning DLTS Application,” Phys. Stat. Sol. 71a, 159–167, May 1982. 103. K. Wada, K. Ikuta, J. Osaka and N. Inoue, “Analysis of Scanning Deep Level Transient Spectroscopy,” Appl. Phys. Lett. 51, 1617–1619, Nov. 1987. 104. J. Heydenreich and O. Breitenstein, “Characterization of Defects in Semiconductors by Combined Application of SEM (EBIC) and SDLTS,” J. Microsc. 141, 129–142, Feb. 1986. 105. K. Dmowski, B. Lepley, E. Losson, and M. El Bouabdellati, “A Method to Correct for Leakage Current Effects in Deep Level Transient Spectroscopy Measurements on Schottky Diodes,” J. Appl. Phys. 74, 3936–3943, Sept. 1993. 106. D.S. Day, M.J. Helix, K. Hess and B.G. Streetman, “Deep Level Transient Spectroscopy for Diodes with Large Leakage Currents,” Rev. Sci. Instrum. 50, 1571–1573, Dec. 1979. 107. E. Simoen, K. De Backker, and C. Claeys, “DeepLevel Transient Spectroscopy of Detector Grade High Resistivity, Float Zone Silicon,” J. Electron. Mat. 21, 533–541, May 1992. 108. A. Broniatowski, A. Blosse, P.C. Srivastava and J.C. Bourgoin, “Transient Capacitance Measurements on Resistive Samples,” J. Appl. Phys. 54, 2907–2910, June 1983. 109. T. Thurzo and F. Dubecky, “On the Role of the Back Contact in DLTS Experiments with Schottky Diodes,” Phys. Stat. Sol. 89a, 693–698, June 1985. 110. J.H. Zhao, J.C Lee, Z.Q. Fang, T.E. Schlesinger and A.G. Milnes, “The Effects of the Nonabrupt Depletion Edge on DeepTrap Profiles Determined by DeepLevel Transient Spectroscopy,” J. Appl. Phys. 61, 5303–5307, June 1987; errata ibid. p. 5489. 111. S.D. Brotherton, “The Width of the NonSteady State Transition Region in Deep Level Impurity Measurements,” SolidState Electron. 26, 987–990, Oct. 1983. 112. D. Stievenard and D. Vuillaume, “Profiling of Defects Using Deep Level Transient Spectroscopy,” J. Appl. Phys. 60, 973–979, Aug. 1986. 113. D.C. Look, Z.Q. Fang, and J.R. Sizelove, “Convenient Determination of Concentration and Energy Level in DeepLevel Transient Spectroscopy,” J. Appl. Phys. 77, 1407–1410, Feb. 1995; “Depletion Approximation in Semiconductor Trap Filling Analysis: Application to EL2
REFERENCES
114. 115. 116.
117.
118.
119. 120.
121.
122.
123. 124.
125. 126. 127. 128.
129. 130. 131. 132.
307
in GaAs,” SolidState Electron. 39, 1398–1400, Sept. 1996; D.C. Look and J.R. Sizelove, “Depletion Width and Capacitance Transient Formulas for Deep Traps of High Concentration,” J. Appl. Phys. 78, 2848–2850, Aug. 1995. K.B. Nielsen and E. Andersen, “Significance of Blackbody Radiation in DeepLevel Transient Spectroscopy,” J. Appl. Phys. 79, 9385–9387, June 1996. L.R. Weisberg and H. Schade, “A Technique for Trap Determination in LowResistivity Semiconductors,” J. Appl. Phys. 39, 5149–5151, Oct. 1968. M.G. Buehler and W.E. Phillips, “A Study of the Gold Acceptor in a Silicon p+ n Junction and an nType MOS Capacitor by Thermally Stimulated Current and Capacitance Measurements,” SolidState Electron. 19, 777–788, Sept. 1976. C. Dehn, H. Feick, P. Heydarpoor, G. Lindstr¨om, M. Moll, C. Sch¨utze, and T. Schulz, “Neutron Induced Defects in Silicon Detectors Characterized by DLTS and TSC,” Nucl. Instrum. Meth. A377, 258–274, Aug. 1996. C. Szeles and K.G. Lynn, “PositronAnnihilation Spectroscopy,” in Encycl. Appl. Phys. 14, 607–632, 1996; R. KrauseRehberg and H.S. Leipner, Positron Annihilation in Semiconductors, Springer, Berlin, 1999. P. AsokaKumar, K.G. Lynn, and D.O. Welch, “Characterization of Defects in Si and SiO2 Si Using Positrons,” J. Appl. Phys. 76, 4935–4982, Nov. 1994. M. Fujinami, A. Tsuge, and K. Tanaka, “Characterization of Defects in SelfIon Implanted Si Using Positron Annihilation Spectroscopy and Rutherford Backscattering Spectroscopy,” J. Appl. Phys. 79, 9017–9021, June 1996. M. Fujinami, T. Miyagoe, T. Sawada, and T. Akahane, “Improved Depth Profiling With Slow Positrons of Ion implantationinduced Damage in Silicon,” J. Appl. Phys. 94, 4382–4388, Oct. 2003. A. Rich and J. Van House, “Positron Microscopy,” in Encycl. Phys. Sci. Technol., Academic Press, 13, 365–372, 1992; G.R. Brandes, K.F. Canter, T.N. Horsky, P.H. Lippel, and A.P. Mills, Jr., “Scanning Positron Microscopy,” Rev. Sci. Instrum. 59, 228–232, Feb. 1988. F. Reif, Fundamentals of Statistical and Thermal Physics, McGrawHill, New York, 1965, 161–166. O. Engstr¨om and A. Alm, “Thermodynamical Analysis of Optimal Recombination Centers in Thyristors,” SolidState Electron. 21, 1571–1576, Nov./Dec. 1978; “Energy Concepts of InsulatorSemiconductor Interface Traps,” J. Appl. Phys. 54, 5240–5244, Sept. 1983. C.D. Thurmond, “The Standard Thermodynamic Functions for the Formation of Electrons and Holes in Ge, Si, GaAs, and GaP,” J. Electrochem. Soc. 122, 1133–1141, Aug. 1975. J.A. Van Vechten and C.D. Thurmond, “Entropy of Ionization and Temperature Variation of Ionization Levels of Defects in Semiconductors,” Phys. Rev. B14, 3539–3550, Oct. 1976. A. Mircea, A. Mitonneau and J. Vannimenus, “Temperature Dependence of Ionization Energies of Deep Bound States in Semiconductors,” J. Physique 38, L41–L43, Jan. 1972. F. Hasegawa, “A New Method (the ThreePoint Method) of Determining Transient Time Constants and Its Application to DLTS,” Japan. J. Appl. Phys. 24, 1356–1358, Oct. 1985; J.M. Steele, “Hasegawa’s Three Point Method for Determining Transient Time Constant,” Japan. J. Appl. Phys. 25, 1136–1137, July 1986. P.C. Mangelsdorf, Jr., “Convenient Plot for Exponential Functions with Unknown Asymptotes,” J. Appl. Phys. 30, 442–443, March 1959. A.A. Istratov and O.F. Vyvenko, “Exponential Analysis in Physical Phenomena,” Rev. Sci. Instrum. 70, 1233–1257, Feb. 1999. C. Lanczos, Applied Analysis, PrenticeHall, Englewood Cliffs, NJ, 1959, 272 ff–. J.L. Benton and L.C. Kimerling, “Capacitance Transient Spectroscopy of Trace Contamination in Silicon,” J. Electrochem. Soc. 129, 2098–2102, Sept. 1982.
308
DEFECTS
133. V. Pandian and V. Kumar, “Singlegate Deep Level Transient Spectroscopy Technique,” J. Appl. Phys. 67, 560–563, Jan. 1990. 134. E. Losson and B. Lepley, “New Method of Deep Level Transient Spectroscopy Analysis: A Five Emission Rate Method”, Mat. Sci. Eng. B20, 214–220, June 1993.
PROBLEMS 5.1
Using t2 t1 C0 nT (0) exp((Ec − ET )/kT ) exp − − exp − τe T = ; δC = γn σn 2ND τe τe t1 t2 − exp − = C0 exp − τe τe 2
(a) Show that when δC is plotted versus temperature, the peak DLTS value, δCmax , occurs for t1 (r − 1) t2 − t1 = where r = t2 /t1 . τe = ln(t2 /t1 ) ln(r) (b) Show that δCmax = C0 ((1 − r)/r r/(r−1) ). Hint: Define x = exp(−t1 /τe ). 5.2
Using the equations in Problem 5.1, (a) Show that when t2 ≫ t1 , E ln(Co /δC) ≈ ln(γn σn t1 ) − where E = EC − ET . 2 T kT ln(Co /δC) (b) Show that a plot of ln versus 1/T allows E and σn to be T2 extracted. ln
(c) Plot δC versus T for Co = 10−13 F , E = 0.4 eV, σn = 10−15 cm2 , and γn = 1.07 × 1021 cm−2 s−1 K−2 , for t1 = 1 ms and r = 2, 5, 10, 100, and 500. Plot all five curves on the same figure. ln(Co /δC) versus 1/T for the high temperature branch of the δCT (d) Plot ln T2 curve of (iii) for r = 500 and extract E and σn . This technique is discussed in Ref. 133. 5.3
In the boxcar DLTS approach, the peak of the δCT curve is used to determine τe and the relevant temperature T for points on an Arrhenius plot. This gives only one point per temperature scan. More data points lead to better Arrhenius plots. One way to obtain more data points is to use more points of a given δCT curve than just the peak value. For example, one can use points at δCmax , 0.75δCmax , and 0.5δCmax , as shown in the Fig. P5.3. We know that τe (δCmax ) = (t2 − t1 )/ ln(t2 /t1 ) = t1 (r − 1)/ ln(r) (see Eq. (5.49). Determine the two values each for:
PROBLEMS
309
C
0.5 δCmax 0.75 δCmax δCmax
T(Κ)
Fig. P5.3
(a) τe,0.5 = τe (0.5δCmax ) (b) τe,0.75 = τe (0.75δCmax ), all four in terms of t1 for r = 2. This technique is discussed in Ref. 134. The deeplevel transient spectroscopy (DLTS) curve in Fig. P5.4 was obtained by the boxcar method on a Schottky barrier diode on an ntype Si substrate for t1 = 0.5 ms, t2 = 1 ms. 0 −1 × 1015 Peak 1 −2 × 1015 dC (F)
5.4
−3 × 1015 t1 = 0.5 ms, t2 = 1 ms −4 × 1015 150
200
250
300 T (K)
Peak 2 350
400
450
Fig. P5.4
Other curves gave: t1 (ms) 0.5 1 2 4 8
t2 (ms) 1 2 4 8 16
T1 max (K) 234 227 220 213 207
δC1 max (F ) −15
−1.25 × 10 −1.25 × 10−15 −1.25 × 10−15 −1.25 × 10−15 −1.25 × 10−15
T2 max (K)
δC2 max (F )
376 364 352 341 331
−3.125 × 10−15 −3.125 × 10−15 −3.125 × 10−15 −3.125 × 10−15 −3.125 × 10−15
Determine E = Ec − ET , NT and the intercept σn for both peaks. C0 = 5 × 10−12 F , ND = 1015 cm−3 , γn = 1.07 × 1021 cm−2 s−1 K−2 .
310
5.5
DEFECTS
The capacitance transients for peak 2 in Problem 5.4, were measured for filling pulse widths tf = 5 ns and tf = ∞, for t1 = 1 ms and t2 = 2 ms. Other curves gave:
tf (ns) δC (F )
0.5 5.9 × 10−17
1 1.15 × 10−16
2 2.19 × 10−16
3 3.31 × 10−16
5 4.77 × 10−16
7 6.13 × 10−16
10 7.72 × 10−16
20 1.07 × 10−15
∞ 1.25 × 10−15
Determine τc , cn , σn and NT from these data. Use vth = 107 (T /300)0.5 , n ≈ ND . 5.6
Consider a Schottky diode at zero bias with deeplevel impurities NT . Light is incident on this device generating electronhole pairs uniformly. All deeplevel impurities are filled with holes while the light is “on” as shown in Fig. P5.6(a). Then at t = 0, the light is turned off and a reversebias voltage V1 is applied simultaneously. ntype
V
Ec ET Ev
NT
(a) −V1 Draw occupancy of N T in the spacecharge region
W(t = 0+)
(b)
−V1 Draw band diagram and occupancy of NT
(c)
Fig. P5.6
PROBLEMS
311
(a) On the band diagram, Fig. P5.6(b), draw the occupancy of NT at t = 0+ , i.e., immediately after the light is turned off. (b) Draw the band diagram and the occupancy of NT as t → ∞ in Fig. P5.6(c). In both cases concern yourself only with the spacecharge region. Don’t worry about the quasineutral region. The deeplevel impurities are acceptors, NT < ND . The deeplevel transient spectroscopy data in Fig. P5.7(a) were obtained by the boxcar method on a Schottky barrier diode on an ntype Si substrate. γn = 1.07 × 1021 cm−2 s−1 K−2 , ND = 1015 cm−3 , Co = 1 pF. In this device it is known that the emission rate can be represented by en = σn vth Nc exp(−E/kT ), where σn = σno exp(−Eb /kT ) The data for σn versus T are given in Fig. P5.7(b). Determine E = Ec − ET , NT , σno , and Eb . (See Appendix 5.1) 0
t1 = 0.5 ms, t2 = 1 ms 1/2 2/4 4/8 8/16
−5 × 10−15
−1 × 10−14
−1.5 × 10−14
−2 × 10−14 220
240
260
280
250
300
T (K) (a) 10−15
10−16 σn (cm2)
δC (F)
5.7
10−17
10−18 150
200 T (K) (b)
Fig. P5.7
312
5.8
DEFECTS
Plot δC versus T (150K ≤ T ≤ 300K), similar to Fig. P5.7(a), using the boxcar DLTS Eq. (5.48) for an nSi sample with two energy levels in the band gap using the values: γn = 1.07 × 1021 cm−2 s−1 K−2 ,
ND = 1015 cm−3 , Co = 1 pF, E1 = 0.25 eV, E2 = 0.4 eV, σn1 = 10−16 cm2 , σn2 = 10−15 cm2 ,
NT 1 = 5 × 1012 cm−3 , NT 2 = 8 × 1012 cm−3 , t1 = 1 ms, t2 = 2 ms. 5.9
The deeplevel transient spectroscopy data in Fig. P5.9 were obtained by the boxcar method on a Schottky barrier diode on a ptype Si substrate. The diode area is 0.02 cm2 and the diode bias voltage was varied from zero to reverse bias voltage of 5V during the measurement. Ks = 11.7, γp = 1.78 × 1021 cm−2 s−1 K−2 , NA = 1015 cm−3 , Vbi = 0.87 V. Determine ET − Ev , NT , and the intercept σp for each of the impurities. 0.0 × 100
δC (F)
−5.0 × 10−15 −1.0 × 10−14 t1 = 0.5 ms, t2 = 1 ms 1 = ms, 2 ms 2 = ms, 4 ms 4 = ms, 8 ms
−1.5 × 10−14 −2.0 × 10−14 150
200
250 Τ (Κ)
300
350
Fig. P5.9
5.10 Determine and plot δC versus T for a Schottky diode on an ntype Si substrate containing two types of impurities. Use the following parameters: γn = 1.07 × 1021 cm−2 s−1 K−2 , ND = 5 × 1015 cm−3 , Co = 104 pF. Impurity 1 : Ec − ET 1 = 0.3 eV, NT 1 = 1012 cm−3 , σn1 = 10−15 cm2 ;
Impurity 2 : Ec − ET 2 = 0.5 eV, NT 2 = 5 × 1011 cm−3 , σn2 = 5 × 10−16 cm2 .
Use the boxcar equations with t1 = 1 ms, t2 = 2 ms and the temperature range 150 ≤ T ≤ 350 K. 5.11 A deeplevel acceptor impurity is diffused uniformly into an ntype Si wafer. The wafer was originally doped with arsenic to ND = 1015 cm−3 . Calculate and plot the resistivity versus deeplevel impurity density (1014 ≤ NT ≤ 1017 cm−3 ) on a loglog plot for ET = 0.46, 0.56, and 0.66 eV. Plot all three curves on one figure to compare.
PROBLEMS
313
You have to first solve for EF using the equations below. Knowing EF you can then find n and p and then determine ρ. Charge neutrality requires − p + n+ D − n − nT = 0
where p = ni exp((Ei − EF )/kT ); n = ni exp((EF − Ei )/kT ) n+ D = ρ=
NT ND ; n− T = 1 + exp((EF − ED )/kT ) 1 + exp((ET − EF )/kT ) 1 q(µn n + µp p)
Use: ND = 1015 cm−3 , ni = 1010 cm−3 , T = 300 K, µn = 1400 cm2 /V s, µp = 450 cm2 /V s, EG = 1.12 eV, Ei = 0.56 eV, ED = Ec − 0.045 eV. It is easiest to use Ev = 0 as a reference energy. 5.12 The deeplevel transient spectroscopy data in Fig. P5.12 were obtained on a Schottky barrier diode on an ntype Si substrate containing two impurities. γn = 1.07 × 1021 cm−2 s−1 K−2 , ND = 1015 cm−3 , C0 = 1 pF. Determine E = Ec − ET , σn , and NT for each deeplevel impurity. 0
−1 × 10−17 δC (F)
0.5 ms, 1 ms 1 ms, 2 ms −2 × 10−17
2 ms, 4 ms t1 = 4 ms, t2 = 8 ms
−3 × 10−17 150
200
250
300
350
400
T (K)
Fig. P5.12
5.13 Consider interface trapped charge or interface state density Dit at the SiO2 /Si interface of an MOS device. The device is heavily inverted and all interface states are filled with electrons. Determine the density of interface states still filled with electrons, Nit = Dit E, 100 µs after the surface is driven into depletion and electrons are emitted from interface states during the 100 µs. Dit = 5 × 1010 cm−2 eV −1 , T = 300 K, σn = 10−15 cm2 , vth = 107 cm/s, Nc = 2.5 × 1019 cm−3 , k = 8.617 × 10−5 eV/K, EG (Si) = 1.12 eV. The electron emission time constant from interface states at energy Eit is given by τe =
exp[(Ec − Eit )/kT ] σn vth Nc
314
DEFECTS
5.14 The Arrhenius plot of a deeplevel impurity in Si is shown in Fig. P5.14. Determine Ec − ET and σn . 1010
τeT2 (sK2)
108
106
104 102 0.003
0.004
0.005
0.006
0.007
1/T (K−1)
Fig. P5.14
Use γn = 1.07 × 1021 cm−2 s−1 K−1 , k = 8.617 × 10−5 eV/K. NT C(t) =1− exp(−t/τe ) for ND = 1015 Co 2ND cm−3 , NT = 5 × 1012 cm−3 , σn = 10−15 cm2 , Ec − ET = 0.35 eV, γn = 1.07 × 1021 cm−2 s−1 K−1 , for T = 200 K, 225 K and 250 K over the time interval: 0 < t < 0.002 s.
5.15 Calculate and plot C(t)/Co given by
5.16 A Schottky diode on an ntype substrate, containing a deeplevel impurity, is zero biased for some time. Next, the device is reverse biased at t = 0. The charge density in the reversebiased spacecharge region at t = 0+ , immediately after applying the reversebias pulse, is ρ = qND . The deeplevel impurity is: donor acceptor. Give your reason. 5.17 Identify the two deeplevel impurities in Fig. P 5.17.
Neutral
EC
EC
ET
ET
EV
(i)
Neutral
EV
(ii)
Fig. P5.17
Deeplevel impurity (i) is a: donor acceptor. Give your reason. Deeplevel impurity (ii) is a: donor acceptor. Give your reason.
PROBLEMS
315
5.18 There are two defects in the transmission electron micrograph in Fig. P 5.18.
Fig. P5.18
Identify them and state whether they are point, line, plane, or volume defects. 5.19 A DLTS plot of δC versus T is shown in Fig. P5.19 for a certain impurity with energy level ET = ET 1 and density NT = NT 1 . On the same figure draw the curve for an impurity with ET = ET 2 > ET 1 and NT = NT 2 < NT 1 . t2 /t1 is unchanged. 0
δC (pF)
−0.01
−0.02
−0.03
−0.04 200
t1 = 5 × 10−4 s t2 = 10−3 s
220
240 260 Temperature (K)
280
300
Fig. P5.19
5.20 A DLTS plot of δC versus T is shown in Fig. P5.19. On the same figure draw the curve when both t1 and t2 are increased, but t2 /t1 is unchanged.
316
DEFECTS
5.21 Consider an ntype semiconductor doped with ND donor atoms/cm3 with energy level ED shown in “Before” in Fig. P5.21. All donors are ionized. Next, a deeplevel impurity at energy level ET is introduced into the ntype semiconductor wafer, shown in “After”. The deeplevel impurity is a: donor acceptor. Give your reason. The wafer resistivity: increases decreases remains unchanged. Give your reason. +
+
+
+
+
EC ED EF
+
+
+
+ ET
EV
Before
+
After
EC ED EF EV
Fig. P5.21
5.22 The DLTS spectrum of impurity 1 in an ntype semiconductor is shown in Fig. P5.22. It has an energy level ET 1 , density NT 1 , and capture cross section σn1 .
T (a)
δC
δC
ln(τeT 2)
(a) Show the effect of decreasing σn1 on the spectrum in Fig. P5.22(a) and on the ln(τe T 2 ) − 1/T plot in Fig. P5.22(b). (b) On Fig.5.22(c), draw the DLTS spectrum for impurity 2 with energy level ET 2 , where Ec − ET 2 < Ec − ET 1 , NT 2 < NT 1 , and σn2 = σn1 in this case.
1/T (b)
Fig. P5.22
REVIEW QUESTIONS • Name some common defects in Si wafers.
• What do metallic impurities do in Si devices? • Name some defect sources.
• What are point defects? Name three point defects.
• Name a line defect, an area defect, and a volume defect. • How do oxidationinduced stacking faults originate?
• Why is emission generally slower than capture? • What determines the capacitance transient?
T (c)
REVIEW QUESTIONS
317
• Where does the energy for thermal emission come from?
• Why do minority and majority carrier emission have opposite behavior? • What is deeplevel transient spectroscopy (DLTS)? • What parameters can be determined with DLTS? • What advantage does Laplace DLTS have?
• What is positron annihilation spectroscopy and for what defect measurement is it
most useful?
6 OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
6.1
INTRODUCTION
The discussions in this chapter are applicable to all insulatorsemiconductor systems. However, the examples are generally directed at the SiO2 Si system. The most important aspect of device scaling for this chapter is the thinner oxide with each successive technology node. Thin oxides with their respective higher leakage currents, have a pronounced effect on many of the methods in this chapter. Capacitancevoltage and oxide thickness measurements must be more carefully interpreted for thin, leaky oxides. Oxide Charges:1 There are four general types of charges associated with the SiO2 Si system shown on Fig. 6.1. They are fixed oxide charge, mobile oxide charge, oxide trapped charge and interface trapped charge. This nomenclature was standardized in 1978. The abbreviations of the various charges are given below. In each case, Q is the net effective charge per unit area at the SiO2 Si interface (C/cm2 ), N is the net effective number of charges per unit area at the SiO2 Si interface (number/cm2 ), and Dit is given in units of number/cm2 ·eV. N = Q/q, where Q can be positive or negative, but N is always positive. (1) Interface Trapped Charge (Qit , Nit , Dit ): These are positive or negative charges, due to structural defects, oxidationinduced defects, metal impurities, or other defects caused by radiation or similar bond breaking processes (e.g., hot electrons). The interface trapped charge is located at the Si–SiO2 interface. Unlike fixed charge or trapped charge, interface trapped charge is in electrical communication with the underlying silicon. Interface traps can be charged or discharged, depending on the surface potential. Most of the interface trapped charge can be neutralized by lowtemperature (∼450◦ C) hydrogen or Semiconductor Material and Device Characterization, Third Edition, by Dieter K. Schroder Copyright 2006 John Wiley & Sons, Inc.
319
320
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
+
+ + x
SiO2
(3)
(4) x (1)
+
x
+
x
(2)
+ Si
Fig. 6.1 Charges and their location for thermally oxidized silicon. Reprinted after Deal by permission of IEEE ( 1980, IEEE).
forming gas (hydrogen/nitrogen mixture) anneals. This charge type has been called surface states, fast states, interface states and so on. It has been designated by Nss , Nst and other symbols in the past. (2) Fixed Oxide Charge (Qf , Nf ): This is a positive charge near the Si–SiO2 interface. The charge density, whose origin is related to the oxidation process, depends on the oxidation ambient and temperature, cooling conditions, and on silicon orientation. Since the fixed oxide charge cannot be determined unambiguously in the presence of moderate densities of interface trapped charge, it is usually measured after a lowtemperature (450◦ C) hydrogen or forming gas anneal which minimizes interface trapped charge. The fixed oxide charge is not in electrical communication with the underlying silicon. Qf depends on the final oxidation temperature. The higher the oxidation temperature, the lower is Qf . However, if it is not permissible to oxidize at high temperatures, it is possible to lower Qf by annealing the oxidized wafer in a nitrogen or argon ambient after oxidation. This has resulted in the wellknown “Deal triangle” in Fig. 6.2, which shows the reversible relationship between Qf and oxidation and annealing.2 An oxidized sample may be prepared at any temperature and then subjected to dry oxygen at any other temperature, with the resulting value of Qf being associated with the final temperature and any Qf value resulting from a previous oxidation can be reduced to a constant value. Fixed charge was often designated as Qss in the past.
1 × 1012
Qf /q (cm−2)
8 × 1011
Dry O2
6 × 1011
Dry N2 or Ar
4 × 1011 2 × 1011 0 500
700
900 1100 Temperature (°C)
1300
Fig. 6.2 “Deal triangle” showing the reversibility of heat treatment effects on Qf . Reprinted after Deal et al.2 with permission of the publisher, the Electrochemical Society, Inc.
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
321
(3) Oxide Trapped Charge (Qot , Not ): This positive or negative charge may be due to holes or electrons trapped in the oxide. Trapping may result from ionizing radiation, avalanche injection, FowlerNordheim tunneling, or other mechanisms. Unlike fixed charge, oxide trapped charge is sometimes annealed by lowtemperature ( 0 and Uˆ s = −1 for Us < 0. The intrinsic Debye length LDi is LDi =
Ks ε0 kT 2q 2 ni
(6.10)
The highfrequency C –V curve results when the minority carriers in the inversion charge are unable to follow the ac voltage. The majority carriers at the scr edge are able to follow the ac signal thereby exposing more or less ionized dopant atoms. The dc voltage sweep rate, given by Eq. (6.5), must be sufficiently low to generate the necessary inversion charge. The highfrequency semiconductor capacitance in inversion is3
CS,hf = Uˆ S
Ks ε0 [eUF (1 − e−US ) + e−UF (eUS − 1)/(1 + δ)] 2LDi F (Us , UF )
(6.11)
with δ given by δ=
US 0
(eUS − US − 1)/F (US , UF ) eUF (1 − e−U )(eU − U − 1) dU 2[F (U, UF )]3
(6.12)
An approximate expression, accurate to 0.1–0.2% in strong inversion, is4
CS,hf =
q 2 Ks εo NA 2kT {2UF  − 1 + ln[1.15(UF  − 1)]}
(6.13)
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
325
When the dc bias voltage is changed rapidly with insufficient time for inversion charge generation, the deepdepletion curve results. Its high or lowfrequency semiconductor capacitance is CS,dd = √
Cox [1 + 2(VG − VF B )/V0 ] − 1
(6.14)
where V0 = qK s ε0 NA /Cox 2 . The total capacitance is given by C=
Cox CS Cox + CS
(6.15)
The gate voltage is related to the oxide voltage, the surface potential, and the flatband voltage VF B through the relationship kT Ks tox F (US , UF ) VG = VF B + φs + Vox = VF B + φs + Uˆ S qKox LDi
(6.16)
Ideal lowfrequency (lf), highfrequency (hf) and deep depletion (dd) C –V curves are shown in Fig. 6.5 for Qit = 0 and VF B = 0. They coincide in accumulation and depletion but deviate in inversion, because the inversion charge is unable to follow the applied ac voltage for the hf case and does not exist for the dd case. Which of these three curves is obtained during a C –V measurement depends on the measurement conditions. Consider an MOSC on a psubstrate with the dc gate voltage swept from negative to positive voltages. Superimposed on the dc voltage is an ac voltage of typically 10–15 mV amplitude. All three curves are identical in accumulation and depletion. The curves deviate from one another when the device enters inversion. If the dc voltage is swept sufficiently slowly to allow the inversion charge to form and if the ac voltage is of a sufficiently low frequency for the inversion charge to be able to respond to the ac probe frequency, then the lowfrequency curve is obtained. If the dc voltage is
1
1
0.8
CFB/Cox C/Cox
C/Cox
0.8
Clf
0.6 0.4
Chf
0.2 0
−3
−1 1 3 Gate Voltage (V) (a)
0.6 0.4
Chf
0.2
Cdd −5
CFB/Cox Clf
5
0
Cdd −5
−3
−1 1 3 Gate Voltage (V)
5
(b)
Fig. 6.5 Lowfrequency (lf), highfrequency (hf), and deepdepletion (dd) normalized SiO2 Si capacitancevoltage curves of an MOSC; (a) psubstrate NA = 1017 cm−3 , (b) nsubstrate ND = 1017 cm−3 , tox = 10 nm, T = 300 K.
326
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
50
200
Capacitance (pF)
Capacitance (pF)
250
150 100 50 0 −3
−2
−1 0 1 Gate Voltage (V) (a)
2
3
0.03 V/s
40
Equilibrium Deep Depletion
30
20
0.3 V/s 3 V/s
0
0.5
1 1.5 2 2.5 Gate Voltage (V)
3
(b)
Fig. 6.6 Effect of sweep direction and sweep rate on the hf MOSC capacitance on psubstrate, (a) entire C –VG curve, (b) enlarged portion of (a) showing the dc sweep direction; f = 1 MHz. Data courtesy of Y.B. Park, Arizona State University.
swept sufficiently slowly to allow the inversion charge to form but the ac probe frequency is too high for the inversion charge to be able to respond, then the highfrequency curve is obtained. The deepdepletion curve obtains for either high or lowfrequency if the dc sweep rate is too high and no inversion charge can form during the sweep. The most commonly measured curve is the highfrequency curve. However, the true hf curve is not always easy to obtain. Consider the C –VG curve in Fig. 6.6. The true or equilibrium curve is shown by the dashed line. If the bias is swept from −VG to +VG there is a tendency for the C –V curve to go into partial deep depletion and the resulting curve will be below the true curve, especially for high generation lifetime material. We showed the limitation on the ac frequency in Eq. (6.5). This limitation also holds for the dc bias sweep rate; the sweep rate for high lifetime material must be extremely low. When the bias is swept from +VG to −VG , inversion charge is injected into the substrate. The inversion layer/substrate junction becomes forward biased and the resulting capacitance will be above the true curve. The true curve is, in general, only obtained by setting the bias voltage and waiting for the device to come to equilibrium, then repeating this procedure to generate the C –V curve pointbypoint. If the pointbypoint procedure is inconvenient, then the +VG → −VG sweep direction is preferred for psubstrates since the deviation of the capacitance from its true value is generally less than it is for the −VG → +VG sweep.
Exercise 6.1 Problem: What happens to Chf when the measurement temperature is raised? Solution: According to Eq. (6.5) the minority carriers respond to higher sweep rates when ni increases and they respond to higher probe frequencies as T increases, i.e., low frequency behavior should be observed at high probe frequencies. This is illustrated in Fig. E6.1. The data points are experimental data and the solid lines are calculated lf curves. At room temperature the hf curve is measured and there is large discrepancy between the measured and calculated lf curves. As temperature increases, some of the inversion layer carriers are able to respond and the hf curve begins to show lf characteristics. Finally
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
327
1 300°C 0.8
C/Cox
200°C T = 300°C
0.6 0.4
200°C
175°C
0.2
25°C 25°C
0 −5
−4
−3
−2 −1 0 Gate Voltage (V)
1
2
3
Fig. E6.1 Measured hf (points) and calculated lf (lines) curves of an MOSC. ND = 2.6 × 1014 cm−3 , tox = 30 nm, f = 10 kHz. Data courtesy of S.Y. Lee, Arizona State University.
at T = 300◦ C, the hf curve coincides with the lf curve. Hence Chf and Clf measured at T = 300◦ C are identical in this example. The temperature at which this happens, also depends on parameters other than ni , e.g., τg , W , and Cox .
6.2.2
Flatband Voltage
The flatband voltage is determined by the metalsemiconductor work function difference φMS and the various oxide charges through the relation VF B = φMS −
Qit (φs ) 1 tox x 1 tox x Qf − − ρm (x) dx − ρot (x) dx 0 Cox Cox Cox tox Cox 0 tox
(6.17) where ρ(x) = oxide charge per unit volume. The fixed charge Qf is located very near the Si–SiO2 interface and is considered to be at that interface. Qit is designated as Qit (φs ), because the occupancy of the interface trapped charge depends on the surface potential. Mobile and oxide trapped charges may be distributed throughout the oxide. The xaxis is defined in Fig. 6.3. The effect on flatband voltage is greatest, when the charge is located at the oxidesemiconductor substrate interface, because then it images all of its charge in the semiconductor. When the charge is located at the gateoxide interface, it images all of its charge in the gate and has no effect on the flatband voltage. For a given charge density, the flatband voltage is reduced as the oxide capacitance increases, i.e., for thinner oxides. Hence, oxide charges usually contribute little to flatband or threshold voltage shifts for thinoxide MOS devices. The flatband voltage of Eq. (6.17) is for a uniformly doped substrate, with the gate voltage referenced to the grounded back contact. For an epitaxial layer of doping density Nepi on a substrate of doping density Nsub , the builtin potential at the episubstrate junction modifies the flatband voltage to5 Nsub kT ln (6.18) VF B (epi ) = VF B (bulk ) ± 2q Nepi
328
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
1 1000 nm 500 nm 200 nm 100 nm 50 nm 20 nm 10 nm 7 nm 5 nm 3 nm tox = 2nm
CFB/Cox
0.8 0.6 0.4 0.2 0 1014
1015
1016 NA
Fig. 6.7
1017
1018
1019
(cm−3)
CF B /Cox versus NA as a function of tox for the SiO2 Si system at T = 300 K.
The plus sign in Eq. (6.18) is for ptype and the minus sign for ntype material, assuming the substrate and the epitaxial layer doping densities are of the same type, either both acceptors or both donors. To determine the various charges, one compares theoretical and experimental capacitancevoltage curves. The experimental curves are usually shifted with respect to the theoretical curves as a result of the charges and the work function difference of Eq. (6.17). The voltage shift can be measured at any capacitance, however, it is frequently measured at the flatband capacitance CF B and is designated the flatband voltage VF B . For ideal curves, VF B is zero. The flatband capacitance is given by Eq. (6.15) with CS = Ks εo /LD , where LD = [kT K s εo /q 2 (p + n)]1/2 ≈ [kT K s εo /q 2 NA ]1/2 is the Debye length defined in Eq. (2.11). For Si with SiO2 as the insulator, CF B normalized by Cox , is given as √ −1 136 T /300 CF B = 1+ √ Cox tox NA or ND
(6.19)
with tox in cm and NA (ND ) in cm−3 . In Fig. 6.7, CF B /Cox is plotted versus NA as a function of oxide thickness. The flatband capacitance can be easily calculated when the doping density is uniform and when the wafer is sufficiently thick. The calculation becomes more difficult when the doping is nonuniform and numerical techniques may have to be employed.6 For thin silicon layers, e.g., silicononinsulator, the active semiconductor layer may be so thin that it cannot accommodate the spacecharge region of the MOSC. Then special precautions must be used to determine CF B . Graphical and analytical methods have been used.7 The analytical methods rely on a measure of the capacitance, which is 90% or 95% of the oxide capacitance. The voltage for this capacitance is then related to the flatband voltage.8
Exercise 6.2 Problem: Determine the flatband voltage of an MOS capacitor. Solution: The flatband voltage must be accurately known to determine CF B . Calculating CF B , as described, allows VF B to be determined, provided all the parameters in Eq. (6.17)
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
329
25 1/(Chf/Cox)2
VFB 20 d[1/(Chf/Cox)2]/dVG 15
•
10 5 0 −3
−2
−1
0
1
2
3
Gate Voltage (V) Fig. E6.2
are well known. That may not always be the case. One way to determine VF B experimentally is to plot (1/Chf )2 or 1/(Chf /Cox )2 versus VG as shown in Fig. E6.2. This curve corresponds to the data in Fig. 6.5(a). The lower knee of this curve occurs at VG = VF B . Such a transition is sometimes difficult to determine. Differentiating this curve and finding the maximum slope of the left flank of this differentiated curve occurs at VF B . Differentiating this differentiated curve a second time results in a sharply peaked curve whose peak coincides with VF B . The second differentiation usually introduces a great deal of noise, but smoothing the data helps. This method is discussed in R.J. Hillard, J.M. Heddleson, D.A. Zier, P. RaiChoudhury, and D.K. Schroder, “Direct and Rapid Method for Determining Flatband Voltage from Nonequilibrium Capacitance Voltage Data,” in Diagnostic Techniques for Semiconductor Materials and Devices (J.L. Benton, G.N. Maracas, and P. RaiChoudhury, eds.), Electrochem. Soc., Pennington, NJ, 1992, 261–274. Finite Gate Doping Density. We have so far neglected the effect the gate may have on the C –VG curve, other than the metalsemiconductor work function difference. Polycrystalline Si is a common gate material, with doping densities around 1019 –1020 cm−3 . What is the effect of this? Consider the MOSC in Fig. 6.8, consisting of a ptype substrate and an n+ polysilicon gate. For negative gate voltage, substrate and gate are accumulated and we can treat the gate as a metal. However, for positive gate voltage, not only is the substrate depleted and eventually inverted, but the gate can also be depleted and perhaps inverted. Instead of Cox in series with CS , there is now an additional gate capacitance Cgate , reducing overall capacitance. The measurement of gate doping density by a C –V technique is discussed in Chapter 2. The effect of gate depletion is illustrated on the C/Cox –VG curves in Fig. 6.9. Note the additional capacitance drop for +VG . This drop increases as ND in the gate decreases. Such polysilicon gate depletion changes the threshold voltage of MOSFETs, reduces the drain current, and increases the gate resistance. All of these effects reduce circuit speed. On the other hand, gate and source/drain overlap capacitances are also reduced, which tends to increase circuit speed. A recent study has shown the overall effect to be negative, i.e., circuit speed is reduced.9
330
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
−VG
+VG n+ Gate
n+ Gate
Cgate Cox CS
Cox pSubstrate
pSubstrate
Fig. 6.8 Schematic illustration of an MOSC with finite gate doping density, showing gate depletion for positive gate voltage.
1 Metal ND = 2 × 1020
C/Cox
0.8
1020 cm−3 7 × 1019 5 × 1019 2 × 1019
0.6 0.4 tox = 2 nm
0.2 0 −5
NA = 1017 cm−3 −3
−1
1
3
5
Gate Voltage (V)
Fig. 6.9 Lowfrequency capacitancevoltage curves for a metal gate and various n+ polySi gate doping densities. Simulation courtesy of D. Vasileska, Arizona State University.
Exercise 6.3 Problem: How are the C –V curves of MOS devices affected by quantization and FermiDirac statistics? Solution: Equations describing the C –V curves above are frequently derived using simplified assumptions. One modification to these assumptions is the depletion of the polySi gate. Other modifications, significant for sub 10 nm oxide thicknesses, include FermiDirac (F –D) instead of MaxwellBoltzmann statistics and inversion layer quantization. Both of these effects must be considered for devices in strong accumulation or inversion. In this degenerate condition, the free carriers occupy discrete energy states in the conduction band reducing the substrate capacitance. Simulations and experiments confirm these effects. Simulated results are shown in Fig. E6.3, where tox,phys is the physical oxide thickness. These curves include F –D, quantization, and gate depletion effects. The substrate is inverted and the gate accumulated (Cgate = Cinv ) at +VG and for −VG the substrate is accumulated and the gate inverted (Cgate = Cacc ). Cinv is calculated at VG = VF B − 4 V and Cacc is calculated at VG = VF B + 3 V. This figure shows the gate capacitance to be less than the oxide capacitance by at least 10% for tox < 10 nm. Hence extracting oxide thicknesses from C –V measurements will yield incorrect tox if the data are not properly analyzed. These effects are discussed in K.S. Krisch, J.D. Bude, and L. Manchanda,
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
331
1
Cgate/Cox
Metal 0.9 2 × 1020 −VG
1020
+VG
6 × 1019 cm−3
0.8 4
6
8
10
tox,phys (nm)
Fig. E6.3 Simulated Cgate /Cox ratio versus tox,phys for metal and n+ polySi/pSi structure (ND = 1017 cm−3 ). Oxide leakage current is neglected. Simulation courtesy of D. Vasileska, Arizona State University.
“Gate Capacitance Attenuation in MOS Devices With Thin Gate Dielectrics,” IEEE Electron Dev. Lett. 17, 521–524, Nov. 1996; D. Vasileska, D.K. Schroder, and D.K. Ferry, “Scaled Silicon MOSFET’s: Degradation of the Total Gate Capacitance,” IEEE Trans Electron Dev. 44, 584–587, April 1997.
6.2.3
Capacitance Measurements
High Frequency: Highfrequency C –V curves are typically measured at 10 kHz–1 MHz. The basic capacitance measuring circuit in Fig. 6.10 consists of the device to be measured and an output resistor R. The MOS device is represented by the parallel G/C circuit, with G the conductance of the scr and C its capacitance. An ac current i flows through the device and the resistor, giving the output voltage as R RG(1 + RG) + (ωRC)2 + j ωRC R vi = vi = vi −1 Z R + (G + j ωC) (1 + RG)2 + (ωRC)2 (6.20) For RG ≪ 1 and (ωRC)2 ≪ RG, Eq. (6.20) reduces to vo = iR =
vo ≈ (RG + j ωRC)vi
(6.21)
i
G
C
~ vi R
Fig. 6.10
vo
Simplified capacitance measuring circuit.
332
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
S R − +
Vo = −IR
dVG /dt = a Time (a)
Fig. 6.11
I
VG(t)
VG(t)
I
− +
CF Vo = −(C/CF)∆VG
∆VG Time (b)
Block diagram of circuits to measure the current and charge of an MOS capacitor.
The output voltage has two components: the inphase RG and the outofphase j ωRC, with vo = RGv i for the 0◦ phase and ωRCvi for the 90◦ phase components. Using a phase sensitive detector, one can determine the conductance G or the capacitance C, knowing R and ω = 2πf . Low Frequency: CurrentVoltage: The lowfrequency capacitance of an MOSC is usually not obtained by measuring the capacitance, but rather by measuring a current or a charge, because capacitance measurements at low frequencies are very noisy. In the quasistatic or linear ramp voltage method, the current is measured in response to a slowly varying voltage ramp in Fig. 6.11(a).10 The opamp circuit with a resistive feedback connected to the MOSC gate is an ammeter. The resulting displacement current is given by dQG dVG dVG dQG = =C (6.22) I= dt dVG dt dt For a linear voltage ramp, dVG /dt is constant, I is proportional to C, and the lowfrequency C –V curve is obtained, if dVG /dt is sufficiently low.
Exercise 6.4 Problem: What is the effect of gate leakage current on the lf C –V curve? Solution: It is important that the gate leakage current be as low as possible, because gate current adds or subtracts from the displacement current. This leads to an erroneous capacitance, because the current is no longer proportional to the capacitance in that case. The gate capacitor becomes very lossy due to high leakage, and the gate capacitance rolls up or down in the inversion and accumulation regions of the C –V curve and it is no longer possible to extract Cox directly. The rolloff varies with the gate leakage current, so that for two gate dielectrics with the same thickness and different leakage currents, different Cox and tox are obtained. Example C –V curves are shown in Fig. E6.4. A good discussion of these problems can be found in C. Scharrer and Y . Zhao, “High Frequency Capacitance Measurements Monitor EOT (Equivalent Oxide Thickness) of Thin Gate Dielectrics,” Solid State Technol. 47, Febr. 2004.
333
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
1000 tox = 2.9 nm
CG (F)
800 3.9 nm 4.8 nm
600 400 200 0 −4
Fig. E6.4
−3
−2
−1
0 1 VG (V)
2
3
4
Quasistatic curves for no oxide leakage (lines), oxide leakage current (points).
LowFrequency: ChargeVoltage: In the quasistatic I –V method in Fig. 6.11(a), leakage currents are included in the I –V plot. Moreover, the ammeter in conjunction with the capacitor is a differentiator and tends to exaggerate noise spikes or nonlinearities in the voltage ramp. The Q–V quasistatic method alleviates some of the limitations of the I –V quasistatic method. Initially the MOSC was placed in the feedback loop of an opamp and it was charged with a constant current,11 and later modified.12 Analog and digital versions13 have been proposed and a commercial version is shown schematically in Fig. 6.11(b).14 This circuit is an integrator, reducing the effects of spurious signals. The MOSC is connected with its gate to the opamp and its substrate to the voltage source in Fig. 6.11 to minimize stray capacitance and noise. This technique, also called the feedback charge method, uses a voltage step input V to the virtual ground opamp. The capacitance is determined by measuring the transfer of charge in response to this voltage increment. The feedback capacitor CF is initially discharged by closing the lowleakage current switch S. When the measurement starts, S is opened and VG causes charge Q to flow onto capacitor CF , giving the output voltage Q (6.23) Vo = − CF With Q = CVG Vo = −
C VG CF
(6.24)
with the output voltage proportional to the MOSC capacitance. Gain is introduced into the measurement for C > CF by choosing the capacitance ratio C/CF appropriately. Incrementing VG generates a Clf versus VG curve. Additionally, when Q changes, a current Q/t flows. This current should only flow during the transient time period until the device reaches equilibrium. Hence, Q/t is a measure of whether equilibrium has been established and is used to determine the time increments at which VG should be changed to measure the equilibrium lowfrequency C –V curve.14 The method is well suited for MOS measurements since it has high noise immunity, because sizable voltages rather than low currents are measured, and since voltage steps rather than precise linear voltage ramps are used.
334
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
1
C/Cox
0.8
CFB/Cox
0.6
Ideal
0.4 0.2 0 −3
VFB −2
0 −1 Gate Voltage (V)
1
2
Fig. 6.12 Ideal (line) and experimental (points) MOSC curves. NA = 5 × 1016 cm−3 , tox = 20 nm, T = 300 K, CF B /Cox = 0.77.
6.2.4
Fixed Charge
The fixed charge is determined by comparing the flatband voltage shift of an experimental C –V curve with a theoretical curve and measure the voltage shift, as shown in Fig. 6.12. CF B is calculated from Eq. (6.19) or taken from Fig. 6.7, provided the oxide thickness and the doping density are known or determined as in Exercise 6.2. To determine Qf , one should eliminate or at least reduce the effects of all other oxide charges and reduce the interface trapped charge to as low a value as possible. Qit is reduced by annealing in a hydrogen ambient at temperatures around 400–450◦ C. Pure hydrogen is rarely used due to its explosive nature. Forming gas, a hydrogennitrogen mixture (∼5–10% H2 ), is commonly used. When the SiO2 is covered by Si3 N4 , Qit annealing is more difficult due to the imperviousness of the nitride.15 Qf is related to the flatband voltage by the equation Qf = (φMS − VF B )Cox
(6.25)
where φMS must be known in order to determine Qf . Equation (6.25) assumes that interface traps play a negligible role in fixed charge density measurements. Methods to determine φMS are given in Section 6.2.5. The normalized flatband capacitance is 0.77 and VF B = −0.3 V for the example in Fig. 6.12. Since φMS is required to determine Qf from C –V flatband voltage shifts, there is as much uncertainty in the fixed charge as there is in φMS . For example, the uncertainty in Nf = Qf /q, according to Eq. (6.25), is related to the uncertainty in φMS for SiO2 with Kox = 3.9 by Nf =
2.16 × 1013 Kox εo φMS = φMS (V ) cm−2 qtox tox (nm)
(6.26)
For an uncertainty in the metalsemiconductor work function difference of φMS = 0.05 V, Nf = 5.4 × 1011 cm−2 for tox = 2 nm. This kind of uncertainty is higher than typical fixed charge densities, showing the importance of knowing φMS accurately.
335
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
A second method to determine Qf dispenses with a knowledge of φMS . Rewriting Eq. (6.25) as Qf tox Qf = φMS − (6.27) VF B = φMS − Cox Kox εo suggests a plot of VF B versus tox with slope Qf /Kox ε0 and intercept φMS . This method, described in more detail in the next section, requires MOS capacitors with differing tox . However, it is more accurate because it is independent of φMS . Since the published literature shows variations of φMS by as much as 0.5 V, it is obviously important to determine φMS for a given process and not rely on published values. 6.2.5
GateSemiconductor Work Function Difference
The metalsemiconductor work function difference φMS is indicated in Fig. 6.13 for a flatband metaloxidesemiconductor potential band diagram with zero oxide charges. VG = VF B assures that the bands in the semiconductor and in the oxide are flat. For zero oxide or interface charge, VF B = φMS from Eq. (6.17). Note that all quantities are given in potentials in Fig. 6.13, not in energies. φM and φM ′ are the metal and effective metal work function, φS is the semiconductor work function, χ and χ ′ are the electron and effective electron affinity. All other symbols have their usual meanings. From Fig. 6.13, ′ φMS = φM − φS = φM − (χ ′ + (Ec − EF )/q)
(6.28)
Here φM ′ , χ ′ , and (Ec − EF )/q are constants for a given gate material, semiconductor, and temperature. For p and nsubstrates, Eq. (6.28) becomes φMS
kT kT NA ND ln ln ; φMS = K + φF = K + = K − φF = K − q ni q ni
(6.29)
where K = φM ′ − χ ′ − (Ec − Ei )/q and (Ec − EF )/q = (Ec − Ei )/q + φF = (Ec − Ei )/q + (kT /q) ln(NA /ni ). φMS depends not only on the semiconductor and the gate material, but also on the substrate doping type and density.
Vacuum Level
fM
c f′M
fS
c′
EF/q Potential
VG
Fig. 6.13
Ec/q
fF
Ei/q EF/q
Ev/q
Potential band diagram of a metaloxidesemiconductor system at flatband.
336
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
EG/2q
VFB
fF VFB
fF
EG/2q
Fig. 6.14 flatband.
Potential band diagram of (a) n+ polySi/p substrate, and (b) p+ polySi/n substrate at
Figure 6.14 shows the band diagram for an n+ polySip substrate and for a p + polySin substrate MOSC. Since both gate and substrate have the same electron affinity, we find (6.30) φMS = φF (gate) − φF (substrate) The Fermi level for n+ polySi gates coincides approximately with the conduction band and with the valence band for p + polySi gates, giving φMS (n+ gate) ≈ −EG /2q − (kT /q) ln(NA /ni ) and φMS (p + gate) ≈ EG /2q + (kT /q) ln(ND /ni ). For n+ gates on nsubstrates, φMS (n+ gate) ≈ −EG /2q + (kT /q) ln(ND /ni ), where NA and ND are the substrate doping densities. Early φMS determinations used photoemission measurements.16 With a voltage applied between a semitransparent gate and the substrate, no current flows in the absence of light because of the insulating nature of the oxide. Photons of sufficient energy strike the gate and excite electrons from the gate into the oxide. Some of these electrons drift through the oxide to be collected as photocurrent. Electrons are excited from the semiconductor into the oxide and flow to the gate for positive gate voltages and the barrier height of the semiconductor/oxide interface is determined. For negative gate voltages, electrons are excited from the gate into the oxide and flow to the semiconductor leading to the gate/oxide barrier. Photoemission measurements determine φMS only indirectly. A more direct measure utilizes Eq. (6.27), repeated here VF B = φMS −
Qf Qf tox = φMS − Cox Kox εo
(6.31)
A plot of VF B versus oxide thickness has a slope of −Qf /Kox ε0 and an intercept on the VF B axis of φMS .17 This method is more direct, as it measures the capacitance of MOS capacitors. Furthermore, since the flatband voltage is measured, it ensures zero electric field at the semiconductor surface eliminating Schottky barrier lowering corrections. The oxide thickness can be varied by oxidizing the wafer to a given thickness, measuring VF B , etching a portion of the oxide, remeasuring VF B and so on. This method ensures that the same spot on the oxide is measured each time. Oxide etching does not affect the fixed charge, since Qf is located very near the SiO2 Si interface. Sometimes the oxide is
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
337
etched in strips to different thicknesses, or oxides can be grown to different thicknesses on different wafers and MOS capacitors formed, assuming Qf to be the same for all samples. Plots of VF B − tox are shown in Fig. 6.15.18 The MOS capacitors with SiO2 gate dielectric were fabricated on ptype Si substrates. 40–200 nm thick polySi was deposited on the gate dielectric followed by 80–200 nm hafnium. Silicidation was done by furnace annealing at 420◦ C or rapid thermal annealing at temperatures from 600◦ C to 750◦ C for 1 min. and the samples were annealed in forming gas at 420◦ C for 30 min. φMS depends on oxidation temperature, wafer orientation, interface trap density, and on the low temperature Dit anneal.19 The work function of polySi gate devices should depend on the doping density of the gate. One report shows a φMS maximum at phosphorus and arsenic densities of 5 × 1019 cm−3 , with the work function difference decreasing above and below this density.20 The dependence of φMS on doping density is shown in Fig. 6.16 for the SiO2 /Si system with polySi gates.
0.2 Flatband Voltage (V)
p+ polySi 0 pHfSi
−0.2 −0.4
Undoped HfSi −0.6 n+ polySi
nHfSi
−0.8 −1 0
5
10
15
20
Oxide Thickness (nm)
Fig. 6.15 Flatband voltage versus oxide thickness; ptype Si substrates. 40–200 nm thick polySi plus 80–200 nm hafnium silicided at 420◦ C or rapid thermal annealed at 600◦ C to 750◦ C for 1 min. Annealed in forming gas at 420◦ C for 30 min. Adapted from ref. 18.
1.2 0.8 fMS (V)
0.4
a b p+ polySi/ nSi substrate
0 −0.4
n+ polySi/ pSi substrate
−0.8 −1.2 1014
a 1015
1016 NA, ND
1017
c d 1018
(cm−3)
Fig. 6.16 φMS as a function of doping density for polySi/SiO2 /Si MOS devices. The numbers refer to references. The references are: a,21 b,22 c,23 and d 20 .
338
6.2.6
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
Oxide Trapped Charge
Charge can become trapped in the oxide during device operation even if not introduced during device fabrication. Electrons and/or holes can be injected from the substrate or from the gate. Energetic radiation also produces electronhole pairs in the oxide and some of these electrons and/or holes are subsequently trapped in the oxide. The flatband voltage shift VF B due to oxide trapped charge Qot is obtained from VF B = VF B (Qot ) − VF B (Qot = 0)
(6.32)
assuming all other charges remain unchanged during the oxide trapped charge introduction. Contrary to Qf , the oxide trapped charge is usually not located at the oxide/semiconductor interface, but is distributed through the oxide. The distribution of Qot must be known for proper interpretation of C –V curves. Trapped charge distributions are measured most commonly by the etchoff and the photo I –V methods. In the etchoff method, thin layers of the oxide are etched. The C –V curve is measured after each etch and the oxide charge profile is determined from these C –V curves. The photo I –V method is nondestructive and more accurate than the etchoff method. It is based on the optical injection of electrons from the gate or from the substrate into the oxide. Electron injection depends on the distance of the energy barrier from the injecting surface and on the barrier height. Both barrier distance and barrier height are affected by oxide charge and gate bias. Photo I –V curves yields both the barrier distance and the barrier height. A good discussion of the method can be found in ref. 24 and references therein. Occasionally the technique is useful to monitor the flatband voltage continuously.25 A determination of the charge distribution in the oxide is tedious and therefore not routinely done. In the absence of such information, the flatband voltage shift due to charge injection is generally interpreted by assuming the charge is at the oxidesemiconductor interface using the expression Qox = −Cox VF B 6.2.7
(6.33)
Mobile Charge
Mobile charge in SiO2 is due primarily to the ionic impurities Na+ , Li + , K+ , and perhaps H+ . Sodium is the dominant contaminant. Lithium has been traced to oil in vacuum pumps and potassium can be introduced during chemicalmechanical polishing. The practical application of MOSFETs was delayed due to mobile oxide charges in the early 1960s. MOSFETs were found to be very unstable for positive gate bias but relatively stable for negative gate voltages. Sodium was the first impurity to be related to this gate bias instability.26 By intentionally contaminating MOSCs and measuring the C –V shift after biastemperature stress, it was shown that alkali cations could easily drift through thermal SiO2 films. Chemical analysis of etchedback oxides by neutron activation analysis and flame photometry was used to determine the Na profile.27 The drift has been measured with the isothermal transient ionic current method, the thermally stimulated ionic current method, and the triangular voltage sweep method.28 The mobility some oxide contaminants is given by the expression29 µ = µo exp(−EA /kT )
(6.34)
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
339
where for Na: µ0 = 3.5 × 10−4 cm2 /V·s (within a factor of 10) and EA = 0.44 ± 0.09 eV; for Li: µ0 = 4.5 × 10−4 cm2 /V·s (within a factor of 10) and EA = 0.47 ± 0.08 eV, for K: µ0 = 2.5 × 10−3 cm2 /V·s (within a factor of 8) and EA = 1.04 ± 0.1 eV, and for Cu, µ0 = 4.8 × 10−7 cm2 /V·s and EA = 0.93 ± 0.2 eV.29 The oxide electric field is given by VG /tox , neglecting the small voltage drop across the semiconductor and gate. The drift velocity of mobile ions through the oxide is vd = µVG /tox and the transit time tt is tt =
t2 t2 tox = ox = ox exp(EA /kT ) vd µVG µo VG
(6.35)
Equation (6.35) is plotted in Fig. 6.17 for the three alkali ions and for Cu. For this plot the oxide electric field is 106 V/cm, a common oxide electric field for such measurements, and the oxide thickness is 100 nm. For thinner or thicker oxides, the transit time change according to Eq. (6.35). Na and Li drift very rapidly through the oxide. Typical measurement temperatures lie in the 200 to 300◦ C range and only a few milliseconds suffice for the charge to transit the oxide. Mobile charge densities in the 5 × 109 –1010 cm−2 range are generally acceptable in integrated circuits. BiasTemperature Stress: The biastemperature stress (BTS) method is one of two techniques to determine the mobile charge. However, in contrast to roomtemperature C –V measurements for Qf determination, for mobile charge measurements the temperature must be sufficiently high for the charge to be mobile. Typically the device is heated to 150 to 250◦ C, and a gate bias to produce an oxide electric field of around 106 V/cm is applied for 5–10 min. for the charge to drift to one oxide interface. The device is then cooled to room temperature under bias and a C –V curve is measured. The procedure is then repeated with the opposite bias polarity. The mobile charge is determined from the flatband voltage shift, according to the equation Qm = −Cox VF B
(6.36)
Temperature (°C) 104 500
300
0
100
Drift Time (s)
2
10
Cu K
100
Li
10−2
Na tox = 100 nm VG = 10 V
10−4 1
2
3
4
1000/T (K−1) Fig. 6.17
Drift time for Na, Li, K, and Cu for an oxide electric field of 106 V/cm and tox = 100 nm.
340
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
The reproducibility of BTS measurements becomes questionable as mobile ion densities approach 109 cm−2 . For example, the flatband voltage shift in a 10 nm thick oxide due to the drift of a 109 cm−2 mobile ion density is 0.5 mV. Changing the gate area does not help since one measures voltage shifts, not capacitance. There is sometimes a question of whether a measured flatband voltage shift is due to oxide trapped charge or due to mobile charge. A simple check to discriminate between the two is the following: Consider an MOSC on a ptype substrate whose C –V curve is initially measured with moderate gate voltage excursions giving C –V curve (a) in Fig. 6.18. We assume that as a result of the modest gate voltage excursion charge is neither injected into the oxide nor does mobile charge move. Next, a BTS test is done with positive gate voltage. Keeping the oxide electric field around 1 MV/cm causes mobile charge to drift, but the electric field is insufficient for appreciate charge injection. If the C –V curve after the BTS is curve (b) in Fig. 6.18, then the drift is due to positive mobile charge. For higher gate voltages at room temperature, there is a good chance that electrons and/or holes can be injected into the oxide and mobile charge may also drift, making that measurement less definitive. Triangular Voltage Sweep: In the triangular voltage sweep (TVS) method the current is measured instead of the capacitance.30 The MOSC is held at an elevated, constant temperature of 200 to 300◦ C and the lowfrequency C –V curve is measured. Clf is usually not obtained by measuring the capacitance, but rather by measuring a current or charge, as discussed in Section 6.2.3. TVS is based on measuring the charge flow through the oxide at an elevated temperature in response to an applied timevarying voltage. The charge flow is detected either as a current or as a charge. For a mobile ion density of 109 cm−2 , the resulting current is I = 34 pA for a sweep rate of 0.01 V/s and gate area of 0.01 cm2 . The charge in a charge sensing measurement is Q = 1.6 pC. Both of these are within typical measurement capability. The current is determined by applying a slowly varying voltage ramp, as shown in Fig. 6.11(a), and measuring the current. If the ramp rate is sufficiently low, the measured current is the sum of displacement and conduction current due to the mobile charge. The current I is defined by dQG (6.37) I= dt 1
C/Cox
0.8 (b)
0.6
(a)
0.4 0.2 0 −4
Fig. 6.18
−2
0 Gate Voltage (V)
2
4
C –VG curves illustrating the effects of mobile charge motion.
FIXED, OXIDE TRAPPED, AND MOBILE OXIDE CHARGE
341
With QG = −(QS + Qit + Qf + Qot + Qm ), the current can be written as24 I = Clf
dVF B α− dt
(6.38)
where α = dVG /dt is the gate voltage ramp rate. Integrating both sides from −VG1 to +VG2 gives
VG2
−VG1
(I /Clf − α) dVG = −α{VF B [t (VG2 )] − VF B [t (−VG1 )]}
(6.39)
Let us assume that at −VG1 all mobile charges are located at the gateoxide interface (x = 0) and at VG2 all mobile charges are located at the semiconductoroxide interface (x = tox ). Then considering mobile charge only we find from Eq. (6.17), −α{VF B [t (VG2 )] − VF B [t (−VG1 )]} = α
Qm Cox
(6.40)
and Eq. (6.39) becomes VG2
−VG1 (I /Clf
− α)Cox dVG = αQm
(6.41)
As shown in Exercise 6.1, the hf and lf C –V curves coincide at high temperatures and the mobile charge is obtained by measuring the hf and lf curves and taking the area between the two curves, as illustrated in Fig. 6.19.31 The integral of Eq. (6.41) represents the area between the lf and the hf curves in Fig. 6.19. One may ask why the lf curve exhibits the mobile charge hump, when Clf and Chf coincide. The reason is that during the lf current measurement, not only does the inversion charge respond to the probe frequency, but the mobile charge also drifts. For high temperature and high frequency capacitance measurements, only the inversion charge is detected.
1000 tox = 100 nm
Capacitance (pF)
900 800
Nm = 1.3 ×
1010
cm−2 lf
700 600 500
4.1 × 109 cm−2
400 300 −3
hf −2
−1 0 1 Gate Voltage (V)
2
3
Fig. 6.19 Clf and Chf measured at T = 250◦ C. The mobile charge density is determined form the area between the two curves.
342
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
Sometimes two peaks are observed in I –VG curves at different gate voltages. These have been attributed to mobile ions with different mobilities. For an appropriate temperature and sweep rate, highmobility ions (e.g., Na+ ) drift at lower oxide electric fields than lowmobility ions (e.g., K+ ). Hence, the Na peak occurs at lower gate voltages than the K peak. Such discrimination between different types of mobile impurities is not possible with the biastemperature method. This also explains why sometimes the total number of impurities determined by the BTS and the TVS methods differ. In the BTS method one usually waits long enough for all the mobile charge to drift through the oxide. If in the TVS method the temperature is too low or the gate ramp rate is too high, it is possible that only one type of charge is detected. For example, it is conceivable that highmobility Na drifts but lowmobility K does not. The TVS method also lends itself to mobile charge determination in interlevel dielectrics, not just gate oxides, since a current or charge is measured instead of a capacitance. Other Methods: The electrical characterization methods are dominant because they are easily implemented and are very sensitive. The BTS method has a sensitivity of about 1010 cm−2 and the TVS method can detect densities as low as about 109 cm−2 . However, electrical methods cannot detect neutral impurities nor the sodium content in chemicals, furnace tubes etc. Analytical methods that have been employed for sodium detection include radiotracer,32 neutron activation analysis,33 flame photometry,34 and secondary ion mass spectrometry (SIMS). For SIMS it is important to take surface charging by the positive or negative ion beam into account, because it can alter the ionic distribution and give erroneous distribution curves.35
6.3
INTERFACE TRAPPED CHARGE
Interface trapped charge, also known as interface traps or states, are attributed to dangling bonds at the semiconductor/insulator interface. Their density is most commonly reduced by forming gas anneal. A good overview of the nature of interface trapped charge and methods for its characterization can be found in refs. 24, 36, 37. 6.3.1
Low Frequency (Quasistatic) Methods
The lowfrequency or quasistatic method is a common interface trapped charge measurement method. It provides information only on the interface trapped charge density, but not on their capture crosssections. In this chapter we use the terms “interface trapped charge” and “interface traps” interchangeably. Before discussing characterization techniques, it is useful to discuss the nature of interface traps. One model attributes donorlike behavior to Dit below Ei and acceptorlike behavior to Dit above Ei as shown in Fig. 6.20(a). Although this model is not universally accepted, there is experimental evidence for it.38 Donor interface traps below EF are occupied by electrons and hence neutral. Those with energies EF < E < Ei are unoccupied donors and hence positively charged. Those above Ei are unoccupied acceptors and hence neutral. As a result, at flatband, Dit contributes a positive net charge. For positive gate voltage (Fig. 6.20(b)) some of the acceptor states lie below EF and there is a net negative charge while for negative gate voltage (Fig. 6.20(c)) there is a more net positive charge. Hence, according to Eq. (6.17) the C –V curves shift to the left for negative gate voltage and to the right for positive gate voltage.
343
INTERFACE TRAPPED CHARGE
Dit A
"0"
D
"+" "0"
"−"
A: Acceptors, D: Donors
"0"
Ec
"+" "0"
Ei EF Ev
"0"
(a)
(c)
(b)
Fig. 6.20 Semiconductor band diagrams illustrating the effects of interface traps; (a) VG = 0, (b) VG > 0, (c) VG < 0. Electronoccupied interface traps are indicated by the small horizontal heavy lines and unoccupied traps by the light lines.
1
1
0.6
Dit ≠ 0
0.8
Dit = 0 Clf/Cox
Chf/Cox
0.8
0.4 0.2 0 −3
0.6
Dit ≠ 0
0.4 0.2
−2
0
−1
Dit = 0
0 −2
1
0
−1
1
Gate Voltage (V)
Gate Voltage (V)
(a)
(b)
2
1
Clf/Cox
0.8
Before Stress After Stress
0.6 0.4 0.2 0 −2
−1
0
1
2
Gate Voltage (V) (c)
Fig. 6.21 Effect of Dit on MOSC capacitancevoltage curves. (a) Theoretical highfrequency, (b) theoretical lowfrequency and (c) experimental lowfrequency curves. Gate voltage stress generated interface traps.
The effect of interface traps on both hf and lf C –V curves is illustrated in Fig. 6.21. If interface traps cannot follow the ac probe frequency, they do not contribute a capacitance and the equivalent circuits are those of Fig. 6.4 with Cit = 0. However, interface traps can follow the slowly varying dc bias. As the gate voltage is swept from accumulation to inversion, the gate charge is QG = −(QS + Qit ) assuming no oxide charges. In contrast to the ideal case, where Qit = 0, now both semiconductor and interface traps must be charged. The relationship of surface potential to gate voltage differs from Eq. (6.16) and
344
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
the hf C –V curve stretches out as shown in Fig. 6.21(a). This stretchout is not the result of interface traps contributing excess capacitance, but rather it is the result of the C –V curve stretchout along the gate voltage axis. Interface traps do respond to the probe frequency at low measurement frequencies, and the curve distorts because the interface traps contribute interface trap capacitance Cit and the curve stretches out along the voltage axis, shown in Fig. 6.21(b). For φs = φF , the upper half band gap donortype and lower half band gap acceptortype interface traps cancel one another, leading to the coincidence of the ideal and distorted C –V curves. Experimental curves are shown in Fig. 6.21(c) before and after oxide stress induced by gate current through the oxide. The basic theory of the quasistatic method was developed by Berglund.38 The method compares a lowfrequency C –V curve with one free of interface traps. The latter can be a theoretical curve, but is usually an hf C –V curve determined at a frequency where interface traps are assumed not to respond. “Low frequency” means that interface traps and minority carrier inversion charges must be able to respond to the measurement ac probe frequency. The constraints for minority carrier response are discussed in Section 6.2.1. The interface trap response has similar limitations. Fortunately, the limitations are usually less severe than for minority carrier response and frequencies low enough for inversion layer response are generally low enough for interface trap response. The lf capacitance is given by Eq. (6.4) in depletioninversion as −1 1 1 + (6.42) Clf = Cox CS + Cit where we have replaced Cb + Cn by CS , the lf semiconductor capacitance. Cit is related to the interface trap density Dit by Dit = Cit /q 2 , giving Dit =
1 q2
Cox Clf − CS Cox − Clf
(6.43)
Equation (6.43) is suitable for interface trap density determination over the entire band gap.
Exercise 6.5 Problem: Why is Cit = q 2 Dit used here when most text use Cit = qD it ? Solution: Cit = qD it is quoted in well respected texts, e.g., Nicollian and Brews on p. 195.24 But . . . if we substitute units, something is not right. With Dit in cm−2 eV−1 (the Coul F Coul = = usual units) and q in Coul the units for Cit are cm2 eV cm2 Coul − Volt cm2 Coul Coul using eV = Coul − Volt; Volt = . This suggests that the correct definition should F be Cit = q 2 Dit . We must keep in mind, however, that in the expression E(eV) = qV , q = 1 not 1.6 × q10−19 ! Hence Cit = q 2 Dit = 1 × 1.6 × 10−19 Dit . If Dit is given in cm−2 J−1 , then Cit = (1.6 × 10−19 )2 Dit . This was pointed out to me by Kwok Ng and can be found in his book K.K. Ng, Complete Guide to Semiconductor Devices, 2nd Ed., WileyInterscience, New York, 2002, p. 183.
INTERFACE TRAPPED CHARGE
345
Clf and CS must be known to determine Dit . Clf is measured as a function of gate voltage and CS is calculated from Eq. (6.7). In Eq. (6.7), the capacitance is calculated as a function of surface potential φs but in Eq. (6.43) Clf is measured as a function of gate voltage. Hence, we need a relationship between φs and VG . Berglund proposed39 φs =
VG2
VG1
(1 − Clf /Cox ) dVG +
(6.44)
where is an integration constant given by the surface potential at VG = VG1 . The integrand is obtained by integrating the measured Clf /Cox versus VG curve with VG1 and VG2 arbitrarily chosen, since the integration constant is unknown. Integration from VG = VF B makes = 0, because band bending is zero at flatband. Integration from VF B to accumulation and from VF B to inversion gives the surface potential over most of the band gap range. If the integration is carried out from strong accumulation to strong inversion, the integral should give [φs (VG2 ) − φs (VG1 )] = EG /q. A value higher than EG /q indicates gross nonuniformities in the oxide or at the oxidesemiconductor interface, making the analysis invalid. Various approaches to determine the surface potential based on lf and hf C –V curves have been proposed.40 Kuhn proposed fitting the experimental and theoretical Clf versus φs curves in accumulation and strong inversion.10 Plotting (1/Cs )2 against φs gives a line with slope NA and intercept if NA is uniform. If it is nonuniform, then no unique value of is obtained. These methods are generally based on measuring charge using an operational amplifier with a capacitor in the feedback loop. In one circuit, Dit is determined and plotted directly as a function of φs .41 The determination of Dit from Eq. (6.43) and (6.44) is quite time consuming and a simplified approach was proposed by Castagn´e and Vapaille.42 It eliminated the uncertainty associated with the calculation of CS in Eq. (6.43) and replaced it with a measured CS . From the hf C –V curve, we find from Eq. (6.15), CS =
Cox Chf . Cox − Chf
(6.45)
Substituting Eq. (6.45) into (6.43) gives Dit in terms of the measured lf and hf C –V curves as Cox Chf /Cox Clf /Cox Dit = 2 − (6.46) q 1 − Clf /Cox 1 − Chf /Cox Equation (6.46) gives Dit over only a limited range of the band gap, typically from the onset of inversion, but not strong inversion, to a surface potential towards the majority carrier band edge where the ac measurement frequency equals the inverse of the interface trap emission time constant. This corresponds to an energy about 0.2 eV from the majority carrier band edge. The higher the frequency the closer to the band edge can be probed. Typical hf and lf curves are shown in Fig. 6.22. Data for Dit − φs typically have a U shaped distribution with a minimum near midgap and sharp increases toward either band edge, as shown in Fig. 6.26. It is very important when using the technique based on Eq. (6.43), that the integration constant be well known. Small errors in have a large effect on Dit near the band edges.43 Errors can also be introduced by surface potential fluctuations due to inhomogeneities in oxide charge and/or substrate doping density.44 Errors in Dit extraction are also introduced by neglecting quantummechanical effects in the inversion capacitance.45 The conventional
346
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
1 Clf
C/Cox
0.8 0.6 0.4 ∆C/Cox
Chf
0.2 0 −3
Fig. 6.22 traps.
−2
−1
0 1 2 Gate Voltage (V)
3
4
5
High and lowfrequency C –VG curves showing the offset C/Cox due to interface
0.9
Dit (cm−2 eV−1)
1013
0.8 0.7
1012
0.6 0.5 0.4
1011 0.3 1010 109 0.001
0.2 Chf/Cox = 0.1 tox = 10 nm 0.01
0.1
1
∆C/Cox
Fig. 6.23
Interface trapped charge density from the hf curve and the offset C/Cox .
quasistatic technique underestimates the interface state density if the quantummechanical effect is significant, which becomes more critical as the doping density is increased. It is not always necessary to determine Dit as a function of surface potential. For example, for process monitoring it is frequently sufficient to determine Dit at one point on the C –V curve. A convenient choice is the minimum Clf where the technique is most sensitive. This point corresponds to a surface potential in the light inversion region near midgap, (φF < φs < 2φF ). To extract Dit , Eq. (6.46) is plotted in Fig. 6.23 for SiO2 with tox = 10 nm. To use the figure, measure Clf /Cox and Chf /Cox , then determine C/Cox = Clf /Cox − Chf /Cox and find Dit from the graph (C/Cox is defined in Fig. 6.22).46 For oxide thicknesses other than 10 nm, multiply Dit from Fig. 6.22 by 10/tox with tox in nm. Other graphical techniques have also been proposed.47 For highfrequency curves, the measurement frequency must be sufficiently high that interface traps do not respond. The usual 1 MHz frequency may suffice, but for devices with high Dit there will be some response due to interface traps. If possible, one should
INTERFACE TRAPPED CHARGE
347
use higher frequencies, but care must be used to ascertain that series resistance effects do not become important. It is easier to measure Clf when sweeping from inversion to accumulation, because minority carriers need not be generated thermally since they already exist in the inversion layer. Series resistance and stray light can also influence the curve.48 A detailed accounting of the errors in extracting Dit is given by Nicollian and Brews.24 The lower limit of Dit that can be determined with the quasistatic technique lies around 1010 cm−2 eV−1 . However, as oxide thickness decreases, the lf curve contains an appreciable oxide leakage current component, rendering quasistatic results questionable. The charge voltage method is well suited for MOS measurements and can also determine the additive constant of Eq. (6.44) by comparing experimental and theoretical φs versus W curves, where W is the spacecharge region width obtained from the experimental hf C –V curve. 6.3.2
Conductance
The conductance method, proposed by Nicollian and Goetzberger in 1967, is one of the most sensitive methods to determine Dit .49 Interface trap densities of 109 cm−2 eV−1 and lower can be measured. It is also the most complete method, because it yields Dit in the depletion and weak inversion portion of the band gap, the capture crosssections for majority carriers, and information about surface potential fluctuations. The technique is based on measuring the equivalent parallel conductance GP of an MOSC as a function of bias voltage and frequency. The conductance, representing the loss mechanism due to interface trap capture and emission of carriers, is a measure of the interface trap density. The simplified equivalent circuit of an MOSC appropriate for the conductance method is shown in Fig. 6.24(a). It consists of the oxide capacitance Cox , the semiconductor capacitance CS , and the interface trap capacitance Cit . The captureemission of carriers by Dit is a lossy process, represented by the resistance Rit . It is convenient to replace the circuit of Fig. 6.24(a) by that in Fig. 6.24(b), where CP and GP are given by Cit 1 + (ωτit )2 qωτit Dit GP = ω 1 + (ωτit )2 CP = CS +
(6.47) (6.48)
where Cit = q 2 Dit , ω = 2πf (f = measurement frequency) and τit = Rit Cit , the interface trap time constant, given by τit = [vth σp NA exp(−qφs /kT ]−1 . Dividing GP by ω makes Eq. (6.48) symmetrical in ωτit . Equations (6.47) and (6.48) are for interface traps
Cox
Cox Rit
CS
Cox G P Cm
CP
Rit
Gm CS
Cit
Gt
Cit rs
(a)
(b)
(c)
(d)
Fig. 6.24 Equivalent circuits for conductance measurements; (a) MOSC with interface trap time constant τit = Rit Cit , (b) simplified circuit of (a), (c) measured circuit, (d) including series rs resistance and tunnel conductance Gt .
348
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
with a single energy level in the band gap. Interface traps at the SiO2 Si interface, however, are continuously distributed in energy throughout the Si band gap. Capture and emission occurs primarily by traps located within a few kT/q above and below the Fermi level, leading to a time constant dispersion and giving the normalized conductance as49 qDit GP = ln[1 + (ωτit )2 ] ω 2ωτit
(6.49)
Equations (6.48) and (6.49) show that the conductance is easier to interpret than the capacitance, because Eq. (6.48) does not require CS . The conductance is measured as a function of frequency and plotted as GP /ω versus ω. GP /ω has a maximum at ω = 1/τit and at that maximum Dit = 2GP /qω. For Eq. (6.49) we find ω ≈ 2/τit and Dit = 2.5GP /qω at the maximum. Hence we determine Dit from the maximum GP /ω and determine τit from ω at the peak conductance location on the ωaxis. GP /ω versus f plots, calculated according to Eqs. (6.48) and (6.49), are shown in Fig. 6.25. The calculated curves are based on Dit values from a detailed interface extraction routine from the experimental data also shown on the figure. Note the much broader experimental peak. Experimental GP /ω versus ω curves are generally broader than predicted by Eq. (6.49), attributed to interface trap time constant dispersion caused by surface potential fluctuations due to nonuniformities in oxide charge and interface traps as well as doping density. Surface potential fluctuations are more pronounced in pSi than in nSi.50 Surface potential fluctuations complicate the analysis of the experimental data. When such fluctuations are taken into account, Eq. (6.49) becomes q GP = ω 2
∞
−∞
Dit ln[1 + (ωτit )2 ]P (Us ) dUs ωτit
(6.50)
where P (Us ) is a probability distribution of the surface potential fluctuation given by
(Us − U s )2 1 P (Us ) = √ (6.51) exp − 2σ 2 2πσ 2 with U S and σ the normalized mean surface potential and standard deviation, respectively. 2 × 10−10
GP/w(S·s/cm2)
Single Level Continuum 1 × 10−10
Statistical/ Experiment 0 102
103
104
105
106
w(s−1)
Fig. 6.25 Gp /ω versus ω for a single level [Eq. (6.48)], a continuum [Eq. (6.49)], and experimental data.37 For all curves: Dit = 1.9 × 109 cm−2 eV−1 , τit = 7 × 10−5 s.
INTERFACE TRAPPED CHARGE
349
The line through the data points in Fig. 6.25 is calculated from Eq. (6.50). Note the good agreement between theory and experiment when φs fluctuations are considered. An approximate expression giving the interface trap density in terms of the measured maximum conductance is49 2.5 GP (6.52) Dit ≈ q ω max Capacitance meters generally assume the device to consist of the parallel Cm − Gm combination in Fig. 6.24(c). A circuit comparison of Fig. 6.24(b) to 6.24(c) gives GP /ω in terms of the measured capacitance Cm , the oxide capacitance, and the measured conductance Gm as 2 ωGm Cox GP = 2 (6.53) ω Gm + ω2 (Cox − Cm )2 assuming negligible series resistance. The conductance measurement must be carried out over a wide frequency range. A comparison of interface traps determined by the quasistatic and the conductance techniques is shown in Fig. 6.26. Note the broad energy range over which the quasistatic method yields Dit and the good agreement over the narrower range where the conductance method is valid. The portion of the band gap probed by conductance measurements is typically from flatband to weak inversion. The measurement frequency should be accurately determined and the signal amplitude should be kept at around 50 mV or less to prevent harmonics of the signal frequency giving rise to spurious conductances. The conductance depends only on the device area for a given Dit . However, a capacitor with thin oxide has a high capacitance relative to the conductance, especially for low Dit and the resolution of the capacitance meter is dominated by the outofphase capacitive current component. Reducing Cox by increasing the oxide thickness helps this measurement problem. For thin oxides, there may be appreciable oxide leakage current. In addition, the device has series resistance which has so far been neglected. In the more complete circuit in Fig. 6.24(d), Gt represents the tunnel conductance and rs the series resistance.
2 × 1012 Conductance Dit (cm−2eV−1)
Quasistatic (a)
1 × 1012 (b) Ev
0 0
0.2
0.4
0.6
0.8
1 Ec
Energy (eV) Fig. 6.26 Interface trapped charge density versus energy from the quasistatic and conductance methods. (a) (111) nSi, (b) (100) nSi. After ref. 50 and 51.
350
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
Equation (6.53) now becomes52 2 ω(Gc − Gt )Cox GP = 2 2 ω Gc + ω (Cox − Cc )2
(6.54)
where Cc = Gc =
Cm (1 − rs Gm )2 + (ωrs Cm )2 ω 2 r s Cm Cc − G m rs Gm − 1
(6.55) (6.56)
Cm and Gm are the measured capacitance and conductance. The series resistance is determined by biasing the device into accumulation according to24 rs =
Gma 2 G2ma + ω2 Cma
(6.57)
where Gma and Cma are the measured conductance and capacitance in accumulation. The tunnel conductance is determined from Eq. (6.56) as ω → 0.52 Equation (6.54) reverts to Eq. (6.53) when rs = Gt = 0. Several models have been assumed to explain the experimental conductances.53 In general it is necessary to use one of these models to extract Dit and σp with confidence. Schemes have been proposed for analyzing data by taking pairs of values of Gp /ω having a predetermined relationship of either frequency54 or magnitude.55 For example, Gp /ω curves can be determined at two frequencies and the appropriate parameters are found from universal curves. Brews uses a single Gp /ω curve and determines the points where the curve has fallen to a fraction of its peak value and then utilizes universal curves to determine Dit and σp .55 Noras presents an algorithm to extract the relevant parameters.55 In yet another simplification, a single hf C –V and G–V curve suffices to determine Dit .56 Instead of changing the frequency and holding the temperature constant, it is also possible to change the temperature and hold the frequency constant.57 This has the advantage of not requiring measurements over a wide frequency range and one can chose a frequency for which series resistance is negligible. Elevated temperature measurements enhance the sensitivity near midgap allowing the detection of trap energy levels and capture crosssections.58 It also is possible to use MOSFETs instead of MOSCs and measure the transconductance instead of the conductance but still use the concepts of the conductance method.59 This permits interface trap density determination on devices with the small gate areas associated with MOSFETs without the need for special MOSC test structures. 6.3.3
High Frequency Methods
Terman Method: The roomtemperature, highfrequency capacitance method developed by Terman was one of the first methods for determining the interface trap density.60 The method relies on a hf C –V measurement at a frequency sufficiently high that interface traps are assumed not to respond. They should, therefore, not contribute any capacitance. How can one measure interface traps if they do not respond to the applied ac signal? Although interface traps do not respond to the ac probe frequency, they do respond to the
INTERFACE TRAPPED CHARGE
351
slowly varying dc gate voltage and cause the hf C –V curve to stretch out along the gate voltage axis as interface trap occupancy changes with gate bias illustrated in Fig. 6.21(a). In other words, for an MOSC in depletion or inversion additional charge placed on the gate induces additional semiconductor charge QG = −(Qb + Qn + Qit ). With VG = VF B + φs + Vox = VF B + φs + QG /Cox
(6.58)
it is obvious that for a given surface potential φs , VG varies when interface traps are present, leading to the C –V “stretchout” in Fig. 6.21. The stretchout produces a non parallel shift of the C –V curve. Interface traps distributed uniformly through the semiconductor band gap produce a fairly smoothly varying but distorted C –V curve. Interface traps with distinct structure, for example peaked distributions, produce more abrupt distortions in the C –V curve. The relevant equivalent circuit of the hf MOSC is that in Fig. 6.4(c) with Cit = 0, that is Chf = Cox CS /(Cox + CS ) where CS = Cb + Cn . Chf is the same as that of a device without interface traps provided CS is the same. The variation of CS with surface potential is known for an ideal device. Knowing φs for a given Chf in a device without Qit allows us to construct a φs versus VG curve of the actual capacitor as follows: From the ideal MOSC C –V curve, find φs for a given Chf . Then find VG on the experimental curve for the same Chf , giving one point of a φs versus VG curve. Repeat for other points until a satisfactory φs − VG curve is constructed. This φs − VG curve contains the relevant interface trap information. The experimental φs versus VG curve is a stretchedout version of the theoretical curve and the interface trap density is determined from this curve by24 Dit =
Cox q2
CS Cox dVG dVG −1 − 2 = 2 dφs q q dφs
(6.59)
where VG = VG –VG (ideal) is the voltage shift of the experimental from the ideal curve, and VG the experimental gate voltage. The method is generally considered to be useful for measuring interface trap densities of 1010 cm−2 eV−1 and above,61 and has been widely critiqued. Its limitations were originally pointed out to be due to inaccurate capacitance measurements and insufficiently high frequencies.62 A later, theoretical study concluded that Dit in the 109 cm−2 eV−1 range can be determined provided the capacitance is measured to a precision of 0.001 to 0.002 pF.63 For thinner oxides, the voltage shift associated with the interface traps also decreases. An assumption of the Terman method is that the measured Chf curve does not contain appreciable interface state capacitance. Simulations have shown that the difference between the true highfrequency C –V curve and the 1 MHz curve is on the same order of the difference between the “no Dit ” curve and the 1 MHz curve, because the interface state capacitance is small, but nonnegligible, compared to the voltage stretchout for thin dielectrics.64 For thicker dielectrics, the interface state capacitance is the same, but the voltage stretchout increases. Both interface trap capacitance and voltage stretchout scale with Dit making this method questionable for thin oxides. To compare experimental with theoretical curves, one needs to know the doping density exactly. Any dopant pile up or outdiffusion introduces errors. Surface potential fluctuations can cause fictitious interface trap peaks near the band edges. The assumption that interface traps do not follow the ac probe frequency may not be satisfied for surface potentials near flatband and towards accumulation unless exceptionally high frequencies
352
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
are used. Lastly, differentiation of the φs versus VG curve can cause errors. Large discrepancies were found for Dit determined by the Terman technique compared with deep level transient spectroscopy (DLTS).65 GrayBrown and Jenq Method: In the GrayBrown method, the highfrequency capacitance is measured as a function of temperature.66 Reducing the temperature causes the Fermi level to shift towards the majority carrier band edge and the interface trap time constant τit increases at lower temperatures. Hence interface traps near the band edges should not respond to typical ac probe frequencies at low temperatures whereas at room temperature they do respond. This method should extend the range of interface traps measurements to Dit near the majority carrier band edge. The hf C –V curves are measured from room temperature to typically T = 77 K. The interface trap density is obtained from the flatband voltages at those temperatures. Just as the interface trap occupancy changes with gate voltage in the Terman method, so it changes with temperature in this method. It is this change that is analyzed and Dit is extracted from the experimental data. The original measurements were made at 150 kHz and gave characteristic peaks of interface traps near the band edges. Theoretical calculations later indicated that these peaks were an artifact by using too low ac probe frequencies.67 Frequencies near 200 MHz should be used to maintain highfrequency conditions near the band edges. It is useful as a fast, qualitative indicator of interface traps. In particular, an hf C –V measurement at 77 K shows a “ledge” in the curve.66, 68 This ledge voltage is related to the interface trap density over part of the band gap. A method related to the GrayBrown technique is the Jenq technique.69 The MOS device is biased into accumulation at room temperature. Then it is cooled to T = 77 K and swept from accumulation to deep depletion, driven into inversion by illumination or short circuiting the sourcedrain of a MOSFET, and then swept from inversion to accumulation. The hysteresis between the two curves is proportional to the average interface trap density over typically the central 0.7–0.8 eV of the band gap. A comparison of average Dit determined by this technique and by charge pumping shows excellent agreement over the 3 × 1010 ≤ Dit ≤ 1012 cm−2 eV−1 range.70 6.3.4
Charge Pumping
In the charge pumping method, originally proposed in 1969,71 a MOSFET is used as the test structure, making it suitable for interface trap measurements on smallgeometry MOSFETs instead of largediameter MOS capacitors. We explain the technique with reference to Fig. 6.27. The MOSFET source and drain are tied together and slightly reverse biased with voltage VR . The time varying gate voltage is of sufficient amplitude for the surface under the gate to be driven into inversion and accumulation. The pulse train can be square, triangular, trapezoidal, sinusoidal, or trilevel. The charge pumping current is measured at the substrate, at the source/drain tied together, or at the source and drain separately. Let us begin by considering the MOSFET in inversion shown in Fig. 6.27(a). The corresponding semiconductor band diagram—from the Si surface into the substrate—is shown in Fig. 6.27(c). For clarity we show only the semiconductor substrate on this energy band diagram. The interface traps, continuously distributed through the band gap, are represented by the small horizontal lines at the semiconductor surface with the filled circles representing electrons occupying interface traps. When the gate voltage changes from positive to negative potential, the surface changes from inversion to accumulation
INTERFACE TRAPPED CHARGE
Electrons V recombine G with holes
VG Trapped electrons
t1
t VR
VR n
t2 t VR
VR n
n Channel electrons
n Channel holes
p
p Icp
Icp (b)
(a) Channel
To S/D
Ec
Trapped electrons
(c)
353
Ev Hole barrier (d)
(e)
(f)
Fig. 6.27 Device crosssections and energy bands for charge pumping measurements. The figures are explained in the text.
and ends up as in Fig. 6.27(b) and (f). However, the important processes take place during the transition from inversion to accumulation and from accumulation to inversion. When the gate pulse falls from its high to its low value during its finite transition time, most electrons in the inversion layer drift to source and drain and electrons on those interface traps near the conduction band are thermally emitted into the conduction band (Fig. 6.27(d)) and also drift to source and drain. Those electrons on interface traps deeper within the band gap do not have sufficient time to be emitted and will remain on interface traps. Once the hole barrier is reduced (Fig. 6.27(e)), holes flow to the surface where some are captured by those interface traps still occupied by electrons. Holes are indicated by the open circles on the band diagrams. Finally, most traps are filled with holes as shown in Fig. 6.27(f). Then, when the gate returns to its positive voltage, the inverse process begins and electrons flow into the interface to be captured. Eight holes flow into the device in Fig. 6.27(b). Two are captured by interface traps. When the device is driven into inversion, six holes leave. Hence, eight holes in, six out result in a net charge pumping current, Icp , that is proportional to Dit . The time constant for electron emission from interface traps is τe =
exp(Ec − E1 )/kT ) σn vth Nc
(6.60)
where E1 is the interface trap energy measured from the bottom of the conduction band. The concepts of electron and hole capture, emission, time constants, and so on are discussed in Chapter 5. For a square wave of frequency f , the time available for electron emission is half the period τe = 1/2f. The energy interval over which electrons are emitted
354
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
is, from Eq. (6.60), Ec − E1 = kT ln(σn vth Nc /2f )
(6.61)
For example, Ec − E1 = 0.28 eV for σn = 10−16 cm2 , vth = 107 cm/s, Nc = 1019 cm−3 , T = 300 K and f = 100 kHz. Hence, electrons from Ec to Ec − 0.28 eV are emitted while those below Ec − 0.28 eV are not emitted and therefore recombine with holes, when holes come rushing in. The hole capture time constant is τc =
1 σp vth ps
(6.62)
where ps = hole density/cm3 at the surface. τc is very small for any appreciable hole density. In other words, emission, not capture, is the rate limiting process. During the reverse cycle when the surface changes from accumulation to inversion, the opposite process occurs. Holes within an energy interval E2 − Ev = kT ln(σp vth Nv /2f )
(6.63)
are emitted into the valence band and the remainder recombine with electrons flowing in from source and drain. E2 is the interface trap energy measured from the top of the valence band. Those electrons on interface traps within the energy interval E = EG − (Ec − E1 ) − (E2 − Ev ) E ≈ EG − kT [ln(σn vth Nc /2f ) + ln(σp vth Nv /2f )]
(6.64)
recombine. A detailed discussion of these concepts is given in ref. 72. Qn /q electrons/cm2 flow into the inversion layer from the source and drain but only (Qn /q –Dit E) electrons/cm2 flow back into the sourcedrain. Dit E electrons/cm2 recombine with holes. For each electronhole pair recombination event, an electron and a hole must be supplied. Hence Dit E holes/cm2 also recombine. In other words, more holes flow into the semiconductor than leave, giving rise to the charge pumping current Icp in Fig. 6.27. Dit E holes being supplied at rate of f Hz to a MOSFET with gate area AG gives the charge pumping current Icp = qAG f D it E. In our example E ≈ 1.12 − 0.56 = 0.56 eV. Substituting numerical values for a 10 µm × 10 µm gate area, a 100 kHz pump frequency, an interface trap density Dit = 1010 cm−2 eV−1 , and E = 0.56 eV gives Icp ≈ 10−10 A. As predicted, Icp has been found to be proportional to both gate area and pump frequency. The gate voltage waveform can be of various shapes. Early work used square waves. Later trapezoidal73 and sinusoidal74 waveforms were used. The waveforms can be constant base voltage in accumulation and pulsing with varying voltage amplitude V into inversion as illustrated in Fig. 6.28(a), or varying the base voltage from inversion to accumulation keeping V constant as in Fig. 6.28(b). The current saturates for the former, while for the latter it reaches a maximum and then decreases. The letters “a” to “e” on Fig. 6.28 correspond to the points on the current waveforms. The plot of charge pumping current versus gate voltage in Fig. 6.28(a) depends somewhat on sourcedrain voltage VR in Fig. 6.27. The nonsaturating characteristic sometimes observed for VR = 0 has been attributed to the recombination of those channel electrons
INTERFACE TRAPPED CHARGE
355
Depletion Icp
b
Strong accum.
Icp
c
Weak accum. b
Weak inversion d
a
a
Vbase
∆V
Strong inversion e
VFB VT
a b a
b
c
∆V
d (a)
(b) e ∆V
Fig. 6.28
Bilevel charge pumping waveforms.
unable to drift back to source and drain. This current is the “geometrical component” of Icp , with the total charge pumping current given by73 Icp = AG f [qDit E + αCox (VGS − VT )]
(6.65)
where α is the fraction of the inversion charge that recombines with holes before drifting back to the sourcedrain and AG is the gate area. The geometrical component is negligible for MOSFETs with short gate lengths or for gate pulse trains with moderate rise and fall times, giving the channel electrons sufficient time to drift back to source and drain. The basic charge pumping technique gives an average value of Dit over the energy interval E. It does not give an energy distribution of the interface traps. Various refinements have been proposed to obtain energydependent interface trap distributions. Elliot varied the pulse base level from inversion to accumulation keeping the amplitude of the gate pulse constant.75 Groeseneken73 varied the rise and fall times of the gate pulses while Wachnik75 used small pulses with small rise and fall times to determine the energy distribution of Dit . For a trapezoidal waveform, the recombined charge per cycle, Qcp = Icp /f , is given by73 VF B − VT  √ Qcp = 2qkT D it AG ln vth ni σn σp ζ 1 − ζ VGS f
(6.66)
where D it is the average interface trap density, VGS the gate pulse peakpeak amplitude, and ζ the gate pulse duty cycle. The slope of a Qcp versus log(f) plot gives Dit and the intercept on the log(f) axis yields (σn σp )1/2 . By using a voltage controlled oscillator, one can sweep the frequency continuously and plot Qcp versus log(f) to extract D it and (σn σp )1/2 .76 A plot of Qcp as a function of log(f) in Fig. 6.29 shows the expected linear
356
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
7 × 10−14 6 × 10−14
Qcp (C)
5 × 10−14 4 × 10−14 3 × 10−14 2 × 10−14
T = 300 K
1 × 10−14
A = 1.25 × 10−4 cm2
0 101
102
103
104
105
Frequency (Hz)
Fig. 6.29
MOSFET Qcp versus frequency; D it = 7 × 109 cm−2 eV−1 . Data adapted from. ref. 77.
dependence. The departure from linearity is due to traps not at the SiO2 Si interface, but within the oxide, discussed later in this section. The interface trap distribution through the band gap and capture crosssections can be determined with a trilevel waveform with an intermediate voltage level Vstep ,78 illustrated in Fig. 6.30, switching the device from inversion to an intermediate state near midgap, and then to accumulation instead of from inversion to accumulation directly. At point (a), the device is in strong inversion with interface traps filled with electrons. As the waveform changes to (b) electrons begin to be emitted from interface traps, starting with the traps nearest the conduction band. The gate voltage remains constant to point (c). For tstep ≫ τe , where τe is the emission time constant of interface traps being probed, all traps above ET have emitted their electrons and only those below ET are available for recombination when holes come in to recombine with the electrons at point (d) on the waveform. This gives a charge pumping current that saturates as tstep increases. For tstep < τe , fewer electrons have time to be emitted and more are available for hole recombination giving a correspondingly higher charge pumping current.
a VH VT c Vstep
b
tstep
d
VL Ec
ET Ev (a)
Fig. 6.30
(b)
(c)
(d)
Trilevel charge pumping waveform and corresponding band diagrams.
INTERFACE TRAPPED CHARGE
357
0.6
Icp (pA)
0.5
0.4 te 0.3 10−7
10−6
10−5 10−4 tstep (s)
10−3
10−2
(a)
Trap Density (cm−3)
1022 Al2O3
1020 1018
Insulator/Si Interface
1016
SiO2
1014 1012 −0.6
−0.5
−0.4
−0.3
−0.2
−0.1
0
Depth (nm) (b)
Fig. 6.31 (a) Icp as a function of tstep showing τe at the point where Icp begins to saturate. Reprinted after Saks et al. (Ref. 79) by permission of IEEE ( 1990, IEEE); (b) insulator trap density versus insulator depth from the insulator/Si interface for Al2 O3 and SiO2 . Data adapted from. ref. 80.
A typical Icp versus tstep plot in Fig. 6.31(a) shows the Icp saturation and the tstep = τe breakpoint. From the emission time τe one can determine the capture crosssection according to the expression τe =
exp(Ec − ET )/kT σn vth Nc
(6.67)
For a discussion of Eq. (6.67) see Chapter 5. By varying Vstep one can probe interface traps through the band gap. Of course, the surface potential must be related to Vstep by one of the techniques discussed in Section 6.3.1. The interface trap density is determined from the slope of the Icp versus tstep curve according to the expression79 Dit = −
dIcp 1 qkT AG f d ln tstep
(6.68)
358
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
The trilevel charge pumping current can be expressed as80 tstep ET − Ec exp − Icp = qAG f Dit ET − kT ln 1 − 1 − exp kT τe
(6.69)
Equation (6.69) simplifies for low and high tstep Icp (tstep → 0) ≈ qAG f Dit EG ; Icp (tstep → ∞) ≈ qAG f Dit ET
(6.70)
demonstrating that various portions of the band gap can be probed with the trilevel charge pumping approach. Furthermore, by reducing the pulse frequency, one can probe traps within the insulator. In this case, electrons tunnel into and out of those traps from the channel with the tunneling time depending exponentially on the trap distance from the interface.80 Example trap distributions are shown in Fig. 6.31(b) illustrating the higher trap density in Al2 O3 compared to SiO2 . Charge pumping can also determine the spatial variation of interface traps along the MOSFET channel by varying the drain and/or source bias leading to “AG ” variations caused by the drainsource spacecharge region extending into the channel region.81 Another method is the variation of voltage pulse amplitudes, thereby probing regions of the channel with varying threshold and flatband voltage.81 – 82 Charge pumping has also been used to determine the oxide trap density close to the SiO2 Si interface.83 The charge recombined per cycle, Qcp = Icp /f , should be independent of frequency. However, Qcp increases as the waveform frequency is reduced from typical frequencies of 104 –106 Hz to 10–100 Hz. At low frequencies there is sufficient time for electrons to tunnel to traps located in the oxide and to recombine there. Such traps are sometimes referred to as border traps.84 Charge pumping can also be implemented by varying the temperature and keeping the gate waveform frequency constant.85 For silicononinsulator MOSFETs, there are two SiO2 /Si interfaces and charge pumping currents depend on the state of the back interface. It is highest with the bottom interface in depletion.86 Interface trap densities determined by various measurement techniques are shown in Fig. 6.32. The charge pumping current is assumed to be due electronhole pair recombination at interface traps with Icp given by Eq. (6.65). For thin oxides, there is an additional gate
Dit (cm−2eV−1)
1013 Quasistatic
1012 Spectrosc. CP
1011 1010 109
2 Level CP
0
0.2
3 Level CP 0.4
0.6
DLTS 0.8
1
Energy (eV)
Fig. 6.32 Interface trap density as a function of energy through the band gap for various measurement techniques. Data after ref. 88.
INTERFACE TRAPPED CHARGE
359
3 Before Before After After
∆V = 1 V
Icp (pA)
2
1 0.3 V 0 −1
−0.8
−0.6 −0.4 Vbase (V)
−0.2
0
Fig. 6.33 Charge pumping current versus base voltage for two voltage pulse heights before and after gate leakage current correction. tox = 1.8 nm, f = 1 kHz. Adapted from ref. 87.
current that adds to the charge pumping current. Jcp = 4 × 10−3 A/cm2 for f = 1 MHz, Dit = 5 × 1010 cm−2 eV−1 , and E = 0.5 eV. The gate oxide leakage current can easily exceed this value. The charge pumping to gate oxide leakage current density ratio is qfD it E 4 × 10−3 Jcp = ≈ JG JG JG
(6.71)
Fig. 6.33 shows the effect of gate oxide leakage current on Icp .87 At sufficiently low frequencies, the gate leakage current dominates and can be subtracted from the total current. 6.3.5
MOSFET Subthreshold Current
The drain current of a MOSFET operated at gate voltages below threshold (subthreshold) is89 qVDS q(VGS − VT ) 1 − exp − (6.72) ID = ID1 exp nkT kT where ID1 depends on temperature, device dimensions and substrate doping density; n, given by n = 1 + (Cb + Cit )/Cox , accounts for the charge placed on the gate that does not result in inversion layer charge. Some gate charge is imaged as spacecharge region charge and some as interface trap charge. Ideally n = 1, but n > 1 as the doping density increases (Cb ∼ NA 1/2 ) and as the interface trap density increases (Cit ∼ Dit ). The usual subthreshold plot is log(ID ) versus VGS for VDS ≫ kT /q. Such a plot has a slope of q/[ln(10)nkT ]. The slope is usually expressed as the subthreshold swing S, which is that gate voltage necessary to change the drain current by one decade, and is given by ln(10)nkT 60nT 1 = ≈ mV/decade (6.73) S= Slope q 300 with T in Kelvin.
360
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
The interface trap density, obtained from a plot of log(ID ) versus VG is Cb Cox qS −1 − 2 Dit = 2 q ln(10)kT q
(6.74)
requiring an accurate knowledge of Cox and Cb . The slope also depends on surface potential fluctuations. This is the reason that this method is usually used as a comparative technique in which the subthreshold swing is measured, then the device is degraded and remeasured. The change in Dit is given Dit =
Cox (Safter − Sbefore ) ln(10)qkT
(6.75)
The assumption in Eq. (6.75) is that the interface trap creation is uniform along the MOSFET channel. This is generally not the case when the MOSFET is stressed with gate and drain voltages and Dit gives an average value. Subthreshold MOSFET curves are shown in Fig. 6.34 before and after stress, causing a threshold voltage shift and a slope change. For the SiO2 Si interface, interface traps in the upper half of the band gap are acceptors and those in the lower half are donors with the demarcation between the two occurring at about half the band gap. Hence when the surface potential coincides with the Fermi level, as shown in Fig. 6.35(a) by φs = φF at the surface, interface traps in the upper half are empty of electrons and neutral, and those in the lower half are occupied by electrons, hence also neutral, and the traps do not contribute to a gate voltage shift. We define a voltage Vso as Vso = VT − Vmg
(6.76)
where Vmg is the midgap gate voltage, which is typically the gate voltage at ID ≈ 0.1–1 pA. Increasing the gate voltage from Vmg to VT fills interface traps in the upper half of the band gap with electrons (Fig. 6.35(b)). The subthreshold curve shifts, causing Vso to change from Vso1 to Vso2 . From this shift the interface trap density change Nit is90 Vit Cox (6.77) Vit = Vso2 − Vso1 and Nit = Dit E = q 10−6 Drain Current (A)
10−7 10−8
Before stress
10−9
∆VT
After stress
10−10 10−11 10−12 10−13
∆Dit = 5 × 1011 cm−2eV−1 0
0.2
0.4 0.6 Gate Voltage (V)
0.8
1
Fig. 6.34 MOSFET subthreshold characteristics before and after MOSFET stress. The change in slope results in a stressgenerated Dit = 5 × 1011 cm−2 eV−1 .
INTERFACE TRAPPED CHARGE
Ec
fF
Ei ∆E
Ev
fs = fF
Vmg
361
EF
fs = 2fF VT (b)
(a)
Fig. 6.35
Band diagrams for midgap and threshold voltages.
where Nit is the increased interface trap density within the energy interval E shown in Fig. 6.35(b). E usually covers the range from midgap to strong inversion. Since at midgap the interface traps do not contribute any voltage shift, a shift at Vmg must then be due to oxide trapped charge according to Vot = Vmg2 − Vmg1 and Not =
6.3.6
Vot Cox q
(6.78)
DCIV
The DCIV method is a dc current technique.91 We explain it with reference to the MOSFET in Fig. 6.36(a). With the source S forward biased, electrons are injected into the pwell. Some electrons diffuse to the drain to be collected and measured as drain current ID . Some electrons recombine with holes in the pwell bulk (not shown) and some recombine with holes at the surface below the gate. Only the surfacerecombining electrons are influenced by the gate voltage. The holes lost by recombination are replaced by holes from the body contact leading to body current IB . In contrast to a regular MOSFET with the source usually grounded, here the source is forward biased. In some DCIV publications the source is referred to as the emitter, the drain as the collector, the
S
B
G
D ID
IB p+
n+ IB
VGB = 0 +
n
xx x + IC n
p Well VGB > 0 n+
p Well
p Well VGB < 0
n Substrate
n+ p Well Sub (a)
(b)
Fig. 6.36 (a) MOSFET configuration for DCIV measurements and (b) crosssections showing the spacecharge regions and the encircled surface generation regions.
362
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
body as the base, and the currents as the collector and base currents and the nsubstrate has been used as the electron injector/source. The electronhole pair surface recombination rate depends on the surface condition. With the surface in strong inversion or accumulation, the recombination rate is low. The rate is highest with the surface in depletion.92 The body current is given by IB = qAG ni sr exp(qVBS /2kT )
(6.79)
where sr is the surface recombination velocity given by sr = (π/2)σo vth Nit
(6.80)
with σo the capture crosssection (assuming σn = σp = σo ). Although the MOSFET in Fig. 6.36 resembles a bipolar junction transistor, it has the additional feature that the region between source (S) and drain (D) can be varied with the gate voltage. When the gate voltage exceeds the flatband voltage, a channel forms between S and D and the drain current will increase significantly. For VGB = VT , the ID − VGB curve saturates. If charge is injected into the oxide, leading to a VT shift, the drain current will also shift. It is this shift that can be used to determine oxide charge. We should point out that the interface trap density determined with the subthreshold slope method samples the band gap between midgap and strong inversion, while the DCIV body current samples the band gap between subthreshold and weak accumulation, i.e., surface depletion. By varying the gate voltage, different regions of the device are depleted (Fig. 6.36(b)) and those regions can be characterized, allowing spatial Dit profiling. Experimental DCIV data are shown in Fig. 6.37 for a MOSFET before and after gate current stress.93 A clear peak is observed at maximum surface recombination around VGB = 0. In this example the method was used to determine interface trap generation caused by gate oxide current stress and plasma charging damage. A comparison of interface traps determined by charge pumping and DCIV, gave very similar results.81 Both techniques allow lateral trap profiling.
30 Body Current (pA)
820 s stress 20
No stress
10
0 −1
0
1
Gate Voltage (V)
Fig. 6.37 DCIV measured body currents. (a) control wafer, (b) stressed with −12 mA/cm2 gate current density. VBS = 0.3 V, W/L = 20/0.4 µm, tox = 5 nm. Data adapted from ref. 93.
INTERFACE TRAPPED CHARGE
6.3.7
363
Other Methods
A sensitive method to determine Dit is deeplevel transient spectroscopy, covered in Chapter 5. The charge transfer loss in chargecoupled devices (CCD) is also a sensitive indicator of interface trap densities,94 but is not practical if a CCD has to be specially fabricated as the test structure. In the surface charge analyzer method, the oxide in an MOSC is replaced by a mylar sheet and the gate is replaced by an optically transparent, electrically conducting layer.95 By exposing the sample to above band gap light, that creates ehp in the semiconductor through the transparent gate, the ac surface photovoltage is given by95 q(1 − R) W (6.81) δVSP V = 4f Ks εo where is the incident photon flux density, W the spacecharge region width, and f the modulated light frequency. W is determined from a measurement of δVSPV . With the mylar sheet about 10 µm thick, the measured series mylaroxide capacitance is dominated by Cmylar and the total charge is Q = QS + Qox + Qit = −CVG ≈ −Cmylar VG
(6.82)
Knowing W allows QS to be determined. Qox and Qit are then determined by the usual MOSC analyses. Changing the bias voltage drives the Si surface into inversion, depletion, or accumulation. Since the electrode is separated from the sample by the 10 µm thick mylar film, its small probe capacitance is dominant and leakage current is suppressed. The interface trap density and energy are given by96 Dit (E) =
Ks εo q 2W
1 dQ −1 qNA dW
E = EF − Ei + qφs = kT ln
(6.83)
NA ni
−
qNA W 2 2Ks εo
(6.84)
Since the spacecharge region width W is measured instead of the capacitance, this technique is independent of oxide thickness, in contrast to some of the earlier methods that depend sensitively on tox and their interpretation becomes difficult for thin oxides with high oxide leakage currents. Furthermore, there is no need for quantum mechanical and gate depletion corrections. It is, however, influenced by the substrate doping density and NA should not be higher than about 1017 cm−3 . The technique can be used as an inline method to obtain surface charge information, e.g., follow various cleaning cycles. In one comparison between the SCA and conventional MOSC methods, the SCA method fared very well, especially due to its shorter measurement cycle, since devices need not be fabricated.95 It has also been used to determine Dit for SiO2 , HfO2 , and Si3 N4 for equivalent oxide thicknesses of 1–3 nm.96 Crystallographic structural information on interface traps can be obtained from electron spin resonance (ESR) measurements,97 but the method is relatively insensitive and Dit ≥ 1011 cm−2 eV−1 is required. ESR was instrumental in identifying dangling bonds at the SiO2 /Si interface as interface traps.98 Figure 6.38 shows the two major Si oriented surfaces and the associated dangling bonds, designated Pb , Pb0 , and Pb1 centers.
364
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
Pb0
Silicon (100)
Fig. 6.38
6.4
Pb1
Si
O
H
Pb
Silicon (111)
Silicon surface for (100) and (111) orientation showing the Pb0 , Pb1 , and Pb centers.
OXIDE THICKNESS
The oxide thickness is an important parameter for the interpretation of many of the techniques discussed in this chapter. Electrical, optical and physical methods are used in its determination, including C –V , I –V , ellipsometry, transmission electron microscopy (TEM), Xray photoelectron spectroscopy (XPS), medium energy ion scattering spectrometry (MEIS), nuclear reaction analysis (NRA), Rutherford backscattering (RBS), elastic backscattering spectrometry (EBS), secondary ion mass spectrometry (SIMS), grazing incidence Xray reflectometry (GIXRR), and neutron reflectometry. We discuss the C –V method here and mention other methods briefly. Some of them are detailed in later chapters. A recent joint study by numerous techniques (MEIS, NRA, RBS, EBS, XPS, SIMS, ellipsometry, GIXRR, neutron reflectometry and TEM) compared oxide thicknesses of 10 carefully prepared samples covering oxide thicknesses of 1.5 to 8 nm.99 There are three thickness offsets: water and carbonaceous contamination equivalent to ∼1 nm and adsorbed oxygen mainly from water at an equivalent thickness of 0.5 nm. The existence of an interfacial layer between silicon dioxide and silicon is accepted by a majority of the technical community. There is approximately 1 monolayer (ML) of an interfacial layer at the SiO2 /Si interface.100 There is evidence for up to ∼1 ML of additional substoichiometric oxide located within the first 0.5 to 1 nm of the interface. Each characterization method probes slightly different aspects of the interface. Xray reflectivity and Xray photoelectron spectroscopy support the presence of stress as do infrared IR measurements. Xray photoelectron spectroscopy shows the presence of at least a monolayer film of incompletely oxidized silicon. Infrared spectroscopy further supports the presence of substoichiometry at the interface. Thus ellipsometry observes a slab of mixed dielectric constant. Stress within the oxide layer itself, i.e., above the interface plane, is supported by Xray reflectivity and Xray photoelectron spectroscopy. Ellipsometry determines thickness based on optical models that include an interfacial layer. The long wavelength of ellipsometry and the need to sample a large area results in an averaged sampling of interfacial optical properties. 6.4.1
CapacitanceVoltage
It would seem that capacitancevoltage data lend themselves to oxide thickness determination with the MOS device in strong accumulation. Complications arise for thin oxides that render conventional methods questionable. These complications include FermiDirac rather than Boltzmann statistics, quantization of carriers in the accumulation layer, polySi gate depletion, and oxide leakage current. The capacitance of the depleted gate and of the accumulation layer, being in series with the oxide capacitance, lead to thicker effective oxides than simple theory would predict.101
OXIDE THICKNESS
365
In the Maserjian, the McNutt and Sah, and the Kar methods, the following assumptions are made: the interface trap capacitance is negligible in accumulation at 100 kHz1 MHz, the differential interface trap charge density, between flatband and accumulation is negligible, the oxide charge density is negligible, and quantization effects are neglected. The relevant equations are for the McNuttSah method102
dChf ,acc 1/2 q
=
(Cox − Chf ,acc )
dV 2kT Cox
(6.85)
where Chf ,acc is the highfrequency accumulation capacitance. A plot of (dChf ,acc /dV )1/2 versus Chf ,acc yields Cox as the intercept on the Chf ,acc axis and from the slope. For the Maserjian method103 1 = + Cox
1 Chf ,acc
2 b2
1/3
1 Chf ,acc
dChf ,acc 1/6
dV
(6.86)
where b is a constant. One plots Chf ,acc −1/2 (dChf ,acc /dV )1/6 versus 1/Chf ,acc . If a linear fit is obtained, then its intercept on the 1/Chf ,acc axis yields 1/Cox . With quantization effects, the equation becomes104 1 Chf ,acc
1/4
d(1/C 2 1 hf ,acc )
= +s
Cox dV
(6.87)
where s is a constant. Equation (6.87) has a simpler form than Eq. (6.86). In this case, one plots 1/Chf ,acc versus (d(1/Chf ,acc 2 )/dV )1/4 . For a linear fit, its intercept on the 1/Chf ,acc axis yields 1/Cox . For the Kar method105 1 Chf ,acc
1 = + Cox
1 2β
1/2
d(1/C 2
hf ,acc )
,
dV
(6.88)
where β is a constant. Here, one plots 1/Chf ,acc versus (d(1/Chf ,acc 2 )/dV )1/2 . For a linear fit, its intercept on the 1/Chf ,acc axis yields 1/Cox . This method has been successfully used for 1–8 nm thick highK dielectrics. A variation of the Maserjian method is based on the following equations.106 The capacitance with the device in accumulation is 1 1 1 Kox εo A dQacc = + ; Cox = ; CS = C Cox CS tox dφs
(6.89)
(6.90)
with Qacc = K exp
qφs 2kT
giving CS =
qQacc . 2kT
Using VG = VF B + φ s −
Qacc 2kT CS → VG − VF B − φ s = − . Cox q Cox
(6.91)
366
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
2.6 2.5 1/C (cm2/µF)
2.4 2.3 2.2
7.3 nm (7 nm optically)
2.1 2 1.9 1.8 1.7
5.8 nm (5.5 nm optically) 0
0.5
1
1.5
2
2.5
3
3.5
4
1/(VG − VFB) (V −1)
Fig. 6.39 1/C versus 1/(VG − VF B ) for two oxide thicknesses. Reprinted after Vincent et al. (Ref. 106) by permission of IEEE ( 1997, IEEE).
Combining Eqs. (6.89) and (6.91) gives 1 2kT 1 2kT 1 1 1 = − ≈ − . C Cox qCox VG − VF B − φs Cox qCox VG − VF B
(6.92)
The approximation in Eq. (6.92) holds for (VG − VF B ) ≫ φs , valid in strong accumulation. Equation (6.92) suggests a plot of 1/C versus 1/(VG − VF B ), as illustrated in Fig. 6.39. The 1/C axis intercept is 1/Cox . Although polySi gate depletion affects the second term of Eq. (6.92), it does not alter the intercept and can be neglected. A more accurate approach without the Eq. (6.92) approximation is given in ref. 107. The oxide thickness can also be determined from a plot of gate corona charge versus gate voltage of an MOS capacitor discussed in Chapter 9. One can also vary the frequency of the applied signal. Measuring the circuits in Figs. E6.5(a) and (b) at two different frequencies, allows the various components in Fig. 6.4(a) to be determined108 C=
Gt (1 + rs Gt ) f12 CP2 1 (1 + D12 ) − f22 CP2 2 (1 + D22 ) GP = + ωrs C ;D = 2 2 ωCP ωC f1 − f2
(6.93)
where D1 and CP 1 refer to measured values at frequency f1 and D2 and CP 2 at f2 . Gt =
ω2 CP C(1 + D 2 ) − (ωC)2
Gt D − 2 rs = 2 ωCP (1 + D ) Gt + (ωC)2
(6.94) (6.95)
A detailed analysis of the twofrequency method has shown that D should be less than 1.1.109 For thin oxides, the device area must be reduced for D < 1.1 but the device must remain sufficiently large not to be limited by the capacitance meter’s lower measurement limit. Reductions of Gt and rs lead to higher D, implemented by reducing the device area
OXIDE THICKNESS
367
because Gt ∼ area and rs ∼ 1/area 1/2 due to spreading resistance. The minimum radial frequency, determined from Eq. (6.93) 1 Gt 1+ ωmin = (6.96) C rs Gt leads to the minimum dissipation factor Dmin = 2 rs Gt (1 + rs Gt )
(6.97)
Figure 6.40 shows the dependence of measurement error on device area and oxide thickness. For a f = 1 MHz oxides to about 1.5 nm can be measured. The frequency in Fig. 6.40 refers to the higher of the two frequencies. Treating the MOSFET as a transmission line leads to the capacitance110 C ≈ Cm
1 + cosh (K) 1 + sinh (K)/K
6.98
where K = (rs′ G′t L2 )1/2 and Cm is the measured capacitance, L the gate length and W Zdc 4 2 ′ cosh−1 (/square) (6.99) rs = L Ydc 4 − Zdc Ydc 2 − Zdc Ydc 2 cosh−1 1 2 − Zdc Ydc G′t = (S/cm2 ) (6.100) WL Zdc 4 Ydc 4 − Zdc Ydc where W is the gate width. The measurement is a dc measurement with the MOSFET source and substrate (or CMOS well) grounded. The gate voltage is swept over an appropriate voltage range and the dc gate admittance Ydc is determined from the slope of the IG − VGS curve. At each gate voltage, the drain voltage is swept from −15 mV to
Device Area (µm2)
105
D = 1.1
104
f = 1 MHz
103
Error < 4%
f = 600 kHz
102 D = 1.1
Cmin = 1 pF
101 1
10 Oxide Thickness (nm)
Fig. 6.40 Measurement error dependence on device area and oxide thickness. The twofrequency measured capacitance is in error less than 4% in the shaded region. At higher frequencies the D = 1.1 border shifts to thinner oxides. Adapted from ref. 109.
368
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
+15 mV and the slope of the ID − VDS yields the dc drain impedance Zdc . Both rs ′ and Gt ′ are strongly gate voltage dependent and need to be accurately measured. Corrections are required for longer gates, because the increased channel resistance leads to reduced capacitance. Similarly, thinner oxides lead to higher gate current and increased channel voltage drop and require corrections. The method has proven successful for oxides as thin as 0.9 nm.
Exercise 6.6 Problem: What is the effect of gate leakage current and series resistance on C –V behavior? Solution: In accumulation with no interface traps, the equivalent circuit from Fig. 6.24 becomes Fig. E6.5(a). Following Chapter 2, we convert it to the parallel and series equivalent circuits in Figs. E6.5(b) and (c) where
C G 2 . ; CS = C 1 + CP = (1 + rs G)2 + (ωrs C)2 ωC
CS
Cox
C
Gt
GP
Cs
CP RS
rs
(a)
2 × 10−6 Capacitance (F)
(c)
(b)
Ideal CP, 100 kHz CP, 200 kHz CS, 100 kHz CS, 200 kHz
1.5 × 10−6 1 × 10−6
5 × 10−6 0 × 10−0 −3
−2
−1 0 Gate Voltage (V)
1
2
(d)
Fig. E6.5 (a) MOSC equivalent circuit with tunnel conductance and series resistance, (b) parallel, (c) series equivalent circuits, and (d) calculated C –VG curves.
STRENGTHS AND WEAKNESSES
369
To understand the basic concepts, we have used a simple constant series resistance rs = 0.5 , tox = 3 nm, NA = 1017 cm−3 , and Gt = exp(1/VG ) for VG < 0. The resulting CP and CS as well as the ideal (rs = Gt = 0) capacitances are shown in Fig. E6.5(d). CP decreases and CS increases as a result of Gt , making oxide thickness extraction more difficult. Of course, the actual dependence of Gt on gate voltage differs from this simple model, but it illustrates the main concept. This kind of behavior has been experimentally verified, e.g., D.P. Norton, “CapacitanceVoltage Measurements on Ultrathin Gate Dielectrics,” SolidState Electron. 47, 801–805, May 2003.
6.4.2
CurrentVoltage
Oxide currentvoltage characteristics are discussed in Chapter 12. Here we briefly give the relevant equations and how they relate to oxide thickness. The current flowing through an insulator is either FowlerNordheim (FN) or direct tunnel current. The FN current density is B (6.101) JF N = AEox2 exp − Eox where Eox is the oxide electric field and A and B are constants. The direct tunnel current density is B(1 − (1 − qVox / B )1.5 ) AVG kT C exp − (6.102) Jdir = 2 tox q Eox where B is the semiconductorinsulator barrier height and Vox the oxide voltage. Both currents are very sensitive to oxide thickness. Tunneling currents also contain a small oscillatory component. These oscillations arise due to the quantum interference of electrons and show a strong dependence on oxide thickness, suggesting that these oscillations can be used for oxide thickness determination.111 6.4.3
Other Methods
Ellipsometry, discussed in Chapter 10, is suitable for oxides into the 1–2 nm regime. Variable angle, spectroscopic ellipsometry is especially suited for oxide thickness measurements. Transmission Electron Microscopy, discussed in Chapter 11, is very precise and usable to very thin oxides, but sample preparation is tedious. Xray Photoelectron Spectroscopy and other beam techniques are discussed in Chapter 11. 6.5
STRENGTHS AND WEAKNESSES
Mobile Oxide Charge: The strength of the bias temperature stress method is its simplicity requiring merely the measurement of a C –V curve, albeit at elevated temperatures. Its weakness is that the total mobile charge density is measured. Separation of various species is not possible. Furthermore, occasionally the C –V curve becomes distorted due to interface trapped charge and the flatband voltage is difficult to determine. The main strengths of the triangular voltage sweep method are its ability to differentiate between different mobile charge species, its higher sensitivity, and the fact that the method is fast because the sample does not need to be heated and cooled; it needs only to be
370
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
Subthreshold ID − VG
Jenq
DLTS Gray/Brown
Quasistatic
lf CV
Ec
hf CV
heated. Since a current or charge is measured, this method lends itself to determination of mobile charge in interlevel dielectrics, which is not possible with capacitance methods. Its weakness is the increasing oxide leakage current for thin oxides. Interface Trapped Charge: For MOS capacitors the choice for the most practical methods lies between the conductance and the quasistatic methods. These are the two most widely used techniques. The strength of the conductance method lies in its high sensitivity and its ability to give the majority carrier capture cross sections. Its major weakness is the limited surface potential range over which Dit is obtained and the required effort to extract Dit , although simplified methods have been proposed. The main strengths of the quasistatic method (both the I –V and the Q–V ) are the relative ease of measurement and the large surface potential range over which Dit is obtained. A weakness for the I –V version is the current measurement requirement. The currents are usually low because the sweep rates must be low to ensure quasiequilibrium. The Q–V version alleviates some of these problems. For both techniques, increased gate oxide leakage currents are problematic for thin oxides, making the methods difficult or impossible. For MOSFETs the choice is charge pumping, subthreshold current, and DCIV methods. The chief strengths are the direct measurement of the current, which is proportional to Dit and the fact that measurements can be made on regular MOSFETs with no need for special test structures. Charge pumping has been used to determine a single interface trap.112 It can also determine the insulator trap density. Its main weaknesses are that unless special measurement variations and interpretations are used, one gets a single value for an average interface trap density  not the energy distribution of Dit and the measurement is sensitive to gate leakage current. The subthreshold method is simpler to implement than charge pumping but is difficult to interpret for interface trap measurement. It is more useful when determining the change of interface trap density following hot electron stressing or energetic radiation exposure. DCIV yields results similar to CP, but the measured current is related to the surface recombination velocity and the capture crosssection needs to be known to extract the interface trap density.
Ei
Ev
Charge Pump. Conductance
Fig. 6.41 Ranges of energy in the band gap of a ptype Si substrate over which interface trap charges are determined by various characterization techniques.
APPENDIX 6.1
371
The various energies over which interface trap charges can be determined are shown in Fig. 6.41. A good discussion of various interface trap charge measurement techniques with their strengths and weaknesses is given in ref. 113. Oxide Thickness: Among the electrical techniques, MOS C –V measurements are most common. However, thin oxide leakage currents make the measurement interpretation more difficult. Occasionally, I –V data are used for thickness extraction. Ellipsometry is routinely used for oxide thickness measurements, being sensitive to very thin oxides. However, the optical parameters of the layer must be known and for thin oxides the insulator may be inhomogeneous. Among the physical characterization techniques, XPS is suitable for very thin oxides. An excellent overview of SiO2 and nitrided oxide including fabrication and characterization issues is given by Greene et al.114
APPENDIX 6.1 Capacitance Measurement Techniques Most capacitance measurements are made with capacitance bridges or capacitance meters. In the vector voltagecurrent method of Fig. A6.1, ac signal vi is applied to the device under test (DUT) and the device impedance Z is calculated from the ratio of vi to the sample current ii . A highgain operational amplifier with feedback resistor RF operates as a currenttovoltage converter. With the input to the opamp at virtual ground, the negative terminal is essentially at ground potential, because the high input impedance allows no input current to the opamp, ii ∼ io . With ii = vi /Z and io = −vo /RF , the device impedance can be derived from vo and vi as Z=−
R F vi vo
(A6.1)
where the device impedance of the parallel G–C circuit in Fig. A6.1 is given by Z=
G j ωC − 2 G2 + (ωC)2 G + (ωC)2
(A6.2)
It consists of a conductance, the first term, and a susceptance, the second term. The voltages vo and vi are fed to a phase detector and the conductance and susceptance of DUT RF G ii – vi
~
C
+
io vo
vi Phase Detector
Zx
Z
Fig. A6.1
Schematic circuit diagram of a capacitanceconductance meter.
372
OXIDE AND INTERFACE TRAPPED CHARGES, OXIDE THICKNESS
Hi
Lo
G
VGS < VT
Lo Cov
Cch
Hi C
C1
Cov
C
2
(a)
(b)
Fig. A6.2 Threeterminal capacitance measurement connections: (a) the measurement principle, (b) a MOSFET.
the sample are obtained by using the 0◦ and 90◦ phase angles of vo referenced to vi . The zero degree phase angle gives the conductance G while the 90◦ phase angle gives the susceptance or the capacitance C. Although this method uses a simple circuit configuration and has relatively high accuracy, it is difficult to design a feedback resistor amplifier with io in exact proportion to ii at high frequencies. An autobalance circuit incorporating a null detector and a modulator overcomes this problem.115 More detailed discussions of capacitance measurement circuits, probe stations, and other capacitance measurement hints can be found in the book by Nicollian and Brews.24 Some capacitance meters are threeterminal while others are fiveterminal instruments. One of the terminals in either instrument is ground while the others connect to the device under test. The fiveterminal instrument operates much like a fourpoint probe with the outer two terminals supplying the current and the inner two terminals measuring the potential. The ground terminal on these instruments gives additional flexibility by eliminating stray capacitances. Two examples with the ground terminal in a capacitance meter are shown in Fig. A6.2. Consider a threeterminal device with conductance G and capacitance C, which also has stray capacitances C1 and C2 shown in Fig. A6.2(a). By connecting the DUT to the capacitance meter (HiLo) and the two stray capacitances to ground, C1 and C2 are eliminated from the measurement by shunting them to ground. The MOSFET of Fig. A6.2(b) is arranged to determine the gatesource and gatedrain overlap capacitances Cov , by shunting the oxide capacitance in the channel region, Cch , to ground. To determine Cch , one connects the gate and substrate to the capacitance meter and shunts the source and drain to ground. The internal structure of the device, e.g., substrate resistance or CMOS well resistance, play a role in capacitance measurements of the type in Fig. A6.2(b) especially for small capacitances.116
APPENDIX 6.2 Effect of Chuck Capacitance and Leakage Current When device capacitance is measured at the wafer level, with the wafer resting on a chuck, precautions must be observed for the measurement setup not to influence the results. Consider the experimental arrangement in Fig. A6.3(a). The “Hi” terminal of
373
APPENDIX 6.2
Hi
Lo
GP rs
Hi p+
+
n
I2 I1
Lo
n+ CP
p
~
V
I1
C1
I2
C1
(b)
(a)
Cm (pF)
12 8
10−5 S
4
10−4 S
0
(7.46)
and the solution of Eq. (7.25) is18 n(t) =
τeff t t − exp − Go exp − 1 − τeff /τflash τflash τeff
(7.47)
For τeff < τflash , the sample is in quasi steadystate during the measurement. Hence, the flash lamp decay time must be sufficiently long for the QSSCP measurement to be valid. An example QSSCP plot is shown in Fig. 7.10, illustrating the increasing SRH lifetime with injection level followed by lifetime decrease due to Auger recombination. 7.4.3
ShortCircuit Current/OpenCircuit Voltage Decay (SCCD/OCVD)
The recombination lifetime can be determined by monitoring the pn junction voltage, current, and short circuit current decay after optical generation of excess carriers.38 – 40 The combination opencircuit voltage decay/shortcircuit current decay method was developed for characterizing the lifetime, diffusion length, and surface recombination velocity of solar cells in which the base width is typically on the order of or less than the minority carrier diffusion length, making the determination of these parameters difficult. In contrast to most other methods in which only a single parameter is measured, two measurements the shortcircuit current and the opencircuit voltage  are necessary to determine τr and sr . The theory is based on a solution of the minority carrier differential equation [Eq. A7.13] subject to the boundary conditions40 sr 1 ∂n(x, t) =− for x = d n(x, t) ∂x Dn n(0, t) = 0
(7.48a) (7.48b)
RECOMBINATION LIFETIME—OPTICAL MEASUREMENTS
403
1200 SRH Recomb.
1000
teff (µs)
800
Auger Recomb.
600 400 200 0 1012
1013
1014 1015 1016 Injection Level (cm−3)
1017
Fig. 7.10 Effective recombination lifetime versus injection carrier density obtained with the QSSPC technique. Adapted from ref. 37.
for the shortcircuit current, and ∂n(x, t) = 0 for x = 0 ∂x
(7.49)
for the opencircuit voltage method. So far we have only concerned ourselves with substrate minority carrier recombination in n+ p junctions. There is, of course, also minority carrier recombination in the scr and in the heavily doped n+ emitter. The minority carriers are swept out of the scr by the electric field in times on the order of 10−11 s under shortcircuit conditions. The emitter lifetime is generally much lower than the base lifetime, and emitter contributions play a role only during the early phase of the current decay.41 Emitter recombination causes carriers from the base to be injected into the emitter where they recombine at a faster rate. However, the voltage decay is determined by the base recombination parameters for long times.42 If the asymptotic decay rate is measured after the initial transient, then a decay time, representative of base recombination, is observed.41 The current decay is found to be exponential with time, with the time constant determined by the time dependence of the excess carrier density. The voltage decay can be significantly influenced by the junction RC time constant, which can be very large for largearea junction devices. This effect is reduced by measuring the smallsignal voltage decay with a steadystate bias light to reduce R.43 One might expect the current and voltage decays to be identical for devices with the base much thicker than the minority carrier diffusion length because sr is no longer important. This is indeed the case. Both have the asymptotic time dependence Isc , Voc ∼
exp(−t/τB ) √ t
(7.50)
This method is one of few allowing both the lifetime and surface recombination velocity at the back surface to be determined, by measuring the current and voltage decays of the same device. Being a transient technique, it is subject to higherorder decay time constants and possible trapping. These potential sources of error are considerably reduced by measuring the time constants asymptotically toward the end of the decay and using a bias light.
404
7.4.4
CARRIER LIFETIMES
Photoluminescence Decay (PLD)
Photoluminescence decay is another method of monitoring the time dependence of excess carriers. Excess carriers are generated by a short pulse of incident photons with energy hν > EG . The excess carrier density is monitored by detecting the time dependence of the light emitted by the recombining electronhole pairs. The PL signal is higher for efficient lightemitting direct band gap semiconductors, e.g., GaAs or InP, than for indirect band gap semiconductors, e.g., Si or Ge, for which photoluminescence is quite inefficient. Instead of optical excitation, electronbeam excitation can also been used in transient cathodoluminescence. The excess carrier density and time decay expressions are those discussed in Section 7.4.1. We expect PL decay to follow those considerations, except that the PL intensity is given by d
P L (t) = K
n(x, t) dx
(7.51)
0
where K is a constant accounting for the solid angle over which the light is emitted and for the reflectivity for the radiation emitted from the sample and d is the sample thickness. A complication arises if selfabsorption takes place, where some of the photons generated by the recombination radiation are absorbed by the semiconductor. Once absorbed they can create ehps. The lifetime expression becomes44 1 τP L
=
1 τnon−rad
+
1 1 + τS γ τrad
(7.52)
where τnon−rad , τrad and τs are the nonradiative, the radiative, and the surface lifetimes; γ is the photon recycling factor. Selfabsorption is not important for indirect bandgap semiconductors since the optical absorption coefficient is low for near bandgap photons, but it can be important for direct bandgap semiconductors. A discussion of PL lifetime determination is given in ref. 45. PL decay has been used to map the lifetime in Si power devices by scanning the excitation beam across the device.46 7.4.5
Surface Photovoltage (SPV)
The steadystate surface photovoltage method determines the minority carrier diffusion length using optical excitation. The diffusion length is related to the recombination lifetime through the relation Ln = (Dτr )1/2 . SPV is an attractive technique, because (1) it is nondestructive and contactless, (2) sample preparation is simple (no contacts, junctions, or high temperature processing required), (3) it is a steadystate method relatively immune to the slow trapping and detrapping effects that can influence transient measurements, and (4) the equipment is commercially available. The SPV technique was first described in 195747 to determine diffusion lengths in Si48 – 49 and GaAs.49 The sample is assumed to be homogeneous and of thickness d in Fig. 7.11. One surface is chemically treated to induce a surface spacecharge region (scr) of width W . The scr is the result of surface charges, not due to a bias voltage. The surface with the induced scr is uniformly illuminated by chopped monochromatic light of energy higher than the band gap, with the back surface kept in the dark. The light is chopped to enhance the signal/noise ratio using lockin techniques. The wavelength is varied during the measurement. Some of the optically generated minority carriers diffuse toward the illuminated surface to be collected by the scr, establishing a surface potential or surface
RECOMBINATION LIFETIME—OPTICAL MEASUREMENTS
VSPV
405
sr s1
F(l) pType
V′SPV
0
d
W
x
Fig. 7.11 Sample crosssection for SPV measurements. The optically transparent, electrically conducting contact to the left of the sample allows light to reach the sample and the voltage to be measured.
photovoltage voltage VSPV relative to the grounded back surface. VSPV is proportional to the excess minority carrier density n(W ) at the edge of the scr. The precise relationship between n(W ) and VSPV need not be known, but it must be a monotonic function. Light reaching the back surface produces an undesirable SPV signal that can be detected by its large amplitude, by a reversal in signal polarity over the SPV wavelength range, or by a signal decrease with increasing illumination at the longer wavelengths. The excess carrier density through the wafer for lowlevel injection is given by Eq. (A7.4). In principle, it is possible to extract the diffusion length Ln from that expression for arbitrary W , d, and α. In practice, several constraints are imposed on the system to simplify data extraction. The undepleted wafer should be much thicker than the diffusion length and the scr width should be small compared to Ln . The absorption coefficient should be sufficiently low for αW ≪ 1, but sufficiently high for α(d − W ) ≫ 1. The light diameter should be large compared to the sample thickness, allowing a onedimensional analysis and lowlevel injection should prevail. The assumptions d − W ≥ 4Ln ; W ≪ Ln ; αW ≪ 1; α(d − W ) ≫ 1; n ≪ po
(7.53)
allow Eq. (A7.4) to be reduced to n(W ) ≈
αLn (1 − R) (s1 + Dn /Ln ) (1 + αLn )
The excess carrier density at x = W is related to the surface photovoltage by kT qVSPV qVSPV for VSPV ≪ − 1 ≈ npo n(W ) = npo exp kT kT q
(7.54)
(7.55)
giving VSPV =
(kT /q)(1 − R)Ln npo (s1 + Dn /Ln )(Ln + 1/α)
(7.56)
VSPV is proportional to n for VSPV < 0.5kT /q. Typical surface photovoltages are in the low millivolt range, ensuring a linear relationship. s1 is the surface recombination velocity at x = W , not at the surface, where sr is the surface recombination velocity, as illustrated in Fig. 7.11.
406
CARRIER LIFETIMES
During SPV measurements, Dn and Ln are assumed to be constant. Furthermore over a restricted wavelength range the reflectivity R can also be considered constant. The surface recombination velocity s1 is usually unknown. However, if n(W ) is held constant during the measurement, the surface potential is also constant, and s1 can be considered reasonably constant. This leaves α and as the only variables. There are two SPV implementations: (1) constant surface photovoltage and (2) constant photon flux density. In method (1), VSPV = constant implies n(W ) is constant. A series of different wavelengths is selected during the measurement with each wavelength providing a different α. The photon flux density is adjusted for each wavelength to hold VSPV constant, allowing Eq. (7.56) to be written as =
npo (s1 + Dn /Ln )(Ln + 1/α) 1 VSPV = C1 Ln + (kT /q)(1 − R)Ln α
(7.57)
where C1 is a constant. Then is plotted against 1/α for constant VSPV . The result is a line whose extrapolated intercept on the negative 1/α axis ( = 0) is the minority carrier diffusion length Ln , shown in Fig. 7.12(a). The slope of such a plot is C1 which contains the surface
8 × 109
F (Photons/cm2•s)
VSPV = 10 mV, npo = 105 cm−3 6 × 109
s1 = 1000 cm/s, Dn = 30 cm2/s R = 0.3
4 × 109 2 × 109
Ln
0 −0.005
0
0.005 1/a (cm) (a)
0.01
0.015
150
1/VSPV (V−1)
F = 5 × 109 ph/cm2•s, npo = 105 cm−3 s1 = 1000 cm/s, Dn = 30 cm2/s 100
R = 0.3
50 Ln 0 −0.005
Fig. 7.12
0
0.005 1/a (cm) (b)
0.01
0.015
(a) Constant voltage, (b) constant photon flux density SPV plots for Si samples.
RECOMBINATION LIFETIME—OPTICAL MEASUREMENTS
407
recombination velocity s1 . While it is difficult to extract s1 from all the other parameters contained in C1 , it is possible to observe changes in s1 by comparing SPV plots before and after a process that changes surface recombination. For the constant photon flux density implementation, we write Eq. (7.56) as 1 VSPV
=
npo (s1 + Dn /Ln )(Ln + 1/α) 1 = C2 Ln + (kT /q)(1 − R)Ln α
(7.58)
where C2 is a constant. A plot of 1/VSPV versus 1/α gives Ln as illustrated in Fig. 7.12(b). VSPV changes during the measurement, hence surface recombination may vary during the measurement. The versus 1/α plot is a straight line for wellbehaved samples. A detailed theoretical study has shown the constant surface photovoltage method to give correct results even considering recombination in the spacecharge region.50 A detailed theoretical and experimental comparison of the PCD and SPV methods has shown the lifetimes determined by these techniques to be identical, provided one considers effects such as surface recombination, sample thickness, and so on.51
Exercise 7.1 Problem: How can iron in Si be detected with lifetime/diffusion length measurements? Solution: Since τSRH ∼ 1/NT , it should be possible to determine NT by measuring τSRH . 1/2 Further, since Ln ∼ τSRH , one should be able to determine NT from minority carrier diffusion length measurements also. Some impurities in Si have unique characteristics, e.g., iron forms pairs with boron in ptype Si. For a Fecontaminated, Bdoped Si wafer at room temperature, the iron forms FeB pairs. Upon heating at 200◦ C for a few minutes or illuminating the device (>0.1 W/cm2 light intensity), the FeB pairs dissociate into interstitial iron (F ei ) and substitutional B. The recombination properties of F ei differ from those of FeB, as shown by the effective diffusion lengths in Fig. E7.1(a). By measuring the diffusion length or lifetime before (Ln,i , τeff ,i ) and after (Ln,f , τeff ,f ) FeB pair dissociation, NFe is 1 1 1 1 16 − [cm−3 ] − 2 =C NFe = 1.06 × 10 τeff ,f τeff ,i L2n, f Ln,i with diffusion lengths in µm and lifetimes in µs. The diffusion lengths as a function of Fe density for a range of NFe are shown in Fig. E7.1(b). The prefactor, usually assumed as 1.06 × 1016 µm2 /cm3 , varies from 2.5 × 1016 µm2 /cm3 at NB = 1013 cm−3 to 7.5 × 1015 µm2 /cm3 at NB = 1017 cm−3 (D. H. Macdonald, L. J. Geerligs, and A. Azzizi, “Iron Detection in Crystalline Silicon by Carrier Lifetime Measurements for Arbitrary Injection and Doping,” J. Appl. Phys. 95, 1021–1028, Feb. 2004). The measurement has some restrictions. The diffusion lengths must be measured under lowinjection conditions. The most reliable technique for this is SPV, since it operates in true low injection. PCD and QSSPC suffer from reduced sensitivity at lowinjection and are also affected by minority carrier trapping at low injection causing a majority carrier excess, which distorts the photoconductance that is due to minority and majority carriers. Voltagebased techniques such as SPV are not affected by trapping because
408
CARRIER LIFETIMES
1.5
Normalized F
NFe = 1.1 × 1013 cm−3 1
0.5 Lni 0 −100
Lnf
−50
0
50 1/a (µm)
100
150
(a)
Ln,eff (cm)
100
10−1 FeB
Fei 10−2
sr = 100 cm/s 10−3 9 10
1010
1011 1012 NFe (cm−3)
1013
1014
(b)
Fig. E7.1 (a) Surface photovoltage plot for ironcontaminated Si sample, (b) effective minority carrier diffusion length versus iron density showing the “before” and “after” F eB pair breaking data.
they detect only minority carriers. As a result of these considerations, the widely used photoconductancebased lifetime techniques generally operate at mid to high injection levels. However, even for lowinjection SPV measurements, if the doping density is outside the 1–3 × 1015 cm−3 range, the prefactor is not constant, due to the properties of F ei and FeB: the energy level of the FeB center is relatively shallow, and its impact on the lowinjection lifetime depends on the doping density. On the other hand F ei , being a deep center, yields a doping densityindependent lowinjection lifetime. Since the prefactor C is determined by the difference of the inverse lifetimes, it also varies with the doping density. The factor C varies sensitively with injection level from C = 3 × 1013 µs/cm3 to −3 × 1013 µs/cm3 . It becomes negative for n > 2 × 1014 cm−3 (see McDonald et al. above), i.e., the lifetime decreases after dissociation for low injection but increases for high injection! The FeB pairing time constant, after dissociation, is given by 4.3 × 105 T 0.68 exp τpairing = NA kT
RECOMBINATION LIFETIME—OPTICAL MEASUREMENTS
409
A good discussion can be found in G. Zoth and W. Bergholz, “A Fast, PreparationFree Method to Detect Iron in Silicon,” J. Appl. Phys. 67, 6764–6771, June 1990 and Macdonald et al., above. The references for the experimental data are: O.J. Antilla and M.V. Tilli, “Metal Contamination Removal on Silicon Wafers Using Dilute Acidic Solutions,” J. Electrochem. Soc. 139, 1751–1756, June 1992; Y. Kitagawara, T. Yoshida, T. Hamaguchi, and T. Takenaka, “Evaluation of OxygenRelated Carrier Recombination Centers in HighPurity CzochralskiGrown Si Crystals by the Bulk Lifetime Measurements,” J. Electrochem. Soc. 142, 3505–3509, Oct. 1995; M. Miyazaki, S. Miyazaki, T. Kitamura, T. Aoki, Y. Nakashima, M. Hourai, and T. Shigematsu, “Influence of Fe Contamination in CzochralskiGrown Silicon Single Crystals on LSIYield Related Crystal Quality Characteristics,” Japan. J. Appl. Phys. 34, 409–413, Feb. 1995; A.L.P. Rotondaro, T.Q. Hurd, A. Kaniava, J. Vanhellemont, E. Simoen, M.M. Heyns, and C. Claeys, “Impact of Cu and Fe Contamination on the Minority Carrier Lifetime of Silicon Substrates,” J. Electrochem. Soc. 143, 3014–3019, Sept. 1996. Chromium in silicon forms CrB pairs. When these pairs dissociate, the lifetime increases (K. Mishra, “Identification of Cr in ptype Silicon Using the Minority Carrier Lifetime Measurement by the Surface Photovoltage Method,” Appl. Phys. Lett. 68, 3281–3283, June 1996).
The condition W ≪ Ln is generally satisfied for singlecrystal Si samples, but that may not be true for other semiconductors. For example, the diffusion length in GaAs is often only a few microns. In amorphous Si it is even shorter. In such a situation the intercept is given by52 (W/Ln )2 1 = −Ln 1 + (7.59) α 2(1 + W/Ln ) Equation (7.59) reduces to (7.57) for W ≪ Ln . For W ≫ Ln the 1/α intercept is −W/2, independent of the diffusion length. The scr width can be reduced with steadystate light on the device when W ≫ Ln . In Eqs. (7.57) and (7.58) the photon flux density is plotted against the inverse absorption coefficient. It is not the absorption coefficient, however, but the wavelength that is varied during the measurement. An accurate wavelengthabsorption coefficient relationship is therefore very important for SPV measurements. Any error in that relationship leads to incorrect diffusion lengths. Various equations have been proposed. A fit to recent α − λ data for silicon is given by53 2 83.15 − 74.87 [cm−1 ] (7.60) α= λ with the wavelength λ in µm, valid for the 0.7 to 1.1 µm wavelength range typically used for Si. An expression that gives reasonable agreement with experimental GaAs absorption data54 is 2 286.5 − 237.13 [cm−1 ] (7.61) α= λ for the 0.75 to 0.87 µm wavelength range. For InP55 2 252.1 − 163.2 [cm−1 ] α= λ is a reasonable approximation for the 0.8 to 0.9 µm wavelength range.
(7.62)
410
CARRIER LIFETIMES
The reflectance R in Eq. (7.54) is usually considered to be constant. However, there is a weak wavelength dependence for Si, given by56 R = 0.3214 +
0.03565 0.03149 − λ λ2
(7.63)
for 0.7 < λ < 1.05 µm with λ in µm. SPV measurements have become very common in the semiconductor industry, largely due to the availability of commercial equipment. Diffusion lengths are routinely measured, because they are a good measure of process cleanliness. Monitoring of furnace tube cleanliness, detection of metallic contamination of incoming chemicals, and control of photoresist ashing are but a few examples for SPV applications.57 A crucial component of SPV is the surface treatment to create the surface scr. The ASTM method recommends boiling nSi in water for one hour.56 For pSi a oneminute etch in 20 ml concentrated HF + 80 ml H2 O is recommended. This method works best when care is taken in earlier preparation steps not to produce a stain film by withdrawing the sample from an HFcontaining etch directly into air. Otherwise, a low or unstable SPV is likely to result. The stain can be avoided by quenching the HFcontaining etch thoroughly with deionized water before withdrawing the sample into air. Another surface treatment for Si samples is a standard Si clean/etch,58 removing any residual SiO2 in buffered HF and treating nSi in an aqueous solution of KMnO4 . For pSi, the KMnO4 step is omitted. Schottky and pn junction diodes are also suitable for SPV measurements. In both cases, one makes contact to the device directly, without the need for capacitive contacts, yielding a higher surface photovoltage. The metal must be partially transparent for Schottky diodes.59 It may be necessary to observe certain precautions.60 Aluminum, 10–20 nm thick, is sufficiently transparent to be suitable. It also possible to use liquid contacts.61 The size of the optical beam has an influence on the measured diffusion length. For a beam diameter less than about 30Ln , the diffusion length is reported to be larger than the true value.62 As with all diffusion length measuring techniques, the true diffusion length can only be determined for samples thicker than 4Ln . Effective diffusion lengths are determined for thinner samples,63 but for samples thinner than Ln , it is difficult to extract the correct diffusion length.64 Further complications arise if the sample consists of regions of different diffusion lengths as found in Si wafers that have undergone a denuding and oxygen precipitation cycle. The extraction of the diffusion length then becomes quite complicated.65 The SPV technique has also been implemented with ac photosignals.66 A photon beam is scanned across the sample and the resulting ac photovoltage is detected with a capacitive probe and displayed on a TV monitor.
Exercise 7.2 Problem: Is it possible to determine Ln when d < Ln ? Solution: The term was calculated and plotted versus 1/α as a function of Ln using Eq. (A7.4) for Si. Fig. E7.2(a) shows a good linear fit to the calculated data for d ≈ 4Ln as expected, but beyond that there is poor linearity and the simple analysis of Eq. (7.57) does not work. For x = 0, d ≪ Ln , and αd ≫ 1 Eq. (A7.4) becomes n(0) =
(1 − R) d − 1/α (1 − R)ατ sr2 αd + αD − Dd/L2n − sr2 ≈ (α 2 L2n − 1) sr1 sr2 d/D + Dd/L2n + sr1 + sr2 (1 − α −2 L−2 n ) sr1 d + D
RECOMBINATION LIFETIME—OPTICAL MEASUREMENTS
411
F (photons/s•cm2)
4 × 109 Ln = 100 µm
3 × 109
150 200 300 500
2 × 109
1 × 109
750; 1000
0 −400
−200
0 1/a (µm)
200
400
(a)
1/F (photons/s•cm2)−1
2 × 109 Ln = 1000 µm
d = 500 µm
500 1 × 109 200
0
0
250
500 1/a (µm) (b)
750
1000
Fig. E7.2 Constant voltage SPV plots (a) exact equation, (b) approximate equation. sr1 = 104 cm/s, sr2 = 104 cm/s, Dn = 30 cm2 /s, VSPV = 10 mV, R = 0.3, npo = 105 cm−3 , d = 500 µm.
where the approximation holds for high sr2 . A plot of 1/ versus 1/α, according to (1 − R) d − 1/α 1 ≈ −2 −2 n(0)(1 − α Ln ) sr1 d + D has a 1/α intercept that is neither the sample thickness d nor Ln . It is obvious from these figures that the diffusion length cannot be reliably determined when Ln exceeds the sample thickness.
7.4.6
SteadyState ShortCircuit Current (SSSCC)
The steadystate shortcircuit current method is related to the SPV method. The sample must contain a collecting junction such as a pn junction or Schottky diode, and the shortcircuit current is measured as a function of wavelength. Using the same assumptions as
412
CARRIER LIFETIMES
VF
VB
IF
Jsc
IB Pt Electrode Wafer
Laser F(l) 1−2% HF pType
Window
d
n+ (a)
1−2% HF
(b)
Fig. 7.13 Measurement schematic for (a) the shortcircuit current diffusion length measurement method and (b) for the ELYMAT double surface method.
those of the SPV method [Eq. (7.53)], the shortcircuit current density of the n+ p junction of Fig. 7.13(a) is, according to Eq. (A 7.9), given by Lp Ln + (7.64) Jsc ≈ q(1 − R) Ln + 1/α Lp + 1/α The diffusion length is generally low for heavily doped layers, allowing the second term to be neglected for an n+ p junction, and the shortcircuit current density becomes Ln (7.65) Jsc ≈ q(1 − R) Ln + 1/α Neglecting ehp generation in the n+ layer and in the spacecharge region is permissible if these regions are narrow and if α is not too high. Equation (7.65) has been used in two ways to extract the diffusion length. In one technique the current is held constant by adjusting the photon flux density as the wavelength is changed.67 Equation (7.65) then becomes = C1 (Ln + 1/α)
(7.66)
where C1 = Jsc /q(1 − R)Ln . Ln is the intercept on the negative 1/α axis when is plotted against 1/α. In a second technique, Eq. (7.65) is written as68 1 = (X − 1)Ln α
(7.67)
where X = q(1 − R)/Jsc . Here 1/α is plotted against (X − 1) and the diffusion length is given by the slope of this plot. A check on the data is provided by the extrapolated lines passing through the origin. Both methods neglect carrier collection from the n+ region and the scr. The shortcircuit current methods are in principle similar to SPV, but they require a junction to collect the minority carriers. In practice, it is easier to measure a current than an opencircuit voltage. However, junction formation may alter the diffusion length. Two implementations not requiring permanent junctions make use of mercury contacts or liquid semiconductor contacts. In the mercury contact method, two Hg probes are
RECOMBINATION LIFETIME—OPTICAL MEASUREMENTS
413
pressed against one side of the sample and modulated light is incident on the other side. From an analysis of the frequencydependent photocurrent, one can extract the lifetime and diffusion coefficient.69 A different implementation, the electrolytical metal tracer (ELYMAT), shown schematically in Fig. 7.13(b), uses electrolytesemiconductor junctions at the front and at the back surface to map the photo response which is related to the diffusion length.70 The wafer is immersed in an electrolyte (normally, but not necessarily, 1%–2% HF in H2 O). The electrolyte serves the dual function of photocurrent collection as well as wafer surface passivation. The front and back induced photocurrents IF and IB are measured in response to laser beam excitation of the sample. For light with short penetration depth, moderate wafer diffusion lengths, and negligible back surface recombination, the front current IF is measured. For penetrating light and low front surface recombination, the back current IB is measured. The currents are given by70 IB ≈
Imax (1 + srf /Dn α) Imax ≈ cosh(d/Ln ) + (srf Ln /Dn ) sinh(d/Ln ) cosh(d/Ln )
IF ≈ Imax ; Imax ≈ qA(1 − R)(1 − exp(−αd))
(7.68a) (7.68b)
where A is the area, srf the surface recombination velocity at the front surface, and the photon flux density. The approximation in the first equation holds for low srf , as observed in an HF solution. Measuring IF and IB allows Ln to be determined. Using laser excitation with two different wavelengths and voltage bias, allows the surface recombination velocity and the minority carrier diffusion length as well as depthdependent diffusion length to be determined. Scanning the laser produces diffusion length maps rapidly with no mechanical motion. Although submersing the sample in a dilute HF solution ensures low surface recombination, at times it is useful to control surface effects further, e.g., using an oxidized Si wafer with a solution that does not etch SiO2 , e.g., CH3 COOH. Then biasing the solution with respect to the sample, the Si surface can be accumulated, depleted or inverted. Such “electrostatic passivation” further reduces surface recombination.71 7.4.7
Free Carrier Absorption
The free carrier absorption lifetime method is a noncontacting technique, relying on optical ehp generation and optical detection using two different wavelengths. As illustrated in Fig. 7.14, a pump beam using photons with energy hν > EG creates ehps. The readout is based on the dependence of the free carrier absorption of photons with hν < EG on the density of free carriers. The probe beam transmitted photon flux density t is given by t =
(1 − R)2 i exp(−αf c d) 1 − R 2 exp(−2αf c d)
(7.69)
where αf c is the free carrier absorption coefficient, d the sample thickness, and R the reflectivity. For ntype semiconductors the absorption coefficient is72 αf c = Kn λ2 n
(7.70)
where Kn is a materials constant and λ the wavelength of the probe beam. For nSi, Kn ≈ 10−18 cm2 /µm2 , and for pSi, Kp ≈ (2–2.7) × 10−18 cm2 /µm2 .72 – 73 A small correction to Kn in Eq. (7.70) has been suggested.74
414
CARRIER LIFETIMES
IR Probe Beam
Scan Directions
Hot Plate IR Laser
Pump Laser
Infrared Radiation
Detector
Pulsed Pump Laser
Sample (a)
(b)
100
teff[µs]
90
>160 160 150 140 130 120 110 100
80
Y [mm]
70 60 50
90 80 70 60 50 40 30 20
40 30 20 10
EG creates ehps in the sample. By taking the difference of the IR radiation through the sample with and without the laser, one measures the free carrier absorption due to the excess carriers. Taking twodimensional images of the IR radiation over the entire wafer, allows for rapid measurements. The system is calibrated with a set of Si wafers of varying doping densities. The transmissivity of these wafers successively placed between the camera and the black body is measured. The signal differences are then due to the differences in freecarrier absorption of the samples. One needs to apply a correction to account for the fact that in the calibration procedure of ptype wafers only the IR absorption of holes is measured while in an actual measurement lasergenerated electronhole pair generation must be considered. Knowing the laser generation rate G′ = (1 − R) (cm−2 s−1 ) and the sample thickness d, the effective lifetime is dn (7.74) τeff = G′ A twodimensional lifetime map obtained in 50 s with this technique is shown in Fig. 7.14(c). No scanning is required, since both black body and excitation laser are broad area sources, covering the entire sample. The black body emits over a wide wavelength range with a peak wavelength at λpeak ≈
3000 µm T
(7.75)
A hot plate at T = 350 K, has its peak wavelength at λpeak ≈ 8.6 µm—a suitable wavelength for free carrier absorption measurements. Just as carriers absorb IR radiation, they also emit IR radiation. According to Kirchhoff’s law they emit the same power as they absorb to remain at a given temperature. Hence, the sample itself will emit IR radiation
416
CARRIER LIFETIMES
and can be used to determine the lifetime. The sample is still excited with a laser and the difference signal is acquired as in the transmission system. Both emission and absorption have been used for lifetime measurements.80 7.4.8
Electron Beam Induced Current (EBIC)
Electron beam induced current is used to measure minority carrier diffusion length, minority carrier lifetime, and defect distribution. In contrast to photons that typically create one ehp pair upon absorption, an absorbed electron of energy E creates γ Ebs E 1− (7.76) Nehp = Eehp E electronhole pairs.81 Ebs is the mean energy of the backscattered electrons, γ the backscattering coefficient and Eehp the average energy required to create one ehp (Eehp ≈ 3.2EG ; for Si Eehp = 3.64 ± 0.03 eV).82 The backscattering term γ Ebs /E is approximately equal to 0.1 for Si and 0.2–0.25 for GaAs over the 2 to 60 keV electron energy range. The electron penetration depth or range Re is given by83 Re =
2.41 × 10−11 1.75 E ρ
[cm]
(7.77)
where ρ is the semiconductor density (g/cm3 ) and E the incident energy (eV). For Si and GaAs, Re (Si) = 1.04 × 10−11 E 1.75 cm and Re (GaAs) = 4.53 × 10−12 E 1.75 cm. It is instructive to calculate the ehp density generated by an electron beam of energy E and beam current Ib . The generation volume tends to be pear shaped, as shown in Chapter 11, for atomic numbers Z < 15. For 15 < Z < 40 it approaches a sphere, and for Z > 40 it becomes hemispherical. We approximate it as a sphere of volume (4/3)π(Re /2)3 , for simplicity. Combining Eqs. (7.76) and (7.77) gives the generation rate G=
Nehp Ib 8.5 × 1050 ρ 3 Ib = 3 (4/3)πq(Re /2) Eehp E 4.25
[cm−3 s−1 ]
(7.78)
neglecting the backscattered term in Eq. (7.76). For Si with a beam current of 10−10 A, Eehp = 3.64 eV and E = 104 eV the generation rate is G = 3 × 1024 ehp/cm3 · s. The interaction of an electron beam with the semiconductor sample can take place for a variety of geometries. One of these is shown in Fig. 7.15(a). The electron beam induced current IEBIC collected by the junction changes by moving the beam in the xdirection. Changes in the zdirection are produced by changing the beam energy. The ebeam creates ehps at a distance d from the edge of the scr. Some of the minority carriers diffuse to the junction to be collected, and IEBIC decreases with increasing d due to bulk and surface recombination. IEBIC can be expressed as84 d qG′ Re Lnn −n (7.79) = Cd exp − IEBIC = (2π)1/2 d n Ln where G′ = Ib Nehp /q, provided sr ≫ Dn /Ln , Ln ≪ d, Re ≪ d, Re Ln ≪ d 2 , and lowlevel injection prevails. The exponent n depends on surface recombination. For sr → 0, n = 1/2 and for sr → ∞ n = 3/2. A plot of ln(IEBIC d n ) versus d should give a straight
RECOMBINATION LIFETIME—ELECTRICAL MEASUREMENTS
Ib
Ib
x z
d
d
sr
W
Fig. 7.15
417
IEBIC
IEBIC
z
pType
pType
(a)
(b)
(a) Conventional EBIC implementation, (b) depth modulation by electron beam energy.
line of slope −1/Ln . Since sr is generally not known, n is also unknown. One method to determine n is to plot ln(IEBIC d n ) versus d and vary n until a straight line results.85 For the configuration in Fig. 7.15(b), IEBIC is86 2sr F z − (7.80) IEBIC = I1 exp − Ln π where I1 is a constant and F depends on sr and on the ehp generation point. The second term in Eq. (7.80) vanishes for d = Ln and Ln is found by recording Iph versus z.87 Surface recombination plays an important role in EBIC measurements.88 Instead of determining the diffusion length from the steadystate photocurrent as a function of lateral motion or beam penetration, one can use a stationary pulsed beam and extract the minority carrier lifetime from the transient analysis. An approximate expression for IEBIC for high sr , is88 τ 2 τn t d n 1− (7.81) − IEBIC (t) = K1 exp t Ln 4t τn valid for d ≫ Ln for Fig. 7.15(b). Theory predicts that IEBIC does not decay immediately after the injection has ceased. Instead, there is a delay that is more pronounced the further the beam is from the junction. For optical excitation, the technique is known as optical beam induced current (OBIC), with considerations very similar to EBIC except for a different generation expression.89 – 90 Most EBIC measurements are made as illustrated in Fig. 7.15 and the method is fairly straightforward for long diffusion lengths. For short diffusion length measurements, the sample can be beveled to enhance the depth.91 Surface recombination effects are reduced if the beam penetration is increased. This can be directly tested by plotting ln(IEBIC ) versus d for various beam energies. The plot should approach a straight line for higher energies. 7.5 7.5.1
RECOMBINATION LIFETIME—ELECTRICAL MEASUREMENTS Diode CurrentVoltage
The pn junction diode forward current depends on recombination of excess carriers and is the sum of spacecharge region, quasineutral region (qnr), and surface recombination
418
CARRIER LIFETIMES
10−2 qnr
Current (A)
10−4 10−6 10−8
scr
10−10
Io,scr Io,qnr
−12
10
10−14
Fig. 7.16
0
0.1
0.2 0.4 Voltage (V)
0.5
0.6
pn junction I –V curve showing spacecharge and quasi neutral region currents.
currents. In reverse bias, it is generation in the various regions that is measured. In most analyses, surface recombination is neglected and the current density is qV qV − 1 + J0,qnr exp −1 J = J0,scr exp nkT kT qni W D D n p (7.82) ; J0,qnr = qn2i F + J0,scr = τscr NA Ln ND Lp where F is a correction factor that depends on the sample geometry, e.g., denuded zones on defective substrates, epitaxial layers on heavily or lightly doped substrates, silicononinsulator (SOI), etc. It is, in general, a complicated function of the active layer thickness, the diffusion lengths and doping densities in the layer and the substrates, and possible interface recombination velocity at the layersubstrate interface. Equation (7.82) is plotted in Fig. 7.16. Extrapolating the qnr line to V = 0 yields I0,qnr . For a p+ n junction NA ≫ ND and although τn in a heavilydoped region is much lower than τp in the lightlydoped substrate, it is often permissible to neglect the first term in the J0,qnr term because NA is very high, giving J0,qnr ≈ qn2i F
Dp ND Lp
(7.83)
Knowing ni , F , Dp , and ND allows Lp to be determined. Consider the device crosssections in Fig. 7.17. Neglecting electron injection into the p+ region for simplicity, the current in the forwardbiased p+ n junction in Fig. 7.17(a) with d < Ln depends on hole recombination in the scr (1), in the qnr (2), and at the surface (3). The correction factor is given by65 F =
(sr Lp /Dp ) cosh(d/Lp ) + sinh(d/Lp ) cosh(d/Lp ) + (sr Lp /Dp ) sinh(d/Lp )
(7.84)
Figure 7.17(b) shows an nsubstrate consisting of a denuded zone (1) of width d (Lp1 , NA ) on a precipitated substrate (2) (Lp2 , NA ). An epitaxial layer (1) of thickness d (Lp1 , NA1 ) on a substrate (2) (Lp2 , NA2 ) is shown in (c) and (d) shows an SOI wafer. Correction factors have been derived for these cases.92 For the epitaxial device in Fig. 7.17(c) F ≈
(1 + NA2 /NA1 ) exp(Dp /Lp ) + (1 − NA2 /NA1 ) exp(−Dp /Lp ) (1 + NA2 /NA1 ) exp(Dp /Lp ) − (1 − NA2 /NA1 ) exp(−Dp /Lp )
(7.85)
RECOMBINATION LIFETIME—ELECTRICAL MEASUREMENTS
p+ (1)
n Lp
sr
V
(3)
(2)
V
419
(1) Lp1 NA
(1) s Lp1 r NA1
V
d
d
(a)
(c) (2) Lp2 NA
(2) Lp2 NA2
(1) (2) s Lp, r NA
V
d
d
(b)
(d)
(3)
Fig. 7.17 pn junction cross sections (a) recombination mechanisms in the nsubstrate for d < Lp , (b) denuded zone on precipitated substrate, (c) epitaxial layer on substrate, and (d) SOI wafer.
Although correction factors can, in principle, be applied, it is fraught with difficulties, because the lifetimes in the epi layer and the substrate and the interface recombination velocity at the episubstrate interface are rarely known. Some of the pitfalls in the interpretation of such measurements are given in ref. 93. A recent study concluded that the most effective techniques to characterize epitaxial layers are generation lifetime techniques.94 Instead of extrapolating the forwardbiased currentvoltage characteristics, one can also use the reversebias currentvoltage curve.95 Under reverse bias, where V < 0, Eq. (7.82) becomes qni W Dp Dp qni W Dn 2 ≈− − qni F + − qn2i F (7.86) Jr = − τg NA Ln ND Lp τg ND Lp Plotting Jr versus W gives a curve with slope related to the generation lifetime τg and intercept giving J0,qnr , illustrated in Fig. 7.18. The scr width is determined from reversebiased capacitancevoltage data, but the true capacitance must be measured,96 especially for small area diodes where perimeter, corner, and parasitic capacitances are important. 6
Reverse Current (pA)
5
Cmeas
4 3
Ccorr
2 Io,qnr
1
200 µm × 200 µm 0
0
1
2 3 SCR Width (µm)
4
5
Fig. 7.18 Reverse leakage current versus scr width for measured and corrected capacitance. Adapted from ref. 96.
420
CARRIER LIFETIMES
The actual diode leakage current consists of areal, peripheral, corner, and parasitic currents according to97 Ir = AJA + P JP + NC JC + Ipar where A is the diode area, P the diode perimeter (JP in units of A/cm), NC the number of corners (JC in units of A/corner) and Ipar is a parasitic current. 7.5.2
Reverse Recovery (RR)
The diode reverserecovery method was one of the first electrical lifetime characterization techniques.98 – 100 A measurement schematic and currenttime and voltagetime responses are shown in Fig. 7.19. In Fig. 7.19(b) the current is suddenly switched from forward to reverse current by changing switch position S, whereas in 7.19(c) the current is gradually changed, typical of power devices in which currents cannot be switched very abruptly. For a description of the method, let us consider Figs. 7.19(a) and (b). A forward current If flows through the diode for t < 0 and the diode voltage is Vf . Excess carriers are injected into the quasineutral regions, leading to low device resistance. At t = 0 the current is switched from If to Ir , with Ir ≈ (Vr − Vf )/R. The small diode resistance is neglected because the diode remains forward biased during the initial time of Ir flow. Currents can be switched very quickly in minority carrier devices because only a change
t=0
R
S If
Vr Id (a)
Id
Id
If
If t1 t2
t I0
t3
t
I0
ts
Ir
Ir Vd
Vd
∆Vd
Vf
Vf t
0
Vr
t
0
Vr (b)
(c)
Fig. 7.19 Reverse recovery circuit schematic, (b) current and voltage waveforms for abruptly switched current, and (c) current and voltage waveforms for ramped currents.
RECOMBINATION LIFETIME—ELECTRICAL MEASUREMENTS
421
in the slope of the minority carrier density gradient at the edge of the scr is required. The diode voltage, in contrast, is proportional to the log(excess carrier density) at the scr edge. The voltage hardly changes during this period and the diode remains forward biased although the current has reversed direction. The voltage step Vd is due to the ohmic voltage drop in the device.101 The excess carrier density decreases during the reverse current phase as some carriers are swept out of the device by the reverse current and some carriers recombine. The excess minority carrier densities at the edges of the scr are approximately zero at t = ts , and the diode becomes zero biased. For t > ts , the voltage approaches the reversebias voltage Vr and the current approaches the leakage current I0 . The Id − t curve is conveniently divided into the constantcurrent storage phase, 0 ≤ t ≤ ts , and the recovery phase, t > ts . The storage time ts is related to the lifetime by99 1 ts = (7.87) erf τr 1 + Ir /If with “erf”, the error function, defined and approximated by x 0.095879 0.74785 0.34802 2 −z2 − e dz ≈ 1 − + erf (x) = √ 1 + 0.4704x (1 + 0.4704x)2 (1 + 0.4704x)3 π 0 × exp(−x 2 )
(7.88)
An approximate charge storage analysis that considers the charge Qs remaining at t = ts gives102
Qs If − ln 1 + (7.89) ts = τr ln 1 + Ir If τ r Qs /Ir τr can be considered a constant for many cases. A plot of ts versus ln(1 + If /Ir ) is shown in Fig. 7.20. The lifetime is found from the slope and the intercept is (1 + Qs /Ir τr ). The slope is constant only if the second term in Eq. (7.89) is constant. Various approximations have been derived for QS , and it is found to be approximately constant provided Ir ≪ If .103 The effect of recombination in the heavily doped emitter can be virtually eliminated by keeping Ir ≪ If .104 The plot 800
ts (ns)
600
400
200
0
tr = 180 ns 1
10 1 + If /Ir
100
Fig. 7.20 Storage time versus (1 + If /Ir ). Reprinted after Kuno102 by permission of IEEE ( 1964, IEEE).
422
CARRIER LIFETIMES
of Fig. 7.20 becomes highly curved if these conditions are not met and a unique lifetime can no longer be extracted. For Fig. 7.19(c) the lifetime is related to t1 , t2 , and t3 by105 τr ≈ (t2 − t1 )(t3 − t1 ) (7.90)
where t3 is defined as the time for Id = 0.1Ir . The junction displacement current Ij = Cj dVj /dt is neglected in all of these expressions because it constitutes only a small fraction of the total current.100 What is τr in Eqs. (7.87) and (7.90)? To first order it would seem to be the base lifetime in pn junctions. For shortbase diodes, it is an effective lifetime representing both bulk and surface recombination.106 A problem in forwardbiased pn junctions is the existence of excess carriers in both quasineutral regions and in the scr. The emitter is generally much more heavily doped than the base and the emitter lifetime is much lower than the base lifetime. Hence, one would expect emitter recombination to have a significant influence on the RR transient. This is particularly troublesome for high injection conditions, leading to appreciably reduced lifetimes.107 – 108 However, the emitter can alter the measured lifetime from its true base value even at low and moderate injection levels. 7.5.3
OpenCircuit Voltage Decay (OCVD)
The opencircuit voltage decay method measurement principle is shown in Fig. 7.21(a).109 – 110 The diode is forward biased and at t = 0 switch S is opened and the voltage, decaying due to recombination of excess carriers, is detected as in Fig. 7.21(b). The voltage step Vd = If rs is due to the ohmic voltage drop in the diode when the current ceases and can be used to determine the device series resistance as discussed in Chapter 4.101 OCVD is similar to the optically excited, opencircuit voltage decay method in Section 7.4.3. In contrast to RR, in the OCVD method the excess carriers all recombine; none are swept out of the device by a reverse current since the current is zero. The excess minority carrier density np in the quasineutral region at the edge of the scr in a psubstrate, is related to the timevarying junction voltage Vj (t) by qVj (t) −1 (7.91) np (t) = npo exp kT where npo is the equilibrium minority carrier density. The junction voltage is np (t) kT ln Vj (t) = +1 q npo
(7.92)
A measure of the voltage time dependence is a measure of the excess carrier time dependence. t =0
R ∆Vd
Vd
S
+
Vo
Vd −
Junction Capacitance
Shunt Resistance
Ideal t
0 (a)
Fig. 7.21
(b)
Open circuit voltage decay (a) circuit schematic and (b) voltage waveform.
RECOMBINATION LIFETIME—ELECTRICAL MEASUREMENTS
423
The diode voltage is Vd = Vj + Vb , where Vb is the base voltage, neglecting the voltage across the emitter. How can there be a base voltage when there is no current flow during the decay? The base or Dember voltage is the result of unequal electron and hole mobilities and is given by111 (b + 1)np (t) kT b − 1 ln 1 + Vb (t) = (7.93) q b+1 npo + bppo with b = µn /µp . The Dember voltage is negligible for low injection levels, and we will not consider it further, but may not be negligible for high injection levels. We assume that Vd (t) ≈ Vj (t), given by Eq. (7.92), and will simply use V (t) for the timevarying device voltage. For d ≫ Ln and lowlevel injection110 kT t (7.94) ln erfc V (t) = V (0) + q τr where V (0) is the diode voltage before opening the switch and erfc(x) = 1 − erf (x) is the complementary error function. Equation (7.94), plotted in Fig. 7.22, obtains for V (t) ≫ kT /q. The curve has an initial rapid decay followed by a linear region with constant slope. The slope is (kT /q) exp(−t/τr ) kT /q dV (t) =− √ ≈− √ dt τr (1 − τr /2t) πtτr erfc 1/τr
(7.95)
where the approximation holds for t ≥ 4τr . Equation (7.95) can be further simplified by neglecting the second term in the bracket. For t ≥ 4τr the lifetime is determined from the slope according to kT /q (7.96) τr = − dV (t)/dt As Fig. 7.22 shows, the curve becomes linear for t > 4τr . A word of caution regarding Eq. (7.96). The assumption in the derivation leading to this equation is that recombination is dominated by quasineutral region recombination 0.6
V(t) (V)
0.5
0.4
0.3 V(0) = 0.55 V 0.2
0
2
4
6
8
10
t/tr
Fig. 7.22
Open circuit voltage decay waveform according to Eq. (7.94).
424
CARRIER LIFETIMES
with the simple exponential voltage dependence exp(qV /kT ). For scr recombination the dependence becomes exp(qV /nkT ), where the diode ideality factor n lies typically between 1 and 2. Equation (7.96) should contain n as a prefactor. Of course, as the diode voltage drops from V (0) ≈ 0.7 V or so to zero, n is likely to vary from 1 to a value closer to 2, and since one usually does not know what n is, it is generally taken as unity. Due to the low emitter lifetime, excess emitter carriers recombine more rapidly than excess base carriers causing carriers from the base to be injected into the emitter during the voltage decay, and reducing the voltage decay time. Fortunately this effect becomes negligible for t ≥ 2.5τb , where τb is the base lifetime, and the V (t) − t curve becomes linear with slope (kT /qτb ) regardless of emitter recombination or bandgap narrowing.112 Under high level injection, the lifetime is given by113 τr = −
2kT /q dV (t)/dt
(7.97)
subject to the restrictions: the excess carrier density in the base is uniform and the base excess carrier density is higher than the base doping density. The 2 accounts for high injection effects. The high injection level V − t curve frequently exhibits two distinct slopes. Unusual V − t responses, shown in Fig. 7.21(b), are sometimes observed for nonnegligible diode capacitance or low junction shunt resistance. Capacitance tends to extend the V − t curve, giving the curve a smaller slope leading to too high lifetimes.114 Spacecharge region recombination and shunt resistance cause the V − t curve to drop faster than observed for quasineutral bulk recombination only. A variation of the OCVD method that has been found to be useful for devices exhibiting such decay curves is to switch an external resistor and capacitor into the measurement circuit and differentiate the curve to extract the lifetime.115 Another possible anomaly is a peak in the V − t curve near t = 0 due to emitter recombination.116 A variation of OCVD is the smallsignal OCVD method in which the diode is biased to a steadystate voltage, by illuminating the device and imposing a small electrical pulse on the “optical” bias.43, 117 With the pulse “on,” additional carriers are injected, and with it “off,” these additional carriers recombine. This method is used to measure τr under bias conditions and also to reduce capacitance and shunt resistance effects. A comparison of the RR and the OCVD techniques favored OCVD for its ease and accuracy.107 In OCVD the lifetime can be extracted from that part of the V − t curve where base recombination dominates, whereas in RR storage time measurements there is some averaging over a voltage range that includes at the lower current the scr recombination current. During OCVD the experimental considerations are relaxed since the carriers decay by recombination only.
7.5.4
Pulsed MOS Capacitor
The principle of the pulsed MOS capacitor (MOSC) recombination lifetime measurement technique is divided into two methods. In the first of these for an MOSC biased into strong inversion in Fig. 7.23(a) and point A in 7.23(d), the inversion charge density is Qn1 = (VG1 − VT )Cox
(7.98)
RECOMBINATION LIFETIME—ELECTRICAL MEASUREMENTS
VG1
VG2
425
VG1
∆Qn
Equilibrium pType
Recombination
(a)
Generation
(b)
(c)
C Cox
B
A
CA, CB CC
C VG1 VG
VG2
VG t
tp ∆VG (d)
Fig. 7.23 Pulsed MOS capacitor recombination lifetime measurement. The device behavior at various voltages is shown in (a), (b), and (c) and the C –VG and VG − t curves in (d).
A voltage pulse of amplitude −VG and pulse width tp superimposed on VG1 reduces the gate voltage during the pulse period to VG2 = VG1 − VG shown in Fig. 7.23(b) and by point B in 7.23(d). The inversion charge is Qn2 = (VG2 − VT )Cox < Qn1
(7.99)
The charge difference Qn = (Qn1 − Qn2 ) is injected into the substrate, as indicated in Fig. 7.21(b). What happens to Qn ? Minority carriers in an inversion layer do not recombine with majority carriers because they are separated by the electric field of the scr. However, those minority carriers injected into the substrate are surrounded by holes and can recombine. Let us now consider two extremes. First, for a wide pulse (tp > τr ) the injected minority carriers have sufficient time to recombine. When the gate voltage returns to VG1 only Qn2 is available, and the MOSC is driven into partial deep depletion, shown in Fig. 7.23(c) and by point C in 7.23(d). Thermal ehp generation subsequently returns the device to equilibrium, point A. Second, for a narrow pulse (tp ≪ τr ), the device goes through similar stages as in the first case except the injected minority carriers have insufficient time to recombine because the pulse width is less than the recombination lifetime and the capacitance sequence in Fig. 7.23(d) is CA → CB → CA . For intermediate pulse widths, the capacitance lies between CC and CA .
426
CARRIER LIFETIMES
The capacitance at the end of the injection pulse is a measure of how many minority carriers have recombined during the pulse period. For a simple exponential decay of the minority carriers118 t 1 1 =K Qn (t) = Qn (0) exp − − τr CA2 CC2
(7.100)
where K is a constant. To determine the lifetime, the pulse width is varied and the capacitance CC is measured for each pulse width and ln(1/CA 2 − 1/CC 2 ) is plotted against tp ; τr is obtained from the slope of this plot. A more detailed theory shows the exponential time decay of the carriers in Eq. (7.100) to be too simplistic because minority carriers recombine not only in the quasineutral substrate but also in the scr and at the surface.119 This pulsed MOSC recombination lifetime measurement method has not found wide acceptance because most capacitance meters are unable to pass the required narrow pulses undistorted. It is easier to modify the experimental arrangement by coupling the device to the capacitance meter through a pulse transformer at its input terminals.120 A variation of the pulsed MOSC technique, based on charge pumping, has been proposed for MOSFETs.121 When a MOSFET is pulsed from inversion into accumulation, most of the inversion charge leaves the channel through the source and the drain. However, a small fraction of the charge is unable to reach either source or drain and recombines with majority carriers. This fraction, proportional to the pulse frequency, is detected as a substrate current. As the frequency increases to the point where the time between successive pulses is on the order of τr , the substrate currentpulse frequency relationship becomes nonlinear, and τr can be extracted from the current. The second pulsed MOSC method is based on an entirely different principle  the measurement of the relaxation time of an MOSC when pulsed into deep depletion. We assume that prior to applying the depleting gate voltage, the device is in equilibrium and illustrate the technique in Fig. 7.24, where the MOSC capacitance is driven from A to B by a depleting voltage step. Thermal generation returns the device to equilibrium, shown by the path B to C, in Fig. 7.24(a). The return to equilibrium on the C − t diagram is typically as shown in Fig. 7.24(b). The recovery time tf is determined by the thermal ehp generation in the semiconductor and at the oxidesemiconductor interface. The thermal generation rates in Fig. 7.25 are (1) bulk scr generation characterized by the generation lifetime τg , (2) lateral surface scr generation characterized by the surface generation velocity sg , (3) surface scr generation under the gate characterized by the
C
C A
A
C
Cinv Ci
B VG1 VG
0 (a) Fig. 7.24
C
Cinv B
Ci
tf
0
t
(b)
The C –VG and C − t behavior of an MOSC pulsed into deep depletion.
RECOMBINATION LIFETIME—ELECTRICAL MEASUREMENTS
427
VG
W
s′g
tg d
Ln
(4)
sc
Fig. 7.25
(2) sg
(3)
(1)
pType (5)
Thermal generation components of a deepdepleted MOS capacitor.
surface generation velocity s’g , (4) quasineutral bulk generation characterized by the minority carrier diffusion length Ln , and (5) back surface generation characterized by the generation velocity sc . Components 1 and 2 depend on the scr width, discussed in Section 7.6.2, and 3–5 are independent of the scr width. The capacitance depends on the gate voltage and on the inversion charge Qn as122 Cox C(t) = 1 + 2(VG′ (t) + Qn (t)/Cox )/V0
(7.101)
where V ′ G (t) = VG (t) − VF B and V0 = qKs ε0 NA /Cox 2 . Solving Eq. (7.101) for V ′ G and differentiating with respect to t gives 1 dQn qKs εo NA dC dVG =− − dt Cox dt C3 dt
(7.102)
with dVF B /dt = 0. In Eq. (7.102) we have dropped the time dependence designation “(t)” for simplicity. Equation (7.102) is an important equation relating the gate voltage rate of change with time to inversion charge and capacitance rate of change with time. For the pulsed capacitor, VG is constant, dVG /dt = 0, and Eq. (7.102) solved for dQn /dt becomes qKs εo Cox NA dC dQn =− dt C3 dt
(7.103)
where dQn /dt represents the thermal generation rates in Fig. 7.25 qn2 Dn qni W qni sg AS dQn = G1 + G2 + G3 + G4 + G5 = − − − qni sg′ − i ′ (7.104) dt τg AG NA Ln
428
CARRIER LIFETIMES
where AS = 2πrW is the area of the lateral scr (assuming the lateral scr width to be identical to the vertical scr width W ) and AG = πr 2 is the gate area. Ln ′ is an effective diffusion length that couples bulk and back surface generation and is given by122 L′n = Ln
cosh(d/Ln ) + (sc Ln /Dn ) sinh(d/Ln ) (sc Ln /Dn ) cosh(d/Ln ) + sinh(d/Ln )
(7.105)
The surface generation velocity sc depends on the type of back contact. For a psemiconductormetal contact, the surface generation velocity is very high. A pp+ semiconductormetal has low sc because the lowhigh pp+ contact is a minority carrier barrier.123 The first two terms in Eq. (7.104) are scr widthdependent generation rates. Here we consider the last two scr widthindependent rates. Those with an ni dependence all exhibit identical temperature dependence. However, G4 has a ni 2 dependence, causing it to increase faster with temperature. This is the basis for the recombination lifetime measurement. G4 dominates for temperatures above about 75◦ C. When dQn /dt = −qn2i Dn /NA Ln ′ is substituted into Eq. (7.103)122 C= √
Ci 1 − t/t1
(7.106)
where t1 = (Ks /Kox )(Cox /Ci )2 (NA /ni )2 (tox /2)(Ln ′ /Dn ) and Ci is defined in Fig. 7.24. The measurement consists of a Ct plot. When quasineutral region generation dominates, 1 − (Ci /C)2 plotted against t has a slope of 1/t1 . The diffusion length is determined from t1 . To ensure that qnr generation dominates, the [1 − (Ci /C)2 ] versus t curve should be linear. If it is not, then the measurement temperature is probably too low. 7.5.5
Other Techniques
ShortCircuit Current Decay: For reverserecovery, the diode current is switched from forward to reverse; for opencircuit voltage it is switched from forward to zero current. In the shortcircuit current decay method the current is switched from forward current to shortcircuit current or zero voltage. Emitter minority carriers play a relatively minor role in this measurement because they recombine very quickly when the diode is shortcircuited.124 – 125 Conductivity Modulation: The conductivity modulation technique was developed to measure the recombination lifetime in epitaxial layers with thicknesses less than the minority carrier diffusion length. The measured lifetime is neither affected by substrate recombination nor by recombination in heavily doped regions. The structure consists of alternate n+ and p+ stripes diffused or implanted into a pepi layer on a p+ substrate. All p+ stripes are connected to each other, and all n+ stripes are connected to each other forming a lateral n+ pp+ diode. The spacing between stripes is smaller than the minority carrier diffusion length. The lateral diode is forward biased. A small ac voltage is superimposed on the dc bias, and the ac current due to recombination in the epitaxial layer is measured and related to the recombination lifetime.126 By applying a dc voltage to the p+ substrate, it is possible to profile the lifetime through the epitaxial layer.
GENERATION LIFETIME—ELECTRICAL MEASUREMENTS
7.6 7.6.1
429
GENERATION LIFETIME—ELECTRICAL MEASUREMENTS GateControlled Diode
The generation lifetime τg is determined by junction leakage current and MOS capacitor storage time measurements. One device to characterize the generation parameters is the threeterminal gatecontrolled diode, consisting of a p substrate, an n+ region (D), a circular gate (G) surrounding the n+ region, and a circular guard ring (GR) surrounding the gate in Fig. 7.26. The gate is sometimes located in the center surrounded by a circular n+ region. The gate should overlap the n+ region slightly to prevent potential barriers. The guard ring should be close to the gate and bias the semiconductor into accumulation to isolate the gatecontrolled diode from the rest of the wafer. Devices can also be decoupled by doping the semiconductor between the devices more heavily. We give here the necessary background for generation lifetime and surface generation velocity measurements. Figure 7.26 shows three generation regions: (1) the diode scr (J), (2) the gateinduced scr (GIJ), and (3) the depleted surface (S) under the gate. Each region contributes a current with the total current IJ + IGI J + IS . Let us first consider the semiconductor under the gate with the diode shortcircuited to the substrate (VD = 0). The surface is accumulated for VG < VF B , at flatband for VG = VF B , depleted for VF B < VG < VT and inverted for VG > VT . Accumulation and flatband conditions remain unchanged when the diode is reverse biased, but depletion and inversion conditions change. For diode voltage VD = 0, depletion holds for 0 < φs < VD + 2φF and inversion for φs ≥ VD + 2φF , with the surface potential φs related to the gate voltage by Eq. (6.16) and φF = (kT /q) ln(NA /ni ). The diode is biased at a constant voltage VD1 , and the gate voltage is varied. The surface under the gate is accumulated for negative gate voltage −VG1 , illustrated in Fig. 7.27(a). The measured current is the diode scr generated current IJ shown in Fig. 7.27(a) and by point A in (d). The current increase for more negative gate voltages has been attributed to weak breakdown of the gateinduced n+ p+ junction at the surface. At VG = VF B the semiconductor is at flatband, the diode scr width is the same at the surface as in the bulk. D
G
GR
n+ (3)
(2) (1)
pType
Fig. 7.26 The gatecontrolled diode. D is the n+ p diode, G the gate, and GR the guard ring, illustrating the various generation mechanisms and locations.
430
CARRIER LIFETIMES
−VG1
VD1
VD1
VG2
n+
WG IJ
IJ
IGIJ
IS
W
pType
pType
I
I
(b)
(a) VD1
VG3
I B
n+
IS C
IGIJ IJ
A IJ
pType
−VG1 0 VFB
IGIJ VG2
VG3
VG
I
(c)
(d)
Fig. 7.27 Gatecontrolled diode in (a) accumulation, (b) depletion, (c) inversion; (d) shows the currentvoltage characteristic with points A, B, and C corresponding to (a), (b), and (c).
The surface under the gate depletes for VG > VF B , and the current increases rapidly, due to the surface generation current IS and the gateinduced scr current IGIJ in Fig. 7.27(b). Higher gate voltages lead to a more gradual current increase as the scr under the gate widens. Gate voltage VG2 (point B in Fig. 7.27(d)) is characteristic of this part of the currentvoltage curve, the surface potential lies in the range 0 < φs < VD1 + 2φF , and the scr width under the gate is given by
WG,dep
Ks tox = Kox
2(VG − VF B ) −1 1+ V0
(7.107)
assuming no inversion charge. The surface inverts for surface potential φs ≥ VD1 + 2φF , and the gate scr width pins to
WG,inv =
2Ks εo (VD1 + 2φF ) qNA
(7.108)
GENERATION LIFETIME—ELECTRICAL MEASUREMENTS
431
The junction scr width is WJ =
2Ks εo (VD1 + Vbi ) qNA
(7.109)
with Vbi = (kT /q) ln(NA ND /ni 2 ) the builtin potential. Surface generation drops precipitously when the surface inverts and IS effectively disappears, as shown by the inverted surface in Fig. 7.27(c). Further gate voltage increases beyond the inversion voltage give no further current changes. This is also evident from Eq. (7.15), which shows high surface generation for a depleted surface when ps and ns are low and low surface generation when either ps or ns is high. Thermal generation is reduced for heavily inverted surfaces, because most interface traps are occupied by electrons. Assuming zero surface generation, the current is due to the junction current IJ and the fieldinduced junction current IFIJ , shown in Fig. 7.27(c) and by C in Fig. 7.27(d). Experimental currentvoltage curves are shown in Fig. 7.28. In these curves the current does increase for +VG due to diode nonidealities not discussed here. There is a sufficiently high reverse bias for the mobile carrier density to be negligible in the scr and at the depleted surface. The bulk and surface generation rates are given by Eqs. (7.20) and (7.22). The bulk scr generation current is qG × volume and the surface component is qGS × area, where volume and area are the thermal generation volume and area. The total current is I = IJ + IGI J + IS with IJ =
qni WJ AJ qni WG AG ; IGIJ = ; IS = qni sg AG τg,J τg,G
(7.110)
where τg,J and τg,G are the generation lifetimes in the diode and gate region, respectively. To extract the generation parameters one must measure or calculate the various scr widths. The widths can be experimentally determined from capacitance measurements, but it is usually more convenient to calculate them using Eqs. (7.107) to (7.109). To determine the surface generation velocity, one usually makes I –VG measurements at low diode voltages (VD ≈ 0.5–1V), thereby increasing the importance of surface current relative to bulk current. It is also possible, of course, to determine the generation lifetime 400 VD = 2 V
Current (pA)
300
200
1.5 V
100
1V 0.5 V
0 −1
Fig. 7.28
0
1 2 3 Gate Voltage (V)
4
5
Experimental gatecontrolled diode currentvoltage characteristics.
432
CARRIER LIFETIMES
under the gate separately from the generation lifetime under the n+ diffusion and to profile both as a function of depth.127 The theory discussed so far was originally proposed by Grove and Fitzgerald.128 It is based on several simplifying assumptions. It assumes the current to be due to scrgenerated current only. This is a reasonable assumption for Si devices at room temperature, but the quasineutral current component may not be negligible for highlifetime devices. The ratio of the bulk scr current to the bulk quasineutral region current, that is, component 1 to component 4 in Eq. (7.104), becomes √ √ NA W τr τr NA W Ln Iscr = = √ (7.111) ≈ 36 Iqnr n i Dn τ g τg n i Dn τ g for NA /ni = 106 , W = 2 µm, Dn = 30 cm2 /s and Ln = (Dn τr )1/2 . For τg = τr = 1 µs we find the ratio to be 36,000, and scr current clearly dominates and for τg = 1 ms and τr = 100 µs, it is 360. The ratio approaches unity for temperatures above room temperature. When the ratio in Eq. (7.111) approaches unity, quasineutral region current becomes important and Eq. (7.110) no longer holds. The assumption of total depletion of the surface before inversion has been shown not to be the case.129 The lateral surface current inverts the surface weakly for all but a very small fraction of the channel for gate biases far below the gate voltage required to invert the surface strongly. Active devices are frequently surrounded by implantationdoped/thickoxide channel stops. These channelstop sidewalls contribute additional current, and the gatecontrolled diode is an effective test structure to measure this current.130 7.6.2
Pulsed MOS Capacitor
The pulsed MOS capacitor lifetime measuring technique is commonly used to determine τg . Many papers have been written on the basic method, first proposed by Zerbst in 1966,131 and on subsequent variations. A review of the various methods can be found in Kang and Schroder.132 We give the most relevant concepts and equations here for three popular versions of this method, leaving the details to the published literature. Zerbst Plot: The MOS capacitor is pulsed into deep depletion, and the capacitancetime curve is measured, as shown in Fig. 7.29. An experimental roomtemperature C − t curve is shown in Fig. 7.29(a). The capacitance relaxation is determined by thermal ehp generation, which can be written as qni (W − Winv ) qni sg AS qni (W − Winv ) dQn =− − − qni seff = − − qni seff (7.112) dt τg AG τg,eff where Winv = (4Ks εo φF /qNA )1/2 and τg,eff is defined by considering only the scr generation rates qni (W − Winv ) qni sg AS 2πrsg (W − Winv ) W − Winv dQn,scr =− − = −qni + dt τg AG τg πr 2 2sg τg qni (W − Winv ) qni (W − Winv ) 1+ =− =− τg r τg,eff (7.113) The effective scr width (W − Winv ) approximates the actual generation width and ensures that at the end of the C − t transient the scr generation becomes zero. The term qni seff
GENERATION LIFETIME—ELECTRICAL MEASUREMENTS
433
Capacitance (pF)
20
15
10
5
0
0
20
40
60 Time (s) (a)
80
100
120
−d[(Cox/C)2]/dt (s−1)
5 4 3 2 tg,eff = 229 µs
1
seff = 0.32 cm/s 0
0
0.5
1 (Cinv/C−1) (b)
1.5
2
Fig. 7.29 (a) C − t response and (b) Zerbst plot. Reprinted with permission after Kang and Schroder.132
accounts for the scr widthindependent generation rates (surface generation under the gate and in the quasineutral region) with seff = sg′ +
n i Dn NA L′n
(7.114)
The scr width is related to the capacitance C through W = Ks εo
Cox − C Cox C
(7.115)
Combining Eqs. (7.103), (7.112) and (7.115) gives
−
d dt
Cox C
2
=
2ni Cox τg,eff NA Cinv
2Kox ni seff Cinv −1 + C Ks tox NA
using the identity (2/C 3 ) dC/dt = −[d(1/C)2 /dt].
(7.116)
434
CARRIER LIFETIMES
Equation (7.116) is the basis of the wellknown Zerbst plot, −d(Cox /C)2 /dt versus (Cf /C − 1), shown in Fig. 7.29(b). The curved portion near the origin is when the device approaches equilibrium and the curvature at the other end of the straight line has been attributed to fieldenhanced emission from interface and/or bulk traps.133 The slope of the straight line is 2ni Cox /NA Cf τg,eff and its extrapolated intercept on the vertical axis is 2ni Kox seff /Ks tox NA . The slope is a measure of the scr generation parameters τg and sg , whereas the intercept is related to the scr widthindependent generation parameters s ′ g , Ln and sc . seff obtained from the intercept should not be interpreted as the surface generation velocity as is sometimes done. It includes not only the quasineutral bulk generation rates, but a more detailed analysis of the C − t response shows that the inherent inaccuracy of the (W − Winv ) approximation for the generation width can lead to a nonzero intercept even if seff = 0.134 It is instructive to examine the two axes of the Zerbst plot for a better insight into the physical meaning of such a plot. For the identity that leads to Eq. (7.116), we find from Eq. (7.103) and (7.116) −
d dt
Cox C
2
∼
dQn Cinv ; − 1 ∼ W − Winv dt C
(7.117)
The Zerbst plot vertical axis is proportional to the total ehp carrier generation rate or to the generation current and the horizontal axis is proportional to the scr generation width. So this rather complicated plot is nothing more than a plot of generation current versus scr width. The measured C − t transient times are usually quite long with times of tens of seconds to minutes being common. The relaxation time tf is related to τg,eff by135 – 136 tf ≈
10NA τg,eff ni
(7.118)
This equation brings out a very important feature of the pulsed MOSC technique, which is the magnification factor NA /ni built into the measurement. Values of τg,eff range over many orders of magnitude, but representative values for high quality silicon devices lie in the range of 10−4 to 10−2 s. Equation (7.118) predicts the actual C − t transient time to be 10 to 104 s. These long times point out a virtue of this measurement technique. To measure lifetimes in the microsecond range, it is only necessary to measure capacitance recovery times on the order of seconds. The time magnification factor in Eq. (7.118) is also a disadvantage. Such long measurement times preclude mapping of large number of devices. Several approaches have been proposed to reduce the measurement time. Equations (7.112) and (7.114) show seff ∼ ni 2 . As the temperature is raised, this scr widthindependent term becomes more important and the relaxation time is considerably reduced. The Zerbst plot is shifted vertically retaining the slope determined by τg,eff .136 As pointed out in Section 7.5.4, the temperature should not be so high that quasineutral generation dominates, for then it is impossible to extract τg,eff . A tf reduction is also attained by illuminating the sample.137 The measurement time can also be reduced by driving the MOSC into deep depletion by a voltage pulse and then into inversion by a light pulse. Subsequently, a series of small pulses of opposite polarity and varying amplitudes are superimposed on the depleting voltage, driving the device into weaker inversion and then into depletion. C and dC/dt are determined after each pulse to construct a Zerbst plot. The total measurement time
GENERATION LIFETIME—ELECTRICAL MEASUREMENTS
435
can be reduced by as much as a factor of 10.138 In yet another simplification the scr width is calculated from the C − t response, and ln(W ) is plotted against time.139 Such a plot is nearly linear. The line can be extrapolated to tf without recording the entire curve by using only the initial portion of the C − t response. One caution about MOSC generation lifetime measurement is the possibility of gate oxide currents for thin oxides.140 After pulsing the device into deep depletion, the inversion layer builds up as a function of time until equilibrium is attained. If part of this inversion layer leaks through the oxide during the measurement, obviously the measurement time is extended, leading to an incorrect τg,eff . Solutions to this problem are using lower gate voltages for which gate oxide leakage current is negligible or using a constant charge approach, as discussed for the coronaoxidesemiconductor method later in this section. Another issue for thin oxides is that tunneling electrons or holes when they enter the semiconductor from the gate have sufficient energy to generate additional ehps by impact ionization.141 A contactless capacitance measurement technique uses a metal probe held slightly less than one micrometer above the sample. C –V and C − t measurements have been implemented without the need of a permanent contact on the sample.142 Pulsed capacitor measurements can also be implemented in silicononinsulator (SOI) samples, where the SOI MOSFET drain current is measured, illustrated in Fig. 7.30. The device is biased above threshold (VG > VT ) with some back gate bias VGB1 . The back gate bias is then pulsed to VGB2 and the resulting drain current transient is measured. The analysis is similar to C − t analyses and τg,eff can be extracted.143 It is also possible to extract the SOI recombination lifetime. With the SOI MOSFET back gate grounded, the front gate is switched from depletion or accumulation to strong inversion. The minority carriers to form the inversion channel are rapidly supplied by the source/drain regions. The positive front gate pulse leads to a scr region extension, but the majority carriers expelled from this region cannot be removed instantaneously and are stored in the neutral body, inducing a temporary increase in the body potential, reducing the threshold voltage and increasing the drain current. Equilibrium is reached through carrier recombination to remove the excess majority carriers.144 CurrentCapacitance: The Zerbst technique requires differentiation of the experimental data and a knowledge of NA . The currentcapacitance technique requires neither, but one must measure the current and the capacitance of a pulsed MOSC. The current is I = AG
Buried Oxide
Si Film pType VGB
Fig. 7.30
VDS n+
p
dW dQn + qNA dt dt
(7.119)
ID
VGS n+
VGB
t
VGB1 VGB2 ID t
Generation lifetime measurement schematic for SOI devices.
436
CARRIER LIFETIMES
10
I/(1 − C/Cox) (pA)
8 6 4 2 0
tg,eff = 226 µs seff = 0.16 cm/s 0
2
6
4 (1/C1/Cinv) (10
10
8
−1
F )
Fig. 7.31 Current versus inverse capacitance plot for the device whose Zerbst plot is shown in Fig. 7.29. Reprinted with permission after Kang and Schroder.132
where the first term is the generation and the second term the displacement current. The currentcapacitance relationship is133 qKs εo A2G ni I = 1 − C/Co x τg,eff
1 1 − C Cinv
+ qAG ni seff
(7.120)
From the C − t and the I − t curve one plots I/(1 − C/Cox ) versus (1/C − 1/Cf ). The slope of this curve gives τg,eff and the intercept gives seff , as shown in Fig. 7.31. For a generation lifetime profile, Eq. (7.120) can be written as qKs εo A2G ni d(Cox /C)/dt Cox d[I /(1 − C/Cox )]/dt
τg,eff =
(7.121)
By measuring current and capacitance simultaneously and differentiating the data, it is possible to plot a profile of τg,eff directly without knowing the doping profile. In a modified currentcapacitance method, leading to much reduced measurement times, the scr generation current density145 Jscr =
Cox qni (W − Winv ) J = + qni seff Cox − C τg,eff
(7.122)
is combined with the scr width W = KS εo Ag
1 1 − C Cox
(7.123)
The current and the highfrequency capacitance are measured simultaneously immediately after pulsing into deep depletion. The pulse duration is just long enough to measure the capacitance and the current. From these data the scr width W and the scr current density Jscr are determined. The pulse height is continuously increased, probing deeper
437
GENERATION LIFETIME—ELECTRICAL MEASUREMENTS
into the sample. The measurement time is determined solely by the acquisition time of the capacitance meter and the ammeter multiplied by the number of data points. Jscr is plotted versus W and the slope of this curve yields the effective generation lifetime according to τg,eff =
qni (W − Winv ) dJscr /dW
(7.124)
Such a plot is similar to Fig. 7.31. The doping concentration need not be known. Linear Sweep: In the linear sweep technique a linearly varying voltage is applied to the gate of an MOSC of a polarity to drive the device into depletion. We showed in Chapter 6 that for sufficiently slow sweep rates, the equilibrium C –VG curve is traced out. We also know that when the sweep rate is high, the pulsed MOSC deepdepletion curve is obtained. For intermediate sweep rates, an intermediate trace is swept out, shown in Fig. 7.32, lying between the deepdepletion and equilibrium curves. The interesting point about this curve is its saturation characteristic.146 Assume the voltage sweeps from point A in Fig. 7.32 to the right. For voltages more positive than VB , the scr widens beyond Winv , with the capacitance driven below Cinv . Electronhole pair generation attempts to reestablish equilibrium, but the gate voltage continues to drive the device into deep depletion, further increasing W . This in turn enhances the generation rate that is proportional to W . At the voltage Vsat the attempt by the linearly varying gate voltage to drive the device into deeper depletion is exactly balanced by the generation rate holding it at that capacitance. The capacitancevoltage curve saturates at Csat . For a constant sweep rate, dVG /dt = R, Eq. (7.102) becomes qKs εo Cox NA dC dQn =− − Cox R dt C3 dt
(7.125)
Using the generation rate expression Eq. (7.112), leads to −
d dt
Cox C
2
=
2 V0
qKs εo ni (Cinv /C − 1) qni seff + −R Cinv Cox τg,eff Cox
C A
Low sweep rate (equilibrium)
B Cinv
Intermediate (sat’n)
Csat
High (deep depl) 0
Fig. 7.32
VB
Vsat
VG
Inversion, saturation, and deepdepletion MOSC curves.
(7.126)
438
CARRIER LIFETIMES
6
R (V/s)
4
2 tg,eff = 200 µs sg,eff = 0.2 cm/s 0
0
0.2
0.4 Cinv/Csat − 1
0.6
0.8
Fig. 7.33 Linear ramp plot for the device whose Zerbst plot is shown in Fig. 7.29. Reprinted with permission after Kang and Schroder.132
When the device enters saturation, Csat changes neither with voltage nor with time and the left side of Eq. (7.126) becomes zero and R=
qKs εo ni (Cinv /Csat − 1) qni seff + Cinv Cox τg,eff Cox
(7.127)
Equation (7.127) gives the relationship between the linear sweep rate R and the generation parameters τg,eff and seff . In the experiment, a series of C –VG curves at different linear sweep rates are plotted. The Csat values are taken from these curves, and a plot of R versus (Cinv /Csat − 1) yields a straight line of slope qKs εo ni /Cinv Cox τg,eff and intercept qni seff /Cox . Similar to the Zerbst plot, τg,eff is obtained from the slope and seff from the intercept. Experimental data for the linear sweep method are shown in Fig. 7.33 for the device whose Zerbst plot is shown in Fig. 7.29. Note the good agreement between the experimentally determined values for τg,eff and seff . The linear sweep technique does not require the acquisition of an entire C − t curve, nor the differentiation of the experimental data. It does, however, require multiple saturating C –VG curves. For those devices with high lifetimes and consequent long C − t transients, it is found that very low sweep rates are required, with resultant long data acquisition times. The use of a feedback circuit, with the capacitance preset to a certain value and the linear sweep rate adjusting itself through feedback to maintain this preset value, reduces the data acquisition time.147 Computer automation of the linear sweep technique has also been developed.148 The technique has also been adapted for lifetime measurements in silicononinsulator materials.149 CoronaOxideSemiconductor: The coronaoxidesemiconductor (COS) technique is illustrated in Fig. 7.34 (corona charge characterization is discussed in Chapter 9).150 Positive or negative charge from a corona source is deposited on the semiconductor sample surface. In Fig. 7.34, negative charge is deposited on an oxidized pSi wafer to bias the substrate into accumulation followed by a smaller area positive charge driving the sample
GENERATION LIFETIME—ELECTRICAL MEASUREMENTS
439
V Corona source +
Inversion charge Accumulation charge − − − +++ − − −
Kelvin probe
V(t)
− − − +++ − − −
Wafer Wafer chuck High speed stage
Fig. 7.34
Coronapulsed deepdepletion measurement apparatus.
into deep depletion. The relaxation to equilibrium is monitored by measuring the Kelvin probe voltage as a function of time. The ability to deposit both negative and positive charge has the distinct advantage over MOSC measurements of providing a zerogap guard ring, reducing perimeter generation. The gate and oxide voltages of an MOSC or COSC are VG = VF B + Vox + φs ; Vox =
QS QG =− Cox Cox
(7.128)
with QG the gate charge density and QS the semiconductor charge density. Equation (7.128) becomes VG − VF B = φ s −
QS Qb − Qn = φs − Cox Cox
(7.129)
where Qn is the inversion charge density and Qb the bulk charge density. After corona charge is deposited, QG and Vox remain constant. Differentiating Eq. (7.128) leads to dφs dVG = (7.130) dt dt assuming dVF B /dt = 0. The bulk charge density is Qb = −qNA W = − 2qKs εo NA φs
(7.131)
where W is the spacecharge region width. With QG and QS constant with time dQn dQb dQn dQS dW =0=− + =− − qNA dt dt dt dt dt
(7.132)
or, using Eq. (7.131), Ks εo dφs Ks εo dVG qKs εo NA dφs dQn =− =− =− dt 2φs dt W dt W dt
(7.133)
440
CARRIER LIFETIMES
4
dVG/dt (V/s)
tg = 47 µs
126 µs 2
540 µs
0
0
5
10
15
20
25
W(W−Winv) (µm)2
Fig. 7.35
COS generation lifetime plot.
With dQn /dt given by Eq. (7.112) qni W dVG = dt Ks εo
W − Winv + seff τg,eff
(7.134)
The dependence of the voltage rate of change on W (W − Winv ) is shown in Fig. 7.35. The linear relationship is in good agreement with the prediction of Eq. (7.134). The slopes of these lines give τg,eff . All lines intersect at the origin, implying seff to be negligibly small.
7.7
STRENGTHS AND WEAKNESSES
Recombination Lifetime: Recombination lifetime or diffusion length measurements have become ubiquitous in the semiconductor industry, because they are a good indicator of wafer contamination. Among the optical recombination lifetime measuring methods, the microwave reflection or inductive coupling photoconductance decay technique is commonly used. Its major strength is the contactless nature and rapid measurement. Its major weakness is the unknown surface recombination velocity. If the sample thickness can be changed, then both the bulk lifetime and the surface recombination velocity can be extracted. The quasisteadystate photoconductance method is a more recent method and has found wide acceptance in the photovoltaic community. Its main strength is a measure of the lifetime as a function of injection level in one measurement. One of its disadvantages is the large sample area (several cm2 ) precluding high density mapping. Free carrier absorption through the use of black body emitters is an interesting method allowing a lifetime map to be obtained in a very short time through the use of two dimensional imagers. Another common optical technique is surface photovoltage. A chief application is the detection of iron in pSi. It is a low injection level method and is not subject to trapping. The opencircuit voltage decay method is the most common electrical recombination lifetime method. It is easy to interpret, but a junction diode is required. Measured τr or Ln mean little for thin layers, e.g., epitaxial layers on highly doped substrates, denuded
APPENDIX 7.1
441
zones on heavily precipitated substrates, or silicononinsulator films. Such layers are best characterized through generation lifetime measurements.94 Generation Lifetime: The generation lifetime is commonly determined with the pulsed MOS capacitor. The Zerbst plot implementation is the most common, but the current versus inverse capacitance is easier to interpret because the doping density of the sample need not be known. Since τg is measured in the spacecharge region of a reversebiased device (diode or MOS device), it lends itself easily for the characterization of thin layers, e.g., epitaxial layers on highly doped substrates,94 denuded zones on heavily precipitated substrates, or silicononinsulator films. Furthermore, since the scr width can be varied by an applied voltage, it is possible to generate a τg depth profile, that is difficult to do with τr measurements, because the measurement depth for τr and Ln measurements is the minority carrier diffusion length. To avoid contact formation, one can use the coronaoxidesemiconductor approach, replacing the metal or polySi gate with corona charge.
APPENDIX 7.1 Optical Excitation Steady State: We consider the ptype semiconductor of Fig. A7.1. It is a wafer of thickness d, reflectivity R, minority carrier lifetime τ , minority carrier diffusion coefficient D, minority carrier diffusion length L, and surface recombination velocities sr1 and sr2 at the two surfaces. Monochromatic light of photon flux density , wavelength λ, and absorption coefficient α, is incident on one side of this wafer. Carriers generated by absorbed photons diffuse in the xdirection and the wafer is infinite in the y − z plane, allowing edge effects to be neglected. The steadystate, smallsignal excess minority carrier density n(x) is obtained from a solution of the onedimensional continuity equation d 2 n(x) n(x) + G(x) = 0 (A7.1) − D dx 2 τ
R sr1
sr2
F(a) t, D, L
pType
0
Fig. A7.1
d
x
Homogeneous ptype sample geometry with optical excitation.